410 99 23MB
English Pages XV, 537 [540] Year 2020
Graduate Texts in Physics
Keh Yung Cheng
III–V Compound Semiconductors and Devices An Introduction to Fundamentals
Graduate Texts in Physics Series Editors Kurt H. Becker, NYU Polytechnic School of Engineering, Brooklyn, NY, USA JeanMarc Di Meglio, Matière et Systèmes Complexes, Bâtiment Condorcet, Université Paris Diderot, Paris, France Morten HjorthJensen, Department of Physics, Blindern, University of Oslo, Oslo, Norway Bill Munro, NTT Basic Research Laboratories, Atsugi, Japan William T. Rhodes, Department of Computer and Electrical Engineering and Computer Science, Florida Atlantic University, Boca Raton, FL, USA Susan Scott, Australian National University, Acton, Australia H. Eugene Stanley, Center for Polymer Studies, Physics Department, Boston University, Boston, MA, USA Martin Stutzmann, Walter Schottky Institute, Technical University of Munich, Garching, Germany Andreas Wipf, Institute of Theoretical Physics, FriedrichSchillerUniversity Jena, Jena, Germany
Graduate Texts in Physics publishes core learning/teaching material for graduate and advancedlevel undergraduate courses on topics of current and emerging ﬁelds within physics, both pure and applied. These textbooks serve students at the MS or PhDlevel and their instructors as comprehensive sources of principles, deﬁnitions, derivations, experiments and applications (as relevant) for their mastery and teaching, respectively. International in scope and relevance, the textbooks correspond to course syllabi sufﬁciently to serve as required reading. Their didactic style, comprehensiveness and coverage of fundamental material also make them suitable as introductions or references for scientists entering, or requiring timely knowledge of, a research ﬁeld.
More information about this series at http://www.springer.com/series/8431
Keh Yung Cheng
III–V Compound Semiconductors and Devices An Introduction to Fundamentals
123
Keh Yung Cheng Department of Electrical and Computer Engineering University of Illinois at UrbanaChampaign Urbana, Illinois, USA Department of Electrical Engineering National Tsing Hua University Hsinchu, Taiwan
ISSN 18684513 ISSN 18684521 (electronic) Graduate Texts in Physics ISBN 9783030519018 ISBN 9783030519032 (eBook) https://doi.org/10.1007/9783030519032 © Springer Nature Switzerland AG 2020 This work is subject to copyright. All rights are reserved by the Publisher, whether the whole or part of the material is concerned, speciﬁcally the rights of translation, reprinting, reuse of illustrations, recitation, broadcasting, reproduction on microﬁlms or in any other physical way, and transmission or information storage and retrieval, electronic adaptation, computer software, or by similar or dissimilar methodology now known or hereafter developed. The use of general descriptive names, registered names, trademarks, service marks, etc. in this publication does not imply, even in the absence of a speciﬁc statement, that such names are exempt from the relevant protective laws and regulations and therefore free for general use. The publisher, the authors and the editors are safe to assume that the advice and information in this book are believed to be true and accurate at the date of publication. Neither the publisher nor the authors or the editors give a warranty, expressed or implied, with respect to the material contained herein or for any errors or omissions that may have been made. The publisher remains neutral with regard to jurisdictional claims in published maps and institutional afﬁliations. Cover image: © Victoria/Fotolia This Springer imprint is published by the registered company Springer Nature Switzerland AG The registered company address is: Gewerbestrasse 11, 6330 Cham, Switzerland
Preface
Since 1990, the creation of the World Wide Web and the strong surge of personal computer popularity, which promotes Internet usage, created a steep increase of Internet trafﬁc. In the meantime, wireless communication systems also have evolved rapidly through several generations with everincreasing bandwidth. To handle the vast amount of information trafﬁc flow, highspeed and widebandwidth networks are needed, which require IIIV compound semiconductorbased highspeed electronic and photonic devices. Furthermore, the realization of the ptype GaN not only led to widespread applications of IIInitridebased lightemitting diodes (LEDs) for solidstate lighting and fullcolor displays but also unlocked the opportunities for the development of nextgeneration power electronics using widebandgap semiconductors. On the other hand, miniaturization of the feature size of siliconbased integrated circuits is rapidly approaching the limit of Moore’s law. Taking advantage of the very high electron mobility of some IIIV alloys, the integration of compound semiconductor devices on silicon offers another opportunity for future developments. So the ﬁeld has continued to expand rapidly. Although a number of books devoted to speciﬁc subjects on compound semiconductors and devices are available with the emphasis on the state of the art, a single monograph providing a complete discussion of the whole ﬁeld is still lacking. It is not the purpose of this book to give an exhaustive treatment of compound semiconductors and devices. Rather, this book conveys the relevant fundamental physics, and material and device concepts, of IIIV compound semiconductors in a coherent manner within a single text, so as to provide the reader with basic concepts and ideas needed for understanding related literature and developments. The preliminary concepts gained also serve as foundations for more advanced studies of compound semiconductorbased optoelectronics and highspeed electronic devices. The content of this book was developed based on a onesemester course for beginning graduate students and advanced seniors in the Department of Electrical and Computer Engineering (ECE) at the University of Illinois at UrbanaChampaign (UIUC). Normally, the students in this course have the background
v
vi
Preface
in electromagnetic theory and have been exposed to semiconductors at the level of Streetman and Banerjee, SolidState Electronics Devices, 6th ed. (Prentice Hall 2006). Certain students may have gained the knowledge of solidstate physics. Students from other engineering disciplines such as materials science and engineering also attended the class. Because of the diverse background of students interested in these subjects, introductory materials are included throughout the book to help bring all students to the same starting point. The book is organized into four parts: Semiconductor fundamentals, Compound semiconductor materials, Properties of heterostructures, and Heterostructure devices. The book starts with a concise introduction to the historical development of the semiconductor industry and the relevance of IIIV compound semiconductors. Chapters 2 and 3 introduce basic semiconductor concepts with supplementary materials on concepts beyond silicon. It also serves as a brief review for those who are familiar with the topics. Chapter 4 describes the physical properties of compound semiconductors including some distinctive features of multielement alloys. The material technologies of preparing compound semiconductor crystals in bulk or thin ﬁlm forms and postgrowth modiﬁcation of material structures are presented in Chap. 5. The unique properties of heterostructures formed in compound semiconductors are then introduced in Chaps. 6–8. In Chap. 6, the alignments of energy bands at heterojunctions are derived ﬁrst for the construction of heterostructures. Then strain effects on bandedge energies are discussed. The fundamental electrical and optical properties of heterostructures follow in Chaps. 7 and 8, respectively. Finally, important highspeed devices and photonic devices are presented in the last two chapters. Two of the widely used heterostructure highspeed devices—high electron mobility transistor (HEMT) and heterojunction bipolar transistor (HBT)— are discussed in Chap. 9. In addition, the key breakthroughs that led to the successful development of long sought after IIIV MOSFETs are also discussed. Chapter 10 deals with photonic devices including various semiconductor injection lasers, LEDs, quantumwell infrared photodetectors, and an integrated optoelectronic device—the transistor laser. To assist students in probing further into the subject matter discussed, cited journal articles and a list of general references are added at the end of each chapter. Each chapter also contains an assortment of problems at its end to assess students’ ability to apply the principles of the chapter. Finally, it is my great pleasure to acknowledge a number of people who have encouraged me to take the charge of developing this book. I thank colleagues of the ECE Department at UIUC who have collaborated with me on various inspiring IIIV compound semiconductorrelated device research projects, particularly Profs. Milton Feng, Nick Holonyak Jr., K. C. Hsieh, and the late ShunLien Chuang. I am especially grateful to Nick Holonyak Jr. for many stimulating discussions during the coffee hours on technical issues as well as on his personal experience in early days of semiconductor developments. I am grateful to James Hutchinson for proofreading the whole manuscript. The continuous guidance and encouragement offered by Dr. Alfred Y. Cho of Bell Laboratories over the years are highly
Preface
vii
appreciated. The National TsingHua University in Hsinchu, Taiwan, provided an ideal writing environment through the Ho Chin Tui chair professorship. Finally, I wish to thank my wife Kuo Ping for her encouragement and patience during the course of this endeavor. Walnut Creek, California, USA
Keh Yung (Norman) Cheng
Contents
1
2
.... .... ....
1 1 1
.... .... ....
4 7 9
Atomic Bonding and Crystal Structures . . . . . . . . . . . . . . . . . . . . . 2.1 Crystal Structures and Symmetry . . . . . . . . . . . . . . . . . . . . . . . 2.1.1 Crystal Structures . . . . . . . . . . . . . . . . . . . . . . . . . . . . 2.1.2 Crystallographic Notation—Miller Indices . . . . . . . . . . 2.1.3 Lattice Symmetries . . . . . . . . . . . . . . . . . . . . . . . . . . . 2.2 Ionic Bond and Interatomic Forces . . . . . . . . . . . . . . . . . . . . . 2.3 Covalent Bond and sp3 Hybrid Orbit . . . . . . . . . . . . . . . . . . . . 2.3.1 General Properties of Covalent Bond Formation . . . . . . 2.3.2 Directional Property of Covalent Bonds . . . . . . . . . . . . 2.3.3 sp3 Hybrid Orbit . . . . . . . . . . . . . . . . . . . . . . . . . . . . 2.3.4 Mixed IonicCovalent Bonds . . . . . . . . . . . . . . . . . . . 2.4 Major Semiconductor Crystal Structures . . . . . . . . . . . . . . . . . . 2.4.1 Diamond Structure . . . . . . . . . . . . . . . . . . . . . . . . . . . 2.4.2 ZincBlende Structure . . . . . . . . . . . . . . . . . . . . . . . . . 2.4.3 Wurtzite Structure . . . . . . . . . . . . . . . . . . . . . . . . . . . 2.5 Reciprocal Lattice, Diffraction Condition, and Brillouin Zone . . . 2.5.1 Crystal Diffraction . . . . . . . . . . . . . . . . . . . . . . . . . . . 2.5.2 Reciprocal Lattice . . . . . . . . . . . . . . . . . . . . . . . . . . . 2.5.3 Properties of the Reciprocal Lattice Vector . . . . . . . . . 2.5.4 Diffraction Condition . . . . . . . . . . . . . . . . . . . . . . . . . 2.5.5 The Brillouin Zone . . . . . . . . . . . . . . . . . . . . . . . . . . . References . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . .
11 12 12 14 16 19 23 23 26 29 31 32 32 33 35 38 38 39 42 44 47 55
Introduction . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 1.1 Historical Perspective . . . . . . . . . . . . . . . . . . . . . . . . . . . 1.1.1 Rise of the Semiconductor Industry . . . . . . . . . . . 1.1.2 Development of III–V Compound Semiconductor Industry . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 1.2 Future Outlooks . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . References . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . .
ix
x
3
4
Contents
. . . . . . . .
. . . . . . . .
. . . . . . . .
. . . . . . . .
. . . . . . . .
57 57 58 60 64 67 67 70
. . . . . . . . .
. . . . . . . . .
. . . . . . . . .
. . . . . . . . .
. . . . . . . . .
72 75 75 77 80 81 84 88 93
. . . . .
. . . . .
. . . . .
. . . . .
. 93 . 97 . 98 . 99 . 103
Compound Semiconductor Crystals . . . . . . . . . . . . . . . . . . . . . 4.1 Structural Properties . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 4.1.1 Lattice Constant . . . . . . . . . . . . . . . . . . . . . . . . . . 4.1.2 Cleavage Properties . . . . . . . . . . . . . . . . . . . . . . . 4.1.3 Lattice Vibration—Phonons . . . . . . . . . . . . . . . . . 4.2 Electrical Properties . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 4.2.1 Effective Mass . . . . . . . . . . . . . . . . . . . . . . . . . . . 4.2.2 Mobility . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 4.2.3 Intentional Impurity . . . . . . . . . . . . . . . . . . . . . . . 4.2.4 Deep Levels . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 4.3 Free Carrier Concentration and the Fermi Integral . . . . . . . . 4.3.1 Free Carrier Concentrations in 3D Semiconductors . 4.3.2 Free Carrier Concentrations in 2D Semiconductor Structures . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 4.3.3 Carrier Concentration in the Multiple Valley Limit . 4.4 Surface States in Compound Semiconductors . . . . . . . . . . . 4.5 III–V Compound Semiconductors . . . . . . . . . . . . . . . . . . . 4.5.1 Lattice Constant . . . . . . . . . . . . . . . . . . . . . . . . . . 4.5.2 Bandgap Energy . . . . . . . . . . . . . . . . . . . . . . . . . .
. . . . . . . . . . . .
. . . . . . . . . . . .
. . . . . . . . . . . .
105 106 106 107 108 113 113 117 122 127 132 132
. . . . . .
. . . . . .
. . . . . .
136 137 138 141 141 144
Electronic Band Structures of Solids . . . . . . . . . . . . . . . . . . . 3.1 Free Electron Theory and Density of States . . . . . . . . . . 3.1.1 OneDimensional System . . . . . . . . . . . . . . . . . 3.1.2 ThreeDimensional System . . . . . . . . . . . . . . . . 3.1.3 Density of States (DOS) . . . . . . . . . . . . . . . . . . 3.2 Periodic Crystal Structure and Bloch’s Theorem . . . . . . . 3.2.1 Bloch’s Theorem . . . . . . . . . . . . . . . . . . . . . . . 3.2.2 Reduced Zone Representation . . . . . . . . . . . . . . 3.2.3 Empty Lattice Model—Energy Band Calculation for an FCC Crystal . . . . . . . . . . . . . . . . . . . . . . 3.3 Nearly Free Electron Approximation and the Energy Gap 3.3.1 Origin of Bandgaps . . . . . . . . . . . . . . . . . . . . . 3.3.2 Energy Gap—A Quantitative Approach . . . . . . . 3.4 The Kronig–Penney Model . . . . . . . . . . . . . . . . . . . . . . 3.4.1 Theoretical Model . . . . . . . . . . . . . . . . . . . . . . 3.4.2 Analysis . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 3.5 Effective Mass . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 3.6 Band Structures of Common Semiconductors . . . . . . . . . 3.6.1 General Trend of Energy Band Structure in Semiconductors . . . . . . . . . . . . . . . . . . . . . . 3.6.2 Valence Band . . . . . . . . . . . . . . . . . . . . . . . . . 3.6.3 Conduction Band . . . . . . . . . . . . . . . . . . . . . . . 3.6.4 Band Structures of Wurtzite Crystals . . . . . . . . . References . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . .
Contents
5
6
xi
4.6
III–N and Dilute III–V–N Compound Semiconductors 4.6.1 III–N Compounds . . . . . . . . . . . . . . . . . . . . 4.6.2 Dilute IIIVN Compounds . . . . . . . . . . . . . . References . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . .
. . . .
. . . .
. . . .
. . . .
. . . .
. . . .
. . . .
149 149 153 158
Material Technologies . . . . . . . . . . . . . . . . . . . . . . . . . . . . 5.1 Growth of Bulk Crystals . . . . . . . . . . . . . . . . . . . . . . 5.1.1 Phase Equilibria . . . . . . . . . . . . . . . . . . . . . . 5.1.2 Crystal Growth Techniques . . . . . . . . . . . . . . 5.2 Epitaxy . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 5.3 LiquidPhase Epitaxy . . . . . . . . . . . . . . . . . . . . . . . . 5.3.1 LPE Apparatus . . . . . . . . . . . . . . . . . . . . . . . 5.3.2 Phase Diagram . . . . . . . . . . . . . . . . . . . . . . . 5.3.3 LPE Growth Techniques . . . . . . . . . . . . . . . . 5.4 VaporPhase Epitaxy . . . . . . . . . . . . . . . . . . . . . . . . . 5.4.1 Chloride VPE . . . . . . . . . . . . . . . . . . . . . . . 5.4.2 Metalorganic Chemical Vapor Deposition . . . 5.5 Molecular Beam Epitaxy . . . . . . . . . . . . . . . . . . . . . . 5.5.1 MBE Apparatus . . . . . . . . . . . . . . . . . . . . . . 5.5.2 In Situ Surface Diagnosis Techniques . . . . . . 5.5.3 Flux Control of Molecular Beams . . . . . . . . . 5.5.4 Variations of Molecular Beam Sources . . . . . 5.6 Postgrowth Modiﬁcation of Material Structures . . . . . 5.6.1 ImpurityInduced Layer Disordering (IILD) of QuantumWell Heterostructures . . . . . . . . . 5.6.2 Wet Oxidation of AlContaining IIIV Alloys References . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . .
. . . . . . . . . . . . . . . . . .
. . . . . . . . . . . . . . . . . .
. . . . . . . . . . . . . . . . . .
. . . . . . . . . . . . . . . . . .
. . . . . . . . . . . . . . . . . .
. . . . . . . . . . . . . . . . . .
. . . . . . . . . . . . . . . . . .
161 162 162 164 170 171 172 173 174 176 176 180 182 183 184 187 188 190
. . . . . . . 190 . . . . . . . 195 . . . . . . . 201
Heterostructure Fundamentals . . . . . . . . . . . . . . . . . . . . . . . 6.1 Energy Band Alignment . . . . . . . . . . . . . . . . . . . . . . . . 6.1.1 Anderson’s Electron Afﬁnity Model . . . . . . . . . 6.1.2 ModelSolid Theory . . . . . . . . . . . . . . . . . . . . . 6.1.3 Empirical Band Alignment Models . . . . . . . . . . 6.2 Strained Layer Structures . . . . . . . . . . . . . . . . . . . . . . . 6.2.1 Critical Layer Thickness (hc) . . . . . . . . . . . . . . . 6.2.2 Cubic Crystal Under Stress . . . . . . . . . . . . . . . . 6.2.3 Strain Effect on BandEdge Energies . . . . . . . . . 6.3 BandEdge Energies in Strained Ternary and Quaternary Alloys . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 6.4 Strained Nitrides with Wurtzite Crystal Structure . . . . . . 6.4.1 BandEdge Energies of Strained Nitrides . . . . . . 6.4.2 Natural Band Alignments of IIINitrides . . . . . . 6.5 Construction of Heterostructure Band Diagrams . . . . . . . 6.5.1 Anisotype Np Heterojunctions . . . . . . . . . . . . . 6.5.2 Anisotype pN Heterojunctions . . . . . . . . . . . . .
. . . . . . . . .
. . . . . . . . .
. . . . . . . . .
. . . . . . . . .
. . . . . . . . .
203 204 204 206 210 214 214 217 223
. . . . . . .
. . . . . . .
. . . . . . .
. . . . . . .
. . . . . . .
228 231 231 234 235 235 237
xii
Contents
6.5.3 Isotype Nn and Pp Heterojunctions . . . . . . . . . . . . . . 237 6.5.4 Current Conﬁnement in Double Heterostructures . . . . . 238 References . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 241 7
8
Electrical Properties of Compound Semiconductor Heterostructures . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 7.1 Abrupt Heterojunction Under Equilibrium . . . . . . . . . . . 7.1.1 Qualitative Analysis of a pN Heterojunction in Equilibrium . . . . . . . . . . . . . . . . . . . . . . . . . 7.1.2 Equilibrium nN Heterojunction . . . . . . . . . . . . 7.2 pN Heterojunction Under Bias . . . . . . . . . . . . . . . . . . . 7.2.1 Potential Distribution Proﬁle . . . . . . . . . . . . . . . 7.2.2 Carrier Injection Across the pN Heterojunction . 7.3 QuantumWell Heterostructures . . . . . . . . . . . . . . . . . . . 7.3.1 Inﬁnitely Deep Square Potential Well . . . . . . . . 7.3.2 Realistic QW with Finite Depth Barriers . . . . . . 7.3.3 Hole Energy Levels in the QW . . . . . . . . . . . . . 7.3.4 Strained Quantum Wells . . . . . . . . . . . . . . . . . . 7.3.5 Inﬁnite Deep Triangular Quantum Well . . . . . . . 7.4 Superlattices and Minibands . . . . . . . . . . . . . . . . . . . . . 7.4.1 Square Barrier . . . . . . . . . . . . . . . . . . . . . . . . . 7.4.2 Resonant Tunneling Through Double Barriers . . 7.4.3 Superlattice and Miniband . . . . . . . . . . . . . . . . 7.4.4 Density of States in Superlattice . . . . . . . . . . . . 7.5 Heterostructures in Electric Fields . . . . . . . . . . . . . . . . . 7.5.1 Uniform Electric Field on a Bulk Semiconductor—Franz–Keldysh Effect . . . . . . . 7.5.2 Quantum Well in an Electric Field—QuantumConﬁned Stark Effect (QCSE) . . . . . . . . . . . . . . 7.6 Polarization Fields in Wurtzite Heterostructures . . . . . . . References . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . .
. . . . . 243 . . . . . 243 . . . . . . . . . . . . . . . . .
. . . . . . . . . . . . . . . . .
. . . . . . . . . . . . . . . . .
. . . . . . . . . . . . . . . . .
. . . . . . . . . . . . . . . . .
243 248 251 251 252 256 256 261 264 265 266 270 270 272 274 275 277
. . . . . 277 . . . . . 279 . . . . . 280 . . . . . 287
Optical Properties of Compound Semiconductor Heterostructures . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 8.1 Basic Optical Properties of Dielectric Medium . . . . . . . . . . . 8.1.1 Maxwell’s Equations . . . . . . . . . . . . . . . . . . . . . . . 8.1.2 Electrical and Optical Constants in a Lossless (r = 0) Dielectric . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 8.1.3 Electrical and Optical Constants in a Lossy (r 6¼ 0) Medium . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 8.1.4 Dielectric Constant . . . . . . . . . . . . . . . . . . . . . . . . . 8.2 Absorptions in Semiconductors . . . . . . . . . . . . . . . . . . . . . . 8.2.1 Allowed Direct Transition Between Bands . . . . . . . . 8.2.2 Indirect (Nonvertical) Transitions Between Indirect Valleys . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 8.2.3 Transitions in Highly Doped Semiconductors . . . . . .
. . 289 . . 289 . . 289 . . 290 . . . .
. . . .
292 294 298 300
. . 303 . . 305
Contents
8.2.4 Exciton Absorption . . . . . . . . . . . . . . . . . . . . . . . 8.2.5 Absorption Due to Isoelectronic Traps . . . . . . . . . . 8.3 Radiative Transition Between Discrete States . . . . . . . . . . . 8.3.1 Photon Density Distributions . . . . . . . . . . . . . . . . . 8.3.2 Einstein’s A and B Coefﬁcients . . . . . . . . . . . . . . . 8.3.3 Absorption and Stimulated Emission . . . . . . . . . . . 8.4 Optical Transitions Between Energy Bands . . . . . . . . . . . . 8.4.1 Direct and Indirect Bandgaps . . . . . . . . . . . . . . . . 8.4.2 BandtoBand Transitions in Bulk Semiconductors . 8.4.3 Fermi–Dirac Inversion Factor, Transparency, and Gain . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 8.4.4 Optical Absorption and Gain in Quantum Wells . . 8.5 Nonradiative Auger Recombination Processes . . . . . . . . . . References . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 9
Heterostructure Electronic Devices . . . . . . . . . . . . . . . . . . . . . . 9.1 Metal–Semiconductor FieldEffect Transistors (MESFETs) . 9.1.1 Basic Operation Principles . . . . . . . . . . . . . . . . . . 9.1.2 Current–Voltage Characteristics . . . . . . . . . . . . . . . 9.1.3 Transconductance and Equivalent Circuit of MESFET . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 9.1.4 HighSpeed Figure of Merit . . . . . . . . . . . . . . . . . 9.1.5 MESFET Fabrication and Performance . . . . . . . . . 9.2 Modulation Doping and TwoDimensional Electron Gas (2DEG) . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 9.2.1 ModulationDoped (MD) Heterostructures . . . . . . . 9.2.2 Scattering Mechanisms in MD Heterostructures . . . 9.3 HighElectronMobility Transistor Basics—A Triangular Quantum Well Approach . . . . . . . . . . . . . . . . . . . . . . . . . . 9.4 Operation Properties of the HEMT . . . . . . . . . . . . . . . . . . 9.4.1 Isolated Heterojunction Under Equilibrium . . . . . . 9.4.2 Charge Control by Gate Bias in HEMT . . . . . . . . . 9.4.3 Current and Voltage Characteristics of HEMT . . . . 9.4.4 Microwave Noise Performance . . . . . . . . . . . . . . . 9.5 Optimal Design of the HEMT . . . . . . . . . . . . . . . . . . . . . . 9.5.1 DX Center in SiDoped AlGaAs/GaAs HEMT and Delta Doping . . . . . . . . . . . . . . . . . . . . . . . . . 9.5.2 Pseudomorphic HighElectronMobility Transistors (pHEMT) . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 9.6 GaNBased HEMT Structures . . . . . . . . . . . . . . . . . . . . . . 9.6.1 PolarizationInduced Sheet Charges at Heterojunctions . . . . . . . . . . . . . . . . . . . . . . . . 9.6.2 Sheet Carrier Concentration of 2DEG . . . . . . . . . .
xiii
. . . . . . . . .
. . . . . . . . .
. . . . . . . . .
309 312 315 315 317 319 324 324 325
. . . .
. . . .
. . . .
326 330 332 336
. . . .
. . . .
. . . .
339 340 340 343
. . . 346 . . . 348 . . . 349 . . . 351 . . . 352 . . . 354 . . . . . . .
. . . . . . .
. . . . . . .
358 362 362 365 369 370 371
. . . 372 . . . 375 . . . 375 . . . 376 . . . 378
xiv
Contents
9.7
Heterojunction Bipolar Transistors (HBTs) . . . . . . . . . . . . . 9.7.1 Introduction . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 9.7.2 Basic Theory of Heterojunction Bipolar Transistors 9.7.3 Band Discontinuity of Heterostructures . . . . . . . . . 9.7.4 HighFrequency Operation of HBT . . . . . . . . . . . . 9.7.5 Basics of HBT Processing . . . . . . . . . . . . . . . . . . 9.8 III–V MetalOxideSemiconductor FieldEffect Transistors . 9.8.1 III–V Alloy Surfaces and SemiconductorOxideMetal Interfaces . . . . . . . . . . . . . . . . . . . . . 9.8.2 Atomic Layer Deposition (ALD) . . . . . . . . . . . . . . 9.8.3 Oxides Deposition on III–V Substrates . . . . . . . . . 9.8.4 Highj Dielectric/III–V MOSFET Development . . . References . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . .
10 Heterostructure Photonic Devices . . . . . . . . . . . . . . . . . . . . . . 10.1 Device Physics of Heterostructure Lasers . . . . . . . . . . . . . 10.1.1 Basic Diode Laser Structure . . . . . . . . . . . . . . . . 10.1.2 WaveGuiding and Conﬁnement Factor . . . . . . . . 10.1.3 Threshold Condition in Fabry–Perot Cavity . . . . . 10.1.4 Threshold Current Density and Photon Density . . 10.1.5 Laser Output Power and Efﬁciency . . . . . . . . . . . 10.1.6 Characteristic Temperature . . . . . . . . . . . . . . . . . 10.2 Structures and Properties of Injection Lasers . . . . . . . . . . 10.2.1 StripeGeometry Lasers . . . . . . . . . . . . . . . . . . . 10.2.2 DistributedFeedback Laser . . . . . . . . . . . . . . . . . 10.3 Laser with QuantumConﬁned Active Region . . . . . . . . . . 10.3.1 QuantumWell Laser . . . . . . . . . . . . . . . . . . . . . 10.3.2 TypeII QuantumWell WType Lasers . . . . . . . . 10.3.3 Quantum Dot and Quantum Wire Lasers . . . . . . . 10.4 VerticalCavity SurfaceEmitting Lasers . . . . . . . . . . . . . . 10.4.1 Threshold Current Density . . . . . . . . . . . . . . . . . 10.4.2 Distributed Bragg Reﬂector Mirrors . . . . . . . . . . . 10.4.3 Resonant Periodic Gain in VCSELs . . . . . . . . . . 10.4.4 Current and Optical Conﬁnements in VCSELs . . . 10.4.5 Characteristics of VCSELs . . . . . . . . . . . . . . . . . 10.5 LightEmitting Diodes . . . . . . . . . . . . . . . . . . . . . . . . . . . 10.5.1 Efﬁciency of LEDs . . . . . . . . . . . . . . . . . . . . . . . 10.5.2 Materials and Technology Evolution . . . . . . . . . . 10.6 Quantum Cascade (QC) Lasers . . . . . . . . . . . . . . . . . . . . 10.6.1 QC Laser Active Region Designs . . . . . . . . . . . . 10.6.2 Threshold Current and Waveguide Designs . . . . . 10.6.3 Quantum Cascade Laser Operation Characteristics 10.6.4 Interband Cascade Lasers—TypeII QC Laser . . .
. . . . . . . . . . . . . . . . . . . . . . . . . . . . .
. . . . . . .
. . . . . . .
. . . . . . .
382 382 383 387 389 397 399
. . . . .
. . . . .
. . . . .
400 404 408 412 416
. . . . . . . . . . . . . . . . . . . . . . . . . . . . .
. . . . . . . . . . . . . . . . . . . . . . . . . . . . .
. . . . . . . . . . . . . . . . . . . . . . . . . . . . .
419 419 419 421 423 427 431 432 433 434 440 444 444 448 449 458 458 460 461 463 464 466 467 469 472 474 477 481 484
Contents
10.7 QuantumWell Infrared Photodetectors (QWIPs) . . . . . . . 10.7.1 Operation Principles of QWIPs . . . . . . . . . . . . . 10.7.2 Dark Current . . . . . . . . . . . . . . . . . . . . . . . . . . 10.7.3 Photoconductive Gain . . . . . . . . . . . . . . . . . . . . 10.7.4 Detectivity . . . . . . . . . . . . . . . . . . . . . . . . . . . . 10.7.5 Experimental Results . . . . . . . . . . . . . . . . . . . . 10.8 Transistor Lasers . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 10.8.1 Basic Device Structure and Operation Principles 10.8.2 Effective Minority Carrier Lifetime in Transistor Lasers . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 10.8.3 Voltage Modulation of a Transistor Laser . . . . . 10.8.4 Excited State Operation of a Transistor Laser . . 10.8.5 LightEmitting Diodes with Tilted BaseCharge Distribution . . . . . . . . . . . . . . . . . . . . . . . . . . . References . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . .
xv
. . . . . . . .
. . . . . . . .
. . . . . . . .
. . . . . . . .
. . . . . . . .
486 486 488 490 492 493 497 497
. . . . . 500 . . . . . 503 . . . . . 506 . . . . . 508 . . . . . 512
Appendix A: Values of Important Physical Constants . . . . . . . . . . . . . . . 515 Appendix B: Important Physical Properties of Some Indirect Semiconductors . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 517 Appendix C: Important Physical Properties of Direct III–V Binary Semiconductors . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 519 Appendix D: Important Physical Properties of Wurtzite III–Nitride Semiconductors . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 521 Appendix E: Bandgap Energy of III–V Semiconductor Ternary Alloys . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 523 Appendix F: Bandgap and Polarization Parameters of Wurtzite IIINitride Semiconductor Ternary Alloys . . . . . . . . . . . . . 525 Index . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 527
Chapter 1
Introduction
Abstract Nowadays, people of the world take their vast benefits for granted—in mobile smartphones, laptop and tablet computers, smart watches, ATMs, electrical vehicles, and numerous other electronic devices. The core technology centered in all these device applications is the microchip, which consists of billions of transistors. The transistor was presciently called the ‘nerve cell’ of the Information Age by William Shockley. December 16, 1947, marks the beginning of the Information Age when John Bardeen and Walter Brattain invented the transistor at Bell Laboratories. It can be said that the transistor is the most important artifact of the twentieth century which deeply affects human civilization. In this chapter, the evolution of the transistor after Bardeen and Brattain’s work from discrete device to verylargescale integrated circuits, from elemental Ge, Si, to IIIV compound semiconductors, and from transport device to photonic device applications is concisely discussed. The necessity of using IIIV compound semiconductors for highspeed and highpower optoelectronic devices is also examined.
1.1 Historical Perspective 1.1.1 Rise of the Semiconductor Industry On December 23, 1947, John Bardeen and Walter Brattain demonstrated the first transistor they invented at Bell Telephone Laboratories (BTL), Murray Hill, New Jersey (Fig. 1.1). The p–n–p point contact transistor was made on an ntype germanium semiconductor. Inspired by this invention, William Shockley conceived the bipolar junction transistor design in early 1948 by replacing twopoint contacts of the transistor with p–n junctions. Due to the increased device structure complexity, until late 1950, a working junction transistor was finally made from a germanium crystal grown by the doubledoped Czochralski method. To improve the device performance, other fabrication techniques such as alloying and diffusion were pursued. In late 1954 the first germanium transistor fabricated using diffusion was made with performance superior to that of the best commercially available transistors of the time. But the
© Springer Nature Switzerland AG 2020 K. Y. Cheng, III–V Compound Semiconductors and Devices, Graduate Texts in Physics, https://doi.org/10.1007/9783030519032_1
1
2
1 Introduction
Fig. 1.1 This publicity photo accurately depicts the working relationship that led to the invention of the transistor at BTL: Brattain handles the apparatus, Bardeen enters data, and Shockley looks on. Courtesy AIP Emilio Segrè Visual Archives, Brattain Collection
germanium transistor has serious drawbacks such as leaky reverse currents and poor hightemperature characteristics. So, the crucial question at the time was whether to continue improving germaniumbased transistors or concentrate on a different semiconductor material—silicon. Silicon has much larger bandgap energy than germanium (1.124 vs. 0.664 eV), which means ordersofmagnitude smaller reverse leakage currents than germanium at normal operating temperatures. Therefore, John Moll, who led a group to develop p–n–p–n switches at BTL, insisted on using silicon instead of germanium. Since there are three p–n junctions in the switch structure, the innermost junction could not be easily formed using grownjunction or alloying techniques. Diffusion was the only real alternative. However, the high melting temperature of silicon made processing silicon at extremely high temperature a daunting problem. To solve the hightemperature diffusion problem, Moll’s group collaborated with Carl Frosch from the BTL chemistry department. In early 1955, during a diffusion experiment, Frosch accidentally ignited hydrogen gas and introduced water vapor into the diffusion chamber, causing the growth of a silicon dioxide film on the silicon surface. The oxide formed a smooth, hard, protective layer that kept the silicon from degrading at high processing temperatures. Soon, transistor development within the Bell System, and later in the rest of the industry, would focus on silicon as the material and diffusion as the processing technology.
1.1 Historical Perspective
3
Although most of the early semiconductor technology advances took place within the Bell System, the integrated circuits concept was developed simultaneously in Texas and California. In 1958, Jack Kilby of Texas Instruments and Robert Noyce of Fairchild Semiconductor independently came up with the idea of integrating active and passive device components on a single slice of semiconductor material. Kilby concentrated on how to make a circuit that connected discrete silicon or germanium components using wires and solder. With the advent of diffusion and photolithography technologies developed at Bell Telephone Laboratories and Shockley Semiconductor Laboratory, Noyce focused on making electrical connections to all necessary p–n junctions and resistors on the same silicon wafer underneath a protective layer of silicon dioxide using the planar processing technique. This basic integrated circuit (IC) structure resembles today’s most advanced verylargescale integrated circuits. In the same year, a group led by M. M. Atalla at BTL found that by carefully cleaning the surface and applying a very pure oxide layer, it could drastically reduce the surface states at the silicon–oxide interface. With the surface states under control, Atalla and Dawon Kahng demonstrated the first metaloxidesilicon fieldeffect transistor (MOSFET) in 1960—the kind of device that has come to dominate integrated circuits and microchips. Through technology diffusion, new product development, and market expansion, the silicon semiconductor industry revenue rapidly reached $1.0 billion in 1961. But it took the industry another two decades to achieve revenue of $10 billion. The situation changed by the early 1980s. The advancements in integration technologies allowed Intel, founded by Noyce and Gordon Moore in 1968, to produce microprocessors in earlytomid 1970s using the MOS process. The microprocessor is a CPU on a chip and could be used in a wide range of applications. For example, the Atari 8800 introduced in 1975 for hobbyists, using the Intel 8080 microprocessor, was essentially a rudimentary computer. Soon, many companies, including Apple and Microsoft, transformed the hobbyists’ toy into a personal computer (PC) with more capabilities that was easier to use. Eventually, the PC became the worldwide driver for the semiconductor industry and the rapidly expanding information technology (IT) industry. The semiconductor industry revenue achieved $100 billion in 1993. In 1969, the US Defense Department’s Advanced Research Projects Agency (ARPA) initiated an experimental network project—ARPANET—to link computers at scientific laboratories across the country so that researchers might share computer resources. Additionally, it might be possible to connect computers in a network redundantly, so that if one line went down, a message could take another path. The network started out with four sites near the west coast. The ARPANET sites eventually extended to nineteen universities and research institutes from coast to coast. In 1989, the ARPANET was terminated, replaced by a network established by the National Science Foundation (NSF)—NSFNET. By that time anyone on a college campus with a connection to the campus network could become an Internet user. In 1990, the creation of the World Wide Web, a multimedia branch of the Internet, by researchers at CERN, the European Laboratory for Particle Physics near Geneva, Switzerland, made the Internet easier to navigate. At the same time, PC popularity surged, further promoting Internet use. The steep increase in Internet use helped further expansion
4
1 Introduction
of the siliconbased semiconductor industry. Meanwhile, to handle the vast information traffic, highspeed and widebandwidth networks are needed, which produces high demand for compound semiconductorbased highspeed electronic and photonic devices.
1.1.2 Development of III–V Compound Semiconductor Industry Since the invention of integrated circuits, the semiconductor industry has been dominated by silicon due to several favorable key attributes including the formation of excellent dielectric layer of silicon dioxide, the high thermal conductivity, and the use of lowpower complementary MOS (CMOS) circuitry that enables the integration of veryhighdensity circuits over large wafers (≥12 ). However, due to the nature of an indirect energy band structure, silicon is not an efficient lightemitting material and its electron mobility is relatively low. The active devices supporting the highspeed networks, therefore, have to rely on III–V compound semiconductors, such as GaAs and InP. These compound semiconductors have several major advantages over their elemental semiconductor counterpart: First, efficient light emission is readily achievable from these direct energy band structure semiconductors. The direct energy gap also leads to the second advantage, high electron mobility and high saturation velocity. The carrier drift velocity in a direct bandgap semiconductor increases linearly with a moderate applied electric field. In indirect bandgap semiconductors, the multiplicity of the conduction band minima increases the electron scattering probability under high fields. Therefore, the drift velocity saturates under high fields. In contrast, the scattering probability of direct bandgap semiconductors is minimized, and a strong velocity overshoot is observed before the velocity saturation occurs. Third, some of the most popular crystals of III–V compounds can be prepared in semiinsulating forms. The use of these semiinsulating substrates can eliminate speeddegrading parasitic capacitance. It also simplifies the electrical isolation of devices. Next, by mixing two or three III–V binary compounds, one can prepare a series of ternary or quaternary compounds with greater freedom in the selection of crystal lattice constant and/or bandgap energy (Fig. 1.2). Finally, the most important attribute of III–V compounds is the creation of new function devices utilizing bandgap engineering in heterostructures, where semiconductor thin films with different energy bandgaps are stacked together forming devices with designed electrical and optical properties (Fig. 1.3). Quantumwell lasers and highelectronmobility transistors are two examples. In 1952, the semiconductor nature of III–V compounds was first reported independently by Heinrich Welker of Siemens, West Germany, and a group at the Ioffe Institute, Russia. Inspired by the demonstration of the first laser, a solidstate ruby laser was developed in May 1960 by Theodore Maiman of the Hughes Research
1.1 Historical Perspective
5
Fig. 1.2 Lattice constant as a function of valley bandgap energy of zincblende structure III–V compound semiconductors at zero temperature. The bandgap energy of ternaries follows the line connecting the constituent binaries. Reprinted with permission from [1], copyright AIP Publishing
Fig. 1.3 a Type I, b staggered type II, and c brokengap type II bandedge alignments in semiconductor heterostructures. The energy band diagrams of flat band, ntype heterostructures, and ptype heterostructures are shown in the left, middle, and right panels, respectively
6
1 Introduction
Laboratory, and three groups (GE, IBM, and MIT Lincoln Laboratory) independently demonstrated GaAs homojunction injection lasers in 1962 using diffused p–n junction structures. The first ternary alloy (GaAsP) laser emitting in the visible spectrum (710 nm) was also reported at about the same time by Nick Holonyak Jr. at GE. The next year, J. G. Gunn discovered microwave oscillation due to the transferred electron effect in direct bandgap III–V compounds. These important early inventions precisely highlight the strength of III–V semiconductor alloys over silicon—their lightemitting and highspeed properties. Compared to silicon, compound semiconductors are more complex in terms of material preparation. Heterostructure devices are entrenched in the grown layer structures, not formed by postgrowth diffusion processing commonly used in silicon IC fabrication. Thus, further advance of compound semiconductor technologies relies on the successful development of heteroepitaxial growth technologies. For example, independently suggested by Herb Kroemer and Zhores Alferov in 1963, the incorporation of the doubleheterojunction (DH) structure can improve the device efficiency of injection lasers. At the time, the threshold current density of GaAs injection lasers was nearly 105 A/cm2 , which is too high even for roomtemperature pulse operation. However, roomtemperature cw DH laser operation was finally demonstrated in 1970 after the successful demonstration of the liquid phase epitaxy (LPE) technique to grow AlGaAs on GaAs in 1967. To improve the uniformity and growth rate control of LPEgrown layers, two major epitaxy techniques have been developed. Alfred Cho of Bell Laboratories pioneered the molecular beam epitaxy (MBE) technique and demonstrated MBE growth of AlGaAs and GaP in 1969. At Rockwell International, H. M. Manasevit first reported metalorganic chemical vapor deposition (MOCVD) of compound semiconductors on foreign substrates such as sapphire in 1968. With further developments, both MBE and MOCVD techniques have proved to have the characteristics of producing highquality uniform multiple layered structures with excellent morphology, sharp interface, and precise doping and thickness control. These attributes ultimately formed the basis for successful growth of innovative bandgapengineered devices with neverbeforerealized electrical and optical properties. In 1975, the quantumwell laser operation was demonstrated using MBEgrown AlGaAs/GaAs multilayer structures, where the quantum size effect occurred in very thin GaAs layers. The phrase quantumwell laser was first used in 1978 by Holonyak et al. to describe their MOCVDgrown laser structures. One additional advantage of these ultrathinlayer structures is that highquality strained layers can be achieved to further modify the energy band structure and enhance the laser performance. The ability to precisely make quantum wells has had a farreaching impact, ranging from classroom physics to revolutions in electronic and optical devices for the consumer electronics, computers, and communications industries. Today, the global communication network relies on highspeed laser diodes and sensitive photodiodes to transmit and receive extremely high capacity information optically over hundreds of kilometers in lowloss optical fibers. Highelectronmobility transistors (HEMTs) are utilized as highspeed circuit components and in highfrequency,
1.1 Historical Perspective
7
lownoise, direct broadcast satellite and wireless communications. The heterojunction bipolar transistor (HBT) is the key component to enabling the efficient performance and small size of cellular phones. Further development of these highspeed electronic devices will likely hasten the implementation of ultrawidebandwidth communication systems. Another important development of compound semiconductor technology is the invention of the visible (red) lightemitting diode (LED) in 1962 by Holonyak using GaAsP ternary alloys. The performance (lumens/watt) of (As,P)based LEDs increased 10 × per decade from 1970 to 2000 using GaP:Zn,O and GaP:N materials, and AlGaAs/GaAs and AlGaInP/GaAs heterostructures, progressively. However, the emission color of these LEDs was restricted by the bandgap energy of these alloys to between red and orange. Nevertheless, these LEDs have been used for many applications including instrument panels, displays, vehicle break lights, and traffic signals. In order to expand LED emissions to cover the full visible spectrum, specifically the blue–green band, GaN has been investigated since the early 1970s. However, the lack of suitable ptype dopants prevented it from forming useful p–n junction devices. In 1989, Isamu Akasaki and Hiroshi Amano of Nagoya University in Japan finally made the breakthrough; they obtained ptype conduction in Mgdoped GaN using postgrowth annealing to remove hydrogen passivation and activate acceptors. This key discovery led Shuji Nakamura of Nichia in Japan to demonstrate the first InGaN/GaN blue LED grown by MOCVD. Now the LEDs with three primary colors are realized for making fullcolor displays. More important, white light LEDs for lighting applications are readily attainable using yellowphosphoruscoated blue LEDs. As a general illumination lighting source, white light LED products surpass many conventional lighting technologies (including incandescent and fluorescent light sources) in energy efficiency, lifetime, and versatility and rival them in color and light quality. At the other end of the spectrum, innovative bandgapengineered devices utilizing intersubband transitions in quantum wells, such as quantum cascade (QC) lasers, extend the laser emission wavelength well into the midinfrared (midIR), which is not available from bulk materials. Large area and uniform midIR quantumwell infrared photodetectors (QWIPs) based on the same intersubband transitions were also developed. These midIR devices are critical for future planetary exploration, biomedical, and security applications.
1.2 Future Outlooks Due to limitations in the material properties of silicon, III–V compound semiconductors have dominated photonic and highspeed electronic devices. This trend is likely to continue in the fastgrowing wireless communications and Internet applications. The ability to form heterostructures further enhances the ability of compound semiconductors to form new quantum effect devices and efficient photonic devices.
8
1 Introduction
It is expected that III–V compound semiconductors will continue to thrive in highspeed, widebandwidth, and lowpower consumption devices and circuits. In addition, the realization of the ptype GaN not only led to widespread applications of IIINbased LEDs for solidstate lighting and fullcolor displays but also enabled the development of nextgeneration power electronics using widebandgap semiconductors. The inherent properties of the bulk GaN, including a wide bandgap, higher electron mobility, and excellent thermal conductivity, allow IIIN materialbased power electronic devices to operate efficiently at higher voltages and power densities, higher frequency and temperature than silicon semiconductors, yielding significant energy savings. However, the realization of the full potential of widebandgap semiconductorbased power devices depends on the development of costeffective substrates. On the other hand, miniaturization of the feature size of ICs to increase the density of components has been the foundation of the 50yearlong steady advance of silicon technology. In 1965 Moore wrote an Electronics article based on an analysis of the cost of IC production where he claimed that at any given time there was a component density that led to the lowest cost per component [2]. Moore further proclaimed that the minimum cost point had been moving out in density by a factor of two per year. This statement, commonly referred to as Moore’s law, became the metronome of the industry advancement. The exponential increase of transistor count per unit area as a function of time has been faithfully delivered by the industry since 1970. The minimum transistor gate length also decreases with time exponentially (Fig. 1.4). However, the semiconductor industry faces increasingly difficult challenges in technology as well as cost as it moves into production at feature sizes below 100 nm. To keep up the CMOS performance with scaling, strained SiGe channel material
Fig. 1.4 Feature size versus time in silicon ICs. Major device technology milestones are also listed
1.2 Future Outlooks
9
(90/65 nm node) and highκ gate dielectrics (45/32 nm node), even nonplanar multigate structures (22/16 nm node) of MOSFETs have been incorporated. Although 5nmnode CMOS circuits are on the horizon, further reduction of the feature size to below 2 nm will push the device structure into the quantum regime. At that moment, the silicon technology will reach the point at which significant materials and device innovations will be required to sustain further development. One possible situation for the future is the hybrid material system where silicon, germanium, and III–V compound semiconductors are integrated together on silicon wafers. For example, taking advantage of the very high electron mobility in GaInAs and high hole mobility in germanium, advanced CMOS circuits consisting of nGaInAs channel and pGe channel MOSFETs might be fabricated together on the silicon wafer. One may also imagine the incorporation of optical interconnects within a silicon wafer using integrated compound semiconductor lasers and Si/SiO2 waveguides to improve the speed of the circuits. Thus, the distinction between silicon and compound semiconductors in terms of their roles in device applications may become less well defined.
References 1. I. Vurgaftman, J.R. Meyer, L.R. RamMohan, J. Appl. Phys. 89, 5815 (2001) 2. G. E. Moore, Electronics 19, 114–117 (1965, April); and Proc. IEEE 86, 82 (1998)
Further Reading 1. M. Riordan, L. Hoddeson, Crystal fire (W. W. Norton & Co., New York, 1997) 2. R.K. Bassett, To the Digital Age (John Hopkins University Press, Baltimore, 2002) 3. J. Orton, The Story of Semiconductors (Oxford University Press, 2004)
Chapter 2
Atomic Bonding and Crystal Structures
Abstract On December 23, 1947, John Bardeen and Walter Brattain demonstrated the world’s first transistor at Bell Telephone Laboratories. The pointcontact transistor was made in the area of a large singlecrystalline grain on a piece of reused polycrystalline germanium. Above the Ge slab was a polystyrene wedge structure where, at the bottom tip of the wedge, the goldfoil emitter and collector electrodes make point contacts, separated by ~50 µm, to the ntype Ge base. In this device, the injection of both electrons and holes into a semiconductor was first demonstrated. Shortly after that, the zone refining process was developed by William Pfann for the growth of silicon and germanium crystals of predetermined purity. Today, transistors, lightemitting diodes, injection lasers, integrated circuits, and many other semiconductor devices are made from single crystals of semiconductor material with extremely high purity. There are other semiconductor devices which are not made from singlecrystal material, though they could be and their operation is usually obtained as if they were. Hence, a study of the basic properties of crystal structures is necessary for a meaningful explanation of the operation of semiconductor devices. In this chapter, the tetrahedron bond structure—the basic building block of major semiconductor crystals—is first derived from atomic sp3 orbitals. The reciprocal lattice is then introduced as an alternative but powerful approach to investigate the lattice structure of the crystal. For example, crystal diffraction results are best discussed in the reciprocal lattice space. Finally, the Brillouin zone concept is introduced.
© Springer Nature Switzerland AG 2020 K. Y. Cheng, III–V Compound Semiconductors and Devices, Graduate Texts in Physics, https://doi.org/10.1007/9783030519032_2
11
12
2 Atomic Bonding and Crystal Structures
Fig. 2.1 Schematic of the pointcontact bipolar transistor invented by Bardeen and Brattain of Bell Telephone Laboratories in 1947. The polystyrene wedge covered with gold foil on two sides was held against the Ge with a spring to form emitter and collector contacts. The ntype Ge slab forms the base of the transistor. Minority carrier (hole) injection was demonstrated for the first time
2.1 Crystal Structures and Symmetry 2.1.1 Crystal Structures The solids of primary interest for us are semiconductors that have all their atoms arranged in a regular pattern in three dimensions (3D). Such solids are called single crystals, and the arrangement of atoms is termed the crystal structure. The basic 3D building blocks that pack together to fill all the space of the crystal are called the unit cells. A unit cell can be seen as a parallelepiped defined by three lengths a, b, and c and three angles α, β, and γ as shown in Fig. 2.2. By changing the lengths and angles of the parallelepiped, while making sure to fill all the space, a number of crystal structures can be built. Depending on the specifications about the lengths Fig. 2.2 Definition of axes, dimensions and angles for a general unit cell
2.1 Crystal Structures and Symmetry
13
Table 2.1 Seven crystal classes and related Bravais lattices System
Unit cell
Bravais lattice
Cubic
a = b = c, α = β = γ = 90°
P (primitive), I (bodycentered), F (facecentered)
Hexagonal
a = b = c, α = β = 90°, γ = 120°
P (rhombohedral)
Tetragonal
a = b = c, α = β = γ = 90°
P, I P, I, F, C (basecentered)
Orthorhombic
a = b = c, α = β = γ = 90°
Monoclinic
a = b = c, α = β = 90° = γ
P, C
Trigonal
a = b = c, 120° > α = β = γ = 90°
P (rhombohedral)
Triclinic
a = b = c, α = β = γ
P
and the angles, these crystal structures are classified into seven systems as listed in Table 2.1. Some structures can be derived from other crystal structures. For example, under a uniaxial stress, such as in a strained quantum well, a cubic crystal can be transformed into an orthorhombic structure. Additionally, these basic structures are further modified by four different 3D unit cells: (a) The primitive unit cell (symbol P) has a lattice point at each corner and forms a minimum volume. (b) The bodycentered unit cell (symbol I) has a lattice point at each corner and one at the center of the cell. (c) The facecentered unit cell (symbol F) has a lattice point at each corner and one at the center of each face. (d) The basecentered unit cell (symbol A, B, or C) has a lattice point at each corner and one pair of opposite faces; e.g., a Ccentered cell has lattice points in the centers of the ab faces. When combing these four types of lattice with seven possible unit cell forms, 14 Bravais lattices are produced. For example, the simple cubic is the primitive unit cell of the cubic system while the bodycentered cubic and facecentered cubic correspond to the modified (I and F, respectively) cubic unit cells (Fig. 2.3). It is important to note that the lattice point represents equivalent positions in a crystal structure and not atoms. A lattice point could be occupied either by an atom, a complex ion, a single molecule, or a group of molecules.
Fig. 2.3 Four basic 3D Bravais lattices most relevant to semiconductor crystals. The facecentered cubic and hexagonal crystal structures are particularly important in semiconductor physics
14
2 Atomic Bonding and Crystal Structures
2.1.2 Crystallographic Notation—Miller Indices In semiconductor technologies, we often make devices and circuits on a particular crystallographic plane or a particular direction of semiconductor crystals. This particular crystal plane is usually described by its Miller indices, which are established as follows. Consider a 3D lattice, a portion of which is shown in Fig. 2.4, where A, B, C, and O are lattice points; a, b, and c are translational unit vectors; and n1 , n2 , and n3 are the proper integers. Thus the plane ABC can be defined by vectors OA (=n1 a), OB (=n2 b), and OC (=n3 c). For reasons that will become clear when the properties of reciprocal lattices are explored in Sect. 2.5, we shall find it useful to refer to the ABC plane as the (hkl) plane, where hkl is a set of integers which expresses the ratio h: k: l=
1 1 1 : : n1 n2 n3
(2.1)
Thus the plane ABC has the Miller indices of (hkl) which are a set of the smallest integers that satisfy (2.1). For example, for the plane whose intercepts are 2, 1, 3, the reciprocals are 1/2, 1, and 1/3; the smallest three integers having the same ratio are (362). If a plane cuts an axis (say, the aaxis) on the negative side of the origin, the corresponding index is negative, indicated by placing a bar (minus sign) above the ¯ index as (hkl). For an intercept at infinity, the corresponding index is zero. Figure 2.5 illustrates the Miller indices of some important plans in a cubic crystal. The indices (h00) may denote a plane parallel to both b and caxes, e.g., the (100) plane, and the indices (hk0) represent a plane parallel to the caxis. The normal to the plane with indices (hkl) is the direction [hkl]. In a cubic crystal there are six cubic faces: (100), ¯ ¯ and (001). ¯ This set of equivalent planes of a cubic crystal (010), (001), (110), (010), may be denoted as a group by {100}. The family of plane directions in the cubic crystal may be expressed as 100. For hexagonal crystal structures, there are four coordinates, namely the a1 , a2 , a3 , and c axes as shown in Fig. 2.6. The angle between adjacent ai ’s is 120°. Therefore, it is common to use a set of four Miller indices, expressed in terms of the reciprocal intercepts with respect to the vectors a1 , a2 , a3 , and c as (hkjl). However, it can be Fig. 2.4 Description of the construction of Miller indices for the plane passing through the lattice points A, B, and C. a, b, and c are unit vectors and n1 , n2 , and n3 are integers
c C n 3c O n1a A a
n2b
B
b
2.1 Crystal Structures and Symmetry
15
Fig. 2.5 Miller indices of some important planes in a cubic crystal
Fig. 2.6 Four unit vectors used to formulate Miller indices for a hexagonal crystal
a2

c
(1100) a1
a3
proved that the sum of h, k, and j of a plane is always zero. Thus the added index j serves as a check and does not provide any new information. For example, the shaded surface shown in Fig. 2.6 cuts a1 and a2 at 1 and −1, respectively, and is parallel to ¯ according to a3 and c. Thus this plane may be designated as 1100 h: k: j: l =
1 1 1 1 : : : = 1 : −1 : 0 : 0 1 −1 ∞ ∞
where h + k + j = 1 − 1 + 0 = 0. The Miller indices of the base of the hexagonal crystal, or the basal plane, are (0001).
16
2 Atomic Bonding and Crystal Structures
2.1.3 Lattice Symmetries As discussed earlier, a singlecrystal solid has all its atoms arranged in a regular pattern in three dimensions. The unit cells or building blocks of the crystal are shaped as 14 basic parallelepipeds of Bravais lattices. Any two locations in the crystal having identical atomic environment can be achieved through a simple translation action on the unit cells following T = n1 a + n2 b + n3 c
(2.2)
where T is the translation vector; a, b, and c are the unit vectors; and n1 , n2 , and n3 are integers. In addition, lattice points can be recurred into themselves by other operations including (a) reflection at a plane, (b) inversion through a point, (c) rotation about an axis, and (d) rotationinversion about an axis. Using simple cubic structure as an example, these operations are illustrated in Fig. 2.7. Through the operation of reflection at a mirror plane, the x–y plane in Fig. 2.7a, point P may transform to point Q. This symmetry is expressed mathematically by a coordinate transformation x = x, y = y, and z = –z. The tensor representation of the mirror reflection operation in the x–y plane is expressed as ⎡
⎤⎡ ⎤ ⎡ ⎤ 10 0 x x ⎣ 0 1 0 ⎦⎣ y ⎦ = ⎣ y ⎦ 0 0 −1 z −z
(2.3)
The presence of a mirror plane in a crystal is represented by the symbol m. The inversion symmetry operation (Fig. 2.7b) may be described by the coordinate transformation x = –x, y = –y, and z = –z. It may also be expressed by the transformation of the position vector r = –r at the inversion point. The symbol of the inversion symmetry is I¯. The other symmetry operation is the rotation about an axis. The axis of rotation is named an nfold axis if the angle φ of rotation to carry a unit cell into itself is equal to φ = 2π /n. In this example, Fig. 2.7c, a 90° rotation about the axis will bring point P to point Q or a fourfold symmetry. All possible rotation operations
z
(a)
(b) P
P
Q
Q
P
P
r
y
x
(d)
(c)
r
Q Q
S R
Fig. 2.7 Symmetry operations in a cubic crystal. a Reflection at a plane, b inversion through a point, c rotation about an axis, and d rotationreflection about an axis
2.1 Crystal Structures and Symmetry
17
are one, two, three, four, and sixfold symmetry, which correspond to rotations by 2π, π, 2π /3, π /2, and π /3 radians. These are the only five allowed rotation symmetry operations since they are consistent with a crystal’s requirements for translational symmetry. The symmetry operations may be combined with one another in various ways. For example, there is a rotationreflection compound operation to carry the lattice into itself. As shown in Fig. 2.7d, a 90° (fourfold) rotation about an axis parallel to the zaxis through the center of the cube combining with a mirror reflection at the x–y plane will bring points P and Q to S and R, respectively. This combined operation is represented by the symbol n¯ for the nfold rotation symmetry. Conversely, every crystal may be described by a particular combination of symmetry elements that strongly influence its material properties. More specifically, this combination determines the nature of independent components of the tensors describing macroscopic material properties. To illustrate this correlation, we examine the dielectric constant of the material using the symmetry concept and tensor representation. By definition, D = E or ⎤ ⎡ ⎤⎡ ⎤ 11 12 13 Ex Dx ⎣ D y ⎦ = ⎣ 21 22 23 ⎦⎣ E y ⎦ Dz 31 32 33 Ez ⎡
(2.4)
For a cubic crystal, there are four threefold (along diagonals as shown in Fig. 2.8) and three fourfold (along three major axes) rotation axes. When rotating along [111] for 120°, it brings, for example, x → y, y → z and z → x. In tensor form, it is ⎤ ⎡ ⎤⎡ ⎤ 11 12 13 Ey Dy ⎣ Dz ⎦ = ⎣ 21 22 23 ⎦⎣ E z ⎦ Dx 31 32 33 Ex ⎡
¯ Fig. 2.8 Rotation symmetry operations along a [111] and b [111] axes of a cubic crystal
(2.5)
18
2 Atomic Bonding and Crystal Structures
Equations (2.4) and (2.5) are essentially the same and their components can be compared. By examining Di in both equations, we can deduce the relations of some tensor components Dx = 11 E x + 12 E y + 13 E z = 31 E y + 32 E z + 33 E x
(2.6a)
D y = 21 E x + 22 E y + 23 E z = 11 E y + 12 E z + 13 E x
(2.6b)
and
By comparison, we have 11 = 22 = 33 , 13 = 21 = 32 , and 12 = 31 = 23 . The threefold rotation symmetry exists along the other rotation axes. A rotation of ¯ 120° about [111] will bring x → −y, y → z, z → −x (Fig. 2.8b), or ⎤ ⎡ ⎤⎡ ⎤ 11 12 13 −E y −D y ⎣ Dz ⎦ = ⎣ 21 22 23 ⎦⎣ E z ⎦ −Dx 31 32 33 −E x ⎡
(2.7)
Comparing (2.4), (2.5), and (2.7), we find 12 = −23 = 31 and 13 = 21 = −32 . In order to fulfill both these results obtained from the two different rotation axes, we conclude that i j = 0 for i = j and 11 = 22 = 33 . Thus, ⎤ 11 0 0 = ⎣ 0 11 0 ⎦ 0 0 11 ⎡
(2.8)
Therefore, the simple cubic crystal has an isotropic dielectric constant . Using a similar approach, we can calculate the dielectric constant tensors in other crystals. For hexagonal crystals, the dielectric constant tensor has the form 11 0 0 = 0 11 0 0 0 33
(2.9)
if the zaxis is chosen to be the axis of sixfold symmetry and the x and yaxes are the two perpendicular axes in the basal plane. Thus, the symmetry considerations help us find the relations that may exist between the matrix elements in a material parameter tensor such as the dielectric constant tensor. Therefore, we can expect the less symmetric zincblende crystal structure of GaAs to have an anisotropic dielectric constant and nonlinear optical properties.
2.2 Ionic Bond and Interatomic Forces
19
2.2 Ionic Bond and Interatomic Forces Ionic crystals are generally transparent insulators of inorganic compounds. The crystal structures of some ionic crystals are simple, such as NaCl and CsCl, while others are extremely complex. For the purpose of studying the properties of ionic bonding, we consider the simple compound NaCl. Sodium (Na), an alkali metal, has a single 3s valence electron outside the closed shell, whereas chlorine (Cl), a halogen, is one electron short of having a complete outer 3p shell. As shown in Fig. 2.9, an electron transfer from the alkali metal to the halogen results in closedshell configurations in both Na+ and Cl− ions. During this electron transfer process, there are four major energy exchanges involved in forming the ionic bond. First, the energy given up when a neutral (Cl) atom gains an electron and becomes a negative ion (anion) is called the electron affinity. It increases the energy of the system and has a positive value. Second, the energy necessary to remove an electron from the (Na) atom creating a positive ion (cation) is simply the ionization energy—a negative energy value. Third, the Coulomb force between Na+ and Cl− ions keeps these ions together in a Na+ Cl− ionic crystal, and a lowering of potential energy occurs. Therefore, the Coulomb attraction force has a positive energy value. Finally, when the electron shells of the neighboring ion cores start to overlap, a repulsive force must be considered. The repulsive energy is a result of the Pauli exclusion principle for a closed ion shell. Energy is required to prevent the collapse of the lattice and is considered a negative term. The balance of competing requirements for attractive and repulsive components of the electrostatic interaction warrants that highly symmetric crystal structures ensue with maximized volumes. Figure 2.10 shows two of the simplest ionic crystal structures of all—the rock salt structure of NaCl and the cesium chloride (CsCl) structure. The NaCl structure can be viewed as an FCC crystal with a basis containing one Na+ ion at (0, 0, 0) and one Cl− ion at (1/2, 1/2, 1/2). The other way of constructing the NaCl structure is to position alternatively with Na+ or Cl− ions at the lattice sites of a simple cubic crystal. Each ion is surrounded by six nearestneighbor ions of the opposite type in 100 directions. The CsCl structure is based on the simple cubic crystal structure with a basis containing one Cs+ ion at (0,0,0)
Fig. 2.9 Electron configuration in NaCl. The outer ring represents the shell of n = 3. The dashed arrow indicates the electron transfer from Na to Cl resulting in closed shell configurations in Na and Cl ions. The Coulomb attraction between two ions and repulsive force between cores are also shown
20
2 Atomic Bonding and Crystal Structures
(a)
(b)
Fig. 2.10 Two typical ionic crystal structures: a NaCl and b CsCl. The ionic radii of Na+ , Cs+ , and Cl− are 0.875 Å, 1.455 Å, and 1.475 Å, respectively
and one Cl− ion at (1/2, 1/2, 1/2). The structure looks like BCC but, strictly speaking, is not since different ions occupy the two lattice sites at the body center and corners. There are eight nearestneighbor ions of the opposite type in 111 directions. The total energy required to separate the atoms in the solid into isolated neutral atoms and vice versa is called the cohesive energy or binding energy, E 0 . Since the ionization energy of the positive ion and the electron affinity of the negative ion very nearly cancel each other, the major contribution to the binding energy is the electrostatic energies. We can formulate these relations in the following equation: E T (r ) ∼ = E Coul (r ) + E Rep (r )
(2.10)
where E T is the sum of the Coulomb attraction energy E Coul and the energy of the repulsive force E Rep at a positive ion–negative ion separation distance r. In a NaCl crystal structure, surrounding any Na+ are six neighboring Cl− ions, 12 nextnearestneighboring Na+ ions, and so forth. The Coulomb energy can be calculated as
6 12 q2 q2 6 24 8 − √ + √ − √ + √ − · · · = −1.748 = E Coul = − 4π 0 r 1 4π 0 r 3 4 2 5 q2 (2.11) −α 4π 0 r where α is the Madelung constant which has the values of 1.641, 1.638, and 1.763 for wurtzite, zincblende, and CsCl structures, respectively. The negative sign of E Coul represents the net attractive force between ions. Since the repulsive force decreases rapidly as the distance between ions increases, it has a powerlaw form of E Rep =
A ∝ r −n rn
(2.12)
2.2 Ionic Bond and Interatomic Forces
21
Fig. 2.11 Total potential energy as a function of the separation of two ions. The dotdashed and dashed curves correspond to contributions of repulsive and Coulomb attraction forces, respectively. r 0 is the equilibrium separation of ions
where A and n are constants and E Rep has a positive value. Thus the sum of (2.11) and (2.12) gives the total energy. E T (r ) = −
αq 2 A + n 4π 0 r r
(2.13)
A qualitative expression of E T (r) is plotted in Fig. 2.11. At equilibrium, r = r 0 , αq 2 nA dE T = − n+1 = 0 2 dr 4π 0 r0 r0 where r 0 is the equilibrium interatomic distance of the ionic crystal. Thus, r0n−1 =
4π 0 n A αq 2
(2.14)
The cohesive or binding energy E 0 is obtained from the total energy E T (r) at r = r0.
1 αq 2 1− E 0 = E T (r0 ) = E Coul + E Rep r0 = − 4π 0 r0 n
(2.15)
For stability of the crystal, n must be greater than unity. Of course it should be possible to determine it from an exact quantum mechanical treatment of the problem. However, from a fit to experimental quantities, n has been determined to be in the range 6–10. Therefore, the Coulomb attraction force becomes the major contributor to the cohesive energy. In general, the ionic bond is a nondirectional bond. It forms a close atomic packing to maximize the number of bonds per unit volume and to minimize the bonding energy per unit volume. Due to the size difference between ions, it can form either a simple cubic or FCC structure to avoid anion–anion or cation–cation contact. The condition that determines the crystal structure can be understood by using a ‘hard sphere’ model. Imagine the atoms as small hard spheres. When identical atoms are
22
2 Atomic Bonding and Crystal Structures
assembled in a layer, the most compact arrangement is the closepacked structure in which every sphere has six touching neighbors. This plane array, as shown in Fig. 2.12, has a hexagonal symmetry and is assigned as layer A. To build up a closepacked solid in 3D we must now add a second layer, B. The spheres of the second layer will sit in half of the holes of the first layer as shown in Fig. 2.13. When we come to add the third layer, C, there are two possible positions where it can fit. First, it could be positioned on top of layer B so that its atoms sit in the holes of layer B which were also holes in layer A. A fourth layer identical to layer A can then be added and the ABCABC sequence continued. This is known as cubic close packing and produces a FCC lattice. The stacking layer surfaces simply correspond to the {111} surface of the FCC structure. An alternative form of close packing is to position the third layer C identically to layer A, to fit on top of layer B. When we repeat this sequence, the pattern of ABABAB produces a hexagonal closepacked (HCP) structure. For cations and anions of similar size, the simple cubic structure (CsCl) is preferred to achieve the highest packing density. Otherwise, it will form an FCC structure (NaCl). Due to their large cohesive energies, these alkali halides, which are among the most stable ionic crystals, have large bandgaps. For example, the bandgaps for NaCl and CsCl are 8.5 and 8.4 eV, respectively. Fig. 2.12 Hard spheres arranged in a closepacked layer structure
Fig. 2.13 Two layers of closepacked spheres
2.3 Covalent Bond and sp3 Hybrid Orbit
23
2.3 Covalent Bond and sp3 Hybrid Orbit 2.3.1 General Properties of Covalent Bond Formation Atoms in molecule or solid can ‘share’ their electrons to form a covalent bond. The simplest example is the N2 molecule. The nitrogen atom has an electron configuration of 1s2 2s2 2p3 . The 2p shell needs six valence electrons to fill its outermost orbit. This can be accomplished by sharing six electrons (three from each atom) between two nitrogen atoms (Fig. 2.14). These shared electrons orbit the two nitrogen atoms, spending equal time with each. Therefore they do not specifically belong to a particular nitrogen atom, but are shared by both. These shared electrons ‘bond’ two nitrogen atoms into a nitrogen molecule. We shall discuss the physics of the bond formation in detail next. To illustrate the relation of electron distribution behavior and bonding formation, we use the H2 + ion as an example, in which the two protons are held together by one electron. For an isolated hydrogen atom, the wave function has a spherical symmetric form of 1 exp(−r/a0 ) ψ(1s) = πa03
(2.16)
where a0 is the Bohr radius. The wave functions of two nearby but independent hydrogen atoms, as described by (2.16), are shown in Fig. 2.15a. As the protons are brought closer together to form the H2 + ion, the interaction between the electron and two protons leads to two possible wave functions as derived by quantum mechanical calculation. The two lowest energy states have either symmetric (even) wave function or antisymmetric (odd) wave function. The change in sign for the antisymmetric wave merely means that the two wave functions associated with ions are 180° out of phase. From these wave functions, the corresponding probability densities of the electron distribution can be easily estimated as shown in Fig. 2.16. For the antisymmetric wave function, there is no electron near the center of the system. In the case of symmetric wave function, there is a high probability of an electron existing in the middle of the two nuclei. Different electron distributions directly relate to the energy profile of the system. The potential energy of the system is given as
Fig. 2.14 Schematic of the formation of covalent bonding in a nitrogen molecule. The circles in each nitrogen atom represent the unfilled 2p valence electron states
24
2 Atomic Bonding and Crystal Structures
Fig. 2.15 Formation of bonding and antibonding combinations of atomic orbitals in diatomic hydrogen molecules with a single bonding electron. a The wave functions of two nearby hydrogen atoms. b The antisymmetric wave function and c symmetric wave function formed in a H2 + ion
Fig. 2.16 Probability density of the electron distribution in a H2 + ion with a antisymmetric and b symmetric wave functions
E PE = −E e−n + E n−n
(2.17)
where −E e–n represents the electron–nucleus attraction energy and E n–n represents the nucleus–nucleus repulsion energy (Fig. 2.16b). The high probability of finding electrons in between two nuclei increases the attractive force contribution (more negative) to E PE . As shown in Fig. 2.17, this decreases the potential energy distribution near the center and forms the primary mechanism for the covalent bonding Fig. 2.17 Potential energy of the H2 + ion (solid curves). The dashed curve is the potential energy of a single hydrogen nucleus
EPE A
B
r
2.3 Covalent Bond and sp3 Hybrid Orbit
25
Fig. 2.18 Energy level diagram shows the relative position of bonding (E b ) and antibonding (E a ) energies with respect to isolated ψ(1s) state energy (E s ). The related wave functions are also shown
(bonding state). In the antisymmetry case, the lack of electrons in between two cores means it is unfavorable to form a covalent bond (antibonding state). In other words, the spatial overlap of the wave functions ψ A and ψ B leads to the splitting of the original energy level E s , associated with the ψ(1s) state, into a higher and a lower molecular energy level (Fig. 2.18). The molecular orbital corresponding to the higher energy level is the antibonding state. The bonding state is where the electron occupies the lowerlying bonding orbital, thereby giving rise to a reduction in the total energy. This energy reduction corresponds to the binding energy of the covalent bond. Now, let us turn our attention to hydrogen molecules where there are two valence electrons. When forming covalent bonding in H2 molecules, the two valence electrons are shared equally by the two nuclei. The symmetric electron wave functions from the two electrons have the same quantum numbers n, l, and m. They, then, must have opposite spin orientations (s = ± 1/2) or antiparallel spins to comply with the Pauli exclusion principle. Thus, in a covalent bond the two shared electrons must have antiparallel spins, and this is also known as the electronpair bond. This concept applies to other materials, such as N2 , which has been discussed earlier. The six 2p electrons in a N2 molecule are bound in pairs with spins aligned antiparallel in each pair as shown Fig. 2.19a. We further examine this idea in water (H2 O) and phosphine (PH3 ) (Fig. 2.19). The oxygen has an electron configuration 1s2 2s2 2p4 , and phosphorous has an electron configuration 1s2 2s2 2p6 3s2 3p3 . Since the s electrons in the outer shell already have
Fig. 2.19 Electronpair bond formed in between a pair of electrons in p orbital with antiparallel spin in a N2 , b PH3 , and c H2 O. The dotted arrows indicate hydrogen electrons which make pairbonds with p electrons of phosphorous and oxygen
26
2 Atomic Bonding and Crystal Structures
their spins paired, only the p electrons need to be considered. For a phosphorous atom, there are three electrons that have unpaired spins, whereas for an oxygen atom, two of the four electrons already have paired spins leaving two electrons having unpaired spins. Therefore, a phosphorous atom is capable of making three electronpair bonds with three hydrogen atoms in PH3 , and an oxygen atom is capable of forming two electronpair bonds in H2 O.
2.3.2 Directional Property of Covalent Bonds In forming covalent bonds, the accumulated electrons in between the nuclei result in the overlapping of wave functions. A strong bond is formed if there is a maximum wave function overlap. The orbital wave functions of an atom can be derived using a simple model of a hydrogen atom consisting of a proton and a single electron that interact through electrostatic attraction. The wave function in 3D space is expressed as ψ(r, θ, φ) = R(r )Θ(θ )Φ(φ) where R, Θ, and Φ are the radial, azimuthal, and angular wave functions, respectively. The algebraic expressions for some of the wave functions are given below.
r 1s 2 : ψ100 = N100 exp − a0
r r 2 2s : ψ200 = N200 2 − e − a0 2a0 ⎧ ⎪ ψ210 = N210 ar0 exp − 2ar 0 cos θ ⎪ ⎪ ⎨ 2 p 6 : ψ211 = N211 ar0 exp − 2ar 0 sin θ exp(iφ) . ⎪ ⎪ ⎪ ⎩ ψ211¯ = N211¯ r exp − r sin θ exp(−iφ) a0 2a0
(2.18a) (2.18b)
(2.18c)
where a0 is the Bohr radius. The superscripts to s and p above indicate the allowed degeneracy of the state. The radial wave functions for the 2s state (ψ 200 ) and 2p state (ψ 210 ) are shown in Fig. 2.20a. The probability density distributions of the s states are always spherically symmetric, while the p, d, f states, etc., have angular dependence. For example, ⎧ ⎨ ψ210 2 ∝ r 2 exp − r cos2 θ a 0 ⎩ ψ21±1 2 ∝ r 2 exp − r sin2 θ a0
(2.19)
Figure 2.21 shows the shape of the probability density distributions for 2s and 2p states in space for a hydrogen atom. However, it is not ψ2 itself but the integration of ψ2 over the volume that represents the correct electron distribution in a 3D system. In a spherical system like the hydrogen atom model, the volume increases rapidly
2.3 Covalent Bond and sp3 Hybrid Orbit
27
Fig. 2.20 a Radial wave functions Rnl (r) and b radial probability density ψ2 r 2 of the 2s (ψ 200 ) and 2p (ψ 210 ) states of the hydrogen atom as a function of radial distance r in the unit of Bohr radius a0
Fig. 2.21 Electron density distributions of 2s and 2p states for a hydrogen atom. The polar (z) axis is oriented vertically
with the radius r and the larger values of r should be weighted heavily. Therefore, it is more interesting to find the probability that the electron is between r and (r + dr), ψ2 dυ = ψ2 r 2 sin θ dr dφdθ = ψ2 4πr 2 dr ∝ ψ2 r 2 .
(2.20)
Figure 2.20 shows the electron wave functions and the corresponding radial probability densities (ψ2 r 2 ) of 2s and 2p states in a hydrogen atom. Note that the radial
28
2 Atomic Bonding and Crystal Structures
probability density distributions of s and p states overlap heavily. More 2s electrons than 2p electrons are occupying states at larger r. As we will see in the next section, these results have important consequences in determining crystal structures of semiconductors. Consider the case of mixing s and p orbital wave functions. The s orbits (l = 0) of an atom always have a spherical symmetry, i.e., ψ s = g(r). For p orbits (l = 1), the wave functions are angularly dependent as described in (2.18c). Consequently, the spatial distribution of the wave functions leads to a strong orientation dependency in covalent bonding. Let us take a closer look at the spatial overlap between s and p wave functions. Since the linear combination of ψ 210 and ψ 21±1 is also a solution to the Schrödinger wave equation, we can transform the polar components of wave functions to the Cartesian coordinates with ⎧ ⎨ x = r sin θ cos φ (2.21) y = r sin θ sin φ ⎩ z = r cos θ Thus, ⎧ ⎨ ψ211 + ψ211¯ ∝ x ψ − ψ211¯ ∝ y ⎩ 211 ψ210 ∝ z
(2.22)
Letting R(r) = rf (r), we can express the three p wave functions as ψ px = x f (r ), ψ py = y f (r ), and ψ pz = z f (r )
(2.23)
The shapes of ψ s and ψ p ’s are shown in Fig. 2.22. Each p orbital extends along a specific coordinate axis, e.g., the xaxis for the ψ px orbital. Therefore, when ψ s and ψ p overlap to form a covalent bond, only certain ψ p orientations will provide a maximum overlap of electron distributions with ψ s . The covalent bond will be formed along one of these orientations to achieve a bond of maximum strength.
Fig. 2.22 Spherical s orbital and three p orbitals each directed along a different Cartesian axis
2.3 Covalent Bond and sp3 Hybrid Orbit
29
2.3.3 sp3 Hybrid Orbit In semiconductor crystals, the atomic bonds are not structured in the form of pure s or p wave function but a mixture of them. We will use the electron configuration of the methane (CH4 ) molecule to illustrate the hybrid orbitals. For a carbon atom, the electron configuration is shown in Fig. 2.23a (1s2 2s2 2p2 ). The inner s orbitals are all full. For the 2p orbital, there are only two unpaired electrons available for four single valence electrons from hydrogen atoms to form electronpair bonds. A closer examination reveals that the energy levels of 2s and 2p states are very close to each other, and, as shown in Fig. 2.20b, the probability density ψ(2p)2 r 2 overlaps heavily with ψ(2s)2 r 2 . Therefore, one of the two electrons in the 2s state can be elevated to the empty 2p state. Promoting one of the two electrons to the empty 2p state increases the energy of the system. But this allows four electrons from hydrogen atoms to form more electronpair bonds, which decreases the total energy of the system. Thus, the electron configuration of a carbon atom is changed into 1s2 2s1 2p3 in a methane molecule. This new configuration has a maximum of four unpaired electrons and is ready to form CH4 molecules by bonding with electrons from four hydrogen atoms. The electron configuration of the methane molecule now looks like that shown in Fig. 2.23b. The 2s1 p3 configuration in methane is called sp3 hybridization. If an sorbital is mixed with three porbitals, four sp3 hybrids are generated. The wave functions of the four sp3 hybrid orbitals in a CH4 molecule can be derived by linear combinations of s and p state (2.23) wave functions. ⎧ ψ111 ⎪ ⎪ ⎨ ψ11¯ 1¯ ⎪ ψ11 ⎪ ⎩ ¯ 1¯ ψ1¯ 11 ¯
(a)
1s2
= 21 ψs = 21 ψs = 21 ψs = 21 ψs
+ ψx + ψx − ψx − ψx
+ ψy − ψy + ψy − ψy
+ ψz − ψz − ψz + ψz
(2.24)
(b)
2s2
2p2
1s2
2s1p3
Fig. 2.23 Electronpair bond formed in a carbon atom, and b CH4 . The dotted boundary indicates the bonding orbitals. The dotted arrows are sites available for electronpair bonds
30
2 Atomic Bonding and Crystal Structures
(a)
(b)
sp3
z

[111]
H
[111] H
sp3 sp3
 
C
sp3
[111]
H
x
H
[111]
y
Fig. 2.24 a A set of four sp3 orbitals forms a tetrahedron with each sp3 orbital containing a large lobe and a small lobe. The large lobes point to the corners of the tetrahedron and can be used to share electrons in covalent bonds. b The sp3 hybrid orbitals of carbon in a CH4 molecule, each having an electron distribution directed toward one of the four alternating corners of a cube
Four sp3 orbitals are identical in shape, each one having a large lobe and a minor lobe as shown in Fig. 2.24a. The four orbitals are oriented in the space such that the large lobes form a tetrahedral arrangement. These new hybrid orbitals on carbon are used to share electron pairs with the 1s orbitals from the four hydrogen atoms to form a methane molecule, as shown in Fig. 2.24b. Once the methane molecule is formed, there is no extra unpaired free bond to link with other methane molecules. Therefore, a CH4 crystal can only be formed by van der Waals bonding force. The bonding structure of CH4 is a tetrahedron structure that is determined by optimizing repulsive forces between hydrogen atoms. The tetrahedron bond structure represents the basic form of all semiconductor crystals. For example, the silicon atom has an electron configuration of 1s2 2s2 2p6 3s2 3p2 . The four unpaired electrons in the 3s and 3p states form sp3 hybrid orbits for crystal bonding. Each Si atom is bonded with four neighboring Si atoms in a tetrahedron structure shown in Fig. 2.25a. This basic tetrahedron structure can propagate indefinitely in all directions as illustrated in Fig. 2.26. As will be discussed in more detail in Sect. 2.4, the resultant crystal has a diamond structure. For GaAs, the Ga (1s2 2s2 2p6 3s2 3p6 3d 10 4s2 4p1 ) and As (1s2 2s2 2p6 3s2 3p6 3d 10 4s2 4p3 ) can also bind in the diamondlike (zincblende) structure with tetrahedron coordination (Fig. 2.25b). Each Ga atom is surrounded by four (a)
109°28'
Si
(b)
Si
Si
Ga
Si Si
As
As
Fig. 2.25 Tetrahedron bond structure of a Si and b GaAs
As As
2.3 Covalent Bond and sp3 Hybrid Orbit
31
Fig. 2.26 An infinite tetrahedron arrangement of a covalent bonded diamond cubic structure. Reprinted with permission from [1], copyright Oxford University Press
As atoms and vice versa. The shared bonding electrons consist of five electrons from the As atom and three electrons from the Ga. The total number of electrons per atom is the same as in the case of the diamond structure of carbon or silicon.
2.3.4 Mixed IonicCovalent Bonds In pure covalent crystals like Si and diamond, the binding orbital between the nearest neighbors is a linear combination of hybridized orbitals from each atom and the wave function of the binding orbital can be expressed as ψb ∼ ψ1 + ψ2
(2.25)
where ψ 1 and ψ 2 are the wave functions of the two nearestneighbor atoms. Due to symmetry, the electrons shared in a bond must spend, on the average, ‘equal time’ on each atom. This leads to a symmetrical distribution of the electron density and to a purely covalent bond. In compound semiconductors, the bonding orbitals are less ideal than the pure covalent bond and the sharing of bonds is not so obvious. Consider GaAs as an example, where there are three and five valence electrons associated with Ga (4s2 4p1 ) and As (4s2 4p3 ) atoms, respectively. On average, there are four bonds per Ga atom sharing with four As atoms. In the simplest picture, each group V atom donates an electron to a group III atom so that each atom has four valence electrons with sp3 hybrid orbitals. This situation can be expressed as − + Ga 4s 2 4 p 1 + As 4s 2 4 p 3 → Ga 4s 1 4 p 3 + As 4s 1 4 p 3
(2.26)
However, this also leads to the formation of III− and V+ ions. The situation can be seen partially as electron sharing and partially as electron transfer. Shared electrons
32
2 Atomic Bonding and Crystal Structures
Table 2.2 Crystal structure and ionicity for III–V compound semiconductors. (W = wurtzite structure; ZB = zincblende structure) [2] III–V
Structure
Ionicity
III–V
Structure
Ionicity
III–V
Structure
Ionicity
AlN
W
0.449
GaN
W
0.500
InN
W
0.578
AlP
ZB
0.307
GaP
ZB
0.374
InP
ZB
0.421
AlAs
ZB
0.274
GaAs
ZB
0.310
InAs
ZB
0.357
AlSb
ZB
0.426
GaSb
ZB
0.261
InSb
ZB
0.321
in the bonding states spend a greater fraction of time on the cation, similar to a partially ionic bond. Thus, the timeaveraged wave function for a bonding electron is ψb ∼ ψcov + λψion
(2.27)
where ψ cov and ψ ion are wave functions for completely covalent and ionic forms, respectively. The weighting factor λ, called the ionicity parameter, determines the degree of ionicity (f i ): fi =
λ2 − 1 λ2 + 1
(2.28)
Another measure of ionicity in a compound is the difference in the electronegativity of its constituent elements as suggested by Linus Pauling. The electronegativity of an element represents the power of an atom to attract an electron to itself in a compound. Therefore, the electronegativity difference is well correlated with the ionicity of a compound. For purely covalent crystals such as Si and Ge, f i = 0. For III–V compound semiconductors, the theoretical ionicity values along with their crystal structures are listed in Table 2.2. It is interesting to note that compounds with large ionicity value (f i ≥ 0.45), e.g., IIInitride compounds, tend to crystallize in wurtzite structure rather than zincblende crystal structure.
2.4 Major Semiconductor Crystal Structures 2.4.1 Diamond Structure To generate a large silicon crystal, we must always fit silicon atoms together in the fournearestneighbor pattern suggested in Fig. 2.25a. A section of a crystal so formed, also called a unit cell of the crystal, is shown in Fig. 2.27. The atoms in the lower lefthand corner of this figure are accentuated to indicate the fundamental nature of Fig. 2.25a in the crystal construction. This type of lattice structure is characteristic of many important semiconductor crystals including diamond, Si, and Ge
2.4 Major Semiconductor Crystal Structures
33
Fig. 2.27 Diamond structure. Each atom is symmetrically surrounded in an imaginary cube (enclosed by dotted lines) by four nearest neighbors
a
and is called the diamond structure. The diamond crystal structure can be commonly described as two interpenetrating FCC structures that are displaced relative to one another along the body diagonal. In a tetrahedral configuration, each atom in the structure is surrounded by four nearestneighbor atoms. In Fig. 2.27, if we define one of the corners of the first FCC structure as the origin, the position of the origin of the second FCC structure is at [¼,¼,¼]a in terms of thebasis unit vector where √ 3/4 a. The unit cell a is the lattice constant. The nearestneighbor distance is cube has four atoms in its interior, an atom in the center of each of its faces (each of which is to be thought of as ‘shared’ with an adjoining cube in a large crystal), and eight atoms at the cube vertices (each of which is shared with seven other elementary cubes). Thus, the number of atoms in a crystal is eight times the number of elementary cubes; or, equivalently, there are eight atoms in a cube of size a3 . The other way of constructing the diamond lattice is to use four tetrahedral structures (Fig. 2.25a) as building blocks within a unit cell. As shown in Fig. 2.28, the bottom half of the unit cell is formed by joining two tetrahedral structures diagonally. The top half of the unit cell has the same arrangement but is rotated 90° with respect to the bottom half diagonal.
2.4.2 ZincBlende Structure The zincblende crystal structure is closely related to the diamond structure. The only difference is that in zincblende structures, there are two different types of atoms in the lattice. As shown in Fig. 2.29, the two different atoms occupy alternating lattice sites. In each tetrahedral cubic structure, the center atom is different from the atoms located at corners. The diamond structure of elemental semiconductors has the highest symmetry among all semiconductors. However, it lacks many of the symmetrical features
34
2 Atomic Bonding and Crystal Structures
Fig. 2.28 Construction of a diamond lattice structure using tetrahedral structures as building blocks
Fig. 2.29 Zincblende crystal structure. Two types of atoms are arranged alternately with each atom surrounded by four nearest neighbors of different types of atoms
a
enjoyed by primitive cubic. Compared to the diamond crystal structure, the symmetry ¯ of zincblende structure is further reduced. The physical structures of (111) and (1¯ 1¯ 1) surfaces are the same for diamond structure but different for zincblende crystal. For ¯ is a sheet of example, in GaAs the (111) consists entirely of Ga atoms, while (1¯ 1¯ 1) As atoms. Because of the different surface constituents, these two types of surface show very different chemical properties. Further, due to the nature of partially ionic bonding in zincblende structure, electric dipoles exist between the neighboring Ga and As atoms along 111. Although, at equilibrium, the net internal electric field is zero as the individual dipole moments get canceled out, compressions along 111 will cause atoms to move closer and induce a net internal electric field. This piezoelectric effect in compound semiconductors enhances carrier scattering which reduces
2.4 Major Semiconductor Crystal Structures
35
the carrier mobility. More detailed discussions on the physical properties of III–V compounds with zincblende structure will be given in Chap. 4.
2.4.3 Wurtzite Structure The wurtzite structure has the same tetrahedral coordination as the zincblende structure. It is the disposition of secondnearest neighbors which produces a hexagonal crystal. Figure 2.30 shows the unit cell of the hexagonal closepacked (HCP) structure. The basic HCP is formed by interlacing two basic hexagonal structures along the caxis. The second hexagonal lattice is displaced from the first by c/2 along the caxis and by 2a/3 and a/3 in the a1  and a2 directions, respectively. Only three atoms from the base of the second hexagonal are enclosed inside the first hexagonal unit cell. Each atom has twelve nearest neighbors: six in its own plane and three each in the planes above and below. The primitive unit cell has a rhombohedral√structure as outlined. In the HCP structure, the c and aaxes are related by c = 2a 2/3. The wurtzite structure is formed by interlacing two identical HCP structures containing different atoms, e.g., groupIII (Ga) and groupV (N) atoms, respectively, along caxis. The displacement of the two lattices is the bond length of 3c/8. This arrangement of atoms can be seen from the primitive unit cell structure illustrated in Fig. 2.31. The hexagonal unit cell of a wurtzite crystal structure is shown in Fig. 2.32. It is clear that along the caxis, layers containing atom A and atom B are staggered similarly to the (111) surface in the zincblende structure. Next, we shall investigate why the nearestneighbor atomic arrangement is the same for both zincblende and wurtzite structures but different for the secondnearest neighbors. In both structures, the bonds are covalent in nature with a certain fraction of ionicity. For zincblende crystals, the electron–electron repulsive force dominates the bondforming mechanism, leading to the tetrahedral structure. The second nearest neighbors are also arranged by optimizing the repulsive forces between atoms. As shown in Fig. 2.33a, using zincblende 111 GaN as an example, the secondnearest Fig. 2.30 Unit cell of the hexagonal closepacked (HCP) structure. The three atoms from the second hexagonal inside the unit cell are shown as dark spheres. The primitive cell is outlined and defined by unit vectors a1 , a2 , and c
36
2 Atomic Bonding and Crystal Structures
Fig. 2.31 Primitive unit cell of the wurtzite structure
c
a
Fig. 2.32 Unit cell of the wurtzite structure. The hexagonal boundary is outlined with dashed lines
Ga atoms in the top (111) plane are positioned in between the N atoms in the lower (111) plane. The two types of atoms in the neighboring (111) planes tend to minimize the repulsive force by maximizing the separation. For the wurtzite GaN structure, the high fraction of ionicity (0.5) implies that atoms are more ionized into Ga− and N+ . As shown in Fig. 2.33b, the cations and the anions tend to align along the caxis by the strong Coulomb attraction force. Therefore, the preferred crystal structure of GaN is the wurtzite structure. The layered structures shown in Fig. 2.33 containing atom A and atom B are similar in that they are staggered along the caxis and the 111 axis in wurtzite structure and
2.4 Major Semiconductor Crystal Structures
(a)
37
(b) Ga
axis
N
Ga–
caxis
N+
Fig. 2.33 Secondnearestneighbor bond arrangements along a 111 axis in zincblende and b caxis in wurtzite GaN crystals
zincblende structure, respectively. But the similarity stops here. The alignment of cations and anions along the caxis in wurtzite crystals such as GaN can easily induce a piezoelectric field by a mechanical stress applied along the same direction. The relative movements between cations and anions, caused by lattice vibrations above finite temperatures, break the equilibrium of the total electric field of the system. A net spontaneous polarization electric field is induced in the crystal along the caxis. Thus, the (0001) cplane is a polar surface. However, for some crystal planes containing mixed anions and cationsthat have equal numbers of bonds pointing out of ¯ ¯ aplane, the net spontaneous polarization the plane, e.g., 1100 mplane and 1120 field is zero. These are nonpolar planes with caxis parallel to the layer surface as shown in Fig. 2.34. Any crystal plane inclined between plane and cplane a nonpolar ¯ , 1122 ¯ and 2021 ¯ . is a semipolar plane including 1011
¯ a plane and Fig. 2.34 Nonpolar and semipolar crystal planes in wurtzite IIIN crystals. a 1120 ¯ semipolar plane and b 1100 ¯ ¯ and 2021 ¯ semipolar planes 1122 mplane and 1011
38
2 Atomic Bonding and Crystal Structures
2.5 Reciprocal Lattice, Diffraction Condition, and Brillouin Zone 2.5.1 Crystal Diffraction The lattice structure of a crystal can be deduced by diffraction experiments using radiation of a wavelength comparable with lattice dimensions. Xrays with proper energy are widely used as the diffraction sources to study semiconductor crystals. A suitable combination of Xray wavelength λ and incident angle θ will enhance the diffraction according to Bragg’s law nλ = 2dhkl sin θ
(2.29)
where d hkl is the lattice spacing and n is an integer (Fig. 2.35). Thus Xrays of a single wavelength directed on a crystal at an arbitrary angle will not be reflected. Currently, the two most widely used Xray diffraction techniques are the following: The Laue method utilizes Xrays of many wavelengths at a single angle of incidence, and the rotating crystal method allows monochromatic rays to encounter the crystal at a variety of angles. The Laue method uses a narrow beam of broadband Xrays to shine on a single crystal as shown in Fig. 2.36a. A diffraction beam will emerge for any Xray wavelength satisfying the Bragg condition. All backscattered diffraction beams are recorded simultaneously in the photographic plate positioned between the crystal and the Xray source. Each recorded diffraction ‘spot’ represents a specific wavelength that fits the Bragg condition. Therefore the crystal structure information recorded in the photographic plate is in the frequency domain. On the other hand, the rotating crystal method, shown in Fig. 2.36b, uses a monochromatic Xray beam, shaped from a broadband source through multiple Bragg reflections from separate crystals, as the diffraction source on a crystal rotating at a constant speed. At any rotation angle θ that fulfills the Bragg condition, a diffraction beam emerges. Since the orientation (θ ) of the crystal is varying as a function of time, the diffraction beams are recorded as ‘peaks’ in the time domain. For the same crystal subjected to diffraction Fig. 2.35 Reflection of a parallel beam of Xrays from two adjacent (hkl) planes of atoms in a crystal. The path difference between two Xrays has to be an integer multiplication of the path difference of 2d hkl sin θ for constructive reinforcement
2.5 Reciprocal Lattice, Diffraction Condition, and Brillouin Zone
39
Fig. 2.36 a Laue diffraction method arrangement using broadband Xray source. b A rotating crystal Xray diffraction arrangement using monochromatic Xrays selected by Bragg reflection from a separate single crystal
measurements using both Laue and rotating crystal methods, the different diffraction results presented in the frequency and time domains are equivalent. In fact, because the frequency (f = 1/t) is the inverse of time (t), the Fourier transform allows us to convert diffraction results from time to frequency domains, and vice versa. Just as a timevarying quantity can be described as a sum of Fourier components in the frequency domain, so the spatial properties of a crystal can be described as the sum of Fourier components in Fourier space, known as the reciprocal space which has a dimension of length–1 . This leads to the concept of the reciprocal lattice. In the discussion that follows, we shall see that the reciprocal lattices are associated with the Bragg diffraction condition in a crystal. Later in Chap. 3 we will apply the Fourier transformation to associate wave functions in real space (in length) and momentum space (in length–1 ).
2.5.2 Reciprocal Lattice So far we have described the crystal structure in terms of the realspace lattice points of atomic positions. However, to understand the wave diffractions by crystals, as described in the last section, it is more convenient to describe the crystal structure from the point of view of crystal planes. A set of (hkl) planes of the crystal structure is completely specified by the unit vector of the plane n and the interplane spacing d hkl . The overall structure of the crystal is then completely specified by the set of values of n and d hkl . This specific way of relating crystal structures to values of n and d hkl is cumbersome. Conversely, a much more useful representation is to define a vector which uniquely relates to each set of n and d hkl of the realspace lattice points G hkl = 2π n/dhkl
(2.30)
40
2 Atomic Bonding and Crystal Structures
It is obvious that this vector has the dimension of inverse length and can be used to define the socalled reciprocal lattice. Thus, every crystal structure has both a realspace lattice and a reciprocal lattice associated with it. To further explore the concept of reciprocal lattice vectors, the interactions of a wave with a periodic physical quantity of a crystal are illustrated below. In crystal diffraction measurements, the condition for the constructive interference of a wave scattered from the lattice points depends on the detailed unit cell structure of the crystal. Thus, the scattering intensity of the incident wave is determined by the spatial distribution of atoms within each cell. In periodic lattice structures, Fourier transformation can be applied to relate the direct lattice and wave vector domains. In a 1D system of a periodic lattice with a period a along x, the scattering wave density ρ satisfies the condition ρ(x + a) = ρ(x)
(2.31)
Using Fourier transformation, the 1D wave density becomes ρ(x) =
∞ ∞ 2nπ 2nπ 2nπ a0 + x + bn sin x = x (2.32) cn exp i an cos 2 a a a −∞ n=1
where 1 cn = a
a/2 −a/2
2nπ x dx ρ(x) exp −i a
(2.33)
is the Fourier coefficient. A displacement of x = ma, where m is an integer, leads to an identical ρ(x), hence satisfying the periodic requirement. Assume 2π /a ≡ k is the wave vector associated with the direct lattice spacing a. The 1D scattering wave density is expressed in terms of the wave vector k and the lattice vector x by ρ(x) =
∞
cn exp(ink · x)
(2.34)
−∞
In 3D periodic systems, ρ(r + T ) = ρ(r)
(2.35)
where T = h a + k b + l c is the translation vector. We can use the same equation with a minor modification as shown below: cG exp(i G · r n ) (2.36) ρ(r ) = n
2.5 Reciprocal Lattice, Diffraction Condition, and Brillouin Zone
41
The wave vector k and lattice vector x are replaced by G and rn , respectively. In order to preserve the translation invariance of ρ(r) with respect to the lattice vector rn , the vector G must fulfill certain conditions. Just like the 1D case, the product of G and rn has to preserve the periodic property of the lattice. Thus, G · r n = 2mπ and r n = n 1 a + n 2 b + n 3 c
(2.37)
where m is an integer for all n1 , n2 , and n3 , and a, b, c are the unit vectors of the lattice. Assume vector G can be expressed as G = ha∗ + kb∗ + l c∗
(2.38)
where h, k, l are integers and a*, b*, c* are unit vectors of a different coordination system. Then G · r n = ha∗ + kb∗ + l c∗ · (n 1 a + n 2 b + n 3 c) = 2mπ The relations between a, b, c and a*, b*, c* are derived as follows. For example, in the case of n2 = n3 = 0, we have G · r n = n 1 ha · a∗ + ka · b∗ + l a · c∗ = 2mπ For an arbitrary choice of n1 , this can only be satisfied by a · a∗ = 2π and a · b∗ = a · c∗ = 0 This implies a general expression of G i · r j = 2π δi j
(2.39)
where Gi and rj are the ith and jth components of vectors G and rn , respectively, and δi j =
1 for i = j 0 for i = j
(2.40)
The conditions stated above of a · a* = 2π and a · b* = a · c* = 0 imply a* = k 1 (b × c), or a* is perpendicular to the plane containing b and c. Therefore a · a∗ = 2π = k1 (a · b × c) and k1 =
2π (a · b × c)
(2.41)
42
2 Atomic Bonding and Crystal Structures
This leads to the definition of the reciprocal lattice unit vectors a*, b*, and c*, ⎧ b×c ⎪ ⎪ a∗ = 2π ⎪ ⎪ · b × c) (a ⎪ ⎨ c×a ∗ b = 2π ⎪ (a · b × c) ⎪ ⎪ a×b ⎪ ⎪ ⎩ c∗ = 2π (a · b × c)
(2.42)
and G = ha* + kb* + lc* is the reciprocal lattice vector. Whether this G satisfies the periodicity requirement can be examined by using the following example. Assuming G is the solution, it should possess the periodic property of ρ(r + T ) =
cG exp(i G · r)ex p(i G · T ) = ρ(r)
G
exp(i G · T ) = exp i hh + kk + ll = exp(iu) = sin(2uπ ) +cos(2uπ ) = 1 where u = (hh + kk + ll ) = integer. Thus, ρ(r + T ) =
cG exp(i G · r) = ρ(r)
(2.43)
G
The periodicity is maintained in the 3D reciprocal lattice.
2.5.3 Properties of the Reciprocal Lattice Vector As shown in Fig. 2.37, in direct lattice, the (hkl) plane intersects with a, b, and caxes at 1/h, 1/k, and 1/l, respectively. The three position vectors extending from the c
Fig. 2.37 Geometry of the direct lattice (hkl) plane and related vectors
N
1/l
R Q
1/k
P
a
1/h
(hkl) plane
b
2.5 Reciprocal Lattice, Diffraction Condition, and Brillouin Zone
43
origin to these three intersections are a/h, b/k, and c/l. Using these three vectors, we can define three vectors lying along the edges of the (hkl) plane as indicated by QP =
a b c b c a − , PN = − , and N Q = − h k h l k l
A linear combination of the above three vectors (QP × D + PN × E + NQ × F) forms a general vector R lying in the (hkl) plane: R=
a b c (D − E) + (F − D) + (E − F) h k l
(2.44)
where D, E, and F are integers. It can be further simplified by assuming A = D − E, B = F − D, C = E − F, and A + B + C = 0. Thus,
c A
a b B C +B +C = a+ b+ c (2.45) R=A h k l h k l
B C A R · G hkl = a+ b+ c · ha∗ + kb∗ + l c∗ h k l
B C A h+ k+ l = A+ B +C =0 (2.46) = h k l Therefore, R ⊥ Ghkl . The reciprocal lattice vector defined by Ghkl = ha* + kb* + lc* lies perpendicular to the direct lattice (hkl) plane. We now show that with the aid of Fig. 2.38 the separation of the planes in the direct lattice d hkl is equal to 2π /Ghkl . dhkl = r · n = r ·
Fig. 2.38 Construction for the determination of the spacing between successive (hkl) planes. n is the surface normal unit vector
G hkl a ha∗ + kb∗ + l c∗ 2π = · = G hkl  G hkl  G hkl  h
(2.47)
44
2 Atomic Bonding and Crystal Structures
The perpendicular distance of the adjacent (hkl) planes is dhkl =
2π 2π or dhkl = √ G hkl  h2 + k2 + l 2
(2.48)
2.5.4 Diffraction Condition From Fig. 2.35, the Bragg law of diffraction (2.29) requires nλ = 2d hkl sin θ. It is also possible to express the diffraction condition with the reciprocal lattice vector. Instead of considering the wavelength λ of the radiation which interacts with the crystal, we shall now consider the initial and final wave vectors k, k of a reflected diffraction. Assume a wave vector k associated with a wavelength λ is incident on the (hkl) plane and encounters an elastic diffraction or elastic scattering where there is no change in λ. Therefore, the diffracted wave vector k = k = 2π/λ
(2.49)
The change of k, shown in Fig. 2.39, is
k = k − k = 2kn sin θ =
4π G hkl 4π sinθ n = sin θ G hkl  λ λ
(2.50)
The change k is in the direction of the surface normal and perpendicular to the (hkl) planes. Since d hkl = 2π /Ghkl  and 2d sin θ = nλ, then
2dhkl k = sinθ G hkl (2.51) λ k = G hkl Fig. 2.39 The change in wave vector when undergoing an elastic scattering at the (hkl) plane
(2.52)
2.5 Reciprocal Lattice, Diffraction Condition, and Brillouin Zone
45
Fig. 2.40 Ewald construction for the Laue diffraction condition from a crystal in the reciprocal lattice. The incident Xray beam has a wavelength λ
or k = k + G hkl
(2.53)
Thus the scattering vector k is equal to a reciprocal lattice vector Ghkl . This is the 3D Bragg diffraction condition. In the Laue method of Fig. 2.36a, the array of diffraction spots from a crystal, recorded on the photographic film, thus corresponds to the set of points generated by Ghkl in the reciprocal lattice space. This can be represented graphically by the Ewald sphere construction shown in Fig. 2.40. We start by drawing a vector corresponding to the incident Xray beam, whose length is 2π /λ and which terminates at a point O of the reciprocal lattice. Note that the tail of the vector AO does not necessarily have to rest on a reciprocal lattice point. A sphere with a radius k or 2π /λ is constructed about point A as the center. The diffraction condition is satisfied whenever the spherical surface coincides with points of the reciprocal lattice where k = k + Ghkl . The vector OB or Ghkl that connects the two reciprocal lattice points coinciding with the sphere must be normal to the (hkl) plane of the direct lattice. Using simple trigonometric relations, we can verify in the following that Ghkl satisfies the Bragg condition. From (2.48), Ghkl has a length 2nπ /d hkl , where n is an integer. From Fig. 2.40, the length OB can also be expressed as 4π sin θ /λ. Equating these two expressions for the length of the vector OB leads to the Bragg condition. The diffraction condition of a real crystal surface can also be correlated to the reciprocal lattice using the Ewald sphere construction scheme. For example, the reflection highenergy electron diffraction (RHEED) method is commonly used to study crystal surfaces as shown in Fig. 2.41. Electrons having energy of 5–30 keV, corresponding to an electron wavelength of less than the lattice constant, are incident
46
2 Atomic Bonding and Crystal Structures
Fig. 2.41 Schematic diagram of the RHEED arrangement showing the incident electron beam at an angle θ ≤ 5° to the sample surface. The elongated spots indicate the intersection of the Ewald sphere with diffraction rods. (Reprint with permission from [3], copyright AIP Publishing.)
on the crystal surface at a low glancing angle of ≤5°. The diffraction of the incoming primary electron beam by the twodimensional (2D) atomic network of surface atoms leads to the appearance of streaks normal to the shadow edge on the fluorescence screen. The conditions for constructive interference of the elastically scattered electrons may be inferred using the Ewald sphere construction in the reciprocal lattice. Due to the loss of periodicity in the dimension above the crystal surface, the surface layer is represented by rods in a direction normal to the real surface in the reciprocal space (Fig. 2.42). The reciprocal lattice rods are labeled with only two Miller indices, h and k. Diffraction occurs where the Ewald sphere cuts a reciprocal lattice rod and the diffraction beam is labeled with the Miller index (hk) of the rod causing it. It should be noted that due to the high electron acceleration energy, the radius of the Ewald sphere is much larger than the separation of the rods. The wavelength of the incident electron beam λ is related to the energy by
(a)
(b)
Fig. 2.42 a Ewald sphere construction for a reconstructed semiconductor surface in reciprocal lattice space. The realspace lattice atoms are shown as circles. (Reprint with permission from [4], ¯ copyright Elsevier) b Diffraction pattern from the GaAs (001) − (2 × 4) surface along the 1¯ 10 azimuth
2.5 Reciprocal Lattice, Diffraction Condition, and Brillouin Zone
2 2π 2 E= 2m λ
47
(2.54)
Thus, at 5 keV, λ = 0.0174 nm. The radius of the Ewald sphere is k = 2π /λ = 362 nm−1 . If the surface lattice network has a lattice constant a of 5 Å, then the distance between adjacent rods in reciprocal space will be 2π /a = 12.57 nm−1 . As a result, the intersection of the nearly flat Ewald sphere and rods occurs along their length, resulting in a streaked diffraction pattern as illustrated in Fig. 2.42a. However, due to the finite surface roughness, the short diffraction streaks transform into elongated lines. Figure 2.42b is a typical RHEED pattern for a smooth (001) surface of GaAs.
2.5.5 The Brillouin Zone An alternative expression of the Bragg diffraction condition can be derived by rewriting (2.53) as 2 k = (k + G)2
(2.55)
2 k = k 2 + G 2 + 2k · G
(2.56)
or
Since k = k , (2.56) can be expressed as 2k · G + G 2 = 0
(2.57)
k · (G/G) = k · n = G/2
(2.58)
or
Equation (2.58) corresponds to a geometric structure that describes the locus of all points satisfying the Bragg condition, called the Bragg plane (Fig. 2.43). This is a plane that is the perpendicular bisector of a reciprocal lattice vector G. The Bragg law is only satisfied for those incident wave vectors whose tips lie on the Bragg plane in reciprocal space when the vector origin is tied to a reciprocal lattice point. Since the reciprocal lattice of a periodic direct lattice is also periodic and infinite in extent, it is most useful only to require the use of a limited volume of reciprocal lattice, or kspace. This volume is called the first Brillouin zone. The Bragg plane simply forms one of the faces of the first Brillouin zone. As shown in Fig. 2.44, the smallest 2D polyhedron centered at the origin and enclosed by perpendicular bisectors of reciprocal lattice vectors, i.e., Bragg planes, forms the (first) Brillouin zone.
48
2 Atomic Bonding and Crystal Structures
Fig. 2.43 Geometrical representation of the Bragg diffraction condition. Diffraction only occurs for an incident wave vector whose tip lies on the Bragg plane if its origin is tied to a reciprocal lattice point
G/2 O
k
G/2
n k'
G
Fig. 2.44 First Brillouin zone formed in the reciprocal space for a 2D oblique lattice. It is shown bisecting the midpoints of six shortest reciprocal lattice vectors from the center of this lattice structure
The points on the Brillouin zone boundary are special because every wave with k extending from the origin to the zone boundary gives rise to a Bragg reflected wave. It is obvious from Fig. 2.43 that k = k + G is satisfied on these boundaries. The interference of the incident primary waves and the Bragg reflected waves produces a ‘standing wave.’ This is important for the understanding of Xray diffraction and the formation of a bandgap in the electronic structure of semiconductor materials. (a) Example for a 2D square lattice The reciprocal lattice of a square direct lattice, whose lattice spacing is a, is also a square lattice of spacing 1/a (Fig. 2.45). The reciprocal lattice vector pointing from the origin to a lattice point (u, v) can be expressed as G = (2π /a)(uix + viy ) where u and v are integers. According to the Bragg condition, for k = k x ix + k y iy 2k · G + G 2 =
4π 2 4π uk x + vk y + 2 u 2 + v 2 = 0 a a
(2.59a)
or π 2 u + v2 = 0 f k x , k y = uk x + vk y + a
(2.59b)
2.5 Reciprocal Lattice, Diffraction Condition, and Brillouin Zone
49
Fig. 2.45 Construction of the first (dashed line boundary) and second (solid line boundary) Brillouin zones (BZ) in a 2D reciprocal lattice space. The square direct lattice has a lattice spacing a
This is a straight line of k x and k y . The intersections on the x and yaxes are ⎧
π u 2 + v2 ⎪ ⎪ on xaxis ⎨ kx = − a u
2 2 π u +v ⎪ ⎪ ⎩ ky = − on yaxis a v
(2.60)
To construct the smallest rectangle, we calculate k x and k y with the smallest possible u and v. At u = 0 and v = ± 1, we have k y = ± π /a. Similarly, at v = 0 and u = ± 1, we have k x = ± π /a. The four constant k’s form a square. This is the first Brillouin zone as shown in Fig. 2.45. Alternatively, bisecting the midpoints of four shortest reciprocal lattice vectors from the origin can also form the first Brillouin zone. For the second Brillouin zone, k x ± k y = ± 2π /a for u = ± 1 and v = ± 1. The higherorder Brillouin zones can be constructed through the same procedures. For example, using u = 0, v = ± 2 and v = 0, u = ± 2, the third zone boundaries are defined. On the Brillouin zone boundary, the wave vectors must follow the Bragg condition. For example, the Bragg condition of the first Brillouin zone, n = 1, becomes 2a sin θ = λ
(2.61)
For an incident wave of a wavelength λ, as seen in Fig. 2.45, the wave vector is k =
k02 +
π 2 a
=
2π λ
(2.62)
50
2 Atomic Bonding and Crystal Structures
and ky λ π/a 2π 1/a = = = · sin θ = 2 2a k x2 + k 2y k02 + (π/a)2 k02 + (π/a)2
(2.63)
Thus, 2a sin θ = 2a · (λ/2a) = λ, fulfilling the Bragg law. Therefore the Brillouin zone construction exhibits all the wave vectors that can be Bragg diffracted by the crystal. Other waves get weakened and eventually cease to exist. (b) 3D Brillouin zone of a FCC crystal As we will discuss in Chap. 3, the Brillouin zone concept is essential for the development of the energy band structure of semiconductors. The construction of Brillouin zones in 3D semiconductor crystals follows a procedure similar to that for the 2D case. Since most semiconductor crystals have either zincblende or wurtzite lattice structure, we shall investigate the Brillouin zones of the basic FCC and simple hexagonal structures. First, we need to transform the primitive unit cell of the FCC structure into reciprocal lattice spacing. As shown in Fig. 2.46, the translation vectors which define the primitive unit cell of the FCC lattice are a = (a/2)(b + c), b = (a/2)(c + a), c = (a/2)(a + b)
(2.64)
where a/2 defines the size of the unit cell. The translation vectors a , b , and c are vectors pointing from the origin to three neighboring facecentered surface lattice points, √ respectively. The formed cubic volume of the primitive cell is a · b × c = 3 a /2 2. Fig. 2.46 Primitive unit cell of an FCC crystal structure is formed by three translation vectors a , b , and c . These translation vectors point from the origin toward the surface atoms diagonally
c
Primitive cell a
a' b' b c'
a
2.5 Reciprocal Lattice, Diffraction Condition, and Brillouin Zone
51
z
Fig. 2.47 Reciprocal translation vectors a*, b*, and c* of the FCC crystal structure. The lattice points at the body centers are drawn as larger dark spheres
c*
y
x
Then the primitive translation vectors in the reciprocal lattice are calculated following (2.42) as ⎧
2π 2πa 2 (−a + b + c)/4 b × c ⎪ ∗ ⎪ a = = = 2π (−a + b + c) ⎪ ⎪ 3 ⎪ a /4 a ⎪ a · b × c
⎨ 2πa 2 (a − b + c)/4 2π c ×a = = b∗ = 2π (a − b + c) 3 ⎪ a /4 a a ·b ×c
⎪ ⎪ ⎪ 2πa 2 (a + b − c)/4 a × b 2π ⎪ ⎪ ⎩ c∗ = 2π = = (a + b − c) a 3 /4 a a ·b ×c
(2.65)
¯ , 111 ¯ , and 111¯ ] directions of a cubic These are vectors oriented along the 111 lattice, respectively. We can plot (2.65) as shown in Fig. 2.47 and realize that these are the primitive translation vectors of a BCC lattice! Thus, the reciprocal of an FCC lattice is a BCC lattice. The volume of the primitive cell in the reciprocal lattice is a* · b* × c* = 4(2π /a)3 . To construct the first Brillouin zone from these reciprocal translation vectors, we shall derive a general form of Ghkl : G hkl = ha∗ + kb∗ + l c∗ =
2π [(−h + k + l)a + (h − k + l)b + (h + k − l)c] a (2.66)
In a BCC lattice, there are eight nearest neighbors from the bodycentered lattice point along 111 (Fig. 2.48). For h = k = l = ± 1, there are eight reciprocal lattice vectors pointing to each corner of the BCC structure. The boundaries of the first Brillouin zone are located at G/2, and
52
2 Atomic Bonding and Crystal Structures
Fig. 2.48 First Brillouin zone of the facecentered cubic lattice in reciprocal space. Six pyramidshaped volumes (one shown in gray lines) are excluded since they are intersected by second nearest neighbors
1 π π G 111 = = (±a ± b ± c) 2 d 111 a
(2.67)
These eight vectors generate eight Brillouin zone surfaces halfway between the origin and the nearest points of the lattice, which form a regular octahedron. However, this is not the first Brillouin zone since the planes arising from the second nearest neighbors between bodycenter lattice points intersect it. Therefore, the six pyramidshaped corners in the 100 directions extending outside the first zone are excluded. The final form of the first Brillouin zone for an FCC lattice becomes a truncated octahedron (Fig. 2.48). The volume enclosed by the first Brillouin zone is also known as the Wigner–Seitz primitive cell of the reciprocal lattice. The eight hexagonal faces arise from the planes halfway to the atoms at the corners, while the six smaller square faces are halfway to the atoms in the middle of the next cells. As expected, these unit cells can fit together to fill the whole space as demonstrated in Fig. 2.49. Fig. 2.49 Way in which the first Brillouin zone cells of an FCC lattice can fill the whole space
2.5 Reciprocal Lattice, Diffraction Condition, and Brillouin Zone
53
Fig. 2.50 Construction of the first Brillouin zone for the plane simple hexagonal lattice. The reciprocal lattice points are shown at six corners and the origin
(c) 3D Brillouin zone of a simple hexagonal crystal The reciprocal lattice of a simple hexagonal lattice is another simple hexagonal lattice rotated 30° about the caxis. If the basic lattice translations for the direct lattice in the basal plane and along the caxis are, respectively, a and c, then for the reciprocal √ lattice they are a* and c*, where a* = 4π/ 3a and c* = 2π /c. Figure 2.50 shows seven points of the reciprocal lattice of a simple hexagonal lattice. If we take the central point √ O as origin, the other six lie at the corners of a regular hexagon of side a* = 4π/ 3a and are the six nearest neighbors. The first Brillouin zone is formed by connecting bisectors of the lines joining √ O to the other six nearest neighbors. It ∗ / 3 = 4π /3a and hence covers a unit cell is a hexagon √ whose sides have length a √ area of (a ∗ )2 3/2 = 8π 2 / 3a 2 . It should be noted that the hexagon forming the first Brillouin zone has the same orientation as the hexagons of the direct lattice. Fig. 2.51 First Brillouin zone for the simple hexagonal lattice. Some lattice points of the reciprocal lattice are also shown
54
2 Atomic Bonding and Crystal Structures
The 3D first Brillouin zone of the simple hexagonal lattice is obtained simply by introducing planes parallel to the caxis through the sides of the hexagon and two planes perpendicular to the caxis, each at distance c*/2 from O. The first Brillouin zone is therefore a hexagonal prism of height c* = 2π /c whose axis is parallel to the caxis of the direct lattice. The hexagonal of side 4π /3a is oriented same direction in the √ 3 as the hexagons of the direct lattice. It occupies a volume of 16π / 3 /a 2 c. The first Brillouin zone is shown in Fig. 2.51, together with some points of the reciprocal lattice. Problems 1. Both AsH3 and SiCl4 are common gases for semiconductor growth and processing. Discuss their molecular bonding properties. 2. The ionic radii of Na, Cs, and Cl are 0.875 Å, 1.455 Å, and 1.475 Å, respectively. (a) For NaCl, the FCC structure is the preferred crystal structure. Verify that this structure prevents anion–anion or cation–cation contact. (b) Verify that the simple cubic structure has a higher atomic packing density than the FCC structure in CsCl crystals. 3. Calculate the atomic packing density for the following crystal structures: (a) (b) (c) (d)
Simple FCC Simple hexagonal closepacked (HCP) Diamond Wurtzite.
4. Assume the cube containing a tetrahedron bond structure has a length a on each side. Calculate the bond length of the tetrahedron bond in terms of length a. Also, determine the angle between two tetrahedron bonds. 5. The primitive unit cell of a hexagonal closepacked (HCP) structure can be defined by unit vectors a and c. Prove √ that, using the incompressible spheres model, the ratio between c and a is 8/3. 6. The primitive unit cell of a wurtzite structure can be defined by unit vectors a and c (Fig. 2.31). Derive the relations between a, c, and the bond length. 7. Prove that the reciprocal lattice of a simple hexagonal lattice is another simple hexagonal lattice. Determine the new lattice constants along the aaxis and caxis. 8. (a) Derive the reciprocal lattice of the BCC structure. What is the new crystal structure? (b) What is the angle between G110 and G101 ? 9.
Make a plot of the first two Brillouin zones of a primitive rectangular twodimensional lattice with axes a, b = 2a. 10. Derive the dielectric constant tensor for a simple tetragonal crystal. 11. The hexagonal crystal is called an optically uniaxial crystal and has two principal dielectric constants: 33 along the caxis and 11 in the basal plane. Show that the dielectric constant tensor of hexagonal crystals can be expressed as
2.5 Reciprocal Lattice, Diffraction Condition, and Brillouin Zone
55
⎡
⎤ 11 0 0 = ⎣ 0 11 0 ⎦. 0 0 33 Note: This can be done by considering a rotation of θ = π /3 about the caxis. The new coordinates (x and y ) are related to the original coordinates through
x = x cos θ + y sin θ . y = y cos θ − x sin θ
References 1. 2. 3. 4.
M. Prutton, Introduction to Surface Physics (Oxford University Press, 1994) J.C. Phillips, Rev. Mod. Phys. 42, 317 (1970) B. Bolger, P.K. Larsen, Rev. Sci. Instrum. 57, 1363 (1986) P.K. Larsen, P.J. Dobson, J.H. Neave, B.A. Joyce, B. Bolger, J. Zhang, Surf. Sci. 169, 176 (1986)
Further Reading 1. C. Kittel, Introduction to Solid State Physics, 6th edn. (Wiley, 1986) 2. H. Ibach and H. Lüth, Solid State Physics, 2nd edn. (Springer, Berlin, 1996) 3. S. Wang, Fundamentals of Semiconductor Theory and Device Physics (PrenticeHall, 1989)
Chapter 3
Electronic Band Structures of Solids
Abstract The property that distinguishes semiconductors from other materials concerns the behavior of their charged carriers, in particular the existence of gaps in their electronic and photonic transition spectra. The microscopic behavior of charged carriers in a solid is most conveniently specified in terms of the electronic band structure. The metals are good conductors with overlapped conduction and valence bands, while insulators such as ionic crystals have large bandgaps of over 8 eV. The semiconductor crystals have a finite energy bandgap between metals and insulators. The purpose of this chapter is to develop the basic understanding of energy bandgap formation in solids. We start our discussion by first developing the free electron theory based on quantum theory in which the Fermi–Dirac statistics are used instead of the classical Boltzmann statistics. Then the spatial periodic potential of a solid is introduced according to Bloch’s theorem. Finally, the interference at Brillouin zone boundaries leads to constructive and/or destructive interferences of electron waves forming the energy bandgap.
3.1 Free Electron Theory and Density of States The simplest model for describing electrons in solids is to assume that the valence electrons of an atom are free to move anywhere throughout the volume of the material. This is an appropriate model for a metallic solid. Of course, for an isolated atom, the electrons are confined by the large barrier of the Coulomb potential well and cannot move away from the nucleus. But when atoms bond together to form crystals, the potential barriers between atoms are lowered by the bonding energy. The simple model further assumes that the periodically arranged nuclei or the cores of the atoms are stationary and the core electrons shield the nuclear charge completely. Thus the potential appears qualitatively as shown in Fig. 3.1 where a constant electrostatic potential exists everywhere in the solid. Any potential ‘bump’ associated with individual atoms is smoothed out. This allows valence electrons to move freely within the crystal as free electrons. Therefore, we can use a ‘particle in a box’ approach to treat the problem. Furthermore, we neglect any electron–electron interactions by allowing only one free electron in the system. © Springer Nature Switzerland AG 2020 K. Y. Cheng, III–V Compound Semiconductors and Devices, Graduate Texts in Physics, https://doi.org/10.1007/9783030519032_3
57
58
3 Electronic Band Structures of Solids
Fig. 3.1 Schematic of the potential within a perfectly periodic crystal lattice of positive cores. The vacuum level V 0 is the energy that the electron must acquire in order to leave the crystal
3.1.1 OneDimensional System The simplified ‘one free electron theory’ in 1D can be pictured as a finite potential well with a well depth V 0 and width L shown in Fig. 3.2. The only electron in the well has energy of E < V 0 . Since the barrier height of the well is finite, there are bound to be leakage waves outside the well. The 1D Schrödinger wave equation of this system outside the well is −
2 d2 ψ + V0 ψ = Eψ 2m dz 2
(3.1)
Since E < V 0 , the solution of the wave function is ψ = A exp(−αz) + B exp(αz)
(3.2a)
and α= Fig. 3.2 Illustration of a finite square potential well experienced by an electron in the 1D free electron model
2m(V0 − E)/2
(3.2b)
V = V0
E
z
V=0 0
L
3.1 Free Electron Theory and Density of States
59
where V 0 – E is the work function, and E is the kinetic energy of the electron. At z = ∞, ψ approaches 0, and B = 0. Thus, for z > L, the decay wave function outside the crystal is ψ(z) = A exp(−αz)
(3.3)
In GaAs, V 0 – E ~ 4 eV and using the electron effective mass of 0.063m0 , we have α ~ 2.57×107 cm−1 . This means the amplitude of the wave function ψ(z) drops to 1/e in 3.89 Å or about a monolayer of atomic thickness. Therefore, under practical situations, we can neglect the penetration depth outside the crystal and use the infinite well approximation instead. The solution within the well becomes ψ(z) =
A sin(k z z), 0 ≤ z ≤ L 0, elsewhere
(3.4)
where the wave vector k z = nπ /L and n = 1, 2, 3…. The first three wave functions are plotted in Fig. 3.3. Replacing the solutions (3.4) in the wave equation (3.1), we have −
2 2 2 d2 A sin(k z z) = k ψ = Eψ 2 2m dz 2m z
(3.5)
The energy eigenvalue is related to the wave vector by E= Fig. 3.3 First three wave functions of a free electron in a square potential well of length L
2 k z2 2m
(3.6)
n=3
n=2
n=1
z 0
L
60
3 Electronic Band Structures of Solids
Fig. 3.4 Energy E plotted as a function of k according to (3.6)
E
0
k
In the 1D free electron model, as shown in Fig. 3.4, the energy eigenvalue is a parabolic function of the wave vector k z .
3.1.2 ThreeDimensional System (a) Wave function ψ(x, y, z) The general expression of the 3D wave function is −
2 2 ∇ ψ(x, y, z) + V0 ψ(x, y, z) = Eψ(x, y, z) 2m
(3.7)
Using the infinite well approximation, we only have to consider ψ(x, y, z) inside the crystal (a cube of side L), where V = 0. Solving the wave equation by separation of variables, assuming ψ(x, y, z) = X(x) Y (y) Z(z), we get −
∂2 X 2 ∂ 2Y ∂2 Z Y Z 2 + X Z 2 + XY 2 = E XY Z 2m ∂x ∂y ∂z
(3.8a)
or −
2 2m
1 ∂2 X 1 ∂ 2Y 1 ∂2 Z + + 2 2 X ∂x Y ∂y Z ∂z 2
=E
(3.8b)
This equation is equivalent to three independent equations in X, Y, and Z. For example, the Xrelated equation is −
2 ∂ 2 X = X Ex 2m ∂ x 2
where E x is a constant. The solution of the wave equation in x is
(3.9)
3.1 Free Electron Theory and Density of States
61
X = A x sink x x + Bx cosk x x
(3.10a)
and kx =
2m E x 2
(3.10b)
Again, similar to the 1D system, we can use the condition of V 0 = ∞ at x = 0 and x = L such that ψ(0) = ψ(L) = 0. Thus, Bx = 0 and X = A x sink x x
(3.11a)
and kx =
nx π L
(3.11b)
The wave functions of Y and Z can be solved in the same manner. We come to the final solution of the wave function in 3D as
ψ(x, y, z) = Asin(k x x)sin k y y sin(k z z)
(3.12a)
and kx =
nyπ nx π nz π , ky = , kz = L L L
(3.12b)
where nx , ny , and nz are positive integers or quantum numbers which specify the relationship of ψ in the x, y, and zdirections. The amplitude A is calculated through the normalization process using ∫ ψ ∗ ψdxdydz = 1. v
L A
L sin (k x x)dx
2
2
0
sin k y y dy
0
Since ∫ sin2 (ax)dx =
x 2
−
L sin2 (k z z)dz = 1
2
sin(2ax) , 4a
(3.13)
0
for a = k i = ni π/L,
sin(2ax) L sin(2n i π ) − sin 0◦ =0 = 4a 4a 0 Therefore, L sin2 (k x x)dx = 0
x L L = 2 0 2
(3.14a)
62
3 Electronic Band Structures of Solids
and A = (2/L)3/2 .
(3.14b)
The final solution of the wave function becomes ψ(x, y, z) =
3/2
2 sin(k x x) sin k y y sin(k z z) L
(3.15a)
and kj =
ni π for j = x, y, z and n i = 1, 2, 3, . . . L
(3.15b)
(b) Energy eigenvalues (E) The allowed energy levels can be derived by inserting the wave function solution (3.15a) into the 3D wave function (3.7) −
2 2 ∂ 2ψ ∂ 2ψ ∂ 2ψ ∇ ψ = Eψ and ∇ 2 ψ = + + 2m ∂x2 ∂ y2 ∂z 2
(3.16)
The second derivative terms in (3.16) are calculated using the wave function solution (3.15a) as follows: 2 2 ∂ 2ψ 2 ∂ ψ 2 ∂ ψ = −ψk , = −ψk , = −ψk z2 x y ∂x2 ∂ y2 ∂z 2
(3.17)
Then the wave equation becomes −
2 2 2 ∂ 2 ψ ∂ 2ψ ∂ 2ψ = k x + k 2y + k z2 ψ = Eψ + + 2 2 2 2m ∂ x ∂y ∂z 2m
(3.18)
which leads to the energy eigenvalues of E=
2 2 2 k 2 = k x + k 2y + k z2 2m 2m
(3.19)
Thus, E ∝ k 2 = k x2 + k 2y + k z2
(3.20)
In classical theory, the kinetic energy of a particle with momentum p can be expressed as K .E. =
1 2 p2 = px + p 2y + pz2 2m 2m
(3.21)
3.1 Free Electron Theory and Density of States
63
Since our discussions of the total energy of the free electron involve kinetic energy only, the expressions of energy in (3.19) and (3.21) are identical. The allowed energy eigenvalues indicate that p = k
(3.22)
This is the de Broglie relationship, and p is the crystal momentum. However, it should be stressed that the wave vector k for electron wave functions in a periodic potential is not a measure of true physical momentum. As will be discussed later, the physically distinct values of the wave vector (crystal momentum) of an electron in a crystalline lattice—as opposed to those of a free particle, which can take any value—are restricted by the first Brillouin zone. Further, the energy functions also contain the wave nature of the electron motion in the potential well. For n = 1 in (3.15b), k = π /L, and the allowed wavelength is λ = 2π /k = 2L or k = 2π /λ. The wavelength is related to the particle nature of the electron through λ=
2π h 2π =√ = k p 2m E
(3.23)
Therefore, the electron with a momentum p will be diffracted like a wave with a wavelength λ in a crystal! Since k = nπ /L, the energy eigenvalue can also be expressed as a function of n as E=
2 π 2 2 2 π 2 2 n x + n 2y + n 2z n = 2m L 2m L
(3.24)
or
E ∝ n 2x + n 2y + n 2z = n 2
(3.25)
The results of (3.19) and (3.24) indicate that the 3D constant energy surface in n or kspace is a sphere. For each k i determined by ni there is a corresponding λi or mode. Each allowed energy state corresponding to a point ni can be displayed in the nspace with positive integer coordinates nx , ny , and nz . It is obvious that the energy eigenvalues are degenerate for nx = ny = nz . For example, for (nx , ny , nz ) equals (1, 2, 3), (1, 3, 2), (2, 3, 1), (2, 1, 3), (3, 1, 2), or (3, 2, 1), there are six degenerate energy states with the same energy. The number of degenerate states increases dramatically with increasing energy.
64
3 Electronic Band Structures of Solids
3.1.3 Density of States (DOS) In many situations, such as when computing the electron distribution, it is necessary to know how the electrons are distributed in the energy spectrum. This could be done through the use of (3.24) to derive a density of states. Consider a 2D crystal lattice in nspace where nz = 0, as shown in Fig. 3.5. Each lattice point is defined by a pair of (nx , ny ). Since k i = ni π /L = 2π /λi , each point corresponds to a specific mode of wave oscillation. The number of normal modes of oscillation inside a finite area defined by a rectangular box is simply the number of lattice points within nx ny . In the 3D case, the number of normal modes of oscillation is N ≡ nx ny nz , which forms an orthorombic volume. In a crystal the spacing between these points is extremly close. For example, the wavelength of, say, a 3 eV electron is h/(2 mE)1/2 ∼ = 7 Å and k = 2π /λ ∼ = 9×107 cm−1 . For a 1 cm3 cube, the number of oscillation modes in one coordinate direction is kL/π ~ 3 × 107 ! Therefore, we shall replace ni by dn and N ≈ dN = dnx dny dnz . Due to the large number of modes, they form a continuous band instead of discrete states. Since ni are all positive integers, as shown in Fig. 3.6, one need only count the ni in the first octant of the constant energy sphere. The number of normal modes in the first octant is 1 4π n 3 (3.26a) N = 8 3
ny
nx
ny
nx 0
1
2
3
4
Fig. 3.5 Schematic of the states of an electron in a 2D infinte well. The circle corresponds to a constant energy
3.1 Free Electron Theory and Density of States
65
Fig. 3.6 Spherical surface corresponding to constant energies E and E + dE plotted in the momentum (n) space of a particle
where kL L n= = π π
2m E 2
(3.26b)
Then, including the two possible spins into the total number, we have 3/2 2m E 3/2 L 3 2 4π 1 3 2m E L N = 2N = = 8 3 2 π 3π 2 2
(3.27)
The number of electron states within an energy interval dE, between E and E + dE, is dN =
3 2m 3/2 √ L dN dE = EdE dE 2π 2 2
(3.28)
The density of states (DOS) is defined as the number of states per unit energy interval near E per unit volume. It is expressed as D3D (E) =
dN dE
1 1 2m 3/2 √ −3 −1
= E cm eV L3 2π 2 2
(3.29)
In the 2D case, such as in a quantum well, N =
π L 2 2m E π n2 N = · 2· 2 = 4 4 π 2
(3.30)
Thus, dN m L2 = dE π 2
(3.31)
66
3 Electronic Band Structures of Solids
Fig. 3.7 Density of states distributions in bulk (3D), quantum well (2D), quantum wire (1D), and quantum dot (0D) structures
and D2D (E) =
dN dE
1 m = = constant cm−2 eV−1 2 2 L π
(3.32)
In the 1D case, such as in a quantum wire, N = n = kL/π. 2L N = 2N = π
2m E 2
(3.33)
Then dN L = dE π
2m 2 E
(3.34)
and D1D (E) =
dN dE
1 1 = L π
1 2m ∝ √ cm−1 eV−1 E E
(3.35)
Finally, when the volume of the 3D confinement of a potential well reduces to contain only one energy state, the structure becomes a quantum dot. Since there are two electrons allowed per state E 0 , one spinup and one spindown, the DOS of zerodimension (0D) is given as
3.1 Free Electron Theory and Density of States
D0D (E) = 2δ(E − E 0 )
67
(3.36)
The delta function indicates that only when E = E 0 is there a state. The DOS as a function of energy for 3D, 2D, 1D, and 0D distributions is plotted in Fig. 3.7.
3.2 Periodic Crystal Structure and Bloch’s Theorem The simple model of the free electron theory using oneelectron approximation of a square potential well has been successful in accounting for some physical properties of solids, in particular those of metals. However, in crystals, the ‘free’ electron situation is not very accurate. Therefore, this overly simplified model needs refinements in order to improve its ability to explain the properties of semiconductors. One obvious addition to the model is to add the spatial dependence of the potential experienced by a valence electron in a crystal. The effect of the added potential associated with the ion cores is particularly pronounced in periodic ioncore potentials. However, this also imposes a concomitant constraint on the wave functions that describing the motion of an electron in the periodic potential. Fortunately, this added constraint can be treated easily using the theory that Felix Bloch proposed in 1928.
3.2.1 Bloch’s Theorem The free electron theory developed so far has used the square well approximation that leads to the sinusoidal wave function solutions of (3.15a). In our present assumption, to simplify the discussions, all deviations from a perfect periodicity will be neglected. This means that even the surface effects are removed by assuming an infinitely extended potential. For an infinite 1D system with a uniform potential energy of V (=constant), the wave function is now represented by a traveling plane wave of the form ψk (z) = A exp(ikz)
(3.37)
This leads to a uniform distribution function of ψk∗ ψk = ψk2 = A2 = constant. Therefore, the system is translationally invariant. Now a periodic potential energy is introduced to the system. This potential is the sum of the electrostatic potential due to ion cores of lattice atoms and the potential due to all other outer electrons. The charge density from outer electrons would have the same average value in every unit cell of the crystal and would also be periodic. Thus the total potential has the periodicity of the lattice. Based on this reasoning, Bloch argued that the total potential energy V (z) with a periodicity of the lattice could be substituted into the 1D Schrödinger equation.
68
3 Electronic Band Structures of Solids
−
2 d 2 ψ + V (z)ψ = Eψ 2m dz 2
(3.38)
He concluded that the wave functions, which satisfy (3.38), subject to such a periodic potential, must be of the form ψk (z) = u k (z) exp(ikz)
(3.39)
where uk (z) are functions with the same periodicity of the lattice. The theory leading to (3.39) is known as Bloch’s theorem, and functions uk (z) are called Bloch functions. To discuss Bloch’s theorem, let us first examine a 1D crystal, shown in Fig. 3.8, which has a linear array of atoms with interatomic (lattice) spacing a. Since the potential has the periodicity of the lattice, then V (z) = V (z + a)
(3.40)
for any value of z. For such a periodic potential system, the wave function solutions shall repeat after N unit cell length, where N is an arbitrary number. Then ψ(z) = ψ(z + N a)
(3.41)
for any value of z. In view of the translational symmetry of the system, the wave functions of the neighboring unit cells can be related by an expression of the form ψ(z + a) = λψ(z)
(3.42)
where λ is a function to be determined. This means that for the location separated by N unit cells, ψ(z + N a) = λ N ψ(z) = ψ(z)
(3.43)
Fig. 3.8 Periodic potential for a linear atomic lattice. We may assume that the wave functions of all eigenstates must repeat after some arbitrary number N of unit cells
3.2 Periodic Crystal Structure and Bloch’s Theorem
69
Comparing (3.41) and (3.43) shows that λN = 1 and λ must be one of the N roots of unity: λ = exp(i2π P/N )
(3.44)
where P is an integer representing the number of complete cycles in the distance Na. Therefore, we can relate the wave vector k to P by k = 2π P/Na. Then, for ψ(z + a), λ = exp(ika)
(3.45)
Thus, one form of the wave function is ψ(z + a) = exp(ika)ψ(z)
(3.46)
An equivalent and general form of the above equation is that the wave function is the modulated plane wave ψ(z) = exp(ikz)u k (z)
(3.47)
where uk (z) is a periodic function which also has the translational periodicity of the lattice. This is the onedimensional Bloch function. It is clear from (3.42), (3.45), and (3.47) that u k (z + a) = exp[−ik(z + a)]ψ(z + a) = exp[−ik(z + a)]λψ(z) = exp[−ik(z + a)] exp(ika)ψ(z) = exp(−ikz)ψ(z) = u k (z)
(3.48)
The function uk (z) is thus periodic with a period a. We can expand this 1D result to 3D crystal systems with a periodic potential function proportional to the periodicity of the lattice, shown as V (r) = V (r + T ) and T = n 1 a + n 2 b + n 3 c
(3.49)
The wave functions which satisfy the corresponding Schrödinger wave equation have the form of a plane wave with a propagation constant k modulated by a function uk (r) whose periodicity is that of the crystal lattice.
ψk (r) = u k (r) exp(i k · r) u k (r) = u k (r + T )
(3.50)
70
3 Electronic Band Structures of Solids
3.2.2 Reduced Zone Representation The 1D Bloch function of (3.39) can be written as ψ(z) = u k (z) exp(i2π Pz/N a)
(3.51)
In this equation, as will become clear next, it is not necessary to use the value for P which is larger than ±(N/2), corresponding with k = ±(π /a). Any excess periodicity can be transferred into the uk (z) factor of the Bloch function. We notice that the range of wave vector from k = –(π /a) to k = +(π /a) corresponds to the first Brillouin zone in reciprocal lattice of the 1D lattice with a lattice spacing of a. Thus it is useful to examine the Bloch wave function near the origin of the kspace. For the 3D case, the Bloch wave function whose wave vectors differ from ψ k (r) by a reciprocal lattice vector G according to k + G = k
(3.52)
is also equivalent in terms of the electron energy. It shows ψk+G (r) = u k+G (r) exp[i(k + G) · r] = u k+G (r) exp(i G · r) exp(i k · r) = u k (r) exp(i k · r) Thus, ψk+G (r) = ψk (r)
(3.53)
Here, we used u k+G (r) = u k (r) and exp(i G · r) = exp(i2mπ ) = 1. The Schrödinger wave equations for ψ k and ψ k+G can be expressed, respectively, as H ψk = E k ψk
(3.54)
H ψk+G = E k+G ψk+G
(3.55)
and
Using (3.53), we can combine these wave equations into E k ψk = E k+G ψk+G
(3.56)
E k = E k+G
(3.57)
or
3.2 Periodic Crystal Structure and Bloch’s Theorem
71
Thus, the translational realspace periodicity of the lattice potential imposes periodicity on the energy eigenvalues and wave functions in reciprocal kspace. To examine the energy–momentum relationships of the electron, one needs only know these functions for k values in the first Brillouin zone, k . For example, as shown in Fig. 3.9, assume π /a ≤ k ≤ 3π /a in a 1D system with a lattice constant a, or k=
π π 2π + k and − < k < a a a
(3.58)
Then, ψk (z) = u k (z) exp(ikz)
= {u k (z) exp[i(2π/a)z]} exp ik z
(3.59)
where exp[i(2π /a)z] is a periodic function with the same periodicity as uk (z). We can rewrite the term inside the curly bracket as a new periodic function u k (z) with the same periodicity. Thus,
ψk (z) = u k (z) exp ik z .
(3.60)
This reduces the Bloch wave number to the range –π/a ≤ k ≤ π/a, which is the first Brillouin zone. Other higherorder wave vectors can also be reduced to the first Brillouin zone using the reduced zone representation.
Fig. 3.9 Energy as a function of wave vector for electrons in a onedimensional crystal of lattice constant a, where the amplitude of the periodic potential is set to zero. The continuous energy function is shown as a multiplevalued function of k in the shaded first Brillouin zone using the reduced zone representation
72
3 Electronic Band Structures of Solids
3.2.3 Empty Lattice Model—Energy Band Calculation for an FCC Crystal In the free electron model, it is simple to discuss electron energy and wave vector without regard for the crystallography of the solid. As soon as we take the periodic potential into consideration, the Brillouin zone boundaries (surfaces) in kspace become particularly important. Therefore, the following discussion of the relationship between energy and momentum for electrons in crystals will be in kspace. For the free electron model, the allowed energy values are distributed continuously in a parabolic form of E=
2 k 2 2m
(3.19)
When a finite periodic potential distribution is added, the periodic lattice information needs to be incorporated. Since we consider one electron in the crystal lattice only, without including electron–electron wave interactions, this approach is also called the empty lattice model. The 3D parabolic Ek relationship is modified with the incorporation of the reciprocal lattice vector G as E=
2 k + G2 2m
(3.61)
where k = k x a + k y b + k z c and G = ha* + kb* + lc*. As we have discussed in Sect. 2.5, G contains the lattice information for a specific crystal structure. For FCC crystals, using the translation vectors of the Gvector from (2.65) leads to E FCC
2 = 2m
2 2 2π 2π (−h + k + l) + k y + (h − k + l) a a 2 2π + kz + (3.62) (h + k − l) a kx +
By properly adjusting the system of units used, the expression can be reduced to
2 E = (k x + G x )2 + k y + G y + (k z + G z )2
(3.63)
where Gx , Gy , and Gz are integers to be selected for different energy states. Based on this equation, we can calculate the Ek curves, or the electronic band structure, along the 100 and 111 axes in the reduced zone representation.
3.2 Periodic Crystal Structure and Bloch’s Theorem
73
(a) 100 As shown in Fig. 3.10, along [100], k y = k z = 0, and E = (k x + G x )2 + G 2y + G 2z . The lowest energy state is located at Gx = Gy = Gz = 0 and E = k x2 . The Ek curve follows a parabola and E = 1 at k x = 1. Figure 3.11 shows the lowest three Ek curves along [100]. To continue, using the reduced zone scheme, the next E needs to start at E = 1 (k x = 1) and increase as k x approaches zero. By trial and error, there are two possible G’s that match this condition. However, G(−1, −1, 0) is not selected due to the lack of continuation in the third Brillouin zone and other diffraction directions. The appropriate G’s are (Gx , Gy , Gz ) = (–2, 0, 0), and E = (k x – 2)2 . Started from k x = 1, E = 1, the Ek curve increases toward k x = 0, E = 4.
kz
Fig. 3.10 Brillouin zone of the facecentered cubic lattice. The high symmetry points , L, X, and K correspond to the zone center, 111, 100, and 110 directions, respectively
L (111) X K
(100)
kx
ky
E
Fig. 3.11 Band structure for a free electron in an FCC lattice along [100] and [111] in the first Brillouin zone. For each curve, the selected G’s and degeneracy (in brackets) are indicated
4
3
(–2,0,0) [1]
(–1,–1,–1) [1]
(–1,±1,±1) [4] 2
1
3/4
(0,0,0) [1]
(0,0,0) [1] k
√3/2
0 L
[111]
[100]
1 X
k
74
3 Electronic Band Structures of Solids
The next higher energy level is E = 3 at k x = 0. This energy level matches the second lowest energy state along [111] shown next. This can be calculated by setting (Gx , Gy , Gz ) = (–1, ±1, ±1), which has a fourfold degeneracy. The Ek dispersion relationship is E = (k x – 1)2 + 2. At k x = 1, E = 2, and at k x = 0, E = 3. (b) 111 In the reciprocal lattice of FCC structures, assuming the first Brillouin zone boundary along 100, measured from the zone center , has a length of k max = 1. From the geometry of the Wigner–Seitz √ cell shown in Fig. 3.10, the Brillouin zone boundary along 111 has a length of ( 3/2) k max and k x = k y = k z . The lowest energy
√ isat (Gx , 2 2 2 2 3/2 kmax , Gy , Gz ) = (0,0,0). E = k x +k y +k z = k . At k = 0, E = 0, and at k = E = 3/4.
√ 3/2 kmax . This The next energy level should have an energy of 3/4 at corresponds to a set of (Gx , Gy , Gz ) = (–1, –1, –1). Then
2 E = (k x − 1)2 + k y − 1 + (k z − 1)2
= k x2 + k 2y + k z2 − 2 k x + k y + k z + 3 √ = k 2 − 2 3k + 3
(3.64)
where we recognized that
2
k x + k y + k z = k x2 + k 2y + k z2
+ 2 k x k y + k y k z + k z k x = 3k 2 and kx + k y + kz =
√
3k
(3.65)
According to (3.64), at k = 0, E = 3, and at k = 0.868 k max , E = 3/4. This Ek curve is also shown in Fig. 3.11. One can continue the process along [110] and other major directions of the FCC crystal to complete the Ek diagram shown in Fig. 3.12. In the free electron theory, where the potential induced by the core ions is neglected, the energy band is a continuous parabola. However, the above results indicate that the motion of electrons is not free, but is constrained by the spatial arrangement of the periodic potential associated with the lattices. Nevertheless, in this simple ‘one’ electron model, it allows the Bloch function wave of all energies to extend without attenuation through a crystal.
3.3 Nearly Free Electron Approximation and the Energy Gap
75
Fig. 3.12 Band structure for a free electron in an FCC lattice in the first Brillouin zone. Reprinted with permission from [1], copyright Wiley
3.3 Nearly Free Electron Approximation and the Energy Gap 3.3.1 Origin of Bandgaps The Ek dispersion curve of ‘one’ free electron in a 1D system with a small periodic potential function, equivalent to the lattice constant of semiconductors, can be represented by a parabolic curve centered on a reciprocal lattice point. The possible electron states are not restricted to that single parabola in kspace, but are equally as likely to be found on a parabola shifted by any Gvector as shown in Fig. 3.13. This is due to the periodic property of E, i.e.,
E(k) = E(k + G) = 2 /2m k + G2 Fig. 3.13 Energy bands for an electron in a 1D periodic array of potential with a periodicity of a plotted in the repeatedzone scheme
(3.66)
E
k –4/a
–2/a
0
2/a
4/a
76
3 Electronic Band Structures of Solids
However, when there is only one electron in the system, the electron–electron wave interactions are missing, and the resulting energy band structure shows only the crystal structural property, e.g., as illustrated in Fig. 3.12 for FCC lattices. Of course, in reality, there are extremely large quantities of electrons available in semiconductors. To improve the model, we shall allow more electrons in the crystal lattice such that the electron–electron wave interactions could be included. When an electron wave propagates through the crystal lattice, it gets scattered in all directions from the lattice atoms. Because of the periodic nature of the lattice, in certain directions, waves scattered by many lattice points interfere constructively and a strong scattered beam results. For example, the Bragg condition for an incident wave normal to the crystal plane with a lattice periodicity of a is nλ = 2a or k = nπ /a. The wave vector that fulfills the Bragg condition simply equals one half of the reciprocal lattice vector G, i.e., k = ± G/2. In general, since the scattering from the lattice involves all wave numbers, a plane wave of wave number k and energy E(k) will mix with other electron waves with wave number k + Gn for all n’s. The mixing becomes strong only when the electron waves propagating through the crystal lattice are of equal energy where E(k) = E(k ± G) or k = k ± G or k = ± Gn /2. Again, the Bragg condition for strong reflection occurs at k = ± Gn /2. Therefore, the backscattering becomes very strong, and the electron is unable to propagate through. The forward and back reflected waves establish a standing wave in the crystal. Assuming the contributions from the nearest neighboring waves dominate the resulting waves, the contribution from other reciprocal lattice vectors can be neglected. The wave functions at the edge of the first Brillouin zone at ± G/2 = ±π /a are ψ(+π/a) = A exp(ik · r ) = A exp(i Gz/2)
(3.67a)
ψ(−π/a) = A exp[i(G/2 − G)z] = A exp(−i Gz/2)
(3.67b)
and
The resultant forward (ψ + ) and reflected (ψ – ) plane waves are
ψ+ ∼ exp(i Gz/2) + exp(−i Gz/2) ∼ cos(π z/a) ψ− ∼ exp(i Gz/2) − exp(−i Gz/2) ∼ sin(π z/a)
(3.68)
The corresponding electron probability densities are
ρ+ = ψ+∗ ψ+ ∼ cos2 (π z/a) ρ− = ψ−∗ ψ− ∼ sin2 (π z/a)
(3.69)
As illustrated in Fig. 3.14, the probability density of ψ + (solid curve) peaks at the valleys of the potential energy function, and the associated electrons spend more time at the lower potential region. Thus, electrons associated with ψ + have a lower
3.3 Nearly Free Electron Approximation and the Energy Gap Fig. 3.14 Schematic illustration of the relationship between a electron charge density distribution and b the ion core positions in a 1D lattice
(a)
cos2( z/a)
sin2( z/a)
V(z)
(b) +
77
a +
+
+
+
z
Fig. 3.15 Electronic band structure for a 1D crystal with periodicity a in the nearly free electron approximation. Many electrons are presented. The dashed curve shows the continuous Ek curve of the free electron model
total energy. The peaks of the probability density of ψ – (dashed curve) correspond to the peaks of the potential energy function and have a higher total energy. The degeneracy of the two states, ψ + and ψ – , with different energies at certain wave numbers, breaks the continuity of the parabolic Ek dispersion curve and forms the energy gap (Fig. 3.15). At k = ± nπ/a, the wave functions of the upper and lower boundaries of the energy gap are ψ – and ψ + , respectively. There is no allowed energy value in between ψ + and ψ – at the zone boundary, and an energy bandgap exists in this forbidden region.
3.3.2 Energy Gap—A Quantitative Approach The behavior of the energy bands in the vicinity of the bandgaps can be analyzed by considering the Schrödinger equation for a translational periodic potential energy expressed in terms of Fourier expansion. In a 1D lattice similar to that shown in Fig. 3.14b, the periodic potential with a periodicity a is expressed as V (z) = V (z + a). The Fourier transformation of the symmetric periodic function is
78
3 Electronic Band Structures of Solids
V (z) =
Vn exp(i2nπ z/a)
(3.70)
n
Since V (z) is an even function, by neglecting the sine term, V (z) becomes V (z) ∼ = V0 +
[2Vn (z) cos(2nπ z/a)] n
= V0 + V1 (z) + V2 (z) + · · ·
(3.71)
Further neglecting higherorder terms, the lattice potential function can be represented as V (z) ≈ V0 + V1 (z)
(3.72)
V1 (z) = 2V1 cos(2π z/a) = V1 exp(i2π z/a) + exp(−i2π z/a)
(3.73)
and
where V 1 is a constant. The wave functions of this lattice structure can be expressed as ψ(z) = u(z)exp(ikz). Due to Bragg diffraction at zone boundaries, the incident and reflected waves form constructive interference. At the first Brillouin zone boundary, k = ± π /a, the wave functions are ψ(z) = A1 exp(ikz) + A2 exp(−ikz) = A1 exp(iπ z/a) + A2 exp(−iπ z/a)
(3.74)
where A1 and A2 are constants, and ∂ 2 ψ(z) = −k 2 ψ(z) ∂z 2
(3.75)
Replacing (3.72) and (3.75) in the Schrödinger wave equation 2 ∂ 2 ψ + [E − V (z)]ψ = 0 2m ∂z 2
(3.76)
it becomes −
2 k 2 ψ(z) + E − V0 − V1 (z) ψ(z) = 0 2m
(3.77)
3.3 Nearly Free Electron Approximation and the Energy Gap
79
2 k 2 and using ψ(z) = A1 exp(ikz) + A2 exp(−ikz), the wave Letting E k ≡ 2m equation becomes (E − E k ) A1 exp(ikz) + A2 exp(−ikz) = V0 + V1 (z) A1 exp(ikz) + A2 exp(−ikz)
(3.78)
Regrouping, we have (E − E k − V0 ) A1 exp(ikz) + A2 exp(−ikz) = V1 exp(i2kz) + exp(−i2kz) A1 exp(ikz) + A2 exp(−ikz) = V1 A1 exp(−ikz) + A2 exp(ikz) + A1 exp(i3kz) + A2 exp(−i3kz) (3.79) By neglecting the higherorder terms and comparing exponential terms on each side, we obtain the following two equations as functions of A1 and A2 : (E − E k − V0 )A1 − V1 A2 = 0
(3.80)
−V1 A1 + (E − E k − V0 )A2 = 0
(3.81)
The nontrivial solutions of these equations are when the determinant equals zero, yielding (E − E k − V0 )2 − (−V1 )2 = 0
(3.82)
This second order equation has two energy eigenvalues: E ± = E k + V0 ± V1 at k = ±
π a
(3.83)
The Ek curve at the first Brillouin zone boundary breaks open by a value of 2V 1 with equal amounts above and below the value for the free electron model. Recall that V i is the Fourier coefficient of the small periodic lattice potential. Therefore, as shown in Fig. 3.15, the width of the forbidden energy bands is small compared to that of the allowed bands. Equation (3.83) can be used to calculate the values of A1 and A2 . By replacing E ± into (3.80), we find A1 = A2 for E + and A1 = −A2 for E −
(3.84)
80
3 Electronic Band Structures of Solids
This leads to the solutions of the wave functions in the first Brillouin zone (3.74) as
ψ+ (z) = A exp(ikz) + exp(−ikz) = 2 A cos(π z/a) ψ− (z) = A exp(ikz) − exp(−ikz) = 2i A sin(π z/a)
(3.85)
These are the same qualitative results we obtained in (3.68). The ψ + (z) and ψ – (z) functions near the zone boundary represent two traveling waves of equal amplitude. The interference of these two waves generates two standing waves which represent two different electron distributions with respect to the lattice potential. The difference in potential energy associated with these two standing waves leads to a splitting of the energy bands at the zone boundary as shown in Fig. 3.15. Thus, in the nearly free electron approximation, by considering many electrons propagating through the periodic crystal lattice, bandgaps are formed in the otherwise continuous parabolic energy band.
3.4 The Kronig–Penney Model In the free electron approximation discussed above, the periodic potential energy of the electron was assumed to be small compared to its total energy, and the wave functions for electrons on neighboring atoms overlap heavily. This model led to the energy band structure where the width of the forbidden energy bands was found to be small compared to that of allowed bands. The other important approach, the tightbinding approximation, proceeds from the opposite point of view, where the atoms of the crystal are so far apart that the wave functions for electrons associated with neighboring atoms overlap only to a small extent. Thus the wave functions and allowed energy levels of the crystal will be closely related to the wave functions and energy levels of isolated atoms. The resulting allowed energy bands are narrow in comparison with the forbidden bands. Depending on the particular solid to be studied, we will use the free electron approximation, the tightbinding approximation, or a mixture of the two. Of course, there are very many advanced methods for full calculations of semiconductor energy bands, but the topic is too complex for an adequate treatment in this book. Fortunately, we still can learn some interesting properties about the appearance of energy gaps when an ‘adjustable’ periodic potential is added by studying a simple 1D model suggested by R. de L. Kronig and W. G. Penney. In the Kronig–Penney model, the depth, width, and periodicity of the potential wells can be varied to simulate the environment that electrons will experience under the condition of the nearly free electron model, the tightbinding approximation, or a mixture of the two.
3.4 The Kronig–Penney Model
81
3.4.1 Theoretical Model The Kronig–Penney model uses a simplified rectangular periodic potential energy for a 1D lattice potential as shown in Fig. 3.16. The total interatomic distance is (a + b), of which the potential energy is V 0 over the range b. The onedimensional lattice potential energy function is V (z) =
0, in region I (0 < z < a) V0 , in region II (−b < z < 0)
(3.86)
Using this periodic potential V (z) in the wave equation of the system 2 ∂ 2 ψ + [E − V (z)]ψ = 0 2m ∂z 2
(3.87)
the corresponding solutions are
ψI (z) = A exp iα z + B exp −iα z
ψII (z) = C exp β z + D exp −β z
(3.88)
and
α =
2m E ,β = 2
2m(V0 − E) 2
(3.89)
However, this approach is not suitable for such a potential distribution where the periodic property of the lattice structure is not properly addressed. The Kronig– Penney model incorporates Bloch’s theorem in the wave equation to overcome this problem. Assume the solution of the wave equation has the form of ψ(z) = u(z) exp(ikz).
(3.90)
Fig. 3.16 Onedimensional periodic square well potential energy used in Kronig–Penney model
82
3 Electronic Band Structures of Solids
where k has a real value. Using this in the Schrödinger wave equation, the general form of the wave equation becomes du 2m E 2mV d2 u 2 − k − 2 + 2 u=0 + 2ik dz 2 dz
(3.91)
Equation (3.91) reduces to the following two equations in these two regions: (1) In region I, V = 0:
d2 u I du I 2 + 2ik − k − α 2 u I = 0 and α = dz 2 dz
2m E 2
(3.92)
(2) In region II, V = V 0 :
du II 2 d2 u II − k − β 2 u II = 0 and + 2ik 2 dz dz 2m(E − V0 ) β= 2
(3.93)
Note that β becomes an imaginary number for E < V 0 . These two equations are a differential equation of the form df d2 f + b f = 0 or m 2 + am + b = 0 +a dz 2 dz
(3.94)
The solutions of this equation are f = A exp(m 1 z) + B exp(m 2 z)
(3.95)
This leads to the solutions of the wave equations:
u I (z) = A exp[i(α − k)z] + B exp[−i(α + k)z], 0 < z < a u II (z) = C exp[i(β − k)z] + D exp[−i(β + k)z], −b < z < 0
(3.96)
The factors A, B, C, and D are derived by using the continuity rules at –b, 0, and a. It leads to the following conditions: (i)
At z = 0, u I = u II , A+B =C+D
(3.97)
(α − k)A − (α + k)B = (β − k)C − (β + k)D
(3.98)
(ii) At z = 0, u I = u II ,
3.4 The Kronig–Penney Model
83
(iii) At x = a and –b, u I = u II , A exp[i(α − k)a] + B exp[−i(α + k)a] = C exp[−i(β − k)b] + D exp[i(β + k)b]
(3.99)
(iv) At x = a and –b, u I = u II , (α − k)A exp[i(α − k)a] − (α + k)B exp[−i(α + k)a] = (β − k)C exp[−i(β − k)b] − (β + k)D exp[i(β + k)b]
(3.100)
The coefficients A, B, C, and D can be determined as the solution of a set of four simultaneous linear equations in those quantities. For a nontrivial solution, the determinant of the coefficients must be zero, that is, ⎡
1 ⎢α − k ⎢ ⎣ exp[i(α − k)a] (α − k)ei(α−k)a
1 −(α + k) exp[−i(α + k)a] −(α + k)e−i(α+k)a
−1 −(β + k) − exp[−i(β − k)b] −(β + k)e−i(β−k)b
⎤ −1 ⎥ β +k ⎥=0 − exp[i(β + k)b] ⎦ (β + k)ei(β+k)b (3.101)
Thus, for E > V 0 , after expanding the determinant and rearranging, (3.101) can be expressed as 2 α + β2 sin(αa) sin(βb) + cos(αa) cos(βb) = cos[k(a + b)] − 2αβ
(3.102)
However, in the range 0 < E < V 0 , according to (3.93), β is imaginary. It is common to express (3.102) in a different form. Letting β = iγ = i
2m(V0 − E) 2
(3.103)
in this region and noting that cosh(z) = cos(iz) and isinh(z) = sin(iz), (3.102) can be rewritten as 2 γ − α2 sin(αa)sinh(γ b) + cos(αa)cosh(γ b) = cos[k(a + b)] (3.104) 2αγ We may use (3.102) or (3.104) to find the energy eigenvalues for various periodic lattice potential settings. Nevertheless, since cos(z) on the righthand side has a real value in the range of ± 1, any result of cosk(a + b) larger than one is not a solution.
84
3 Electronic Band Structures of Solids
3.4.2 Analysis Both (3.102) and (3.104) represent a rather involved problem unless we consider some set of simplified conditions. In the following, we shall discuss models with the potential function designed to replicate the nearly free electron approximation or the tightbinding approximation. (a) Nearly free electron model In the limit of the nearly free electron model, the weak periodic potential function is achieved by using the tall but thin barriers in the Kronig–Penney model. We assume that V 0 ≈ ∞, b ≈ 0, and V 0 b remains finite and small. The electron in this model is nearly free except near the extremely thin periodic barriers, which can be easily tunneled through. Under these conditions, for V 0 > E, and lim sinh(γ b) ≈ γ b and lim cosh(γ b) ≈ 1
V0 →∞ b→0
V0 →∞ b→0
(3.105)
Equation (3.104) is reduced to
mV0 b sin(αa) + cos(αa) = cos(ka) ·a 2 αa
(3.106)
It can also be written as a function of energy, sin(αa) + cos(αa) = cos(ka) f (E) = P αa
(3.107)
where P=
m(V0 b)a ∝ (V0 b)a 2
(3.108)
is a measure of the ‘effective area’ of each periodic barrier. The lefthand side of (3.107) is clearly a function of α which √ is proportional √ to E. Therefore, we can plot f (E) in (3.107) as a function of E and impose a limit of –1 ≤ f (E) ≤ 1 to yield the allowed solutions shown in Fig. 3.17. We note that the ordinate is (1 + P) for α = 0, where sin(αa) ≈ αa, and it is ±1 for α equal to any multiple of (π /a), regardless of the value of P. The left side of (3.107) contains a [sin(αa)]/ (αa) term, which is a sinc function, with the same periodicity and phase as cos(αa). Since the amplitude of the sinc function decreases quickly with increasing α, its contribution diminishes after a few periods. Therefore, for a small P, the resultant f (E) has a shape similar to cos(αa) beyond several times of (π /a). Note that, consistent with our earlier discussions of the free electron model, the forbidden bands are narrower than the allowed energy bands.
3.4 The Kronig–Penney Model
85
Fig. 3.17 Plot of the left side of (3.107) for P = 2 as a function of α. The allowed states are located within 1 ≥ f (E) ≥ –1, and the shaded areas are the forbidden regions
In the following, we shall discuss two extreme cases of the nearly free electron model. (i) Case I: P → ∞ Since P is a product of (V 0 b) and a, where (V 0 b) is finite and small, an infinite P means that the lattice constant (a+b) is near infinity. This is equivalent to the case of discrete atoms. In the range of –1 ≤ f (E) ≤ 1, the only possible solution of (3.107) is when sin(αa) ≈ 0 or αa = ± nπ for n = 1, 2, 3, … We can deduce the allowed energy states as nπ = α=± a
2m E 2
(3.109)
or E=
2 nπ 2 n = 1, 2, 3, . . . 2m a
(3.110)
The allowed E’s are discrete levels as seen in an isolated atom. (ii) Case II: P → 0 Since (V 0 b) is a small and finite, the condition of P approaching zero implies that the lattice constant (a + b) is also near zero. The electron wave functions can easily tunnel through the thin barriers and act like a pool of free electrons. The solution (3.107) reduces to cos(αa) = cos(ka) or
(3.111)
86
3 Electronic Band Structures of Solids
α=k=
2m E 2
(3.112)
Therefore, E = 2 k 2 /2m, and the allowed energy states form a continuous band. (b) Tightbinding approximation This approach takes a point of view opposite to that of free electron model. It is based on the assumption that the atoms of the crystal are so far apart that the wave functions for neighboring electrons overlap only to a small extent. If we keep V 0 and a fixed and vary d = (a + b), we see that as b becomes large, sinh(γ b) ≈ cosh(γ b) ≈ exp(γ b)/2.
(3.113)
Thus the general solution of the Kronig–Penney model becomes
γ 2 − α2 2αγ
sin(αa) + cos(αa)
exp(γ b) = cos[k(a + b)] 2
(3.114)
Since b is a large number and both b and γ are positive, it is clear that cos[k(a + b)] ≤1 only if
γ 2 − α2 2αγ
sin(αa) + cos(αa) = 0
(3.115)
2αγ − γ2
(3.116)
(αa)tan(αa) ∼ = γ a
(3.117)
or tan(αa) ≈
α2
This equation has an equivalent form of
for V 0 > E, where γ is a function of α and γ . This expression is similar to the solution of an isolated finite depth quantum well with a well depth of V 0 and a width of 2a. This implies that the allowed energy bands are very narrow in the tightbinding approximation, which leads to a nearly linear relationship between f (E) and E in each allowed narrow energy band. However, as shown in Fig. 3.18, the solution (3.115) still maintains the shape of a sinc function. We know that in a twodimensional system, the line equation of a linear function between point 1 at (x 1 , y1 ) and point 2 at (x 2 , y2 ) can be written as y − y1 y2 − y1 = x − x1 x2 − x1
(3.118)
3.4 The Kronig–Penney Model
87
Fig. 3.18 Plot of the left side of (3.115) as a function of α. The allowed states are located within 1 ≥ f (E) ≥ –1, and the shaded areas are the forbidden regions. The allowed energy bands are between E 1 and E 2 , E 3 and E 4 , E 5 and E 6 , etc
We can apply (3.118) to derive the allowed energy states. In the lowest (first) allowed energy band, between E 1 and E 2 , the line equation can be expressed as f (E) − f (E 1 ) f (E 2 ) − f (E 1 ) = E − E1 E2 − E1
(3.119)
For the allowed energy states, f (E 1 ) = f (E 4 ) = f (E 5 ) = f (E 8 ) = · · · = +1, f (E 2 ) = f (E 3 ) = f (E 6 ) = f (E 7 ) = · · · = –1, and f (E) = cos[k(a + b)], which lead to the following results. In the first allowed energy band, according to (3.119),
E − E1 cos[k(a + b)] − 1 = −2 E2 − E1
(3.120)
If we assume the first allowed energy band width is E 1 = E 2 − E 1
(3.121)
then (3.120) can be expressed in terms of E 1 as E = E1 +
E 1 {1 − cos[k(a + b)]} 2
(3.122)
The result of (3.122) is plotted in Fig. 3.19a. Note that, in contrast to the free electron theory, the minimum allowed energy state is a nonzero value. The second allowed energy band is between f (E 3 ) = –1 and f (E 4 ) = +1. The line equation has the form of cos[k(a + b)] + 1 = 2
E − E3 E4 − E3
(3.123)
88
3 Electronic Band Structures of Solids
Fig. 3.19 Plot of the Ek curve of the a first and b second allowed energy bands using tightbinding approximation
(a)
E
E2 E1 E1 – /d
0
(b)
E
k
/d
E4 E2 E3 0
– /d
/d
k
This is rearranged below to show the allowed energy function. E = E3 +
E 2 {1 + cos[k(a + b)]} 2
(3.124)
where E 2 = E 4 – E 3 . This cosine function (3.124) is plotted in Fig. 3.19b. Using this process for higher energy bands, we can construct the complete energy band diagram. In Fig. 3.20, we note that there are discontinuities at k = ±nπ /a, where energy gaps exist. The minimum allowed energy state is not zero and has a finite value. At higher energies, the allowed states become wider.
3.5 Effective Mass Before we move on to examine the realistic energy band structure of common semiconductors, let us now consider the motion of an electron in the crystal under the influence of an applied electric field. First, if the Bloch function uk (z) in (3.39) is set to be a constant, then the wave function has the form of exp(±ikz), corresponding to a perfectly free electron of momentum p = èk whose energy would be E=
2 k 2 2m
(3.125)
3.5 Effective Mass
89
Fig. 3.20 Plot of the Ek curve according to the tightbinding approximation (solid curves) compared with the free electron mode (longdashed curves). The reduced zone representation is plotted as shortdashed curves
where k is a propagation constant. This relation is shown as the longdashed curve in Fig. 3.20. Under this condition, p = èk is the crystal momentum and has a value close to the real momentum of a moving particle. However, in a real crystal, the nonzero periodic potential function leads to discontinuities in the Ek curve at k = ±nπ /d. The true instantaneous momentum of an electron is no longer a constant of the motion, while the crystal momentum èk is a perfectly welldefined constant value for a given energy state. Since there exist allowed wave functions with different k’s, we shall use the group velocity to relate the electron ‘wave packet’ following υg =
1 dE dω = dk dk
(3.126)
where E = èω. Again, this equation shows that the instantaneous momentum of the traveling electrons at the Brillouin zone boundaries is no longer a constant of the motion. Suppose an electric field F is applied such that, over a distance dz in a period dt, the group velocity of the electron increases by dυ g . The rate of change of electron energy due to the applied field is dE = −q Fdx = −q Fυg dt
(3.127)
Then, using (3.126) and (3.127) we see that dE =
q F dE dE dk = − dt dk dk
(3.128)
qF dt
(3.129)
Therefore, dk = −
90
3 Electronic Band Structures of Solids
or
dp dk = = −q F = F dt dt
(3.130)
where p is the crystal momentum. Equation (3.130) indicates simply that the time rate of change of crystal momentum equals the force, F. Thus it is the analogue of Newton’s law, showing that the crystal momentum of the electron in a periodic lattice changes under the influence of an applied electric field in the same way as does the true momentum of a free electron in free space. Differentiating (3.126) with respect to time, the result is dυg 1 d = dt dt
dE dk
1 d2 E dk 2
=
dk dt
=
dk 1 d2 E 2 dk 2 dt
(3.131)
Using (3.130), the magnitude of acceleration a can be written as a=
dυg dk 1 d2 E F = 2 2 = ∗ dt dk dt m
(3.132)
where the effective mass m* is defined as m∗ ≡
2
d2 E/dk 2
(3.133)
or ∗
m =
1 ∂2 E 2 ∂ki ∂k j
−1 (3.134)
for the nonspherical constant energy surface case. We can check this concept in a free electron system with mass m0 where E=
2 k d2 E 2 2 k 2 dE = , , and = 2m 0 dk m0 dk 2 m0
Then the effective mass simply equals the free electron mass as expected, i.e., 2
= m0 m∗ = 2 d E/dk 2
(3.135)
To further illustrate the relationship between the Ek curve, group velocity, and m*, a tightbinding limit model is used for two specific simple E(k) variations in Fig. 3.21.
3.5 Effective Mass
91
(a)
– /d
(b)
(c)
(d)
E(k)
0
/d
k
– /d
E(k)
0
(e)
g
m*
(f)
/d
k
g
m*
Fig. 3.21 Variation of a, d electron energy, b, e electron velocity, and c, f effective mass with reduced wave vector for states in a band of onedimensional crystal. The Ek curve is a cosine function for the left panel, and in the form of (1 + coska) for the right panel
Assume, in one case, that E = (E/2)(1 − cos kd)
(3.136)
It represents the Ek dispersion curve of the lowest band, where E is the allowed energy bandwidth. Under an applied electric field, the group velocity and effective mass are calculated as dE 1 dE = sin kd (3.137) υg = dk 2 and 22 2
= 2 seckd m∗ = 2 d E d E/dk 2
(3.138)
As shown in Fig. 3.21b, the resultant group velocity is not a constant within the first Brillouin zone. Rather, it oscillates from zero to a maximum, then going through a minimum and back up to maximum again. Since the zone boundaries ±π/d are equivalent using the periodicity of kspace, the zero velocity at the zone boundaries corresponds to the standing wave nature of the electron waves due to Bragg reflections. Furthermore,
92
3 Electronic Band Structures of Solids
x(t) =
q Ftd E 1 − cos 2q F E = (1 − cos kd) 2q F
υg (t)dt =
(3.139)
where k = (qFt)/è. The results of (3.137) and (3.139) show that electrons oscillate in both k and real space, rather than accelerating uniformly as they would do the absence of a periodic potential. This velocity oscillation is equivalent to a mass change at critical points in kspace shown in Fig. 3.21c. The electron mass has a constant positive value near the zone center but becomes negative on the zone boundary. One unusual property of the effective mass is that at wave vectors corresponding to the maximum and minimum velocities, the effective mass goes to infinite. This marks the point where a deceleration must begin to slow down the electron. The other peculiar property is that the effective mass has regions in which it is negative. A negative m* means that the acceleration resulting from the externally applied electric field is in a direction opposite to that of the applied field; this is the effect of electron reflection due to the periodic crystal lattice. In the second tightbinding limit model, as shown in Fig. 3.21d, the E(k) variation can be represented by
E = E /2 (1 + cos kd)
(3.140)
It resembles the Ek curve of the valence band in a semiconductor with an allowed energy bandwidth of E. By the same procedures, we can derive the group velocity and effective mass as displayed in Fig. 3.21e, f, respectively. The Ek dispersion curve shown in Fig. 3.21a is very much like the conduction band edge of a direct bandgap semiconductor such as GaAs. We shall use it to discuss some properties related to semiconductor materials. Since the electron effective mass is a function of k within the first Brillouin zone, what value of k should be used for determining m*? Ideally, in a perfect crystal, under the influence of an applied electric field, the electron takes a periodic motion indefinitely within the first Brillouin zone as described by (3.137) and (3.139). This is known as the Bloch oscillation with a frequency ω = qFd/è, and there have been many attempts to observe and utilize it as a possible terahertz (THz) radiation source. However, all attempts to observe Bloch oscillation in conventional bulk solids have failed. For all reasonable applied fields, the Bloch oscillation is destroyed by scattering with impurities, defects, and phonons, before a single oscillation cycle is completed. The existence of such periodic oscillations in THz (1 THz = 1012 Hz) range was finally experimentally observed in 1993 in a semiconductor superlattice structure [2]. The multiple periods of GaAs/AlGaAs thin layers form superlattices that have a lattice periodicity much larger than the lattice constant of GaAs. This large lattice periodicity reduces the width of the Brillouin zone in kspace such that the scattering loss is suppressed. Therefore, in real semiconductors, the electron only travels a short range of the
3.5 Effective Mass
93
periodic Ek curve due to scattering events. The two dominant scattering processes are phonon scattering due to lattice vibration, and impurity and defect scattering. In high quality semiconductor materials, phonon scattering dominates the carrier relaxation process near room temperature and above. Through these processes, an electron can lose its energy quickly and move to the zone center of the Ek curve where the potential energy is the lowest. Near the zone center, the energy can be approximated by a parabolic function of k or E = A(k – k 0 )2 . The effective mass has a constant value of m* = è2 /2A, and the dynamical behavior of the electron will be the same as that of a free particle with this effective mass. For indirect bandgap semiconductors like Si and Ge, although the minimum conduction band edge is not located at the point, the energy is still a parabolic function of k. The effective mass will also be a constant similar to that of the direct bandgap material.
3.6 Band Structures of Common Semiconductors The introduction of the lattice influence in terms of a small periodic potential function in a 1D nearly free electron system leads to the development of the energy bandgap concept. When we move from the 1D to the 3D nearly free electron system incorporating the effect of a small periodic potential, we encounter not only the increased dimension but also new possibilities that arise with the availability of more dimensions. For example, for an electron moving through a 3D crystal, an energy bandgap in one kdirection may be bridged by an allowed band in another kdirection. This possibility of the 3D system gives rise to the existence of overlapping bands, which is not possible in a 1D system. Typical energy bands for a diamond structure crystal are shown in Fig. 3.22. These Ek curves may be compared with the empty lattice model of a FCC crystal given in Fig. 3.12.
3.6.1 General Trend of Energy Band Structure in Semiconductors The tetrahedral bonds of diamond and zincblende semiconductor structures are derived from the sp3 hybrid orbit. By linear combination of spherically symmetric slike waves with three directional plike waves, as expressed in (2.24), four sp3 hybrids are produced. These four sp3 hybrid orbitals form a tetrahedron bond structure, which is the basic arrangement of all semiconductor crystals. Figure 3.23 shows schematically the evolution of the s and plike atomic states to the conduction and valence bands in hybridized elemental semiconductor systems. Atomic s and pstates are hybridized to form sp3 hybrid bonds which then can form bonding and antibonding combinations between orbitals on neighboring atoms pointing along the common bond. Finally, these molecular orbitals associated with bonding and
94
3 Electronic Band Structures of Solids
Fig. 3.22 Typical energy bands for a diamondlike crystal structure. Reprinted with permission from [3], copyright Wiley
antibonding levels become broadened into bands by interactions between hybrid orbitals on the same atom, the valence band being formed from bonding orbitals and the conduction band from antibonding orbitals. Therefore, the states are purely slike or plike. At the zone center ( point), the bottom of the valence band is therefore slike, and the top is plike and triply degenerated when spinorbit coupling is neglected. Similarly, at point, the bottom of the conduction band is purely slike. The development of the energy band structure for a polar (compound) semiconductor proceeds in the same way. Hybrids are formed on both atom types and then form bonding and antibonding states with the other hybrid in the bond. Finally, the valence and conduction bands are formed from the broadened bonding and antibonding levels. Using Ge as an example, the true energy bands and the nearly free electron bands are compared in Fig. 3.24. The true bands are obtained by combining pseudopotential calculations with experimental optical measurement data. The nearly free electronlike bands in Fig. 3.24b are remarkably similar to those at the bottom of the valence band and the upper part of the conduction band of the ‘true’ band structure (Fig. 3.24a), except that bandgaps at certain critical points in the Brillouin zone do not occur in the nearly free electron band structure. The other feature displayed in Fig. 3.24 is that Ge is an indirect bandgap semiconductor. Its maximum of the valence band is located at , and the minima in the conduction band are located
3.6 Band Structures of Common Semiconductors
95
Fig. 3.23 Development of energy band structure of silicon. The single sstates (E s ) and pstates (E p ) on each atom are transformed to four hybrid states (E h ), which are combined with neighboring hybrids to form bonds. The bonding (E b ) and antibonding (E a ) levels finally broaden into energy bands in the crystal
Fig. 3.24 Energy bands of germanium. a Energy band obtained by pseudopotential calculations. Reprinted with permission from [4], copyright American Physical Society, b energy band calculated using the nearly free electron model
96
3 Electronic Band Structures of Solids
in the 111 directions at the Lpoint. On the other hand, GaAs is a direct bandgap semiconductor with both the maximum of the valence band and the minimum of the conduction band located at the point. Therefore, it is instructive to examine the trends in the band structures of tetrahedrally bonded semiconductors, specifically the III–V compounds exhibiting mixed ioniccovalent bonding. For group IV elements, there is an increase in metallic tendency (metallicity) on going from C to Sn when increasing the atomic number. With increasing metallicity, as expected, the conduction band minimum at the point drops faster than at X or L. At some point, the semiconductor turns into direct bandgap material. Indeed the indirect bandgaps of diamond, silicon and germanium turn into direct in αSn. This trend is also true for III–V compounds. The lowest conduction band drops more quickly at the point than at X or L with increasing metallicity, so the III–V compounds become direct bandgap semiconductors. The Alcompounds and GaP are the exceptions with indirect bandgaps. The energy band structures of Si and GaAs are shown in Fig. 3.25. On the other hand, for III–V compounds, there is an increase in ionicity which has a tendency to increase the bandgap energy. For example, the III–V nitride compounds with wurtzite crystal structure have bandgap energies much larger than 2 eV.
Fig. 3.25 Detailed energy band structures of a Si and b GaAs. Reprinted with permission from [4], copyright American Physical Society
3.6 Band Structures of Common Semiconductors
97
3.6.2 Valence Band Consider the pz orbit in a cubic crystal. As shown in Fig. 3.26a, the wave functions are polarized along the zdirection. Electrons move easily along the zdirection. This corresponds to a light effective mass shown as the Ek curve with a small radius of curvature (Fig. 3.26b). On the other hand, electrons moving in x and ydirections are very restricted and have a heavy effective mass, shown as the slow varying Ek curve. The same property can be said about px  and py like orbits. The combined 3D Ek diagram of the valence band turns out to be a complex composition. As shown in Fig. 3.27, there are heavyhole, lighthole, and splitoff bands. The maximum of the heavy and lighthole bands degenerate at k = 0. Away from the point, the heavyand lighthole bands with different radii of curvature in the Ek curve result. Near the zone center, they can be described as E(k) = E v −
2 k 2 2m 0 m h
(3.141)
where mh equals mhh or mlh for heavy holes or light holes, respectively. Although widely used for its simplicity and convenience, it must be stressed that this approximation is valid only near the vicinity of the zone center. In realistic situations, the bands are both nonparabolic and anisotropic, depending on the direction of k as (a)
Easy travel direction
pz
x y
z
Fig. 3.26 Valence band constructed from pz orbitals. a Regular arrangement of pz orbitals. b Ek curves of pz orbitals only; the band is ‘light’ along k z and ‘heavy’ along k x or k y
Fig. 3.27 Total band structure at the top of the valence band for tetrahedral semiconductors
98
3 Electronic Band Structures of Solids
well as its location from the zone center. The simple spherical surfaces predicted by (3.141) are modified into complex warped spheres. The nonspherical hole dispersion relation near the zone center can be described by Luttinger parameters. The situation becomes even worse if the cubic symmetry is broken by introducing strain in the material. The decoupling of the spinorbit splitoff band from the top of the valence band is caused by the interaction of the electron spins (s = ±1/2) of the valence electrons with the magnetic moment (l = 1 for pstate) arising from their orbital motion, which yield a total angular momentum j = l + s = 3/2 and 1/2. The separation between the top of the heavy/lighthole bands and the spinorbit splitoff band, so , increases with atomic number, essentially because the greater the nuclear charge, the greater the internal magnetic field experienced by the orbiting electron. Thus, so is very small for Si (0.04 eV), fairly large for GaAs (0.34 eV), and quite large for InSb (0.81 eV).
3.6.3 Conduction Band (a) Direct bandgap materials The conduction band originates from slike orbitals which have a spherical symmetry. For III–V compounds such as GaAs, the conduction band minimum is located at the zone center ( point), and these are called direct bandgap semiconductors. Near the conduction band minimum, the band can be described by E(k) = E c +
2 k 2 2m 0 m e
(3.142)
Thus the constant energy surface of the conduction band has a spherical shape. For direct bandgap semiconductors, the radius of the Ek curve of the lowest conduction band is relatively small, leading to a light electron effective mass. In GaAs, m ∗e ∼ = 0.063m0 is the electron effective mass. (b) Indirect bandgap materials For indirect bandgap semiconductors, the shape of the lowest conduction band minimum is more complex. In Si (and diamond), the minima are located along 100 about 85% of the way to the Xzone boundary. As illustrated in Fig. 3.28, there are six directions and, therefore, six equivalent minima in a cubic crystal. Due to their offcenter location, these minima (valleys) have anisotropic Ek relationships along k x , k y , and k z . k 2y k z2 2 (k x − k0 )2 E(k) = E c + + + 2m 0 mL mT mT
(3.143)
3.6 Band Structures of Common Semiconductors
99
Fig. 3.28 a The Brillouin zone of Si with six equivalent constant energy surfaces along direction. b Enlarged view of one of the constant energy volumes, showing longitudinal and doubly degenerated transverse masses mL and mT , respectively
Fig. 3.29 Brillouin zone of Ge with constant energy surfaces for the eight equivalent Lvalleys
where the subscripts L and T indicate longitudinal and transverse components, respectively. In Si, mL = 0.92 and mT = 0.19. As mentioned earlier, Ge also has indirect bandgap with the conduction band minima along 111 in the Lpoint. In Ge, as shown in Fig. 3.29, there are eight ellipsoidal equivalent valleys located at the zone boundaries where mL = 1.59 and mT = 0.082. Since only half of the constant energy surface is located inside the first Brillouin zone, the degenerate factor g is 4, not 8.
3.6.4 Band Structures of Wurtzite Crystals Although the crystal structure of most III–V compounds is zincblende, the IIInitride alloys prefer the formation of wurtzite crystal structure. Since both structures are characterized by the tetrahedral lattice arrangement, as discussed in Sect. 2.4, the nearestneighbor environments are identical with only slight differences in the next nearestneighbor arrangements. It is necessary to go beyond next nearest neighbors before both positional and directional differences occur. One can regard the wurtzite
100
3 Electronic Band Structures of Solids
structure along the caxis as a cubic zincblende lattice slightly deformed along the body diagonal of [111]. Figure 3.30 compares the Brillouin zone of zincblende and wurtzite crystal structures. A correspondence is obtained between the [111] direction L in zincblende structure and the [0001] direction in wurtzite. Therefore, a strong similarity between the band structure of zincblende and wurtzite crystals can be expected. However, in contrast to the more symmetric cubic zincblende crystal, the inplane (basal plane) behavior of the energy bands is different from the behavior along the [0001] axis (the caxis) in wurtzite crystal. The anisotropic hexagonal structure, when including spinorbit interaction, leads to energy splitting in the valence band edges. The valence band structure for GaN is shown in Fig. 3.31. The heavyhole (HH) and lighthole (LH) bands no longer degenerate at k = 0 and separated by the spinorbit interaction (so ). The crystalhole (CH) valence band
Fig. 3.30 Brillouin zone of zincblende and wurtzitetype materials. Reprinted with permission from [5], copyright American Physical Society
Fig. 3.31 Valence band structure of wurtzite GaN. Reprinted with permission from [6], copyright AIP Publishing
3.6 Band Structures of Common Semiconductors
101
results from the crystalfield splitting energy (cr ). The topmost three valence band energy levels at k = 0 (E 1 , E 2 , and E 3 , in decreasing order) are E 1 = 1 + 2
E2 =
E3 =
1 − 2 +
(1 − 2 )2 + 823 2
1 − 2 −
(1 − 2 )2 + 823 2
(3.144a)
(3.144b)
(3.144c)
where E 1 is labeled as HH band, E 2 is labeled as LH band, and E 3 is labeled as CH band. We also assumed 1 = cr , 2 = 3 = so
(3.145)
In general, cr and so have positive values for IIInitrides except that AlN has a negative cr . Thus, the top valence band of AlN is E 2 instead, and the valence bands from top to bottom are CH, HH, and LH, respectively. Note that the valence band energy splitting E 1 – E 2 and E 1 – E 3 are measurable quantities through interband optical transition measurements whereas cr and so are parameters of theory, obtainable indirectly by fitting experimental energy splitting. All IIInitride semiconductor alloys have direct bandgaps. The bottom of the conduction band in GaN and InN is well approximated by a parabolic dispersion relationship, while a greater anisotropy in AlN than GaN is predicted due to the reduced lattice symmetry. The conduction bandedge energy is deduced by adding the bandgap energy to E 1 . E c = E g + 1 + 2
(3.146)
Problems 1. Calculate the first two Ek curves along the [110] axis for a BCC crystal using the 3D free electron model. 2. For an artificial twodimensional square lattice structure shown below, calculate the first two energy bands for free electrons along the X, XK, and K directions.
102
3 Electronic Band Structures of Solids
3. Calculate and plot the density of states as a function of energy in the conduction band of a GaAs/AlGaAs quantum well for the first three bound states located at 25, 100, and 225 meV above the conduction band edge. The electron effective mass of GaAs in the conduction band is m* = 0.067m0 . 4. Derive the density of states for a quantum dot system. In a quantum dot system, the quantum confinement is threedimensional. 5. Suppose the Ek relation is given by E = E 0 + (E/2)(1 − cos ka). For very small k. prove that the parabolic approximation holds and determines the effective mass. 6. For the delta function periodic potential (V 0 ~ ∞, b ~ 0 and V 0 b is small but finite or P 1), use the Kronig–Penney model to calculate (a) The energy of the lowest energy band at k = 0. (b) The bandgap at k = π /a. 7. Derive the following solution of the Kronig–Penney model for a crystal: 2 α + β2 − sin(αa) sin(βb) + cos(αa) cos(βb) = cos[k(a + b)] 2αβ by setting the determinant of wave functions (3.101) to zero. 8. Consider a simple cosine approximation to the shape of an energy band as E(k) =
E (1 − cos ka). 2
(a) For small k, prove that the parabolic approximation holds and υ(k) ∼ = k/m ∗ . (b) Many semiconductors have a saturation velocity for electrons of around 107 cm/s. How much of the first Brillouin zone do electrons need to explore to reach this velocity? Assume the initial position of electrons is at the zone center. For calculations, use the velocity equation of part (a) and the following material parameters of GaAs: m* = 0.067m0 and lattice constant a0 = 5.653 Å. 9. Consider a single electron in a perfect crystal. Starting from k = 0 in an empty band, the electron is accelerated by a constant electric field –F toward +k. Assume E = (E/2)(1 − cos ka) and k = (q F)t = Ft. (a) Find the velocity of the electron. (b) Prove that the position of the electron in real space as a function of time is q Fa E 1 − cos t x(t) = 2q F
3.6 Band Structures of Common Semiconductors
103
The electron oscillates in real space, rather than accelerating uniformly as in the free electron model. This periodic motion of an electron in a periodic crystal structure is called the Bloch oscillation. (c) The Bloch oscillation frequency is ω = q Fa/. For F = 108 V/m, calculate the Bloch oscillation frequency in GaAs. (d) In semiconductors, due to scattering with defects, the Bloch oscillation of electrons in the Brillouin zone cannot be observed. Assuming the average electron can only travel one tenth of the first Brillouin zone, design a GaAs/AlAs superlattice structure such that the Bloch oscillation can be measured. The lattice constants of GaAs and AlAs are 5.653 Å and 5.660 Å, respectively.
References 1. F. Herman, in An Atomistic Approach to the Nature and Properties of Materials, ed. by J.A. Pask (Wiley, New York, 1967) 2. C. Waschke, H.G. Roskos, R. Schwedler, K. Leo, H. Kurz, K. Kohler, Phys. Rev. Lett. 70, 3319 (1993) 3. D. Long, Energy Bands in Semiconductors (WileyInterscience, New York, 1968) 4. J.P. Chelikowsky, M.L. Cohen, Phys. Rev. B14, 556 (1976) 5. J.L. Birman, Phys. Rev. 115, 1493 (1959) 6. I. Vurgaftman, J.R. Meyer, J. Appl. Phys. 94, 3675 (2003)
Further Reading 1. C. Kittel, Introduction to Solid State Physics, 6th edn. (John Wiley & Sons, 1986) 2. H. Ibach, H. Lüth, Solid State Physics, 2nd edn. (Springer, 1996) 3. W.A. Harrison, Elementary Electronic Structures (World Scientific, 1999)
Chapter 4
Compound Semiconductor Crystals
Abstract As we learned from previous chapters, silicon has a diamond crystal structure with pure covalent bonding. Due to its nature as a single element, the Si crystal structure is highly symmetric. Since there are two different elements in binary III– V compounds, the basic diamond structure turns into zincblende crystal structure, which destroys some of the symmetry observed in Si. This lower symmetry in crystal structure leads to band structures with different features which, in turn, give the unique properties not available to Si. Using GaAs as an example, the main advantages over Si are (a) Larger bandgap: The larger bandgap leads to a low intrinsic carrier concentration (ni ) suitable for hightemperature operation. (b) Smaller effective mass: The effective mass is inversely proportional to the carrier mobility. The higher mobility contributes to highspeed operation. (c) Direct bandgap: The location of the lowest conduction band minimum also varies with a decreasing degree of crystal symmetry in III–V compounds. Some of them have both the conduction band minimum and the valence band maximum located at the zone center. These are called direct bandgap semiconductors. This allows for their use in photonic device and transfer electron device applications. (d) Heterostructures: Additionally, binary III–V compounds can form ternary and quaternary compounds, which leads to an expanded selection of lattice constants and bandgap energies. New heterostructure and quantum effect devices then become possible. In this chapter, the basic structural, transport, doping, and surface properties of III–V binaries are introduced first. The variation of lattice constant and energy gap in ternary and quaternary alloys are discussed next.
The history of preparation of III–V compounds goes back to the late nineteenth century. Since no naturally occurring III–V crystals have been found, the early work was to prepare these compounds. During the early twentieth century, before WWII, a wide range of the compounds, such as AlSb, AlN, AlP, AlAs, InP, InAs, InSb, and GaN, was studied for their crystal chemistry and structure without realizing the semiconducting nature of these compounds. After the war, work continued in both Russia and the Western world. In 1950, N. A. Goryunova, a Ph.D. student at Leningrad State University, came to the conclusion that compounds with the zincblende structure are not only structural analogs of group IV elements, but they are © Springer Nature Switzerland AG 2020 K. Y. Cheng, III–V Compound Semiconductors and Devices, Graduate Texts in Physics, https://doi.org/10.1007/9783030519032_4
105
106
4 Compound Semiconductor Crystals
also semiconductors. She substantiated the idea with exploratory experiments and reported the results in her Ph.D. thesis in 1951. These ideas are contained in a summary of intermetallic compounds reported by A. F. Ioffe, where he pointed out that InSb, HgSe, and HgTe are semiconductors like silicon. Ioffe’s work was included in papers by A. I. Blum, N. P. Mokrovski, and A. R. Ragel [1]. At about the same time, in 1952, H. Welker in West Germany published his classical paper on new semiconducting compounds, including the important III–V compound semiconductor GaAs and applied for patents on III–V compound semiconductor devices and their method of manufacturing [2]. He was recognized in the Western world as the pioneer of III–V compound semiconductors. In the USA, the first discussion of the unique properties of III–V compound semiconductors was held at the American Physical Society March Meeting at Durham, North Carolina, in 1953. The materials discussed at this meeting were mainly Sbrelated compounds, e.g., InSb and AlSb. Research on III–V compounds got more attention after the demonstration of semiconductor injection lasers in 1962 and the discovery of coherent microwave oscillation in transfer electron devices in 1963. These important early inventions precisely highlight the strength of III–V compound semiconductors over silicon—their lightemitting and highspeed properties.
4.1 Structural Properties 4.1.1 Lattice Constant The lattice constant of a III–V compound zincblende crystal can be estimated by using the tetrahedron covalent radii defined by L. Pauling. Assuming the atoms pack in as hard spheres, the lattice constant (a) is simply related to the tetrahedron covalent radii (r III and r V ) by 4 a = √ (rIII + rV ) 3
(4.1)
For all III–V compounds, except AlSb, as shown in Table 4.1, the error between the calculated and experimental results is less than 1%. Although this is a remarkably close fit, the accuracy is not good enough for predicting lattice constants of new compounds. In heterostructures, a latticemismatch of ≤0.1% is required to avoid the formation of misfit dislocations. In most III–V compounds, this tolerance is less than 0.0005 Å. Therefore, we have to rely on experimental lattice constant values. For IIInitride compounds, their crystal structure is wurtzite. The lattice constants a and c are related to the tetrahedron covalent radii by √ 8 2 2 a = √ (rIII + rV ) and c = (rIII + rV ) 3 3
(4.2)
4.1 Structural Properties
107
Table 4.1 Measured lattice constant (in Å) of III–V compounds as compared to calculated values from covalent radii (value in parenthesis) of each pair of III and V elements rV P (1.10Å)
As (1.18Å)
Sb (1.36Å)
N (0.70Å)
r III
Cal.
Exp.
Cal.
Exp.
Cal.
Exp.
Cal.
Exp.
Al (1.26Å)
5.450
5.464
5.635
5.660
6.051
6.136
a: 3.20 c: 5.227
a: 3.112 c: 4.982
Ga (1.26Å)
5.450
5.451
5.635
5.653
6.051
6.096
a: 3.20 c: 5.227
a: 3.189 c: 5.185
In (1.44Å)
5.866
5.869
6.051
6.058
6.466
6.479
a: 3.495 c: 5.706
a: 3.54 c: 5.70
For nitride compounds, a and c indicate the lattice constants in the (0001) plane and along the caxis, respectively
4.1.2 Cleavage Properties The side views and 3D structures of a zincblende crystal along the [111], [110], and [100] directions are shown in Fig. 4.1. For silicon, the cleavage plane is in {111} due to its slightly larger separation between the two planes. For compound semiconductors, {111} is not the favored cleavage plane. This is because the two opposite surfaces [111]
[100]
[110]
d d/ 3
[001]
3d/2
0] [01
[100] Fig. 4.1 (Top row) Side views of bond structures of (111), (110), and (100) surfaces of a zincblende crystal. The dashed line indicates a plane parallel to the surface and d is the bond length. The thicker lines in (111) side view represent double bonds. (Second row) The 3D structures of [111], [110], and [100] planes in zincblende structure. The shaded plane corresponds to the dashed line in the top panel
108
4 Compound Semiconductor Crystals
are filled with different atoms where an electrostatic attraction force is formed upon cleaving. The (111) surface occupied by group III atoms is called the (111)A surface. The one filled with group V atoms is the (111)B surface. Because of this chemical difference, these two surfaces show very different characteristics in etching and epitaxial growth processes. On each side of the (110) cleaved plane, there are equal numbers of group III and group V atoms. Because there is no electrostatic attraction between the two sides, this is the easy cleavage plane among III–V compounds. The atoms on the [100] plane have double bonds and have the strongest bonding among three directions discussed here.
4.1.3 Lattice Vibration—Phonons The vibration of crystal lattice at a finite temperature is represented, in quantum mechanics, by phonons. As discussed in Sect. 2.5 and in later sections, phonon scattering due to lattice vibration plays a critical role in the carrier relaxation process, which determines many important basic properties of the semiconductor including effective mass, carrier recombination, and thermal conductivity, etc. The periodicity of the lattice means that phonons have band structure in much the same way as electrons, as discussed later in this section. The crystal lattice can be visualized as an array of point masses connected by springs. The masses are just the core ions. The length of the spring can be seen as the equilibrium bond length. It resists any attempt to change its length. The force between the neighboring atoms linked with the spring is governed by Hooke’s law, F = αx, where α is the Hooke’s law constant. To examine the lattice vibration property of III–V compound semiconductors, a 1D diatomic linear chain model shown in Fig. 4.2 will be used to represent the diatomic primitive unit cell structure. The lighter atoms with a mass m and the heavier atoms with a mass M are arranged alternately with an equal separation of a in between.
2n2
2n1
2n
2n+1
2n+2
m
M
m
M
m
a u2n1
M
a u2n
F2n1
......
u2n+1
F2n+1
Fig. 4.2 Onedimensional row of springs and masses in a linear chain diatomic model of III–V compounds. These springlinked masses are allowed to vibrate longitudinally through displacements ui
4.1 Structural Properties
109
Let us first discuss the 1D motion along the linear chain only, i.e., longitudinal vibration, without concerning the sideways motion. It is assumed that the only significant force interactions between atoms are direct nearestneighbor interactions. Therefore, the net force acting upon the 2nth atom can be seen as interactions through two springs connecting to atoms (2n + 1) and (2n − 1). The force equation is given as F2n = α(u 2n+1 − u 2n ) − α(u 2n − u 2n−1 ) = α(u 2n+1 + u 2n−1 − 2u 2n )
(4.3)
where ui ’s are the displacements of the ith atoms. In obtaining (4.3), we note that the force acting on the 2nth atom from the (2n–1)th atom is opposite to that from the (2n + 1)th atom. The force between nearest neighbors can be expressed by Hooke’s law and Newton’s second law as ⎧ ⎪ ⎪ d2 u 2n ⎪ ⎨ F2n = m = α(u 2n+1 + u 2n−1 − 2u 2n ) dt 2 (4.4) ⎪ 2 ⎪ u d ⎪ 2n+1 ⎩ F2n+1 = m = α(u 2n+2 + u 2n − 2u 2n+1 ) dt 2 The periodic solutions to these two equations are in the forms of
u 2n = A exp[i(ωt − 2nka)] u 2n+1 = B exp{i[ωt − (2n + 1)ka]}
(4.5)
where ω is the oscillation frequency of atoms. The displacement of the (2n + 2)th and (2n − 2)th atoms can be expressed as
u 2n+2 = A exp{i[ωt − (2n + 2)ka]} = u 2n exp(−2ika) u 2n−1 = B exp{i[ωt − (2n − 1)ka]} = u 2n+1 exp(2ika)
(4.6)
Replacing all the relevant u’s in the force equation for the (2n +1)th atom, we find
−Mω2 u 2n+1 = α 1 + exp(−2ika) u 2n − 2u 2n+1
(4.7)
Solving for u2n+1 , we have u 2n+1 =
α 1 + exp(−2ika) u 2n 2α − Mω2
(4.8)
The force equation for the (2n)th atom has the form
−mω2 u 2n = α 1 + exp(−2ika) u 2n+1 − 2u 2n
(4.9)
Combining (4.8) and (4.9), it is found that 2α − mω2 2α − Mω2 − 4α 2 cos2 ka = 0
(4.10)
110
4 Compound Semiconductor Crystals
Rearranging the equation in terms of ω, we obtain ω4 −
2α(m + M) 2 4α 2 sin2 ka ω + =0 mM mM
(4.11)
The solution of the ωk dispersion relation has the form ⎡ 2 ω± =
α(m + M) ⎣ 1± mM
⎤
1−
2
4m Msin ka ⎦ (m + M)2
(4.12)
The positive sign group of the ωk dispersion curve is called the optical branch, and the negative sign group is called the acoustical branch because the energies associated with these two modes of vibrations are in the optical and acoustical range of the frequency spectrum, respectively. The dispersion curves of phonons vibrating longitudinally are shown in Fig. 4.3. Near the zone center, at k = 0, ω+ has a maximum value of ω+ (0) =
2α(m + M) and ω− (0) = 0 mM
(4.13)
The oscillation frequency of the acoustical branch for small values of k, sinka ≈ ka, becomes ω− (0) ≈ ka
2α (m + M)
(4.14)
Here we assumed (1+ x)1/2 = 1 + x/2 − x 2 /8 + … ≈1+ x/ 2. The frequency of the acoustical branch near the zone center is a linear function of k.
Fig. 4.3 Phonon dispersion curves for a 1D linear diatomic crystal with longitudinal vibrations
4.1 Structural Properties
111
The smallest allowed wavelength in this diatomic system should equal twice the lattice constant (2a), which is λ = 4a. Therefore, the first zone boundary is located at k = ± 2π /λ = ±π /2a, and where the two roots become
√ ω+ = 2α/m √ ω− = 2α/M
(4.15)
For m = M, a forbidden frequency band is formed. The relative movement of the two atoms in the unit cell can be calculated by taking the ratio of u2n+1 and u2n . α 1 + exp(−2ika) u 2n+1 B = = exp(−ika) 2 u 2n 2α − Mω A
(4.16)
α exp(−ika) + exp(ika) B 2α = = coska A 2α − Mω2 2α − Mω2
(4.17)
or
For the acoustical branch, ω = ω– (0) = 0 at k = 0, thus (4.17) leads to A = B. As shown in Fig. 4.4, the displacements in the longitudinal acoustic (LA) branch are like sound waves, where the two atoms in each unit cell move in the same direction by almost the same distance. It appears as if the whole crystal has been compressed or stretched over a small region. This creates alternating zones of compression and dilation. In a crystal, these waves can propagate in three directions. If we choose the 100 direction in a cubic crystal, one acoustic mode is longitudinal and the other two are transverse. In the transverse acoustic (TA) modes, the atoms vibrate in the plane normal to the direction of wave propagation, similar to an electromagnetic wave in free space. The atoms and their center of mass move together as in longwavelength acoustical vibrations. For the optical branch, using the values k = 0 and ω = ω+ (0) in (4.17), we find that B/A = – m/M. As shown in Fig. 4.5, the heavy and light atoms move in opposite
Fig. 4.4 Motion of the atoms in longitudinal acoustic (LA) mode for a 1D chain of alternating light and heavy atoms. The two types of atoms move together in transverse acoustical (TA) mode of the same crystal system. Displaced positions of moving atoms are shown as gray circles
112
4 Compound Semiconductor Crystals
Fig. 4.5 Motion of the atoms in longitudinal optical (LO) mode for a 1D chain of alternating light and heavy atoms. The two types of atoms move in opposite directions in the transverse optical (TO) mode
directions and the displacement is inversely proportional to the mass of the atom. In the longitudinal optical (LO) mode, both the light and heavy atoms vibrate back and forth in the same direction in which the wave travels. Similar to the TA modes, in the transverse optical (TO) modes, the atoms vibrate in the plane normal to the direction of wave propagation, but the atoms move in opposite directions. Both Si and GaAs have two atoms in each primitive cell, allowing two different modes of vibrations close to that of Fig. 4.3. The experimental phonon dispersion curves of GaAs, shown in Fig. 4.6, are very similar to those predicted by the 1D model. The doubly degenerated transverse branches are also displayed. The LO phonon energy in the zone center of GaAs is 36 meV. We also notice that the oscillation frequency for TO phonons is smaller than that of LO phonons at the zone center. In compound semiconductors, the relative displacement of the two atoms, as in the optical mode, sets up an electric dipole. This leads to the formation of a polarization field and an electric field, which can interact with electromagnetic waves. Electrons can be scattered rapidly by the electric field associated with the polar LO phonons, raising their frequency. Purely transverse vibrations do not generate dipoles, so this effect is absent. This polar nature is not seen in elemental semiconductors because all atoms are identical and there is no transfer of charge. Since phonons are the quantum mechanical equivalents of lattice vibrations, there are abundant phonons available in semiconductor crystals at room temperature. For a wave of frequency ω, the crystal momentums of photons and phonons are both given by èk and k = ω/υ, where υ is the velocity of the wave. For an electromagnetic wave, υ = c = 3 × 108 m/s. The velocity of a lattice wave is similar to that of a sound wave, and its amplitude is smaller by about five orders of magnitude. Therefore, for the same frequency, the momentum of a phonon is much higher than that of a photon. This finite momentum associated with the phonon becomes very important in connecting electrons and photons in a semiconductor. In an indirect bandgap semiconductor, as discussed in Chap. 8, phonons can provide high enough momentum to satisfy
4.1 Structural Properties
113
Fig. 4.6 Left: Phonon dispersion curves along [100] from to X for a GaAs crystal at room temperature. The transverse mode branches are doubly degenerated. (Reprinted with permission from [3], copyright American Physical Society) Right: Measured dispersion curves for phonons in Si along [100]. (Reprinted with permission from [4], copyright American Physical Society)
momentum conservation required to excite an electron from the valence band to the conduction band by absorbing or emitting a photon with the proper energy. Phonons also play an equally important role in the light emission process in direct bandgap semiconductors. Electrons in higher states inside the conduction band need to relax to the band minimum before they can recombine with holes residing near the valence band maximum for photon generation. The relaxation process relies on phonons, with energy èω, to dissipate extra energy into heat and to conserve momentum.
4.2 Electrical Properties 4.2.1 Effective Mass The electron concentration in a nondegenerate semiconductor is calculated by integrating the electron distribution above the conduction band edge and formulated as
114
4 Compound Semiconductor Crystals
∞ n=
D(E) f (E)dE
(4.18)
Ec
where D(E) is the density of states of a bulk semiconductor and has the form 1 2m DOS 3/2 √ D(E) = E 2π 2 2
(4.19)
where mDOS stands for the DOS effective mass. In a nondegenerated semiconductor, where E c − E F > 3kT, the Fermi–Dirac distribution function f (E) can be approximated by the Boltzmann distribution function to simplify the calculation. E c − E F −1 Ec − E F f (E) = 1 + exp ≈ exp − kT kT
(4.20)
This leads to a nondegenerate electron concentration of
Ec − E F n = Nc exp − kT
(4.21)
where N c is the effective density of states in the conduction band and has a value of
2π m DOS kT Nc = 2 h2
3/2
= 2.509 × 10
19
m DOS T m 0 300
3/2
−3 cm
(4.22)
For a parabolic conduction band with spherical energy surface, like GaAs, mDOS simply equals me *. For nonspherical energy surface, the DOS effective mass used for carrier concentration calculation is modified according to the procedures outlined below. For example, in Si and AlAs, the conduction band is nonspherical (ellipsoidal) and has multiple valleys. For an ellipsoidal energy surface along k x , it can be expressed as E − Ec =
2 k 2y p 2y + pz2 2 k z2 2 (k x − k x0 )2 ( px − px0 )2 + + = + 2m L 2m T 2m T 2m L 2m T
(4.23)
This ellipsoidal surface can transform into a spherical surface through a coordinate transformation process and is expressed as E − Ec =
px
2
2 2 + p y + pz 2m
2 p = 2m
(4.24)
√ √ √ where px = ( px − px0 ) m /m L , p y = p y m /m T , and pz = pz m /m T . The volume of p space in the spherical shell bounded by radii p and p + d p for a
4.2 Electrical Properties
115
single ellipsoidal is dV p = 4π p 2 d p and p d p = m dE. Thus, √ 3/2 dV p = 4 2π m E − E c dE
(4.25)
Since dV p = dpx dpy dpz and dV p = d px d p y d pz , dV p and dV p are related through dV p =
m L m 2T
(m )3/2
√ dV p = 4 2π m L m 2T E − E c dE
(4.26)
for one ellipsoidal energy surface. For g equivalent valleys, the total DOS effective mass becomes 1/2 (m DOS )3/2 = g m L m 2T
(4.27)
In the valence band, there is a single peak containing multiple bands, i.e., lighthole and heavyhole bands. Similarly, the DOS function is also modified to include the multiband effect. E F − Ev p = plh + phh = (Nvl + Nvh ) exp − kT 2π kT 3/2 E F − Ev 3/2 m lh + m hh exp − =2 (4.28) h2 kT where N vl and N vh are the effective density of states in the lighthole band and heavyhole band, respectively. Therefore, the DOS effective mass of the valence band becomes 3/2
3/2
3/2
m DOS = m lh + m hh
(4.29)
The calculated effective DOS and intrinsic carrier concentration (ni ) in Si and GaAs are listed in the Table 4.2. In addition, there is another type of effective mass associated with the conductivity. The conductivity is related to the effective mass in the form of σ =
Table 4.2 Effective density of states and intrinsic carrier concentration of Ge, Si, and GaAs
nq 2 τ m ∗c
(4.30)
(cm−3 )
Ge
Si
Nc
1.04 × 1019
3.2 × 1019
4.7 × 1017
Nv
5×
1.8 ×
9.4 × 1018
ni
2.33 ×
1018 1013
GaAs 1019
1.02 ×
1010
2.1 × 106
116
4 Compound Semiconductor Crystals
where n is the carrier concentration, q is the electron charge, τ is the carrier relaxation time, and m ∗c is the conductivity effective mass. For semiconductors with a spherical energy surface, such as GaAs, the conductivity effective mass has a simple form of m ∗c = m ∗e
(4.31)
For nonspherical energy surfaces of the conduction band, as for Si and AlAs, the conductivity has a tensor form of ⎡
⎤ ∂ 2 E/∂k x2 ∂ 2 E/∂k x k y ∂ 2 E/∂k x k z ni q τ ⎣ 2 σi = ∂ E/∂k y k x ∂ 2 E/∂k 2y ∂ 2 E/∂k y k z ⎦ 2 ∂ 2 E/∂k z k x ∂ 2 E/∂k z k y ∂ 2 E/∂k z2 2
(4.32)
for each ellipsoidal surface. Since ∂ 2 E/∂ki ∂k j = 0 for i = j, so that all the offdiagonal elements of the tensor are zero. Using Si as an example, the major axes of the ellipsoidal energy surface lie along the coordinate axes of kspace. The conductivity ¯ ellipsoids along k z becomes tensor for, say, [001] and [001] ⎡
σ(001)
⎤ 0 1/m T 0 2 = σ([001] 1/m T 0 ⎦ ¯ ) = n (001) q τ ⎣ 0 0 0 1/m L
(4.33)
where mx = my = mT and mz = mL . Since all six ellipsoids are equivalent energy = n (010) = n (010) = n (001) = n (001) minima (Fig. 3.28), n (100) = n (100) ¯ ¯ ¯ = n/6. By summing up conductivities of all six ellipsoids, one can write the total conductivity as ⎡ ⎤ 1 2 1 0 0 + 3 m m T L ⎢ ⎥ ⎢ ⎥ 1 2 1 0 0 (4.34) + σ = nq 2 τ ⎢ ⎥ 3 mT mL ⎣ ⎦ 1 2 1 0 0 + mL 3 mT This leads to the conductivity and the conductivity effective mass of nq 2 τ 1 2 = + mL mT m ∗c 1 1 1 2 = + ∗ mc 3 mL mT
nq 2 τ σ = 3
(4.35) (4.36)
In general, the carrier effective mass is a constant for nondegenerate semiconductors. However, the conduction band effective mass of a degenerated semiconductor
4.2 Electrical Properties
117
becomes dependent on doping concentration. At high doping levels, in ntype semiconductor the Fermi level moves close to, or even into, the conduction band. Since the nonparabolicity of the band becomes significant, the effective mass increases with doping level for carrier density larger than 1018 cm−3 .
4.2.2 Mobility The mobility (μ) is defined as the drift velocity (vd ) per unit electric field intensity (F). μ≡
υd qτ = ∗ cm2 /Vs F m
(4.37)
where τ is the relaxation time or the inverse of scattering probability (1/τ ). The equilibrium drift velocity is determined from the balance between the electric fieldinduced acceleration and scattering generated deceleration. If the scattering mechanisms are assumed to act independently, the total probability of a scattering event occurring in the differential time dt is the sum of the individual events. Thus, 1 1 ≡ τ τj j
(4.38)
where τ j is the relaxation time for each scattering mechanism. Since the mobility is proportional to τ, according to Matthiessen’s rule, the total carrier mobility is the inverse sum of each individual contribution. 1 μtotal
≡
1 1 1 1 1 1 = + + + + μ μ μ μ μ μ j i l po pe al j
(4.39)
The major scattering mechanisms included in compound semiconductors are impurity scattering (μi ), lattice scattering (μl ), polar scattering (μpo ), piezoelectric scattering (μpe ), and alloy scattering (μal ). The total mobility is thus limited by the dominant scattering mechanisms occurring in the semiconductor, as illustrated in Fig. 4.7. For holes, the mobility is low compared to electrons, mainly due to the heavy effective mass associated with the heavyhole band. Due to the degeneracy of the heavy and light holes, the interaction between these two bands also contributes to the extra scattering. In the following, we briefly discuss the mobility due to major scattering mechanisms.
118
4 Compound Semiconductor Crystals
Fig. 4.7 Temperature dependence of the mobility for highpurity ntype GaAs showing the separate and combined scattering processes. Reprinted with permission from [5], copyright AIP Publishing
(a) Impurity scattering (µi ) The calculation of the mobility for ionized impurity scattering is based upon the scattering of charged particles by Coulomb potential of nuclei, which was originally developed by E. Rutherford to explain the scattering of αparticles. The resultant mobility has a temperature dependence of T 3/2 . −1/2 3/2 T μi ∝ Ni−1 m ∗
(4.40)
where N i is the ionized impurity concentration. The impurity scattering is the major mobility limiting mechanism at low temperatures for both elemental and compound semiconductors. (b) Lattice (deformation potential) scattering (µl ) The vibrations of lattice atoms at finite temperatures cause a local variation in the energies of the conduction and valence band edges. The abrupt changes in the band edges further cause increased electron deflections. The energy step height is related to the degree of lattice compression/dilation defined by the deformation potential. At low temperatures, the thermal energy available to excite opticalmode lattice vibrations is quite limited. So we shall consider only the scattering by LA phonons. The temperature dependence of the lattice scattering has a form of T −3/2 .
4.2 Electrical Properties
119
−5/2 −3/2 μl ∝ Ξ −2 m ∗ T
(4.41)
where is the deformation potential. This is the major scattering mechanism in the hightemperature region for elemental semiconductors, but not for III–V compounds. However, experimental data show that, in both Si and Ge, the temperature dependences deviate quite considerably from the T −3/2 law in the region dominated by lattice scattering. As discussed in the previous section, lattice vibrations generate both acoustic and optical branches of phonons. In (4.41), only the lowfrequency acoustical mode is considered. In silicon or AlAs, there are six equivalent conduction band minima in the first Brillouin zone. Electrons scatter between these valleys, forming an intervalley scattering process. The large momentum change involved requires the participation of highenergy phonons, both acoustical and optical. Consider the opticalmode phonon contribution, the intervalley scattering mobility shows a different temperature dependence of the following form: −5/2 −1 T exp ωop /kT μop ∝ m ∗
(4.42)
where ωop is the optical phonon energy. (c) Polar scattering (µpo ) In compound semiconductors, when responding to lattice vibrations, the two neighboring atoms move in opposite directions in the optical phonon modes. Because of the nonzero ionicity, the relative movement of neighboring atoms constitutes an electric polarization, which in turn produces an electric field. Deflection of the motion of free carriers by the field limits the mobility of carriers. Thus, the electron mobility in III–V compounds is limited by polar scattering instead of acoustical mode scattering in the hightemperature region. Polar scattering becomes the most dominant scattering mechanism in compound semiconductors at high temperatures. μpo ∝
−1/2 , T > θl (m ∗ )−3/2 (T /θl ) ∗ −3/2 exp(θl /T ) − 1 , T < θl (m )
(4.43)
where θl = ωl /k is the equivalent temperature associated with longitudinal optical phonons. Since the polar scattering mobility is inversely proportional to (m*)3/2 , the large difference in electron mobility and hole mobility in III–V compounds is explainable by (4.43). (d) Piezoelectric scattering (µpe ) A polarization electric field induced in an ionic crystal, such as II–VI compounds and IIIN alloys, by the applied mechanical stress, or vice versa, is called the piezoelectric effect. The electric field accompanying the lattice vibrations can interact with electron motion through the lattice. Since zincblende III–V compounds are not pure covalent crystals, but mixtures of covalent and ionic bonding, there exist finite piezoelectric fields. The piezoelectric scattering mobility is
120
4 Compound Semiconductor Crystals
3/2 −1/2 μpe ∝ m ∗ T
(4.44)
This is the main scattering mechanism which limits the mobility in ionic II–VI compounds, but it is less important for zincblende III–V compounds. (e) Alloy scattering (µal ) When mixing binary compounds into ternary or quaternary alloys, the lattice constant, according to Vegard’s law, is proportional to the composition ratio of the binaries. A close examination indicates that the bond lengths associated with each individual binary do not change significantly, as shown in Fig. 4.8. Using an extended xray absorption fine structure (EXAFS) technique, in InGaAs alloys, the measured GaAs and InAs nearneighbor distances change by only 0.04 Å over the whole alloy composition range. However, the virtual crystal model that follows Vegard’s law requires a change in average nearneighbor spacing of 0.17 Å. Therefore, the compound can be seen as a mixture of clusters of binary alloys instead of a completely random material. The carriers moving through regions containing different proportions of binaries may suffer scattering as −5/2 −1 −2 −1/2 S u T μal ∝ m ∗
(4.45)
where S represents the degree of randomness (S = 1 for complete random composition), and u is the alloy scattering potential. It turns out that this is the limiting Fig. 4.8 Nearneighbor distance versus InAs mole fraction x in the Inx Ga1−x As ternary alloy measured by EXAFS. The dashed line represents the average cation–anion spacing according to Vegard’s law. Reprinted with permission from [6], copyright American Physical Society
4.2 Electrical Properties
121
Fig. 4.9 Temperature dependence of the electron Hall mobility in In0.53 Ga0.47 As. The contribution due to alloy scattering dominates the total mobility near 100 K. Reprinted with permission from [7], copyright Elsevier
scattering mechanism in the middle temperature range for ternary and quaternary compounds. Figure 4.9 shows the dominance of alloy scattering in electron Hall mobility near 100 K in an In0.53 Ga0.47 As ternary alloy latticematched to InP. (f) Highfield phenomena As shown in (4.37), the carrier mobility is determined by the total scattering events occurring inside the semiconductor. If scattering rates were fixed, mobility would remain constant and carrier velocity would be limited by the magnitude of the applied electric field. In fact, under the increasing applied electric field, new scattering mechanisms come into play as carrier energies increase. Under a moderately highfield (~104 V/cm) condition, carriers may acquire sufficient energy to excite acoustic phonons within the semiconductor lattice. Increased phonon scattering is particularly pronounced between multiple conduction band minima in indirect bandgap materials. This leads to a sublinear rate of the mobility change with increasing applied field. For further increases of the field to above 105 V/cm, the energy gained by carriers is transferred to lattice heating through optical phonon emission (~60 meV in Si and ~36 meV in GaAs), resulting in a saturated drift velocity (or mobility) with a value of about 107 cm/s. The velocity–field characteristics for electrons in Si, GaAs, and InP are shown in Fig. 4.10. Between the initial rolloff and final velocity saturation, the velocity–field behavior of electrons in the direct bandgap semiconductor is quite different from that in Si. As shown in Fig. 4.10, GaAs and InP display an anomalous peak in drift velocity corresponding to a negative differential resistance. This is the basis of microwave oscillation in compound semiconductors, known as the Gunn effect. To
122
4 Compound Semiconductor Crystals
Fig. 4.10 Velocity–field characteristics for GaAs, InP, and Si [8]. Reprint with permission from [9], copyright American Physical Society
understand this, one must look into semiconductor band structures, e.g., Fig. 3.25. For GaAs, the conduction band has a number of satellite valleys at L and X minima with 0.31 meV and 0.51 meV above the valley minimum, respectively. At low field, electrons are in the valley, characterized by a light effective mass of 0.063m0 so that the lowfield mobility is high. At intermediate field, electrons may gain enough energy to be transferred into the lowest satellite valleys. For GaAs, the lowest satellite energy band minima are located at L valleys with a heavy effective mass of 0.85m0 and a high density of states (×50 than valley) for scattering electrons, leading to lower mobility. Thus the electron transfer between and L valleys results in a downturn in electron velocity as shown in Fig. 4.10. The transfer electron effect has been utilized in devices to generate negative resistance and microwave oscillations.
4.2.3 Intentional Impurity In III–V compounds, intentional impurities are selected from columns adjacent to column III or V of the periodic table. Elements from group II predominantly occupy group III sites to form ptype impurities. Substitution of group V elements by group VI impurities would result ntype materials. Group IV impurities can occupy either cation or anion sites and are amphoteric dopants. The energy required to ionize a dopant is called the activation energy, which is mainly determined by the Coulombic interaction between the impurity atom and the attached charge carrier. The hydrogen atom model can be applied to understand the shallow donors in III–V compounds. We derived the ionization energy for a hydrogen atom as
4.2 Electrical Properties
123
(4.46) where Ry is the Rydberg energy. To apply this model to shallow donors, we have to make two modifications. First, the effective mass of electrons in semiconductors is very different from the free electron mass. Second, the dielectric constant of semiconductors is much larger than the free space value. Then the donor ionization energy required for the n = 1 level is (4.47) The donor Bohr radius is given by (4.48) The calculated ionization energy and Bohr radius for a hydrogenlike donor in GaAs with r = 12.85 and m ∗e = 0.067 m0 are 5.5 meV and 102 Å, respectively. The bound state wave function of the impurity extends much farther than the unit cell of the lattice (~5 Å). This result provides the justification for using effective mass and the dielectric constant of the semiconductor in these calculations. The calculated activation energy is smaller than or comparable to the thermal energy kT at room temperature. Therefore, all shallow donor impurities can be considered as activated at room temperature. The application of the hydrogen model to acceptors in III–V compounds is complicated by their degenerate valence band structure. In the limit of strong spinorbit interaction—that is, for spinorbit splitting (so ) much larger than the acceptor energy— only the heavyhole and lighthole bands are included for acceptor binding energy calculation. The calculated results of the effective Bohr radius and effective Rydberg energy are found to be functions of Luttinger parameters, γ 1 , γ 2 , and γ 3 , which describe the valence band shapes near the center of the Brillouin zone. Table 4.3 lists the calculated acceptor ionization energy for the major III–V compounds, which agrees reasonably well with experimental results. The measured values for each compound are given below. Following is a summary of the most commonly used dopants in III–V compound semiconductors. (a) Group II impurities incorporate on the anion sites of III–V compounds to form shallow acceptors. Table 4.3 Calculated acceptor ionization energy of selected III–V compounds [8] Material
AlSb
GaP
GaAs
GaSb
InP
InAs
InSb
Ea
42.4
47.5
25.6
12.5
35.3
16.6
8.6
124
4 Compound Semiconductor Crystals
Beryllium (Be) is a major shallow acceptor in III–V compounds. It has an ionization energy of 28 and 41 meV in GaAs and InP, respectively. Except at the highest concentration ≥1019 cm−3 , Be diffuses slowly in GaAs and the diffusion coefficient as a function of temperature has the form D = D0 exp(−E a /kT )
(4.49)
with the activation energy E a = 1.95 eV and D0 = 2×10−5 cm2 /s. However, at very high doping concentrations of ~1020 cm−3 , Be redistributes severely which can degrade the device performance. Be is widely used in molecular beam epitaxy (MBE)growth, ion implantation, and as Au–Be alloy for ptype ohmic contact metallization. Zinc (Zn) is another major shallow acceptor in III–V compounds besides Be. The ionization energy is 31 meV in GaAs and 47 meV in InP. Due to its high vapor pressure, Zn is not suitable for MBE. In chemical vapor deposition (CVD), Zn is a popular dopant. Zn diffuses rapidly at high concentration and its diffusion rate is concentration dependent. The AuZn alloy is commonly used as a ptype ohmic contact metallization. Magnesium (Mg) is a shallow acceptor impurity in III–V compounds with an ionization energy of 28 meV in GaAs and 41 meV in InP. Mg has a strong affinity for oxygen. Elemental Mg can form MgO easily during the doping process, which leads to a low doping incorporation coefficient at high growth temperature (>500 °C). Recently, it was found that Mg is an efficient ptype dopant in IIInitride compounds grown by both MBE and metalorganic chemical vapor deposition (MOCVD). Nevertheless, the doping efficiency is low with deep ionization energy of ≥150 meV. Cadmium (Cd) is a shallow acceptor in GaAs and InP with ionization energies of 35 and 56 meV, respectively. It has a very high vapor pressure, approximately 1–2 orders of magnitude higher than Zn. It is a useful dopant in liquid phase epitaxy (LPE) growth of InP for temperature ≤550 °C with a maximum doping concentration of ~1018 cm−3 . (b) Group VI impurities incorporate on the cation sites of III–V compounds to form shallow donors. Sulfur (S) is a shallow donor in III–V compounds with an ionization energy of 6 meV in GaAs. It has a high vapor pressure, and the incorporation depends strongly on the epitaxial growth temperature. This makes the accurate control of doping concentration from a solid sulfur source difficult. However, hydrogen sulfide (H2 S) is the most common doping precursor used in CVD for ntype doping of III–V compounds. Selenium (Se) is also a high vapor pressure shallow donor in III–V compounds similar to sulfur. It has an ionization energy of 6 meV in GaAs. Hydrogen selenide (H2 Se) is a commonly used gaseous doping source of Se. However, the doping
4.2 Electrical Properties
125
memory effect of using H2 Se is the major drawback. The memory effect manifests itself by a lack of abruptness of doping profiles. Tellurium (Te) is an efficient shallow donor in III–V compounds. It has an ionization energy of 30 meV in GaAs. This is much larger than the calculated 5 meV due to a correction associated with the big Te atom. Elemental Te has been used as an ntype doping source in LPE growth of GaAs. Diethyltellurium [(C2 H5 )2 Te, DETe] has been used as a Te doping precursor for MOCVD and metalorganic MBE (MOMBE) growth of GaAs and InP. (c) Group IV dopants Group IV impurities incorporated into III–V compounds share some interesting characteristics. First, they all are amphoteric, i.e., they can occupy either the group III or the group V sites to become donors or acceptors, respectively. Second, they autocompensate. A group IV impurity that predominantly occupies the cation sites as a donor can also occupy the anion sites. This causes compensation and lowers the doping efficiency. Third, the electrically activated impurities saturate at high doping concentration. The autocompensation increases at high doping level and leads to the saturation of the free carrier concentration. Fourth, the free carrier concentration depends on growth temperature and V/III flux ratio during growth. For example, as shown in Fig. 4.11, when growing silicondoped GaAs by liquid phase epitaxy, the type of conductivity depends on the growth temperature and the Si concentration in the liquid. At a fixed Si concentration above 4 × 10−4 atomic fraction in the growth solution, the GaAs shows n and ptype conductivities when grown at high and low temperatures, respectively. Carbon (C) is a shallow acceptor in GaAs (26 meV) but a donor in InP (43 meV) and InAs. Carbon is a stable impurity and diffuses very slowly. Its temperaturedependent diffusion coefficient in GaAs follows (4.49) with an activation energy Fig. 4.11 Effect of growth temperature and Si concentration in the liquid on the doping behavior of Si in LPE grown GaAs
126
4 Compound Semiconductor Crystals
E a = 1.75 eV and D0 = 5 × 10−8 cm2 /s. Compared to Be, at 800 °C, the diffusion coefficient of C is almost two orders of magnitude smaller. It is an unintentional dopant in MOCVD when using metalorganic Ga and Al precursors. CCl4 and CBr4 are commonly used gaseous carbon doping sources. A very high acceptor level (~1020 cm−3 ) is easily achieved in many III–V compounds. These behaviors make C the most ideal ptype dopant for the base region of III–V heterojunction bipolar transistors (HBT). Silicon (Si) is a stable shallow donor (4–6 meV) in most III–V compounds at low concentration. The temperaturedependent diffusion coefficient in GaAs has an activation energy E a = 2.45 eV and D0 = 4 × 10−4 cm2 /s. It strongly compensates in the high concentration regime (~5×1018 cm−3 ). It has been widely used as an ntype dopant for epitaxial growth and ion implantation. Gaseous silicon dopant precursors including silane (SiH4 ) and disilane (Si2 H6 ) have been widely used in MOCVD and MOMBE growth. Germanium (Ge) is a strongly amphoteric impurity in III–V compounds. It is a ptype dopant for LPE growth of GaAs, but not popular for MBE and MOCVD growth. AuGe alloy is used for ntype ohmic contact metallization. Tin (Sn) is a weakly compensating shallow donor in III–V compounds with 4– 6 meV ionization energy in GaAs and InP. The major problem of Sn impurity during growth is the tendency to strongly redistribute due to the Sn diffusion and surface segregation. Nevertheless, high electron mobilities in GaAs:Sn are expected due to its low compensation. (d) Hydrogen passivation In III–V semiconductors, hydrogen is not an electrically active impurity. However, during the doping process, hydrogen generated from the carrier gas and/or dopant flux can passivate or neutralize shallow donor or acceptor in semiconductors. Using Si in (Al)GaAs as an example, under normal conditions, the substitutional silicon atom replaces a Ga and bonds with four nearest neighboring As atoms. When hydrogen atoms are incorporated into the lattice, a hydrogen can bond to the Si donor by breaking one of the SiAs bonds and sit in an interstitial site, as shown in Fig. 4.12a. The broken SiAs bonds of the As atom opposite the hydrogen atom are replaced with a lone pair of electrons—one provided by the donor atom and the other from the dangling bond of the As atom. The SiH complex yields a neutral electron count, and the hydrogen has passivated the donor atom. The active donor concentration becomes very low compared to the impurity concentration. Hydrogen passivation of donor atoms has been found for a large number of donors including Si, Sn, Se, and Te. The dissociation of donor hydrogen bond by thermal annealing at temperatures above 400 °C allows hydrogen to diffuse out of the hydrogenated semiconductor and recover the doping concentration. Hydrogen also passivates shallow acceptors in III–V compounds as shown in Fig. 4.12b. The acceptor As bonds are broken, and the hydrogen atom is bonded to the arsenic atom and occupies a site between the acceptor impurity and the neighboring arsenic. The entire hydrogen acceptor complex is neutral, and the hydrogen passivates the acceptor.
4.2 Electrical Properties
127
Fig. 4.12 a The group IV donor (Si)hydrogen complex with hydrogen in an interstitial site and bound to the donor atom. b The group II acceptor (Be)hydrogen complex with hydrogen bound to an As atom. Reprinted with permission from [11], copyright American Physical Society
4.2.4 Deep Levels During the growth or doping of semiconductors, chemical impurities, native defects, or the combination of both, can form deep energy level(s) in the forbidden gap. These deep levels act like traps to capture and annihilate electrons and holes, making the material electrically inactive. Therefore, the deep traps may have many negative effects on the properties of semiconductors, including compensation of intentional impurities, minority carrier lifetime reduction, and reduced mobility and luminescence efficiency. In most cases, we should avoid deep levels in the fabrication of semiconductor materials and devices. Under certain circumstances, we utilize deep levels to control the conductivity of semiconductors. In this section, two particularly important deep levels in III–V compound semiconductors are discussed. (a) DX Centers During the 1970s, the rapid development of compound semiconductors was mostly focused on the Alx Ga1−x As system due to the availability of quality GaAs substrates, among other reasons. It was found that the ntype Alx Ga1−x As with 0.2 ≤ x ≤ 0.4 has some unusual properties as compared to GaAs. Most noticeable are the large donor activation energy and a strong sensitivity of the conductivity to illumination. These properties have profoundly negative effects on the device performance of Alx Ga1−x As/GaAs highelectronmobility transistors (HEMT), as will be discussed in Chap. 9. The origin of the deep center observed in ntype Alx Ga1−x As involves a donor atom and another constituent to form a complex called the donorcomplex (DX) center. The DX center formation mechanism and its properties are discussed below. In Alx Ga1−x As, donors such as Si, Te, or Sn can exist in two different configurations—substitutional and interstitial—as shown in Fig. 4.13. When the incorporated
128
4 Compound Semiconductor Crystals
Fig. 4.13 a Substitutional and b DX configuration of a Si donor in (Al)GaAs. In DX configuration, the Si occupies an interstitial site and has three cations in its immediate vicinity. Reprinted with permission from [11], copyright American Physical Society
Si atom takes the substitutional site, as shown in Fig. 4.13a, it replaces one of the anions of Alx Ga1−x As, e.g., Al or Ga. The Si atom is ~0.8 Å above the tetrahedron base formed by three adjacent As atoms. Due to the covalent bond length difference between Si (1.16 Å) and Al or Ga (1.26 Å), the substitutional configuration is the unrelaxed state for the Si atom. On the other hand, if the donor atom occupies an interstitial site, one of the four arsenic donor bonds is broken (Fig. 4.13b) and the interstitial configuration is the relaxed state. In this configuration, the Si atom is 0.2 Å below the tetrahedral plane defined by three As atoms. When the Si atom relaxes from the substitutional to interstitial configuration, the total displacement of the Si atom between the two configurations is approximately 1 Å. This displacement is large compared to the equilibrium bond length of the host crystal (~2.44 Å). This structural configuration change leads to a change in the electronic configuration of the defect. To illustrate the interplay between structural and electronic configurations, consider the hydrogen molecule as an example. The total energy and nuclei distance of bonding and antibonding states of two hydrogen atoms are shown in Fig. 4.14. The equilibrium distance between the two protons corresponds to a minimum total energy which depends on the electronic state of the molecule. The bonding state has a shorter core distance and lower total energy minima than the antibonding state. For small lattice relaxation, e.g., between bonding and antibonding states of a hydrogen molecule, the direct transitions between the ground (bonding) state and the excited (antibonding) state through absorption and emission are readily allowed. The electron of the bonding state can be excited to the antibonding state vertically and then relaxed to a new core position (configuration) before returning to
4.2 Electrical Properties
129
Fig. 4.14 Bonding and antibonding state energy of a hydrogen molecule as a function of distance between two core atoms. Note, èωa > èωe
the bonding state. This process leads to different absorption energy èωa and emission energy èωe for electron transitions between bonding and antibonding states, known as the FranckCondon shift. However, due to the heavier mass of the nuclear as compared to the electronic mass, the two nuclei do not move during the short time of the electronic transition but the molecule slowly moves to the new configuration, i.e., new core distance. This situation is changed dramatically for large lattice relaxation. Figure 4.15 shows two configurations of such defects. Photon energy of èωa is required to excite the defect from the ground (relaxed) state to the excited (unrelaxed) state. Once the defect has minimized its energy in the excited state, the defect becomes metastable and cannot return to the ground state by means of an optical (vertical) transition. In order for the defect to return from the metastable state to the Fig. 4.15 Schematic configuration coordinate diagram for large lattice relaxation
130
4 Compound Semiconductor Crystals
Fig. 4.16 a Energy diagram model of a DX center in ntype AlGaAs; E c —capture energy barrier, E E —transit emission energy, E t —activation energy, and E 0 —absorption energy of the DX center. b Configuration coordinate diagram of the DX center. Reprinted with permission from [12], copyright American Physical Society
ground state, it has to overcome the capture energy barrier E c through other allowed paths such as thermally excited transitions. Thermal emissions are also allowed to excite the defect from the ground state to the excited state. The thermal emission energy E E = E c + E t is measured from the minimum of the ground state to the top of the thermal barrier. We can use the same analysis to understand the physical mechanism of the DX center. The schematic representations of the relevant energies of the DX center and their representation in the configuration coordinate diagram are shown in Fig. 4.16. Experimentally, these relevant energies have been determined for Sidoped Alx Ga1−x As: E 0 ≥ 1 eV, E t ≈ 150 meV, E c ≈ 150 meV, and E E ≈ 300 meV. Apparently, this is a very deep level, as expected. Since the DX interstitial configuration in Sidoped Alx Ga1−x As is a stable (relaxed) configuration, the substitutional configuration is the excited (unrelaxed) configuration, and a neutral substitutional donor can capture an electron and transform into a DX center, i.e., D0 + e ↔ DX−
(4.50)
where D0 and DX– represent a neutral substitutional donor and a negatively charged DX center, respectively. An ionized shallow donor can also capture two electrons by assuming the DX configuration, i.e., D+ + 2e ↔ DX−
(4.51)
As a consequence, both deep DX– donors and shallow D0 donors coexist in ntype Alx Ga1−x As (0.2 ≤ x ≤ 0.4) at low temperatures. As an example, Fig. 4.17 shows the dependence of the Hall carrier concentration of Sidoped ntype Al0.32 Ga−.68 As on temperature. When measured in dark, the electron concentration remains constant for temperature below ~150 K, with a value of 3.5 × 1017 cm−3 , only a fraction of the
4.2 Electrical Properties
131
Fig. 4.17 Temperature dependence of the Hall electron concentration in ntype Al0.32 Ga0.68 As with a Si doping concentration of 1.5 × 1018 cm−3 . Solid and open circles indicate experimental data measured in the dark and after illumination at low temperatures, respectively. Reprinted with permission from [13], copyright American Physical Society
Si impurity concentration of 1.5 × 1018 cm−3 . The electron concentration increases at temperatures higher than 150 K indicating the thermal ionization of the deep donor center. However, the saturation of the free carrier concentration does not occur even at 300 K confirming that the DX center has large thermal activation energy. Upon illumination with an infrared radiation having a wavelength of 820 nm, which is below the bandgap of Alx Ga1−x As at low temperature, the carrier concentration increases. The increase in carrier concentration persists even after the illumination has been turned off hours or days. This phenomenon is known as the persistent photoconductivity (PPC) effect, a key characteristic of DX center in ntype Alx Ga1−x As. The model of two atomic configurations can explain the phenomenon of PPC. The negatively charged DX center resumes a neutral state, DX0 , under photoionization. This state is unstable, and the Si donor assumes the lowerenergy substitutional D0 configuration. Accompanying the neutral Si donors are the extra free carriers released from the DX– state. At sufficiently low temperatures, the Si cannot assume the DX– configuration due to the large capture barrier (E c ). Thus, the extra carriers remain free persistently. At temperatures higher than ~150 K, the neutral donor can capture an electron and return to the state of a DX center. Therefore, the high PPC concentration can be quenched by heating the sample to a temperature >150 K.
132
4 Compound Semiconductor Crystals
(b) EL2 Level When growing bulk III–V semiconductors, it is unavoidable that some unintentional impurities (Si, C, B, Fe, S, and Mn) are incorporated into crystals. The dominant residual impurity in bulk GaAs crystal grown by liquid encapsulated Czochralski (LEC) technique is the shallow acceptor C with a concentration in the low 1015 cm−3 range. This impurity comes from the graphite heating elements and/or the wall of the stainless steel growth chamber. The residual conductivity would be ptype with a resistivity of 0.1–10 cm. For highspeed device applications, it is necessary to minimize the parasitic capacitance and inductance by using semiinsulating (SI) substrates with a resistivity >107 cm. Many deep impurities have been intentionally introduced in order to achieve high resistivity in compound semiconductors. To achieve SI GaAs, the most noticeable dopant used was Cr. The major drawback is the Cr diffusion and redistribution during hightemperature processing and epitaxial growth. Later, the EL2 defect was identified as the key to achieve undoped SI GaAs grown by the LEC technique. The incorporation of a sufficiently high concentration of EL2 defects allows one to obtain semiinsulating GaAs materials with a resistivity higher than 107 cm. In GaAs there are many deep levels whose chemical origins are unknown. The EL2 defect is one of these deep levels (forming an electron trap) in undoped GaAs. The EL2 level has been identified to be the native As antisite defect, AsGa . The arsenic atom has two excess electrons if occupying a Ga site, i.e., a double donor. The main EL2 donor level, located approximately 0.75 eV below the conduction band edge, compensates for the shallow C acceptor impurities. For high EL2 concentrations, due to their large ionization energy, only a fraction of the EL2 centers will be ionized, while the remaining EL2 centers will be neutral. As a result, the Fermi level is pinned at the EL2 level which is approximately in the midbandgap of the GaAs. Thus, GaAs with sufficiently high concentration of EL2 centers has nearintrinsic characteristics. The EL2 concentration can be controlled during bulk crystal growth via the As/Ga composition in the growth melt (Fig. 4.18). For high As/Ga ratios (As atom fraction ≥0.475) in the growth melt, the concentration of EL2 defects increases, which compensates the shallow C acceptors. At low As/Ga ratios in the growth melt, the shallow C acceptor impurities are not fully compensated, leading to residual ptype conductivity of the bulk GaAs.
4.3 Free Carrier Concentration and the Fermi Integral 4.3.1 Free Carrier Concentrations in 3D Semiconductors The electron and hole concentrations in 3D semiconductor structures are calculated by integrating carrier distributions over appropriate energy ranges.
4.3 Free Carrier Concentration and the Fermi Integral
133
Fig. 4.18 Resistivity of unintentional doped GaAs grown by LEC technique as a function of As atom fraction in the growth melt. An Asrich melt produces semiinsulating GaAs with resistivity >107 cm and a Garich melt gives ptype conductivity. Reprinted with permission from [14], copyright AIP Publishing
⎧ ⎪ ⎪ ⎪ ⎨
n=
∞
Dc (E) f (E)dE
Ec
Ev ⎪ ⎪ ⎪ Dv (E)[1 − f (E)]dE ⎩p=
(4.52)
−∞
where D(E) and f (E) are the DOS and the Fermi–Dirac distribution function, respectively. The DOS of the conduction band and the valence band are ⎧ 1 2m ∗e 3/2 ⎪ ⎪ D E − Ec = (E) ⎨ c 2π 2 2 ⎪ 1 2m ∗h 3/2 ⎪ ⎩ Dv (E) = Ev − E 2π 2 2
(4.53)
In a semiconductor, the carriers are indistinguishable and have to obey the Pauli exclusion principle. The occupation behavior in the energy space is governed by the Fermi–Dirac distribution function f (E) =
1 1 + exp[(E − E F )/kT ]
(4.54)
where E F is the Fermi level. For nondegenerated semiconductors where E − E F > 3kT, the Fermi–Dirac distribution function is simplified to the Boltzmann distribution function and (4.52) is solved analytically. For degenerated semiconductors where E – E F  is less than a few kT, the Fermi–Dirac distribution function cannot be simplified. Using the DOS and f (E) expressed above, one obtains
134
4 Compound Semiconductor Crystals
⎧ √ ∞ ⎪ 1 2m ∗e 3/2 E − Ec ⎪ ⎪ ⎪ n= dE ⎪ 2 2 ⎪ 2π 1 + exp[(E − E F )/kT ] ⎨ Ec
√ ∗ 3/2 Ev ⎪ ⎪ 1 2m h Ev − E ⎪ ⎪ ⎪ p = dE ⎪ ⎩ 2π 2 2 1 + exp[(E F − E)/kT ]
(4.55)
−∞
By replacing η = (E F − E c )/kT and ξ = (E − E c )/kT , the electron concentrations has the form of √ ∞ ξ 1 2m ∗e kT 3/2 dξ n= 2π 2 2 1 + exp[ξ − η]
(4.56)
0
We can reduce (4.56) to a more convenient form by using the Fermi–Dirac integrals defined as 1 F j (η) = Γ ( j + 1)
∞ 0
ξj dξ 1 + exp[ξ − η]
where (j + 1) is the Gamma function. With j = 1/2 and (3/2) = and (4.57), then n = Nc F1/2 (η)
(4.57) √
π /2 in (4.56)
(4.58)
where N c is the effective DOS and F 1/2 (η) is the Fermi–Dirac integral of the order j = 1/2. Their expressions are 2π m ∗e kT 3/2 Nc = 2 and h2 2 F1/2 (η) = √ π
∞ 0
√
ξ dξ 1 + exp[ξ − η]
Table 4.4 lists the Fermi–Dirac integral of orders 1/2 as a function of the reduced Fermi energy η.
1.0 1.2 1.4 1.6 1.8 2.0 2.2 2.4 2.6 2.8 3.0 3.2 3.4 3.6 3.8 4.0
1.5756 1.7900 2.0221 2.2720 2.5393 2.8237 3.1249 3.4423 3.7755 4.1241 4.4876 4.8653 5.2571 5.6623 6.0806 6.5115
η
0.12930 0.15642 0.18889 0.22759 0.27353 0.32780 0.39154 0.46595 0.55224 0.65161 0.76515 0.89388 1.0387 1.2003 1.3791 1.5756
4.0 4.2 4.4 4.6 4.8 5.0 5.2 5.4 5.6 5.8 6.0 6.2 6.4 6.6 6.8 7.0
– 2.0 – 1.8 – 1.6 – 1.4 – 1.2 – 1.0 – 0.8 – 0.6 – 0.4 – 0.2 0.0 0.2 0.4 0.6 0.8 1.0
– 4.0 – 3.9 – 3.8 – 3.7 – 3.6 – 3.5 – 3.4 – 3.3 – 3.2 – 3.1 – 3.0 – 2.8 – 2.6 – 2.4 – 2.2 – 2.0
0.01820 0.02010 0.02220 0.02451 0.02706 0.02988 0.03299 0.03641 0.04019 0.04435 0.04893 0.05955 0.07240 0.08794 0.10671 0.12930
Table 4.4 Fermi–Dirac integral of order +1/2, F 1/2 (η), as a function of reduced Fermi energy η η F1/2 η F1/2 η F1/2 6.5115 6.9548 7.4100 7.8769 8.3550 8.8442 9.3441 9.8546 10.375 10.906 11.447 11.997 12.556 13.125 13.703 14.290
F1/2 7.0 7.2 7.4 7.6 7.8 8.0 8.2 8.4 8.6 8.8 9.0 9.2 9.4 9.6 9.8 10
η
F1/2 14.290 14.886 15.491 16.104 16.725 17.355 17.993 18.639 19.293 19.954 20.624 21.301 21.986 22.678 23.378 24.085
4.3 Free Carrier Concentration and the Fermi Integral 135
136
4 Compound Semiconductor Crystals
For the hole concentration in the valence band, it is convenient to set a new parameter ξp = (E v − E)/kT = −ξ − E g /kT = −(ξ + χ). The integral becomes ∞ ξp 1 2m ∗h kT 3/2 dξ p = Nv F1/2 (−χ − η) (4.59) p= 2 2 2π 1 + ex p ξ p + χ + η 0
or p = Nv F1/2
Ev − EF kT
and Nv = 2
2π m ∗h kT h2
3/2 (4.60)
We assume E v = 0. For nondegenerate ntype semiconductors, where E c − E F kT or F 1/2 (η) 1 or n N c , the Fermi–Dirac distribution can be approximated by Boltzmann distribution function. f (E) ≈ exp[−(E − E F )/kT ]
and
n = Nc exp[−(E c − E F )/kT ]
(4.21)
For ptype semiconductors, carrier concentration equation analogous to this is expressed as p = Nv exp[−(E F − E v )/kT ]
(4.61)
For example, the calculated carrier concentration of a nondegenerate ntype semiconductor with E F − E c = –2kT, using Boltzmann approximation, is n = Nc exp(−2) = 0.13534Nc The Fermi–Dirac integral approach using η = –2 leads to n = 0.12390N c . The calculated electron concentrations using both approaches are quite comparable with a small error of ~4.7%. Now, if the Fermi level is moving closer to E c , say E F − E c = –kT, the calculated carrier concentration error using Boltzmann approximation increases to 12%.
4.3.2 Free Carrier Concentrations in 2D Semiconductor Structures For semiconductors with only 2D spatial freedom, e.g., in a quantum well, the carrier density is
4.3 Free Carrier Concentration and the Fermi Integral
∞ n 2D =
D2D (E) f (E)dE= Ec
137
1 m ∗e ∞ ∫ dE π 2 Ec 1 + exp[(E − E F )/kT ]
(4.62)
By replacing η=
E − Ec EF − Ec and ξ = kT kT
(4.63)
the electron concentrations has the form of n 2D =
1 m ∗e kT ∞ ∫ dξ π 2 0 1 + exp[ξ − η]
(4.64)
The integral is the Fermi–Dirac integral of zero order (j = 0) F0 (η) =
1 1 ∞ ∫ dξ Γ (1) 0 1 + exp[ξ − η]
(4.65)
where (1) = 1 is the Gamma function. The Fermi–Dirac integral of zero order can be solved analytically and has a solution F0 (η) = ln 1 + exp(η)
(4.66)
Thus the 2D carrier density has a form of n 2D = Nc2D ln{1 + exp[(E F − E c )/kT ]}
(4.67)
where Nc2D = m* kT /πè2 . For a nondegenerate 2D system, the Fermi–Dirac distribution can be approximated by Boltzmann distribution function. Thus, n 2D = Nc2D exp[(E F − E c )/kT ]
(4.68)
In the highly degenerate 2D case, E F > E c , exp(n 2D /Nc2D ) 1 and n 2D ≈ Nc2D
EF − Ec kT
(4.69)
4.3.3 Carrier Concentration in the Multiple Valley Limit When the energy differences between conduction band minimums along different crystallography directions are small, electron distribution is not limited to the lowest band. Depending on the energy separation between E F and the conduction band
138
4 Compound Semiconductor Crystals
minima in , L, and Xdirections, the electron distribution in each valley can be calculated. Let ηi =
E F − E ci for i = Γ, L , and X valley kT
(4.70)
In a nondegenerate semiconductor the free carrier concentration including contributions from all valleys is n = NcX exp(η X ) + NcL exp(η L ) + NcΓ exp(ηΓ )
(4.71)
3/2 ∗ −3 2π m ∗ei kT 3/2 19 m ei T cm . = 2.5 × 10 2 h m 0 300 In the case of degenerate semiconductors, one obtains n = i Nci F1/2 (ηi ).
where Nci = 2
4.4 Surface States in Compound Semiconductors In bulk compound semiconductor, the atomic bonds take the sp3 configurations to form the zincblende crystal structure. A side view of the (110) surface along the [001] direction is shown in Fig. 4.19a where both group III and group V atoms are presented. When cleaving, the surface atoms take a relaxed configuration. In GaAs, due to their bond length difference and to minimize energy, on the (110) surface, the As bonds (~1.18 Å) move outward and the Ga bonds (~1.26 Å) move inward after the bonds are broken from the surface (Fig. 4.19b). To minimize their bond energies, the surface bonds of As and Ga atoms are taking s2 p3 and sp2 configurations, respectively, rather than the sp3 configuration of the bulk bonds, and form ‘dangling’ surface bonds. These bonds are available for strong interactions with atoms and molecules of the ambient. The surface states are formed near the center of the forbidden gap as a result of interactions between the ’dangling’ surface bonds and contamination
Fig. 4.19 a Bulk structure of the (110) surface, and b the relaxed configuration of (110) surface of a zincblende semiconductor
4.4 Surface States in Compound Semiconductors
139
and surface imperfections. The surface imperfections are generated by deposited metal, which induces antisite defects or vacancies near the interface. In silicon, the exposed surface atoms are the same and impose less severe surface problems. On polar (100) and (111) surfaces of III–V compounds, the surface atoms do not retain their ideal bulk structure, but undergo surface reconstruction. Depending on the surface condition, whether it is group III or group Vrich, the surface can have different atomic arrangements that are more complex than on a (110) surface. For example, under Asrich conditions, the (100) GaAs surface atoms have periodicities ¯ twice and four times larger than the bulk atomic arrangement in the [110] and [110] directions, respectively. As a result of the surface states, the energy bands are modified near the surface. For an ideal metal–semiconductor interface, the Schottky barrier height (φ b ) is determined by the difference between the work function of the metal (φ m ) and the electron affinity of the semiconductor (χ s ) as shown in Fig. 4.20a. φ b = φ m − χs
(4.72)
In 1947, John Bardeen first recognized the importance of the semiconductor surface while studying metal–semiconductor contacts. He found that a surface space charge layer (surface states) is formed by the presence of surface defects and contaminations (Fig. 4.20b) and characterized by a midgap energy level φ 0 . If the density of surface states is sufficiently high (Bardeen limit: >1012 cm−2 ), it can pin the surface Fermi level near the middle of the bandgap independent of the doping density. He further showed that if the density of the surface states is sufficiently high (≥1013 cm−2 ), the Schottky barrier height becomes a fixed value for each semiconductor independent of the metal work function. φ b = E g − φ0
(4.73)
(a)
(b)
S
S
m
m b
Ec EF Ev
0
Ec EF Surface states
Ev
Fig. 4.20 Energy band diagram of a ideal Schottky barrier, and b metal–semiconductor barrier with high density of surface states. The Fermi level at the semiconductor surface is pinned near the midgap and represented by φ 0
140
4 Compound Semiconductor Crystals
Thus, the surface states play an important role in the physical properties of carrier transport near the semiconductor surface. Due to the nature of high surface state density, this observation has been verified in III–V compounds where the pinning of Schottky barrier heights is commonly observed. Because of this high density of surface states and the lack of robust native oxides to unpin the surface Fermi level, a high performance inversionmode metal–oxide–semiconductor fieldeffect transistor (MOSFET) based on III–V compounds was not demonstrated until late 1990s. Using in situ electron beam evaporated Ga2 O3 (Gd2 O3 ) dielectric film on a clean asgrown GaAs in an ultrahigh vacuum connected multiple chamber MBE growth system, MOS structures have been successfully fabricated on GaAs with a low interface trap density for the first time. The unpinning of the GaAs Fermi level results from the Gd2 O3 restoring the surface As and Ga atoms to nearbulk charge. Later, high performance MOSFETs were demonstrated using ex situ atomic layer deposited (ALD) highκ Al2 O3 and HfO2 films as the gate dielectrics on GaAs and other III–V materials. The metal alkyls used in ALD dielectric process, in particular, trimethyl aluminum for Al2 O3 deposition, enable unpinning the Fermi levels on III–V semiconductors. A more detailed discussion of the development of III–V MOSFETs can be found in Chap. 9. In semiconductors, the danglingbond energy is typically located in the middle of the bandgap, and the interface trap density (Dit ) increases exponentially in the energy ranges close to the band edges. Over the years, a variety of models of semiconductor surface pinning energy were developed. Among others, the charge neutrality level (CNL)based model is more related to the band structures of III–V channel materials and offers a realistic explanation of all experimental results on III–V MOSFETs. The CNL energy level represents a weighted average value over the density of states (DOS). CNL is pushed away by the large DOS of the conduction and valence bands, as shown in Fig. 4.21. Therefore, the semiconductor surface pinning energy CNL is located inside the forbidden gap. If the Fermi level E F is above CNL, the states are of acceptor type and negatively charged if the states are occupied. If the Fermi level E F is below CNL, the states are of donor type and positively charged if the states are occupied. The CNL values above the valence band edges are determined by averaging values derived from various theoretical models as shown in Table 4.5. In general, the calculated CNL is in close agreement with Schottky barrier heights (φ bv ) on ptype IIIV compounds. In general, the surface pinning energies (φ 0 ) calculated from different models are in close agreement with Schottky barrier heights (φ bv ) on ptype III–V compounds (Table 4.5). Figure 4.22 shows the measured Fermi levels on cleaved (110) GaAs, GaSb, and InP surfaces deposited with different metals and overlayers in vacuum. Indeed, the Fermi level is pinned on these compounds and the surface pinning energy matches well with φ bv . Note that in GaSb and InP, both n and ptype materials, the pinning energies are closer to the valence band and conduction band, respectively.
4.4 Surface States in Compound Semiconductors
141
Fig. 4.21 CNL is a weighted average of DOS. A high DOS in the valence band tends to push the CNL toward the conduction band and vice versa. Reprinted with permission from [15], copyright AIP Publishing
Table 4.5 Schottky barrier height (ptype semiconductor) and charge neutrality level (CNL) data of selected III–V compounds [15] Material
AlP
AlAs
AlSb
GaP
GaAs
GaSb
InP
InAs
InSb
φ bv (eV)
1.27
1.002
0.47
0.797
0.562
0.07
0.857
0.58
0.04
CNL (eV)
1.3
0.92
0.4
0.8
0.55
0.06
0.6
0.50
0.15
This indicates that the nature and density of surface states are different for each material.
4.5 III–V Compound Semiconductors 4.5.1 Lattice Constant For binary compounds, all physical parameters of the material are fixed. Thus, they have zero degrees of freedom. By mixing two binaries with a common element, one can form a ternary compound. Two group III or group V elements can share the same sublattice to form III–III –V or III–V–V ternary alloy, respectively. Ternary compounds have one degree of freedom in selecting lattice constant or energy bandgap. The lattice constant, a0 , varies linearly with the alloy composition, following Vegard’s law. Thus, the lattice constant of a ternary compound Ax B1−x C can be expressed as a linear combination of lattice constants of binaries AC and BC.
142
4 Compound Semiconductor Crystals
Fig. 4.22 Fermi pinning level positions for a range of overlayers on GaAs, GaSb, and InP (110) surfaces. Circles represent ntype and triangles represent ptype materials. Reprinted with permission from [16], copyright AIP Publishing
a0 (x) = xaAC + (1 − x)aBC = aBC + (aAC − aBC )x
(4.74)
where x is the composition fraction of binary AC and aMN is the lattice constant of binary MN. The lattice constant and bandgap energy relationship of a number of III–V binary compounds are shown in Fig. 4.23. Furthermore, the quaternary compounds have two degrees of freedom in selecting the lattice constant and energy bandgap independently. The quaternary region in Fig. 4.23 is bounded by either three or four ternaries. In the former case, a typeII quaternary Ax By C1−x−y D such as Gax Aly In1−x−y As is formed by three ternaries ABD, BCD, and ACD. Elements A, B, and C share the same sublattice sites as group III atoms, and D is a group V element. The lattice constant of this III–III –III –V quaternary follows Vegard’s law as a0 (x, y) = aAD x + aBD y + aCD (1 − x − y)
(4.75)
The other quaternary compounds ABx Cy D1−x−y formed by one group III element and three group V elements also fall into this category. It has a III–V–V –V form
4.5 III–V Compound Semiconductors
143
Fig. 4.23 Lattice constant as a function of bandgap energy of III–V compound semiconductors. The bandgap energy of ternaries follows the line connecting the constituent binaries. Solid and dashed lines indicate direct and indirect bandgap, respectively
and follows Vegard’s law as a0 (x, y) = aAB x + aAC y + aAD (1 − x − y)
(4.76)
In the latter case, a typeI quaternary Ax B1−x Cy D1−y is formed by four ternaries ABC, ABD, ACD, and BCD. The group III and group V sublattices are shared by A, B, and C, D, respectively, to form the III–III –V–V quaternary. Its lattice constant is a0 (x, y) = aAC x y + aAD x(1 − y) + aBC (1 − x)y + aBD (1 − x)(1 − y)
(4.77)
For example, the lattice constant of the Gax In1−x Asy P1−y alloy is given by a(x, y) = 5.8687 − 0.4175x + 0.1896y + 0.0124x y Figure 4.24 shows the linear variation of lattice constant with composition in Gax In1−x Asy P1−y alloy following Vegard’s law. In theory, one can mix three III–III –V ternaries with the same group III elements but three different group V elements to form a penternary or quinternary alloy III– III –V–V –V . The lattice constant and bandgap coverage do not extend beyond what one can achieve with quaternaries. Therefore, there have been few reported results on quinternary. In addition, there are physical limits that prevent the formation of compounds in certain composition ranges, under equilibrium growth conditions, where a miscibility gap exists. As shown in Fig. 4.8, the nearestneighbor distance of alloys is not changed significantly. In ternary and quaternary compounds, the distance between group III and group V atoms only changes by 0.4), the alloy has a minimum energy gap in the X valley and the bandgap becomes indirect. For determining the band parameters of quaternary alloy from those of the constituent ternary alloys, a number of approaches with different degree of uncertainties have been developed. A widely adopted method derived using interpolation procedure is shown first. For the typeI quaternary Ax B1–x Cy D1−y , the band parameter is expressed as a weighted sum of the related ternary values as x(1 − x)[yTABC (x) + (1 − y)TABD (x)] x(1 − x) + y(1 − y) y(1 − y)[x TACD (y) + (1 − x)TBCD (y)] + x(1 − x) + y(1 − y)
Q(x, y) =
(4.80)
where T ij ’s represent the ternary semiconductor parameters following (4.78). For typeII quaternaries such as ABx Cy D1−x−y , the band parameter has the form of Fig. 4.25 Composition dependence of the direct energy gap and the indirect energy gap X and L for Alx Ga1−x As
146
4 Compound Semiconductor Crystals
Q(x, y) = x BAB + y BAC + (1 − x − y)BAD − x yCABC − x(1 − x − y)CABD − y(1 − x − y)CACD
(4.81)
where Bij ’s represent the binary semiconductor parameters, and C’s are ternary bowing parameters. Nevertheless, fitting calculated quaternary alloy parameters to experiments is necessary to reach a suitable description of a particular quaternary alloy system. For example, the bandgap of the most important quaternary Gax In1−x Asy P1−y as a function of alloy composition is listed as [17] E g Gax In1−x As y P1−y = 1.35 + 0.668x − 1.068y − 0.069x y + 0.758x 2 + 0.078y 2 − 0.322x 2 y + 0.03x y 2
(4.82)
The composition dependence of energy gap for a quaternary alloy is constructed from energy bandgap versus composition (E g –x, y) relations of the four constituent ternaries. As an example, Fig. 4.26 shows a 3D composition–bandgap energy plot for the quaternary alloy Gax In1−x Asy P1−y . On each sidewall is the E g –x, y relation of one of the four ternary alloys. The four ternaries form the boundary of the quaternary energy gap surface. The base of the 3D plot gives the composition in terms of x and y. The intersection of the direct and indirect energy gap surfaces indicates that most of this system is in the direct bandgap region covering 0.36 to ~2 eV. For practical applications, the compositions latticematched to InP are of considerable interest because Gax In1−x Asy P1−y has an energy gap that covers from 0.74 to 1.35 eV. This allows the construction of a wide range of Gax In1−x Asy P1−y /InP heterostructures for photonic as well as highspeed device applications. Fig. 4.26 Composition dependence of the bandgap energy surface of the quaternary Gax In1−x Asy P1−y alloy. Each sidewall represents the bandgap energy–composition relationship of a constituent ternary alloy. The square base shows the composition in terms of x and y
4.5 III–V Compound Semiconductors
147
Fig. 4.27 xy compositional plane for Gax In1−x Asy P1−y . The xy coordinate of any point in the plane gives the composition. The curved lines are constant direct bandgap energy values that were obtained by projection from the direct energy surface in Fig. 4.26. The composition lattices matched to InP and GaAs are shown as straight lines connected to InP and GaAs corners, respectively
From Fig. 4.26 we can construct the energy gap–lattice constant–composition diagram using the projection of the energy gap surface onto the xy plane. This diagram is given in Fig. 4.27. The constant bandgap energy lines are plotted for a function of composition (x, y). The two straight lines originating from GaAs and InP corners represent the latticematch compositions to GaAs and InP, respectively. The interpolations used above by requiring only the boundary binary and ternary values satisfy a necessary but not sufficient condition for describing the quaternary alloy property inside those boundaries. Thus, it is necessary to determine the quaternary bowing parameter for a better description of the quaternary function Q(x, y). A multivariable quadratic interpolation algorithm has been developed to identity the intrinsic quaternary bowing parameter for modeling the compositional dependence of quaternary alloy bandgaps [18]. For a quaternary alloy Ax B1−x Cy D1−y , the material parameter function Q(x, y) can be plotted as a surface domain enclosed by four boundaries similar to the composition dependence of the bandgap energy surface shown in Fig. 4.26. The four corners of the surface are defined by four binary alloys, and their material parameters are BAC , BAD , BBC , and BBD . Following (4.78), the ternary parameter expressions are TABV = x BAV + (1 − x)BBV + x(1 − x)CABV , V = C, D
(4.83a)
TIIICD = y BIIIC + (1 − y)BIIID + y(1 − y)CIIICD , III = A, B
(4.83b)
148
4 Compound Semiconductor Crystals
where C III−V is the alloy bowing parameter. The quaternary parameter can be expressed in two paths with either x mixing or y mixing: Q CD = yTABC (x) + (1 − y)TABD (x) + y(1 − y)DCD (x),
(4.84a)
Q AB = x TACD (y) + (1 − x)TBCD (y) + x(1 − x)DAB (y).
(4.84b)
Requiring the quaternary function Q(x, y) to be unique inside the quaternary surface domain gives QAB = QCD . D is the quaternary surface bowing parameter and can be estimated as DCD = xCACD + (1 − x)CBCD + x(1 − x)D1 ,
(4.85a)
DAB = yCABC + (1 − y)CABD + y(1 − y)D2 , and
(4.85b)
D1 = D2 = D. Therefore, the quaternary material parameter function Q(x, y) can be expressed as Q(x, y) = y(1 − x)BBC + x y BAC + (1 − y)x BAD + (1 − x)(1 − y)BBD + x(1 − x)(1 − y)CABD + x(1 − x)yCABC + (1 − x)y(1 − y)CBCD + x y(1 − y)CACD + x(1 − x)y(1 − y)D
(4.86)
Letting BBC = B1 , BAC = B2 , BAD = B3 , BBD = B4 , and C ABC = C 12 , C BCD = C 14 , C ACD = C 23 , C ABD = C 34 , the above equation can be compacted into the following form: ⎤ ⎤⎡ ⎡ (1 − x) B1 C12 B2 (4.87) Q(x, y) = y y(1 − y) (1 − y) ⎣ C14 D C23 ⎦⎣ x(1 − x) ⎦ x B4 C34 B3 By matching experimental bandgap values of a quaternary alloy with calculations, the quaternary bowing parameter D is identified and listed in Table 4.6. This equation is valid for both typeI and typeII quaternary alloys. For example, the composition of Gax In1–x Asy P1−y typeI alloy (III–III –V–V ) can be expressed as [B1y B4(1–y) ](1–x) [B2y B3(1–y) ]x with B1 = InAs, B2 = GaAs, B3 = GaP, and B4 = InP. For typeII quaternary alloys with the form of III–III –III –V, one binary can be assigned twice in the same row or column of the alloy matrix with a zero ternary bowing parameter (i.e., B2 = B3 , C 23 = 0). The composition of Alx (Gay In1–y )1−x P typeII alloy is then given by [B1y B4(1–y) ](1–x) B2x . The necessary bandgap and bowing parameters of binary and ternary alloys as well as the quaternary bowing parameters needed in (4.87) for calculating III–V quaternary semiconductor alloy bandgaps are
4.5 III–V Compound Semiconductors
149
Table 4.6 Bowing parameters of ternary and quaternary III–V semiconductor alloys
AlP –0.22 (–0.22) –
AlAs –0.8 (–0.28) –0.15
AlSb –2.7 (–2.7) –
AlP
0.48 (–0.38) 0.19 0 –0.7 (0) –0.15 –2.5 –0.43 (0) –0.25 0 0.48 (–0.38) 0.19
InP –0.1 (–0.27) –0.16
InAs –0.67 (–0.6) –1.2
InSb –1.9 (–0.19) –0.75
InP
–0.65 (–0.2) 0 –0.11 –0.477 (–1.4) –0.15 –0.01 –0.415 (–0.33) –0.1 0 –0.65 (–0.2) 0
GaP –0.19 (–0.24) –
GaAs –1.43 (–1.2) –0.6
GaSb –2.7 (–1.7) –
GaP
0 (–0.13) – 0 0.127–1.31x (–0.055) 0 0 –0.044 (0) –0.3 0 0 (–0.13) –
AlP
DAlInGaP = –0.10 (–0.07)
–0.22 (–0.22) –
AlAs
DAlInGaAs = 0.03
–0.8 (–0.28) –0.15
AlSb –2.7 (–2.7) –
AlP
DAlInGaSb = –2.5
DAlInGaP = –0.10 (–0.07)
The numbers between two binary alloys are: First row—the bowing parameter of the direct bandgap ternary alloy (C ij ), second row—the numbers in the parentheses are the ternary bowing parameters of the indirect bandgap, and third row—the ternary bowing parameter of spinorbit splitting so . Numbers in the shaded boxes are bowing parameters of quaternaries (D) associated with four neighboring binary alloys that form typeI quaternary alloys. Bowing parameters of typeII quaternaries associated with three constituent binary alloys in the same row are shown in the last column [18, 19]
listed in Table 4.6. As examples, the composition dependence of bandgap energy diagrams of both typeI and typeII quaternary alloys are calculated and shown in Fig. 4.28.
4.6 III–N and Dilute III–V–N Compound Semiconductors 4.6.1 III–N Compounds AlN, GaN, InN, and their alloys can crystallize in both wurtzite and zincblende lattice structures. Most of the current substrate materials used to grow these compounds have wurtzite structure, which enhances the formation of the same lattice structure. Therefore, all III–N compounds considered here have a wurtzite crystal structure and can be described by a and caxis lattice constants. However, under certain conditions, it is possible to grow zincblende structure GaN crystals. Due to the lack of suitable substrates, wurtzite III–N epitaxial layers have been grown on sapphires (Al2 O3 ) and SiC along the [0001] direction. Usually, the resulting epilayers contain high density of threading dislocations (≥109 cm−2 ) extending from the heterointerface toward
150
4 Compound Semiconductor Crystals
Fig. 4.28 Examples of calculated composition dependence of bandgap energy diagrams of typeI (Gax In1−x Asy Sb1−y , top) and typeII (Alx Gay In1−x−y P, bottom) III–V quaternary alloys. Available latticematched substrates are shown in thick straight lines, and the shaded area indicates the region with indirect bandgap. Reprinted with permission from [18], copyright AIP Publishing
the surface. Therefore, there has been a continuous effort to develop large area GaN substrate technology. The wurtzite structure GaN consists of two closely spaced hexagonal lattices as described in Sect. 2.4, one formed by gallium atoms and the other by nitrogen atoms. It has ionicity about 0.5 and shows more ionic properties than covalent properties. Thus, one can simply say that an electron is transferred from an N atom to a Ga atom in the wurtzite GaN crystal to form a Ga– anion and N+ cation. Looking along the caxis, as shown in Fig. 4.29, reveals that the (0001) planes
4.6 III–N and Dilute III–V–N Compound Semiconductors
151
Fig. 4.29 Crystal structure of wurtzite GaN along [0001] direction. Reprinted with permission from [20], copyright AIP Publishing
are alternating anion layers and cation layers with the Gaplane and Nplane terminating (0001) and 0001¯ surfaces, respectively. The ionic bonds linking neighboring (0001) planes with charges generate a spontaneous polarization (PSP ) in opposing the direction of 0001¯ . In addition, we also notice a large latticemismatch between GaN and AlN (a/a = 2.4%, c/c = 3.9%). When coupled with the large piezoelectric constants (~1 versus 0.01 in III–V’s), a strong straininduced polarization or piezoelectric polarization (PPE ) forms in IIIN heterostructures. The direction of the polarization follows dilation or contraction of the caxis. The existence of significant spontaneous and piezoelectric polarizations in IIIN heterostructures leads to unique electronic and photonic properties. IIIN layer structures are currently grown using either MBE or MOCVD. These epitaxy techniques will be described in more detail later in Chap. 5. In MBE, molecular beams of Ga and Al are generated from effusion cells using elemental Ga and Al as source materials. Due to the large bond strength of N2 , it is impractical to thermally dissociate N2 into atomic N. Instead, in plasmaassisted MBE (PAMBE), an RF plasma source is generally used to generate atomic nitrogen and N+ for IIIN growth. Ammonia (NH3 ) has also been used as a nitrogen source by direct thermal dissociation on the heated substrate surface at a temperature of ~800 °C. MBE layers are usually grown at ~800 °C directly on (0001) sapphire or cAl2 O3 under Garich surface conditions to achieve a high layer quality. This particular MBE growth condition yields Nterminated Bface or Nface layers, i.e., the GaN growth direction is along 0001¯ capped with a top nitrogen plane. Polarity reversal into Gaterminated Aface or Gaface layer is achievable by inserting a thin AlN layer into the structure. For IIIN layers grown by MOCVD, metalorganics such as trimethylaluminum (TMA) and triethylgallium (TEG) are used to deliver Ga and Al, respectively, and ammonia is used as the nitrogen source. In MOCVD process, IIIN materials are grown at much higher temperatures (~1050 °C) than in MBE. To maintain material quality, very high nitrogen flow inside the MOCVD growth chamber is required. In
152
4 Compound Semiconductor Crystals
Table 4.7 Band structure parameters for wurtzite IIIN binaries [21, 22]
Parameters
GaN
AlN
InN
a (Å)
3.189
3.112
3.54
c (Å)
5.185
4.982
5.70
E gΓ (eV) @ 300 K
3.438
6.138
0.64
addition, a lowtemperature grown Al(Ga)N nucleation layer on (0001) sapphire is needed before the growth of GaN. The nitrogenrich growth condition for the nucleation layer yields a Gaterminated Aface or Gaface layer and a growth direction along [0001] capped with a top gallium plane. This growth direction is opposite to the MBE grown nitrides and causes a sign change in spontaneous polarization. The composition dependences of the energy gaps for the ternary alloys AlGaN, GaInN, and AlInN follow the usual quadratic form, similar to other III–V alloys, of (4.79). E g (Ax B1−x D) = x E g (AD) + (1 − x)E g (BD) + x(1 − x)C
(4.88)
where C is the bowing parameter. The bowing parameter is always negative for these alloys, which reflects a reduction of the alloy energy gaps. The lattice constants, both in (0001) plane (a) and along caxis (c), and energy gaps of the IIIN binaries are listed in Table 4.7. Using bowing parameters of −0.7, −1.4, and −2.5 in AlGaN, GaInN, and AlInN, respectively, along with bandgap energies of binaries, the composition dependence of the direct energy gap on the lattice constant in (0001) plane (a0 ) for these wurtzite structure IIIN ternary alloys is plotted in Fig. 4.30. Fig. 4.30 Composition, in terms of lattice constant in the (0001) plane (a), dependence of the direct energy gap for AlGaN, GaInN and AlInN alloys
4.6 III–N and Dilute III–V–N Compound Semiconductors
153
One interesting property about GaN is the doping behavior. GaN can be doped easily with shallow donors of Si and Ge above 1019 cm−3 . The Si donor ionization energy is about 12–17 meV. However, doping GaN with acceptors to obtain a high concentration of holes was a difficult problem until the late 1980s. It was discovered that ptype doping had been limited by hydrogen passivation of acceptors. To activate hydrogen passivated Mg acceptors, the Mgdoped GaN requires a lowtemperature (~300 °C) heat treatment in the form of lowenergy electron beam irradiation treatment or thermal annealing in vacuum or in nitrogen atmosphere to dissociate hydrogen atoms which form complexes with Mg atoms. One drawback of Mg doping in GaN is its high acceptor ionization energy of ~150 meV which leads to a low doping efficiency. Currently, hole concentrations of mid 1017 cm−3 and mid 1018 cm−3 are achievable in MOCVD and MBE grown layers, respectively.
4.6.2 Dilute IIIVN Compounds The composition dependence of the energy gap for the III–V ternary alloys usually does not follow Vegard’s law due to the randomness in lattice atom distribution and bond length variation. The deviation from a linear interpolation between the two binaries is accounted for by the bowing parameter. When mixing III–V compounds with a small fraction (usually ≤ 2–3%) of nitrogen in dilute nitride compounds such as GaAsx N1−x and GaPx N1−x , a very large bowing in bandgap energy exists (Fig. 4.31). This unusual behavior is probably due to the extremely large bond length difference between N and other group V elements (Table 4.1) and/or the unique isoelectronic property of N in III–V alloys. Isoelectronic centers are formed by substituting one atom of the crystal with another atom of the same valence but with large differences in electronegativity and bond length. The isoelectronic center was first observed in GaP:N where a localized potential well is formed around the nitrogen atom. This potential well allows a nitrogen atom to capture an electron, which in turn can bind a hole by Coulomb attraction, thus forming a bound exciton. A more detailed discussion of isoelectronic traps can be found in Chap. 8. It is the interaction between the spatially localized N isoelectronic level and the conduction band of the underlying nonnitride semiconductor that leads to a splitting of the conduction band into two subbands and a large reduction of the fundamental bandgap. According to the band anticrossing (BAC) model, if the effect on the valence bands is completely neglected, the dispersion relations for the two coupled subbands are expressed as E ± (k) =
! 2 1 C E (k) + E N ± E C (k) − E N + 4V 2 x 2
(4.89)
where E C (k) is the conduction band dispersion of the unperturbed nonnitride semiconductor, E N is the position of the nitrogen isoelectronic impurity level in that
154
4 Compound Semiconductor Crystals
(a)
(b)
Fig. 4.31 a Energy bandgap of GaAs1−x Nx as a function of nitrogen fraction x. b BAC model calculated indirect bandgap energy of GaP1−x Nx along with experimental data. Reprinted with permission from [23], copyright IOP
semiconductor, V is the interaction potential between the two bands, and x is the fraction of nitrogen in the alloy. The values of E N and V for the dilute III–V–N quaternary alloy Ga1−x Inx AsN are [1.65(1–x) + 1.44x − 0.38x(1–x)] and [2.7(1–x) + 2.0x − 3.5x(1–x)], respectively. The values of E N and V are reduced to 1.65 and 2.7, respectively, for GaAsN. As an example, the anticrossing characteristics of the
4.6 III–N and Dilute III–V–N Compound Semiconductors
155
Fig. 4.32 Conduction band dispersion relations for GaAs0.99 N0.01 at room temperature from the BAC model (solid curves). The unperturbed GaAs conduction band (dashed curve) and the position of the N level (thin dashed line) are also shown. Reprinted with permission from [21], copyright AIP Publishing
dispersion relations for the two coupled conduction bands in GaAs0.99 N0.01 are shown in Fig. 4.32. The fundamental energy gap is now governed by the transition from E – to the top of the valence band. One precaution is that the BAC model considers only the interaction between a single, spatially localized nitrogen level and the conduction band of the underlying nonnitride semiconductor. It neglects not only mixing with the L and X valleys, but also nitrogen pairs and clusters. Therefore, the predictive power of the BAC model for an indirect bandgap material, e.g., GaPx N1−x , is more limited. Problems 1.
2. 3.
The diatomic chain model considered for phonon (lattice vibration) characteristics have identical springs but different masses. A model with alternating spring constants, α and β, but the same mass, m, is appropriate for Si, Ge or diamond crystal. Calculate the ωk dispersion relation for crystals with a diamond structure. Determine what fraction of holes in Si and InP are heavy holes. Let m ∗hh (Si) = 0.537, m ∗lh (Si) = 0.153m0 , m ∗hh (InP) = 0.56m0 , m ∗lh (InP) = 0.12m0 . For Ge: m ∗L = 1.59m0 , m ∗T = 0.0823m0 , m ∗hh = 0.28m0 , m ∗lh = 0.043m0 ; and for GaAs: m ∗e = 0.067m0 , m ∗hh = 0.50m0 , m ∗lh = 0.076m0 . (a) (b) (c) (d)
4.
Determine the density of states effective mass mDOS of Ge. Calculate N c and N v of Ge at 300 K. Determine what fraction of holes in Ge and GaAs are heavy holes. Comment on the roomtemperature mobility difference between Ge (μe ~ 3900, μh ~ 1800 cm2 /Vs) and GaAs (μe ~ 9000, μh ~ 400 cm2 /Vs).
The energy differences E c − E F ≥ 3kT and E F − E v ≥ 3kT are defined as thresholds for nondegenerate ntype and ptype semiconductors, respectively.
156
4 Compound Semiconductor Crystals
(a) Determine the n and ptype carrier densities for Si and GaAs at the threshold of nondegeneracy. Commenting the differences between n and ptype materials as well as between Si and GaAs. (b) Calculate n and ptype carrier densities of Si and GaAs at 300 K for E c – E F = 0.2kT and E F – E v = 0.2kT, respectively. 5.
For a linear extrapolation of the density of states effective mass between GaAs and AlAs, the electron effective mass for the indicated conduction band in Alx Ga1−x As is taken as m Γ = (0.067 + 0.083x)m 0 m L = (0.55 + 0.12x)m 0 m X = (0.85 − 0.07x)m 0 . The energy bandgap variations in the X, L, and Γ conduction bands are also provided as follows: E Γ (eV) = 1.424 + 1.247x, for 0 ≤ x ≤ 0.4 E L (eV) = 1.707 + 0.645x, E X (eV) = 1.899 + 0.21x + 0.055x 2 .
6.
Determine the fraction of the electrons is in the X, L, and Γ conduction band valleys of nondegenerately doped ntype (a). Al0.3 Ga0.7 As, and (b). Al0.5 Ga0.5 As. Electron–hole pairs (EHPs) are generated by photoexcitation of an undoped Ga0.47 In0.53 As layer. The increasing EHP concentration causes the quasiFermi level of electrons and holes to move away from the equilibrium Fermi level toward the conduction band and valence band, respectively. One special condition, under a strong photoexcitation, which is important for lasers, occurs when the separation in quasiFermi levels (F c − F v ) = E g , a condition known as ‘transparency’. At what electron concentration (n = p) does the material reach transparency? You have to use Fermi–Dirac integral for both electrons and holes. For Ga0.47 In0.53 As: m ∗e = 0.041m0 , m ∗hh = 0.465m0 , and m ∗lh = 0.0503m0 . Note, at transparency, η – ζ = 0, where η = (Fc − E c )/kT and ζ = χ + η = (Fv − E v )/kT
7.
For Ge: m ∗L = 1.59m0 and m ∗T = 0.0823m0 ; for Si: m ∗L = 0.9163m0 and m ∗T = 0.1905m0 ; and for GaAs: m ∗e = 0.067m0 . The measured roomtemperature electron mobility of ntype Ge, Si, and GaAs samples doped to 2×1017 cm−3 are 2750, 600, and 4000 cm2 /Vs, respectively. (a) Calculate the average relaxation time, τ (scattering probability = 1/τ ), for Ge, Si, and GaAs.
4.6 III–N and Dilute III–V–N Compound Semiconductors
157
(b) Assume, at room temperature, the dominant scattering mechanisms in elemental semiconductors are due to lattice scatterings. The scattering due to optical phonons for Ge can be approximated as μop ∼ = 900(300/T ) exp ωop /kT − 1 The LO phonon frequency, ωop , for Ge is 6 THz. Calculate the lattice scattering mobility, μl (c) Although Ge and GaAs have a similar average relaxation time, the mobility difference is quite large. Comment on the roomtemperature mobility difference between Ge and GaAs. 8.
The ternary GaAsx Sb1−x is direct bandgap over the full composition range. It has a bandgap energy of 0.775 eV at x = 50% where it is latticematched to InP. The roomtemperature bandgap energy and lattice constant of GaAs and GaSb are 1.424 eV and 5.6533 Å, and 0.727 eV and 6.0959 Å, respectively. (a) Find the coefficients a, b, and c of the bandgap energy quadratic equation. (b) Sketch E g versus x.
9.
The ternary InAsx Sb1−x is direct bandgap over the full composition range. It has the smallest bandgap among all III–V compounds at x = 35%. The corresponding emission wavelength at that composition is 11.5 μm. The roomtemperature bandgap energy and lattice constant of InAs and InSb are 0.35 eV and 6.0584 Å, and 0.17 eV and 6.4794 Å, respectively. (a) Find the coefficients a, b, and c of the bandgap energy quadratic equation. (b) Sketch E g versus x and indicate on the sketch the bandgaps when the ternary is latticematched to AlSb (6.1355Å) and GaSb (6.09593Å).
10. Derive the quaternary direct bandgap energy as a function of compositions x and y of the quaternary alloy Gax In1−x Sby As1−y using (4.87). Make a sketch of the E g versus compositions x and y. For the isoenergy curves, show only the curve with E g = 0.6 eV, which corresponds to an eyesafe wavelength of ~2.1 μm. Estimate the compositions latticematched to InAs and GaSb on this curve. 11. From the E g versus composition sketch of the Gax In1−x Asy P1−y quaternary alloy (Fig. 4.27): (a) Find the range of bandgap energies covered by the latticematched alloys on InP and GaAs. (The lattice constant of GaP is 5.45117 Å.) (b) Find the x and y values for the alloy latticematched to Ga0.75 In0.25 As and has bandgap energy of 1.4 eV. (c) Derive the quaternary direct bandgap energy as a function of compositions x and y using (4.87). Compare the results at x = y = 0.5 with that derived from (4.82).
158
4 Compound Semiconductor Crystals
12. The alloy Alx Gay In1−x−y As is a typeII quaternary alloy. (a) Derive the quaternary direct bandgap energy as a function of compositions x and y using (4.87). (b) Make a sketch of the E g versus composition x and y. Mark clearly the boundary of the direct–indirect crossover and show the compositions latticematched to InP, which has a lattice constant of 5.86875 Å. The lattice constants of AlAs, GaAs, and InAs are 5.6605 Å, 5.65325 Å, and 6.0584 Å, respectively. (c) What is the range of the bandgap energy covered by this quaternary alloy latticematched to InP? At which compositions does it have the bandgaps corresponding to 1.3 and 1.55 μm? 13. In an effort to achieve efficient luminescence from group IV semiconductors, the Ge/αSn alloy has been investigated. The lattice constants of αSn and Ge are 6.48 Å and 5.6575 Å, respectively. The calculated transition energies along Γ , L, X valleys of the Gex Sn1−x compound are shown below. Deduce the bandgap energy as a function of composition x for the Γ valley and determine the composition range where this alloy is a semiconductor with direct bandgap energy. Note the material becomes semimetal at E g ≤ 0 eV.
References 1. 2. 3. 4. 5. 6. 7. 8. 9.
A.I. Blum, N.P. Mokrovski, A.R. Ragel. Izvest. Akad. Nauk S.S.S.R., Ser. Fiz. 16, 139 (1952) H. Welker, Z. Naturforsch. 79, 744 (1952) J.L.T. Waugh, G. Dolling, Phys. Rev. 132, 2410 (1963) B.N. Brockhouse, Phys. Rev. Lett. 2, 256 (1959) C.M. Wolfe, G.E. Stillman, W.T. Lindley, J. Appl. Phys. 41, 3088 (1970) J.C. Mikkelsen Jr., J.B. Boyce, Phys. Rev. B28, 7130 (1983) J.D. Oliver Jr., L.F. Eastman, P.D. Kirchner, W.J. Schaff, J. Cryst. Growth 54, 64 (1981) P.M. Smith, M. Inoue, J. Fre, Appl. Phys. Lett. 37, 797 (1980) L. W. James. J. P. van Dyke, F. Herman, D. M. Chang, Phys. Rev. B 1, 3998 (1970)
References
159
10. 11. 12. 13. 14. 15. 16. 17. 18. 19. 20.
A. Baldareschi, N.O. Lipari, Phys. Rev. B9, 1525 (1974) D.J. Chadi, K.J. Chang, Phys. Rev. B39, 10063 (1989) D.V. Lang, R.A. Logan, M. Jaros, Phys. Rev. B19, 1015 (1979) E.F. Schubert, K. Ploog, Phys. Rev. B30, 7021 (1984) D.E. Holmes, R.T. Chen, K.R. Elliot, C.G. Kirkpatrick, Appl. Phys. Lett. 40, 46 (1982) J. Robertson, B. Falabretti, J. Appl. Phys. 100, 014111 (2006) W.E. Spicer, I. Lindau, P. Skeath, C.Y. Su, J. Vac. Sci. Technol. 17, 1019 (1980) E. Kuphal, J. Crystaj Growth 67, 441 (1984) G.P. Donati, R. Kaspi, K.J. Malloy, J. App. Phys. 94, 5814 (2003) I. Vurgaftman, J.R. Meyer, L.R. TamMohan, J. App. Phys. 89, 5815 (2001) O. Ambacher, J. Smart, J.R. Shealy, N.G. Weimann, K. Chu, M. Murphy, W.J. Schaff, L.F. Eastman, R. Dimitrov, L. Wittmer, M. Stutzmann, W. Rieger, J. Hilsenbeck, J. Appl. Phys. 85, 3222 (1999) 21. I. Vurgaftman, J.R. Meyer, J. App. Phys. 94, 3675 (2003) 22. J. Wu, W. Walukiewicz, W. Shan, K.M. Yu, J.W. Ager III, S.X. Li, E.E. Haller, H. Lu, W.J. Schaff, J. Appl. Phys. 94, 4457 (2003) 23. J. Wu, W. Shan, W. Walukiewicz, Semicond. Sci. Technol. 17, 860 (2002)
Further Reading 1. S. Wang, Fundamentals of Semiconductor Theory and Device Physics(PrenticeHall, 1989) 2. S. Adachi, Physical Properties of III–V Semiconductor Compounds (Wiley, 1992) 3. E. F. Schubert, Doping in IIIV Semiconductors (Cambridge, 1993)
Chapter 5
Material Technologies
Abstract Highquality, singlecrystal substrates are essential for the advancement of semiconductor device technologies. The significant development of IIIV compound semiconductor electronic and photonic devices in the last several decades has been a result of the progress made in the preparation of bulk single crystals and in the various epitaxial techniques for growing thin layers. Significant improvements have been made in uniformity, reproducibility, dislocation density control, thermal stability, diameter control, and impurity and dopant control. As discussed in this chapter, single crystals of GaAs and InP have been grown from the melt by one of several techniques that include horizontal Bridgman, vertical gradient freeze (VGF), and liquid encapsulated Czochralski (LEC). Nevertheless, due to problems of the very high vapor pressure of nitrogen at the growth temperature, bulk crystals of IIInitrides are still under development. Among epitaxial growth techniques, molecular beam epitaxy (MBE) and metal organic chemical vapor deposition (MOCVD) have evolved from laboratory experiment tools into viable manufacturing technologies. Hybrid epitaxial techniques such as gas source and metalorganic MBE have also been successfully applied for the growth of many GaAs, InPbased heterostructures. In addition, postgrowth material processing techniques to modify the asgrown quantum wells and superlattices into new alloys with desired physical properties have been introduced. Using selective impurity diffusion or ion implantation, the impurityinduced layer disordering (IILD) process allows the formation of lateral heterojunctions perpendicular to quantum well and superlattice heterostructures such that devices with threedimensional carrier and photon confinement are achieved. The other postgrowth method is to wet oxidize Albearing IIIV alloys into insulators, either on the surface or between semiconductor layers, through lateral oxidation from an edge. The insulating layer provides current confinement as well as optical confinement due to a significant refractive index difference created within the heterostructure.
© Springer Nature Switzerland AG 2020 K. Y. Cheng, III–V Compound Semiconductors and Devices, Graduate Texts in Physics, https://doi.org/10.1007/9783030519032_5
161
162
5 Material Technologies
5.1 Growth of Bulk Crystals 5.1.1 Phase Equilibria In bulk crystal growth by liquid–solid reactions, an important consideration in the equilibrium is the dependence of melting temperature on atomic composition and pressure. Under one atmosphere (1 atm) pressure, the equilibrium of solid with a liquid of binary compound can be described by the temperaturecomposition phase diagram as shown in Fig. 5.1. The temperature at which the solid and liquid have the same composition is the congruent melting point (T F ). Ideally, it happens at a composition of 50% A and 50% B atoms. However, the solid at the congruent melting point does not necessarily have the ideal composition of 50%. Rather, it covers a range of composition around 50% which defines the extent of the solid phase and is called the existence region. In GaAs, the congruent melting point occurs slightly to the Garich side of the stoichiometric composition. Crystals grown with compositions in the existence region different from the 50% value lead to solids that contain nonstoichiometric defects such as vacancies, interstitials, and antisite defects. Therefore it is necessary to suppress the density of these native defects by carefully controlling the stoichiometry of the melt during crystal growth. The main difficulty of growing IIIV compound semiconductor crystals is that many of them decompose at the melting point, releasing the volatile component. The vapor pressure at the melting point is determined by the vapor pressure of the more volatile group V element rather than the group III element, whose vapor pressure is Fig. 5.1 Temperaturecomposition phase diagram of the IIIV binary compound AIII BV . T F is the congruent melting point of the compound AB at which the solid and liquid have the same composition. The existence region is greatly exaggerated
5.1 Growth of Bulk Crystals
163
Fig. 5.2 Partial pressures p of As4 , As2 , As, and Ga along the GaAs liquidus as a function of the reciprocal temperature. Reprinted with permission from [1], copyright Elsevier
lower by several orders of magnitude. Thus growth must take place under a vapor pressure of the volatile group V component to prevent depletion of the group V component from the melt and maintain a stoichiometric composition in the melt during crystal growth. Figure 5.2 shows the partial pressures of As monomers (As), dimers (As2 ), tetramers (As4 ), and Ga in equilibrium with the GaAs liquidus and the solid as a function of reciprocal temperature. Near the melting point, the vapor pressure of As (mainly As4 ) in equilibrium with GaAs (melting point 1238 °C) is ~0.9 atm, while the vapor pressure of P in equilibrium with InP (melting point 1062 °C) is ~25 atm. These high pressures call for special attentions to prevent As or P depletion from the melt during crystal growth. The growth chamber should also be properly designed to withstand high pressures used during growth. For GaN, the vapor pressure of N at the melting temperature (~2500 °C) is extremely high (PM ~ 4.5 × 104 atm). For pressure values below PM , GaN does not melt but decomposes. Thus the standard crystal growth techniques generally used for other IIIV alloys (Bridgman, VGF, LEC) cannot be adopted.
164
5 Material Technologies
5.1.2 Crystal Growth Techniques (a) Crystal growth by pulling from a crucible One of the most important techniques for the growth of semiconductor single crystals from the melt is the Czochralski pulling method. Figure 5.3 shows the basic components of a crystal puller according to the Czochralski technique. Here, the crucible contains the melt of the semiconductor material. The seeded single crystal is held in the seed holder which can be moved up and down and rotated. A furnace or an RF coil is used for heating the crucible and the melt. At the beginning of the pulling process, the seed is dipped into the melt, whose temperature is lowered until a small amount of crystalline material is solidified. The seed is then withdrawn from the melt and rotated to maintain thermal geometry and cylindrical geometry. The melt temperature is lowered slowly, and the diameter of the crystal increases. Once the desired diameter is reached, the lowering of the temperature is stopped. Growth at a constant diameter is maintained until the desired length is grown. The usual pull rates range from 1 to 10 mm/h. In this process the growth rate is determined primarily by the rate of the heat been carried away through the crystal and radiation to the surroundings from the solidliquid interface. The Czochralski technique may readily be used to grow semiconductor crystals including Si, Ge, and IIIV compounds. However, the arsenides and phosphides of indium and gallium have a relatively high vapor pressure at their moderately high melting point. Under normal conditions, these compounds decompose on melting. Fig. 5.3 Czochralski crystal growth furnace with rf induction heating
Seed Growing crystal
RF coil
Melt Crucible
5.1 Growth of Bulk Crystals
165
The result is an In or Garich melt and As or Prich vapor phase. A modified Czochralski technique to prevent loss of group V element from the melt is the encapsulation technique where the melt is covered by a thin layer of low vapor pressure molten material that is less dense. B2 O3 satisfies this requirement and is the commonly used encapsulant. The density of B2 O3 is 1.5 gcm−3 while those of GaAs and InP melts are 5.71 and 5.1 gcm−3 , respectively. It softens and begins to flow at 450 °C but is immiscible with the melts of IIIV compounds. It has a low vapor pressure of only ~0.1 torr at the melting of GaAs. In addition, the growth system is housed inside a pressure chamber such that a counter pressure of an inert gas, which is higher than the partial pressure of the group V element, can be maintained on top of the B2 O3 . This technique is called the liquid encapsulated Czochralski (LEC) technique. LEC furnaces that can be used up to pressures of 100 atm are available commercially. The LEC growth can be done by preparing the compound ex situ first and carrying out the crystal growth subsequently. Alternatively, the compound is synthesized in situ prior to growth in the same system. The second approach is called the highpressure (HP) LEC technique due to the high pressure associated with the in situ synthesis process. The direct synthesis of GaAs occurs at about 700 °C under a highpurity nitrogen or argon pressure of 60 atm. The starting materials for the synthesis are stoichiometric quantities of highpurity Ga and As. A pellet of B2 O3 is placed on top of the charge to encapsulate the melt when molten. Highpurity pyrolytic BN (PBN) crucibles are used to grow consistently pure materials. The use of PBN crucibles has become standard in the growth of undoped semiinsulating GaAs crystals. After the compound is synthesized, the temperature is increased above the melting point of GaAs, and the pressure is reduced to 2–4 atm. Singlecrystal growth then proceeds as in the conventional Czochralski technique. In the growth of InP single crystals by LEC, the compounding is done ex situ due to the extremely high pressure required. The IIInitride compounds yield further technology problems. The melting points and vapor pressures of them are extremely high. Therefore, it is difficult to apply the Czochralski technique, or even a modification of this technique such as LEC, to these compounds. (b) Horizontal gradientfreeze and Bridgman methods The gradientfreeze technique is analogous to the horizontal Bridgman method in that they both produce single crystals by gradual solidification of a molten ingot. The two methods differ only in that solidification by the gradientfreeze technique takes place by the movement of a temperature gradient along the ingot, making the entire system stationary. The horizontal Bridgman method requires the movement of either the furnace or the crucible holding the molten ingot. Figure 5.4 is the schematic of the horizontal gradient furnace used for growing GaAs, InP, and GaSb along with the temperature profile. The growth system consists of a twozone furnace: the lowtemperature zone on the left is used to control the vapor pressure of the volatile component, which is necessary to control the stoichiometry. The hightemperature zone on the right is maintained at a temperature in excess of the melting point of the
166
5 Material Technologies
Fig. 5.4 Horizontal gradientfreeze furnace and a typical temperature profile
Excess arsenic
S eed/crystal
High temp. furnace
Low temp. furnace Furnace windings
Temperature (°C)
1300
Melt
Quartz boat
1238 °C
1100 900 700 500
Distance
compound in such a manner as to provide the desired temperature gradient along the length of the melt. In this technique, a sealed quartz tube contains highpurity (6– 9’s pure) group III metal in a quartz boat at one end and excess highpurity volatile group V element (6–9’s pure) at the other end. A porous quartz plug is placed between the two zones and acts as a radiation shield and diffusion barrier. The quartz boat containing group III metal and the seed is located in the hightemperature zone of the furnace with the group III metal above the melting point of the compound. The group V vapor reacts with group III metal to form the IIIV melt. The temperature at the hightemperature zone is adjusted to melt a small part of the seed when the contact to the melt is made initially. Solidification is achieved by slowly lowering the temperature of the hightemperature zone from an equilibrium state in which the material is completely molten above the melting point, to a state in which the material is completely solid below the melting point. The temperature gradient along the length of the melt causes the freezing point to traverse from the seed end of the melt to the other. The solidified crystal has to be cooled to room temperature at a slow and even rate to reduce thermal stress induced dislocation generation. In these horizontal growth techniques, the shape of the crystal is constrained by the geometry of the quartz boat. The cross section of the crystals is typically Dshaped and seeded in the 111 direction. The (100) oriented circular wafers can be sawed from these crystals but with excessive material loss. In general, significantly lower thermal gradients, and hence reduced convective flows, in the melt and extremely low thermal stresses can be realized in the horizontal technique compared to the Czochralski technique. As a result, owing to the reduced thermal stresses and precise control of group V element overpressure, dislocation densities tend to be much less in these crystals. Typical dislocation densities in GaAs crystals grown by the horizontal Bridgman or the horizontal gradientfreeze technique are below 5000 cm−2 in 7.5 cm wide Dshaped crystals.
5.1 Growth of Bulk Crystals
167
(c) Vertical gradientfreeze (VGF) technique Today the most common process for largescale production of round InP and semiinsulating GaAs single crystals has been LEC. But the LEC technique has several inherent problems. One of the most serious drawbacks with the LEC process is the large axialtemperature gradient needed to maintain diameter control. The resulting thermoelastic stresses in the crystal have been shown to exceed the low yield strength of these compound semiconductors and create a high level of dislocations. Typical dislocation densities for undoped InP and GaAs range from 104 to l05 cm−2 . A second drawback of the LEC process is that the melt is coolest at the top surface. This leads to considerable buoyancydriven convection that creates nonhomogeneities in the crystal dopant and incorporates point defects. These drawbacks of the LEC growth of GaAs and InP have been overcome with the vertical gradientfreeze (VGF) technique where growth in low axial and radialtemperature gradients is combined with the diameter control imposed by a crucible. The VGF growth apparatus consists of a large pressure vessel that contains the heater assembly, a PBN crucible contains the seed in a well at the bottom and polycrystalline IIIV compound above it, and a group V source reservoir located at the coldest point of the growth vessel. The arrangement of the crucible in the vertical furnace and the temperature profile are shown schematically in Fig. 5.5. For growth to occur, the pressure vessel is filled with inert argon gas first to the desired pressure, and the group V heater temperature is raised to increase the group V vapor pressure inside the PBN growth vessel. When the operating group V pressure is established, the polycrystalline IIIV compound charge is melted. To begin solidification, the temperature gradient is controlled such that the liquid–solid interface sweeps upward through the melt. Crystallization starts at the seed in the bottom of Fig. 5.5 Vertical gradientfreeze (VGF) growth system and a typical temperature profile
Pressure chamber Radiation shields Top cap PBN crucible Graphite heater GaAs melt
1238 °C
GaAs crystal GaAs seed Heater winding Arsenic
Temperature
168
5 Material Technologies
the crucible. Because the crucible is cooler at the bottom than at the top, the system is thermally stabilized against convection. During the growth, the group V element from the bottom of the growth vessel sublimates to maintain the appropriate partial pressure and stoichiometry of the melt. After solidification, controlled cooling brings the crystal to room temperature at a rate that minimizes thermal stress and optimizes point defect quenching. Since the VGF system has axialthermal symmetry, low axial and radialtemperature gradients, and slow stable solidification and cooling, the produced crystals contain low levels of thermal stress and high radial uniformity of the electrical properties across wafers. These benefits translate into low dislocation densities of ≤100 to 3000 cm−2 in crystals that are 7.5 cm in diameter. This dislocation density is considerably lower than in LECgrown crystals. (d) Growth of bulk GaN crystals At present, galliumnitridebased photonic and electronic devices are manufactured mainly by heteroepitaxial methods on foreign substrates such as sapphire, silicon, and silicon carbide which lead to IIInitride epilayers with high stress, high dislocation density, and mosaic crystal structure. Due to the extremely high vapor pressure of nitrogen at the melting temperature of GaN, the standard bulk crystal growth techniques generally used for other IIIV alloys cannot be applied. Currently, the main source of GaN substrates is produced by the hydride vaporphase epitaxy (HVPE) technique on sapphire substrates. However, this method suffers from all the drawbacks of using heterogeneous substrates on which the growth is initiated: the GaN layer obtained is highly stressed and bowed. Therefore, many promising growth methods have been explored for preparing GaN bulk crystals including the high nitrogen pressure (HNP) solution growth technique, the Na flux method, and the ammonothermal growth technique [2]. In the HNP method, the decomposition of GaN is inhibited by the use of nitrogen under high pressure. The growth of single crystals is performed in molten gallium and requires temperatures of about 1500 °C and very high nitrogen pressures in the order of 1.5 × 104 atm. High quality GaN crystals have been achieved through the HNP process with a low dislocation density (1.5 diameter) GaN crystals with narrow xray diffraction peak (16 arcsec) and low dislocation density (1000 °C) are required for the growth of GaN because of high bondstrength of NH bond in ammonia precursors. In growing heterostructures by atmospheric pressure MOCVD, changing the layer composition is carried out by switching flows of metalorganic reactant mixtures. The time required to establish a stable flow with minimum turbulence in the reactor prevents the formation of a sharp interface. The growth of indiumcontaining compounds from trimethylindium (TMI) or triethylindium (TEI) is further complicated by the possible formation of adducts between hydrides and indiumalkyls. To minimize these problems, lowpressure MOCVD (LPMOCVD) has been developed. LPMOCVD is usually carried out in a reactor under reduced pressure in the range of 50–100 torr. The large reduction of system pressure and increased flow rate enhance the gasphase transfer of reactants to, and byproducts from, the substrate surface. The practical consequences of these results are very significant. Under lowpressure
182
5 Material Technologies
conditions, the high gas flow rate permits rapid establishment of new gas compositions, which lead to more abrupt changes in composition. Furthermore, a more uniform boundary layer thickness is established under high gas flow rates, leading to good uniformity in layer thickness and composition. Additionally, the reaction rate is slowed, and reaction time is reduced, which, under lowpressure conditions, leads to a minimum adduct formation and a reduced growth rate of about 2–5 μm/h. III V For the growth of AIII x B1−x C ternary compounds by MOCVD under a high V/III flow rate ratio, the solid composition x is determined by x = JAIII / JAIII + JBIII
(5.13)
where J is the flux of the group III element. For the growth of alloys with mixing on a group V sublattice (i.e., AIII CVy DV 1−y ), the solid composition y becomes a nonlinear function of vapor composition. This is because of the unequal pyrolysis rates of different group V reactants at the growth temperature. For example, in GaAs1−y Py , a very large ratio of PH3 to AsH3 is required to produce alloys with a significant phosphorus content below 750 °C.
5.5 Molecular Beam Epitaxy Pioneered by A. Y. Cho at Bell Laboratories, molecular beam epitaxy is an ultrahighvacuum (UHV) deposition technique with several important features. The MBE growth of semiconductor films takes place by the reaction of molecular beams of the constituent elements with a crystalline substrate surface held at a suitable substrate temperature under UHV conditions. The kinetically controlled MBE growth process involves a series of events: adsorption, surface migration and dissociation, and incorporation. In the case of MBE growth of GaAs, in the absence of free surface Ga adatoms, the impinging As2 molecules will simply reevaporate from the surface above 500 °C. Dissociation of adsorbed As2 and subsequent incorporation into the GaAs lattice can occur only when they encounter paired Ga lattice sites while migrating on the surface. Therefore, for the MBE growth of a stoichiometric GaAs epitaxial layer, it is required that only an excess of As species be present while the growth rate is determined by the arrival rate of the Ga flux. The unique feature of MBE is the ability to prepare epitaxial layers with atomic dimensional precision down to a few angstroms. This ability allows the preparation of novel devices with multilayered epitaxial structures tailored to meet specific needs. Because MBE is done in a UHV environment, many surface analysis techniques may be used during the growth process. This makes the MBE process a highly controllable and reproducible epitaxy method.
5.5 Molecular Beam Epitaxy
183
5.5.1 MBE Apparatus The modern MBE system uses a modular configuration that contains a number of building blocks, such as the growth chamber, the sample exchange loadlock, the surface processing chamber, and the surface analysis chamber, which are all interconnected by a UHV transfer tube. A basic MBE system for IIIV compounds is shown in Fig. 5.14. The UHV growth chamber is evacuated with a pumping stack that maintains a base pressure of 10−11 torr. In addition, a liquid nitrogencooled shroud is used to enclose the entire interior surface of the growth chamber in order to minimize contamination from residual water vapor and hydrocarbons during epitaxy. The sample exchange loadlock permits the maintenance of UHV in the growth chamber while changing substrates between successive growth runs. The substrate is typically mounted on a molybdenum substrate holder attached to a sample manipulator for precise positioning within the growth chamber. The substrate holder can rotate continuously to achieve extremely uniform epitaxial layers. Thermal radiation generated by resistance heating from behind the substrate holder is employed to heat the substrate. On the backside of the manipulator is an
Fig. 5.14 Cutaway top view of a molecular beam epitaxy system. Molecular beams are generated from effusion cells and/or gas injectors mounted on the source flange. Opening and closing of different shutters in front of effusion cell orifices determine the heterostructure grown on the heated substrate. Reprinted with permission from [6], copyright AIP Publishing
184
5 Material Technologies
ion gauge for beam flux measurements. When rotating the manipulator into position such that the movable ion gauge is facing the effusion cells, the relative flux of each beam can be estimated. The source flange on the growth chamber contains a viewport and eight or more ports for mounting effusion cells and/or gas injectors. The viewport both facilitates the mounting of an optical pyrometer for substrate temperature measurement and provides a means of directly viewing the substrate during growth. Ultrahighpurity elemental source materials and dopants loaded in PBN effusion cell crucibles are used to generate the desired molecular beams. The effusion cell temperatures are controlled to an accuracy of ±1 °C to provide the precise amount of beam flux. To initiate or terminate the molecular beam flux, each source is provided with its own externally controlled mechanical shutter. Shutters in front of the orifices can be opened and closed within a tenth of a second, which is much shorter than the typical MBE growth rate of one to two monolayers per second, resulting in abrupt interfaces in the range of one atomic layer. Therefore, the sequence of opening and closing different shutters determines the multilayer heterostructure in terms of both composition and doping profile.
5.5.2 In Situ Surface Diagnosis Techniques In addition to the components used directly for the MBE growth process, the growth chamber may contain various pieces of in situ surface analysis equipment to monitor the surface structure and control the growth conditions. For a modern MBE system to be used for the production of devices, only a reflection highenergy electron diffraction (RHEED) apparatus and a movable ion gauge in the growth chamber are essential. The RHEED apparatus provides information concerning substrate cleanliness, smoothness, and surface structure before and during growth as a function of growth conditions. To generate RHEED patterns, as shown in Fig. 5.14, a collimated beam of highenergy electrons in the range of 5–40 keV is directed at an angle of 1–2° toward the sample surface orthogonal to the molecular beam paths. Because the de Broglie wavelength of an electron at this energy is a fraction of the atomic spacing on the surface, a diffraction pattern is formed on the fluorescent screen mounted opposite the electron source. In this configuration, the sample surface can be continuously monitored without interrupting the growth procedure. On an atomically flat surface, it shows a streaked RHEED pattern normal to the shadow edge of the sample. Otherwise, the diffraction pattern from a rough surface is formed mainly in transmission through the surface asperities and exhibits a spotty appearance. Figure 5.15 is an example of the (100) GaAs surface morphology evolution during the initial stages of the MBE growth and their corresponding RHEED patterns. The clean but rough starting surface shows a spotty bulk RHEED pattern as seen in Fig. 5.15a. The RHEED pattern changes from spotty to streaky as the surface is smoothed out.
5.5 Molecular Beam Epitaxy
185
¯ and the correFig. 5.15 40 keV RHEED patterns of a (100) GaAs surface taken at azimuth [1¯ 10] sponding photomicrographs; a after chemical etching and heating to 580 °C, b after depositing 150 Å of GaAs, and c after depositing 1 μm of GaAs. Reprinted with permission from [7], copyright American Vacuum Society
In addition to the spottytostreaky transition in the RHEED patterns of a clean crystal surface during growth, additional light streaks appear halfway between the ¯ azimuth as seen in Fig. 5.15b, c. These added elongated bulk spots along the [1¯ 10] features represent the rearrangement of atoms on the surface in order to accommodate the surface dangling bonds and to minimize the surface free energy. Depending on the surfaceatom coverage conditions and the electron beam incident directions, the pattern of extra diffraction lines between the bulk streaks assumes different forms.
186
5 Material Technologies
For example, the RHEED pattern of the Asrich surface (Fig. 5.15c) shows extra ¯ azimuth and extra ¼ integral order streaks ½ integral order streaks along the [1¯ 10] ¯ azimuth (not (i.e., three additional light streaks between bulk streaks) along the [110] shown). The RHEED patterns of Garich (Gastabilized) surfaces and Asrich (As¯ and [110] ¯ azimuths. stabilized) surfaces are similar, but are interchanged along [1¯ 10] In real space, the two surface structures are related by a simple rotation of 90° about the [001] direction. The relationships between the surface structures and the growth conditions (i.e., the surface phase diagram) of (100) GaAs have been established in terms of As2 /Ga flux ratios and substrate temperatures (Fig. 5.16). From the point of view of practical GaAs growth, the Asstabilized structure is preferred. A highquality smooth (100) GaAs surface can be achieved under this condition. On the other hand, prolonged growth under a Gastabilized condition leads to a dull surface caused by the formation of Ga droplets. Overall, because of its simplicity and in situ nature, the RHEED technique is routinely used in MBE to monitor the surface cleaning process prior to epitaxial growth and to optimize growth conditions during growth.
Fig. 5.16 Arsenictogallium ratio in the molecular beam as a function of the substrate temperature when the transition of an Asstabilized (½ order) surface structure and a Gastabilized (¼ order) ¯ azimuth. During the surface structure takes place. The RHEED patterns are observed in the [1¯ 10] transition, a 1/3 order is observed. Depending on whether the substrate temperature is increasing or decreasing, two sets of transition boundaries are shown. Reprinted with permission from [7], copyright American Vacuum Society
5.5 Molecular Beam Epitaxy
187
5.5.3 Flux Control of Molecular Beams For an ideal Knudsontype effusion cell, the beam flux arriving at the substrate surface positioned at a distance d (cm) from the aperture can be calculated as follows: J = 1.118 × 1022
pA cos θ molecules/cm2 s √ d2 M T
(5.14)
where p (torr) is the pressure in the cell, A (cm2 ) is the area of the aperture, M is the molecular weight, T (K) is the temperature of the cell, and θ is the angle between the beam and the normal of the surface. However, this equation serves only as a guideline because in practice the ideal pinholesize cell aperture is enlarged to enhance the growth rate. The beam fluxes emerging from these nonideal effusion cells are generally determined experimentally. For in situ calibration of beam fluxes and growth rates, the most convenient and routinely used method is the RHEED intensity oscillation technique. As shown in Fig. 5.17, the equilibrium surface existing before growth is smooth, corresponding to high reflectivity of the specular beam. As growth commences, nucleation islands
Fig. 5.17 . Realspace representation of the formation of the first complete monolayer of (001) GaAs with respect to RHEED intensity oscillations. The intensity of the diffracted electron beam decreases as surface roughness increases. θ is the fractional layer coverage. The period of the oscillation (e.g., time span between point A and point E) corresponds to the growth rate of one atomic layer. Reprinted with permission from [8], copyright Elsevier
188
5 Material Technologies
will form at random sites on the surface, leading to a decrease in reflectivity. These islands grow until they coalesce into a smooth surface again. It is expected that the minimum in reflectivity would correspond to 50% coverage by the growing layer. Therefore, the period of the oscillations corresponds precisely to the growth rate of a monolayer. Because the sticking coefficients of the group III elements are unity, once the beam fluxes and the growth rates are calibrated, the alloy composition in the AIII BIII CV alloy is simply determined by the relative group III fluxes reaching the surface. For example, the Al fraction in Alx Ga1−x As can be determined by the relation x=
R(Alx Ga1−x As) − R(GaAs) R(Alx Ga1−x As)
(5.15)
where R is the growth rate.
5.5.4 Variations of Molecular Beam Sources Although MBE has long been successful for the growth of arsenic and antimony compounds, the growth of phosphorus compounds by conventional solid source MBE (SSMBE) had been hampered until 1995 by the high vapor pressure and the allotropic property of solid phosphorus. In that year, a new approach for the growth of Pcompounds by SSMBE was reported [9]. This technique uses a threezone valved cracking cell to generate P2 molecules. The structure of a solidP valved cracking cell consists of a red P oven, a white P condensing reservoir, and a valved thermal cracking region. During operation, the red P oven is heated to an appropriate temperature in order to generate a sufficient amount of P4 vapor. The white P reservoir section during this time period is held at a low temperature to condense the vapor into white P while the valve is closed. After the desired quantity of white P has been collected, both the red P oven and the white P reservoir are returned to ambient temperature to finish the distillation process. The P4 vapor emanating from the white P reservoir is passed through the hightemperature cracking zone and dissociated into P2 at the desired rate via the adjustable flux control valve. The accumulated white P and its associated high vapor pressure enable the condensing reservoir to be operated at room temperature during growth. This capability strongly inhibits the formation of multiple allotropes and makes accurate P flux control possible. Highly reproducible growth of Pcompounds and device structures has been demonstrated. The gas source molecular beam epitaxy (GSMBE) technique, in which the elemental As and P sources are replaced by gaseous AsH3 and PH3 , respectively, represents an alternative approach. A further development of the technology replaces the group III elements with gas sources. This is conveniently accomplished using metalorganic group III species in addition to hydride group V sources. This method
5.5 Molecular Beam Epitaxy
189
is generally referred to as metalorganic molecular beam epitaxy (MOMBE) or chemical beam epitaxy (CBE). Both GSMBE and MOMBE use a growth system design similar to SSMBE with modifications in source delivery and UHV pumping methods. GSMBE and MOMBE use gashandling systems similar to those used by MOCVD to deliver gas sources into the UHV growth chamber for epitaxy. The major distinction between the GSMBE/MOMBE method and MOCVD centers around the pressure regimes involved in each method. Namely, the latter operate under viscous flow and the former under molecular flow conditions. In molecular flow, the pressure inside the growth chamber is low ( E a , the crystal will have an increased solubility for the acceptorlike V III defects. Therefore, the group III selfdiffusion will increase in heavily doped ntype heterostructure when annealed under Asrich condition. However, under Aspoor annealing conditions, the ntype heterostructure remains stable with little intermixing. Similar arguments can be applied to the ptype crystal, where the Fermi level is situated close to the valence band. Under Aspoor annealing conditions, the group III selfdiffusion proceeds via group III interstitials (Gai and Ali ), which are donorlike defects with E = E d . Since E d > E F , most defects are ionized. Through the same argument of ntype structure, the equilibrium concentration of ionized defects is proportional to exp[(E d − E F )/kT ]. The solubility of donorlike group III interstitials will be increased to enhance the group III self diffusion. Nevertheless, ptype heterostructure does not intermix under Asrich annealing conditions. (c) Application of IILD to QW laser fabrication Because IILD allows the fabrication of heterojunctions perpendicular to the thin epitaxial layers, this process can be used to fabricate devices with threedimensional carrier and photon confinement using standard masking procedures of the crystal surfaces and either selective impurity diffusion or ion implantation. This property makes the IILD well suited to the fabrication of both buried heterostructure quantumwell laser diodes and optical waveguides for optoelectronic integrated circuit applications. As an example, Fig. 5.19 shows the crosssectional scanning electron microscope (SEM) image of a double heterostructure QW laser diode after IILD. The starting material is a typical GaAsAlGaAs double heterostructure wafer which forms 1D current and optical confinements along the layer growth direction in fabricated laser diodes. The active region of the device consists of GaAs multiple QWs separated by Alx Ga1−x As (x ~ 0.35) barriers, with barrier and wells sandwiched in a 0.2 μm Alx Ga1−x As waveguide region. An ntype Aly Ga1−y As (y ~ 0.8) lower confining layer and a ptype Aly Ga1−y As upper confining layer complete the structure. A thin (~0.1 μm) heavily doped p+ contact layer is grown on the upper ptype Aly Ga1−y As confining layer in order to aid lowresistance metal contact to the device. To achieve 2D current and optical confinements, Si IILD is then used to process the wafer into
5.6 Postgrowth Modification of Material Structures
195
Fig. 5.19 SEM image of the stripe region after Si diffusion (850 °C, 9.5 h) of the QW heterostructure. The original masking stripe width is 5 μm. Lateral diffusion of the Si has narrowed the active region to ~2.5 μm. Arrows show where the Si, through intermixing of the Alx Ga1−x As (x ~ 0.35) and Alx’ Ga1−x As (x ~ 0.85) regions, flares the waveguide and forms Aly Ga1−y As (x < y < x ). Reprinted with permission from [12], copyright AIP Publishing
buried heterostructure QW laser diodes. As shown in Fig. 5.19, the Si diffusion, which has been masked by a narrow (~5 μm) Si3 N4 stripe, extends on either side of the active region into the lower ntype Aly Ga1−y As confining layer. The Si diffusion converts the crystal to ntype and thus forms a lateral current constraining pn junction in the high gap upper ptype Aly Ga1−y As confining layer. Most important, as the Si diffuses through the QW active region, layer intermixing occurs between the GaAs QWs, the Alx Ga1−x As barriers, and the Alx Ga1−x As waveguide, and also between the waveguide region and the upper and lower Aly Ga1−y As confining layers. The layer intermixing results in an increased bandgap relative to the masked undiffused active region preserved beneath the Si3 N4 mask, thus giving a builtin lateral refractive index step that provides optical confinement. The lateral pn junction formed in the upper confining layer because of the Si diffusion provides current confinement in the laser active region since the high gap junction and the diode active region have different turnon voltages. This form of IILD buried heterostructure offers the advantage of a simplified fabrication process over that of regrown laser diode structures. An added advantage of the IILD is that by utilizing the lateral diffusion of the Si under the Si3 N4 , it is possible to obtain reduced active region widths (≤0.7 μm) and thus lower lasing thresholds.
5.6.2 Wet Oxidation of AlContaining IIIV Alloys The predominance of silicon as the semiconductor material of choice was mainly due to, among other things, its ability to grow a native oxide SiO2 on Si surface. This led directly to the development of the IC industry by providing a convenient patternable
196
5 Material Technologies
mask for impurity diffusion and a highquality oxidesemiconductor interface for MOSFETs. Conversely, the chief shortcoming of IIIV compound semiconductors has been the lack of a highquality native oxide. Although many techniques have been attempted, including anodic and thermal oxidation, a viable oxide has proven elusive. On the other hand, it has been recognized that Alx Ga1−x As with high Alcomposition (x > 0.7) is unstable and deteriorates (hydrolyzed) after long exposure to atmospheric condition. During their studies of the reliability issues involved in high Alcomposition AlGaAs heterostructures, J. Dallessasse and N. Holonyak Jr. discovered that by oxidizing the semiconductor in water vapor at elevated temperatures, a dense and stable oxide of AlGaAs is formed [13]. This AlGaAs native oxide possesses many desirable properties for integrated semiconductor photonic device fabrication including a low index of refraction (~1.63) and good electrical insulating properties. (a) Wetoxidation reactions The wet oxidation of AlGaAs is usually performed by exposing the high Alcomposition layers to water vapor, transported in an inert carrier gas, in an elevated temperature environment of ~350 to 600 °C. The oxidation process proceeds either from the plane surface or the exposed edges of the multilayer structure (lateral oxidation). The reactions of wet oxidation of Albearing IIIV materials are more complex than silicon oxidation, as the interaction of the water molecule with both group III and group V elements needs to be considered. Although the aluminumwater system is well studied in equilibrium and under highpressure conditions, a systematic examination of reactions between Albearing crystalline material, such as AlAs, and water is lacking. Nevertheless, by projecting from the aluminawater system, for the oxidation of Alx Ga1−x As, it is expected that Al(OH)3 forms during the roomtemperature deterioration process, and at temperatures up to ~100–150 °C, AlO(OH) forms at intermediate temperatures, and amorphous γAl2 O3 is formed in the temperature range greater than ~370 °C. It is also noted that, through secondaryion mass spectroscopy (SIMS) studies, arsenic is depleted from the hightemperature oxidized layers as well as near the surface of roomtemperature hydrolyzed layers, supporting the view that the reaction creates a volatile form of arsenic. It is believed that AsH3 is formed as the primary product of the direct reaction with the Alx Ga1−x As crystal. Then AsH3 immediately undergoes a followon reaction with the H2 O to form As2 O3 or elemental arsenic. Thus the likely reactions could be described by 2AlAs + 3H2 O → Al2 O3 + 2AsH3 AlAs + 2H2 O → AlO(OH) + AsH3 AlAs + 3H2 O → Al(OH)3 + AsH3
≥ 370 ◦ C > 150 ∼< 370 ◦ C ≤ 150 ◦ C
(5.26a) (5.26b) (5.26c)
5.6 Postgrowth Modification of Material Structures
197
(b) Oxidation process parameters The wetoxidation rate of Albearing IIIV semiconductors is affected by several process parameters including Alcomposition, layer thickness, and oxidation temperature. Following the model of silicon oxidation, under fixed oxidation temperature and constant gas flow containing oxidizing medium (water vapor), the oxidation thickness as a function of time is described by x02 + Ax0 = Bt
(5.27)
where x 0 is the thickness of the oxide layer, coefficient B is related to the diffusivity of the reactants in the oxide layer, and coefficient A is determined by the oxidesemiconductor interfacereaction rate constant and the gasphase masstransfer coefficient. In the limit of thin oxide thickness or short oxidation time, one obtains a linear growth of oxide layer thickness with time, x0 ∼ = (B/A)t
(5.28)
where B/A is the linear reaction rate constant. This linear behavior is called reactionrate limited case. In the limit of longer oxidation time, a parabolic relationship is approached. x02 ∼ = Bt
(5.29)
Then the oxidation rate is diffusion limited where the rate is determined by the diffusion of water vapor through the oxide to the reaction front. For lateral oxidation of Alx Ga1−x As, the time dependence of the oxidation thickness has also been observed to vary between linear (reactionrate limited) and parabolic (diffusionlimited). However, the origin of the shift of oxidation rate from linear to parabolic relationship is different. During the wetoxidation process, there exists a thin, dense, amorphous region of a few nanometers thick at the oxidation front. Behind this dense mixture of As2 O3 and Al2 O3 is a less dense region of amorphous Al2 O3 that extends to the exposed mesa edge. The time progression of the thickness of this dense region will determine whether linear or parabolic behavior dominates. When the reduction of As2 O3 to As is sufficiently fast to balance the rate of formation of As2 O3 , a thin layer of dense oxide of relatively constant thickness will be formed near the oxidation front. Under this condition, a linear timedependent oxidation rate is expected. However if reaction conditions are changed to preferentially increase the formation of As2 O3 relative to As loss, a steady increasing thickness of the dense, As2 O3 containing layer will form more quickly. This will lead to a diffusionlimited parabolic time dependence of the oxidation rate. This shift from reactionrate limited to diffusionlimited time dependence is favored by increasing oxidation temperature or increasing Al content of Alx Ga1−x As, both of which increase total oxidation rate.
198
5 Material Technologies
Next, the temperaturedependent oxidation rate is considered. Experimental results show that the oxidation rate of Alrich Alx Ga1−x As depends exponentially on oxidation temperature and follows an Arrhenius relationship. It is given by x = x0 exp(−E a /kT ), where x 0 is a constant depending on the material, and E a is the activation energy. As shown in Fig. 5.20, the activation energy maintains a nearly constant value and decreases slowly from 1.90 to 1.85 eV as the AlAsmole fraction increased from 0.9 to 0.96. However, the activation energy of Alx Ga1−x As drops sharply when the AlAsmole fraction is increased beyond 0.96. The activation energies reduce to ~1.75 eV and 1.25 eV for Al0.98 Ga0.02 As and AlAs, respectively. When oxidized at a fixed temperature, this rapid change of activation energy in Alrich Alx Ga1−x As leads to an extremely strong compositional dependence of the oxidation rates. Thus by making a small change in AlAsmole fraction near 1 ≥ x ≥ 0.9, the oxidation rate can be changed by as much as an order of magnitude, leading to a high degree of oxidation selectivity between AlGaAs layers of different Al concentrations. However, this unique property implies that a stringent composition control is critical to precisely regulate the oxidation rate. Furthermore, the oxidation rate of AlGaAs is also influenced by its thickness and heterointerface structures. Specifically, the lateral oxidation rate of AlAs layers departs from a constant rate and decreases sharply for layers thinner than ~60 nm (Fig. 5.21). The drastic reduction of oxidation rate with decreasing AlAs layer thickness is due to the variation of surface energy between AlAs and AlGaAs barriers at the oxide front or change of strain with thickness. This behavior can be used to compensate for the compositional dependence of wet oxidation since thin layers of AlAs may oxidize slower than thick layers of AlGaAs.
2.0
Activation Energy (eV)
Fig. 5.20 Arrhenius activation energy for the oxidation reaction of Alx Ga1−x As versus Alcomposition. Reprinted with permission from [14], copyright IEEE
1.8
1.6
1.4
1.2
1.0
0.90
0.92
0.94
0.96
0.98
AlAs Mole Fraction
1.00
5.6 Postgrowth Modification of Material Structures 10
AlAs @ 400°C
Oxidation Rtae (µm/min)
Fig. 5.21 AlAs oxidation rate at 400 °C versus AlAs layer thickness. Reprinted with permission from [14], copyright IEEE
199
1
0.1
0.01
0
50
100
150
200
250
Layer Thickness (nm)
(c) Application of wet oxidation to device fabrication The wet oxidation of Albearing IIIV alloys converts semiconductor into an insulator that can be used for the design and fabrication of various device structures. The oxide layers can be formed on the surface or through lateral oxidation from an edge to create oxide narrow bands between semiconductor layers. Due to its capability to form insulating layers for current confinement and to provide a significant refractive index difference for optical confinement, a wide variety of devices have consequently been fabricated using the IIIV oxidation process. Edgeemitting lasers with single and multiplestripe geometry have been fabricated using the IIIV surface oxidation process. The oxide layer is formed in the Al0.8 Ga0.2 As upper cladding layer of a GaAsAlx Ga1−x As QW heterostructure laser structure. The high selectivity in oxidation rate between material having different aluminum compositions allows a simple fabrication process that uses the top GaAs contact layer as the oxidation mask. The laser stripe or stripes are defined using photolithography followed by a wet chemical process to etch through the GaAs cap to the Al0.8 Ga0.2 As layer underneath. Then the photoresist is stripped, and the material is oxidized. For example, an oxide layer ~1000–1500 Å thick is formed in a 3 h oxidation at 400 °C using water vapor provided by a 1.4 scfh N2 flow through a water bubbler maintained at 95 °C. In Fig. 5.22, a SEM cross section image for a fabricated laser array consisting of ~3 μm stripes on 4 μm centers over a 200 μm aperture is shown. Stable operation to high output powers (>2.5 W) has been achieved in this laser with surfaceoxide defined multistripe arrays. The lateral wet oxidation at the exposed edges of superlattice samples proved to be a more versatile approach for both edge and surfaceemitting photonic devices.
200
5 Material Technologies
Fig. 5.22 SEM cross section image of a segment of an AlGaAsGaAs multistripe laser. The total array consists of 50 stripes, with a total aperture width of 200 μm. Reprinted with permission from [13], copyright AIP Publishing
It has been shown that lateral oxidation can be confined to a layer having high Alcomposition when kept between two lower composition layers of sufficient thickness. The close proximity of the oxide to the waveguide and quantumwell layers of the laser also demonstrates that the oxide will not degrade device performance even when very close to the device active region. An example of lateral oxidation to form buried apertures for current and optical confinement in a current injection edgeemitting laser is shown in Fig. 5.23. Here, indexguided lasers are formed in the AlGaAsGaAsInGaAs material system to produce lasers operating in the 980 nm wavelength range. The highcomposition Al~0.85 Ga~0.15 As layers on the top and bottom of a lower composition QW region are oxidized from the edge of a stripe mesa to form layers that reduce the active device geometry and confine both optically and electrically. In Fig. 5.23a, the extent of lateral oxidation on the top and bottom confining layers is clearly evident in the crosssectional SEM. Lower composition layers in the laser waveguide and quantumwell region do not show significant oxidation. The Fig. 5.23 a A SEM cross section and b a topdown optical photomicrograph of an AlGaAsGaAsInGaAs stripegeometry QW laser formed via lateral oxidation. The slight difference in the rate of lateral oxidation between the upper and lower oxide layers is due to the small composition difference between the layers (x ~ 0.85 versus x ~ 0.87). Reprinted with permission from [15], copyright AIP Publishing
5.6 Postgrowth Modification of Material Structures
201
large difference in oxidation rates, especially between the upper and lower confining layers, highlights the sensitivity of oxidation rate to the aluminum composition of the oxidized layer. The topdown image shown in Fig. 5.23b also demonstrates a clear demarcation between the edge of the mesa (10 μm width) and the lateral extent of the oxidation front (2.5 μm width). Since the lateral oxidation distance can be controlled through Alcomposition, and oxidation time and temperature, wet oxidation provides a scalable, manufacturable method for forming smalldimension lasers from larger mesas. Application of oxidation to VCSELs (verticalcavity surfaceemitting lasers), i.e., circular lateral confinement, which employ highcomposition Alx Ga1−x As layers to achieve required device performance, is a simple extension and an ideal fit for oxide technology.
References 1. C.D. Thurmond, J. Phys. Chem. Solids 26, 785 (1965) 2. H. Amano, Jpn. J. Apply. Phys. 52, 050001 (2013) 3. R. Dwilinski, R. Doradzinski, J. Garczynski, L.P. Sierzputowski, A. Puchalski, Y. Kanbara, K. Yagi, H. Minakuchi, H. Hayashi, J. Crystal Growth 311, 3015 (2009) 4. M.B. Panish, M. Ilegems, in Progress in Solid State Chemistry, vol. 7, ed. by H. Reiss, J.O. McCaldin (Pergamon Press, New York, 1972), pp. 39–83 5. T. Mizatami, M. Yoshida, A. Usai, H. Watanabe, T. Yuasa, I. Hayashi, Jpn. J. Appl. Phys. vo. 19, L113 (1980) 6. A.Y. Cho, K.Y. Cheng, Appl. Phys. Lett. 38, 360 (1981) 7. A.Y. Cho, J. Vac. Sci. Technol. 8, S31 (1971) 8. B.A. Joyce, P.J. Dobson, J.H. Neave, K. Woodbridge, J. Zhang, P.K. Larsen, B. Bolger, Surf. Sci. 168, 423 (1986) 9. F.F. Briones, Method of producing white phosphorus for molecular beam epitaxy. U.S. Patent 5,482,892, January 9, 1996 10. W.D. Laidig, N. Holonyak Jr., M.D. Camras, K. Hess, J.J. Coleman, P.D. Dupkus, J. Bardeen, 38, 776 (1981) 11. K. Meehan, N. Holonyak Jr., J.M. Brown, M.A. Nixon, P. Gavrilovic, R.D. Burnham, Appl. Phys. Lett. 45, 549 (1984) 12. D.G. Deppe, K.C. Hsieh, N. Holonyak, R.D. Burnham, R.L. Thornton, J. Appl. Phys. 58, 4515 (1985) 13. J.M. Dallesasse, N. Holonyak, J. Appl. Phys. 113, 051101 (2013) 14. K.D. Choquette et al., IEEE Sel. Topic. Quantum Electron. 3, 916 (1997) 15. S.A. Maranowski, A.R. Sugg, E.I. Chen, N. Holonyak Jr., Appl. Phys. Lett. 63, 1660 (1993)
Further Reading 1. V. Swaminathan, A.T. Macrander, Materials Aspects of GaAs and InP Based Structures (PrenticeHall, 1991) 2. A. Denis, G. Goglio, G. Demazeau, Mat. Sci. Eng. R50, 167 (2006) 3. K. Xu, J.F. Wang, G.Q. Ren, Chin. Phys. B 24, 066105 (2015) 4. H.C. Casey, M.B. Panish, Heterostructure Lasers: Part B, Materials and Operating Characteristics (Academic Press, 1978)
202
5 Material Technologies
5. G. Beuchet, Halide and chloride transport vaporphase deposition of InGaAsP and GaAs, in Semiconductors and semimetals, ed. by W. T. Tsang, vol. 22, Part A (Orlando, FL: Academic Press, 1985) pp. 261–297 6. A.Y. Cho, Molecular Beam Epitaxy (American Institute of Physics, New York, 1994) 7. G. B, Stringfellow, Organometallic VaporPhase Epitaxy: Theory and Practice (Academic Press, Boston, 1989) 8. M.B. Panish, H. Temkin, Gas Source Molecular Beam Epitaxy (SpringerVerlag, Berlin, 1993) 9. D.G. Deppe, N. Holonyak, J. Appl. Phys. 64, R93 (1988) 10. N. Holonyak, IEEE Sel. Topic. Quantum Electron 4, 584 (1998)
Chapter 6
Heterostructure Fundamentals
Abstract The development of modern epitaxy methods enables the verification of many core concepts of modern physics and the development of bandgap engineering technology using quantum wells and superlattices. Molecular beam epitaxy (MBE) technology, in particular, not only brings the theory of quantum mechanics from classroom to laboratory through the fabrication of quantumwell structures, but also promotes new discoveries in physics including the fractional quantum Hall effect. In addition, many new physics concepts have been discovered and developed into different physics subdisciplines, including lowdimension (0D and 1D) nanometerscale structures and technologies. With the ability to form highquality heterostructures, new breeds of devices including unipolar quantum cascade lasers, high electronmobility transistors, and quantumwell infrared photodetectors, just to mention a few, have been invented. All these developments rely on the inimitable properties of the heterostructure where the proper energy band alignment provides unique carrier and/or optical confinement. At the inception of III–V heterostructure development, an energy band alignment model based on electron affinity difference between semiconductors was developed. The model provided a simple theoretical basis to promote the development of heterostructure technologies. However, as the epitaxy technique improved, the discrepancy between the simple theoretical predictions and experimental results became undeniable, prompting the development of a number of theoretical bandedge alignment models to include effects of charge redistribution at the heterointerface. Meanwhile, the advancement of epitaxy techniques allows the formation of strained but otherwise highquality thin layers in latticemismatched heterostructure systems. Thus, to properly describe the equilibrium band diagram of a heterostructure, bandedge alignment models capable of treating strain effects are needed. The development of bandedge alignment models including strain effect constitutes the focus of this chapter.
© Springer Nature Switzerland AG 2020 K. Y. Cheng, III–V Compound Semiconductors and Devices, Graduate Texts in Physics, https://doi.org/10.1007/9783030519032_6
203
204
6 Heterostructure Fundamentals
6.1 Energy Band Alignment 6.1.1 Anderson’s Electron Affinity Model In an ideal Schottky barrier structure, we use the vacuum as the reference level to determine the metal–semiconductor barrier height φ b . As shown in Fig. 6.1, under the equilibrium condition, the conduction band edge and the Fermi level of the semiconductor below the vacuum level are represented by the electron affinity χ s and the work function φ s , respectively The work function of the metal is represented by φ m . After forming the metal–semiconductor junction, the Fermi levels on both sides merge into one level to attain an equilibrium condition. This creates an energy barrier in the form of φ b = φ m − χs
(6.1)
Anderson’s model of heterostructures is based on the same idea [1]. It uses the vacuum as the reference energy level to estimate the bandgap discontinuity at the pN heterojunction interface as shown in Fig. 6.2. Note that a lower case p and a capital N have been used to represent the small and large bandgap materials, respectively, in the heterostructure. Using the vacuum level as the reference, the conduction band and valence band discontinuities are defined as E c = χ 1 − χ2 (6.2) E v = E g1 − E g2 − E c and E c + E v = E g2 − E g1 = E g
(6.3)
Fig. 6.1 Formation of the Schottky barrier and its energy band structure: Metal and semiconductor are separated in vacuum (left), and metal–semiconductor contact under equilibrium condition (right)
6.1 Energy Band Alignment
205
Fig. 6.2 Energy band alignments at the pN heterojunction before and after contacting in Anderson’s model
where χ i and φ i represent the electron affinity and work function of the material, respectively. At equilibrium, after the formation of the heterojunction, the Fermi levels on both sides of the heterojunction line up to the same value. At the same time, the electron affinity and work function in both materials, away from the heterointerface, have to maintain constant values. These conditions lead to energy band bending at the heterostructure interface. This band bending is similar to the ideal Schottky barrier except that it occurs on both sides of the interface.
206
6 Heterostructure Fundamentals
This simple model is intuitive and provides a starting point for the understanding of the nature of heterostructures. However, this early theory has a fundamental problem. In the case of an ideal Schottky barrier contact, a flat work function or vacuum level is maintained on the metal side and can be used as a reference level. For an ideal heterojunction inside a bulk solid, there is no vacuum level present to which all energies can be referred. The longrange nature of the Coulomb interaction in a crystal does not allow the zero of energy to be well defined as in an isolated atom. Therefore, there is no unique reference level within each bulk solid with which to compare the potentials for two different solids.
6.1.2 ModelSolid Theory Numerous theoretical approaches have been pursued to derive an accurate bandedge alignment model. It is important to realize that around the heterointerface, the redistribution of electronic charge induces dipole moments across the interface and leads to a shift of the bulk bands. Therefore, one has to perform a calculation in which the interface atoms from both types materials are included. The selfconsistent interface calculations (SCIC), in which the electrons are allowed to adjust to the specific environment induced by the heterointerface, have been used to derive the complete solution of this interface problem. Unfortunately, the computational complexity of the early firstprinciples calculations is very high, which limits their use as a general tool in the exploration and design of novel heterostructures. Therefore a reliable model to predict band offsets for a wide variety of heterostructures, and to do so without heavy calculations, is needed. In the 1980s, several band discontinuity models with varying degrees of success were proposed. These models are W. A. Harrison’s ‘linear combination atomic orbit’ (LCAO) [2], J. Tersoff’s ‘energy level’ [3, 4], M. Cardona and N. E. Christensen’s ‘linear muffintin orbitals’ (LMTO)[5], and C. G. van de Walle’s ‘model solid’ calculations [6, 7]. Among these, only the last two allow the incorporation of misfit strain into the calculation, making them usable in band alignment estimation for a wide range of heterostructures. However, the LMTO treatment of strain effects is more complicated, and an exact solution is not available. This leaves the modelsolid theory of van de Walle as the most convenient and simple model for band alignment estimation including the strain effect. The main idea of the modelsolid theory is to establish an ‘absolute reference energy level’ for each semiconductor in a heterostructure such that the band lineups can be calculated. This reference energy level, E v, av , was derived in the modelsolid theory by averaging the three topmost valence bands at , i.e., the heavyhole, the lighthole, and the spinorbit splitoff bands. The numerical values of E v, av for most of the binary compound semiconductors have been derived by van de Walle and are listed in Table 6.1. Using this reference energy, the position of the topmost valence band for a specific semiconductor can be derived by
12.21
C 11 (1011 dyn/cm2 )
5.42
−1.33
6.00
−0.8
(Data from [7] and [8])
VBO (eV)
5.34
5.66
C 44 (1011 dyn/cm2 )
C 12
dyn/cm2 )
12.50
−3.4
−4.8
d (eV)
(1011
2.47
−2.3
1.16
−2.0
b (eV)
−5.64
−7.17
ac (eV)
av (eV)
0.28
−7.49
so (eV)
2.1641
0.341
1.8989
E gX (eV)
3.003
−6.92
1.424
E gΓ (eV)
5.6611
AlAs
E v, av (eV)
5.65325
GaAs
a0 (Å)
Parameters
−0.59
3.959
4.526
8.329
−3.6
−1.8
1.00
−5.08
−6.67
0.39
1.37 1.07 (L)
0.354
6.0583
InAs
−1.27
7.033
6.203
14.05
−4.6
−1.6
1.7
−8.2
−7.40
0.08
2.2727
2.9903
5.4505
GaP
−1.74
6.15
6.30
13.30
−4.6
−1.5
3.0
−5.7
−8.09
0.07
2.4878
3.5527
5.4672
AlP
−0.94
4.56
5.61
10.11
−5.0
−2.0
0.6
−6.0
−7.04
0.108
2.273
1.3529
5.8697
InP
−0.03
4.322
4.026
8.842
−4.7
−2.0
0.8
−7.5
−6.25
0.760
1.033 0.753 (L)
0.727
6.0959
GaSb
−0.41
4.076
4.341
8.769
−4.3
−1.35
1.4
−4.5
−6.66
0.676
1.616
2.300
6.1355
AlSb
0
3.111
3.735
6.847
−4.7
−2.0
0.36
−6.94
−6.09
0.81
0.63 (0 K)
0.1737
6.4794
InSb
and E gX (Xvalley), spinorbit splitoff so , average valence band energy E v, av , conduction band hydrostatic deformation potential ac , valence band hydrostatic deformation potential av , shear deformation potential b ([001]direction) and d ([111]direction), elastic constants C 11 , C 12 and C 44 , and valence band offset (VBO) with respect to InSb
Table 6.1 Material parameters for III–V binary semiconductor compounds at room temperature: lattice constant a0 , 300 K bandgap energies E gΓ (valley)
6.1 Energy Band Alignment 207
208
6 Heterostructure Fundamentals
E v = E v,av +
so 3
(6.4)
where so is the spinorbit splitoff energy. The value of so is determined experimentally. Once the value of E v is determined, the experimentally determined bandgap value can be used to determine the conduction band edge. Ec = Ev + Eg
(6.5)
Note, the bandgap energy is a temperaturedependent quantity and often described in the empirical Varshni form E g (T ) = E g (0) −
αT 2 β+T
(6.6)
where α (meV/K) and β (K) are fitting parameters and E g (0) is the bandgap energy at absolute zero. In an unstrained heterostructure, once we have determined E c and E v in two semiconductors with similar lattice constant, the band alignment can be calculated using
E v = E vB − E vA
E c = E cB − E cA = E vB + E gB − E vA + E gA
(6.7)
The superscripts A and B correspond to the two semiconductors A and B. Example: GaAs/AlAs Heterojunction From Table 6.1, we have the following parameters: E v,av (GaAs) = −6.92 (eV), so (GaAs) = 0.34 (eV), E g (GaAs) = 1.424 (eV) E v,av (AlAs) = −7.49 (eV), so (AlAs) = 0.28 (eV), E g (AlAs) = 2.164 (eV) Since AlAs has an indirect bandgap, the minimum indirect conduction band value of Xvalley, E gX , is used in the calculation. Then, E v (GaAs) = −6.92 + 0.34/3 = −6.8063 eV E v (AlAs) = −7.49 + 0.28/3 = −7.3967 eV E v = −6.8063−(−7.3967) = +0.5903 eV
6.1 Energy Band Alignment
209
This indicates that the valence band in GaAs is above the valence band in AlAs. The valence band discontinuity E v can also be determined from the valence band offset (VBO) values listed in Table 6.1. Using the empirical VBO values obtained by averaging experimental results, the relative VBO difference between GaAs and AlAs is obtained as VBO(GaAs)−VBO(AlAs) = −0.8−(−1.33) = +0.53 eV The modelsolid theory calculated E v is overestimated by 60 meV over the relative VBO value. The conduction band discontinuity occurs between the direct conduction band of GaAs and the indirect conduction band of AlAs. Therefore, E c (GaAs) = E v (GaAs) + E g (GaAs) = −6.8063 + 1.424 = −5.3823 eV E c (AlAs) = E v (AlAs) + E g (AlAs) = −7.3967 + 2.1641 = −5.2326 eV E c = −5.3823−(−5.2326) = −0.1497 eV The minus sign indicates that the direct conduction band in GaAs is below the indirect conduction band in AlAs. The band discontinuity lineup in GaAs/AlAs heterojunction is ‘typeI,’ meaning that the bandgap of one material (GaAs) is completely inside the bandgap of the other (AlAs). This band alignment is illustrated in Fig. 6.3. At typeI interface, potential barriers exist for both electrons and holes in going from the smaller gap semiconductor to the larger gap semiconductor. This feature is very useful for double heterostructure lasers where both types of carriers can be confined in a single layer to generate stimulated emission. On the other hand, only one type of 2D carrier gas will form at the interface depending on the doping profile Fig. 6.3 Band lineups at the GaAs/AlAs interface. The average valence band E v, av is obtained from the modelsolid theory. Spinorbit splitting and bandgap energies are taken from experiments
210
6 Heterostructure Fundamentals
across the interface. Interfaces formed by III–V compounds, either with different group III elements such as GaAsAlAs or with different group V elements such as GaAsGaP, belong to typeI.
6.1.3 Empirical Band Alignment Models The experimentally determined band discontinuity data is very useful in designing heterostructure devices for specific characteristics. However, new device designs often require this information for alloy combinations for which no experimental data is available. The first step to derive the band discontinuity data is to establish band parameters of all compound semiconductor binary alloys. The band alignment data derived from the modelsolid theory provides a useful guideline but the uncertainty is sometimes too large (≥200 meV) to be useful for device designs. Therefore, it is worthwhile to compare the band discontinuity results of the modelsolid theory with other empirically derived results. Using the existing theories coupled with experimental data, the VBOs of binary III–V alloys with respect to InSb (VBO of InSb is set at 0) are listed in Table 6.1. In deriving these VBO values, the properties of transitivity and commutativity are followed while the values of valence band offsets to be independent of temperature. The transitivity property of band offsets means that the sum of the band offsets at the A–B and B–C interfaces is equal to the A–C interface band offset. The commutative property means that the band offset between two semiconductors is independent of the order in which they are grown. Once the valence band discontinuity E v of two closely latticematched binary alloys is determined from the VBO difference of the heterojunction, the conduction band discontinuity E c is simply obtained by subtracting E v from the bandgap energy difference E g . Example: AlSb/InAs/GaSb heterojunctions The lattice mismatches between binary alloys AlSb, GaSb, and InAs are small, and highquality AlSb and InAs can be grown on GaSb substrates for midinfrared (midIR) device applications. The alignments of conduction and valence bands in this latticematched alloy system are derived from the modelsolid theory and shown in Fig. 6.4. Using values of E v, av , so , and E g from Table 6.1, the maximum valence band edges of AlSb and GaSb are E v (AlSb) = −6.66 + 0.676/3 = −6.4347(eV) E v (GaSb) = −6.25 + 0.760/3 = −5.9967(eV) and E v = −6.4347−(−5.9967) = −0.438(eV)
6.1 Energy Band Alignment
211
Fig. 6.4 Calculated bandgap energy and conduction and valence bandedge discontinuities in latticematched InAs/GaSb/AlSb material systems using modelsolid theory
The valence band edge of AlSb is below that of GaSb by 0.438 eV. The measured relative VBO difference between AlSb and GaSb is –0.38 eV. The discrepancy between the theoretical and averaged measurement values is 58 meV. The conduction band discontinuity occurs between the direct conduction band of GaSb and indirect conduction band E gX of AlSb. E c (AlSb) = E v (AlSb) + E gX (AlSb) = −4.8187 (eV) E c (GaSb) = E v (GaSb) + E g (GaSb) = −5.2697 (eV) and E c = −4.8187−(−5.2697) = 0.4510 (eV) The indirect conduction bandedge minimum in AlSb is above the direct conduction band edge in GaSb leading to a typeI band alignment in AlSbGaSb heterostructure. Next, the band alignments of GaSb and InAs are derived. The maximum valence band edges of GaSb and InAs are E v (GaSb) = −5.9967 (eV) E v (InAs) = −6.67 + 0.39/3 = −6.540 (eV) and E v = −5.9967−(−6.540) = 0.5433 (eV)
212
6 Heterostructure Fundamentals
The valence band edge of GaSb is above that of InAs by 0.5433 eV, which matches with the measured relative VBO difference between GaSb and InAs (0.56 eV) quite well. The minimum conduction band edges of GaSb and InAs are located at E c (GaSb) = −5.2697 (eV) E c (InAs) = E v (InAs) + E g (InAs) = −6.1860 (eV) and E c = −5.2697−(−6.1860) = 0.9163 (eV) Both the conduction and valence band edges in InAs are below that of GaSb forming a ‘typeII’ band discontinuity lineup in the GaSbInAs heterojunction. The GaSbInAs interface is a typical example of the typeII interface alignment. Due to the large difference in average valence band energies E v, av and the spinorbit splitting, so , between GaSb and InAs, in addition to the small bandgap of InAs, the two bandgaps are completely misaligned in energy. This forms a typeII brokengap interface as shown in Fig. 6.4. The conduction band of InAs is below the valence band of GaSb. The electrons and holes are spatially separated and attracted to the InAs and GaSb sides of the interface, respectively. TypeII interfaces are formed in IIIV compound heterostructures with both different group III elements and different group V elements. If we reduce the difference in average valence band energies and spinorbit splitting, and increase the bandgap energy of the smaller gap material by using ternary alloys, the typeII staggered interface results. AlSbInAs and Al0.48 In0.52 AsInP systems are two typical examples. The maximum valence band edges of AlSb and InAs are E v (AlSb) = −6.4347 (eV) E v (InAs) = −6.540 (eV) and E v = −6.4347−(−6.540) = 0.1053 (eV) The valence band edge of AlSb is above that of InAs by 0.1053 eV. However, the measured relative VBO difference between AlSb and InAs is 0.18 eV. The minimum conduction band edges of AlSb and InAs are located at E c (AlSb) = −4.8187 (eV) E c (InAs) = −6.1860 (eV) and
6.1 Energy Band Alignment
213
E c = −4.8187−(−6.1860) = 1.3673 (eV) Both the conduction and valence band edges in InAs are below that of AlSb forming a typeII staggered band discontinuity lineup in AlSbInAs heterojunction. Again, the electrons and holes are spatially separated by the interface and located in the smaller and larger bandgap sides, respectively. The recombination of electrons and holes in a typeII staggered heterostructure results in emission energy below the gap of either semiconductor. This feature is important for the generation of midIR emissions beyond the bandgap energy of the heterostructure. Next, the valence band alignments for unstrained ternary compounds are considered. When the constituent binary compounds are nearly latticematched, using linear extrapolation between two end binary alloys to generate valence band position for ternary compound is appropriate. Otherwise, a straininduced bandgap bowing parameter should be included. More detailed discussions on straininduced effects in ternary and quaternary compounds will be developed in Sect. 6.4. In general, the bowing parameter applies only to the conduction band edge. A linear variation is used for the estimation of valence band discontinuity in ternary alloys. This follows the observation in latticematched Alx Ga1−x As/GaAs and (Alx Ga1−x )0.49 In0.51 P/GaAs systems that the valence band discontinuity follows the composition linearly. A useful empirical technique for determining band alignments of unstrained III–V heterostructures was developed by S. Tiwari and D. J. Frank, which had an estimated accuracy of ≈100 meV [9]. The empirical approach is a consolidation of band discontinuity data based on two principles: the properties of transitivity and commutativity, and the strong correlation observed between barrier height of ptype semiconductor and the valence band discontinuity. The zero point of the energy at each lattice constant has been chosen as the reference level above the ptype semiconductor Schottky barrier height. Once the valence band discontinuity is determined for each lattice constant group, the conduction band discontinuity is simply obtained by adding the bandgap value to the ptype Schottky barrier height (φ bv ) listed in Table 4.5. For Si and Ge, φ bv equals 0.447 and 0.072 eV, respectively. The band discontinuities for ternary compounds are generated from the binary data incorporating bandgap bowing parameters (Table 4.6). The complete roomtemperature conduction bandedge and valence bandedge energies as functions of the lattice constant for unstrained III–V compound semiconductors are compiled in Fig. 6.5. The circles indicate the band edges of the binary semiconductors and the lines show the band edges of the ternary alloys. The portion of the ternary alloy with a direct bandgap is indicated by a solid line.
214
6 Heterostructure Fundamentals
Fig. 6.5 Conduction bandedge and valence bandedge energies plotted as functions of the lattice constant of III–V and elemental semiconductors. The circles indicate the band edges of binaries and the lines show the band edges of ternaries. Reprinted with permission from [9], copyright AIP Publishing
6.2 Strained Layer Structures When an epitaxial layer is grown on a foreign substrate with different lattice constant, the strain is created in such a heterostructure. The strain substantially alters the physical characteristics (e.g., band structure) of the epilayer and provides another degree of freedom for device structure design. Modern photonic and electronic devices take advantage of this added freedom by incorporating strained quantumwell thin layers into heterostructures with superior characteristics. However, in fabricating heterostructure devices, one of the most critical issues in material preparation is to avoid defect generation due to excessive latticemismatch between the substrate and the epitaxial layers. The generated high density of threading dislocation degrades the performance or even causes the device to cease operating. Therefore, it is necessary to examine the strain effect and its influence on bandgap energies closely.
6.2.1 Critical Layer Thickness (hc ) If the lattice mismatch between a bulk substrate and an epitaxial layer is sufficiently small, the first few deposited atomic layers will be strained to match the substrate and its 2D cell structure is shown in Fig. 6.6a. The epilayer is coherently strained,
6.2 Strained Layer Structures
215
Fig. 6.6 Heteroepitaxy of cubic crystal with equilibrium lattice constant a on top of a cubic crystal substrate with lattice constant a0 . a A coherently strained thin layer assumes an inplane lattice constant a0 and a normal lattice constant a⊥ > a. b When the epilayer thickness exceeds the critical layer thickness, hc , misfit dislocations (⊥) are formed at the interface between the two semiconductors
and it maintains a pseudomorphic interface. As the epilayer thickness increases, the homogeneous strain energy increases rapidly. When the epilayer thickness reaches the critical layer thickness hc and beyond, conditions become favorable for ‘misfit dislocations,’ meaning that some atoms within the epilayer are out of registry with the substrate to accommodate a fraction of the misfit as depicted in Fig. 6.6b. Matthews and Blakeslee developed a mechanical balance model for critical layer thickness calculation [10]. In this model, as shown in Fig. 6.7, a preexisting segment of threading dislocation bows and elongates under the influence of the misfit stress. At the critical layer thickness hc , the misfit strain, F H , equals the interface tension, F I , and generates a segment of interfacial dislocation line. Beyond this point, the
Fig. 6.7 Matthews and Blakeslee’s model of misfit dislocation generation at the heteroepitaxy interface. a A segment of threading dislocation exists at the interface of a strained system. b When the epilayer reaches the critical layer thickness, F H = F I , generating a segment of interfacial dislocation line. c With further increase of the layer thickness, the interface becomes incoherent and a misfit dislocation is formed [10]
216
6 Heterostructure Fundamentals
originally coherent interface becomes incoherent and an interface misfit dislocation is generated. For a single epitaxial layer, the equilibrium critical thickness is determined by hc =
1 − vcos2 Θ hc b 1 + ln f 0 8π (1 + v)cosλ b
(6.8)
√ where b = a0 / 2 is Burger’s vector, a0 is the bulk lattice constant of the epilayer, f 0 is the misfit, v is Poisson’s ratio, and = λ = 60° and 30° in cubic and wurtzite crystal structures, respectively. The misfit and Poisson’s ratio are defined as a0 − as  as
(6.9)
C12 C11 + C12
(6.10)
f0 = and ν=
where as is the lattice constant of the substrate, and C 11 and C 12 are Young’s moduli which will be defined in the next section. The critical thickness of a strained multilayer structure is obtained by the same procedure as the singlelayer model except that in the multilayer model, it is now required that F H = 2F I . The factor 2 arises from the fact that in a multilayer structure such as a quantum well, each interface may support a segment of line dislocation. Therefore, h c (multilayer) = 2h c (single layer)
(6.11)
Under normal growth conditions, the Matthews and Blakeslee model gives a fairly good fit to experimental data. However, strain relaxation is a kinetically controlled process. The critical layer thickness is, for example, a function of the growth temperature, which is not counted for in the model. Nevertheless, the Matthews and Blakeslee model is a good starting point to estimate the critical layer thickness. Example: Critical layer thickness of a Ga0.7 In0.3 As/GaAs quantum well The relevant material parameters from Table 6.1 are listed below. C11 (InAs) = 8.329 × 1011 , C12 (InAs) = 4.526 × 1011 , a0 (InAs) = 6.0583 Å C11 (GaAs) = 12.21 × 1011, C12 (GaAs) = 5.66 × 1011 , a0 (GaAs) = 5.6533 Å
6.2 Strained Layer Structures
217
The lattice constant, C 11 and C 12 of the Ga0.7 In0.3 As quantum well are calculated using interpolation from binaries as a0 (x) = 0.7 × 5.6533 + 0.3 × 6.0583 = 5.7748 Å C11 (x) = (0.7 × 12.21 + 0.3 × 8.329) × 1011 = 11.046 × 1011 C12 (x) = (0.7 × 5.66 + 0.3 × 4.526) × 1011 = 5.320 × 1011 Then, we can calculate the Burger’s vector, misfit, and Poisson’s ratio as follows: √ b = a0 (x)/ 2 = 4.083 f 0 = (5.7748−5.6533)/5.6533 = 0.0215 v = 5.320/(11.046 + 5.320) = 0.3251 Using = λ = 60°, we have
◦ hc 1 − 0.3251 cos2 60 4.083 1 + ln 0.0215 8π (1 + 0.3251) cos 60◦ 4.083 0.0954h c −1 = ln(h c /4.083) h c = 4.083 exp(0.0954h c − 1)
hc =
The numerical solution of hc is 32.1 Å. For the Ga0.7 In0.3 As/GaAs quantum well, the critical layer thickness is 2 × 32.1 = 64.2 Å.
6.2.2 Cubic Crystal Under Stress (a) Basic definitions Since most III–V compound semiconductors have a cubic crystal structure, it is reasonable as well as pragmatic to examine a strained cubic crystal first. Stress σ is the force intensity acting on a material. The stress deforms the crystal and generates strain . Depending on applied directions, the stress force can be divided into a shear and a normal component as shown in Fig. 6.8. Shear components of stress σ ij (i = j) will cause the crystal to rotate. In typical semiconductors, this type of deformation is rare and we will assume that σ ij = 0 for i = j. The normal components of stress (σ ij , i = j) will cause the crystal to expand or contract along the crystal axes. The deformed crystal remains rectangular. Since we are only considering normal components, the three normal forces σ 11 , σ 22 , and σ 33 can be abbreviated by σ 1 , σ 2 , and σ 3 . The σ i ’s are defined as positive for outward directed forces. In a uniform crystal, within the elastic limit of the material, the induced strain tensors from the applied stress are simply related by Hooke’s law, = sσ or σ = C, where the proportion constant s and C are the compliance and Young’s modulus of the
218
6 Heterostructure Fundamentals
z
Fig. 6.8 Components of stress tensor, σ ij
y x
σij. crystal, respectively. Under a homogeneous stress σ ij , excluding shear components of stress, the resulting homogeneous strain i j is a linear combination of all components of the stress, where i, j = 1, 2, and 3 corresponding to the crystallographic x, y, and zaxis. Thus, for example, i j = si j11 σ11 + si j12 σ12 + si j13 σ13 + si j21 σ21 + si j22 σ22 + si j23 σ23 + si j31 σ31 + si j32 σ32 + si j33 σ33
(6.12)
and eight similar equations for the other eight components of i j . Alternatively, the generalized Hooke’s law may be also conveniently written as σi j = Ci jkl kl
(6.13)
The Ci jkl are the 81 elastic stiffness coefficients or the elastic moduli of the crystal, where i, j, k, and l take on values of 1, 2, and 3 corresponding to the crystallographic x, y, and zaxis. Under homogeneous stress, a body must experience balanced forces to maintain statistical equilibrium, which implies that some of the strain components must be interrelated to prevent a net rotation of the body. For example, a homogeneous force is applied on the faces along the xaxis and perpendicular to the y and zaxis of a unit cube. The shear components of the stress have to be balanced, e.g., σ23 = σ32 , to prevent any rotation or translation of the crystal body. As a consequence, one must have σi j = σ ji and kl = lk
(6.14)
Ci jkl = Ci jlk and Ci jkl = C jikl
(6.15)
In general,
Thus the number of independent Ci jkl is reduced from 81 to 36 and can be expressed as a 6 × 6 tensor. We can further simplify the notation of Ci jkl by abbreviating the first two and last two suffixes into a pair of single digit number of 1–6 in the following way:
6.2 Strained Layer Structures
219
tensor notation 11 22 33 23,32 13,31 12,21 matri x notation 1 2 3 4 5 6 Now we can transform the elastic constant Ci jkl into Cmn such that Ci jkl = Cmn (i, j, k, l = 1, 2, 3; m, n = 1, 2, . . . 6)
(6.16)
and σi j = Ci jkl kl becomes σm = Cmn n . Thus the array of Cmn is expressed in a 6 × 6 matrix as ⎤ ⎡ C11 C12 C13 C14 C15 C16 ⎢C C C C C C ⎥ ⎢ 21 22 23 24 25 26 ⎥ ⎥ ⎢ ⎢C C C C C C ⎥ (6.17) Cmn = ⎢ 31 32 33 34 35 36 ⎥. ⎢ C41 C42 C43 C44 C45 C46 ⎥ ⎥ ⎢ ⎣ C51 C52 C53 C54 C55 C56 ⎦ C61 C62 C62 C64 C65 C66 By requiring that the symmetry of the crystal be replicated in the elastic coefficient matrix, the matrix can be further reduced. For a cubic crystal, the tensor form of stress and strain is reduced to ⎡ ⎤ ⎡ ⎤⎡ ⎤ σ1 1 C11 C12 C12 0 0 0 ⎢σ ⎥ ⎢C C C ⎢ ⎥ ⎥ ⎢ 2 ⎥ ⎢ 12 11 12 0 0 0 ⎥⎢ 2 ⎥ ⎢ ⎥ ⎢ ⎥⎢ ⎥ ⎢ σ3 ⎥ ⎢ C12 C12 C11 0 0 0 ⎥⎢ 3 ⎥ (6.18) ⎢ ⎥=⎢ ⎥⎢ ⎥ ⎢ σ4 ⎥ ⎢ 0 0 0 C44 0 0 ⎥⎢ 4 ⎥ ⎢ ⎥ ⎢ ⎥⎢ ⎥ ⎣ σ5 ⎦ ⎣ 0 0 0 0 C44 0 ⎦⎣ 5 ⎦ σ6 6 0 0 0 0 0 C44 If only the normal stress is considered in diamond and zincblende crystals, the general form of Hooke’s law can be simplified as ⎡
⎤ ⎡ ⎤⎡ ⎤ σ1 C11 C12 C12 1 ⎣ ⎦ ⎣ ⎦ ⎣ σ = σ2 = C12 C11 C12 2 ⎦ σ3 C12 C12 C11 3
(6.19)
where n measures the fractional increase (n > 0) or decrease (n < 0) of the crystal lattice along the nth axis. The above expression assumed that all the offdiagonal elements are equal, and all the diagonal elements are also equal, leaving us with only two elastic moduli, C 11 and C 12 , in cubic crystals. In common semiconductors, C 11 > C 12 > 0 and has a unit of 1011 dyn/cm2 . In less symmetric crystals, such as III–V compounds, more C mn components may need to be specified. For a hexagonal crystal, e.g., wurtzite structure, the relation between stress and strain is expressed as
220
6 Heterostructure Fundamentals
⎤ ⎡ C11 σ1 ⎢σ ⎥ ⎢C ⎢ 2 ⎥ ⎢ 12 ⎢ ⎥ ⎢ ⎢ σ3 ⎥ ⎢ C13 ⎢ ⎥=⎢ ⎢ σ4 ⎥ ⎢ 0 ⎢ ⎥ ⎢ ⎣ σ5 ⎦ ⎣ 0 σ6 0 ⎡
C12 C11 C13 0 0 0
C13 C13 C33 0 0 0
0 0 0 C44 0 0
⎤⎡ ⎤ 1 0 0 ⎥⎢ ⎥ 0 0 ⎥⎢ 2 ⎥ ⎥⎢ ⎥ 0 0 ⎥⎢ 3 ⎥ ⎥⎢ ⎥ ⎥⎢ 4 ⎥ 0 0 ⎥⎢ ⎥ ⎦⎣ 5 ⎦ 0 C44 6 0 21 (C11 − C12 )
(6.20)
(b) Biaxial strain During the epitaxial growth of latticemismatched layers, stress is applied equally to all inplane lattices (xy plane) such that σ 1 = σ 2 , and no stress is applied along the growth direction (zaxis), σ 3 = 0. For this condition, as shown in Fig. 6.9, the crystal is under biaxial strain. When the lattice constant of the epilayer is smaller than that of the substrate, the stress is directed outward (σ 1 > 0), and the resulting strain is a biaxial tensile strain. In contrast, the stress is directed inward (σ 1 < 0) for epilayer with a larger lattice constant than the substrate and gives rise to biaxial compressive strain. With σ 3 = 0 and 1 = 2 , the strain in the growth direction 3 can be calculated from Hooke’s law (6.19). σ3 = 0 = C12 1 + C12 2 + C11 3 = 2C12 1 + C11 3
(6.21)
Therefore, 3 = −
2C12 1 C11
(6.22)
Here, the inplane strains are defined as 1 = 2 ≡
Fig. 6.9 Relationship between stress and strain
as − ae ae
(6.23)
6.2 Strained Layer Structures
221
where as and ae are the lattice constants of the substrate and the epilayer, respectively. The inplane stress and strain relationship is also derived from Hooke’s law. Using the relationship between the strain components derived above, we can find σ1 = σ2 = C11 1 + C12 2 + C12 3 C12 2 C12 = C11 1 1 + −2 C11 C11
(6.24)
(c) Hydrostatic stress When a uniform pressure is applied equally to all sides of the crystal, the material is under a hydrostatic stress (Fig. 6.10). The inwarddirected stress is defined as a differential pressure change, dP, surrounding the crystal. Applying this relationship to Hooke’s law, we have −dP = 1 C11 + C12 (2 + 3 ) −dP = 2 C11 + C12 (1 + 3 ) −dP = 3 C11 + C12 (1 + 2 )
(6.25)
The above equations can be simplified by adding both sides together. 1 dP = − (C11 + 2C12 )(1 + 2 + 3 ) 3
(6.26)
The strain measures the fractional change of the crystal lattice along a major axis, i.e., n =
as − an an = an an
(6.27)
where as and an are the substrate lattice constant and unstrained lattice constant of the epilayer, respectively. Assume the volume of a cubic crystal is given by V = a1 a2 a3 , where ai defines the length of each side of the cube. Under a uniform pressure, the Fig. 6.10 Schematic of hydrostatic stress applied to a crystal
222
6 Heterostructure Fundamentals
sides of the volume change to (a1 + a1 ), (a2 + a2 ), and (a3 + a3 ). Then the volume change becomes V = (a1 + a1 )(a2 + a2 )a3 + (a1 + a1 )a3 a2 + a2 a3 a1 ∼ = a1 a2 a3 + a1 a3 a2 + a2 a3 a1
(6.28)
In the final form of the volume change, the higherorder terms of ai are neglected for ai ai . Since the strain n ≡ an /an , the total strain of the crystal under the uniform pressure is a1 a2 a3 + + a1 a2 a3 a1 a2 a3 + a1 a3 a2 + a2 a3 a1 = a1 a2 a3
1 + 2 + 3 =
(6.29)
The total strain is, therefore, directly related to the induced fractional volume change. 1 + 2 + 3 ∼ = V /V = d(ln V )
(6.30)
The straininduced volume change also produces a bandgap variation in a semiconductor that is expressed as dE = ad
V = ad (1 + 2 + 3 ) V
(6.31)
where the proportional constant ad (eV) is the hydrostatic deformation potential. Combining dE and dP, we can derive the expression of ad as 1 dE . ad = − (C11 + 2C12 ) 3 dP
(6.32)
Because dE/ dP > 0 and C mn are positive values, ad < 0. This relationship allows one to determine ad from the pressure dependence of the energy gap. The hydrostatic deformation potential ad has a conduction band component (ac ) and a valence band component (av ). They are related by the following equations: ad = ac − av
(6.33a)
E chy = ac
V = ac (1 + 2 + 3 ) V
(6.33b)
E vhy = av
V = av (1 + 2 + 3 ) V
(6.33c)
6.2 Strained Layer Structures hy
223
hy
where E c and E v are straininduced shift of the conduction and valence band edges, respectively.
6.2.3 Strain Effect on BandEdge Energies In a strained lattice structure, due to elastic deformation energy, there is a corresponding bandgap energy change from its equilibrium value. The elastic deformation energy consists of two parts: the hydrostatic term and the shear term. The hydrostatic term is proportional to the change in volume of the crystal lattice created by the strain. The shear term represents the energy shift due to the asymmetry in the strain parallel and perpendicular to the stress plane. By adding these two energy terms into the modelsolid approach, the variation of the band edges in a strained heterojunction can be derived. Again, we will determine the absolute reference energy level first. This energy level in the valence band is modified by the hydrostatic component of the strain and expressed as s = E v,av + E v,av = E v,av + av E v,av
V V
(6.34)
where E v, av is the reference energy level of the unstrained material. The position of the topmost valence band in a biaxialstrained semiconductor becomes s + E v = E v,av
so 3
so 3
(6.35)
C12 as − ae and 3 = −21 ae C11
(6.36)
= E v,av + av (1 + 2 + 3 ) + where 1 = 2 =
Therefore, the topmost valence band can be written as C11 − C12 so E v = E v,av + = E v0 + E vhy + 2av 1 3 C11
(6.37)
hy
where E v0 ≡ E v,av + so /3 is the unstrained valence band edge. E v represents the strain contribution to the valence bandedge shift and is defined as E vhy ≡ av (1 + 2 + 3 ) = 2av 1
C11 − C12 C11
(6.38)
224
6 Heterostructure Fundamentals
When growing epilayers with a larger lattice constant than the substrate, the inplane strain (1 = 2 ) is negative in the compressive strained system. Since av > 0, and C 11 > C 12 > 0, the resulting straininduced valence band shift has a negative value hy (E v < 0). The topmost valence band edge is shifted downward by the compressive strain. For the epilayer with a smaller natural lattice constant than the substrate, the inplane strain becomes positive in the tensile strained system. This leads to a positive valence bandedge shift, where the topmost valence band edge moves upward. Under biaxial strains, the conduction band edge also gets modified by the hydrostatic component of the strain from the unstrained value by an amount of E chy
C11 − C12 V = ac (1 + 2 + 3 ) = 2ac 1 ≡ ac V C11
(6.39)
The new position of the biaxialstrained conduction band edge becomes E c = E v0 + E g + E chy
(6.40)
Since ac is negative in direct bandgap materials, the strain effect on the conduction bandedge shift is opposite to that of the valence band. In compressive strained systems, 1 = 2 < 0, ac < 0, and C 11 > C 12 > 0, the hy resulting straininduced conduction band shift has a positive value (E v > 0). The conduction band edge is shifted upward by the compressive strain. Under tensile hy strains, 1 = 2 > 0 and E v < 0. The conduction band edge is now shifted downward by the tensile strain. The topmost valence band edge of Si, Ge, and most III–V compound semiconductors, such as GaAs, InP, and InAs, is twofold degenerate. For most III–V semiconductors, the splitoff bands are several hundred millielectron volts below the heavyhole and lighthole bands. Therefore, the coupling between these bands can be ignored to simplify discussions. Under latticemismatchinduced biaxial strain, the heavy and lighthole states at k = 0 are split by the shear component of the strain, E vsh . The bandedge energy of the heavyhole band and lighthole band is further modified by E vsh as defined below.
E vsh
1 + 2 − 3 ≡b 2
= b1
C11 + 2C12 C11
(6.41)
where b < 0 is the shear deformation potential. At the zone center (k = 0), the shifts of bandedge energies of heavyhole and lighthole bands due to shear strain are sh E hh = +E vsh = b1
and
C11 + 2C12 C11
(6.42)
6.2 Strained Layer Structures
225
E lhsh = −E vsh = −b1
C11 + 2C12 C11
(6.43)
The general expressions for the biaxialstrained band edges are E v = E v,av +
so sh , E lhsh + E vhy + max E hh 3
(6.44)
so + E g + E chy 3
(6.45)
E c = E v,av +
Under compressive strains, 1 < 0 and b < 0, the resulting shear strain has a positive value (E vsh > 0). The heavyhole band edge is shifted upward and the lighthole band edge moves downward. In tensile strain systems, 1 > 0. This leads to a negative shear strain component (E vsh < 0). The split valence band edges move downward and upward for heavyhole and lighthole bands, respectively. The complete bandgap diagram for cubic semiconductors under different stresses is shown in Fig. 6.11. Combining (6.38) through (6.43), the bandgap energies for conduction band to heavyhole band (C–HH) transition and conduction band to lighthole band (C–LH) transition can be summarized as follows:
hy
E c−hh = E g + E chy − E vhy − E vsh
(6.46)
E c−lh = E g + E chy − E vhy + E vsh
(6.47)
hy
Remember, E c and E vsh are positive and E v is negative under compressive strains. Under tensile strains, these parameters change signs.
Fig. 6.11 Qualitative conduction and valence bandedge shifts for biaxial tensile and compressive strain
226
6 Heterostructure Fundamentals
Since ad = ac − av , it is convenient to group the two hydrostatic strain terms into a single term and redefine as E hy = E chy − E vhy = ad (1 + 2 + 3 ) ≡ −δ E hy
(6.48)
and 1 1 = b (1 + 2 ) − 3 ≡ − δ E sh 2 2
E vsh
(6.49)
The effective bandgap energies are given by 1 E c−hh = E g + E hy − E vsh = E g − δ E hy + δ E sh 2
(6.50)
1 E c−lh = E g + E hy + E vsh = E g − δ E hy − δ E sh 2
(6.51)
Example: Strained Ge/Si heterojunction As an example of the application, we consider the pseudomorphic Si/Ge interface on (001)Si. The relevant material parameters of Si and Ge are listed in Table 6.2. From the table, we found the following unstrained parameters: E v,av (Si) = −7.03 (eV), so (Si) = 0.044(eV) E v,av (Ge) = −6.35 (eV), so (Ge) = 0.30 (eV) The position of the topmost valence band in Si is E v (Si) = −7.03 + 0.044/3 = −7.015 (eV). Since the Ge layer is compressively strained, the valence band is also modified. For the strained Ge, 1 = 2 = (5.4309 − 5.6575)/5.6575 = −0.04005, 3 = 0.03009, so that using av = 1.24, b = −2.9, and V/V = −0.05002, we get the topmost absolute reference energy level as E v (Ge) = E v,av (Ge) + so /3 + E vhy + E vsh = −6.35 + (0.30/3) + 1.24(−0.05) + (−2.9)(−0.04005)[(12.40 + 8.26)/12.40] = −6.1185 (eV) The valence band offset E v = E v (Ge) – E v (Si) = −6.1185− (−7.015) = 0.91(eV). This value agrees well with the experimentally determined value for E v of 0.81 eV.
5.4309
5.6575
Si
Ge
a0 (Å)
0.30
0.044
so (eV) 1.98 −8.24
−6.35
ac (dir) (eV)
−7.03
E v,av (eV) −1.54
4.18
ac (ind) (eV) 1.24
2.64
av (eV)
Table 6.2 Material parameters for semiconductor Si and Ge at room temperature
−2.9
−2.1
b (eV) 0.664
1.124
E g (eV)
12.40
16.577
C 11 (1011 dyn/cm2 )
4.13
6.393
C 12 (1011 dyn/cm2 )
6.2 Strained Layer Structures 227
228
6 Heterostructure Fundamentals
6.3 BandEdge Energies in Strained Ternary and Quaternary Alloys To derive valence band positions for an alloy, linear interpolation between the nearly latticematched pure materials (binary compounds) is appropriate. When the constituent materials are not latticematched, a strain contribution should be included in the calculation. This is because, in the alloy, one material is effectively expanded, whereas the other is compressed. For a ternary alloy Ax B1−x C, the topmost valence band position has the following expression [11]:
a E v (x) = x E v (AC) + (1 − x)E v (BC) + x(1 − x) −3av a0
(6.52)
where a0 = xa0 (AC) + (1 − x)a0 (BC) and a = a0 (AC) − a0 (BC). The last term in the equation shown above includes a bowing parameter C due to hydrostatic strain contribution, where a a = 3[av (AC) − av (BC)] (6.53) C ≡ 3av a0 a0 Example: Ga0.47 In0.53 As/InP latticematched heterojunction From Table 6.1, we have the following parameters: E v,av (GaAs) = −6.92 (eV), so (GaAs) = 0.34 (eV), E g (GaAs) = 1.424 (eV) E v,av (InAs) = −6.67 (eV), so (InAs) = 0.39 (eV), E g (InAs) = 0.354 (eV) E v,av (InP) = −7.04 (eV), so (InP) = 0.108 (eV), E g (InP) = 1.353 (eV) Then, E v (GaAs) = −6.92 + 0.34/3 = −6.806 eV E v (InAs) = −6.67 + 0.38/3 = −6.540 eV Although Ga0.47 In0.53 As/InP heterojunction is a latticematched system, both GaAs and InAs are latticemismatched to InP. Therefore, it is necessary to use (6.52) to calculate the topmost valence band edge of Ga0.47 In0.53 As as follows: E v (Ga0.47 In0.53 As) = 0.47 × E v (GaAs) + 0.53 × E v (InAs) + 3 × 0.47 × 0.53 × (−1.16 + 1.0)(5.653−6.058)/5.87 = −6.6568 eV
6.3 BandEdge Energies in Strained Ternary and Quaternary Alloys
229
E v (InP) = −7.04 + 0.108/3 = −7.004 eV E v = −7.004−(−6.6568) = −0.3472 eV This indicates that the valence band in InP is below the valence band in Ga0.47 In0.53 As. This calculated value is very close to the experiment results (between 0.325 and 0.38 eV) determined by various methods. Next, we will determine the conduction band discontinuity, E c . E c (InP) = E v (InP) + E g (InP) = −7.004 + 1.353 = −5.651 eV E g (Ga0.47 In0.53 As) = x E g (GaAs) + (1 − x)E g (InAs) + x(1 − x)C = 0.47 × 1.424 + 0.53 × 0.354 − 0.47 × 0.53 × 0.477 = 0.7381 eV E c (Ga0.47 In0.53 As) = E v (Ga0.47 In0.53 As) + E g (Ga0.47 In0.53 As) = −6.6568 + 0.7381 = −5.9187 eV E c = −5.651 − (−5.9187) = 0.2677 eV The conduction band edge of InP is 0.2677 eV above Ga0.47 In0.53 As. Therefore, the Ga0.47 In0.53 As/InP heterojunction has a typeI band alignment. Example: Ga0.7 In0.3 As/GaAs strained quantum well for 0.98 μm lasers In this problem, we need to know E v , C 11 and C 12 in order to calculate E c and E v of the Ga0.7 In0.3 As/GaAs system. From the previous examples, we found E v (GaAs) = −6.806 eV, E c (GaAs) = −5.382 eV, and E v (InAs) = −6.54 eV Since this is a strained system, except for C 11 and C 12 , we cannot use linear interpolation between GaAs and InAs to calculate E v . Instead, we use (6.52) to include the strain effect. E v (Ga0.7 In0.3 As) = 0.3E v (InAs) + 0.7E v (GaAs) + 3x(1 − x)[−av (InAs) + av (GaAs)] {(aInAs −aGaAs )/[x aInAs +(1 −x)aGaAs ]} = −6.720 eV Using linear interpolation, we found C 11 (GaInAs) = 10.815 × 1011 and C 12 (GaInAs) = 5.124 × 1011 . Then
230
6 Heterostructure Fundamentals
E c (Ga0.7 In0.3 As) = E v (Ga0.7 In0.3 As) + E g (Ga0.7 In0.3 As) + 2ac 1 (C11 −C12 )/C11 where as − ae 5.653 − 5.775 = −0.0211 = ae 5.775 ac = −6.543 E g (Ga0.7 In0.3 As) = 0.7 × 1.424 1 =
+ 0.3 × 0.354−0.7 × 0.3 × 0.477 = 1.003 eV E c (Ga0.7 In0.3 As) = −6.730 + 1.003 + 0.145 = −5.582 eV E c = −5.382 + 5.582 = 0.20 eV The heavyhole energy level in Ga0.7 In0.3 As can be calculated as follows (6.44) E hh (Ga0.7 In0.3 As) = E v (Ga0.7 In0.3 As) C11 − C12 C11 + 2C12 + 2av 1 + b1 C11 C11 Using linear interpolation, we found av = 1.112 and b = −1.94. Then, E hh (Ga0.7 In0.3 As) = −6.720−0.0145 + 0.0469 = −6.6877 eV E v = −6.806 + 6.6877 = −0.1183 eV Therefore, the Ga0.7 In0.3 As/GaAs system has a typeI heterostructure. The methods of deriving quaternary semiconductor parameters from those of the underlying binary and ternary alloys have been discussed in Sect. 4.5.2. Both quaternary bandgap energy E g and spinorbit splitting so can be derived from (4.87) using bowing parameters listed in Table 4.6. To calculate E v, av using (4.87), the necessary ternary bowing parameters C are obtained according to (6.53). For strained quaterhy nary alloys, additional relevant parameters including E v and δ E sh are needed to derive the valence bandedge energy E v that can be obtained from binary data using Vegard’s law. Example: (Al0.48 In0.52 As)0.6 (Ga0.47 In0.53 As)0.4 /InP latticematched heterojunction For this unstrained III–V quaternary compound, only a onedimensional subset of the vast twodimensional space of compositions (x, y) that is latticematched to a common binary substrate material (i.e., InP) is considered. Then the band parameters of a quaternary alloy may be represented as a combination of two latticematched constituents of ternary alloys. Letting α (e.g., Al0.48 In0.52 As) and β (e.g.,
6.3 BandEdge Energies in Strained Ternary and Quaternary Alloys
231
Ga0.47 In0.53 As) represent two latticematched ternary end point constituents, the combination of α and β with arbitrary composition z forms the latticematched quaternary α 1−z β z . Although the two ternary constituents have identical lattice constants, their binary constituents are not latticematched. Therefore, the expression of the valence band alignment of the quaternary has to include a bowing parameter due to hydrostatic strain contributions. In this example, the composition of the quaternary (z = 0.4) has the form of Alx (Gay In1−y )1−x As with x(AlAs) = 0.288 and y(GaAs) = 0.188. To apply (4.87) to this typeII quaternary alloy, one binary can be assigned twice in the same row or column of the matrix with a zero ternary bowing factor. Let B1 , B2 = B3 , and B4 represent binary parameters of GaAs, AlAs, and InAs, respectively, and C 23 = 0. To calculate E v,av it is necessary to get ternary bowing factors of deformation potentials first. Following (6.53), C12 = 3 avGaAs − avAlAs (aGaAs − aAlAs )/aInP = 0.0053 C14 = 3 avGaAs − avInAs (aGaAs − aInAs )/aInP = −0.0331 C34 = 3 avAlAs − avInAs (aAlAs − aInAs )/aInP = −0.2984 Together with reference energy parameters (E v, av ) B1 = −6.92, B2 = −7.49, B4 = −6.67 (eV), and set D = 0.03 in (4.87), E v,av reaches a value of E v,av (Q) = − 6.9917 (eV). Next we need to calculate so of the quaternary alloy using (4.87) with the following spinorbit splitoff parameters: B1 = 0.341, B2 = B3 = 0.28, B4 = 0.39 (eV), C 12 = 0, C 14 = −0.15, C 34 = −0.15, and D = 0. The result of so (Q) = 0.310 (eV). Thus the valence band edge of the quaternary alloy becomes E v (Q) = E v,av (Q) +
so (Q) = −6.8884eV 3
From the previous example, we found E v,av (InP) = −7.004 eV. Thus E v = −6.8884 + 7.004 = 0.1156eV. The valence band edge of the quaternary is located at a higher energy than InP by 0.1156 eV.
6.4 Strained Nitrides with Wurtzite Crystal Structure 6.4.1 BandEdge Energies of Strained Nitrides The energy band edges of wurtzite crystals are modified under stress similarly to those of the zincblende crystal. For example, for the commonly encountered case of growing a strained wurtzite nitride layer pseudomorphically on the (0001) surface of a sapphire substrate, the epitaxial layer experiences inplane biaxial strain but
232
6 Heterostructure Fundamentals
zero stress along the zdirection. For simplicity, the shear components of stress are neglected (i.e., 4 = 5 = 6 = 0). Therefore, the latticemismatch induced strains are expressed as 1 = 2 =
as − ae 2C13 and 3 = − 1 ae C33
(6.54)
where as and ae are the lattice constants of the substrate and the epitaxial layer, respectively. The second relation is obtained by solving σ3 = 0 in (6.20). The induced strains for other stress conditions can also be derived using proper boundary conditions. The straininduced elastic deformation energy causes a bandgap energy change from its equilibrium value as in the zincblende crystal structure. Again, the elastic deformation energy consists of two parts: the hydrostatic term and the shear term. To describe the valence band structure of GaN under strain, six valence band deformation potentials (Di ) are necessary. The parameters D1 and D2 are associated with the valence band hydrostatic deformation potential, av , and D3 and D4 are related to the shear deformation potential, b. The valence bandedge energies at k = 0 in the strained crystal are modified as ⎧ E 1 = 1 + 2 + λ + θ ⎪ ⎪ ⎪ ⎪ ⎪ ⎪ 1 − 2 + θ 2 1 − 2 + θ ⎨ + λ + E2 = + 223 2 2 ⎪ ⎪ ⎪ ⎪ 1 − 2 + θ 2 − + θ 1 2 ⎪ ⎪ + λ − + 223 ⎩ E3 = 2 2
(6.55)
where 1 = cr , 2 = 3 = so , and the straininduced energy shifts are λ = D1 3 + D2 (1 + 2 )
(6.56)
θ = D3 3 + D4 (1 + 2 )
(6.57)
The conduction band edge at k = 0 is modified and expressed as E c = E g + 1 + 2 + Pc
(6.58)
Pc = acz 3 + act (1 + 2 )
(6.59)
where Pc is the conduction band hydrostatic energy shift and related to the longitudinal and transverse interband deformation potentials a1 and a2 , respectively, as a1 = acz − D1 a2 = act − D2
(6.60)
6.4 Strained Nitrides with Wurtzite Crystal Structure Table 6.3 Band structure parameters for wurtzite nitride binaries: inplane lattice constant a, longitudinal (caxis) lattice constant, bandgap energy at 0 K E g (0), bandgap fitting parameters α and β, spinorbit splitoff energy so , crystalfield splitting energy cr , longitudinal hydrostatic deformation potential a1 , inplane hydrostatic deformation potential a2 , valence band hydrostatic deformation potential D1 and D2 , shear deformation potential D3 and D4 , elastic constants C 11 , C 12 , C 13 , C 33 , and C 44 , piezoelectric coefficients e13 and e33 , and spontaneous polarization Psp [12]
233
Parameters
GaN
AlN
InN
a (Å) @300 K
3.189
3.112
3.545
c (Å) @300 K
5.185
4.982
5.703
E g (0) (eV) @0 K
3.510
6.25
0.69a
α (meV/K)
0.909
1.799
0.41a
β (K)
830
1462
454a
cr (eV)
0.010
−0.169
0.040
so (eV)
0.017
0.019
0.005
a1 (eV)
−4.9
−3.4
−3.5
a2 (eV)
−11.3
−11.8
−3.5
D1 (eV)
−3.7
−17.1
−3.7
D2 (eV)
4.5
7.9
4.5
D3 (eV)
8.2
8.8
8.2
D4 (eV)
−4.1
−3.9
−4.1
C 11 (1011 dyn/cm2 )
39.0
39.6
22.3
dyn/cm2 )
14.5
13.7
11.5
C 13 (1011 dyn/cm2 )
10.6
10.8
9.2
C 33 (1011 dyn/cm2 )
39.8
37.3
22.4
(1011
C 12
(1011
C 44
dyn/cm2 )
10.5
11.6
4.8
e31 (C/m2 )b
−0.34
−0.53
−0.41
e33 (C/m2 )b
0.67
1.50
0.81
−0.034
−0.090
−0.042
Psp
(C/m2 )
a [13] b [14]
The relevant band structure parameters for wurtzite nitride binary alloys are shown in Table 6.3. Thus, the interband transition energy of the system is E c − E 1 = E g + Pc − λ − θ = (acz − D1 )3 + (act − D2 )(1 − 2 ) − D3 3 − D4 (1 + 2 )
(6.61)
Figure 6.12 shows the energy bands of a strained GaN crystal as functions of the inplane strain using E v0 of an unstrained GaN as a reference energy at 0 eV.
234
6 Heterostructure Fundamentals
Fig. 6.12 Band energies of a the conduction band and b the HH, LH, and CH bands of a strained GaN crystal as functions of the inplane strain 1 . The reference energy is set at E v0 of an unstrained GaN crystal. Reprinted with permission from [15], copyright IEEE
6.4.2 Natural Band Alignments of IIINitrides The band discontinuities at the heterojunction of IIIN systems are complicated due to the large electrostatic fields originating from the polar interface and the ionic nature of the wurtzite crystal. Because of this and other straininduced effects, the natural band alignment could not be accurately determined. The measured band alignments of binary IIInitride heterojunctions do not even follow the commutative property such that, e.g., GaN/AlN and AlN/GaN structures are not equivalent. Recently, the ‘natural’ band alignments of wurtzite IIInitride semiconductor heterojunctions have been determined directly on the nonpolar sidefacet of a vertically aligned nanorod array grown along the caxis. The nanorod structure warrants a near fully relaxed lattice structure without the influence of spontaneous and piezoelectric polarization fields. Using microscopicarea photoelectron spectroscopy, the
6.4 Strained Nitrides with Wurtzite Crystal Structure
235
Fig. 6.13 Schematic of ‘natural’ band alignments for InN, GaN, and AlN. The corresponding values of E g , E v , and E c are shown in the graph. The determined VBOs for GaN/AlN, InN/GaN, and InN/AlN heterojunctions are 0.6 ± 0.1 eV, 0.8 ± 0.1 eV, and 1.4 ± 0.1 eV, respectively [16]
VBOs of InN/GaN, GaN/AlN, and InN/AlN are measured to be 0.8 ± 0.1, 0.6 ± 0.1, and 1.4 ± 0.1 eV, respectively. The measured E v along with E g and deduced E c are summarized in Fig. 6.13. TypeI heterostructures are formed between all wurtzite IIInitrides.
6.5 Construction of Heterostructure Band Diagrams Once the conduction band and valence band discontinuities are determined, we can proceed to construct the approximate heterostructure band diagrams without detailed calculation. However, an accurate treatment requires a selfconsistent numerical solution of Poisson’s equation for the electrostatic potential as shown in the next chapter.
6.5.1 Anisotype Np Heterojunctions The band diagram construction method for a heterojunction is very similar to that for a doped homostructure, but we need to take account of the discontinuities E c and E v . Using an Np heterojunction as an example, as shown in Fig. 6.14, one starts with flat bands in each material as determined by Anderson’s rule and the Fermi levels set by the doping on each side. The capital and lower case letters of the Np
236
6 Heterostructure Fundamentals
Ec1
Ec
' Ec1
EF1 ' Ev1 Ev1
Ec2 EF2
qV0 Ev2
Ev
Fig. 6.14 Equilibrium band diagrams (flat band) of a Pn heterojunction before contacting each other. The relative position of the conduction band edge is determined by E c and E v
Ec1 Ec EF1
qVa
Ev1 Ev
Ec2 EF2 Ev2
Fig. 6.15 Completed energy band diagram of an isotype Pn heterostructure under a bias voltage of V a
heterojunction represent that the larger and smaller bandgap semiconductors are ntype and ptype, respectively. To temporarily cancel out the effect of discontinuities, = E c1 – E c and E v1 = E v1 + E v . Now the ‘effective’ bandgap is draw lines E c1 the same on both sides. Next, as shown in Fig. 6.15, align the Fermi levels. The difference in Fermi levels far from the junction is set with the applied voltage, V a . So, E F2 − E F1 = qV a . Then to E c2 , and E v1 to E v2 , with parallel Sshaped curves due to the electrostatic join E c1 potential. The slope of the curve is set by the charge density distribution. Now restore E c1 on side 1 as a line at E c1 + E c and E v1 at E v1 − E v , including the discontinuities in E c and E v at the junction. The band discontinuities are inserted at the midpoints of Sshaped curves. This completes the sketch of the band diagram shown in Fig. 6.15.
6.5 Construction of Heterostructure Band Diagrams
Ec1 EF1
Ec qVa
237
Ec2 EF2
Ev1 Ev Ev2 Fig. 6.16 Energy band diagram of an isotype pN heterujunction under a bias of V a
6.5.2 Anisotype pN Heterojunctions The procedure for constructing the band diagram for a pN heterojunction is similar to that for the Pn heterojunction shown above. The finished band diagram is shown in Fig. 6.16.
6.5.3 Isotype Nn and Pp Heterojunctions Unlike in homostructures, a potential barrier can be formed in heterostructures even when both sides are doped similarly. This type of junction is called the isotype heterojunction as shown in Fig. 6.17. In Nn heterojunctions, the band discontinuity is mostly located in the valence band and acts as a hole blocker. In a properly designed N + n– heterojunction, electrons trapped in the potential energy notch in the conduction band form a twodimensional electron gas (2DEG). Fieldeffect transistors utilizing these electrons conducting parallel to the interface show very interesting properties. On the other hand, the band discontinuity in a Pp heterojunction is mostly across the conduction band and will prevent electrons from flowing through.
Fig. 6.17 Two types of isotype heterostructures: a Nn heterojunction showing the hole blocking due to E v . Electrons may be trapped in the energy notch formed in the conduction band. b Pp heterojunction showing the electron blocking due to E c
238
6 Heterostructure Fundamentals
The combination of isotype and anisotype heterostructures can further confine carriers for new transport and photonic device applications as illustrated in the following sections.
6.5.4 Current Confinement in Double Heterostructures The energy band diagrams for PpN or PnN double heterostructures (DH) are combinations of the anisotype and isotype heterojunctions previously described. In the zerobias P–n–N DH shown in Fig. 6.18, for example, the conduction band discontinuity E c provides a barrier to electrons at the Pn heterojunction and thus confines the injected electrons to the small bandgap nlayer. The valence band discontinuity E v at the nN heterojunction provides a potential barrier to holes and thus prevents hole injection into the Nlayer. These barriers result in both minority and majority confinement by the PnN double heterostructure. When a forward bias is applied, the distribution of V a between the Pn and nN heterojunctions is determined by the requirement of current continuity through the device. The band diagram of a PnN DH under forward bias is shown in Fig. 6.19. The carrier distributions as functions of energy are also shown. Although the DH provides majority and minority carrier confinement at zero bias, the band bending associated with applied bias V a lowers the barrier heights. The electron and hole distribution in the conduction band and valence bands may extend beyond the band discontinuities E c and E v , respectively. The electrons and holes above E c and E v , respectively, can leak out of the nregion. In a DH laser structure, these leakage currents will not contribute to stimulated emission. Another interesting situation in a DH is the carrier accumulation in the active region under a strong forward bias. Due to the carrier confinement by both Pn and nN heterojunctions, the injected carrier concentration exceeds the majority carrier concentration. This is labeled ‘superinjection’ by Zh. I. Alferov [17].
Fig. 6.18 Equilibrium energy band diagram of a PnN double heterostructure. Electrons and holes are blocked by Pn and nN heterojunctions, respectively, and trapped inside the ntype middle layer
6.5 Construction of Heterostructure Band Diagrams
239
Fig. 6.19 The energy band diagram of a PnN double heterostructure under a forward bias V a . Also shown are the electron and hole distributions as functions of energy. Most carriers are trapped inside the smaller bandgap nlayer. Only those carriers with energy higher than the barrier, shown as the shaded areas, can escape
Problems 1. InAsx Sb1−x ternary alloy has the highest electron mobility among all semiconductors. Recently, it has been used as the channel material of the psuedomorphic highelectronmobility transistor (pHEMT). It has also been considered as a channel material for future III–V MOSFET applications. An InAsx Sb1−x /Aly In1−y Sb pHEMT relies on the conduction band discontinuity at the heterojunction to form a high mobility twodimensional electron gas (2DEG). Assume the elastic modulii, C 11 and C 12 , and the deformation potentials, a and b, vary linearly between the two binaries and are listed below (in 1011 dyn/cm2 ): C 11 (AlSb) = 8.769; C 11 (InSb) = 6.669; C 11 (InAs) = 8.329 C 12 (AlSb) = 4.341; C 12 (InSb) = 3.645; C 12 (InAs) = 4.526 (a) Determine the composition x of InAsx Sb1−x which is latticematched to GaSb. (b) Calculate the conduction band discontinuity E c and valence band discontinuity E v between the latticematched InAsx Sb1−x and GaSb. Please use both modelsolid theory and the empirical method by Tiwari and Frank. Is this a typeI or typeII heterostructure? (c) If we wish to grow an InAsx Sb1−x on GaSb with a compressive strain of 1.8%, find the critical layer thicknesses of InAsx Sb1−x . (d) Find the critical layer thicknesses of Al0.8 In0.2 Sb grown on GaSb, (e) Calculate the conduction band discontinuity E c between InAsx Sb1−x (latticematched to GaSb) and strained Al0.8 In0.2 Sb. This value is very important for the pHEMT application. 2. At the 2008 International Electron Device Meeting (https://doi.org/10.1109/ iedm.2008.4796798), Intel demonstrated a pchannel, pseudomorphic, high hole mobility transistor by using compressively strained InSb QW as the channel material. Although the heavyhole band is lifted above the lighthole band in the growth direction under compressive strain, the hole effective mass becomes lighter in the direction parallel to the growth surface. (See Phys. Rev. B, vol. 43, pp. 9649, (1991)). The barrier material is Al0.35 In0.65 Sb.
240
6 Heterostructure Fundamentals
(a) Calculate the critical thickness of the InSb QW grown on Al0.35 In0.65 Sb. The Al0.35 In0.65 Sb barrier material is very thick and unstrained. (b) For a 5 nm InSb QW, determine the strain (), E c and E v . Assume no defects are generated in this heterostructure. 3. Consider the binary alloys AlSb, GaSb, and InAs. The lattice mismatches between these compounds are small, and highquality AlSb/InAs heterostructures can be grown on GaSb substrates. (a) Use the modelsolid theory and the data provided in Table 6.1 to find the band discontinuities, E c and E v , at AlSb/InAs and GaSb/InAs interfaces. Compare your results with experimental values shown in Fig. 6.4. (b) Find the critical layer thickness of InAs and AlSb grown on GaSb. (c) Draw the band diagram (conduction band and valence band) of the following heterostructure grown on GaSb: AlSb/InAs (30 Å)/GaSb (20 Å)/InAs (30 Å)/AlSb The three center layers form the active region of a Wtype laser. Discuss the type of heterostructures formed. (d) Calculate the emission energy of the laser structure of part (c) using the infinite quantumwell approach and the following effective mass data. The emission energy corresponds to the difference between the electron state in InAs QWs and the heavyhole state in the GaSb QW. m ∗e (InAs) = 0.024m 0 , m ∗hh (InAs) = 0.37m 0 , m ∗e (GaSb) = 0.044m 0 , m ∗hh (GaSb) = 0.34m 0 , m ∗e (AlSb) = 0.92m 0 , m ∗hh (AlSb) = 0.94m 0 , 4. Both Gax In1−x As and GaAsy Sb1−y can be grown latticematched on InP substrates. Assume the valence band energy of ternary alloys varies linearly between the two binaries. (A small error will be introduced, but is negligible for latticematched cases like this.) (a) Determine compositions x and y in Gax In1−x As and GaAsy Sb1−y , respectively, that are latticematched to InP. (b) Use the modelsolid theory to find the band discontinuities, E c and E v , at Gax In1−x As/InP and GaAsy Sb1−y /InP interfaces. 5. Strained Gax In1−x As grown on InP substrate is an important heterostructure for both photonic and electronic device applications. The bandgap energy variation of Gax In1−x As is expressed as E g () = 0.358 + 0.589x + 0.477x 2 Assume the elastic modulii, C 11 and C 12 , and the deformation potentials, a and b, vary linearly between the two binaries. (a) Find the critical layer thickness of Ga0.3 In0.7 As grown on InP. (b) Find the conduction band discontinuity, E c , and the valence band discontinuity, E v of strained Ga0.3 In0.7 As thin layer grown on InP.
6.5 Construction of Heterostructure Band Diagrams
241
(c) Determine the band discontinuities, E c and E v , between Al0.48 In0.52 As and InP (d) From the results of parts (b) and (c), calculate the band discontinuities E c and E v between Ga0.3 In0.7 As and Al0.48 In0.52 As (e) For a pHEMT structure consisting of (i) semiinsulating InP substrate, (ii) 12 nmthick undoped Ga0.3 In0.7 As, and (iii) 20 nmthick Sidoped Al0.48 In0.52 As (n ~ 2×1018 cm−3 ), plot the ‘flat’ band diagram; i.e., the Fermi levels are not aligned, for simplicity. However, in the Al0.48 In0.52 As layer, the exact location of E F should be calculated. (f) Plot a realistic qualitative band diagram of the structure of part (e). Assume the contact potential on the Al0.48 In0.52 As side of the Al0.48 In0.52 As/ Ga0.3 In0.7 As heterojunction is ~0.12 eV. 6. The bandgap energy of the quaternary alloy Gax In1−x Asy P1−y latticematched to InP can be expressed by E g (y) = 1.35 − 0.775y + 0.149y2 and x = 0.47y. (a) Determine the composition x and y such that the quaternary has a bandgap corresponding to 1.3 μm. (b) Determine E c and E v between the quaternary and InP. 7. In an Al0.25 Ga0.75 N/GaN highelectron mobility transistor, the undoped Al0.25 Ga0.75 N barrier is 200 Å in thickness and the GaN buffer layer grown on a sapphire substrate is fully relaxed. Calculate the conduction band discontinuity at the heterojunction.
References 1. R.L. Anderson, SolidState Electron. 5, 341 (1962) 2. W.A. Harrison, Electronic Structure and the Properties of Solids (Freeman, San Francisco, 1980) 3. J. Tersoff, Phys. Rev. B30, 4874 (1984); Phys. Rev. B32, 6968 (1985) 4. J. Tersoff, Heterojunction, vol. Discontinuities (North Holland, Amsterdam, 1987). Chapter 1 5. M. Cardona, N.E. Christensen, Phys. Rev. B35, 6182 (1987) 6. C.G. Van de Walle, R.M. Martin, Phys. Rev. B35, 8154 (1987) 7. C.G. Van de Walle, Phys. Rev. B39, 1871 (1989) 8. I. Vurgaftman, J.R. Meyer, L.R. RamMohan, J. Appl. Phys. 89, 5815 (2001) 9. S. Tiwari, D.J. Frank, Appl. Phys. Lett. 60, 630 (1992) 10. J.W. Mathews, A.E. Blakeslee, J. Crystal Growth. 27, 118 (1974) 11. Cardona and Christensen, Phys. Rev. B37, 1011 (1988) 12. I. Vurgaftman, J.R. Meyer, J. Appl. Phys. 94, 3675 (2003) 13. J. Wu, W. Walukiewicz, W. Shan, K.M. Yu, J.W. Ager III, S.X. Li, E.E. Haller, H. Lu, W.J. Schaff, J. Appl. Phys. 94, 4457 (2003) 14. A. Zoroddu, F. Bernardini, P. Ruggerone, V. Fiorentini, Phys. Rev. B64, 045208 (2001) 15. S.L. Chuang, IEEE J. Quantum Electron. 32, 1791 (1996) 16. C.T. Kuo, K.K. Chang, H.W. Shiu, C.R. Liu, L.Y. Chang, C.H. Chen, S. Gwo, Appl. Phys. Lett. 99, 122101 (2011) 17. Z.I. Alferov, V.B. Khalfin, R.F. Kazarinov, Sov. Phys. Solid State. 8, 2313 (1967) [Translated from Fiz. Tverd. Tela. 8, 3102 (1966)]
242
6 Heterostructure Fundamentals
Further Reading 1. H.C. Casey, M.B. Panish, Heterostructure Lasers: Part A (Academic Press, New York, Fundamental Principles, 1978) 2. J.F. Nye, Physical Properties of Crystals (Oxford University Press, New York, 1985) 3. S.L. Chuang, Phys. Photon. Dev., 2nd edn. (John Wiley & Sons, 2009)
Chapter 7
Electrical Properties of Compound Semiconductor Heterostructures
Abstract The pn junction and metal–semiconductor junction are the basic building blocks of modern electronic devices such as diodes and transistors. Under the equilibrium condition, a potential barrier is formed at these junctions such that no net charge carriers flow across the junction. An externally applied forward bias is needed to cause the flow of charged carriers and, thus, the current. In semiconductor heterostructures, as discussed in this chapter, due to the formation of energy band discontinuities in both conduction and valence bands at the heterojunction, extra energy barriers exist without resort to pn junctions. For example, under the equilibrium condition, typeI nN and pPtype heterostructures can block flows of holes and electrons, respectively. Furthermore, a triangular potential well is formed at the heterojunction to generate 2D electron gas in nNtype heterostructures and 2D hole gas in pPtype heterostructures. One important feature of heterostructures is the formation of the quantum well that has a farreaching impact on modern electronic and photonic device advancements. In this chapter, the electrical properties of heterojunctions will be developed first, followed by the analysis of quantumwell heterostructures and superlattices.
7.1 Abrupt Heterojunction Under Equilibrium 7.1.1 Qualitative Analysis of a pN Heterojunction in Equilibrium (a) General solutions of the potential distributions The general procedure of deriving the potential distribution in a pN or nP heterojunction closely resembles that of a homojunction. The mathematics is also based on Poisson’s equation and the charge neutrality condition across the junction and within the depletion region. To illustrate the calculation procedures, a pGaAs/NAlGaAs typeI heterojunction is used as an example. The equilibrium energy band diagram of this anisotype pN heterojunction, as shown in Fig. 7.1, is developed in the following. © Springer Nature Switzerland AG 2020 K. Y. Cheng, III–V Compound Semiconductors and Devices, Graduate Texts in Physics, https://doi.org/10.1007/9783030519032_7
243
244
7 Electrical Properties of Compound Semiconductor Heterostructures
pGaAs
EF
NAlGaAs
Ec
Ec1
qVN
Eg1
Ec2 EF
Ev1
qVp
Eg2
Ev
Ev2
W –xp
0
xN
x
Fig. 7.1 Equilibrium energy band diagram of an anisotype pGaAs/NAlGaAs heterojunction
For a pN heterojunction, the charge neutrality condition requires that q ANa x p = q AN D x N
(7.1)
where A is the cross section of the junction, N a and N D are the doping concentrations, and x p and x N are the depletion widths of the p and Ntype materials, respectively. The distributions of the electric field intensity F and the potential distribution V are derived from Poisson’s equation. q dF ρ d2 V (x) = − = − p − n + N D+ − Na− = − 2 dx dx
(7.2)
Neglecting the free carriers p and n in the depletion region, Poisson’s equation on either side of the heterojunction becomes −
dF = dx
−q N D / N , 0 < x < x N q Na / p , −x p < x < 0
(7.3)
where p and N are the permittivity in the p and Nregions, respectively. The electric field intensities on both sides of the junction are obtained by integration. F=
q N D x/ N + A, 0 < x < x N −q Na x/ p + B, −x p < x < 0
(7.4)
where A and B are constants and can be solved using the boundary condition. Similar to a homojunction, the electric field intensity exists only within the depletion region of a heterostructure, i.e., F= 0 for x ≥ x N and x ≤ −x p . This leads to
7.1 Abrupt Heterojunction Under Equilibrium
F=
245
q N D (x − x N )/ N , 0 < x < xN −q Na x + x p / p , −x p < x < 0
(7.5)
These equations indicate that the electric field intensity is a linear function of position x. F has the following forms on either side of the junction:
F(+) = −q N D x N / N , x = 0+ F(−) = −q Na x p / p , x = 0−
(7.6)
Due to the difference in permittivity ( p = N ), unlike homojunctions, F(+) and F(−) are not equal at the junction. However, the normal displacement vector D = F is continuous at x = 0, which gives N F(+) = p F(−). Since F = −dV/dx, further integration of F gives
2 VN (x) = −(q N D /2 N2)x + (q N D / N )x x N + C, 0 < x < x N V p (x) = q Na /2 p x + q Na / p x x p + D, −x p < x < 0
(7.7)
The constants C and D are determined by setting V p (x) = 0 at x = –x p and V N (x) = V 0 at x = x N . C = V0 − q N D x N2 /2 N and D = q Na x 2p /2 p
(7.8)
The potential distribution across the junction has the following final form: ⎧ ⎪ ⎪ V0 ⎨ V0 − (q N D /2 ∈ N )(x N − x)2 V (x) = ⎪ (q Na /2 ∈ p )(x + x p )2 ⎪ ⎩ 0
xN < x 0 < x < xN −x p < x < 0 x < −x p
(7.9)
Here, V 0 is the total builtin potential and is the sum of potential drop in the pand Nregions, i.e. V 0 = V p + V N . At x = 0, V p (0)= V p . Therefore, V p = V0 − (q N D /2 N )x N2 = q Na /2 p x 2p
(7.10a)
V0 = (q N D /2 N )x N2 + q Na /2 p x 2p = VN + V p
(7.10b)
VN = (q N D /2 N )x N2
(7.10c)
and
However, at x = 0, the potential distribution curve has a kink at the junction to reflect the unequal electric field intensities. By combining (7.10b) into (7.9), the potential distribution across the depletion region on Nside becomes V (x) = q Na x 2p /2 p + (q N D /2 N ) 2x x N − x 2 0 < x < x N
(7.11)
246
7 Electrical Properties of Compound Semiconductor Heterostructures
Fig. 7.2 a Charge carrier, ρ, b electric field intensity, F, and c potential, V, distributions of the pGaAs/NAlGaAs isotype heterojunction
Now, we can plot the charge distribution, electric field intensity, and potential distribution across the pN heterojunction as shown in Fig. 7.2. (b) Depletion width (W) The total depletion width across the pN junction, W, is the sum of x N and x p . W = xN + x p
(7.12)
x N and x p are related through the charge neutrality condition (7.1). By replacing x p or x N in (7.10b) by x N or x p , respectively, the contact potential is related to x N and x p as
7.1 Abrupt Heterojunction Under Equilibrium
247
⎧ ⎪ 2V0 N p Na ⎪ ⎪ ⎪ ⎨ xN = q ND p Na + N N D ⎪ 2V0 N p ND ⎪ ⎪ ⎪ ⎩ xp = q Na p Na + N N D
(7.13)
(c) Bandedge profile Once we know the potential distribution across the pN heterojunction, the bandedge profile can also be derived. Under the equilibrium condition, there is no current flow across the junction. The electron current density is expressed as JN = qμn n F + q Dn
dn =0 dx
(7.14)
where q is the charge, μn is the electron mobility, n is the electron density, and Dn is the electron diffusion coefficient. The diffusion coefficient and mobility are related through Einstein’s relation, Dn = μn (kT/q). Therefore, the electric field intensity becomes F =−
kT (dn/dx) q n
(7.15)
The equilibrium electron density is determined by the Fermi energy, E FN , relative to the conduction band edge, E FN − E c , and is shown below.
E FN − E c and n = Nc exp kT
dn d E FN − E c n dE c =n =− dx dx kT kT dx
(7.16)
We found F(x) =
1 dE c (x) dV (x) =− q dx dx
(7.17)
Therefore, E c (x) =−qV (x). The band edges are parallel to the negative potential distribution. The valence and conduction band edges of the pN heterojunction are plotted in Fig. 7.1 and given by ⎧ −q V0 − E v ⎪ ⎪ ⎪ ⎨ −q V + q 2 N D (x − x)2 − E 0 N v 2∈ N E v (x) = q 2 Na 2 ⎪ − (x + x p ) ⎪ ⎪ ⎩ 2∈ p 0
xN < x 0 < x < xN −x p < x < 0 x < −x p
(7.18)
248
7 Electrical Properties of Compound Semiconductor Heterostructures
E c (x) =
E v (x) + E g1 , x > 0 E v (x) + E g2 , x < 0
(7.19)
7.1.2 Equilibrium nN Heterojunction In an isotype nN heterojunction, the charge redistribution near the junction will also produce a spacecharge region just like in an anisotype heterostructure. Figure 7.3 shows the qualitative equilibrium band diagram of an nGaAs/NAlGaAs heterostructure. Electrons will spill over from the larger bandgap Nregion to the small bandgap nregion as the Fermi levels line up. The charge distribution around the junction (Fig. 7.4) is ρ(x) =
Fig. 7.3 Qualitative equilibrium energy band diagram of an isotype nGaAs/NAlGaAs heterojunction
q ND −q[n(x) − Nd ]
0 < x < xN x a
(7.51)
7.3 QuantumWell Heterostructures
257
Fig. 7.9 Infinitely deep potential well
Thus we can write the 1D timeindependent Schrödinger’s wave equation as −
2 ∂ 2 ψ(z) + V (z)ψ(z) = Eψ(z) 2m ∂z 2
(7.52)
where ψ(z), è, and E are the wave function, Planck constant (è = h/ 2π ), and energy, respectively. For the well width a less than the Bohr radius a B (= 4π 2 /m ∗ q 2 ) of the well material, the potential well is called a quantum well (QW). In the region (0 < z < a) where V = 0, the timeindependent wave equation can be written as ∂ 2ψ + k2ψ = 0 ∂z 2
(7.53)
where k = 2m E/2 The wave function does not exist outside the infinitely deep potential well. The allowed wave functions inside the potential well have the form ψ(z) = A sin kz + B cos kz
(7.54)
where A and B are constants. To determine the constants A and B, we need to use boundary conditions in (7.54). At z = 0, ψ(0) = 0 and B = 0. At z = a, ψ(a) = A sin ka = 0. This condition can be satisfied only when kn a = nπ n = 1, 2, 3, . . . .
(7.55)
k n represents a discrete sequence of values of k, where nπ kn = = a
2m E n 2
(7.56)
Since k is related to the energy E, this condition defines a discrete set of allowed energies
258
7 Electrical Properties of Compound Semiconductor Heterostructures
1 nπ 2 2 kn2 = En = n = 1, 2, 3, . . . 2m 2m a
(7.57)
In contrast to the classical result, the allowed energy states have become discrete levels and their values are proportional to the quantum number n2 . The corresponding wave functions of the system within the potential well, by incorporating k n (7.56), must be of the form nπ z 0 0 when plotted against k. In between λ1 and λ2 , there are only states in the lowest subband. For λ2 < E < λ3 , there are states in the two lowest subbands, n = 1 and 2. For each subband, the 2D electrons contribute to the DOS (cm−2 eV−1 ) in a step function of height (m ∗w π/2 ), starting at λ1 . The total DOS looks like a staircase with jumps at the energies of the subbands.
Fig. 7.11 a Energy levels in an infinite potential well with confinement in z only, b total energy including the transverse kinetic energy for each subband, and c steplike density of states (DOS) of a twodimensional system. The light dashed curve in (c) is the parabolic DOS for unconfined threedimensional electrons
7.3 QuantumWell Heterostructures
261
7.3.2 Realistic QW with Finite Depth Barriers In a realistic QW shown in Fig. 7.12 with a well width L and a finite barrier height V 0 , separate wave equations may be used to describe the wave functions and energy eigenvalues in the well and barrier regions. In the well region, z < L/2, the Schrödinger equation is given by d 2 ψ0 + α 2 ψ0 = 0 dz 2
(7.70a)
and α=
2m ∗w E 2
(7.70b)
The solutions of the wave function in the QW are ψ0 =
A cos(αz) (even function) A sin(αz) (odd function)
(7.71)
In the barrier regions, the wave functions are ψ + and ψ – in the regions of z > L/2 and z < −L/2, respectively. The associated Schrödinger wave equation in the barrier is d2 ψ± − β 2 ψ± = 0 dz 2
(7.72a)
and β=
Fig. 7.12 Finite quantum well of depth V 0 and width L
2m ∗b (V0 − E) 2
(7.72b)
262
7 Electrical Properties of Compound Semiconductor Heterostructures
where m ∗b is the effective mass of the barrier material. The solutions of the wave function in the barrier region have the form ψ± =
B exp[−β(z − L/2)] B exp[β(z + L/2)]
z > L/2 z < −L/2
(7.73)
To solve the constants A and B, we have to apply the connection conditions at the wellbarrier interface, z = L/2. ψ0 = ψ± and
1 dψ± 1 dψ0 = ∗ m ∗w dz m b dz
(7.74)
The second boundary condition for the derivative of wave functions has been modified to include the current flow continuity at the heterointerface. (a) Even function For even functions, at z = L/2, the boundary conditions lead to A cos(αL/2) = B and −α
B B A sin(αL/2) = −β ∗ exp[−β(z − L/2)]z=L/2 = −β ∗ ∗ mw mb mb
Eliminating A and B, we reach the following solution: α β tan(αL/2) = ∗ m ∗w mb
(7.75a)
or
β=
m ∗b α tan(αL/2) (even function) m ∗w
(7.75b)
(b) Odd function For odd functions, we use the same method to find solutions. At z = L/2, the solutions are given by
∗ mb β=− αcot(αL/2) (odd function) m ∗w
(7.76)
The above two equations have no analytical solutions. Therefore, the graphic or numerical method will be used. First, we multiply (L/2) to the above two equations.
7.3 QuantumWell Heterostructures
⎧
L L m ∗b ⎪ ⎪ β tan α L2 = α (even) ⎨ 2 2 ∗ mw
m ∗b ⎪ ⎪ cot α L2 (odd) ⎩ β L2 = − α L2 ∗ mw
263
(7.77)
Replacing β for β m ∗w /m ∗b , the above equations become ⎧ ⎪ L m ∗b L L ⎪ ⎪ β = α tan α 2 (even) ⎪ ⎨ 2 m∗ 2 w ∗ ⎪ ⎪ ⎪ β L = − m b α L cot α L (odd) ⎪ ⎩ 2 2 ∗ mw 2
(7.78)
These equations are the functions of (β L/2) and (αL/2). Also α 2 + β 2 =
2m ∗w E m ∗w 2m ∗b (V0 − E) 2m ∗w V0 + = 2 m ∗b 2 2
(7.79a)
or
L 2 L 2 2m ∗w V0 L 2 α + β = ≡ R2 2 2 2 2
(7.79b)
This is an equation of a circle defined by (β L/2) and (αL/2). The above equation can be solved either graphically or numerically. Since the well width, well effective mass, and barrier height are known values, R can be determined. Replacing (β L/2) by R and (αL/2) in (7.78), the wave functions can be solved numerically through the following equations of (αL/2). Thus, the values of α are determined and can be used for energy states calculation. ⎧ ⎪ L 2 m ∗b L L ⎪ 2− α ⎪ α tan α 2 R = (even) ⎪ ⎨ 2 m ∗w 2 ⎪ L 2 m ∗b L L ⎪ ⎪ 2 ⎪ ⎩ R − α 2 = − m ∗ α 2 cot α 2 (odd) w
(7.80)
In the graphic approach, the intersections of the circle of radius R and the tangent and cotangent functions determine the solution of the allowed wave function in the QW as shown in Fig. 7.13. From the allowed α’s, we can obtain the energy eigenvalues according to (7.70b).
264
7 Electrical Properties of Compound Semiconductor Heterostructures
Fig. 7.13 Solutions of the finite depth 1D potential well using graphical method. The solid and dotted curves represent the even and odd transcendental equations, respectively, where γ = γ m ∗b /m ∗w . The intersections of R and the transcendental equations are the solutions, α 1 L/2, α 2 L/2, and α 3 L/2
7.3.3 Hole Energy Levels in the QW The valence band structure of bulk semiconductors is degenerated near the zone center. The dispersion of the heavy and lighthole bands is very roughly described by E(k) = E v −
2 k 2 2m ∗h
(7.81)
where m ∗h equals the effective mass m ∗hh and m ∗lh for heavy and light holes, respectively. The parabolic and isotropic nature of this simple model does not hold for real semiconductors. The shape of the constant energy surface depends on the direction of k and has the shape of the warped sphere. The complicated situation gets worse if the cubic symmetry of the crystal is broken. In general, despite its shortcomings, we will still use the simple parabolic model for the Ek relation since a precise description is cumbersome. In a quantum well, the potential step along the zdirection further destroys the isotropic nature of the crystal and modifies the band shape as illustrated in Fig. 7.14. Two important features are observed: First, the heavy and light holes are no longer degenerated at k = 0. The wave functions of heavy and light holes have the symmetry of p orbitals (Sect. 3.6). The orientations of p orbitals for heavy holes are oriented Fig. 7.14 Energy band model of holes in a quantum well. The ‘heavy’ and ‘light’ hole bands cross each other, leading to ‘anticrossing’ behavior shown by the dark lines
7.3 QuantumWell Heterostructures
265
Table 7.1 Luttinger parameters of III–V binary compounds [1] III–V
GaAs
AlAs
InAs
GaP
AlP
InP
GaSb
AlSb
InSb
γ1
6.98
3.76
20.0
4.05
3.35
5.08
13.4
5.18
34.8
γ2
2.06
0.82
8.5
0.49
0.71
1.60
4.7
1.19
15.5
γ3
2.93
1.42
9.2
2.93
1.23
2.10
6.0
1.97
16.5
normal to z, while the p orbital orientations for light holes are oriented along z. The heavy mass along z for heavy holes means that the bound state is deep in the QW and thus decoupled from the lighthole energy state. Second, the ‘heavy’ and ‘light’ characters are strongly mixed. For heavy holes, the orientations of p orbitals are in the xyplane and have a lighter inplane mass. This means that the kinetic energy rises rapidly as a function of k in the plane of the QW. On the other hand, the orientation of p orbitals for light holes is perpendicular to that of heavy holes. The lighthole mass is lighter along z and heavy in the xyplane. This means a low binding energy (high kinetic energy) in the QW. The heavy holes are actually lighter, and the light holes become heavier for transverse motion. Therefore, the lighthole and heavyhole bands cross over at some k. The heavyhole and lighthole effective masses along the [100] (zdirection) in a QW are modified in terms of Luttinger parameters (γ i ) as m ∗hh = m 0 /(γ1 − 2γ2 ), m ∗lh = m 0 /(γ1 + 2γ2 )
(7.82)
The Luttinger parameters for IIIV alloys are listed in Table 7.1.
7.3.4 Strained Quantum Wells For a strained quantumwell structure, we can assume that the band edges of the barrier material are unaltered. However, the allowed energy states of the well are modified to include straininduced band discontinuity changes in the well material. The bandedge energy diagrams of strained QWs are compared with an unstrained QW in Fig. 7.15. The bandedge energy of the QW under strain can be calculated using the procedure outlined in Sect. 6.3. Once the bandedge positions of the QW material are determined, the allowed energy states can be calculated using equations from the previous section to include the effective masses of the well and barriers.
266
7 Electrical Properties of Compound Semiconductor Heterostructures
Fig. 7.15 Energy band diagrams for QWs under various stress conditions. The dashed lines of strained structures indicate the location of unstrained band edges. The composition of barriers is the same in all three cases while the composition of the QW is changed to generate strain
7.3.5 Infinite Deep Triangular Quantum Well The triangular potential well is the most common potential well formed in a semiconductor quantum well under an applied bias and at the semiconductor heterointerface. When a constant electric field intensity F is applied to a quantum well, as shown in Fig. 7.16a, the bottom of the potential well tilts up forming a triangular well. To simplify the discussion, let us consider a potential well wide enough so that only the vertical potential barrier at z = 0 and the tilted barrier are considered (Fig. 7.16b). The potential energy distribution of such a structure can be described as V (z) =
q F z = V0 z ∞
(a)
∞
∞
z>0 z≤0
(7.83)
(b)
V(z)
E2 E1
E1 V=0
+
F
–
V=0
z
Fig. 7.16 a Infinitely deep quantum well under an applied electric field, F. b A triangular potential well V (z) = qFz. The dashed lines are the allowed energy states
7.3 QuantumWell Heterostructures
267
where q is the electron charge and V 0 = qF, which is a constant for a specific F. The potential energy increases with z in the tilted region. The wave equation for such a system in the triangular well is −
2 ∂ 2 ψ + q F zψ = Eψ (z > 0) 2m ∂z 2
(7.84)
(a) Airy function Equation (7.84) can be solved rigorously in closed form through the following procedures. The first step to solve this equation is to get rid of the physical quantities E and z and replace them with pure numbers. The physical problem of (7.84) is thereby reduced to a pure mathematical problem. We do this by defining a ‘length unit’ L, which can be done by rearranging the equation into the form −
2 ∂ 2 ψ + (z − b)ψ = 0 2mq F ∂z 2
(7.85)
where b ≡ (E/qF) has a unit of length. The second term has a dimension of (length)+1 , and the first term has the unit of (length)–2 from 1/z2 , so the factor in front of it must have dimensions of (length)+3 . This suggests that we should define the length unit L to eliminate this constant by setting z¯ ≡
2 z−b 3 ,L ≡ L 2mq F
(7.86)
Similarly, we can define an ‘energy unit’ E 0 following (7.83) as E0 = q F L =
(q F)2 2m
1/3 (7.87)
Replacing these in (7.85), the wave equation becomes −L 3
d2 ψ + L z¯ ψ = 0 and dz = Ld z¯ dz 2
(7.88)
It further reduces to a simple form d2 ψ − z¯ ψ = 0 d¯z 2
(7.89)
The solutions of this equation are a linear superposition of modified Bessel functions of the order ±1/3, or Airy functions. These functions have the following asymptotic properties for large z¯
268
7 Electrical Properties of Compound Semiconductor Heterostructures
Fig. 7.17 The Airy function Ai (¯z )
Ai (¯z ) ∼ z¯ −1/4 exp−2¯z 2/3 /3 Bi (¯z ) ∼ z¯ −1/4 exp +2¯z 2/3 /3
(7.90)
Clearly we must reject the Bi solutions as they expand rapidly at z¯ → +∞. Thus ψ(¯z ) ∝ Ai (¯z ) = Ai [(z − b)/L]
(7.91)
The Ai solutions are plotted in Fig. 7.17. Ai (¯z ) decays exponentially in positive (inside the sloped barrier), and there is an infinite number of negative values of where Ai (¯z ) = 0 denoted by an . These values of an are the nth roots of the Airy function. The boundary condition ψ = 0 at z = 0 then requires z¯ = an =
En b = L qFL
(7.92)
for negative z¯ and E 0 = qFL. This leads to the energy eigenvalues of E n = an E 0 = an
(q F)2 2m
1/3 n = 1, 2, 3, . . . .
(7.93)
Once again, numerical techniques must be used to obtain an with an ≈
2/3 3π (4n − 1) 8
(7.94)
So that
E n = an E 0 ≈
2 2m
1/3
2/3 3πq F n = 1, 2, 3, . . . (4n − 1) 8
(7.95)
7.3 QuantumWell Heterostructures
269
The allowed energy levels and the corresponding wave functions of a triangular well are shown in Fig. 7.18. Since the well broadens as the energy is raised, the energy levels get closer together as n increases. The wave functions vanish at z = 0 where the potential barrier is infinitely high. Due to the finite barrier height at z > 0, wave functions penetrate into the barrier and decay exponentially. (b) FangHoward wave function In most discussions involving triangular quantum wells in semiconductors, we are most interested in the energy and waveform of the ground state (n = 1). The ground state of the triangular well can be conveniently obtained by a calculation using the following trial function proposed by Fang and Howard [2]: ψ(z) = Az exp(−αz)
(7.96)
where α is the trial parameter and A is a normalization parameter. This wave function reflects the feature of the waveform derived through rigorous mathematical calculations discussed earlier. The wave function vanishes at z = 0, i.e., at the vertical interface, and decays exponentially in the slope barrier. To evaluate these two parameters, the normalization procedure is applied where ∞
∗
∞
ψ ψdz = A 0
z 2 exp(−2αz)dz = 1
2
(7.97)
0
(7.97) can be solved ∞Equation n n+1 z exp(−az)dz = (n + 1)/a . Thus, 0
using
the
A = 2α 3/2
result
of
(7.98)
The normalized wave function of the ground state in a triangular potential well becomes ψ(z) = 2α 3/2 z exp(−αz) Fig. 7.18 Energy levels and wave functions in an infinitely deep triangular potential well V (z) = qFz
(7.99)
E4 E3 E2 E1 V(z)
270
7 Electrical Properties of Compound Semiconductor Heterostructures
which is the Fang–Howard wave function. Then the energy of the ground state E 1 can be obtained through the calculation of the energy expectation value of the wave function. ∞ E =
∗
∞
ψ H ψdz = 0
0
2 ∂ 2 ψ − + q F z ψdz 2m ∂z 2 ∗
∞ 2 3/2 −αz 2 α ze ∂ 3/2 −αz 3 3 −2αz = − dz 2α ze + 4q F z α e m ∂z 2
(7.100)
0
E = E 1 =
3q F (α)2 + 2m 2α
(7.101)
The energy expectation value is a function of the triangular well potential qF and α. For a fixed qF, the trial parameter α and the energy of the ground state, corresponding to an energy minimum of the potential well, can be derived by taking ∂E/∂α = 0. ∂E α2 3q F = − =0 ∂α m 2α 2
(7.102)
Thus,
α=
3q Fm 22
1/3 (7.103)
Using this calculated trial parameter the energy of the ground state is obtained as
3 3q F 2/3 9q F = E1 = √ 4α 2 2 m
(7.104)
The ground state energy obtained using this result is approximately equal to that calculated from the Airy function approach within an error of ~6%.
7.4 Superlattices and Minibands 7.4.1 Square Barrier A onedimensional potential barrier is located with V (z) = V 0 for 0 ≤ z ≤ a and V (z) = 0 elsewhere. In region I, a wave with energy E is incident from the left onto the barrier as shown in Fig. 7.19. We are interested in the fraction of the incident
7.4 Superlattices and Minibands Fig. 7.19 Energy diagram of a square potential barrier with a barrier width a and height V 0
271
V = V0 I
II
III
E 0
a
z
wave that tunnels through the barrier (region II) into region III and the fraction of the incident wave that gets reflected. The general solutions of the Schrödinger equation in these three regions are ⎧ ⎨ ψ1 (z) = A exp(ik1 z) + B exp(−ik1 z) (Region I) ψ (z) = C exp(ik2 z) + D exp(−ik2 z) (Region II) ⎩ 2 ψ3 (z) = F exp(ik1 z) + G exp(−ik1 z) (Region III) 2m E 2m(E − V0 ) k1 = , k2 = 2 2
(7.105)
A, C, and F are amplitudes of forward propagating waves, and B, D, and G are amplitudes of reflection waves. Since there is no reflection wave in region III, G = 0. Using the fact that the wave function and its derivative are continuous at boundaries, we arrive the following conditions: At x = 0: A + B = C + D and k1 (A − B) = k2 (C − D)
(7.106a)
C exp(ik2 a) + D exp(−ik2 a) = F exp(ik1 a)
(7.106b)
At x = a:
k2 C exp(ik2 a) − D exp(−ik2 a) = k1 F exp(ik1 a)
(7.106c)
Solving the above equations by eliminating C and D, we obtain the amplitude ratios of reflection and transmission waves as 2 k1 − k22 1 − exp(i2k2 a) B (7.107a) = A (k1 + k2 )2 − (k1 − k2 )2 exp(i2k2 a) F 4k1 k2 exp[i(k2 − k1 )a] = A (k1 + k2 )2 − (k1 − k2 )2 exp(i2k2 a)
(7.107b)
272
7 Electrical Properties of Compound Semiconductor Heterostructures
These lead to the probabilities of transmission (T ) and reflection (R) of the system: 2 F 4E(E − V0 ) T = = A 4E(E − V0 ) + V02 sin2 k2 a 2 B V02 sin2 k2 a R = = A 4E(E − V0 ) + V02 sin2 k2 a
(7.108a)
(7.108b)
For E > V 0 , the transmitted flux is not a constant as expected from the classical theory. It becomes unity only when sin k 2 a = 0, i.e., k 2 a = nπ and n = 1, 2, 3 …, and has multiple peaks. For E < V 0 , k 2 becomes imaginary. Let κ = ik 2 and sin k 2 a = i sinh κa. The transmission and reflection coefficients become T =
4E(E − V0 ) 4E(E − V0 ) + V02 sinh2 κa
(7.109a)
R=
V02 sinh2 κa 4E(E − V0 ) + V02 sinh2 κa
(7.109b)
Again, in contrast to the classical theory, the tunneling probability does not reduce to zero when E becomes less than V 0 .
7.4.2 Resonant Tunneling Through Double Barriers In a single QW, the energy eigenvalues are determined precisely by the well width and barrier height. The allowed state in a QW is called a bound state. When the thickness of the two barriers on each side of the QW is reduced as depicted in Fig. 7.20, the confined electron can tunnel out of the QW. In a single square barrier case shown above (Fig. 7.19), the tunneling probability of a wave with an energy of E < V 0 is very small. However, when the wave is confined between two identically thin barriers instead, new physics appears. Since the electron can leak out of the well, the electron is not confined in bound states. Rather, the electron resides in a resonant state. The Fig. 7.20 Schematic of a doublebarrier system where the two barriers have the same thickness
a TL
TR
7.4 Superlattices and Minibands
273
rL tL
e ika
rR
e ika
t L e ika t R t L e ika r R e ika r L e ika t R
tL
....
....
....
....
tL , r L
tR , r R
Fig. 7.21 Transmission and reflection amplitudes in a Fabry–Perot cavity. t R and t L , and r R and r L are the transmission and reflection amplitudes for the right and left mirrors, respectively
energy of this state cannot be precisely determined but is spread into a range /τ , where τ is the lifetime of an electron in the well before it tunnels away. In general, the transmission probability T of two barriers is approximately equal to the product of the values for the two individual barriers, T L T R . In a symmetric structure, where the two barriers are identical, the transmission probability at the resonant state rises dramatically above the product T L T R and reaches its maximum value of unity. This process is called the resonant tunneling. The electron oscillation in and transmission through the barriers of a symmetric doublebarrier system can be treated as an analogous optical Fabry–Perot cavity (Fig. 7.21). An incident plane wave is bouncing back and forth between the two partially transparent mirrors. At each bounce, the wave loses some of its amplitude by transmission through the mirror. Use t R and t L , and r R and r L , as the transmission and reflection amplitudes for the right and left mirrors, respectively. The total wave transmitted through the mirror on the right is the sum of individual transmitted waves at each bounce. t = t L exp(ika)t R + t L exp(ika)r R exp(ika)r L exp(ika)t R + t L exp(ika)r R exp(ika)r L exp(ika)r R exp(ika)r L exp(ika)t R
+ . . . = t L exp(ika)t R 1 + r R r L exp(i2ka) + r R2 r L2 exp(i4ka) + . . . (7.110) This is a geometric series of x = r R r L exp (i2ka), and x < 1. The sum of such a series is 1 + x + x 2 + x 3 + x 4 + . . . = 1/(1 − x) The total transmission amplitude to the right, including the phase factor exp(ika), is given by t=
tL t R exp(ika) 1 − r L r R exp(i2ka)
(7.111)
274
7 Electrical Properties of Compound Semiconductor Heterostructures
If we take the complex reflection amplitudes r L and r R in polar forms such that r L = r L  exp(iφ L ) and r R = r R  exp(iφ R ), the flux transmission coefficient T = t2 becomes T =
1−
√
RL R R
2
TL T R √ + 4 R L R R sin2 (φ/2)
(7.112)
where φ = φ L + φ R + 2ka is the total phase angle and Ri = 1 −√Ti . T peaks √ at sin(φ/2) = 0 or φ = 2nπ . For T L 1 and T R 1, and expanding R L and R R with binomial series, the approximate peak transmission coefficient T pk is given by TL T R 4TL TR T pk = 2 ≈ √ 2 (T L + TR ) 1 − RL R R
(7.113)
T pk equals one when T L = T R despite that the individual transmission coefficient for each barrier is very small.
7.4.3 Superlattice and Miniband When stacking thin layers of latticematched GaAs and AlGaAs alternatively, with fixed thickness and composition, a series of identical QW/barrier structures is formed. The periodic bandedge energy variation of the structure creates an artificial 1D lattice constant in the growth direction in addition to the natural 3D lattice of GaAs and AlGaAs. This structure is called a superlattice. An electron can tunnel from one well to its neighbors in a superlattice similar to that of the doublebarrier structure. Therefore, resonant states with finite energy distribution are replacing the sharp bound states associated with the well. The spreading of the allowed state in a superlattice can also be understood from the general theory of a 1D crystal. Since the period of the superlattice is much larger and the periodic potential is weaker than the crystal lattice, the resultant energy bands and gaps are much smaller. Therefore, the allowed energy bands are called minibands. Since a superlattice is a 1D structure, the Kronig–Penney model is perfect for the understanding of the relationships between the allowed energy, layer thickness, and layer composition in superlattices. The model used to treat the 1D periodic crystal lattice can be directly applied to a superlattice with some modifications. As shown in Fig. 7.22, the conduction band discontinuity E c between the well and the barrier materials becomes the potential barrier height V 0 . The free electron mass used in the original model is now replaced by the effective masses m ∗w and m ∗b in the well and barrier, respectively. Furthermore, the connection rule for the derivative of the wave functions is modified to include the effect of mass change when electrons move from one material into the other; i.e.,
7.4 Superlattices and Minibands
275
Fig. 7.22 Schematic of the conduction band edge in a superlattice heterostructure with well width a and barrier thickness b
1 dψw 1 dψb = ∗ ∗ m w dz m b dz
(7.114)
The final solution for the E < E c case is readily obtained as 1 (η − 1/η) sin(αa) sinh(γ b) + cos(αa) cosh(γ b) = cos λ(a + b) 2 2m ∗b (E c − E) 2m ∗w E γ m ∗w ; α = ; γ = ;d=a+b where η = αm ∗b 2 2
(7.115)
and λ (–π /d < λ < π /d) is the wave number in the superlattice. The interpretation of this result is similar to the model developed in Chap. 3 with modified masses. The allowed energy states are bunched into discrete minibands separated by energy gaps.
7.4.4 Density of States in Superlattice The dispersion of N states in each miniband of an Nperiod superlattice destroys the abruptness of the twodimensional DOS in each well. The DOS of a superlattice can be estimated by considering it as the combination of the onedimensional confinement of a quantum well along the growth direction and a new periodic lattice along the same direction. Set the density of states of the 1D as D1D . The density superlattice of states of the QW has the form D2D = m ∗ / π 2 . Then the threedimensional density of states is given by the integral
D3D
1 = 2
∞
D1D E D2D −∞
m∗ E dE = 2π 2
∞
D1D E d E
(7.116)
−∞
The factor of 1/2 avoids double counting the spin. The value of D1D in a 1D freeelectron system was derived in Chap. 3 and has the form D1D =
1 π
2m ∗ E
(7.117)
276
7 Electrical Properties of Compound Semiconductor Heterostructures
To incorporate the bandedge information of the 1D system, it is replaced by D1D =
2 π ν(E )
(7.118)
2 ∗ 2 where v(E ) is the∗ velocity. Here we used p = k and k = 2m E / to get 2 ν E = 2E /m . For a onedimensional periodic lattice with a periodicity c, the allowed energy band in kspace is approximated by a cosine function with a bandwidth .
E (k) = (/2)(1 − cos kc)
(7.119)
1 dE c = sin kc. ν E = dk 2
(7.120)
and
The sine function is reduced through the cosine function. cos kc = 1 −
E (/2) − E = , /2 /2
(7.121a)
and sinkc =
(/2)2 − [(/2) − E ]2 /(/2).
(7.121b)
Therefore, ν E = (c/) (/2)2 − [(/2) − E ]2
(7.122a)
D1D E = (2/cπ )/ (/2)2 − [(/2) − E ]2 .
(7.122b)
and
The integration of the density of states for a superlattice becomes m∗ D3D = 2π 2
E
dE 2
(/2)2 − (/2) − E −∞ E m∗ m∗ −1 E − (/2) −1 E − (/2) − sin−1 (−∞) sin = sin = (/2) (/2) cπ 2 2 cπ 2 2 −∞ 2 cπ
(7.123)
7.4 Superlattices and Minibands
277
Fig. 7.23 Normalized density of states as a function of energy for a superlattice and a multiple quantum well (thin line) scaled to the same value in the plateau. The two lowest bands have widths 1 and 2
For sin−1 (−∞) = −π /2, the density of states of a superlattice is shown in Fig. 7.23 and given by D3D =
m∗ 1 1 −1 E − (/2) + sin 0≤E ≤ cπ 2 2 π (/2)
(7.124)
The density of states of a superlattice consists of two terms: a stepwise function due to 1D confinement in QWs and an arcsine function originated from the 1D superlattice. When the barriers are thick, the superlattice can be seen as a multiple QW structure. It maintains a steplike density of states. The communication of electrons between wells increases with decreasing barrier thickness and broadens the sharp step of the density of states into an arcsine of width .
7.5 Heterostructures in Electric Fields 7.5.1 Uniform Electric Field on a Bulk Semiconductor—Franz–Keldysh Effect When a semiconductor is placed in an electric field, the absorption coefficient changes with the applied field. The phenomenon observed independently by W. Franz and by L.V. Keldysh is known as the Franz–Keldysh effect [3, 4]. The physical origin of this change can be understood by solving the Schrödinger wave equation of the bulk semiconductor in a uniform electric field. Consider an electron with charge q moving in a uniform electric field F along the zdirection. As shown in Fig. 7.24, the potential energy of the system is V (z) = qFz, which increases with z for F > 0. The onedimensional Schrödinger wave equation has the following form:
278
7 Electrical Properties of Compound Semiconductor Heterostructures
Fig. 7.24 Two wave functions for electrons of different energies in a semiconductor under a uniform electric field F
2 ∂ 2 − + q F z ψ(z) = Eψ(z) 2m ∂z 2
(7.125)
This is the same wave equation in a triangular potential well as has been discussed in Sect. 7.3. The unnormalized solutions of wave functions are
z − (E/q F) q Fz − E (7.126) = Ai ψ(z) = Ai L E0 1/3 1/3 2 (q F)2 where L = and E 0 = = q F L. 2mq F 2m Unlike in triangular quantum wells, there is no confinement for electrons, and they can travel all space. Therefore, we can take any energy value in the wave function solution. The wave functions oscillate for z < E/qF. The undulation becomes more rapid as z¯ = (z − E/q F)/L gets more negative. For z > E/qF, the wave tunnels into the potential and decay gradually. Although there is no obvious confinement in the system, the nature of these waves is standing rather than propagating. This is due to the interference between the incoming and the reflection waves, generated by collision with the potential at z = E/qF. The Franz–Keldysh effect of the electric field dependence of the fundamental absorption edge can be thought of as photonassisted tunneling through the energy gap. In a semiconductor, an optical absorption occurs only if the incident wave with the associated energy, ω, is larger than the bandgap energy. For ω < E g , absorption in a semiconductor is impossible because there is no state available within the forbidden gap. In an electric field, due to the tilted energy band, there are states in both conduction and valence bands at all energies. The electron wave functions in the conduction and valence bands have exponentially decaying amplitude in the energy gap. When there is no photon absorption, a valence band electron must tunnel through
7.5 Heterostructures in Electric Fields
279
Fig. 7.25 Frenz–Keldysh effect on interband absorption. The energy band diagram showing the wavefunction overlap with absorption of a photon of an energy ω < E g
a large triangular barrier with a barrier height E g and a barrier thickness E g /qF to reach the conduction band. However, with the absorption of a photon with energy barrier ω < E g , as shown in Fig. 7.25, the tunneling height is reduced to (E g − ω) and the barrier thickness becomes t = E g − ω /q F. It is clear that the tunneling probability is considerably enhanced with photon absorption and depends on the electric field intensity as well as the photon energy.
7.5.2 Quantum Well in an Electric Field—QuantumConfined Stark Effect (QCSE) The absorption property of quantum wells is also modified by the applied uniform electric field F and is closely related to the Franz–Keldysh effect in bulk semiconductors. It is called the quantumconfined Stark effect (QCSE). The Stark effect generally refers to a shift in the atomic energy upon the application of an electric field. It is well known in atomic physics that, in an electric field F, the 2s and 2p energy states in a hydrogen atom split into E 2 + 3qaF, E 2 , and E 2 –3qaF levels, where E 2 = − 13.6/n2 (n = 2) and a is the Bohr radius. The splitting of the energy level proportions to the first power of the field strength is called the linear Stark effect. Under the electric field, as shown in Fig. 7.26, the electron and hole wave functions in the well are pulled toward the opposite side of the quantum well. The reduced overlap of the two wave functions results in a corresponding reduction in absorption and in luminescence. The electron and hole distributions peak at different portions of the quantum well with an average separation x. The spatial distribution of electrons and holes creates an electric dipole moment p = −qx = 0 α F
(7.127)
where α is the polarizability. This induced dipole moment lowers the state energy by an amount E = − p · F/2 = 0 α F 2 /2. Therefore, the energy separation between the state of the conduction band and the state of the valence band in a quantum well is reduced by the electric field. In addition, the probability of tunneling for low barrier
280
7 Electrical Properties of Compound Semiconductor Heterostructures
(a) F = 0
(b) F ≠ 0
Ec(z)
EQW
>
EQCSE
Ev(z) Fig. 7.26 a Absorption energy E QW between the bound states in a quantum well with flat bands. b Under an applied electric field (F = 0), the tilted bands lower the energy of both bound states and reduce the absorption energy to E QCSE
holes increases rapidly with increasing field F. Finally, the QCSE merges with the Franz–Keldysh effect as the quantumwell width is increased.
7.6 Polarization Fields in Wurtzite Heterostructures As shown in Fig. 7.27, the wurtzite structure GaN has a bilayer structure when viewed along the caxis. The (0001) planes are alternating cation layers and anion layers with Fig. 7.27 Schematic diagram of the crystal structure of a wurtzite Gaface GaN. Reprint with permission from [5], copyright AIP Publishing
7.6 Polarization Fields in Wurtzite Heterostructures
281
the Gaplane and Nplane terminating (0001) and 0001¯ surfaces, respectively. The corresponding (0001) and 0001¯ faces are the Aface and Bface, respectively. The ionic bonds linking neighboring (0001) planes with charges generate a
opposing spontaneous polarization (PSP ) in the direction of 0001¯ . Thus, the spontaneous polarization in Aface and Bface samples will have opposite signs. In addition, we also notice a large latticemismatch between GaN and AlN (a/a = 2.4%, c/c = 3.9%). When coupled with the large piezoelectric constants (~1 versus 0.01 in other IIIV’s), a strong straininduced polarization or piezoelectric polarization (PPE ) forms in IIIN heterostructures. The direction of the polarization follows dilation or contraction of the caxis. The existence of significant spontaneous and piezoelectric polarizations in IIIN heterostructures results in extra charge distribution at the heterojunction and modified energy band profile, which lead to unique electronic and photonic properties. In the absence of external electric fields, the total polarization of a IIInitride heterostructure is the sum of the equilibrium lattice PSP and the straininduced PPE . In this discussion, we consider polarizations along the 0001 axis, since this is the direction along whichepitaxial layers and heterostructures are usually grown. Since (0001) and 0001¯ surfaces of GaN are nonequivalent, the spontaneous polarization for GaN and AlN depends on whether the surface is Ga/Alface or Nface. For IIIN alloys grown on cplane sapphire substrates, the MOCVD and MBE growth methods produce Ga/Alface (Aface) and Nface (Bface) layers, respectively. If we consider the [0001] axis (zaxis) as the epilayer growth direction, the spontaneous polarization for both GaN and AlN is found to be negative. This is because the spontaneous polarization of wurtzite structure GaN crystal is pointing ¯ direction, as shown in Fig. 7.27. The spontaneous polarization of ternary in [0001] IIInitride alloys is given as a function of composition in the following [6]: PSP (Alx Ga1−x N/GaN) = −0.090x − 0.034(1 − x) + 0.021x(1 − x) C/m 2 PSP (Inx Ga1−x N/GaN) = −0.042x − 0.034(1 − x) + 0.037x(1 − x) C/m 2 PSP (Alx In1−x N/GaN) = −0.090x − 0.042(1 − x) + 0.070x(1 − x) C/m 2 (7.128) The net values of the spontaneous polarization for all ternary IIInitride alloys are negative relative to [0001] growth direction. Again, if only the stress along the [0001] growth direction is considered, the straininduced piezoelectric polarization PiPE and the strain components i are related as ⎤⎡ ⎤ ⎡ PE ⎤ ⎡ 0 0 0 1 P1 ⎣ P PE ⎦ = ⎣ 0 0 0 ⎦⎣ 2 ⎦ (7.129) 2 PE P3 3 e31 e31 e33 where e3i are the piezoelectric coefficients. The strain components are
282
7 Electrical Properties of Compound Semiconductor Heterostructures
1 = 2 =
as − ae 2C13 3 = − 1 ae C33
where as and ae are the lattice constants of the substrate and the epitaxial layer, respectively. Thus, the induced piezoelectric field polarization becomes P1PE = P2PE = 0
C13 P3PE = PPE = e31 (1 + 2 ) + e33 3 = 2 e31 − e33 1 C33
(7.130a) (7.130b)
Here we replaced PiPE by PPE for simplicity. Since e31 is negative and e33 , C 13 , and C 33 are positive, the value in the parenthesis of (7.130b) is always negative for all compositions of ternary IIInitrides. The piezoelectric polarization PPE is negative ¯ direction) for tensile strain and positive for compressive strain. (along the [0001] Using the linear extrapolation of the elastic and piezoelectric constants listed in Table 6.3, the nonlinear dependence of the piezoelectric polarization on the alloy composition for IIInitride ternary alloys grown on GaN substrate can be derived as follows [6]: PPE (Alx Ga1−x N/GaN) = −0.0525x + 0.0282x(1 − x) C/m 2 PPE (Inx Ga1−x N/GaN) = 0.148x − 0.0424x(1 − x) C/m 2 PPE (Alx In1−x N/GaN) = −0.0525x + 0.148(1 − x) + 0.0938x(1 − x) C/m 2 (7.131) The piezoelectric polarizations induced in tensilestrained Alx Ga1−x N/GaN and compressively strained Inx Ga1−x N/GaN heterostructures have negative and positive values, respectively, over the whole composition range. However, for the Alx In1−x N/GaN heterostructure, the piezoelectric polarization becomes zero at x ≈ 0.81, where the heterostructure becomes lattice matched. The total polarization P of the wurtzite structure IIInitrides is the sum of the spontaneous and piezoelectric polarization, P = PSP + PPE
(7.132)
Due to the net polarization field in dielectric materials, e.g., GaN and Alx Ga1−x N, a polarizationinduced sheet charge density may exist at the heterostructure interface. For example, at the surface of an Ax B1x N layer as well as at the interface of the Ax B1−x N/GaN heterostructure, where A and B are group III elements, the total polarization changes abruptly, causing a fixed twodimensional polarization sheet charge density σ (C/cm2 ) given by σABN = PABN = PSP (ABN) + PPE (ABN) for surfaces
(7.133)
7.6 Polarization Fields in Wurtzite Heterostructures
283
σABN/GaN = P(bottom) − P(top) = PGaN − PABN = PSP (GaN) − [PSP (ABN) + PPE (ABN)] for interfaces
(7.134)
respectively. Here, the relaxed GaN and tensilestrained Ax B1−x N are used in the heterostructure. The charges at the top of the Ax B1−x N layer are usually compensated for by charged surface states. If there is no additional surface charge, the induced electric field F in Ax B1−x N can be determined from the boundary condition at the surface: D = F + PABN = 0
(7.135)
F = −PABN /
(7.136)
The induced electric field in Ax B1−x N causes the energy band edges to tilt with a constant slope even under equilibrium conditions. The equilibrium energy band diagram and charge density in an Alx Ga1−x N/GaN single heterostructure are shown in Fig. 7.28. The fixed interface sheet charge +σ AlGaN/GaN = + σ pE can attract free electrons to the triangular QW and forms a sheet charge of twodimensional electron gas (2DEG), −σ 2DEG . More discussions of 2DEG at the heterostructure interface will be given in Chap. 9. Next, we turn our attention to a multiple heterojunction structure, such as multiple quantum wells (MQW). The continuity of the displacement flux D normal to the surface in the barrier and well, in the absence of free surface carriers, gives D = w Fw + Pw = b Fb + Pb Fig. 7.28 Band diagram of a strained AlGaN/GaN single heterostructure grown on Aface GaN. The sheet charge density distribution (σ ) in the structure is also shown
(7.137)
284
7 Electrical Properties of Compound Semiconductor Heterostructures
Fig. 7.29 Layer structure of an InGaN/GaN multiple quantumwell heterostructure grown on Aface GaN and the QW energy band profile. Only one QW structure is displayed
where the subscripts w and b represent the parameter in the well and barrier layers, respectively. For a MQW structure, the net voltage drop over one period of barrier (L b ) and well (L w ) is zero. Fw L w + Fb L b = 0
(7.138)
The electric fields in the well and barrier regions are solved using (7.137) and (7.138). Fw =
Lb (Pb − Pw ) b L w + w L b
(7.139a)
Fb =
−L w (Pb − Pw ) b L w + w L b
(7.139b)
We notice that the fields in the well and barrier are opposite in direction. Figure 7.29 shows the layer structure of an Inx Ga1−x N/GaN MQW grown on Aface GaN surface and its energy bandedge profile. In the QW, the electrons and holes are separated spatially even under equilibrium conditions. Problems 1.
The GaAs/Al0.25 Ga0.75 As highelectronmobility transistor (HEMT) is one of the major highspeed devices used in wireless communications. The Al0.25 Ga0.75 As layer is doped with silicon at a doping density of ~1018 cm–3 . The undoped GaAs has a ptype background near ~1014 cm–3 . Other relevant material parameters are listed below.
7.6 Polarization Fields in Wurtzite Heterostructures
285
Relative dielectric constant (r )
m ∗e /m 0
m ∗hh /m 0
m ∗lh /m 0
GaAs
12.85
0.067
0.5
0.076
AlAs
10.06
0.71
0.409
0.153
Draw the band diagram of this p–N heterojunction to scale including the following information: (a) The conduction band discontinuity, E c , and the valence band discontinuity, E v ; (b) Fermi level positions; (c) Contact potential on each side; and (d) Depletion width. (e) Estimate the ground state energy in the triangular quantum well formed at the p–N GaAs/Al0.25 Ga0.75 As heterojunction. An infinitely high barrier at the heterojunction is assumed in this problem. 2. 3.
Derive the depletion width x N and x p of a pN heterojunction as a function of the contact potential V 0 and doping levels, N a and N D . The doping levels in a pGaAs/NAl0.3 Ga0.7 As heterojunction are N a = 5× 1016 cm−3 and N D = 5×1017 cm−3 . The dielectric constant of Alx Ga1−x As is expressed as s = 0 (13.1 − 3.0x). (a) Calculate the contact potential. (b) Calculate the depletion width of the heterojunction. (c) Plot the detail equilibrium band diagram of the pN junction.
4.
5.
(a) Determine the allowed energy levels in the conduction band of a 60 Å GaAs/ Al0.3 Ga0.7 As quantum well using realistic material parameters. The electron effective masses of GaAs and AlAs are 0.067m0 and 0.71m0 , respectively. The conduction band discontinuity between GaAs and Al0.3 Ga0.7 As is E c = 0.2 eV. (b) Repeat part (a) without considering the mass difference between barriers and well. Use the GaAs effective mass of the well in your calculation. Comment on whether this approach is appropriate. At the interface of an undoped AlGaAs/GaAs heterojunction, a triangular quantum well in the conduction band is formed on the GaAs side. Assume the potential barrier is infinitely high at the heterojunction interface and the potential variation on the GaAs side under equilibrium condition can be approximated by a straight line with a value of 5 × 104 V/cm. (a) Estimate the ground state energy of this quantum well. (b) Compare the results obtained using the exact solution of the Airy function and the FangHoward approximation. (c) What is the corresponding well width at the ground state energy? The effective mass of GaAs is m ∗e = 0.067 m 0 for electrons.
286
6.
7.
8.
9.
7 Electrical Properties of Compound Semiconductor Heterostructures
In a rectangular AlGaAs/GaAs quantum well, the well is 0.3 eV deep for electrons. Calculate the ground state energy of an electron in the rectangular GaAs quantum well using the same well width as calculated from the last problem. Which quantum well, rectangular or triangular, gives higher ground state energy, and why? Derive the transmission amplitude (t) of a square barrier structure including the mass difference between the barrier (m ∗b ) and its surroundings (m ∗s ). The barrier has a thickness a and barrier height V 0 . A superlattice structure formed on InP substrate is made of stacking latticematched Ga0.47 In0.53 As and Al0.48 In0.52 As layers alternatively. The conduction band discontinuity between these two ternary alloys is E c = 0.47 eV. The electron effective masses of Ga0.47 In0.53 As and Al0.48 In0.52 As are 0.041m0 and 0.075m0 , respectively. Estimate the bound states in such a superlattice structure where both barriers and wells are equal to 30 Å. Assume the conduction band discontinuity (E c ) at the Al0.3 Ga0.7 As/GaAs interface is 0.2 eV. (a) Calculate the allowed energy states of a 40 Å GaAs/Al0.3 Ga0.7 As quantum well. (b) A single 40 Å Al0.3 Ga0.7 As/GaAs barrier structure is formed. Calculate the transmission coefficient (T ) at the lowest energy level obtained in part (a). (c) An Al0.3 Ga0.7 As/GaAs superlattice has barriers and wells with the same thickness of 40 Å. Estimate the miniband width of the lowest allowed energy band.
10. A triangular quantum well in the conduction band is formed in the InGaN/GaN heterostructure where the undoped InGaN layer has an In composition of 15% and a thickness of 20 nm. (a) Determine the type of the sheet charge created in the quantum well. (b) Calculate the 2D sheet charge density. 11. The purpose of this assignment is to learn how to use SimWindows simulation software by David Winston for calculating the energy band diagram of heterostructures. Other commercial softwares, such as Silvaco Atlas (www. silvaco.com), can also be used. You can download SimWindows simulation program through the following link: http://simwindows.wixsite.com/simwin dows. The active region of an nAl0.3 Ga0.7 As/GaAs (undoped)/pAl0.3 Ga0.7 As doubleheterostucture (DH) diode laser has a 0.1 μm thick undoped GaAs active region. Under a forward bias, electrons and holes are injected into the GaAs active region from n and psides of the DH structure, respectively. Plot the equilibrium energy band diagram of the DH structure using SimWindows as a function of thickness. The thickness range of interest is 0.1 μm (pAlGaAs) −0.1 μm GaAs −0.1 μm (nAlGaAs). The doping concentrations of the n and pdoped AlGaAs
7.6 Polarization Fields in Wurtzite Heterostructures
287
are at the same level of 2 × 1017 cm−3 . Plot the energy band diagram again for the same structure, except with the GaAs layer heavily doped to p = 5 × 1018 cm−3 .
References 1. 2. 3. 4. 5. 6.
I. Vurgaftman, J.R. Meyer, L.R. RamMohan, J. Appl. Phys. 89, 5815 (2001) F.F. Fang, W.E. Howard, Phys. Rev. Lett. 16, 797 (1966) W. Franz, Z. Naturforsch. 13a, 484 (1958) L.V. Keldysh, Soviet Physics, JETP 7, 788 (1958) O. Ambacher et al., J. Appl. Phys. 85, 3222 (1999) O. Ambacher et al., J. Phys. Condens. Matter 14, 3399 (2002)
Further Reading 1. H.C. Casey, M.B. Panish, Heterostructure Lasers: Part A, Fundamental Principles (Academic, New York, 1978) 2. S. Wang, Fundamentals of Semiconductor Theory and Device Physics (PrenticeHall, Englewood Cliffs, 1989) 3. J.H. Davies, The Physics of LowDimensional Semiconductors (Cambridge University Press, Cambridge, United Kingdom, 1998) 4. S.L. Chuang, Physics of Photonic Devices, 2nd edn. (Wiley, New York, 2009)
Chapter 8
Optical Properties of Compound Semiconductor Heterostructures
Abstract Due to the nature of the indirect energy band structure, efficient light emission from silicon is impossible. On the other hand, direct energy band III–V compound semiconductors, such as GaAs, InP, and GaN, are efficient lightemitting materials. By mixing two or three III–V binaries, one can prepare a series ternary or quaternary compounds with added freedoms in the selection of the bandgap energy. Bandgap engineering in heterostructures further allows the creation of new functional devices as will be discussed in Chaps. 9 and 10. Following the discussions of electrical properties of heterojunctions in Chap. 7, we will study their optical properties in this chapter including two major optical processes: the optical absorption and radiative optical transition. The absorption coefficient, spontaneous emission rate, and stimulated emission rate are interrelated through Einstein relations. Finally, the transparency condition of stimulated emission in a semiconductor is discussed.
8.1 Basic Optical Properties of Dielectric Medium 8.1.1 Maxwell’s Equations The timevarying electric and magnetic field intensities are expressed as E(x, y, z, t) = E(x, y, z)exp(iωt) and H(x, y, z, t) = H(x, y, z)exp(iωt). The propagation of electromagnetic waves is governed by the Maxwell’s equations shown below. ⎧ ∂B ⎪ ⎪ ∇×E=− ⎪ ⎪ ∂t ⎪ ⎨ ∂D ∇×H= J+ ∂t ⎪ ⎪ ⎪ ∇·D=ρ ⎪ ⎪ ⎩ ∇·B=0
Faraday’s law Ampere’s law
(8.1)
Gauss’ law Gauss’ law
Here, B is the magnetic flux density, D is the displacement flux density, J is the current density, σ is the conductivity, and ρ is the charge density. The relations between E, H, D, J, and B are © Springer Nature Switzerland AG 2020 K. Y. Cheng, III–V Compound Semiconductors and Devices, Graduate Texts in Physics, https://doi.org/10.1007/9783030519032_8
289
290
8 Optical Properties of Compound Semiconductor Heterostructures
⎧ D = E = 0 E + P ⎪ ⎪ ⎨ J =σE ⎪ B = μH ⎪ ⎩ ∇ · J = −∂ρ/∂t
(8.2)
P, , and μ are the polarization vector, permittivity (or dielectric constant), and permeability of the wave propagation medium, respectively. The permittivity of the free space is 0 . Also, for a linear, homogeneous, and isotropic medium, the polarization vector is related to the applied electric field by P = 0 χ E
(8.3)
D = 0 (1 + χ )E = E
(8.4)
Thus,
where χ is the electric susceptibility. When the wave is propagating across the boundary between two materials, the boundary conditions are ⎧ nˆ · ( D1 − D2 ) = ρs ⎪ ⎪ ⎨ nˆ · (B 1 − B 2 ) = 0 ⎪ nˆ × (E 1 − E 2 ) = 0 ⎪ ⎩ nˆ × (H 1 − H 2 ) = J s
(8.5)
The unit vector nˆ represents the normal of the interface and is oriented from region 2 to region 1.
8.1.2 Electrical and Optical Constants in a Lossless (σ = 0) Dielectric For a plane wave propagating in the zdirection, the electric and magnetic fields have the following characteristics: E(x, y, z, t) = E x (z, t), E y = E z = 0, ∂/∂ x = ∂/∂ y = 0; and H (x, y, z, t) = Hy (z, t), Hx = Hz = 0 The wave equation of such a plane wave is given by ∂ 2 Ex ∂ 2 Ex = μ 0 ∂z 2 ∂t 2 The solution of E x (z, t) is generally written as
(8.6)
8.1 Basic Optical Properties of Dielectric Medium
E x (z, t) = E x (z) exp(iωt)
291
(8.7)
Substituting it in the wave equation gives ∂ 2 Ex = −μ0 ω2 E x = −k 2 E x ∂z 2
(8.8)
√ where k ≡ ω μ0 is the propagation constant. The wave equation has the solution for the wave propagating in the +zdirection: E x = A exp[i(ωt − kz)] = A cos(ωt − kz)
(8.9)
From Faraday’s law, H y is readily found to be Hy =
ω A cos(ωt − kz) k
(8.10)
The propagation of the plane wave in a lossless medium is illustrated in Fig. 8.1. By analyzing the electric field intensity at a fixed time, say t = 0 or t = π /2ω, we find the wavelength of the field to be λ = 2π/k or k = 2π/λ Here, k has the value of the wave number and is called the phase or propagation constant. The wave propagation velocity is deduced from υ = z/t = ω/k. υ=
1 ω =√ k μ0
(8.11)
In free space, the propagation velocity has the speed of light, c, and
Fig. 8.1 Wave propagation in a lossless medium along the zdirection at t = π/2ω. The electric field intensity crosses the zaxis at π/k, 2π/k, 3π/k, etc.
292
8 Optical Properties of Compound Semiconductor Heterostructures
1 c= √ μ0 0
(8.12)
The ratio of the free space velocity to the velocity in a dielectric medium is defined as the refractive index n: n=
= 1+χ 0
(8.13)
The frequency, ν, of the wave in free space and dielectric medium is the same: ν=
c υ = λ λ0
(8.14)
We obtain the wavelength in the dielectric medium as λ = λ0 /n and k = nk0 .
8.1.3 Electrical and Optical Constants in a Lossy (σ = 0) Medium Since σ = 0, the magnetic field intensity has the form ∂ Hy ∂ Ex = σ Ex + − ∂z ∂t
(8.15)
The wave equation becomes ∂ 2 Ex = iωμ0 (σ + iω)E x = K 2 E x . ∂z 2
(8.16)
√ Here K ≡ iωμ0 (σ + iω) = (α/2) + iβ. is the complex propagation constant. The solutions of the wave equation for the +z propagating plane wave are ⎧ ⎨ E x (t) = A exp[−(αz/2) + i(ωt − βz)] = A exp(−αz/2) cos(ωt − βz) (σ + iωt) ⎩ Hy (t) = E x (t) K (8.17) The electric field intensity attenuates in the direction of wave propagation in z, as illustrated in Fig. 8.2. In the lossless medium, the propagation constant term in the wave equation is k 2 = μ0 ω2 = n 2 k02
(8.18)
8.1 Basic Optical Properties of Dielectric Medium
293
x exp(–az/2) π/k y
3π/k
z
2π/k Hy(z,t)
Ex(z,t)
Fig. 8.2 Traveling wave in a lossy medium as represented by (8.17) at t = 0 and α = k/ 2π
In the same manner for the lossy case, 2
K 2 = iωμ0 (σ + iω) = −μ0 ω2 + iσ μ0 ω = −N k02
(8.19)
where N is the complex refractive index with the real part n and imaginary part κ: N = n − iκ
(8.20)
Combining the above two equations with k0 = 2π/λ0 gives the complex dielectric constant :
2 N = n 2 − κ 2 − i2nκ = μ0 ω2 − iσ μ0 ω /k02 σ = 1 + i2 = = −i 0 0 ω
(8.21)
Equating real and imaginary parts gives ⎧ ⎪ ⎨ n2 − κ 2 = = 1 0 σ ⎪ = 2 ⎩ 2nκ = 0 ω
(8.22)
and ⎧ ⎪ ⎪ ⎨n =
1/2 1 + 12 + 22 1/2 ⎪ ⎪ ⎩ κ = √1 −1 + 12 + 22 2 √1 2
(8.23)
Thus, N and ¯ are dependent variables. Furthermore, the complex propagation constant 2 (8.24) K = (α/2) + iβ = −N k02 = i(n − iκ)k0
294
8 Optical Properties of Compound Semiconductor Heterostructures
which gives
α = 4π κ/λ0 ∝ σ β = nk0 = k
(8.25)
The attenuation term α is related to the conductivity and is the absorption coefficient. β is identical to the propagation constant k of the lossless medium. The quantity κ is called the extinction coefficient. Therefore, the electrical properties (ω) and σ (ω) are related to the optical properties n(ω) and α(ω) through equations listed above.
8.1.4 Dielectric Constant In electromagnetic theory, the dielectric constant is related to the applied electric field intensity and polarization. The interaction of a light wave and a bounded electron can be modeled using a dipole oscillator model developed by Hendrick Lorentz in 1878. The electric field of the light wave induces forced oscillations of the atomic dipole through the driving forces exerted on the bound electrons. As shown in the model of Fig. 8.3, the displacement of the atomic dipoles can be seen as damped harmonic oscillators since the oscillating dipoles can lose their energy through an interaction with phonons. We assume that the mass of the nucleus of the host atom is much larger than the electron mass, so the displacement x of the electron is governed by the following equation of motion: m
dx d2 x + βx = −q E(t). + mγ 2 dt dt
(8.26)
where β, γ , and E(t) are the spring constant, damping rate, and the timevarying electric field, respectively. The three terms on the LHS of (8.25) represent the acceleration, damping, and restoring force, respectively. Fig. 8.3 A simple model of a dipole. When interacting with an applied electric field, E, the bound electron vibrates about is equilibrium position while the atom is stationary
+
E
–
x(t)
8.1 Basic Optical Properties of Dielectric Medium
295
The interaction of the atom with a monochromatic light wave of angular frequency ω is considered. For the timedependent electric field with the form E(t) = E 0 exp(−iωt), we look for solutions of the form x(t) = x 0 exp(–iωt). The solution of the equation of motion for a displacement x is x(t) = −
q E 0 /m exp(−iωt) ω02 − ω2 − iωγ
(8.27)
√ where ω0 ≡ β/m is the natural oscillation frequency. The displacement of electrons from their equilibrium position produces a timevarying dipole moment p(t). The resonant polarization PR = Np(t) = –Nqx(t), where N is the atomic density. Therefore, PR is proportional to x(t) according to (8.27). However, the magnitude of PR is small unless the frequency is close to ω0 . The induced timevarying polarization under the influence of the electric field produces an electric displacement flux D = 0 E + P = E. We are interested in the optical response near ω0 , so we include the resonant polarization part into the expression. D = 0 E + P + PR = 0 E + 0 χ E + PR = 0 r E
(8.28)
E N q2 PR = −N q x = m ω02 − ω2 − iωγ
(8.29)
The complex relative dielectric constant is expressed as 1 N q2 r (ω) = 1 + i2 = 1 + χ + 0 m ω02 − ω2 − iωγ
(8.30)
The real and imaginary parts of the dielectric constant are related to the refractive index and absorption coefficient of the medium and are expressed as ⎧ ω02 − ω2 N q2 ⎪ ⎪ = 1 + χ + (ω) ⎪ 1
⎨ 0 m ω2 − ω2 2 + (γ ω)2 0 γω N q2 ⎪ ⎪ ⎪ 2 ⎩ 2 (ω) = m 2 2 0 ω − ω + (γ ω)2
(8.31)
0
The low and highfrequency limits of r (ω) are expressed as ⎧ ⎨ ⎩
r (0) ≡ st = 1 + χ + r (∞) ≡ ∞ = 1 + χ
N q2 0 mω02
(8.32)
296
8 Optical Properties of Compound Semiconductor Heterostructures
where st and ∞ are static and optical relative dielectric constants, respectively. The difference of these two constants is st − ∞ = N q 2 /0 mω02 Near the resonance where ω ≈ ω0 γ , the dielectric constant can be rewritten, using the approximation of δω = (ω0 − ω) and ω02 − ω2 = (ω0 + ω)(ω0 − ω) ≈ 2ω0 δω as ⎧ ⎪ ⎨ 1 (δω) = ∞ − (st − ∞ ) ⎪ ⎩
2ω0 δω 4(δω)2 + γ 2 γ ω0 2 (δω) = (st − ∞ ) 4(δω)2 + γ 2
(8.33)
Figure 8.4 shows the frequency dependence of 1 and 2 predicted by (8.33) for a given set of st , ∞ , γ (s−1 ), and ω0 (rad/s). The frequency response of 1 has a complicated shape with two extremes at (ω0 ± γ /2). For 2 , it is a strong peak function of ω with a maximum value at ω0 and a fullwidth at halfmaximum of γ . Figure 8.4 also shows the refractive index and extinction (absorption) coefficient calculated from 1 and 2√using (8.23). We see that n approximately follows the of ω frequency dependence of 1 (ω), while κ or α is a strongly peaked function √ and more or less follows 2 (ω). The correspondence between n and 1 (ω), and between κ and 2 (ω) would be exact if κ or α were much smaller than n as in weakly absorbing media. In semiconductors, this corresponds to the absorption in the transparent spectral region where E < E g .
Fig. 8.4 Frequency dependence of the a real and b imaginary parts of the complex dielectric constant of a dipole oscillator at frequencies close to resonance calculated with ω0 = 1014 rad/s, γ = 5 × 1012 s−1 , st = 12.1, and ∞ = 10. Also shown are the a refractive index and b extinction coefficient derived from the dielectric constant. Reprinted with permission from [1] copyright Oxford University Press
8.1 Basic Optical Properties of Dielectric Medium
8.1.4.1
297
Refractive Index
The refractive index of a semiconductor is related to its complex dielectric constant (ω) = 1 (ω) + i2 (ω). For most photonic applications, such as lasers, we are interested in the optical transitions with energy smaller than the bandgap energy. In the region below the bandgap, 2 (ω) has no contribution to the optical dispersion and can be neglected. Therefore, we can assume that n∼ =
1 (ω) =
/0
(8.34)
In III–V alloys, n in the transparency region is given by [2, 3] n(ω) =
A
∗
1/2 3/2 Eg 1 ∗ f (y) + B f (x) + 2 E g + so
(8.35)
√ √ 1 2 − with f (z) = 1 + z − 1 − z where x = ω/E g and y = 2
z ω/ E g + so . The two terms in the brackets correspond to the free electron–hole pair contributions arising from the E g and E g + so gaps, respectively. A* and B* are the strength parameters for the fundamental and higherlying band transitions, respectively. The numerical values of A* and B* required to calculate the refractive index are listed below for several important III–V alloys. For Gax In1−x Asy P1−y latticematched to an InP system, by fitting the experimental results, we get: A∗ (y) = 8.40−3.40y and B ∗ (y) = 0.60 + 3.40y Figure 8.5 shows the fitted calculation results of refractive indices up to the bandgap energy for each As composition y between 0 and 1. For the Alx Ga1−x As/GaAs system, the fitted parameters are: A∗ (x) = 6.64 + 16.92x and B ∗ (x) = 9.20−9.22x The measured refractive indices of the Alx Ga1−x As system are plotted for x up to 0.38 in Fig. 8.6a. The roomtemperature refractive indices at energy of 1.38 eV over the whole composition range are shown in Fig. 8.6b. For the Alx Ga1−x N system, only the fundamental transition E g is considered, i.e., the f (y) term in (8.35) is set to be zero. In the transparent spectral region, for x Al < 0.4, the fitting parameters are [4]: A∗ (x) = 9.82661−8.21608x−31.5902x 2 and
298
8 Optical Properties of Compound Semiconductor Heterostructures
Fig. 8.5 Refractive index of Gax In1−x Asy P1−y latticematched to InP up to the bandgap energy for each ycomposition. Reprinted with permission from [2] copyright AIP Publishing
B ∗ (x) = 2.73591 + 0.84249x−6.28321x 2 For alloys with higher Al composition (x Al > 0.4) the fitting parameters are [5]: A∗ (x) = (3.17 ± 0.39)x 1/2 + (9.98 ± 0.27) and B ∗ (x) = −(2.2 ± 0.2)x + (2.66 ± 0.12). Alternatively, the refractive indices of the Alx Ga1−x N system in the transparent spectral region have also been determined using the Kramers–Kronig relations coupled with highaccuracy experimental results of spectroscopic ellipsometry. The results near room temperature are plotted for x up to 0.64 in Fig. 8.7.
8.2 Absorptions in Semiconductors Absorption in semiconductors is expressed in terms of the absorption coefficient α(ω). The absorption coefficient is commonly defined as the fraction of the power loss dI/I per incremental length dz:
8.2 Absorptions in Semiconductors
299
Fig. 8.6 a Refractive index as a function of photon energy for Alx Ga1−x As. b Refractive index of Alx Ga1−x As at an emission wavelength of 1.38 eV. Reprinted with permission from [3] copyright AIP Publishing
300
8 Optical Properties of Compound Semiconductor Heterostructures
Fig. 8.7 Refractive index as a function of photon energy for Alx Ga1−x N at 290 K with x Al = 0, 0.23, 0.45, and 0.64. Reprinted with permission from [6], copyright AIP Publishing
α≡−
dI /I dz
−1 cm
(8.36)
The absorption coefficient associated with the optical process depends on the probability per unit time that an electron will make a transition from the valence band to the conduction band under the influence of radiation of intensity I(ω) at the frequency ω. The problem of calculating this transition probability is, however, strictly quantum mechanical, since the exact energy band structures involved cannot be determined using classical physics. In general, the absorption coefficient for a given photon energy hv is proportional to the transition probability W if from the initial state with an electron density of ni to the final state with nf of available empty state density. This process must be summed for all possible transitions between states separated by an energy difference equal to hv. α(hν) = A
Wi f n i n f
(8.37)
In semiconductors, as illustrated in Fig. 8.8, various optical absorption processes generated by the incident electromagnetic radiation include highlying band transitions, excitons, bandedge absorption, imperfection absorption, free carrier absorption, and Reststrahlen absorption. In the following, only those nearbandedge transitions will be considered in more detail.
8.2.1 Allowed Direct Transition Between Bands For optical transitions between the valence band and conduction band, both momentum conservation and energy conservation conditions have to be fulfilled. Because the momentum of a photon, h/λ (λ ~μm), is very small compared to the crystal momentum, h/a (a ~Å), the photon absorption process should conserve the
8.2 Absorptions in Semiconductors
301
Fig. 8.8 Optical absorption coefficient as a function of photon energy for Si and GaAs at room temperature. The major absorption mechanisms are shown
momentum of the electron. Therefore, for transitions in direct bandgap semiconductors, all the momentumconserving transitions are allowed. As shown in Fig. 8.9, every initial state at E i is associated with a final state at E f such that ω = hν = E f − E i
(8.38)
In a parabolic band, E f = Eg +
2 k 2 2m ∗e
(8.39a)
and Ei = − Therefore,
2 k 2 2m ∗h
(8.39b)
302
8 Optical Properties of Compound Semiconductor Heterostructures
Fig. 8.9 Energy band diagram of a direct bandgap semiconductor. The top of the valence band at the zone center is set to have zero energy
2 k 2 1 1 hν = E f − E i = E g + + ∗ 2 m ∗e mh
(8.40)
Following (3.29), the joint DOS is given by
∗ 3/2 2m r hν − E g D(hν) = 2 2π 3
(8.41)
where m ∗r is the reduced mass given by 1 1 1 = ∗+ ∗ m ∗r me mh
(8.42)
The transition probability from an initial state to a group of final states is derived from the firstorder, timedependent perturbation theory as Wi =
2 2π Mi f D E f
(8.43)
Here M if is the matrix element of the perturbation which connects the states i and f of the system, and D(E f ) is the density of final states. Hence, the absorption coefficient for allowed direct transition is α(hν) = A∗ hν − E g
(8.44)
for which M if is independent of k. The constant A* has a value of ~2 × 104 for GaAs. The absorption coefficients as functions of energy for a number of elemental and III– V compound semiconductors are shown in Fig. 8.10. The direct bandgap material
8.2 Absorptions in Semiconductors
303
Fig. 8.10 Absorption coefficient versus photon energy for selected element and III–V compound semiconductors at room temperature. Reprinted with permission from [7] copyright IEEE
has a rather sharp increase in absorption coefficient at energies slightly larger than the bandgap.
8.2.2 Indirect (Nonvertical) Transitions Between Indirect Valleys The mechanism for indirect optical transitions generally involves the simultaneous emission or absorption of a phonon with the absorption of the photon (Fig. 8.11). The electron, initially at E i in the valence band at k ≈ 0, is raised in a vertical transition to the intermediate state, also at k ≈ 0, in the conduction band. It then absorbs, or emits, a phonon of wave vector ±k p and makes the transition to the conduction band minimum at E f . The photon energy is related to the phonon absorption (−èωp ) or phonon emission (+èωp ) by hνa = E f − E i − ωp
(8.45a)
hνe = E f − E i + ωp
(8.45b)
304
8 Optical Properties of Compound Semiconductor Heterostructures
Fig. 8.11 Energy band diagram of an indirect bandgap semiconductor. The phonon absorptionassisted transition between E i and E f is shown
The transition probability for an indirect transition depends on the total matrix element and the effective density of states. The density of final conduction band states is
(8.46) Dc E f = A c E f − E c = A c δ − E i where δ is the total energy of states above E c and below E v , and is given by δ = hν − E g ± ωp
(8.47)
The density of states in the initial valence band is Dv (E i ) = Av E v − (−E i ) = Av E i
(8.48)
The effective density of states for the transition is δ Dc (E)Dv (E)dE i = Ac Av
δ D(hν) ∝ 0
δ
δ − Ei
E i dE i
(8.49)
0
Therefore,
2 D(hν) = Aa δ 2 = Aa hν − E g ± ωp
(8.50)
Since this is the phononassisted transition, we have to include the probability of phonon absorption or emission in the calculation. The density of phonons with frequency ωp is given by Planck’s law and has a Bose–Einstein distribution.
8.2 Absorptions in Semiconductors
305
N ωp = 1/ exp ωp /kT − 1
(8.51)
The absorption coefficient due to indirect transition involving phonon absorption becomes
2 Aa hν − E g + ωp
αa = exp ωp /kT − 1
(8.52)
For phonon emission process, the probability is proportional to N(èωp ) + 1. The absorption coefficient due to indirect transition involving phonon emission is given by
2 Ae hν − E g − ωp
αe = 1 − exp −ωp /kT
(8.53)
The total absorption coefficient for optically allowed indirect transition is then α = αa + αe
(8.54)
√ As illustrated in Fig. 8.12a, the plot of α versus photon energy should yield a curve consisting of two straightline segments. The extrapolation of the straight lines to α = 0 gives the values of (E g ± èωp ). At very low temperatures, the phonon density is very small, and the segment associated with αa diminishes. Indeed, in a highpurity Si sample measured between 195 and 415 K (Fig. 8.12b), the phonon absorption segment decreases with the reduction of measurement temperature.
8.2.3 Transitions in Highly Doped Semiconductors Absorption in semiconductors depends on the detailed energy band structure of the material including the bandgap energy, the density of states in the vicinity of the band edge, and the type of optical transition allowed. In general, both conduction band and valence band near the band edge can be approximated by parabolic functions for undoped and lightly doped semiconductors as described in the previous sections. However, at high doping concentrations, many characteristics of semiconductors change, such as the density of states distribution near the band edge, the energy of the fundamental gap, and the impurity ionization energy. If the semiconductor is heavily doped, the conduction band becomes considerably filled due to the finite density of states, and the Fermi level is inside the band. Absorption transitions from the top of valence band to the bottom of the conduction band cannot occur due to the band filling effect. Hence, the absorption transition energy shifts from ~E g for undoped semiconductor to >E g in heavily doped ntype semiconductors. The shift of the absorption edge to energy higher than E g due to band filling is called Burstein–Moss
306
8 Optical Properties of Compound Semiconductor Heterostructures
Fig. 8.12 a Temperature dependence of αe and αa . b Square root absorption coefficient as a function of photon energy for a highpurity Si measured at different temperatures. Reprinted with permission from [8] copyright American Physical Society)
shift (Fig. 8.13a). The measured absorption coefficients in ntype GaAs for different doping concentrations are reproduced in Fig. 8.14. The Burstein–Moss shift starts to affect the absorption edge as the carrier density exceeds 6 × 1017 cm−3 . For ptype semiconductors, however, the Burstein–Moss shift is less important. This is due to the high density of states of the valence band originating from the much heavier mass of holes as compared to electrons. Impurities in semiconductors are generally represented as a localized level at a fixed energy with respect to the conduction or valence bands. However, it was observed that the ionization energy for both donors and acceptors decreased as the impurity concentration was increased. The ionization energy of n and ptype GaAs
8.2 Absorptions in Semiconductors
307
Fig. 8.13 Energy diagrams show a the absorption edge shift to higher energy due to band filling in degenerated ntype semiconductor, and b formation of band tails in a heavily doped semiconductor
Fig. 8.14 Measured absorption coefficient in ntype GaAs at room temperature for different doping concentrations. Reprinted with permission from [9] copyright AIP Publishing
goes to zero for free carrier densities near 2 × 1016 cm−3 and 5 × 1018 cm−3 , respectively. These results strongly suggest that impurities in semiconductors can be treated by the localized level concepts only in undoped and lightly doped semiconductors. Thus, the random distribution of impurities in semiconductors is a more realistic assumption. The random distribution of charged impurities in the crystal with high impurity concentration results in potential fluctuations and causes the band edges to vary spatially. This leads to the formation of band tails which contain states with energy below the unperturbed conduction band edge or above the unperturbed valence band edge. Thus, the band tail states extend into the forbidden gap. (Figure 8.13b) These band tail states affect the density of states significantly but only in the vicinity
308
8 Optical Properties of Compound Semiconductor Heterostructures
of the band edge. However, the spatially averaged position of the band edge does not change. At high doping concentrations, the magnitude of the bandgap energy reduces with doping concentration—a phenomenon referred to as bandgap narrowing, bandgap shrinkage, or bandgap renormalization. The main reasons for bandgap narrowing are manybody effects of free carriers. At high free carrier concentrations, the small carriertocarrier distance allows electrons to interact with each other through the longrange Coulomb potential. The carrier–carrier interaction causes other electrons in the vicinity to spatially redistribute in order to reduce the total energy of the electron system. Therefore, bandgap narrowing occurs in heavily doped semiconductors, and the change in energy gap (E g ) follows a onethird power of the doping concentration. The Burstein–Moss shift and bandgap narrowing are two competing effects that cause the Fermi level to change in opposite directions. In heavily doped ntype semiconductors, the Burstein–Moss shift causes the Fermi level to increase while the Fermi level moves downward by bandgap narrowing. As shown in Fig. 8.14, the Burstein–Moss shift prevails in the ntype GaAs due to the light electron effective mass, resulting in a blueshift of the absorption edge. For heavily doped ptype GaAs, a completely opposite behavior is observed as shown in Fig. 8.15. The bandgap narrowing and the formation of band tail states—rather than the Burstein–Moss shift—dominate the nearbandedge optical absorption, as is evident from the redshift of the optical absorption edge with increasing doping concentration.
Fig. 8.15 Measured absorption coefficient in ptype GaAs at room temperature for different doping concentrations. Reprinted with permission from [9] copyright AIP Publishing
8.2 Absorptions in Semiconductors
309
8.2.4 Exciton Absorption Exciton represents a system of electron and hole bound to one another by their mutual Coulomb attraction. A bound electron–hole pair or exciton can be created by the absorption of a photon. The free electron can orbit about the free hole as if this were a hydrogenlike atom with a reduced mass mr . Since the exciton exist in the crystal and not in free space, the binding energy is reduced by the reduced mass and the dielectric constant. m rq 4 1 (m r /m 0 ) Ry =− Ex = − 2h 2 2 n 2 r2 n2
(8.55)
where Ry = 13.6 eV and n is an integer ≥1. Using mr = 0.059m0 and r = 12.85 for GaAs, the lowest exciton energy level (n = 1) has a value of −4.9 meV. Since the exciton can move through the crystal as a unit, it does not have a welldefined potential in the semiconductor energy diagram. The calculated binding energy is customarily referenced to the conduction band minimum. At n = ∞, it merges with the conduction band edge. For the ground state (n = 1) of the exciton, the binding energy is quite small, and the exciton can be easily dissociated at room temperature. Since the electron and the hole of an exciton must move together through the crystal, their translational velocities must be identical. This condition places a restriction on the regions in Ek space where excitons can be found, such that both carriers move at the same velocity (υ ∝ dE/dk). Thus, excitons can be created by photon absorption at any critical point, where dE v dE c − =0 dk dk
(8.56)
In direct bandgap materials, the groundstate level (n = 1) of an exciton is easily observed as an absorption peak on the lower energy side of the absorption edge. The free exciton occurs when the photon energy is hv = E g − E x , where E x is the binding energy of the exciton. At low temperatures, the exciton absorption has a very pronounced transition, which broadens with temperature. Figure 8.16 shows that the exciton feature diminishes in GaAs as the temperature is increased toward room temperature. If the exciton is formed with the simultaneous absorption or emission of a phonon, as seen in indirect transitions, the increase in absorption coefficient occurs at hν = E g − E x ± ωp
(8.57)
for the transition with phonon emission or absorption. With the participation of the phonon in the transition, the exciton may acquire an additional momentum from the phonon, modifying the associated kinetic energy. The addition of the kinetic energy broadens the exciton level into the band. Although no absorption peak is expected, the presence of indirect exciton absorption should still be noticeable as a
310
8 Optical Properties of Compound Semiconductor Heterostructures
Fig. 8.16 Exciton absorption in GaAs at various temperatures. The exciton absorption peak becomes more pronounced at low temperatures. Reprinted with permission from [10] copyright American Physical Society
sharp rise in the absorption coefficient. In addition, since there are two transverse and one longitudinal phonons in each of the acoustic and optical branches of the phonon spectrum, more than one phonon can participate in the transition with various combinations. Therefore, a large number of steps in the absorption edge can be detected. The rich absorption spectra of the indirect bandgap GaP are shown in Fig. 8.17 as an example. In addition to free excitons, a free hole can combine with a neutral donor to form a positively charged excitonic ion complex called a donor bound exciton. As shown in Fig. 8.18, in such a complex, the electron bound to the donor travels in a wide orbit about the donor while the associated hole moves in the electrostatic field of the dipole determined by the instantaneous position of the electron. An electron associated with a neutral acceptor also forms an ‘acceptor bound exciton.’ Due to the twodimensional nature of quantum wells, the exciton binding energy in a quantum well is enhanced due to a large overlap of the electron and hole wave functions. As in the 3D case, the binding energy of the exciton in a quantum well can be derived by solving a 2D hydrogen model. It has the value E x2D = −
1 1 mr q 4 (m r /m 0 )R y = − n = 1, 2, 3, . . . 2h 2 2 (n − 1/2)2 r2 (n − 1/2)2 (8.58)
The diameter of the exciton orbit can also be determined as 4π 2 r = 0.53 ax2D = m rq 2 m r /m 0
(8.59)
8.2 Absorptions in Semiconductors
311
Fig. 8.17 Square root absorption coefficient of GaP measured at different temperatures. Reprinted with permission from [11] copyright American Physical Society
Fig. 8.18 Illustration of an exciton bound to donor, D
For n = 1, the binding energy and orbit radius of an exciton in a GaAs quantum well are 4E x and ~100 Å, respectively. Using MBE growth technique, GaAs/Al0.2 Ga0.8 As QWs with well widths 140 and 210 Å were demonstrated at Bell Laboratories for the first time. When measured at a very low temperature of 2 K, shown in Fig. 8.19, the QW absorption steps are clearly observed with associated exciton peaks. Due to the increased binding energy, in some materials such as InGaAs/InAlAs QW, the excitonic effect could be observed even at room temperature.
312
8 Optical Properties of Compound Semiconductor Heterostructures
Fig. 8.19 Optical absorption spectra of bulk and quantumwell heterostructures. Reprinted with permission from [12] copyright American Physical Society
8.2.5 Absorption Due to Isoelectronic Traps While the probability of radiative recombination taking place in an indirect bandgap semiconductor is extremely low, the situation was changed by the discovery of N isoelectronic traps in GaP in 1965. Such a trap is called isoelectronic because it has the same number of valence electrons as the atom it replaces when it sits substitutionally on the lattice site. The substitution of nitrogen for a group V atom in GaP establishes a shortrange potential well resulting from the combination of the difference in electronegativity between the N atom and the group V atom that it replaces, and the hydrostatic deformation of lattice around the N site that arises from the large covalent radius difference. This potential well allows the N atom to capture an electron, which in turn can bind a hole by Coulomb attraction, thus forming a bound exciton at about 10 meV below the conduction bandedge. Since the electron is bound to the immediate vicinity of the N impurity (real space), the wave function of the electron is diffused in kspace. The wave function of the electron at the isoelectronic trap is much more extensive in kspace. Thus, there is an enhancement near k = 0 () which results in increased electron–hole recombination in the band region. At k = 0, the shallow N isoelectronic trap depth with a favorable conduction band structure leads to an increase of the electron distribution probability by almost three orders of magnitude and enables the generation of relatively efficient green (near bandgap) electroluminescence in GaP:N LEDs.
8.2 Absorptions in Semiconductors
313
Fig. 8.20 Lowtemperature photoluminescence spectrum from a lightly Ndoped GaP crystal. The bound exciton emissions A and B lines are prominent transitions. Reprinted with permission from [13] copyright American Physical Society
The features of the absorption spectrum due to isoelectronic traps in a nitrogendoped GaP have different origins. In a lightly nitrogendoped (~5 × 1016 cm−3 ) sample, the dominant transitions are the near bandgap, zerophonon exciton transition lines A and B, and associated various acoustic and optical phonon replicas (Fig. 8.20). When the doping concentration is increased, neighboring nitrogen traps may interact with each other in pairs and form a new set of energy levels for their own bound excitons. At high nitrogen concentrations, as shown in Fig. 8.21, the interacting isoelectronic centers form a new set of energy levels such as NN1 , NN2 , and NN3 . At even higher concentrations, the NN lines dominate the absorption spectrum, and the A and B lines are absent. Since the binding energy of an exciton bound to paired isoelectronic centers depends on the distance between the two atoms of a pair, the potential well becomes deeper and the binding becomes much tighter by placing two nitrogens close together. Therefore, the strongest binding energy occurs for the nearest pairs, NN1 , which gives the lowest emission energy. The photoluminescence (PL) spectrum of a highly doped GaP sample with a nitrogen concentration of ~1019 cm−3 measured at 77 K is shown in Fig. 8.22. The A line emission is barely seen in the magnified (×170) plot, and the NN1 line and its associated phonon lines dominate the PL spectrum.
314
8 Optical Properties of Compound Semiconductor Heterostructures
Fig. 8.21 Fundamental absorption edge at 2 K of undoped GaP and of GaP doped with 7 × 1018 cm−3 nitrogen. Reprinted with permission from [13] copyright American Physical Society
Fig. 8.22 Lowtemperature (77 K) photoluminescence spectrum of a nitrogendoped GaP at a concentration of 1019 cm−3 . The inset shows a wider scan of 77 K PL spectrum. The A line and direct gap (E Γ ) transition are shown. [14]
8.3 Radiative Transition Between Discrete States
315
8.3 Radiative Transition Between Discrete States 8.3.1 Photon Density Distributions The interaction of light and freecarrier electrons in a semiconductor can take three different pathways—absorption, spontaneous emission, and stimulated emission (Fig. 8.23). The semiconductor will absorb photons (upward transitions) with energy equal to or greater than the bandgap energy. The photogenerated electrons will not stay in the conduction band forever. They will recombine with holes, on average, after one carrier lifetime span. For a direct bandgap semiconductor, this process will generate a spontaneous emission (downward transition) with a wavelength equal to the bandgap energy. If an optical excitation is applied to the semiconductor before the excited electrons in the conduction band reach their lifetime, the excited electrons can recombine with holes prematurely to generate photons in phase with the incident photons. This process is called stimulated emission. The rates of absorption, stimulated emission, and spontaneous emission are interrelated and can be described by Einstein’s relations. The externalexcitationgenerated photon emission and absorption are fundamentally connected through the photon density distribution, which describes the number of available photons participating in the interaction per unit energy/frequency (E = hv) and unit volume. Thus, it has a unit of (photon number/eVcm3 ). To calculate the photon density distribution P(E), we need to know the number of allowed photon states or the photon density of states Dp (E) and the probability that a photon will occupy that state determined by the photon distribution function np . (a) Photon density of states, Dp (E) The photon density of states can be derived similarly to the carrier density of states in a crystal. In a cubic enclosure with a dimension L ( λ) on each side, the allowed modes in terms of wave vector can be determined from the electromagnetic wave equation. The allowed wave vectors are
Fig. 8.23 Schematic of the absorption, spontaneous emission, and stimulated emission processes in a direct bandgap semiconductor
316
8 Optical Properties of Compound Semiconductor Heterostructures
ki = 2π m i /L
i = x, y, z
where mi = 0, ±1, ±2, ±3, … These discrete values (modes) of k x , k y , k z determine discrete values of allowed electric fields and photon energies. The particlelike nature of electromagnetic radiation is represented by photons with energy E = hν = ω = pc where ω = 2π v and the momentum of the photon is p = èk. The photon energy and momentum have the same forms as those of carriers in a crystal. The number of states in kspace is found from the volume in a thin spherical shell of 2 × (4π k 2 dk) divided by the unit volume, (2π /L)3 , which contains one allowed state. The factor of 2 counts for two different types of polarization, TE and TM modes, for a photon. The photon density of states within an interval of dk is the number of states per unit volume V = L 3 . dDp (k) =
k2 2 4π k 2 dk = dk L 3 (2π/L)3 π2
(8.60)
In a dielectric medium with a refractive index n, the wave vector is k=
2π 2π n E 2π = = λ c/(nν) c h
(8.61)
where v is the oscillation frequency. Then, for E = hv, dk =
2πn E dn 2π n ν dn 1+ dE = 1+ dν ch n dE c n dν
(8.62)
where the term in the parentheses is the refractive index dispersion and is unity for free space. The photon density of states within an energy interval dE becomes E dn 8π n 3 E 2 dDp (E) = 1+ dE h 3 c3 n dE
(8.63)
(b) Photon distribution function, np Since photons are indistinguishable, and identical particles do not follow Pauli’s exclusion principle, the average number of photons per state n p is given by the Bose–Einstein distribution law. −1 n p = exp(E/kT ) − 1
(8.64)
total photon density of states within an energy interval dE is given as dDp (E) × The np .
8.3 Radiative Transition Between Discrete States
317
(c) Photon density distributions, P(E) The photon density distribution is the number of photons per unit volume and per unit energy. Therefore, the photon distribution P(E) at a specific energy E is density obtained by dividing dDp (E) × n p with the energy interval dE.
E dn 1+
8π n 3 E 2 n dE photon number/eVcm3 P(E) = 3 3 h c exp(E/kT ) − 1
(8.65)
8.3.2 Einstein’s A and B Coefficients In semiconductors, the available electron states have a continuous band of states within the conduction and valence bands. This is in contrast to two sharp levels for an atomic system. To start, we assume the absorption of a photon of energy èω = E 21 ≥ E g results in an electron transition from a state E 1 in the valence band to a state E 2 within the conduction band as seen in Fig. 8.24. The transition rate between the two discrete states depends on (1) the probability that the upward transition can occur, B12 ; (2) the probability that the state E 1 contains an electron, f 1 ; (3) the probability that the state E 2 is empty, (1 − f 2 ); and (4) the density of photons of energy E 21 , P(E 21 ). Using similar parameters, we also describe the spontaneous emission and stimulated emission processes in the same semiconductor. The absorption, spontaneous emission, and stimulated emission processes are not isolated events but are interrelated through Einstein’s A and B coefficients. (a) Upward transition rate, r12 When absorb a photon with energy E 21 , the electron in the valence band can make an upward transition to an empty state within the conduction band. The transition Fig. 8.24 Absorption process in a semiconductor. An electron in the valence band at E 1 is excited into the conduction band at E 2 when excited with a photon of energy E 21 = E 2 − E 1 . The quasiFermi levels of the conduction and valence bands is F 2 and F 1 , respectively
318
8 Optical Properties of Compound Semiconductor Heterostructures
rate is given as r12 = B12 f 1 (1 − f 2 )P(E 21 )
(8.66)
where f 1 and f 2 are the Fermi–Dirac distribution functions. f1 = f2 =
1 1 + exp[(E 1 − F1 )/kT ] 1 1 + exp[(E 2 − F2 )/kT ]
(8.67a) (8.67b)
where F 1 and F 2 are the quasiFermi levels for the valence band and the conduction band, respectively. (b) Downward transition rate, r21 The absorbed photons can stimulate the emission of a similar photon by the transition of an electron from E 2 to E 1 . The downward transition rate for this process is r21 = B21 f 2 (1 − f 1 )P(E 21 )
(8.68)
where B21 is the downward transition probability. (c) Spontaneous emission rate, s21 The conduction band electrons can spontaneously return to E 1 without interaction with the radiation field, P(E 21 ). The transition probability for this process is represented by A21 , and the spontaneous emission rate is given by s21 = A21 f 2 (1 − f 1 )
(8.69)
At thermal equilibrium, the absorption rate equals the total emission rate r12 = r21 + s21
(8.70a)
F1 = F2
(8.70b)
and
This leads to P(E) =
2 8π n 3 E 21 A21 f 2 (1 − f 1 ) = 3 3 B12 f 1 (1 − f 2 ) − B21 f 2 (1 − f 1 ) h c exp(E 21 /kT ) − 1
It can be rewritten as
(8.71)
8.3 Radiative Transition Between Discrete States
319
2 A21 8π n 3 E 21 = 3 3 B12 exp(E 21 /kT ) − B21 h c exp(E 21 /kT ) − 1
or A21 exp(E 21 /kT ) − A21 =
2 8π n 3 E 21 B12 exp(E 21 /kT ) − B21 3 3 h c
Equating the temperature independent terms gives A21 =
2 8π n 3 E 21 B21 h 3 c3
(8.72)
Then, equating the temperature dependent terms with A21 given above gives B21 = B12
(8.73)
Equations (8.72) and (8.73) represent the Einstein’s A and B coefficients. They indicate that the spontaneous emission rate is related to the absorption rate and the stimulated emission rate.
8.3.3 Absorption and Stimulated Emission (a) Necessary conditions for stimulated emission in semiconductors The necessary conditions for stimulated emission simply require that the photoninduced downward radiative transition rate exceed the upward photon absorption rate, r 21 > r 12 : B21 f 2 (1 − f 1 )P(E 21 ) > B12 f 1 (1 − f 2 )P(E 21 )
(8.74)
Since B21 = B12 , this condition becomes f 2 (1 − f 1 ) > f 1 (1 − f 2 ) or f 2 > f 1
(8.75)
In other words, this is the condition required for population inversion. It further reduces to exp[(F2 − F1 )/kT ] > exp[(E 2 − E 1 )/kT ]
(8.76a)
F2 − F1 > E 2 − E 1
(8.76b)
or
320
8 Optical Properties of Compound Semiconductor Heterostructures
The condition states that in order for the downward stimulated emission rate to exceed the upward absorption rate, the separation of the quasiFermi levels must exceed the photon emission energy. (b) Relation of net stimulated emission rate to the absorption coefficient The interaction of electrons and photons in the solid can be related to the absorption coefficient, α(E 21 ) (cm−1 ). The net absorption rate R(abs) (photon number/eVcm3 s) is the difference between the upward transition rate r 12 and the downward transition rate r 21 . The net absorption rate is also equal to the absorption coefficient times the photon flux, ϕ(E 21 ) = P(E 21 )υ g . R(abs) = r12 − r21 = B12 ( f 1 − f 2 )P(E 21 ) = α(E 21 )P(E 21 )υg
(8.77)
where υ g is the group velocity. In the dielectric medium, the group velocity is expressed as υg =
2π dE c/n dω ∼ c = = = dk h dk 1 + (E/n)(dn/dE) n
(8.78)
Therefore, the absorption coefficient may be written as α(E 21 ) =
B12 ( f 1 − f 2 ) R(abs) = P(E 21 )υg c/n
(8.79)
The numerator of (8.79) is related to the net stimulated emission rate, R(st). The net stimulated emission rate is the difference between the downward transition (stimulated emission) rate r 21 and the upward transition (absorption) rate r 12 . R(st) = r21 − r12 = B12 ( f 2 − f 1 )P(E 21 )
(8.80)
Using the Einstein’s relations and the photon density distribution, this relation reduces to R(st) =
rstim (E 21 ) A21 ( f 2 − f 1 ) = exp(E 21 /kT ) − 1 exp(E 21 /kT ) − 1
(8.81)
Here we defined r stim (E 21 ) ≡ A21 (f 2 – f 1 ) as the stimulated emission rate because of its similarity in form to the spontaneous emission rate in (8.69). The number of photons per state is represented by the term n p = 1/[exp(E 21 /kT ) − 1]. The constant A21 may be replaced by B21 through Einstein’s relation, and the stimulated emission rate is given as rstim (E 21 ) =
2 8π n 3 E 21 B12 ( f 2 − f 1 ) h 3 c3
(8.82)
8.3 Radiative Transition Between Discrete States
321
The stimulated emission rate and the absorption coefficient (8.79) are different by a constant. 2 8π n 2 E 21 α(E 21 ) rstim (E 21 ) = − h 3 c2
(8.83)
The absorption coefficient is measurable and may be used to derive the stimulated emission rate. (c) Relation of spontaneous emission rate to the absorption coefficient The spontaneous emission rate may also relate to the absorption coefficient. It has been defined earlier as s21 = A21 f 2 (1 − f 1 ) ≡ rsp (E 21 )
(8.69)
Using (8.72) and (8.79), we may express s21 in terms of α(E 21 ) given as rsp (E 21 ) =
2 8π n 2 E 21 f 2 (1 − f 1 ) α(E 21 ) h 3 c2 ( f1 − f2 )
(8.84)
Solving for the Fermi–Dirac functions, f 1 and f 2 , we have rsp (E 21 ) =
2 α(E 21 ) 8π n 2 E 21 h 3 c2 exp{[E 21 − (F2 − F1 )]/kT } − 1
(8.85)
Therefore, the spontaneous emission rate is also related to the absorption coefficient. We can also relate the spontaneous emission rate to the stimulated emission rate as rstim (E 21 ) = rsp (E 21 ){1 − exp{[E 21 − (F2 − F1 )]/kT }}
(8.86)
The spontaneous emission rate, the stimulated emission rate, and the absorption coefficient are all interrelated. The spontaneous and stimulated emission rates can be determined from experimentally measured absorption coefficients. (d) Transition probability, B12 Since both r stim (E 21 ) and r sp (E 21 ) are related to the absorption coefficient, it is only necessary to determine α(E 21 ) to obtain the net spontaneous and stimulated emission rates. Also, calculated values of α(E 21 ) may readily be verified by experimental measurements. Therefore, α(E 21 ) becomes the most important parameter to be considered in the analysis of light emission processes. For photon absorption between two discrete levels, the absorption coefficient was derived as n B12 ( f 1 − f 2 ) α(E 21 ) = c
(8.79)
322
8 Optical Properties of Compound Semiconductor Heterostructures
In this equation, the transition probability B12 is unknown and relates the interaction of electrons in the solid with electromagnetic radiation. Using quantum mechanical techniques of timedependent perturbation theory, the transition probability between a single initial state 1 and a single final state 2 is given as:
B12
2 π ∗ I 3 = 1 (r, t)H 2 (r, t)d r 2
(8.87)
V
In this equation, r is the threedimensional spatial vector, ∗1 (r, t) the complex conjugate of the wave function of the initial state, H I the interaction Hamiltonian, and 2 (r, t) the wave function of the final state. In the case of the transition from a continuum of state 1 to a continuum of states 2, the transition probability takes a form of B12 =
2π H12 2 δ(E 2 − E 1 − ω)
(8.88)
and H12 =
1∗ (r, t)H I 2 (r, t)d 3 r
(8.89)
V
This is called Fermi’s Golden Rule. The delta function is used to specify that the energy separation between the two states equals èω. In either case, the transition probability is proportional to a transition matrix M T 2 , which is a function of the bandgap energy and the conduction band effective mass of the semiconductor. The transition probability B also can be evaluated by the method of van Roosbroeck and Shockley, using experimentally determined values of the absorption coefficient [15]. The van Roosbroeck and Shockley relation is that at equilibrium, the optical generation rate of electron–hole pairs is equal to the rate of radiative recombination. This relation has already been described by (8.85), which shows the fundamental relation between the emission spectrum and the observed absorption spectrum. One can also relate the rate of radiative recombination R0 , under equilibrium condition, by the product of the electron density in the upper state n0 , the hole density in the lower state p0 , and the transition probability B as R0 = n 0 p0 B.
(8.90)
The total radiative recombination rate under nonequilibrium conditions becomes R=
np R0 n 2i
(8.91)
8.3 Radiative Transition Between Discrete States
323
This equation implies that the recombination rate increases with increasing carrier concentration, and that R reduces to R0 when the product np approaches the equilibrium intrinsic value n 0 p0 = n 2i . Under nonequilibrium conditions, where the carrier concentration deviates from its equilibrium concentration n0 (or p0 ) by a small amount n = p, then n = n0 + n and p = p0 + p, the recombination rate becomes (n 0 + n)( p0 + p) R0 n 0 p0 n 0 p0 + n 0 p + p0 n + np = R0 n 0 p0
R = R0 + R =
(8.92)
Neglecting the very small term np from the above equation, R ∼ n p + = R0 n0 p0
(8.93)
Assuming n = p, the radiative lifetime of excess carriers is obtained as τ=
1 n 0 p0 n = R R 0 n 0 + p0
(8.94)
For an intrinsic material, n0 = p0 = ni , τ=
ni 1 = 2R0 2n i B
(8.95)
Through this equation, one can relate the transition probability to the measured carrier lifetime. For direct bandgap semiconductors, e.g., GaAs and InP, in which recombination occurs by a direct radiative transition, B ~ 10−10 cm3 /s. For indirect bandgap semiconductors such as Si, Ge, and GaP, the transition probability is smaller by a factor of 103 –104 , a quantity that may vary considerably from one material to another, being dependent upon the nature of the energy band structure. The large difference in transition probability between direct and indirect bandgap materials is also reflected in the shape of measured absorption coefficient curves shown in Fig. 8.10, where steep rise of the absorption coefficient at the bandgap energy is seen in direct bandgap semiconductors. Due to the low transition probability of the indirect material, the absorption coefficient increases slowly for energies near the bandgap energy.
324
8 Optical Properties of Compound Semiconductor Heterostructures
8.4 Optical Transitions Between Energy Bands 8.4.1 Direct and Indirect Bandgaps For efficient optical transitions between the conduction band minimum (E c,min ) and the valence band maximum (E v,max ), the energy conservation and momentum conservation conditions have to be observed.
Momentum conservation: ki ∼ = kf (8.96) Energy conservation: E i − E f = hν where ν is the frequency of the optical radiation, and subscripts i and f represent the initial and final states of the transition, respectively. As illustrated in Fig. 8.25, the momentum conservation condition requires the wave vectors of the initial (k i ) and the final (k f ) states to be the same as seen in a direct bandgap semiconductor, where both E c,min and E v,max are located at k = 0. To fulfill the second condition for energy conservation, the electron–hole recombination generated excess energy must be released by emitting a photon with the equivalent energy. Since the photon has a negligibly small momentum, the momentum conservation condition still holds. Therefore, light emission is possible from a direct bandgap semiconductor with an emission wavelength λ(μm) =
1.2398 1.2398 = Ei − E f E g (eV)
(8.97)
For indirect semiconductors, the momentum associated with photon emission is too small to balance the large difference in momentum change between the initial
Fig. 8.25 Energy band diagrams and optical emission processes of a direct and b indirect semiconductors. The dashed lines indicate nonradiative transitions
8.4 Optical Transitions Between Energy Bands
325
and the final states; therefore, phonon emission is required to fulfill the momentum conservation requirement. The process is given by hve = E i − E f − E p , where E p is the phonon energy. Therefore, efficient light emission from indirect bandgap material is not allowed.
8.4.2 BandtoBand Transitions in Bulk Semiconductors For bandtoband transitions in a semiconductor, as shown in Fig. 8.26, we must consider all participating states in both the conduction and valence bands separated by the photon energy èω. The number of states involved is determined by the density of states Di (E) and the occupation probability f i . For example, the upward transition rate depends on the density of filled states in the valence band, Dv (E)f v , and the density of empty states in the conduction band Dc (E)(1 − f c ). Thus, the absorption coefficient in a semiconductor is the sum of the absorption coefficients at èω for all of the energy levels separated by èω. It is given by ∞ α(ω) = −∞
B12 ( f 1 − f 2 )Dv (E v − E)Dc (E − E c )dE c/n
(8.98)
and πq 2 α(ω) = 0 m 2 cn E
∞
Dv E
Dc E MT 2 f v E
− f c E d E
(8.99)
−∞
Fig. 8.26 Bandtoband optical absorption in a semiconductor. The right panel shows the Ek curves
326
8 Optical Properties of Compound Semiconductor Heterostructures
Here, E’ describes the conduction band edge with E’ = 0 at E c , and E” = E’+E g − èω for the valence band. The transition probability between two single states 1 and 2 is related to the transition matrix element as B12 =
πq 2 MT 2 2 n ω 0
m2
(8.100)
We also obtain the stimulated emission rate from the absorption coefficient shown here: 4π nq 2 E rstim (E) = 0 m 2 c 3 h 2
∞
Dv E
Dc E MT 2 f c E − f v E
d E
(8.101)
−∞
The problem of evaluating α(E) and r stim (E) becomes one of evaluating Dc (E), Dv (E), and M T 2 . Under high injection carrier densities or for high doping levels, such as in injection lasers, the density of states becomes concentration dependent and cannot be represented by the simple parabolic expression. The matrix element for transitions between band tail states in heavily doped semiconductors also differs from that involving free electron and free hole states. Fortunately, since the absorption coefficient is measurable for all energy ranges, we can fit (8.99) using the experimental results. Parameters used to fit experimental α(E) can be applied to evaluate r stim (E). Figure 8.27 is an example of using experimental absorption coefficient results to predict the photoluminescence spectrum of a heavily doped ptype GaAs (1.2 × 1018 cm−3 ). Indeed, it shows that the absorption coefficient is closely related to the spontaneous and stimulated emission processes.
8.4.3 Fermi–Dirac Inversion Factor, Transparency, and Gain The intrinsic absorption coefficient for allowed directtransition in a semiconductor, whose valence band is completely full, where f v (E) = 1, and whose conduction band is completely empty, where f c (E) = 0, was given as α0 (hν) = A∗ hν − E g
(8.44)
q 2 (2m r )3/2 MT 2 2π m 20 cn0 2 (ω) The constant A* was derived by John Bardeen in 1952. This equation applies to the situation where a lowlevel excitation is used such that the conduction band is almost empty and f c (E) = 0 is fulfilled. In contrast, semiconductors under strong excitations have partially filled parabolic conduction and valence bands, and there is stimulated emission allowed in addition and A∗ =
8.4 Optical Transitions Between Energy Bands
327
Fig. 8.27 a Experimental absorption coefficient of a ptype GaAs measured at room temperature. b Measured room temperature photoluminescence spectrum compared with the calculated stimulated emission rate using results in (a). Reprinted with permission from [16] copyright AIP Publishing
328
8 Optical Properties of Compound Semiconductor Heterostructures
Fig. 8.28 Optical transition between the conduction and valence bands and related Fermi–Dirac distributions
to absorption. Under this circumstance, (8.99) has to be used to include the term (f v − f c ) in the calculation of the absorption coefficient and is related to the intrinsic absorption coefficient as α(ω) = α0 (ω)[ f v (k) − f c (k)]
(8.102)
The quantity [f v (k) − f c (k)] is called the Fermi–Dirac inversion factor. Figure 8.28 shows the schematic of the optical transition of èω between the valence band and the conduction band. The corresponding Fermi–Dirac functions f v (k) and f c (k) are also shown. For f v (k) < f c (k), one finds negative absorption, i.e., the gain coefficient. g(ω) = −α(ω)
(8.103)
The condition of f v (k) − f c (k) < 0 satisfies the population inversion condition as shown here: f v (k) − f c (k) =
exp[(E c − Fc )/kT ] − exp[(E v − Fv )/kT ] E c − E v
(8.106)
where F c and F v are quasiFermi levels. The minimum of (8.106) determines a transparency condition where (F c − F v ) equals E g . Above transparency, the semiconductor laser starts to produce gain, or negative absorption, which is essential for the lasing action. In the following, we will evaluate the occupation probabilities in terms of the material parameters and excitation levels. Assuming a parabolic bandedge configuration in both conduction and valence bands, E c (k) and E v (k) are expressed as Ec = Eg +
2 k 2 2m ∗e
(8.107a)
and Ev = −
2 k 2 2m ∗h
(8.107b)
Here we assumed E = 0 at the valence band maximum. For direct transitions, k = 0, and the energy involved is expressed as E = ω − E g =
2 k 2 2 k 2 2 k 2 + = ∗ 2m ∗e 2m h 2m r
(8.108)
Thus, Ec = Eg +
2 k 2 m r mr = E E + g ∗ 2m r m e m ∗e
(8.109a)
and Ev =
mr E m ∗h
(8.109b)
These bandedge energies are used to express f c (E) and f v (E) in terms of effective masses and quasiFermi levels as f c (E) =
1 1
= 1 + exp[(E c − Fc )/kT ] 1 + exp E g + m r /m ∗e E − Fc /kT (8.110a)
330
8 Optical Properties of Compound Semiconductor Heterostructures
Fig. 8.29 a Gainabsorption curve as a function of energy. The dashed line is the intrinsic absorption curve. The Fermi–Dirac inversion factor is also plotted. b Gain curves of an InGaAsP laser under different injected carrier density conditions. The system reaches the transparency condition, f v ≤ f c , at an injected density of ≥1 × 1018 cm−1 . Reprinted with permission from [17] copyright AIP Publishing
f v (E) =
1 1 + exp[(E v − Fv )/kT ]
=
1
1 + exp − m r /m ∗h E − Fv /kT (8.110b)
Once the quasiFermi levels are determined from the injected carrier densities, both f c (E) and f v (E) can be solved as functions of E. Then, the gain (−α) of a specific energy (èω) is determined by multiplying the inversion factor by the intrinsic absorption coefficient, as shown in Fig. 8.29. As the quasiFermi level separation (F c − F v ) increases with increasing carrier injection level, the peak of the gain curve grows quickly. In a properly designed cavity, once the peak gain value surpasses the total loss of the cavity, the lasing action starts.
8.4.4 Optical Absorption and Gain in Quantum Wells The procedures of calculating gain curves in bulk semiconductors are applicable to quantumwell materials with two important modifications. First, the 2D system of quantum well has a steplike DOS profile, which should be included in the absorption coefficient calculation. The other major difference is the restrictions on allowed
8.4 Optical Transitions Between Energy Bands
331
optical transitions. In bulk semiconductors, all vertical transitions between valence and conduction bands are allowed as long as k = 0. The optical transition in quantum wells has to follow the quantum mechanical ‘selection rule’ such that the quantum numbers of the initial and final states are the same, ni − nf = n = 0. For example (Fig. 8.30), from n = 1 heavyhole (HH) state in the valence band, only the transition to n = 1 electron state in the conduction band is allowed. All other transitions are prohibited, since n = 0. The intrinsic absorption coefficient of a multiple quantumwell system has the form of mr Nw Θ(ω − E mn ) (8.111) α02D (ω) ∝ 2 π L m,n where L is the width of each quantum well, N w is the total number of quantum wells, and is the Heaviside step function. Figure 8.31 shows the experimental absorption spectrum of an undoped InGaAs/InAlAs, quantum well measured at 12, 100, and 300 K. The steplike features are clearly illustrated with pronounced exciton peaks near each step edge. Due to the strong binding energy, the excitonrelated peaks are visible in the absorption spectrum even at room temperature. Another interesting feature is the observation of both HH and LH related excitons near the absorption step edges. In bulk semiconductors, due to the degeneracy of the HH and LH bands near the zone center, only a single exciton peak will be observed in the lowtemperature absorption spectrum (Fig. 8.16). However, in a quantum well, the subbands of the heavy and light holes at the zone center are no longer degenerate and show two separate exciton peaks associated with the HH and LH bands, respectively. Once we have determined the intrinsic absorption coefficient, the absorption in a quantum well can be calculated as α(ω) = α02D (ω)[ f v (E) − f c (E)] E
n=1 Eg n=2 HH LH Fig. 8.30 Density of states and direct electronic transitions in a quantum well
(8.112)
332
8 Optical Properties of Compound Semiconductor Heterostructures
Fig. 8.31 Absorption spectra of an InGaAs/InAlAs quantum well measured at various temperatures. Reprinted with permission from [18] copyright IEEE
The construction of the absorption curve in a quantum well is illustrated in Fig. 8.32a. Because of the steplike feature of the intrinsic absorption coefficient, the ideal absorption/gain curve also contains sharp step edges. However, the intraband carrier relaxation due to scattering within the quantum well can cause the broadening of the energy states and, thus, spectral broadening (Fig. 8.32b). The relaxation process is characterized by τ in , the intraband relaxation time of ee or hh interaction, or the reciprocal scattering probability. The energy peak broadening due to intraband scattering, δE in , is related to τ in using the uncertainty principle, δE in = è/τ in . In the ideal relaxationfree case, τ in → ∞. For GaAs, a short intraband relaxation time of 0.1 ps is typically used. Therefore, deformation and reduction of the peak values take place in the gain spectrum. The spectral shape becomes smooth and broad in spite of the sharp steplike DOS.
8.5 Nonradiative Auger Recombination Processes Electrons and holes in a direct bandgap semiconductor can also recombine nonradiatively. Nonradiative mechanisms include recombination at defects, surface recombination, and Auger recombination, among others. For longwavelength semiconductor lasers with a narrow gap, however, the Auger process is generally the predominant nonradiative mechanism. The Auger recombination process involves three particles (two electrons and one hole, or one electron and two holes) and four states as described below. In this process, the energy released during the bandtoband electron–hole recombination is transferred to another electron (or hole) which gets excited to a highenergy state
8.5 Nonradiative Auger Recombination Processes
333
Fig. 8.32 a Gainabsorption curve as a function of energy in a quantum well. The staircase line is the intrinsic absorption curve. The Fermi–Dirac inversion factor is also plotted. b Gain curve of an ideal relaxationfree quantum well has sharp steps. When a short relaxation time of 0.1 ps is incorporated, the gain curve becomes smooth without sharp edges
in the band. This electron or hole then relaxes back to achieve thermal equilibrium by losing its energy to lattice vibrations or phonons. Thus, the Auger process is a nonradiative recombination process. Since there are three particles involved, the Auger recombination rate RA may be approximately written as RA = Cn 3
(8.113)
where n is the injected carrier density in an undoped semiconductor. It is useful to define the carrier lifetime τ A for the Auger process as
334
8 Optical Properties of Compound Semiconductor Heterostructures
τA = n/RA = 1/ Cn 2
(8.114)
The quantity C is called the Auger coefficient. The inversesquare dependence of carrier lifetime on carrier density is used to identify the Auger effect experimentally. In general, bandtoband Auger processes are characterized by a strong temperature dependence and bandgap energy dependence following 3/2
exp −E g /kT . The Auger rate increases rapidly either for high temperkT /E g atures or for narrow bandgap materials. In narrow bandgap semiconductors such as InAs and GaSb, where E g ≈ so , Auger process should be strongly temperature dependent. For example, in an InGaAsP laser (~1.3 μm), the bandtoband Auger process dominates for temperatures exceeding T = 160 K. In large bandgap materials, the Auger process depends on the doping level and become significant in degenerated semiconductors. These dependencies arise from the laws of energy and momentum conservation that the four free particle states involved must satisfy. The energy taken by the third particle in Auger recombination is on the order of the bandgap, which corresponds to a large momentum close to 2m E g . Conservation of momentum requires that the threeparticle system must have large momentum before the interaction can take place, or a threshold energy E T for the processes. The bandtoband Auger processes in a directgap semiconductor are shown in Fig. 8.33. The three processes are labeled CHCC, CHLH, and CHHS where C stands for the conduction band and H, L, and S stand for heavyhole, lighthole, and splitoff valence bands, respectively. For example, the CHCC process involves two electrons and one hole and is dominant in ntype material. In this process, electron 1 (of energy E 1 ) makes a transition to empty state 1 (of energy E 1 ) and the excess energy
Fig. 8.33 Three types of bandtoband Auger processes. Electrons and holes are represented by closed circles and open circles, respectively
8.5 Nonradiative Auger Recombination Processes
335
is transferred to electron 2 (of energy E 2 ), which is excited to state 2 (energy E 2 ). Electron 2 loses its energy to optical phonons when it relaxes back to thermal equilibrium. On the other hand, CHHS and CHLH Auger processes are dominant in ptype semiconductors. The CHHS process involves one electron, one heavy hole, and a splitoffband hole. CHLH is similar to CHHS except that it involves a light hole. Under highinjection conditions commonly present in semiconductor lasers, all three mechanisms must be considered. Problems 1. (a) The direct allowed transition in a direct bandgap semiconductor is described by a general equation of α(hν) = A∗ hν − E g . The proportional constant A* can be expressed as a function of effective masses. 3/2
q 2 2m ∗e m ∗hh / m ∗e + m ∗hh A ≡ nch 2 m ∗e ∗
where n is the index of refraction and c is the speed of light. Calculate A* for GaAs. (b) Using the absorption spectra shown in Fig. 8.12b, calculate the phonon energy near room temperature (291 K) in a highpurity Si crystal. (c) Using the absorption spectrum shown in Fig. 8.16, calculate the bandgap energy of GaAs at 186 K. 2. The active region of an nAl0.3 Ga0.7 As/GaAs/pAl0.3 Ga0.7 As doubleheterostructure (DH) diode laser has a 0.1 μm thick undoped GaAs active region. Under a forward bias, electrons and holes are injected into the GaAs active region from n and psides of the DH structure, respectively. The increasing carrier concentration causes the quasiFermi level of electrons and holes to move toward the conduction band and valence band, respectively. Under the strong carrier injection, the transparency condition is reached when the separation in quasiFermi levels (F c − F v ) = E g . (a) Find the transparency carrier density ntr for GaAs under the condition of equal injection of both types of carriers (n = p). You have to use Fermi–Dirac integral for both electrons and holes. (b) Plot the normalized gain, gn = α(ω)/α0 (ω), or Fermi–Dirac inversion factor (f v – f c ) as a function of energy between 1.3 and 1.6 eV at injection concentrations (n = p) of n0 = 1 × 1018 , 2 × 1018 , 4 × 1018 , and 6 × 1018 cm−3 . Note that the Fermi integral is required to determine quasiFermi levels of the active region. (c) Plot the gain as a function of energy between 1.3 and 1.6 eV at injection concentrations (n = p) similar to those listed in Part (b). Identify the injection concentration(s) for which the transparency condition has not been reached. (d) If the GaAs active region of the same DH laser is heavily doped, calculate the transparency condition by considering only electron injection with hole
336
8 Optical Properties of Compound Semiconductor Heterostructures
density fixed at the doping level of 6 × 1018 cm−3 . Plot the gain curve for injected electron density at 1.5× the transparency condition. Comment on whether this approach is advantageous over the structure with an undoped active region. (e) Plot the equilibrium energy band diagram of the DH structure using SimWindows. Both the doping concentration and thickness of the n and pdoped AlGaAs are at the same level of 1018 cm−3 and 1000 nm, respectively. 3. For erbiumdoped fiber communication application, a 0.98 μm diode laser is used as the pumping source. The active region of the laser has a GaAsGa0.8 In0.2 AsGaAs strained quantum well. The bandgap energy of Gax In1−x As is expressed as E g () = 0.358 + 0.589x + 0.477x 2 (a) Find the transparency carrier density ntr for Ga0.8 In0.2 As under the condition of neutral carrier injection (n = p). You have to use the Fermi–Dirac integral for both electrons and holes. Both the electron and hole effective masses of GaInAs vary linearly between GaAs and InAs. (b) Plot the intrinsic absorption coefficient as a function of energy for the undoped Ga0.8 In0.2 As up to 1.4 eV using α0 (ω) = 104 ω − E g . (c) Plot the normalized gain, gn = α(ω)/α0 (ω), or Fermi–Dirac inversion factor (f v − f c ), as a function of energy between 1 and 1.4 eV at injection concentrations (n = p) of n0 = 5 × 1017 , 1.5 × 1018 , and 5 × 1018 cm−3 . (d) Under steadystate conditions, the current density of a laser diode for carrier neutral injection (n = p) is J ≈ qL z R(n), where L z is the thickness of the undoped active region and R(n) = Br n2 . Plot the normalized gain versus (J/J 0 ) = (n/ntr )2 for L z = 100 Å. J 0 is the transparency current density where n = ntr . (e) Evaluate J 0 for Br = 1.5 × 10−10 cm3 /s.
References 1. M. Fox, Optical Properties of Solids (Oxford, 2001), p. 32 2. S. Adachi, J. Appl. Phys. 53, 5863 (1982) 3. S. Adachi, J. Appl. Phys. 58, R1 (1985); or H. C. Casey Jr., D.D. Sell, M.B. Panish, Appl. Phys. Lett. 24, 63 (1974) 4. G.M. Laws, E.C. Larkins, I. Harrison, C. Molloy, D. Somerford, J. Appl. Phys. 89, 1108 (2001) 5. D. Brunner et al., J. Appl. Phys. 82, 5090 (1997) 6. U. Tisch, B. Meyler, O. Katz, E. Finkman, J. Salzman, J. Appl. Phys. 89, 2676 (2001) 7. G.E. Stillman, V.M. Robbins, N. Tabatabaie, IEEE Trans. Electron Devices 31, 1643 (1984) 8. G.G. MacFarlane, T.P. McLean, J.E. Quarrington, V. Roberts, Phys. Rev. 111, 1245 (1958) 9. H.C. Casey Jr., D.D. Sell, K.W. Wecht, J. Appl. Phys. 46, 250 (1975) 10. M.D. Sturge, Phys. Rev. 127, 768 (1962) 11. P.J. Dean, D.G. Thomas, Phys. Rev. 150, 690 (1966)
References
337
12. R. Dingle, W. Wiegmann, C.H. Henry, Phys. Rev. Lett. 33, 827 (1974) 13. J.J. Hopfield, P.J. Dean, D.G. Thomas, Phys. Rev. 158, 748 (1967) 14. J.N. Baillargeon, Gas Source Molecular Beam Epitaxy of Aluminum Gallium Indium Phosphide for Visible Spectrum Light Emitting Diode. Ph.D. thesis, University of Illinois at UrbanaChampaign, 1990 15. W. van Roosbroeck, W. Shockley, Phys. Rev. 94, 1558 (1954) 16. H.C. Casey Jr., F. Stern, J. Appl. Phys. 47, 631 (1976) 17. N.K. Dutta, J. Appl. Phys. 51, 6095 (1981) 18. G. Livescu, D.B.A. Miller, D.S. Chemla, M. Ramaswamy, T.Y. Chang, N. Sauer, A.C. Gossard, J.H. English, IEEE Quantum Electron. 24, 1677 (1988)
Further Reading 1. H.C. Casey, M.B. Panish, Heterostructure Lasers: Part A, Fundamental Principles (Academic Press, 1978) 2. S. Wang, Fundamentals of Semiconductor Theory and Device Physics (PrenticeHall, 1989) 3. J.I. Pankove, Optical Processes in Semiconductors (PrenticeHall, 1971) 4. M. Fox, Optical Properties of Solids (Oxford, 2001) 5. N.K. Dutta, R.J. Nelson, J. Appl. Phys. 53, 74 (1982)
Chapter 9
Heterostructure Electronic Devices
Abstract Compound semiconductors are excellent candidates for highspeed device applications due to their high electron mobility, the ability to form heterostructures, and the availability of semiinsulating substrates. However, the multicomponent nature and the lack of robust native oxides make the fabrication of compound semiconductorbased metaloxidesemiconductor fieldeffect transistors (MOSFETs) an extremely difficult task. Instead, GaAsbased metal–semiconductor fieldeffect transistors (MESFET) were developed initially. A MESFET utilizes a metal–semiconductor Schottky barrier to replace the MOS gate structure. The charge carriers in the active region (channel) are separated spatially from the control (gate) electrode by a depletion layer formed on the semiconductor surface. Nevertheless, due to the nature of the Schottky barrier and high electron mobility, only nchannel MESFETs were studied and the devices are leaky at high positive biases. With the advancements of epitaxial growth technology and new device concepts, efficient advanced devices were developed. Among many threeterminal device structures, the modulationdoped fieldeffect transistor (MODFET), or highelectronmobility transistor (HEMT), and the heterojunction bipolar transistor (HBT) are the most widely used highspeed devices. In this chapter, after a brief review of the MESFET, the development and working principles of HEMTs and HBTs are discussed in great detail. Then the key concepts of achieving an oxidesemiconductor interface with low interface state density necessary for the fabrication of high performance III–V MOSFETs are discussed.
The HEMT is a voltagecontrolled majority carrier device. It shares the same device geometry as the MESFET except for the details of the active region. The control electrode (gate) is coupled to the active region of the device through a capacitor. The conduction carriers, in the form of the twodimensional electron gas (2DEG), in the active region are generated by modulation doping at the heterostructure interface. The structure of the HBT is similar to that of the homostructure bipolar junction transistor (BJT), with the emitter–base junction replaced by a heterojunction. With properly designed heterojunctions, the device parameters such as doping level and layer thickness can be individually optimized for highspeed and highgain operations. The HBT is a currentcontrolled minority carrier device with the charged © Springer Nature Switzerland AG 2020 K. Y. Cheng, III–V Compound Semiconductors and Devices, Graduate Texts in Physics, https://doi.org/10.1007/9783030519032_9
339
340
9 Heterostructure Electronic Devices
Table 9.1 Comparison of BJT and FET Carriers
Transport
Output control
Input impedance
BJT
Minority
Diffusion
Base current
Low
FET
Majority
Drift
Gate voltage
High
carriers being separated energetically by the energy barriers. The control electrode (base) is resistively coupled to the active device region. The major device attributes of FETs and BJTs are compared in Table 9.1. In late 1990, the inversionmode GaAs MOSFET with a low interface trap density was finally achieved using in situ electron beam evaporated Ga2 O3 (Gd2 O3 ) dielectric film on MBE GaAs. Next, using ex situ atomic layer deposited highκ Al2 O3 and HfO2 films as the gate dielectric, similar devices were demonstrated on GaAs and other III–V materials. Further refinement of oxide deposition methods and development of additional highκ gate dielectrics were exploited in the following two decades. At the moment, III–V MOSFET manufacturing technologies are still under development.
9.1 Metal–Semiconductor FieldEffect Transistors (MESFETs) 9.1.1 Basic Operation Principles As a prelude to the HEMT, the device characteristics of the MESFET are discussed first. The operating principle of the MESFET is identical to that of a junction FET, and its structure is also similar except that the p–n junction is replaced by the Schottky barrier. Most MESFETs use ntype III–V compound semiconductors for the conduction channel because of their high electron mobility and large Schottky barrier height. To minimize the parasitic capacitance, semiinsulating substrates are usually used. A schematic diagram of the MESFET is shown in Fig. 9.1. The active region of the device has a conduction channel thickness a, a gate length L, and a gate width Z. The depletion region has a nonuniform thickness of W (x) along the channel under a large drain bias voltage. Under normal operation, the source is grounded, the gate is reversebiased to modulate the conduction channel, and the drain contact is biased at a proper voltage to collect majority carriers. The effect of the applied drain voltage, V D , with the gate open, on the current–voltage relationship is investigated first. When a small positive V D is applied with V GS = 0, the channel of the MESFET is essentially a uniform resistor with a crosssectional area determined by the width of the device (Z) and the nondepleted channel thickness (a − W ). The channel current I D is a linear function
9.1 Metal–Semiconductor FieldEffect Transistors (MESFETs)
341
Fig. 9.1 Schematic structure and dimension of a metal–semiconductor FET. The shaded region is the depletion region under the gate electrode
Fig. 9.2 General form of the current–voltage characteristics of a MESFET. The pinchoff point defines the saturation drain voltage, V D (sat)
of the drain voltage as shown in Fig. 9.2. The depletion width along the conduction channel has a constant value of 2 V0 (9.1) W = q Nd where V 0 is the contact potential of the Schottky barrier gate, N d is the carrier concentration of the channel, and is the permittivity of the semiconductor. When a moderate V D of a few tenths of a volt is applied with V GS = 0, the V D simultaneously reverse biases the gate–drain metal–semiconductor junction and widens the depletion region near the drain contact. The depletion region width increases along the conduction channel from source to drain. The depletion width closest to the drain contact becomes 2 (9.2) W = (V0 + VD ) q Nd
342
9 Heterostructure Electronic Devices
The narrowing of the conduction channel leads to an increased channel resistance. The increasing of channel current I D deviates from the linear relationship with increasing V D . Continuing to increase V D causes an everincreasing depletion of the channel. Eventually, the conduction channel vanishes near the drain contact, where the depletion width approaches the channel width for V GS = 0. W =
2 [V0 + VD (sat)] = a q Nd
(9.3)
The drain voltage V D becomes the saturation drain voltage V D (sat) and can be represented as VD (sat) =
qa 2 Nd − V0 2
(9.4)
At the saturation voltage and beyond, the drain current becomes saturated, I D (sat) and does not increase with V D . Next, we will investigate the gate bias effect. When the gatetochannel junction of a MESFET is reversebiased, the depletion width gets wider, and V D (sat) will decrease. VD (sat) =
qa 2 Nd − V0 + VGS 2
(9.5)
Since V GS is negative for reverse bias of the gate–channel junction, V D (sat) is decreased as shown in Fig. 9.3. The depletion width W eventually will reach across the channel thickness a when the gate reverse bias is further increased. The gate voltage at which the conduction channel is pinched off when V D = 0 is called the threshold voltage V T . For a gate bias of V GS and V D = 0, the depletion width is expressed as Fig. 9.3 Modification of current–voltage characteristics for V G < 0
ID VGS = 0 VGS < 0
ID(sat)
0
VD(sat)
VD
9.1 Metal–Semiconductor FieldEffect Transistors (MESFETs)
343
2 (V0 − VGS ) q Nd
W =
(9.6)
At the threshold voltage V GS = V T , W = a. This leads to a2 =
2 (V0 − VT ) q Nd
VT = V0 −
qa 2 Nd = V0 − V P 2
(9.7)
(9.8)
We define V P as the pinchoff voltage, which is the potential across the depletion region at the threshold condition (W = a). VP =
qa 2 Nd 2
(9.9)
The depletion width in a MESFET with V GS = 0 can be either greater than or less than the channel thickness because of the contact potential. If W < a, a channel exists with zero gate bias. The device is operated in the depletion mode. On the other hand, if W > a, the depletion region extends across the channel in equilibrium, and no significant channel current can flow. A positive gate voltage must be applied to reduce the depletion width to a value smaller than the channel thickness a. The device is operated in the enhancement mode. Figure 9.4 shows the energy band diagrams of a depletionmode MESFET under V D = 0 and various V GS . A reverse bias on the gate (V GS < 0) is required to modulate the channel width. The threshold voltage V T can also be termed the ‘turnoff’ voltage of the device. For enhancementmode MESFETs, a positive gate bias is required to open the channel. The energy band diagrams for various bias conditions (V D = 0) are shown in Fig. 9.5.
9.1.2 Current–Voltage Characteristics A onedimensional model is used to develop the DC current–voltage (I–V ) characteristics of a MESFET. It is assumed that no breakdown will be induced before the channel is pinched off and the device has a doping density of N d in the channel. Furthermore, the active region of the MESFET has a channel length L, junction width Z, channel depth a, depletion width W (x), and conducting channel width h(x). The origin of the xaxis is located at the edge of the gate adjacent to the source. A schematic of the MESFET structure and the corresponding voltage drop due to the drain bias is shown in Fig. 9.6.
344
9 Heterostructure Electronic Devices
Fig. 9.4 Depletion region profile under the gate and energy band diagrams of depletionmode MESFET under V D = 0 and various V GS (negative)
VGS = 0
VGS = VT
q(V0 – VGS)
qVP
qV0 EF
VGS > VT
qVT
qVGS
Fig. 9.5 Depletion region profile under the gate and energy band diagrams of enhancementmode MESFET under V D = 0 and various V GS (positive)
9.1 Metal–Semiconductor FieldEffect Transistors (MESFETs)
345
VGS
Depletion region
a
VD
h(x)
ntype
Source
W(x) Drain
ID
Vx
dx
x
0
VD
L
Fig. 9.6 Schematic diagram of the conducting channel, dimensions, and potential drop along the channel
The current at position x in the channel is described as ID (x) = A(x)σ F(x) =
Z h(x) dVx ρ dx
(9.10)
where σ is the channel conductivity, ρ is the resistivity of the channel material, √ h(x) = a − W (x), W = (2/q Nd )(V0 − VGS + Vx ) and V P = qa 2 Nd /2. Since the drain current is a constant and independent of x, we can solve I D by integration. L ID 0
Za dx = ID L = ρ
∴
ID = G 0 V P
V0 V0 + Vx − VGS 1− dVx VP 0
V Za 2 (V0 + Vx − VGS )3/2 D Vx − = √ ρ 3 VP 0
VD 2 V0 + VD − VGS 3/2 2 V0 − VGS 3/2 − + VP 3 VP 3 VP
(9.11)
where G0 is the channel conductance at W (x) = 0 and G0 ≡ Za/ρL. This is the complete I–V characteristic equation for all bias conditions. In the low bias region, where V D V 0 − V GS , the I–V characteristics have a linear relationship. We can first rewrite I D in the following form:
346
9 Heterostructure Electronic Devices
ID = G 0
2 VD − √ (V0 − VGS )3/2 3 VP
VD 1+ V0 − VGS
3/2 −1
(9.12)
Then, using Taylor series expansion of (1 + x)n ∼ = (1 + nx) for x 1, we have
3VD /2 2 3/2 1+ −1 ID ≈ G 0 VD − √ (V0 − VGS ) V0 − VGS 3 VP √ V0 − VGS ∝ VD = G 0 VD 1 − √ VP
(9.13)
The drain current simply increases linearly with drain bias voltage. At the other end of the spectrum, the conduction current saturates at high drain bias when the channel is pinched off. The I–V relationship described above is only valid up to pinchoff, where V P = VD (sat) + V0 − VGS . Using this pinchoff voltage relation in (9.11), the saturation current is obtained as ID (sat) = G 0 V P
VD (sat) 2 2 V0 − VGS 3/2 − + VP 3 3 VP
(9.14)
This equation can be further reduced by replacing VD (sat)/V P with 1 − (V0 − VGS )/V P . ID (sat) = G 0 V P
1 − 3
V0 − VGS VP
2 V0 − VGS 3/2 + 3 VP
(9.15)
The typical I–V characteristics of an nchannel depletionmode MESFET are shown in Fig. 9.7. The drain current flows for V GS are less negative than the threshold voltage V T . At sufficiently high drain bias, V B , avalanche breakdown occurs between the gate and drain and the drain current increases abruptly.
9.1.3 Transconductance and Equivalent Circuit of MESFET One of the figures of merit of the MESFET is the transconductance, gm , which describes the effect of the input voltage change on the output current. In the equivalent circuit model, the intrinsic transconductance gmi times the input voltage represents a current source. Under a fixed drain bias, the change in gate voltage leads to a depletion layer width change. Because the space charge in the depletion region changes by QG in a time interval of τ, a drain current change is induced. IDS
Q G or = τ
∂ IDS 1 = ∂ Q G VDS τ
(9.16)
9.1 Metal–Semiconductor FieldEffect Transistors (MESFETs) Fig. 9.7 Typical current–voltage characteristics of a depletionmode MESFET. Breakdowns occur at the breakdown voltages V B
IDS
347
Locus for VD(sat) Linear region
Saturation region VGS > 0 VGS = 0 VGS < 0 VGS ~ VT
0
VB
VDS
The rate of conduction current change with respect to the charge change in the depletion region defines a carrier transient time (τ ) crossing the conduction channel. The intrinsic transconductance, gmi , is then defined as gmi ≡
∂ IDS ∂ IDS ∂ Q G CG = · = ∂ VGS VDS ∂ Q G VDS ∂ VGS VDS τ
(9.17)
C G is the total gate capacitance and C G = C GS + C DG , where C GS and C DG are the gatetosource capacitance and draintogate capacitance, respectively. To increase gmi , we have to reduce τ. The minimization of τ can be achieved either by using materials with high drift velocity or by minimizing the channel length through the reduction of gate length. The approach of increasing the total gate capacitance to achieve high gmi is not practical, since it will limit the frequency response of the device. Next, we examine the property of the drain terminal. For a fixed gate bias, a change in V DS will also change the space charge in the depletion region, ΔQG , which defines a current change, ΔI DS , and leads to a draintogate capacitance C DG . CDG ≡
∂ Q G ∂ VDS VGS
(9.18)
The current–voltage change further defines a draintosource output conductance (Go ): ∂ IDS ∂ IDS ∂ Q Go ≡ = · (9.19) ∂ VDS VGS ∂ Q VGS ∂ VDS VGS
348
9 Heterostructure Electronic Devices
CDG
RG
RD
Gate
Drain +
CGS
gmiV
Go
Co
RS
Source Fig. 9.8 Intrinsic equivalent circuit model of the MESFET including terminal series resistances
where Q is the total charge in conduction channel. Assuming the carrier velocity υ is constant in the conduction channel of an effective length L eff , I DS ~ Q/t, and t ~ L eff /υ, the righthand side of the output conductance (9.19) can be expressed as ∂ IDS ∼ υ and = ∂ Q VGS L eff
∂ Q ≡ Co ∂ VDS VGS
(9.20)
C o defines an output capacitance. ∴ Go =
Co υ L eff
(9.21)
To achieve large Go , high carrier mobility and small gate length are necessary. Figure 9.8 shows a simple intrinsic equivalent circuit model of the MESFET that ignores all parasitic elements except the terminal series resistances RG , RS , and RD .
9.1.4 HighSpeed Figure of Merit The highfrequency performance of a MESFET is usually characterized by parameters related to its ultimate operation frequency. However, these parameters are difficult to measure due to the fact that the performance of the device under testing can depend as much on the measurement circuit as on the device itself. As a result, highfrequency transistors are commonly characterized by frequencydependent gains, deduced from networkanalyzer measurements. The highfrequency performance of the device measured in this way is reasonably independent of the circuit in which it is placed. There are two gains commonly used to deduce the small signal, linearoperation figure of merit of the device. One of these gains is h21 , which is the forward
9.1 Metal–Semiconductor FieldEffect Transistors (MESFETs)
349
Ii
Fig. 9.9 Intrinsic equivalent circuit of a MESFET for frequency response analysis
CDG CGS
VC
gmiVC
current gain with the output shortcircuited. The frequency at which this gain extrapolates to one is the unity shortcircuit current gain frequency f T . Consider the simple intrinsic equivalent circuit of Fig. 9.9. This frequency can be derived as the frequency at which the magnitude of the input current I i equals the magnitude of the ideal output current gmi V C of the transistor. When the output is shortcircuited, Ii  = iω(CGS + CDG )VC  = 2π f T (CGS + CDG )VC = gmi VC fT =
1 2π
gmi CGS + CDG
=
gmi 1 = 2πCG 2π τ
(9.22) (9.23)
This equation shows that f T is a measure of a quantity that is fundamental to the device—the delay time of the current through the conduction channel. The other important figure of merit of the transistor is the maximum frequency of oscillation, f max . At this frequency, the unilateral power gain (U) of the device becomes unity. It is the highest frequency at which the transistor can amplify the power of a signal and can be expressed as fT f max ≈ √ 2 G o (RG + RS ) + 2π f T CDG RG
(9.24)
The f max of a MESFET may be either above or below its f T , depending on the specific circuit values in the above equation.
9.1.5 MESFET Fabrication and Performance A typical fabrication sequence for a highspeed MESFET is shown in Fig. 9.10. The process was designed to maximize the cutoff frequency of the transistor by minimizing the contact resistances, reducing the parasitic in the active conduction channel, and shortening the gate length. An n+ contact layer is added on top of the conduction channel layer outside the gate region to reduce the source and drain contact resistances RS and RD . In addition, a thick channel layer outside the gate area is used to minimize the surface depletioninduced additional resistance. To maintain a
350
9 Heterostructure Electronic Devices
Fig. 9.10 Typical fabrication sequence of submicron GaAs MESFET using the doublerecess process. a Epitaxy and using photoresist (PR) to define device active area, b mesa etch for isolation, c source and drain ohmic contacts deposition, d channel recess etch and gate recess etch using bilayer PR process, e Tgate metal deposition, and f PR liftoff to complete MESFET process
short gate length while minimizing the gate contact resistance RG , the usual practice is to use a ‘T’ gate design where a thick top metal contact with a narrow base is adopted. The gate is situated in a recess of the channel layer in order to control the threshold voltage, V T . The gate recess is usually offcentered and located near the source contact to minimize RS . The gate–drain separation, L GD , is designed to be greater than the depletion width at the breakdown voltage. The fabricated MESFETs are characterized by measuring their I–V characteristics, gm , f T , and f max . Figure 9.11 shows the I–V characteristics of a 0.12 × 50 μm2 dualgate GaAs depletionmode MESFET. The drain currents show weak saturation for the negative gate bias voltages. This is a common behavior called shortchannel effect in MESFETs with gate length less than 0.25 μm. The shortchannel effect is due to the less efficient intervalley transfer of electrons from the valley to the Lvalley at high fields in shortchannel devices. Thus, most electrons stay in the valley when reaching the drain and show as a weaker
9.1 Metal–Semiconductor FieldEffect Transistors (MESFETs) 700
600
700 ID (VDS = 1 V)
600
0.25 V/step
600
500
500
gm (VDS = 1 V)
ID (mA/mm)
500
400 300
300 300 200
200
200
100
100
0 0
0.5
1.0
1.5
2.0
2.5
400
400
0 1.5
Vds (V)
gm (mS/mm)
Top trace Vgs = 0.75 V
Drain current (mA/mm)
351
100
1.0
0.5
0
0.5
0 1.0
VGS (V)
Fig. 9.11 Measured I D V DS characteristics and channel current and transconductance versus gate bias of a dualgate (0.12 μm × 50 μm) GaAs MESFET. Courtesy M. Feng, University of Illinois at UrbanaChampaign
velocity saturation. The parasitic leakage through the semiinsulating substrate also contributes to the lack of current saturation for the more negative gatevoltage region. The transconductance gm is deduced from the drain current variation under various gate bias voltages. Note that the measured gm is the extrinsic transconductance including the effect of RS and expressed as gm =
gmi 1 + gmi RS
(9.25)
The maxima f T and f max of the MESFET are estimated to be 110 and 235 GHz, respectively, and shown in Fig. 9.12. These values are deduced from the measured lowfrequency values of h21 and U max up to 40 GHz using a rolloff of −6 dB/octave.
9.2 Modulation Doping and TwoDimensional Electron Gas (2DEG) As shown in Fig. 4.7, the carrier mobility of a semiconductor is determined by the sum of inverse mobility components (μi ) due to different scattering mechanisms, i.e., μ−1 = (μi )−1 . At a fixed temperature, the lowest mobility component dominates the total carrier mobility. In binary compound semiconductor alloys, the major scattering processes are the optical phonon (polar) scattering at high temperature, the ionized impurity scattering at low temperature, the acoustic phonon scattering due to piezoelectric field, and the acoustic phonon scattering due to deformation potential. With the exception of the impurity scattering, the effect of all scattering mechanisms on electron mobility can be reduced at low temperatures. The total temperaturedependent electron mobility increases with decreasing temperature and reaches a maximum value before decreasing with further reducing temperature. One
352
9 Heterostructure Electronic Devices 50
H21, VDS = 1V, VGS = 0.5V Umax, VDS = 2.5V, VGS = 0.5V
H21, Umax (dB)
40
30
20
10 fmax = 205 GHz 0
108
109
1010
Frequency (GHz)
1011 fT = 120 GHz
Fig. 9.12 Measured unity current gain frequency f T (H21 ) and maximum cutoff frequency f max of the same dualgate (0.12 μm × 50 μm) GaAs MESFET characterized in Fig. 9.11. Courtesy M. Feng, University of Illinois at UrbanaChampaign
way to reduce the ionized impurity scattering at low temperature is to use highpurity materials, as evidenced in Fig. 4.7, where there are fewer ionized impurities. However, for most highspeed device applications, certain doping concentrations have to be maintained. Therefore, this option is not practical. In 1978, R. Dingle and colleagues at Bell Laboratories invented a modulationdoping technique to eliminate the influence of ionized impurity scattering in heterojunction superlattices [1]. By separating the physical location of ionized dopants from generated electrons across the heterojunction, with ionized impurities on the large bandgap semiconductor side and generated conduction electrons on the undoped small bandgap semiconductor side, electron mobility much higher than the equivalent bulk material was achieved at low temperature without sacrificing the carrier concentration. Since these conduction electrons occupy a thin layer (≤100 Å) in the triangular quantum well formed at the heterojunction interface, they can only move easily close to and parallel to the heterojunction interface. These electrons form an electron cloud, or a pseudotwodimensional electron gas (2DEG), in the modulationdoped heterostructure. Based on this concept, a new type of FET, the highelectronmobility transistor (HEMT), was derived.
9.2.1 ModulationDoped (MD) Heterostructures The modulationdoping concept was first developed utilizing heterojunction superlattices as shown in Fig. 9.13. In a superlattice structure with typeI band alignment, quantum wells are formed in both conduction and valence bands. Under equilibrium
9.2 Modulation Doping and TwoDimensional Electron Gas (2DEG)
353
Fig. 9.13 Energy band diagrams for ndoped and undoped GaAsAlx Ga1−x As superlattices. Reprinted with permission from [1], copyright AIP Publishing
conditions, a continuous Fermi level throughout the superlattice causes appreciable band bending, leading to the formation of pseudotriangular quantum wells at heterojunctions. When the superlattice is either uniformly doped (UD) or modulationdoped (MD) with donor impurities, due to the high potential energy associated with the barrier layer relative to the quantum well, electrons associated with donor impurities in barriers will move into quantum wells. In both UD and MD superlattice structures, the carriers confined to the pseudotriangular quantum well form a 2DEG. The ionized impurity scattering in the conduction channel is removed in MD structures, where 2DEG conduction electrons and their parent donor impurities are spatially separated from each other in an irreversible manner. The electron mobility of the 2DEG suffers no ionized impurity scattering, leading to a much higher mobility, especially at low temperatures. Figure 9.14 shows the temperaturedependent electron mobility of bulk, UD and MD GaAs structures. The UD and MD structures used the AlGaAs/GaAs material system. The electron mobility enhancement at low temperatures clearly demonstrates the reduction (or even a lack) of impurity scattering as expected. Since the doped barrier layers are totally depleted in MD superlattice structures, the electron density in the quantum well may greatly exceed the unintentionally doped impurity density. Thus, the concentration of 2DEG is independent of the doping level in the conduction channel. By the same token, an enhanced hole mobility of the twodimensional hole gas (2DHG) is achievable in ptype MD heterostructures.
354
9 Heterostructure Electronic Devices
Fig. 9.14 Temperaturedependent electron mobility for bulk GaAs and several undoped UD and MD superlattices. The crosshatched region includes most of the MD data. Reprinted with permission from [1], copyright AIP Publishing
Of course, a superlattice heterostructure with multiple MD heterojunctions is not necessary for device implementation. With a proper energy band discontinuity, a single MD heterojunction is sufficient to form a 2DEG at the heterostructure interface and to achieve the electron mobility enhancement. In fact, for FET applications, the single MD heterojunction design makes it easy to control the channel charge carriers. The first FET utilizing the highelectronmobility feature of the MD heterostructure has just one heterointerface as shown in Fig. 9.15. This design first demonstrated by engineers at Fujitsu Laboratories in Japan—a highelectronmobility transistor (HEMT) design, as it was called—became the standard structure of future FETs utilizing 2DEG in the conduction channel [2].
9.2.2 Scattering Mechanisms in MD Heterostructures It is important to analyze various scattering mechanisms limiting the mobility in the 2DEG in order to be able to provide interface design rules for yielding highperformance devices. In addition to the bulk scattering mechanisms, some additional scattering mechanisms unique to heterojunctions are introduced here. A GaAs/AlGaAs MD heterostructure similar to the HEMT structure shown in Fig. 9.15 is used to illustrate the properties of added scattering mechanisms. On the semiinsulating GaAs substrate, an undoped GaAs channel layer was first grown, followed
9.2 Modulation Doping and TwoDimensional Electron Gas (2DEG)
355
Depletion layer Ionized donor impurities
Sidoped AlxGa1xAs Undoped AlxGa1xAs
2DEG
0.1 µm t
Electron layer Ec
++ + + +
Fermi level
0.8 µm
Ev
Undoped GaAs (100)oriented, semiinsulating GaAs substrate
Nondoped NAlxGa1xAs Sidoped NAlxGa1xAs
Nondoped GaAs
Fig. 9.15 Layer structure and energy band diagram of an MD GaAsAlx Ga1−x As heterostructure grown by MBE with a spacer layer inserted between the barrier layer and the 2DEG channel. Reprinted with permission from [2, 3], copyright Japanese Society of Physics
by a silicondoped ntype AlGaAs barrier layer to complete the MD heterostructure. The 2DEG channel will be formed at the GaAs/AlGaAs interface just inside the undoped GaAs layer. (a) Coulomb interaction from ionized impurities located in the barrier Since the 2DEG is located right next to the heterointerface, the physical quality of the interface as well as any force exerted that diverts the transport direction toward the interface will affect the nature of carrier scattering. The attraction force due to Coulomb interaction between 2DEG in the conduction channel and its ionized parent donor impurities in the barrier layer will cause electrons to scatter with the heterointerface. The electron mobility is reduced due to this added scattering mechanism. The carrier mobility is thus a function of the 2DEG sheet charge density. At a low barrier doping density (small 2DEG sheet charge density), the Coulomb interaction is weak and the electron mobility is limited by the background scattering in the undoped GaAs channel. For a heavily doped barrier layer structure, the Coulomb interaction dominates the carrier scattering process. The Coulomb scattering problem cannot be totally eliminated but can be reduced by setting back the doping region of the barrier layer away from the heterointerface. This undoped barrier layer inserted between the 2DEG and doped barrier layer is called a spacer layer [4]. Remember, the Coulomb attraction force is inversely proportional to the square of the charge separation distance. For a fixed doping density in the barrier, the Coulomb interaction between the 2DEG and ionized donors weakens with increasing spacer layer thickness, thus increasing electron mobility. However, due to the decreased electron transfer rate from the thicker barrier layer to the conduction channel, for a fixed barrier doping density, the sheet density of the 2DEG will decrease with increasing spacer layer thickness. In practical devices, a compromised spacer layer thickness of 25–30 Å is used to optimize the electron mobility while maintaining a high 2DEG sheet charge density.
356
9 Heterostructure Electronic Devices
(b) Interfaceroughnessinduced scattering Since the 2DEG in the conduction channel of an MD heterostructure is located very close to the heterointerface, any minute interface roughness could induce additional scattering and decrease the carrier mobility. Normally, in MD heterostructures, the AlGaAs barrier layer is grown on top of the GaAs 2DEG channel layer using MBE. The surface morphology of the GaAs channel layer at the heterointerface is critically important. An extremely flat and smooth GaAs/AlGaAs interface is usually achieved under proper growth conditions including a wide range of V/III flux ratio, substrate temperature, and growth rate. This layer structure is convenient for FETlike device fabrication, including HEMT, and is called the normal MD heterostructure. If the layer sequence is reversed such that the GaAs 2DEG channel layer is placed on top of the AlGaAs barrier layer, the structure is called an inverted MD heterostructure. To achieve high electron mobility in such structures, an extremely smooth AlGaAs surface morphology is required. However, only under a very narrow MBE growth window does the AlGaAs show a less rough surface. Figure 9.16 shows the difference in the 77 K electron mobility for normal and inverted MD heterostructures grown at various substrate temperatures with a 75 Å spacer layer. The 2DEG mobilities for normal and inverted MD structures are shown at different scales in the figure. Note that, even using the optimal AlGaAs growth temperature, the electron mobility of the inverted structure is still an order of magnitude smaller than that of the normal structure. (c) Intersubband scattering at high carrier density
Electron mobility (cm2/Vs)
Since the 2DEG is confined in the quasitriangular QW at the heterointerface, electrons are occupying the quantized states of the QW. The ground state gets populated
Inverted structure Normal structure
8x104
8000
6x104
6000
4x104
4000
2x104
2000
600
650
700
750
800
Fig. 9.16 Measured 2DEG mobility of normal and inverted MD GaAs/AlGaAs heterostructures grown at different temperatures. Reprinted with permission from [4], copyright AIP Publishing
9.2 Modulation Doping and TwoDimensional Electron Gas (2DEG)
Electron mobility of modulation doped GaAs
1989
10,000,000 1987
Electron mobility (cm2/Vsec)
Fig. 9.17 Progress of peak mobility achieved in 2DEG as a function of temperature over a span of 12 years Reprinted with permission from [5], copyright AIP Publishing
357
1982
1,000,000
1981
100,000
1980
1979
1978
10,000 5,000 Bulk
0.2
0.5
1
2
5
10
20
50 100 200 400
Temperature (K)
first with electrons transferred from the barrier layer. When the ground state is fully populated, any further increase of the transferred electron density will have to occupy the higher energy states. The scattering probability is increased for the multiplestate system, and it reduces the total electron mobility. The electron mobility values of the modulationdoped heterostructures have progressed steadily since 1978 (Fig. 9.17). In just three years, lowtemperature electron mobility of over one million (cm2 /V s) was achieved in many laboratories. Further improvements of MD heterostructure designs and growth techniques pushed the electron mobility of the 2DEG over the 10 million (cm2 /V s) mark in 1989 at Bell Laboratories. A very thick spacer layer (70 Å) and planar (delta) doping scheme were used to minimize the Coulombinteractioninduced interface scattering. The superlattice buffer layer beneath the GaAs channel was extensively used to guarantee minimized interface roughness scattering. Furthermore, to minimize the background doping concentration in the GaAs channel layer, the MBE system was thoroughly baked at high temperature (>200 °C) to get rid of volatile impurities inside and kept under liquid nitrogen cooling all the time. These grown samples provided a wonderful playground for some solidstate physicists, but have no immediate device application due to the low 2DEG sheet charge density achieved.
358
9 Heterostructure Electronic Devices
9.3 HighElectronMobility Transistor Basics—A Triangular Quantum Well Approach The FET structure based on a 2DEG in the conduction channel was first demonstrated in 1980 by Fujitsu Laboratory of Japan, less than two years after the inception of the MD concept at Bell Laboratories. Therefore, there were different names used for this newly developed FET. The Fujitsu group called it the HEMT (highelectronmobility transistor), Bell Laboratories named it SDHT (selectivelydoped heterofieldeffect transistor), and the group at Thomson CSF in France called it TEGFET (twodimensional electron gas fieldeffect transistor). The name MODFET (modulationdoped fieldeffect transistor) has also been used. Today, HEMT is the most commonly used name for this kind of FET. The basic device structure of the HEMT is very similar to a MESFET, as shown in Fig. 9.18. Similar to a MESFET, the conduction current flows between the source and drain, and the amount of current flow is controlled by the gate bias. However, a HEMT does not use the gate bias to adjust the width of the conduction channel. Rather, the gate bias modulates the Fermi level position and, thus, controls the 2DEG sheet carrier density in the conduction channel. In this section, we will use a simple pseudotriangular QW approach to examine the equilibrium 2DEG sheet carrier density of a heterostructure. An ideal triangular QW structure has an infinitely high vertical barrier on one side and a constant slope on the other side. The eigenenergy solutions of the ideal triangular QW are in the form of the Airy functions. If an ideal triangular QW was assumed for the HEMT structure, electrons transferred from the barrier layer fill the first allowed state (E 0 ) in the QW up to the Fermi level (E F ). Under ideal conditions, carriers of the 2DEG are solely transferred from the doped barrier layer with a doping concentration N d and a depletion layer thickness W d . Thus, the sheet carrier concentration of the 2DEG, N S , simply equals to N d W d (cm−2 ). However, one should notice that the conduction band structure of the HEMT is far from ideal—the pseudotriangular QW has a finite band discontinuity, ΔE c , on one side and a sublinear energy barrier on the channel side as shown in Fig. 9.19 for an AlGaAs/GaAs HEMT.
Fig. 9.18 Schematic structure of a GaAs/AlGaAs highelectronmobility transistor
9.3 HighElectronMobility Transistor Basics—A Triangular Quantum …
359
Fig. 9.19 Heterojunction energy band diagram of the HEMT structure shown in Fig. 9.18. The spacer layer in AlGaAs is removed from the heterojunction interface
Using an ideal triangular QW model, the possible sheet charge density (N S ) is estimated first. From Gauss’ law for an ideal triangular QW, the displacement flux density (D) relates the sheet charge density and the electric field intensity (F) by D = F = ρ S = q N S or F = q N S /
(9.26)
Therefore, the ground state inside the QW, E 0 , can be expressed in terms of N S by E0 =
2 2m ∗
1/3
9πq 2 N S 8
2/3 2/3
≈ γ NS
(9.27)
At T = 0 K, where f (E) = 1, the equilibrium sheet carrier density is given by EF NS ≈
D2D (E) f (E)dE = E0
m∗ (E F − E 0 ) π 2
(9.28)
At a finite temperature, E F NS ≈
D2D (E) E0
=
1 1 + exp[(E 0 − E F )/kT ]
dE
m∗ kT ln{1 + exp[(E F − E 0 )/kT ]} π 2
(9.29)
360
9 Heterostructure Electronic Devices
If we include a thin undoped spacer layer with a thickness of W sp at the interface, a voltage drop V sp will appear across this layer. According to the energy band diagram shown in Fig. 9.20, the conduction band discontinuity E c at 0 K can be expressed as the following: E c = q V0 + q Vsp + E d + E 0 + δ E
(9.30)
⎧ π 2 ⎪ ⎪ ⎪ δ E = EF − E0 = ∗ NS ⎪ ⎪ m ⎨ q Nd Wd2 q N S Wd = V0 = ⎪ 2 2 ⎪ ⎪ ⎪ W q N S sp ⎪ ⎩ Vsp =
(9.31)
where
Here the bottom tip of the triangular QW is set as E = 0. We notice that each term, except E d , in this equation is a function of N S and has a unique solution for each E F . By moving the E d term to the left of the equation, the righthand side of the equation can be expressed in terms of N S . E c − E d = q V0 + q Vsp + E 0 +
π 2 NS m∗
q 2 N S Wsp q 2 N S Wd π 2 q2 + + E0 + ∗ NS = N2 2 m 2 Nd S 2 q Wsp π 2 + + ∗ NS + E0 m
(9.32)
E c − E d =
(9.33)
Fig. 9.20 Heterojunction energy band diagram of the HEMT structure shown in Fig. 9.18. The spacer layer in AlGaAs at the heterojunction interface is included
9.3 HighElectronMobility Transistor Basics—A Triangular Quantum …
361
Assuming an Airy function for the ideal triangular QW and using the appropriate material parameters, one can solve N S selfconsistently. However, the difficulty in solving N S from the above equation lies in the determination of the eigenenergy E 0 , since E 0 depends on the shape of the potential well. In a realistic quasitriangular QW, E 0 cannot be determined exactly. Therefore, instead of solving N S rigorously, one can qualitatively understand the factors that control N S using the following extreme conditions. Assuming the density of states of the ground state subband is so large that the Fermi level is close to the bottom of the well, E F ≈ 0. For a very small spacer layer, W sp ≈ 0, the charges in the AlGaAs barrier are totally depleted by the conduction band discontinuity and transferred to the QW, forming a 2DEG. q2 N 2 and N S ∼ E c − E d ∼ = = 2 Nd S
2 Nd (E c − E d ) q2
(9.34)
For a thick spacer layer, Wsp Wd , the transferred N S is small and we can neglect the term contains N S2 . NS =
q2W
(E c − E d )
(9.35)
sp
For a GaAs/AlGaAs HEMT with N d = 1018 cm−3 , E c = 0.2 eV, and = 12.850 , the sheet electron concentrations under these two extreme conditions are calculated as 1.6 × 1012 cm−2 for Wsp = 0 NS = (9.36) 7.2 × 1011 cm−2 for Wsp = 200 Å These numbers are ~30% overestimated: In the first case, for W sp = 0, E F = 0 and requires a lot more electrons to fill the subband. In the second case, due to the large extent of the spacer layer, only a portion of the doped barrier is depleted. Even at these overestimated values, they are still much smaller than that of a comparable GaAs MESFET with a 0.2 μm conduction channel doped to 1017 cm−3 (2–3×1012 cm−2 ). Since a large N S can reduce the channel resistance and increase current drive capability of the FET, a large N S is desirable for device applications. Therefore, it is critical to maximize the carrier density of the HEMT. Empirically, N S is proportional to N d E c /W sp in a HEMT. Based on this relation, we should select material systems with a large E c , a small W sp , and a maximum N d .
362
9 Heterostructure Electronic Devices
9.4 Operation Properties of the HEMT The operation of the HEMT can be best understood through the analysis of its energy band diagram. Unlike MESFETs, the sheet charge density in a HEMT is controlled by the Fermi level position relative to the QW subbands shown in Fig. 9.21. The Fermi level position in the quasitriangular QW is determined by the work function of the gate metal, barrier layer thickness, doping concentration, conduction band discontinuity, and gate bias. In a properly designed HEMT, through the modulation of the Fermi level, the gate bias voltage V GS directly controls the sheet charge density similar to that of MESFETs. Depending on the device parameters, depletionmode and enhancementmode operations of HEMTs are also expected.
9.4.1 Isolated Heterojunction Under Equilibrium To understand the relationship between the applied gate bias and the Fermi level position or sheet charge density, we first examine the 2DEG heterojunction under equilibrium conditions. In the band diagram shown in Fig. 9.22a, the undoped conduction channel layer and the ntypedoped barrier layer are assigned as regions 1 and 2, respectively. The origin of this 1D diagram is set at the heterointerface with a depletion width of W d into the infinite long barrier layer. We also assumed an undoped spacer layer of W sp on the barrier layer side of the heterojunction, a dopant ionization energy of E d and a potential barrier height of qV b0 formed by the depletion layer at the heterointerface. Under equilibrium, according to Gauss’ law, at the heterointerface, it follows that D1 = D2
(9.37)
Ec
Fig. 9.21 Conduction band diagram of a depletionmode HEMT under a gate bias of V GS < 0. The work function of the metal contact, qφ m , is also shown
q
m
+ + + + + + E1 ++ E 0
Ec
EF
qVGS 0
z
9.4 Operation Properties of the HEMT
363
Fig. 9.22 a Energy band diagram in conduction band, b charge distribution, and c electric field distribution at the heterojunction of a HEMT
1 F1 = 2 F2 = q N S
(9.38)
N S = 2 F2 /q
(9.39)
where D, F, and are the displacement flux density, electric field intensity, and permittivity, respectively. In this section, all discussions concern material 2 only; we will use instead of 2 for simplicity. Assuming donors in the barrier layer are fully ionized between −W d ≤ z ≤ –W sp and remain neutral beyond −W d , Poisson’s equation can be written as
364
9 Heterostructure Electronic Devices
d2 V dF q N (z) =− =− dz 2 dz
(9.40)
And, as shown in Fig. 9.22b, the charge distribution is N (z) =
0, −Wsp < z < 0 Nd , −Wd < z < −Wsp
(9.41)
Thus, in the depletion region of the doped barrier q F=
q Nd z+C
N (z)dz =
(9.42)
Using the boundary condition of F = 0 at z = –W d , we found (Fig. 9.22c) q Nd (z + Wd ) for
F=
− Wd < z < −Ws p
(9.43)
In the spacer layer, F is a constant of F=
q NS
for − Wsp < z < 0
(9.44)
The electric field intensity distribution across the depletion region of the heterojunction is shown in Fig. 9.22c. The electric field intensity in the barrier has a slope of q Nd /. The potential drop across the doped barrier layer (layer thickness W d ) can then be calculated as Vb0 = −
q Nd Fdz = −
q Nd −
z2 + Wd z 2
−W d
(z + Wd )dz = −Wsp
−Wd
−Wsp
=
2 q Nd Wd − Wsp 2
(9.45)
By the same token, the potential drop across the spacer layer becomes −W sp
Vsp = − 0
q NS q NS dz = Wsp
(9.46)
The total potential drop across the barrier is the sum of V b0 and V sp . V = Vb0 + Vsp =
q Nd 2 2 Wd + Wsp 2
(9.47)
9.4 Operation Properties of the HEMT
365
9.4.2 Charge Control by Gate Bias in HEMT In HEMT structures, the doped barrier layer has a finite thickness and a metal Schottky gate is applied on the surface. The Schottky barrier also creates a surface depletion layer. It substantially alters the conduction band shape of the barrier layer and plays an important role in determining the Fermi level position. To simplify the discussion, assume the doped barrier layer is completely depleted. Relative to the surface, as shown in Fig. 9.23, the potential drop across the barrier is defined as V i . Vi = φm − VGS −
1 (E c − E F ) q
(9.48)
This potential difference V i can also be derived from Poisson’s equation. q N (z) dF d2 V =− =− 2 dz dz
(9.49)
and N (z) =
Nd , −Wd ≤ z ≤ −Wsp 0, −Wsp ≤ z ≤ 0
(9.50)
Thus, the electric field intensities in the depleted doped barrier and spacer layers are ⎧ q Nd ⎪ ⎨ z + C1 , −Wd ≤ z ≤ −Wsp q F= (9.51) N (z)dz = q N S ⎪ ⎩ , −Wsp ≤ z ≤ 0
Ec
qVi q(
m
VGS) q
m
E0
EF
qVGS 2
1
E=0 d
sp 0
z
Fig. 9.23 Energy band model of a HEMT under a gate bias V GS < 0. In this model, it is assumed that, under all bias conditions, the barrier layer beneath the gate is completely depleted
366
9 Heterostructure Electronic Devices
Assuming F = q N S / = Fat z = −Wsp , then C1 = F + q Nd Wsp /. The potential drop across the depleted barrier layer can then be calculated as V =−
q Nd Fdz = −
2 −Wd
−W d
−Wsp
q Nd Wsp zdz −
−W d
dz − F −Wsp
−W d
dz
−Wsp
q Nd Wsp −Wd d z−Wsp − F z−W −Wsp −Wsp q Nd 2 2 2 Wd − Wsp + F Wd − Wsp =− − 2Wd Wsp + 2Wsp 2 =−
q Nd
z 2
V =−
−
2 q Nd Wd − Wsp + F Wd − Wsp 2
(9.52) (9.53)
The potential drop across the spacer layer is simply F W sp . Letting V (0) = 0, the potential drop V i can be expressed as 2 q Nd Wd − Wsp − F Wd − Wsp 2 q NS = VP − Wd
Vi = −V − F Wsp = − F Wsp
(9.54)
2 Here we defined a pinchoff voltage of V P = (q Nd /2) Wd − Wsp just like a MESFET. Since Vi = φm − VGS − (E c − E F )/q, we can write the sheet charge density in (9.54) as a function of voltage across the heterostructure. NS =
E c − E F VGS − φm − V P − qWd q
(9.55)
The terms in the parenthesis are all fixed for a particular device structure and are defined as a threshold voltage or offvoltage V T . At an applied gate bias V GS equal to V T , where E F ≤ E 0 , the 2DEG vanishes. VT ≡ φm − V P −
1 (E c − E F ) q
(9.56)
The Fermi level energy E F is usually small compared with other terms and can be neglected. Finally, the distribution of the 2DEG in the triangular QW has a peak at a distance of W from the heterojunction interface. The effective depletion layer thickness should be corrected as (W d +W ). For the values of N S between 5×1011 cm−2 and 1.5×1012 cm−2 in AlGaAs/GaAs HEMTs, W is about 80 Å. The final expression of the sheet carrier density becomes
9.4 Operation Properties of the HEMT
NS ∼ =
367
(VGS − VT ) q(Wd + W )
(9.57)
This equation indicates that the 2DEG density is linearly proportional to the gate bias, V GS . Thislinear relationship is limited by two extremes, N S = 0 and N S = Nd Wd − Wsp , as illustrated in Fig. 9.24. In a HEMT structure with a 2DEG created at zero gate bias, the Fermi level is positioned above the ground state, E 0 . By applying a reverse gate bias, as shown in Fig. 9.24a, the rise of the total Schottky barrier potential energy at the surface leads to a lowering of E F , which reduces the sheet charge density. When the gate bias is equivalent to the threshold voltage, V T , the conduction channel is turned off. On the other hand, as shown in Fig. 9.24b, under forward gate bias condition, the rising Fermi level allows more electrons to be transferred into the triangular QW, contributing to the current conduction. This process will continue until all donors in the barrier are ionized. The 2DEG sheet carrier density becomes saturated with further increasing of V GS . Figure 9.25 shows the experimental results of N S as a function of gate bias in several Al0.3 Ga0.7 As/GaAs HEMT samples with different spacer layer thicknesses. All samples have a doping concentration of N d = 4.6×1017 cm−3 in the barrier layer, except sample No. 76 (N d = 9×1017 cm−3 ). It is clear, in all samples, that N S increases linearly with increasing V GS and saturates at a higher gate bias voltage. The flat saturated region indicates the maximum achievable sheet carrier density in that sample. By extrapolating the linear part of the V GS − N S curve to zero sheet concentration, the threshold voltage is determined. Obviously, the threshold voltage is dependent on the spacer layer thickness due to the V P term involved, which depends on the spacer layer thickness. As expected, for the same device structure, the thinner the spacer layer, the higher the saturated 2DEG density. The channel conduction current density of a HEMT is primarily determined by the sheet charge density, which is controlled by the difference between gate bias voltage and threshold voltage. A closer examination of the threshold voltage reveals that it depends on the layer thickness. For a HEMT structure, φ m and E c are fixed and E F (a)
(b)
VGS < 0 q
VGS > 0 Ec
m
Ec qVGS
E0
q qVGS
m
E0
EF
EF
Fig. 9.24 Energy band diagram of a depletionmode HEMT under different gate biases. a V GS < V T such that the channel is turned off. b Under a high forward gate bias, the 2DEG is saturated
368 10
Sheet carrier concentration, Ns (x1011 cm )
Fig. 9.25 Measured gatevoltage dependence of the sheet carrier density of 2DEG in the GaAs/AlGaAs system. W sp represents the spacer layer thickness in each sample. All samples have N d = 4.6 × 1017 cm−3 except sample No. 76, which has N d = 9.2 × 1017 cm−3 . Reprinted with permission from [6], copyright AIP Publishing
9 Heterostructure Electronic Devices
Wsp =
8
0Å (R98A)
DHEMT Ndepl = 5 x 1010 cm x = 0.3
6
45 Å (R73A)
at 12K
75 Å (R72A) 4 180 Å (R76A) 2
0
Gate voltage, VGS (V)
2 is relatively small. The major term controlling V T is V P = (q Nd /2) Wd − Wsp , which mainly depends on W d . Therefore, one can design the operation mode of the device by selecting the proper barrier thickness as shown in Fig. 9.26. For example, a thick barrier (large W d ) leads to a larger V P and a more negative V T . A conduction channel is formed in such a HEMT structure even at zero gate bias (Fig. 9.26a). One has to apply a gate bias equal to V T to completely deplete the 2DEG, thus forming a depletionmode (normallyon) HEMT. When the barrier layer is reduced to a point such that the Fermi level is well below the ground state (E 0 ) of the triangular QW at
Fig. 9.26 Schematic band diagram at V GS = 0 for a normallyon and b normallyoff HEMTs
9.4 Operation Properties of the HEMT
369
zero bias, V T becomes positive. A positive gate bias is required to induce the 2DEG for current conduction, and the HEMT is an enhancementmode (normallyoff) FET (Fig. 9.26b).
9.4.3 Current and Voltage Characteristics of HEMT The drain–source conduction current can be expressed similarly as in a MESFET. IDS = q Z N S υd (F)
(9.58)
where Z is the gate width, N S is the 2DEG density, and υ d (F) is the electron drift velocity. Since there is a voltage drop, V x , between source and drain, it should be included in the N S expression of (9.57) as NS =
(VGS − VT − Vx ) q(Wd + W )
(9.59)
Depending on the field strength, the drift velocity along the conduction channel can be modeled with a linear region and a saturation region with the critical field intensity, F C , as the deflection point in the υ d versus F plot. υd (F) =
μF for F < FC υsat for F > FC
In the linear region (F < F C ), let F = IDS = q Z N S μF =
(9.60)
dVx : dx
μ Z dVx (VGS − VT − Vx ) dx (Wd + W )
(9.61)
Since the conduction current in the channel remains constant under a fixed drain bias, the total current can be calculated through integration along the channel length, L. L
VDS dx =
IDS 0
0
μ Z (VGS − VT − Vx )dVx (Wd + W )
(9.62)
Thus, the drain current as a function of drain voltage under fixed V GS is expressed as IDS
2 μ Z VDS = (VGS − VT )VDS − L(Wd + W ) 2
(9.63)
370
9 Heterostructure Electronic Devices
2 At very low drain bias, the VDS /2 term is very small and can be neglected. The drain current is linearly proportional to the drain bias. At a sufficiently high drain bias, 2 /2 term becomes significant and leads to a sublinear I DS V GS characteristic. the VDS Further increasing the drain bias, the drain current becomes saturated. The effectiveness of current control by the gate bias voltage is determined by the transconductance, gm . At a fixed V DS , gm is calculated as the variation of drain current per gate bias change.
μ dIDS Z VDS μ ∝ = gm = dVGS VDS L (Wd + W ) L
(9.64)
It is clear that large lowfield electron mobility and a short channel length are required for a HEMT to achieve a high gm at a fixed V DS . Within the linear region, gm increases with increasing V DS . In the saturation region (F ≥ F C ), the drift velocity does not increase with the electric field but has a constant value called the saturation velocity, υ sat . Therefore, the current becomes a constant, I DS (sat) = qZN s υ sat and dIDS (sat) μ Z = [(VGS − VT ) − VDS ] = 0 dVDS L(Wd + W )
(9.65)
From this equation, the threshold saturation voltage is calculated as V DS (sat) = V GS − V T . Using this relation in I DS , the I–V characteristic in the saturation region is expressed as IDS (sat) =
μCb Z (VGS − VT )2 μ Z (VGS − VT )2 = L(Wd + W ) 2 L 2
(9.66)
where Cb = /(Wd + W ) is the capacitance per unit area in the barrier. The transconductance in the saturation region can also be derived as dIDS (sat) μCb Z μ = gm = (VGS − VT ) ∝ dVGS VDS L L
(9.67)
Again, large lowfield electron mobility and a short channel length are required to achieve a high gm in the saturation region.
9.4.4 Microwave Noise Performance The essential elements of the highspeed performance of HEMTs are very similar to those of conventional MESFETs. Therefore, a common microwave equivalent circuit model can be used for both devices. Consider the case where the FET is operating at a frequency below its cutoff frequency, f T , at room temperature. The microwave
9.4 Operation Properties of the HEMT
371
noise performance of the HEMT can be derived from the equivalent circuit by the same classical noise model of the MESFET. The minimum noise figure F min for the HEMT is described as Fmin = 1 + K f ( f / f T ) gm (RG + RS )
(9.68)
where gm , RG , and RS are the transconductance, gate resistance, and source resistance, respectively. K f is a fitting factor and represents the quality of the channel material. Since all external device parameters for both HEMT and MESFET can be made roughly equal, the noise performance difference between the two devices originates in the K f difference. It was suggested that the size of K f is related to excess noise in the drain current, which originates as diffusion noise in the channel. For GaAs MESFETs, K f ≈ 2. In HEMTs, the electrons are narrowly confined to a quantized state along the interface rather than in a 3D configuration. Monte Carlo simulations indicated much lower diffusion coefficients as a function of electric field than those of MESFETs. Experimental K f for HEMTs have values between 1 and 2. Therefore, HEMTs have a better microwave noise performance than MESFETs. In addition, since f T can be much higher for HEMTs, we also expect a lower noise figure in HEMTs.
9.5 Optimal Design of the HEMT Based on discussions above, to achieve high performance, the optimized HEMT structure should incorporate a large E c (≥0.5 eV) for high sheet carrier density N S and high current carrying capability; furthermore, materials with high electron mobility should be selected for efficient highspeed operation, and small gate length (L g < 0.1 μm) should be used to increase the cutoff frequency. In addition, to enhance electron transfer from the barrier into the triangular QW, a small spacer layer thickness (W sp ~ 25 Å) is preferred. However, in practice, it was not straightforward to realize all these requirements in the early development of HEMTs. Specifically, the DX center problem severely limited the use of Alx Ga1−x As with high aluminum content (x ≤ 25%) in the HEMT design. In addition, when increasing the barrier doping level to achieve higher 2DEG density, parallel conduction from free electrons trapped in the barrier and 2DEG could form. To overcome these problems, a pseudomorphic layer and deltadoping designs are incorporated to increase E c and 2DEG density.
372
9 Heterostructure Electronic Devices
9.5.1 DX Center in SiDoped AlGaAs/GaAs HEMT and Delta Doping As discussed in Chap. 4, Sidopants in AlGaAs can take different crystal configurations: interstitial (relaxed state, DX center) or substitutional (excited state). The DX center is a deep trap that requires different energies for capture and emission of electrons. Further, the finite capture barrier makes it difficult to achieve equilibrium at low temperature ( 800 GHz has been demonstrated in InP/InGaAs HBTs [12]. New functions, such as highspeed spontaneous and stimulated light emission, have also been demonstrated in HBTs (lightemitting transistors and transistor lasers) [13]. The HBT inherits all the advantages of the BJT including high cutoff frequency due to the short transient time across the thin base region, uniform turnon voltage which is determined by the builtin potential of the junction, high power capability resulting from the entire emitter area conducting current, and high transconductance which enables lowpower applications. By adding a heterojunction to the BJT, additional advantages emerge. The energy band discontinuity at the emitter–base (EB) heterojunction of a HBT suppresses the diffusion of majority carriers from the base
9.7 Heterojunction Bipolar Transistors (HBTs)
383
into emitter for higher gain. The EB heterojunction also allows the use of a highly doped base region for low base sheet resistance without lowering gain. This means a very thin base layer can be used for a shorter transient time to achieve a higher cutoff frequency. It is expected that HBTs have higher current gain and cutoff frequency than BJT. At the onset of HBT development, only one heterojunction was used at the EB junction of a single heterojunction bipolar transistor (SHBT). The emitter region of the GaAsbased SHBT is replaced by a larger bandgap AlGaAs, and the base– collector (BC) junction remains a GaAs homojunction. To enhance the breakdown voltage performance of a HBT, a larger bandgap material, such as AlGaAs, is used in the collector region. In this case, both EB and BC junctions are replaced by AlGaAs/GaAs heterojunctions to form a doubleheterojunction bipolar transistor (DHBT). Currently, HBTs using different material systems have been developed including Inx Ga1−x P/GaAs, InP/Inx Ga1−x As, Si/Six Ge1−x , and InP/GaAs x Sb1−x for various applications. Obviously, heterojunctions with either typeI or typeII energy band discontinuity can be used in HBT designs.
9.7.2 Basic Theory of Heterojunction Bipolar Transistors The energy band diagram of a type I Np+ n SHBT under normal operation is shown in Fig. 9.38. To generalize the discussion, the heterointerface of the HBT is graded such that the effect of the EB junction energy spike in the conduction band is neglected. The energy bandgap of the emitter and base are E gN and E gp , respectively. A forward Fig. 9.38 Energy band diagram of an Npn HBT, under normal mode operation, showing the various current components and the holeblocking effect of the valence band discontinuity E v at the EB junction
qVN
In
IE
Ir Is
qVEB qVp
Emitter
IC
Base
Ev Ip
qVCB IB
Collector
384
9 Heterostructure Electronic Devices
bias voltage of V EB and a reverse bias voltage of V CB are applied to EB and BC junctions, respectively. The terminal currents of the SHBT are the emitter current I E , base current I B , and collector current I C . These currents are related to internal current components of the injected electron current into base (I n ), the injected hole current into emitter (I p ), the saturation current at the EB junction (I s ), and the recombination current in the base region (I r ) through the following equations: ⎧ ⎨ IE = In + Is + I p I = I p + Ir + Is ⎩ B IC = In − Ir
(9.72)
The above discussions can also apply to BJTs by simply setting E gN = E gp . The ratio of the collector current and base current defines the current gain of the junction transistor. β=
In − Ir IC = IB I p + Ir + Is
(9.73)
To maximize β, the components in the numerator and denominator need to be maximized and minimized, respectively. The maximum current gain (β max ) is simply the ratio I n /I p in the limit of negligible recombination losses. Assuming a nondegenerate case, the approximate injection electron and hole current densities at the EB junction are Jn = qn B υnB = q NE υnB exp(−q VN /kT )
(9.74a)
J p = qpE υ pE = qpB υ pE exp −q V p /kT
(9.74b)
where N E and pB are the doping level in the emitter and base, respectively; υ nB is the electron mean velocity in the base near the EB junction; υ pE is the hole mean velocity in the emitter near the EB junction; and qV N and qV p are the potential barrier height for electrons and holes, respectively. At the heterojunction, q(V p − V N ) = E gN − E gp = E g , we obtain the maximum current gain (β max ) βmax =
In NE υnB = exp E g /kT Ip pB υ pE
(9.75)
The mean velocity ratio of (υ NB /υ pE ) is the least subject to manipulation. To achieve large β max (>100), it is necessary that either N E pB or E g > kT. Energy gap differences that are several kT are readily available. Due to the exponential nature of the (E g /kT ) term, it dominates β max even if N E < pB . Therefore, using heterojunction structures with large E g , very high maximum current gain can be achieved regardless of the emittertobase doping ratio. It simply means that the hole injection current I p is sufficiently suppressed by a large E v and becomes a
9.7 Heterojunction Bipolar Transistors (HBTs)
385
negligible part of the base current compared to the two recombination currents: I B ≈ I s + I r . If we approximate I E by I n , we obtain β∼ =
In Ir + Is
(9.76)
In a HBT with a highly doped base, the recombination current I r is the dominant current component since the saturation current I s I n for a highquality interface. At the same time, the very high doping density translates into a rather short minority carrier lifetime in the base region. Therefore, the bulk recombination current I r , rather than the interface recombination current I s , will dominate the base current. Thus, I B ≈ I r and equals the total minority carriers (Qn ) stored in the base divided by the minority carrier lifetime (τ n ): Qn q An B WB = = Ir ≈ τn 2τn
q AWB NE exp(−q VN /kT ) 2τn
(9.77)
where A is the crosssectional area of the EB junction and W B is the base width of the device. The current gain of a HBT structure with a large E g and high quality interfaces becomes β≡
2τn υnB In NE υnB exp(−q VN /kT ) = = Ir WB (WB /2τn )N E exp(−q VN /kT )
(9.78)
The effect of the base doping on the minority carrier lifetime and the base width in turn directly affects the current gain. Even if for heavy base doping levels the lifetimes may be short, high β’s should be achievable in HBTs with sufficiently thin base region. Furthermore, in a thin base HBT, the electron velocity is likely to approach its saturation velocity of ~107 cm/s, enhancing the current gain. As a result, no serious concerns arise from reduced minority carrier lifetime in HBTs with heavily doped thin (≤ 100 nm) base region. Now we can examine the current gain property of a BJT. In homojunction bipolar junction transistors, E g = 0. The only way to achieve high current gain is to make N E pB . Since the base doping level is kept low, it requires a thick base layer to minimize the base sheet resistance. A thick base layer will eventually limit the cutoff frequency of the BJT. On the other hand, the doping level in the emitter cannot exceed certain limits. A heavily doped emitter will cause other problems. When the emitter degenerates, the Fermi level can move into the conduction band and cause bandgap shrinkage. This is equivalent to a reduction of conduction band discontinuity at the EB junction or E g < 0. A lowering of β max is expected. Therefore, the HBT takes advantage of the exponential dependency of E g to achieve high gain with high base doping concentration. Furthermore, the doping profile of the BJT is graded due to diffusion and/or ion implantation processes used in device fabrication. For HBTs, a much sharper doping profile is achieved by controlling doping properties during epitaxy. The abrupt and heavily doped base region is desirable for achieving high
386
9 Heterostructure Electronic Devices
Fig. 9.39 Gummel plot for InGaP/GaAs HBT. The emitter size of the HBT is 60 × 60 μm2 . Reprinted with permission from [15], copyright IEEE
Base and collector currents (A)
current gain and high cutoff frequency in a HBT. Thus, it is critical to use a suitable ptype dopant that possesses a high doping efficiency and a low diffusivity. For GaAsbased HBTs, carbon has proved to be an ideal ptype dopant among other common candidates such as Zn and Be. It can be easily doped to over 1020 cm−3 in many III–V compound semiconductors with negligible outdiffusion. However, carbon atoms are hard to generate from a solid source, such as graphite, due to their extremely low vapor pressure. Currently, the heavily ptype carbon doping is conveniently achieved using gaseous carbon sources such as CCl4 (in MOCVD) and CBr4 (in MBE). The current gain of a BJT and HBT is commonly measured using the Gummel plot scheme [14]. A Gummel plot shows the base and collector currents as functions of V BE when V CB = 0. The ratio of the measured I C /I B at various V BE gives the current gain. For the ideal case, both I B and I C are dominated by diffusion current component and proportional to exp(qV BE /kT ). We expect a constant gain independent of bias. In real devices, defects and other recombination centers at the EB heterointerface and in the bulk of the base lead to a nonideal base current with an exp(qV BE /mkT ) dependence. The parameter m is referred to as the ideality factor and has a value between 1 (dominated by diffusion current) and 2 (dominated by generationandrecombination current I s ). Therefore, the EB junction property can be determined by the ideality factor (m) of I B . For example, Fig. 9.39 shows the Gummel plot of an InGaP/GaAs DHBT with an emitter size of 60 × 60 μm2 . At low current, m = 1.84 (~2), I B is mostly due to the generationrecombination current in the depletion region of the EB junction and I s is larger than I r . At midtohigh current, m = 1.15 (~1), showing that the bulk recombination current (I r ) in the base region becomes dominant due to its high doping level. The base current eventually departs from m ~ 1 due to the large voltage drops across the parasitic base and emitter resistances, causing the available junction voltage to decrease. For the collector current, it increases with V BE with an ideality factor of m = 1.07, a value which is close to unity. 10
IC
10
IB
10
n=1 10
n=2
10 10 0.4
0.6
0.8
1.0
1.2
Baseemitter voltage, VBE (V)
1.4
9.7 Heterojunction Bipolar Transistors (HBTs)
387
9.7.3 Band Discontinuity of Heterostructures In a typeI heterostructure, a ‘spikeandnotch’ energy band diagram generally appears at the abrupt heterojunction due to the conduction band discontinuity ΔE c as shown in Fig. 9.40 for a SHBT. This energy spike can be removed by using a graded composition in the large bandgap emitter near the heterointerface as used for discussions in the previous section. The existence of the energy spike at the EB junction of an abrupt HBT can modify the current conduction across the heterojunction. Using the simple thermionic emission model, the magnitude of forward current depends on the amount of electrons having enough energy to surmount the potential barrier. In an abrupt HBT, the potential barrier for electrons is simply V N . However, in a graded HBT, the effective potential barrier becomes (V N − E c /q) since the energy spike, E c , has been eliminated by the graded composition design. Therefore, under the same bias condition, the collector current of the abrupt HBT, I n (abrupt), is reduced from the graded HBT, I n (graded), by a factor of In (abrupt) exp(−q VN /kT ) = = exp(−E c /kT ) In (graded) exp[−(q VN − E c )/kT ]
(9.79)
Since the current gain is proportional to exp(E g /kT) in the graded junction case, the current gain of abrupt HBTs is modified by reducing ΔE c from E g in the injection current relation (9.75). Thus βmax
E g − E c NE υnB NE υnB E v = = exp exp pB υ pE kT pB υpE kT
(9.80)
It is clear that a large E v is preferred in abrupt Np+ n HBT structures for a high current gain.
Fig. 9.40 Energy band diagram for HBT with abrupt emitter–base junction
388
9 Heterostructure Electronic Devices
The existence of the energy spike in the conduction band at the EB heterojunction has other effects on device performance. A beneficial effect is that electrons injected from emitter into the base have to overcome the EB junction barrier with higher potential energy and become hot electrons with high saturation velocity. The improved travel speed across the base region leads to a reduced base transient time for high frequency operation. A detrimental effect is that the energy spike can block current flow at bias voltages V CE < E c /q = V off , which is the offset voltage. Also, the triangular QW formed on the base side of the EB junction can trap electrons that lead to an enhanced recombination at the junction. Therefore, the current gain will be reduced due to an increasing I r . Next, we turn our attention to the BC junction. In a SHBT, the same semiconductor is used for both base and collector and the BC junction is a homojunction. Therefore, the same arguments about the BC junction of a BJT can be applied to a SHBT. In DHBTs, the BC homojunction is replaced with a heterojunction. The use of a wide bandgap collector material can improve the power handling capability by the enhanced breakdown voltage. Again, due to the existence of a finite E c , an energy spike forms at the BC junction as shown in Fig. 9.41. This energy barrier (E c ) impedes free collection of electrons by the reversebiased BC junction. It will suppress the collector current until a large V CE is reached to allow collection of electrons by the collector. Thus, it will increase the minority carrier resident time in the base region, which reduces the bandwidth of the device. Therefore, a graded collector junction in the form of composition grading or chirped superlattice structure is usually used to eliminate this problem. For a latticemismatched material system such as InGaAs/InP, this will complicate the growth procedures and may cause interface problems leading to a lower current gain. The collector current blocking mentioned above can be totally avoided by using a typeII DHBT design. This design simplifies the growth of the BC junction without using composition grading. In particular, for the InP/GaAs0.5 Sb0.5 /InP DHBT design
Collector current (mA)
35
(a)
30
(b)
SHBT DHBT
25 20 15 10 5 0 0
2
4
6
8
10
12
InGaP emitter
GaAs base
Collectoremitter voltage (V)
Fig. 9.41 a Comparison of the I–V characteristics of InGaP/GaAs SHBT and DHBT. The base current was stepped from 0 to 400 μm in 100 μA steps. Reprinted with permission from [16], copyright AIP Publishing. b Current blocking at the base–collector junction of an InGaP/GaAs DHBT
9.7 Heterojunction Bipolar Transistors (HBTs)
389
Fig. 9.42 Energy band diagram of an InP/GaAsSb typeII doubleheterojunction bipolar transistor Ev InP Emitter
GaAsSb Base
InP Colletor
shown in Fig. 9.42, it provides a nearly zero conduction band offset (E c = −0.06 eV, E c (InP) < E c (GaAsSb)) for a negligible turnon voltage and no current blocking effect at the BC junction. The large E v of ~0.62 eV and the use of InP collector material provide a large current gain and large breakdown voltage, respectively.
9.7.4 HighFrequency Operation of HBT The highfrequency performance of HBTs is fundamentally determined by the stored minority carrier charge in the transistor that has to be removed from (added to) the transistor before it can turn off (on). Hence, the maximum frequency at which the transistor is capable of operating depends on the junction capacitance charging time and charge carrier transit time. In forward active operation, the forward transit time τ F or the emittertocollector transit time τ EC represents a fundamental limit for the switching speed and maximum frequency of operation of a HBT. The parameter most commonly used to define this maximum frequency of operation is the cutoff frequency f T . This is the frequency at which the common emitter, smallsignal current gain drops to unity under conditions of a shortcircuit load. In practice, parasitic capacitance and resistance of the HBT will slow down the switching of digital circuits and limit the frequency of operation of analog circuits. To include the effect due to parasitic resistances and junction capacitances, the maximum oscillation frequency f max is a good predictor of transistor performance. (a) Emittertocollector transit time The emittertocollector transit time models the excess charge stored in the HBT under normal operation of a commonemitter configuration. This is an extremely important device parameter, since it sets a fundamental physical limit to the switching speed and maximum oscillation frequency of operation of a HBT. The emittertocollector transit time τ EC can be written as the sum of the individual delay times as well as charging times of junction capacitances in the various regions of the HBT. τEC = τE + τB + τC + τBC
(9.81)
390
9 Heterostructure Electronic Devices
where τ E , τ B , τ C , and τ BC are the emitter delay time, base transit time, collector transit time, and base–collector spacecharge layer delay time, respectively. The emitter delay τ E associates the emitter junction charging time involving the emitter–base junction capacitance C E and the dynamic emitter resistance kT /qI C . τE =
kT CE q IC
(9.82)
The base delay τ B represents the transport of electrons through the base layer via drift, diffusion, or ballistic transport. In the limit of diffusion current only, τB ≡
QB IC
(9.83)
with ⎧ ⎪ ⎪ ⎨
q VBE q AWB n B0 QB = exp 2 kT dn n q VBE B0 ⎪ ⎪ = q ADnB exp ⎩ IC = q ADnB dx WB kT Thus, τB =
WB2 2DnB
(9.84)
W B is the base width, DnB is the electron diffusion constant, and nB0 is the equilibrium electron concentration. This result of τ B is valid for HBTs with a uniform base. If the base is nonuniformly doped or has a composition gradient, then the variation in doping and/or bandgap energy gives rise to a builtin electric field across the neutral base region. This builtin field would aid electron transport across the base and hence reduce the base transient time. This situation can be taken into account by modifying the equation as τB =
WB2 γ DnB
(9.85)
where γ is a constant that has a value of 2 ≤ γ ≤ 4. The collector transit time τ C corresponds to the transport time through the collector layer, is classically found to be proportional to the collector thickness W C , and is expressed as τC =
WC 2υsat
(9.86)
9.7 Heterojunction Bipolar Transistors (HBTs)
391
where υ sat is the electron saturation velocity in the collector, typically measured as 3–4 × 107 cm/s. The last term τ BC represents the charging time delay associated with the parasitic BC junction capacitance C BC . For an incremental input voltage change dV BE , the BC junction voltage change is dVBC = dIC (RC + RE + kT /q IC )
(9.87)
where RC and RE are the parasitic collector and emitter resistances, respectively. Therefore, τBC = (RC + RE + kT /q IC )CBC
(9.88)
The total delay associated with a HBT is directly related to the cutoff frequency and can be described as fT =
−1 1 kT = 2π τB + τC + (RE + RC )CBC + (9.89) (CE + CBC ) 2π τEC q IC
Since f T is defined for smallsignal conditions, a smallsignal circuit model, such as the hybridπ model, as shown in Fig. 9.43, can be used to derive an expression for f T . To a first order, the series resistances of three terminals and recombination in the depletion region were neglected. Under the conditions of a shortcircuit load, the smallsignal collector and base currents can be written as
B
i c = gm vbe − iωCμ vbe
(9.90)
i b = gπ vbe + iω Cμ + Cπ vbe
(9.91)
Cμ
ib
C
C
r
E Fig. 9.43 Smallsignal hybridπ circuit model of HBT
gmVbe
ic
E
392
9 Heterostructure Electronic Devices
where gπ = 1/r π (r π is the equivalent input resistance), ω = 2π f, gm is the transconductance, C π is the BE junction diffusion capacitance, and C μ is the BC junction diffusion capacitance. The commonemitter current gain can be written as β=
gm − iωCμ ic g ∼ = m = ib gπ + iω Cμ + Cπ gπ + iω Cμ + Cπ
(9.92)
If we define β 0 = gm r π , the equation can be simplified as β=
β0 1 + iωrπ Cμ + Cπ
(9.93)
At low frequencies, the current gain maintains a constant value of β = β 0 . As the frequency increases, the second term in the denominator of the equation becomes large with respect to unity, and β can be approximated by β =
β0 2π f rπ Cμ + Cπ
(9.94)
At high frequencies, β begins to roll off with a limiting rolloff rate of −20 dB/decade (∝1/f ). The frequencydependent gain values are determined from Sparameters measured with microwave network analyzers. The gain values (in dB) as functions of frequency are usually plotted in a semilog fashion under constant V CE = V BE and I C as shown in Fig. 9.44a. For very highspeed devices, the gain at frequencies exceeding the limit of instrument capacity was obtained by extrapolating −20 dB/decade lines from a bestfit average of the measured current gain. Since τ EC is a function of the collector current, the cutoff frequency is also a function of the collector current as illustrated in Fig. 9.44b. At low collector currents, the
Fig. 9.44 a RF response and performance figure extrapolations for 0.25 × 16 μm2 InP/InGaAs SHBT. Reprinted with permission from [17], copyright IEEE. b f T and f max as a function of collector current density of a 0.35 × 8 μm2 typeII InP/GaAsSb DHBT. Reprinted with permission from [18], copyright American Vacuum Society
9.7 Heterojunction Bipolar Transistors (HBTs)
393
depletion capacitance term (τ BC ) in (9.89) dominates and hence f T increases with I C . At medium currents, the transit time terms become larger than the depletion capacitance term, and f T ceases to rise with collector current. At high collector currents, the cutoff frequency decreases markedly due to high current effects, especially the Kirk effect which will be described later. The other important highfrequency parameter for a HBT is the maximum oscillation frequency f max , where the unilateral power gain (U) drops to unity. The unilateral or Mason gain is the maximum gain obtained by conjugate matching of inputs and outputs of the device, together with the use of a lossless feedback network to tune out any internal device feedback. The derived expression of the maximum oscillation frequency is f max =
fT 8πC BC R B
(9.95)
which shows that the f max is determined not only by the f T but also by BC junction capacitance C BC and the base resistance RB . It is clear that a high ptype doping concentration in the base region leads to a low base sheet resistance and an improved f T , both of which enhance the f max . On the other hand, the increase in f T due to reduced τ BC by higher collector doping could increase C BC and may cause a decrease in f max , depending on the relative importance of τ BC in f T . Therefore, for highfrequency circuit applications, a careful optimization of these two parasitics is required. (b) Kirk effect The reduction of f T at high collector current mentioned in the last section is due to a base widening or Kirk effect. Consider Poisson’s equation in the depletion region of the BC junction: ρ q dF = = ( p − n + Nd ) dx
(9.96)
where p and n are mobile charges and N d is the fixed (ionized) charges. In the reversebiased collector of Npn HBT structures, p ≈ 0 and electrons injected from the emitter are transported across the BC junction by drift under high field situations. The electron concentration relates the drift current density J n by n = J n /qυ sat , where υ sat is the electron saturation velocity. Thus, 1 Jn dF = q Nd − dx υsat
(9.97)
This equation indicates that the slope of the electric field intensity depends on the difference of qN d and J n /υ sat . Under low current density, the contribution from the mobile electrons can be neglected and dF/dx is unchanged (Fig. 9.45). At sufficiently
394
9 Heterostructure Electronic Devices
Fig. 9.45 Electric field intensity distribution in the fully depleted collector region under large collector current density. With further increase of collector current density, the slope of the electric field intensity curve changes from positive to negative as indicated by the arrow
large collector current density, the BC depletion region can extend all the way to the n/n+ subcollector boundary. For a fixed V CB , the depleted collector region where the electric field F exists is fixed and dF/dx still maintains a positive slope. With further increasing the collector current density (J C ), the mobile charge in the depletion region becomes significant and cannot be neglected. This leads to a decreasing F with increasing J C or a decreasing dF/dx slope. At certain J C , F = 0 and the depleted collector layer turns into a neutral layer. Holes can be injected freely from the base into the adjacent neutral collector region. With the injected holes, the conductivity type of the collector adjacent to base changes from n to p. Thus, the effective base thickness is increased at high collector current density, which degrades the cutoff frequency of the HBT as shown in Fig. 9.44b. (c) Device scaling and surface passivation Earlier studies of HBTs have shown that a significant component (>75%) of the total device delay was associated with the intrinsic forward delay of the device, primarily the base and collector transit times. Therefore, an effective method to increase the cutoff frequency f T of the HBT is through vertical scaling of the base and collector epitaxial layers. Vertical scaling strictly involves the design of layer thicknesses, doping levels, and bandgap engineering to reduce device transit time, thereby increasing device bandwidth. Figure 9.46 shows the experimental relationship between vertical scaling and base/collector transit times. The base transit time is clearly illustrated by two slopes. For thicker bases, the classic diffusion transport dominates and is proportional to (W B )2 . As the base thickness is scaled below the mean free path for electrons (~30 nm), the ballistic transport dominates with a linear dependence on W B . However, as the base and collector layers are thinned, parasitic resistances and capacitances also increase—specifically the base resistance, RB , and the base/collector capacitance, C BC . The increase of these parasitic components acts to severely degrade the maximum oscillation frequency f max of the device.
9.7 Heterojunction Bipolar Transistors (HBTs)
395
Fig. 9.46 Experimental results on the relationship between vertical scaling of InGaAs/InP SHBT and base/collector transit times
For effective reduction of transit times in HBTs without incurring significant increases in charging delays, vertical and lateral scaling must be simultaneously employed in order for submicron devices to achieve high performance. Lateral scaling refers to device topology design and processing techniques used to reduce parasitic capacitances and resistances to further enhance device speed. Lateral scaling also has the benefit of providing lower power operation and more efficient heat removal; reducing the emitter length lowers the thermal resistance of the HBT, allowing for higher current densities and lower junction temperatures. Figure 9.47 shows the peak f max and f T values versus emitter dimensions of InP/InGaAs SHBTs. For the 0.25 μm emitter width (W E ), a 76% improvement in f max is observed from reducing emitter lengths (L E ) from 12 μm to 1 μm; shrinking the emitter width from 0.4 μm to 0.25 μm results in an l8% f max increase. Beyond a certain point, however, scaling has detrimental effects on device performance due to physical limitations imposed by shrinking device dimensions. The
Fig. 9.47 Experimental results on the relationship between emitter lateral scaling of InGaAs/InP SHBT and cutoff frequency
396
9 Heterostructure Electronic Devices
significant drop in f T observed in Fig. 9.47 for emitter lengths 8 μm and smaller on a standard InGaAs emitter cap is attributed to an increase in emitter resistance due to smaller contact areas. Ideally, scaling theory predicts that f T should remain constant regardless of emitter length. However, the finite cap doping causes large increases in contact resistance for these emitter areas. The emitter cap cannot be doped higher due to solid solubility limits, but emitter contact resistance can be reduced through emitter cap engineering by using a narrowbandgap cap material such as InAs. InAs provides a better contact material because of the smaller bandgap, higher doping capability, and higher thermal conductivity when compared to a standard InGaAs cap. The utilization of an InAs emitter cap is shown to reduce the emitter contact resistance by a factor of 2 in submicron HBT devices. The contact resistance reduction enhances the scalability of the emitter by allowing the emitter length to scale to dimensions smaller than 4 μm before the f T degradation occurs. Overall, lateral scaling is often dependent on process maturity, relying on advanced fabrication techniques to counteract the effects of vertical scaling on f max . Therefore, for HBT development using a new material system, the best indication of the system’s potential is determined by the f T of the transistor. It is assumed that as the process matures, the power gain of the device will be increased through technological advances. In general, the HBT has a vertical geometry with an intrinsic device size defined by the emitter contact area. The base contact is designed to surround the intrinsic base region underneath the emitter. Unavoidably, there is an exposed extrinsic base region between the base contact and the intrinsic base area. Consequently, in HBTs made of materials with a high surface recombination velocity (SRV), such as GaAs (SRV > 106 cm/s), some minority carriers injected from the emitter recombine with the base majority carriers on the exposed surfaces resulting in the extrinsic base surface recombination current. This base current component is proportional to the magnitude of the emitter periphery rather than the emitter area. As the size of the emitter is reduced, the emitter perimetertoarea ratio increases and surface recombination current becomes a major part of the overall base current. The current gain of such a scaled down GaAs–base HBT is substantially reduced from that of a large device whose perimetertoarea ratio is small. The surface recombination current problem can be reduced by passivating the exposed extrinsic base region that is not directly under the emitter with an emitter ledge as shown in Fig. 9.48. A thin ledge of emitter material left surrounding the emitter mesa can dramatically reduce surface recombination current and improve device scaling. The exposed ledge layer outside Fig. 9.48 Crosssectional drawing of a HBT with emitter ledge passivation. The emitter ledge (hatched area) is totally depleted such that the base current underneath is not affected
9.7 Heterojunction Bipolar Transistors (HBTs)
397
the emitter mesa is totally depleted, and no carriers are available for recombination at the surface. Therefore, the base current is not affected and current gain is preserved. On the other hand, the free Inx Ga1−x As surface shows more ideal surface characteristics with a small SRV of 103 cm/s for an In composition x ~ 0.5. Therefore, for HBT materials with low SRV such as in InP/InGaAs HBTs, the surface recombination current is not significant even in small devices and the surface passivation is not required.
9.7.5 Basics of HBT Processing The design of HBTs is intimately interwoven with the technologies used for their fabrication. Therefore, any study of the HBT would be incomplete without understanding the fabrication technology. A typical HBT process developed at the University of Illinois at UrbanaChampaign (UIUC) is discussed below for either InGaP/GaAs or InP/InGaAs highfrequency HBTs. Other research groups may have developed their own HBT process steps, but the principal ideas discussed below remain the same. The standard InGaP/GaAs HBT structure is a single heterojunction device grown on a semiinsulating GaAs substrate that employs a carbondoped GaAs base, a latticematched InGaP emitter, and a thin InGaAs emitter contact layer. Figure 9.49 shows a series of device profiles detailing the highspeed HBT process
Fig. 9.49 Crosssectional diagrams of UIUC HBT process: a postemitter contact liftoff, b postbase etch, c postbase contact liftoff, d postcollector etch, e postisolation etch, f postcollector contact liftoff, g postpolyimide/SiNx passivation, h postSiNx via etch, and i postoverlay metal liftoff
398
9 Heterostructure Electronic Devices
Fig. 9.50 Left: Top view SEM micrograph of a fully fabricated GaAsSb/InP DHBT before planarization with an emitter size of 0.25 × 5 μm2 . Right: Crosssectional SEM micrograph of a completed GaAsSb/InP DHBT with an emitter size of 0.35 × 5 μm2 . Courtesy M. Feng, University of Illinois at UrbanaChampaign
sequence. Initially, in Fig. 9.49a, nonalloyed metal contacts are deposited on the InGaAs emitter contacting layer. The cap and emitter material are then selectively chemically etched using the emitter metal as a mask, and this etch is followed by a selective InGaP emitter etch. This etching sequence provides an approximately 0.2 μm undercut beneath the emitter metal, which is necessary for the deposition of selfaligned, nonalloy base contact (Fig. 9.49c). After the base metallization, the base and collector are chemically etched, leaving the subcollector exposed (Fig. 9.49d). Before the collector metallization, an etch of approximately 1000 Å into the substrate is performed to electrically isolate the HBT (Fig. 9.49e). Next, the collector contacts are deposited on the collector mesa and overlap the edge of the isolation mesa (Fig. 9.49f). By allowing this overlap, the active collector contact area near the edges of the mesa is maximized and the collector contact resistance is reduced. The HBT device structure has now been defined. Figure 9.50a shows the scanning electron microscope (SEM) topview micrograph of a fully fabricated singlefinger GaAsSb/InP DHBT with an emitter size of 0.25 × 5 μm2 . At this point, the HBT has a nonplanar topology. In order to make the HBT structure more planar to facilitate both via etching and the formation of planar probe pads for highfrequency testing, a planarization process (Fig. 9.49g) is required. The spinon polyimide followed by a deposited Si3 N4 layer completes the planarization process. Contact vias are defined using standard photolithography process (Fig. 9.49h). After the vias have been etched, a 1 μm layer of overlay metallization is deposited to form the probe pads and interconnect metallization. In the last step, an airbridge process is utilized to produce a second level of plated interconnect metallization allowing emitter fingers to connect to commonemitter probe pads. The crosssectional SEM micrograph of a GaAsSb/InP DHBT with an emitter size of 0.35 × 5 μm2 is shown in Fig. 9.50b.
9.8 III–V MetalOxideSemiconductor FieldEffect Transistors
399
9.8 III–V MetalOxideSemiconductor FieldEffect Transistors Silicon metaloxidesemiconductor fieldeffect transistor (MOSFET)based integrated circuit (IC) technology is the dominant semiconductor technology used by all electronics industries with a 2018 worldwide sales of over $470 billion. Miniaturization of the feature size of ICs to increase the density of components has been the foundation of the over 50yearlong steady advance of silicon technology. Following Moore’s law, the exponential increase of transistor count per unit area as a function of time has been faithfully delivered by the industry since 1970. The minimum transistor gate length also decreases with time exponentially by incorporating strained SiGe channel material, highκ gate dielectrics, and nonplanar multigate structures (see Fig. 1.4). Although 5nmnode CMOS circuits are on the horizon, further reduction of the feature size to below 2 nm will push the device structure into the quantum regime. At that moment, the silicon technology will reach the point at which significant materials and device innovations will be required to further technology developments. One possible solution for the future is the hybrid material system in which silicon, germanium, and III–V compound semiconductors are integrated together on silicon wafers. For example, taking advantage of the very high electron mobility in GaInAs and high hole mobility in germanium, advanced CMOS circuits consisting of nGaInAs channel and pGe channel MOSFETs might be fabricated together on the silicon wafer. Because of their high bulk electron mobility, III–V MOSFETs have long been pursued in hopes of achieving performance superior to that of their Si counterpart. However, due to the high surface state density, the realization of unpinned surface Fermi level in III–V compound semiconductors had been elusive until two decades ago. In searching for a low defect density, thermodynamically stable gate dielectric, native oxide and deposited oxide using a variety of deposition techniques have been investigated. Unlike the SiO2 /Si system, the native surface species in III–V materials are complicated. For example, the stable oxides of GaAs consist of As2 O3 , As2 O5 , Ga2 O3 , Ga2 O, and GaAsO4 with different thermodynamic properties. Among all native oxides in this system, the Asoxides are the least stable while Ga2 O3 is the most stable oxide. When the lowtemperaturegrown oxides are annealed at higher temperature, the composition of the oxide layer changes significantly. As temperature increases, the less stable Asoxides either evaporate away or are converted to the most stable oxide in the system (Ga2 O3 ) along with elemental arsenic located at the interface. The pinning of the Fermi level at the GaAsoxide interface has been unambiguously correlated with significant amounts of As2 O3 , As2 O5 , and elemental As present in native oxides. In order to fabricate functional III–V MOSFETs, it is necessary to completely remove the surface native oxide first before a stable and robust dielectric can be deposited. Thus, the successful development of III–V MOSFET technology relies strongly on the surface passivation and interface control technology.
400
9 Heterostructure Electronic Devices
9.8.1 III–V Alloy Surfaces and SemiconductorOxideMetal Interfaces The semiconductor surface state model was first proposed by John Bardeen in 1947 to explain the Fermi level pinning phenomenon at the metal–semiconductor (M–S) interface. It is assumed that the distribution of surface states becomes chargeneutral if the states are filled to a particular energy level, φ 0 (above E V = 0), inside the forbidden gap. In the strong pinning limit, the metal Fermi level is pinned by the interface states at φ 0 . The pinning energy level φ 0 is then the charge neutrality level of the interface states. Since then, two principal models, the intrinsic model of metalinduced gap states (MIGS) and the extrinsic model of defect states, have been developed. In the intrinsic case, a semiconductor in contact with a metal contains intrinsic states inside its band gap which are the evanescent tails of the metal wave function decaying into the semiconductor. These states are the danglingbond states of the broken surface bonds of the semiconductor and called MIGS. On the other hand, in the extrinsic case, the interface states are introduced near the surface by processinginduced bond disorder (e.g., disorder caused by metal deposition, etching, or chemisorption of oxygen). In general, both types of interface states, MIGS and defects, could cause pinning. However, there is no universally accepted model for the MS interface. Nevertheless, these studies of MS contact have enriched our understanding of the chemistry and physics of III–V surfaces, such that III–Voxide interface models can be developed. (a) Empirical CNL model of MS interfaces In semiconductors, the danglingbond energy is typically located inside the band gap and the interface trap density (Dit ) increases exponentially in the energy ranges close to the band edges. The Dit distribution forms a Ushaped continuum of donor and acceptortype states with its minimum, or the pinning energy, located at the charge neutrality level (CNL). The CNL energy level represents a weighted average value over the density of states. CNL is pushed away by the large DOS of the conduction and valence bands from the intrinsic energy level E i , as shown in Fig. 4.21. Therefore, the semiconductor surface pinning energy CNL is located inside the forbidden gap for most semiconductors. If the Fermi level E F is above CNL, the states are of acceptor type and negatively charged if the states are occupied. If the Fermi level E F is below CNL, the states are of donor type and positively charged if the states are occupied. The CNL energies can be calculated from their pseudopotential band structures. The CNL values (above E v = 0) of III–V binaries are determined by averaging values derived from various theoretical models as shown in Table 4.5. The experimental CNL values of the semiconductors can be extracted from Schottky barrier heights. In general, the calculated CNL is in close agreement with Schottky barrier heights (φ bv ) on ptype III–V binary compounds. Thus, one can determine the surface pinning energy of III–V binary and ternary compound semiconductors empirically based on the valence band alignment method developed by S. Tiwari and D. J. Frank (Sect. 6.1). Figure 9.51 shows the complete roomtemperature conduction bandedge
9.8 III–V MetalOxideSemiconductor FieldEffect Transistors
401
Fig. 9.51 Energy alignment of CNL with the band edges of elemental and III–V semiconductors at MOS interfaces plotted as a function of the lattice constant of semiconductors. For III–V compounds, the circles indicate the band edges of binaries and the lines show the band edges of ternaries
and valence bandedge energies as a function of the lattice constant for unstrained III– V compound semiconductors. This is the same figure that Tiwari and Frank derived (Fig. 6.5) for band discontinuity determination except the zero point of the energy is now representing the charge neutrality level (CNL) or trap neutral level (φ 0 ) for each lattice constant group. In the case of Si, the stateoftheart SiO2 /Si interface has very low interface trap density of 109 –1010 /cm2 −eV. Although the energy separation between CNL is ~0.6 eV and ~0.5 eV from the conduction band minimum (CBM) and valence band maximum (VBM), respectively, the Fermi level is unpinned. Thus, highperformance nMOSFETs and pMOSFETs are routinely fabricated. In the case of GaAs, CNL is far away from CBM (~0.8 eV) and VBM (~0.6 eV) so that both GaAs nMOSFET and pMOSFET are difficult to realize when significant interface traps presented. It is interesting to note that CNL is inside the conduction band of InAs. This indicates that InAsbased nMOSFETs are easy to realize. For example, T. Brody and H. Kunig, in 1966, demonstrated both enhancement and depletionmode MOSFETs using evaporated SiO2 on InAs film prepared by coevaporation method. One interesting ternary system is InGaAs where the CBM of Inrich InGaAs intersects CNL at x InAs ~ 0.75. Thus, Inrich InGaAs nMOSFET is relatively easy to achieve. For device applications, the next important issue after unpinning the Fermi level is achieving strong electron inversion in III–V MOSFETs. This can be explained using the distribution of the density of the surface states Dit as a function of the energy as shown in Fig. 9.52. It is assumed that the Dit distribution from VBM to CBM (with energy E CBM ) is nearly parabolic in a logarithmic scale due to the significant interface traps at III–V interfaces. The minimum value of Dit depends on the surface processing techniques. For simplicity, the Dit value at CBM is fixed at 1014 cm2 −eV
402
9 Heterostructure Electronic Devices
Fig. 9.52 Schematic for the parabolic Dit distribution within energy band of GaAs and In0.53 Ga0.47 As. The CNL is aligned 0.8 eV and 0.27 eV below CBM for GaAs and In0.53 Ga0.47 As, respectively. The shaded area shows the builtup negative charges in interface traps after Fermi level moves from CNL to CBM. Reprinted with permission from [19], copyright AIP Publishing
for all III–V compounds and has a minimum value located at CNL (with energy E CNL ). Assuming the strong electron inversion occurs when the Fermi level reaches CBM, the number of interfacetrapped negative charges Qit can be calculated by integrating Dit from E CNL to E CBM . It is obvious that the dominant factor is the energy difference between E CNL and E CBM . The builtin negative charges Qit to prevent a strong inversion charge to participate in transport are larger for the material with a deep CNL below CBM. For example, in GaAs, with the CNL located ~0.8 eV below CBM, it builds up ~10−6 C/cm2 negative charges to prevent a strong inversion charge to participate in transport. In contrast, the CNL and CBM potential difference for In0.53 Ga0.47 As latticematched with InP is only 0.27 eV. The builtup negative charge is only ~3.4 × 10−7 C/cm2 , a factor of three smaller than that in GaAs. Therefore, it is much easier to realize an inversionmode In0.53 Ga0.47 As/InP MOSFET than a GaAs MOSFET. (b) Highκ dielectrics and oxidesemiconductor (OS) interfaces Scaling of the silicon complementary metaloxidesemiconductor (CMOS) FET technology is at the center of Moore’s law. The exponential increase of transistor count per unit area as a function of time has been faithfully delivered by the industry since 1970. The minimum transistor gate length also decreases with time exponentially. However, when the feature size is reduced to below 65 nm, the SiO2 gate dielectric layer becomes so thin (1 eV) conduction band offset for MOSFET applications.
404
9 Heterostructure Electronic Devices
Table 9.3 Experimental bandgap energy (E g ), dielectric constant (κ), electron affinity (EA), and optical dielectric constants (∞ ) of various highκ oxides along with the calculated charge neutrality level energy above the valence band edge (E CNL ) [20–22] E g (eV)
κ
E CNL (eV)
EA (eV)
aAl2 O3
6.3
7.5 [21]
3.2
3
∞ 3.2
HfO2
6
25
3.7
2.2
4
ZrO2
5.8
25
3.6
2.4
4.8
Y2 O3
5.7
15
2.4
1.84
4.4
La2 O3
6.0
30
2.4
1.9
4
Gd2 O3
6
10 [22]
2.4
2.5
3.8
Table 9.4 Calculated conduction band offsets (E c , in eV) of various highκ oxides on III–V semiconductors [20] Al2 O3
HfO2
ZrO2
Y2 O3
La2 O3
Gd2 O3
GaP
0.67
0.77
0.73
1.65
1.65
1.2
InP
1.7
1.72
1.64
2.6
2.6
2.1
AlAs
0.97
1.05
1.0
1.9
1.9
1.5
GaAs
1.46
1.52
1.42
2.4
2.4
1.9
InAs
2.38
2.54
2.44
3.4
3.4
2.9
GaSb
1.50
1.58
1.53
2.46
2.46
2.0
InSb
2.08
2.18
2.14
3.06
3.06
2.62
GaN
0.86
1.15
1.08
2.02
2.02
1.57
9.8.2 Atomic Layer Deposition (ALD) Atomic layer deposition (ALD) is a vaporphase film growth method used to deposit ultrathin, uniform, conformal, and pinholefree films onto a substrate. It was invented in the 1970s for the production of largearea flatpanel displays. Strong interest in ALD by the semiconductor industry began in the mid1990s stemming from the need for nonnative oxides for continuous scaling of Si MOSFET devices. In 2007, Intel successfully integrated an ALD Hfbased highκ dielectric process into its 45nmnode mass production technology. In the meantime, efforts to find nonnative oxides on GaAs with low interfacial states density have found a solution in UHV deposition of amorphous Ga2 O3 (Gd2 O3 ) and singlecrystal Gd2 O3 on GaAs surface. After this breakthrough in material science, both depletionmode and enhancementmode GaAs MOSFETs were demonstrated using Ga2 O3 (Gd2 O3 ) as a gate dielectric along with an ion implantation process. The investigation of ALD highκ Al2 O3 and HfO2 on GaAs and other III–V materials for the fabrication of III–Vbased MOSFETs started in 2001 at Bell Labs. Soon after in 2003, GaAs MOSFETs with ALD Al2 O3 gate dielectric were successfully demonstrated. Since then, the research
9.8 III–V MetalOxideSemiconductor FieldEffect Transistors
405
Fig. 9.53 Schematic representation of an ALD growth cycle leading to the formation of a binary dielectric film using selflimiting surface chemistry. a Precursor A is pulsed and reacts with surface, b excess precursor and reaction byproducts are purged with inert carrier gas, c precursor B is pulsed and reacts with surface, and d excess precursor and reaction byproducts are purged with inert carrier gas. Above procedures are repeated until the desired material thickness is achieved
of ALD highκ dielectrics on III–V substrates has been extended to other material systems including Inx Ga1−x As, InP, InSb, GaSb, and GaN. (a) Principles of ALD An ideal ALD process consists of exposing the substrate surface alternatively to different precursors in a cyclic manner. It differs from CVD technique by keeping the precursors strictly separated from each other in the gas phase. As shown in Fig. 9.53, the process of one ALD growth cycle involves exposure of the substrate surface to alternating precursors A and B introduced sequentially without overlapping. In each alternate precursor pulse, the precursor molecules fully react with the surface in a selflimiting fashion that leaves no more than one monolayer (ML) at the surface. This ensures that the chemisorption reaction stops once all of the reactive sites on the substrate have been occupied. This automatic control of the amount of material deposited is a key feature of ALD. After terminating the pulse of precursor A, an inert gas (typically N2 or Ar) purge follows to remove the excess of unreacted precursor and gaseous byproducts. The second precursor B is then introduced following an inert gas purge to complete one reaction cycle. It should be noticed that only in an ideal case is a monolayer of desired material formed per each reaction cycle. In practice, the material thickness is determined by the nature of the precursorsurface interaction and only a fraction of a monolayer is formed. The ALD cycle can be performed multiple times to increase the film thickness. Typically, the process of ALD is performed at relatively low temperatures (104 ) at V CC = 0.5 V. Recent demonstration of highperformance devices described above has already laid a solid foundation in achieving this goal. Second, for CMOS logic applications, there is a need for pchannel MOSFETs with very high hole mobility. Although III–V materials show 10–20 times better electron mobility compared to Si, their hole mobility is comparable to that of Si. To improve the hole mobility in III–V materials, one approach is to use compressively strained III–V channels in MOSFETs. Alternatively, other novel materials exhibiting high hole mobility, e.g., strained Ge quantum wells, can be used as the pchannel materials. Finally, to take advantage of the advanced development of Si IC technologies and the highspeed, lowpower capabilities of III–V devices, it is desirable to monolithically integrate III– V devices selectively onto the Si platform. To achieve this goal, one has to solve two significant challenges, namely the latticemismatch and thermal mismatch between Si and III–V’s. Problems 1. Refer to the experimental results of an Al0.3 Ga0.7 As/GaAs HEMT reported in [6]. (a) Estimate the threshold voltage V T for three samples (R96A, R73A, and R72A). (b) The 2DEG in the triangular quantum well has a sinewavelike distribution perpendicular to the conduction channel. What is the average concentration peak of the 2DEG located W away from the heterojunction interface? The results can be calculated using the equation NS =
2 (VGS − VT − Vx ) q(Wd + W )
Assume V DS = 0 and comment on your results in terms of whether they are realistic. (c) Estimate W again using Howard–Fang approximation for the triangular QW at the interface. Also discuss your results. 2. In an Al0.2 Ga0.8 As/Ga0.85 In0.15 As pseudomorphic highelectronmobility transistor (pHEMT), the Al0.2 Ga0.8 As barrier is uniformly doped at a level of 2 × 1018 cm−3 . At the Al0.2 Ga0.8 As/Ga0.85 In0.15 As interface, there is an undoped spacer layer on the Al0.2 Ga0.8 As side. (a) Calculate the sheet carrier concentration in the triangular Ga0.85 In0.15 As quantum well for different spacer layer thickness (W sp ) of 25 Å and 100
414
9 Heterostructure Electronic Devices
Å. Assume the donor level in Al0.2 Ga0.8 As is sufficiently deep (E d = 50 meV) so that the Fermi level is pinned there. The dielectric constant of Ga0.85 In0.15 As is 13.41ε0 . (b) Plot the equilibrium energy band diagram of the whole pHEMT structure, including metal contact, for the W sp = 25 Å case using SimWindows. Assume the total Al0.2 Ga0.8 As barrier has a thickness of 150 Å and the undoped Ga0.85 In0.15 As 2DEG channel is 100 Å thick. The whole structure is grown on top of an undoped GaAs substrate. The metalAl0.2 Ga0.8 As work function qφ m equals ~0.9 eV. (c) Repeat part (a) for a modulationdoped Al0.3 Ga0.7 As/GaAs heterostructure with a 25 Å spacer layer and E c = 0.2 eV. This HEMT structure has the same doping level in the Al0.3 Ga0.7 As barrier. The dielectric constant of GaAs is 12.850 . (d) Now the 2DEG channel material of the pHEMT is replaced with a GaAs0.8 Sb0.2 layer, but keep all other materials unchanged. For Wsp = 25 Å, calculate the sheet carrier concentration in the triangular GaAsSb QW. Will this material system outperform the Al0.2 Ga0.8 As/Ga0.85 In0.15 As pHEMT structure? Why? The relevant material parameters are listed below: For Ga0.85 In0.15 As: m ∗e /m 0 = 0.025(1 − x) + 0.71x − 0.0163x(1 − x) For GaAs0.8 Sb0.2 : m ∗e /m 0 = 0.00634 − 0.0483x − 0.0252x 2 . 3. The 2DEG with a sheet carrier density of 1013 cm−2 is obtained at the interface of an Alx Ga1−x N/GaN HEMT structure grown by MOCVD. The Alx Ga1−x N barrier is undoped and has a thickness of 30 nm. Using parameters provided in the reference article [9], verify that the Alcomposition (x) of the Alx Ga1−x N barrier is about 0.2 as shown in Fig. 11 of the referenced article. 4. Repeat Problem 3 with uptodate material parameters of Alx Ga1−x N shown below: E c (x) ≈ 2.12x, E g (x) = xE g (AlN) + (1–x)E g (GaN) − 0.7x(1–x). Dielectric constant (x) = 9.5 − x, m*(x) = 0.22me , qφ m (x) = 1.3x + 0.84 (eV). PSP (Alx Ga1−x N/GaN) = −0.090x − 0.034(1 − x) + 0.021x(1 − x) c/m2 PPE (Alx Ga1−x N/GaN) = −0.0525x + 0.0282x(1 − x) c/m2 Assuming the Alcomposition of the Alx Ga1−x N barrier in the Alx Ga1−x N/GaN HEMT is x = 0.2, calculate the 2DEG sheet carrier density at the Alx Ga1−x N/GaN interface.
9.8 III–V MetalOxideSemiconductor FieldEffect Transistors
415
5. The active region of a pchannel pseudomorphic highholemobility transistor (pHHMT) has a compressively strained InSb channel material and an Al0.35 In0.65 Sb barrier. For a 5 nm InSb QW sandwiched between Al0.35 In0.65 Sb barrier, the typeI band discontinuities, E c and E v , are determined as 0.342 and 0.254 eV, respectively. Assume the 200 Å thick Al0.35 In0.65 Sb barrier consists of a uniformly Bedoped layer of p = 1018 cm−3 and an undoped spacer layer, W sp = 70 Å. (a) Calculate the sheet carrier concentration in the triangular InSb quantum well. Assume the acceptor level in Al0.35 In0.65 Sb is sufficiently deep (E a = 40 meV) so that the Fermi level is pinned there. (b) Plot the equilibrium energy band diagram of the whole pHHMT structure, including metal contact, using SimWindows. The plot should extend into the AlInSb buffer layer for 200 Å. Assume the metalAl0.35 In0.65 Sb work function qφ m equals ~0.16 eV. 6. In pursuing highspeed HBTs, InPbased material systems are the most promising. One of the systems being actively studied is based on using GaSb0.5 As0.5 latticematched to InP as the base material. (a) Find the band discontinuity values between latticematched GaSb0.5 As0.5 and InP. Is this a typeI or typeII heterojunction? (b) In Ga0.47 In0.53 As/InP NpN DHBTs, the valence band discontinuity between InP emitter and Ga0.47 In0.53 As base is 0.36 eV. The E c in this typeI heterojunction is 0.252 eV. By replacing the Ga0.47 In0.53 As with latticematched GaSb0.5 As0.5 , the maximum current gain can be improved. Calculate the maximum current gain improvement. (c) Compare the properties of GaSb0.5 As0.5 /InP and Ga0.47 In0.53 As/InP HBTs. 7. Gax In1−x P is a useful material for visible lightemitting and HBT applications. (a) Calculate the composition x and band gap energy of Gax In1−x P latticematched to GaAs. (b) Using modelsolid theory, calculate the band discontinuities between latticematched Gax In1−x P and GaAs. (c) In Al0.3 Ga0.7 As/GaAs HBTs, the valence band discontinuity between Al0.3 Ga0.7 As emitter and GaAs base is 0.132 eV. By replacing the Al0.3 Ga0.7 As with latticematched Gax In1−x P the maximum current gain can be improved. Calculate the magnitude of current gain improvement. (d) Does Gax In1−x P offer any advantages over Al0.3 Ga0.7 As as the barrier layer in an Gax In1−x P/GaAs highelectron mobility transistor? Why? Note, the conduction band discontinuity in the Al0.3 Ga0.7 As/GaAs system is 0.263 eV. 8. Mini project: During the last 60 years, the density and feature size of Si ICs have followed Moore’s law faithfully through device scaling. However, the current Si
416
9 Heterostructure Electronic Devices
technology will hit a feature size limit in the near future. New channel materials for increased electron and hole mobility, well above those achievable in strained Si, are needed. As gate dielectric scaling becomes increasingly difficult, carrier transport enhancement will become essential for current enhancement in the advanced FETs of future CMOS generations. One of the major problems encountered in developing FETs based on materials other than Si is the large disparity between electron and hole mobility. In order to design complementary FETs (i.e., one nchannel and one pchannel, and not limited to MOSFET), a material system with high hole mobility is required. In this problem, the goal is to design a pchannel quantum well FET (QWFET) similar to the highholemobility QWFET reported by Intel in 2008. (M. Radosavljevic et al., 2008 IEEE IEDM Tech. Dig., https://doi.org/10.1109/iedm.2008.479 6798) Your work should meet the following requirements: • Select a material system among all available III–V materials for high hole mobility. Explain why you select it. However, you cannot copy the structure reported by Intel. Recall that in Chap. 6, we learned that under compressive strain, the heavyhole band is lifted above the lighthole band in the growth direction (perpendicular to surface). But in the direction parallel to the surface (perpendicular to the growth direction), the effective mass becomes lighter. (See S. L. Chuang, Phys. Rev., B43, 9649, 1991.) • The selected material system should be able to form QWFET structures with high crystal quality. Of course, highquality heterostructures prepared on metamorphic substrate structures are allowed. (That means you can use materials with any lattice constant as the substrate). • Design the layer structure of a QWFET based on the material system selected. We restrict the selection of FET structure to QWFETs (including pseudomorphic structures). Provide detailed material and device parameters such as E v , N S and layer structures along with full energy band diagram. For heterostructures, the energy band discontinuities should be calculated. The portion of gate contact should also be included. • To simplify the calculation, set the spacer layer thickness as W sp = 25 Å and the acceptor level in the barrier layer as E a = 40 meV. The Schottky barrier height of the barrier layer can be determined following the method reported by Tiwari and Frank (Appl. Phys. Lett., 60, 630, 1992). • Your final device layer structure should be a depletion mode FET at zero gate bias.
References 1. R. Dingle, H.L. Stormer, A.C. Gossard, W. Wiegmann, Appl. Phys. Lett. 33, 665 (1978) 2. T. Mimura, S. Hiyamizu, T. Fujii, K. Nanbu, Jpn. J. Appl. Phys. 19, L225 (1980)
References 3. 4. 5. 6. 7. 8. 9.
10. 11. 12. 13. 14. 15. 16. 17. 18. 19. 20. 21. 22. 23. 24.
25.
417
S. Hiyamizu, J. Saito, K. Nanbu, T. Ishikawa, Jpn. J. Appl. Phys. 22, L609 (1983) H. Morkoc, T.J. Drummond, R. Fischer, J. Appl. Phys. 53, 1030 (1982) L. Pfeiffer, K.W. West, H.L. Stormer, K.W. Baldwin, Appl. Phys. Lett. 55, 1888 (1989) K. Hirakawa, H. Sakaki, J. Yoshino, Appl. Phys. Lett. 45, 253 (1984) E.F. Schubert, K. Ploog, Phys. Rev. B30, 7021 (1984) A. Kastalsky, R.A. Kiehl, IEEE Trans. Electron. Dev. 33, 414 (1986) O. Ambacher, J. Smart, J.R. Shealy, N.G. Weimann, K. Chu, M. Murphy, W.J. Schaff, L.F. Eastman, R. Dimitrov, L. Wittmer, M. Stutzmann, W. Rieger, J. Hilsenbeck, J. Appl. Phys. 85, 3222 (1999) I.P. Smorchkova, C.R. Elsass, J.P. Ibbetson, R. Vetury, B. Heying, P. Fini, E. Haus, S.P. DenBaars, J.S. Speck, U. Mishra, J. Appl. Phys. 86, 4520 (1999) H. Kroemer, Proc. IRE 45, 1535 (1957) W. Snodgrass, W. Hafez, N. Harff, M. Feng, IEDM Tech. Dig. (11–13 Dec 2006) N. Holonyak, Jr., M. Feng, IEEE Spectrum, 43(2), 50 (2006) H.K. Gummel, Proc. IEEE 57, 2159 (1969) A.W. Hanson, S.A. Stockman, G.E. Stillman, I.E.E.E. Electron, Dev. Lett. 14, 45 (1993) M.T. Fresina, Q.J. Hartman, D.A. Ahmari, N.F. Gardner, G.E. Stillman, J. Appl. Phys. 77, 5437 (1995) W. Hafez, J.W. Lai, M. Feng, I.E.E.E. Electron, Dev. Lett. 24, 436 (2003) B.W. Wu, B.F. ChuKung, M. Feng, K.Y. Cheng, J. Vac. Sci. Technol., B 24, 1564 (2006) P.D. Ye, J. Vac. Sci. Technol., A 26, 697 (2008) J. Robertson, J. Vac. Sci. Technol., A 31, 050821 (2013) M.D. Groner, F.H. Fabreguette, J.W. Elam, S.M. George, Chem. Mater. 16, 639 (2004) M. Hong, J. Kwo, A.R. Kortan, J.P. Mannaerts, A.M. Sergent, Science 283, 1897 (1999) M. Passlack, M. Hong, J.P. Mannaerts, Appl. Phys. Lett. 68, 1099 (1996) C.L. Hinkle, A.M. Sonnet, E.M. Vogel, S. McDonnell, G.J. Hughes, M. Milojevic, B. Lee, F.S. AguirreTostado, K.J. Choi, H.C. Kim, J. Kim, R.M. Wallace, Appl. Phys. Lett. 92, 071901 (2008) M. Hong, H.W. Wan, K.Y. Lin, Y.C. Chang, M.H. Chen, Y.H. Lin, T.D. Lin, T.W. Pi, J. Kwo, Appl. Phys. Lett. 111, 123502 (2017)
Further Reading 1. 2. 3. 4. 5.
C. Weisbuch, B. Vinter, Quantum Semiconductor Structures (Academic Press, 1991) J.H. Davies, The Physics of LowDimensional Semiconductors (Cambridge, 1998) B.G. Streetman, S. Banerjee, Solid State Electronic Devices, 6th edn. (PrenticeHall, 2006) S.M. Sze, HighSpeed Semiconductor Devices (Wiley, 1990) C.W. Wilmsen (ed.), Physics and Chemistry of III–V Compound Semiconductor Interfaces (Plenum Press, New York, 1985) 6. S. Oktyabrsky, P.D. Ye (eds.), Fundamentals of IIIV Semiconductor MOSFETs (Springer, New York, 2010) 7. S.M. George, Chem. Rev. 110, 111 (2010)
Chapter 10
Heterostructure Photonic Devices
Abstract The light emitters made of III–V alloys are the most important and widely used photonic devices because Si and Ge do not emit light due to their indirect band structures. The semiconductor laser is similar to the solidstate ruby laser and Ar+ gas laser in that the emitted radiation is highly monochromatic and produces a highly directional beam of light. However, the semiconductor laser is much smaller (on the order of 0.25 mm long) than other lasers and is easily modulated at high frequencies simply by modulating the injected current. Because of these unique properties, the semiconductor laser is one of the most important light sources for opticalfiber communication. It also has many applications in consumer electronics such as optical reading, laser printing, and face ID, to mention just a few. In addition, semiconductor lasers have significant applications in many areas of basic research and technology, such as highresolution gas spectroscopy and atmospheric pollution monitoring. A related important photonic device is the lightemitting diode (LED), which has a device structure very similar to the semiconductor injection laser but without a resonant optical cavity. Today, visible LEDs play a leading role in displays and solidstate lighting applications. In this chapter, the device physics, structures, and characteristics of many types of heterostructure lasers are discussed. The current status and challenges of visible LEDs are briefly reviewed. In addition, the quantum cascade laser based on unipolar intersubband transitions for longwavelength applications is introduced. Also discussed is the midinfrared quantumwell infrared photodetector, operating based on the same unipolar intersubband optical transition. Finally, the concept of optoelectronic integration is demonstrated in the transistor laser where both transistor and laser operation are realized simultaneously in the same device.
10.1 Device Physics of Heterostructure Lasers 10.1.1 Basic Diode Laser Structure The basic structure of a semiconductor injection laser is similar to that of a pn junction diode as shown in Fig. 10.1. Like all other types of laser, it has a gain medium, an optical cavity, and an excitation source. The pn junction, which usually © Springer Nature Switzerland AG 2020 K. Y. Cheng, III–V Compound Semiconductors and Devices, Graduate Texts in Physics, https://doi.org/10.1007/9783030519032_10
419
420
10 Heterostructure Photonic Devices
Fig. 10.1 Basic structure of a laser diode in the form of a Fabry–Perot cavity
Current
Active layer ptype
Cleaved back facet
ntype
Sawed sidewall
Coherent Emission
100 µm
Cleaved front facet
lies in the (100) plane, forms the active region (gain medium) of the laser diode, which is a part of the optical cavity. A current flowing through the pn junction supplies electrons and holes for light generation through radiative recombination. A pair of parallel (110) planes is cleaved perpendicularly to the (100) plane of the junction to form cavity mirrors. The two remaining sides of the diode are either roughened or electrically isolated to eliminate lasing in directions other than the main one. The structure is called a Fabry–Perot cavity. When a forward bias is applied to the laser diode, a current flows through the pn junction as the excitation source. Initially at low current, there is spontaneous emission in all directions. As the bias is increased, eventually a threshold current density J th is reached at which the stimulated emission occurs and a monochromatic and highly directional beam of light is emitted from the junction (Fig. 10.1). As discussed later, in order to achieve efficient and reliable operation of laser diodes, it is necessary to design devices with a low threshold current density J th . In 1962, when laser diodes were first demonstrated in diffused GaAs and GaPx As1−x pn homojunction structures, the threshold current density J th was about 5.0 × 104 A/cm2 at room temperature. Most studies were done at liquid nitrogen temperature (77 K) or lower. Such a large current density imposes serious difficulties in operating the laser continuously at 300 K. To reduce the threshold current density, heterostructure lasers have been proposed and built using epitaxial techniques. Figure 10.2 shows schematic representations of the bandgap under forwardbiased conditions, the refractive index change, and the optical field distribution of light generated at the pn junction for a homostructure and a double heterostructure (DH). The lack of carrier confinement under forward bias condition in the homojunction structure laser is evident from the low potential barriers. Consequently, only under very high injection conditions are there enough carriers for the laser to reach population inversion. The very small index change ( n¯ 1 = n¯ 3
(10.1)
the electromagnetic radiation with a ray angle θ at the active layer/cladding layer interface exceeding the critical angle θc = sin−1 (n¯ 1 /n¯ 2 ) is totally reflected into the active layer. Therefore, when the refractive index in the active region is larger than the index of its surrounding cladding layers, (10.1), the propagation of electromagnetic radiation is guided in a direction parallel to the layer interfaces along the zdirection. For idea DH lasers, the refractive index steps at each heterojunction can be made as
422
10 Heterostructure Photonic Devices
Fig. 10.3 Ray trajectories of the guided wave in a threelayer dielectric waveguide of a semiconductor laser. The intensity distribution of the optical waveguide mode is also shown. The shaded region represents the fraction of the mode within the active region
large as 10% or more and provide a welldefined waveguide. However, due to the finite difference in refractive indices in most structures, a portion of the electromagnetic radiation leaks out of the active region into cladding layers. The evanescent wave in the cladding layer will not participate in lasing action in the active layer and becomes a portion of the cavity loss. The ratio of the optical energy within the active layer to the total energy both within and outside the active layer defines a confinement factor . Consider the transverse electric (TE) wave E y (x, z, t) which is polarized transversely to the direction of propagation (zdirection) along the ydirection in a threelayer symmetric dielectric waveguide. The even mode of E y (x, z, t) is given by E y = A cos(κ x) exp[i(ωt − βz)]
(10.2)
where β = 2π/λ is the propagation constant, κ 2 = n¯ 22 k02 − β 2 , k0 = 2π/λ0 , and λ = λ0 /n¯ 2 . The even mode magnetic field H x (y, z, t) can be found from Hx = −(i/ωμ0 ) ∂ E y /∂z
(10.3)
The average power propagating in the waveguide is determined by the Poynting vector, P ∝ E y Hx∗ ∝ E y 2 , where Hx∗ is the complex conjugate. The confinement factor for the symmetrical threelayer dielectric waveguide with a thickness of d can be obtained for the even TE waves as 2 E y (x)2 dx ∫d/2 ∫d/2 0 0 cos (κ x)dx = = 2 ∞ 2 2 ∫d/2 ∫∞ E y (x) dx 0 cos (κ x)dx + ∫d/2 cos (κ x) exp −2γ (x − d/2) dx 0
10.1 Device Physics of Heterostructure Lasers
423
Fig. 10.4 Confinement factor for the fundamental mode as a function of active layer thickness for the Alx Ga1x As/GaAs symmetric threelayer slab dielectric waveguide
= 1+
cos2 (κd/2) γ [(d/2) + (1/κ) sin(κd/2) cos(κd/2)]
−1 (10.4)
where γ 2 = β 2 − n¯ 21 k02 in cladding layers. Similar expressions may be obtained for odd TE waves as well as for the transverse magnetic (TM) waves. Figure 10.4 shows the variation of the calculated confinement factor in an Alx Ga1x As/GaAs DH structure for the fundamental mode with active layer thickness d. It can be seen that decreases rapidly for d < λ/n¯ 2 (≈0.25 μm), where the active layer thickness becomes less than the wavelength of the radiation. Representing the fraction of the propagating mode within the active layer by is an essential concept for understanding the influence of the active layer thickness on the gain coefficient necessary to reach the lasing threshold.
10.1.3 Threshold Condition in Fabry–Perot Cavity In Chap. 8, it was shown that when the excitation satisfies the necessary condition of population inversion for stimulated emission, the absorption coefficient α(E) reduces to zero. Also, the gain coefficient g(E) is related to α(E) as g(E) = −α(E)
(10.5)
where g(E) is defined as positive when radiation is emitted and α(E) is negative when radiation is absorbed. At this point, g(E) = α(E) = 0, the system reaches the
424
10 Heterostructure Photonic Devices
transparency condition, which is determined solely by the material property of the active layer. However, since there are other losses in a practical laser diode, additional gain is needed for the laser diode to reach the lasing threshold. Consider a Fabry–Perot laser diode cavity, which consists of a gain medium truncated by a pair of parallel reflection surfaces. The lasing condition can be obtained by considering the plane wave reflection between parallel, partially reflecting mirror surfaces as shown in Fig. 10.5. The cavity length is L. The transmission and reflection coefficients of the left mirror facet are indicated by t 1 and r 1 , respectively. These parameters of the right mirror are indicated by t 2 and r 2 , respectively. A plane wave electric field E i is incident on the left cavity mirror so that E x is t 1 E i inside the left boundary and t1 E i exp(−K L) just inside the right boundary, where K is the complex propagation constant (= γ + iβ). The first path of the field transmitted through the right mirror is t1 t2 E i exp(−K L), and the reflected field is t1 r2 E i exp(−K L). The next path of the wave transmitted through the right mirror becomes t1 t2 r1r2 E i exp(−3K L) and so on. The sum of these transmitted fields through the right mirror gives E t = t1 t2 E i exp(−K L) 1 + r1r2 exp(−2K L) + r12 r22 exp(−4K L) + · · ·
t1 t2 exp(−K L) (10.6) = Ei 1 − r1r2 exp(−2K L) The oscillation condition is reached when the denominator of (10.6) goes to zero, where a finite transmitted wave E t is obtained with zero E i . Thus r1r2 exp(−2K L) = 1
(10.7)
Using K = i(n¯ − i κ)k ¯ 0 in (10.7) with k0 = 2π/λ0 and κ¯ = α λ0 /4π , it becomes ¯ 0 )L] = 1 r1r2 exp(−αL) exp[−2i(2π n/λ
(10.8)
The above equation represents a wave making a round trip of 2L inside the cavity to the starting point with the same amplitude and phase. It of course contains two parts representing the amplitude and the phase of the oscillating wave. The amplitude requirement for oscillation is Fig. 10.5 Oscillation condition for a gain medium with parallel reflecting surfaces in a Fabry–Perot cavity
10.1 Device Physics of Heterostructure Lasers
r1r2 exp[(g − αi )L] = 1
425
(10.9)
The negative α in (10.8) has been replaced by the net gain, which equals the difference between the model gain g and the total internal losses α i . In the gain term, the confinement factor represents the fraction of the mode energy contained within the active region that contributes to gain. The gain can be rearranged as the sum of the total internal loss (α i ) and mirror loss (α m ): g = αi + αm = αi + (1/2L) ln(1/R1 R2 )
(10.10)
αm = (1/2L) ln(1/R1 R2 )
(10.11)
and
The reflection coefficients are replaced with the power reflectances R1 = r1r1∗ ≈ and R2 = r2 r2∗ ≈ r22 . Intrinsic loss in semiconductors with good crystal quality lies in the range α i = 5–10 cm−1 . According to discussions in Chap. 8, the peak of the gain curve increases and shifts to higher energy with the injection level. Empirically, the gain peak position gp or gmax follows the injection carrier density in a nearly linear fashion as illustrated in Fig. 10.6. One can write
r12
g p = a(n − n tr )
(10.12)
where gp is the peak gain, a = ∂g p /∂n is the differential gain coefficient, and n tr is the transparency carrier density. For n > n tr , there is a positive gain. However, to reach the threshold, more gain achieved by a higher carrier injection is needed to Fig. 10.6 Schematic of the change in laser gain spectra as a function of carrier injection of an InGaAsP/InP laser. Reprinted with permission from [1], copyright AIP Publishing
426
10 Heterostructure Photonic Devices
overcome internal and mirror losses. At the threshold, g p = gth = a(n th − n tr ) and n th is the threshold carrier density. The phase condition of oscillation is 4π n¯ L/λ0 = 2mπ m(mode number) = 1, 2, 3, . . .
(10.13)
mλ0 = 2n¯ L
(10.14)
or
For a typical laser diode, the mode number m can be very large since λ0 L. Figure 10.7 shows the lasing spectrum and the gain curve of a typical laser diode operating just above the threshold. The profile of the gain curve is usually broad, and multiple modes, whose gain is larger than the total loss, are allowed to lase simultaneously. This lasing mode reflecting a light wave situation in the oscillation direction of the laser cavity is called the longitudinal mode. Equation (10.14) can be used to derive the longitudinal mode spacing. Differentiation of this equation yields λ0 dm + mdλ0 = 2Ld n¯
(10.15)
For adjacent mode, dm = −1, and (10.14) can be substituted for m to give dλ0 =
Fig. 10.7 Longitudinal mode emission spectrum and the gain profile of a FP laser diode
λ20 2n¯ L[1 − (λ0 /n)(d ¯ n/dλ ¯ 0 )]
(10.16)
10.1 Device Physics of Heterostructure Lasers
427
for the spacing between adjacent longitudinal modes. Since the refractive index change is near zero for adjacent modes, the mode spacing dλ0 can be simplified as dλ0 = λ0 ∼ = λ20 /2n¯ L = λ0 /m
(10.17)
For a GaAs laser diode with L = 250 μm, λ0 = 0.85 μm, and n¯ ~ 3.5, the calculated mode number is ~2060 with a mode spacing of ~0.4 nm.
10.1.4 Threshold Current Density and Photon Density To analyze the interaction between injected carriers and photons in a semiconductor laser so that the threshold current density and other dynamic properties can be derived, it is necessary to use the coupled rate equations which determine the time variation of the density of the two species. For the derivation of threshold current density, only the gain–loss relation, without the phase condition, is considered during the lasing action. For the active layer structure shown in Fig. 10.8 (d = thickness, L = length, and w = width), the rate of change of the injected electron density n is J ∂n = Dn ∇ 2 n + − R(n) ∂t qd
(10.18)
where Dn is the carrier diffusion coefficient, J = I/wL is the injected current density, and R(n) is the rate of recombination loss. The first two terms on the righthand side represent carrier injection rate increase through diffusion and injection, respectively. The total recombination rate is expressed as R(n) = Anr n + Br n 2 + Cn 3 + Rstim
(10.19)
where Anr , Br , C, and Rstim are the nonradiative, radiative, Auger and stimulated recombination rate coefficients, respectively. Under steady state and n = p, ∂n = Dn ∇ 2 n = 0 ∂t Fig. 10.8 Geometry and dimensions of a FP cavity laser diode
I w
d L
(10.20)
428
10 Heterostructure Photonic Devices
This leads to J = qd R(n)
(10.21)
Near the threshold condition, Rstim ≈ 0, and Anr = C = 0 for the laser with high material quality. Therefore, R(n) = Br n 2 ≈ n/τs , and, below threshold, the current density is related to the injected carrier density n by J=
qdn τs
(10.22)
where τ s is the carrier lifetime. When the injection current density at or just above threshold, J = Jth , n = n th , and g = gth = a(n th − n tr ). Replacing gth with (αi + αm )/ , the threshold carrier density becomes n th = n tr + (αi + αm )/a
(10.23)
This leads to the threshold current density of qd αi + αm n tr + Jth = τs a
(10.24)
This relationship between J th and d is illustrated in Fig. 10.9 for 300 μm long InGaAs/InP lasers emitting at 1.3 μm. The curve shows a minimum J th at an optimal Fig. 10.9 Measured threshold current density at room temperature as a function of the active layer thickness for 1.3 μm InGaAsP DH lasers. Reprinted with permission from [2], copyright Japanese Society of Physics
10.1 Device Physics of Heterostructure Lasers
429
active layer thickness d 0 . When the active layer thickness is large, d > d 0 , the confinement factor becomes saturated close to unity. The value in the parenthesis turns into a constant and J th proportions to d in a linear fashion. For d < d 0 , is a small number and decreases rapidly with reducing active layer thickness. Therefore, the second term containing , which represents the cavity loss, dominates the threshold current density. For thin active layer, the threshold current density increases rapidly with deceasing d. At the same time, the rate of change in photon density N of the oscillating mode in the laser cavity can be described by the following photon rate equation: N ∂N = β Rsp + Rst − ∂t τph
(10.25)
where Rsp and Rst are the spontaneous emission rate and stimulated emission rate, respectively, and τ ph is the photon lifetime. β is the spontaneous emission factor that approximately equals the inverse of the optical mode number of the cavity. Therefore, the first term on the righthand side represents the photon increase due to spontaneous recombination of the oscillation mode. The last term takes account of the decrease of the photon density in the mode by escape of photons from the resonator, as well as by scattering and other losses not directly connected with radiating transitions. The spontaneous emission rate can be expressed in the form Rsp = n/τs
(10.26)
The stimulated emission rate has the same form as the net absorption rate derived in Chap. 8 (8.77) and is expressed as Rst = υg g p N =
c a(n − n tr )N n¯
(10.27)
When the laser is operated just above threshold, under steadystate condition, ∂ N /∂t = 0 and β 1, the rate equation reduces to
1 c = 0 and N = 0 N a(n − n tr ) − n¯ τph
(10.28)
Through the above equation, the photon lifetime can be determined as a function of the differential gain, carrier density, and the confinement factor. 1 c = a(n − n tr ) τph n¯
(10.29)
The optical emission processes in the laser cavity also change the number of injected excess carriers, which is controlled by the current injection following
430
10 Heterostructure Photonic Devices
(10.22). Under steadystate lasing conditions, the electron rate equation for high carrier injection, neglecting spontaneous emission, is R(n) =
n n J = + Rst = + υg g p N qd τs τs
(10.30)
and N=
J n − qd τs
1 υg g p
(10.31)
Using υg g p = (c/n)a(n ¯ − n tr ) and υg g p = 1/τph , N can be expressed as N=
τph J τph n¯ 1 n tr τph + − = (J − Jth ) qd τs ac qd
(10.32)
¯ where Jth = (qd/τs ) n tr + n/acτ ph is the threshold current density. It is clear that N ∝ J − Jth
(10.33)
Figure 10.10 shows the variations of the injected carrier density n and the photon density N as functions of the injected current density J. Following the assumption made above, the spontaneous emissions are neglected. Below the threshold current density J th the photon density vanishes, and the electron concentration increases linearly with the pumping current (10.22). Above the threshold, the photon density increases linearly but the injected carrier density remains constant or pinned at nth . This is because of the rather long carrier lifetime (~10−9 s) compared with the short photon lifetime (~10−12 s) such that, at J ≥ J th , all carriers recombine immediately once injected into the cavity. If spontaneous emissions are not omitted, there is a minor deviation from the idealized behavior below threshold, as indicated by the dashed line in Fig. 10.10. Fig. 10.10 Variations of injected carrier density (n) and generated photon density (N) as functions of injection current density
10.1 Device Physics of Heterostructure Lasers
431
10.1.5 Laser Output Power and Efficiency Before lasing, the light generated from the laser takes the form of spontaneous emission. At the threshold, a change from spontaneous emission to stimulated emission is observed, and light output is emitted with a high efficiency after lasing. The output power is formulated as follows:
photon photon effective volume photon P= energy density of the cavity escape rate wd L υg αm = (ω)(N ) P=
ω υg αm τph (J − Jth )wL q
(10.34)
Since (J − Jth )wL = (I − Ith ) and 1/τph = υg (αi + αm ), the output power is rewritten as P=
αm ω (I − Ith ) q αi + αm
(10.35)
Clearly, the output power is a linear function of injection current above the threshold. Figure 10.11 shows the typical light output power from one mirror facet of the laser diode as a function of the injection current or the L–I curve. However, the linear relation deteriorates by Joule heating at highcurrent densities. The slope of the laser output characteristic L–I curve defines the external differential quantum efficiency ηd , which is expressed by a ratio of the photon number emitted out of a laser cavity to injected carrier number. Fig. 10.11 Light–current (L–I) curve for a laser diode. The dashed line represents the onset of power saturation
432
10 Heterostructure Photonic Devices
ηd =
αm P/ω = I /q αi + αm
(10.36)
A typical ηd of a laser diode is about 50–80%, where the emission from both mirror facets is taken into account. In the above discussion, injected carriers are assumed completely converting into photons inside the laser diode without any loss. If the spontaneous emission is no longer neglected, only a fraction of the total photons created goes into the laser mode. In addition, there are nonradiative transitions and leakage currents. An internal quantum efficiency ηi , which indicates a ratio of generated photon number to injected carrier number in the active layer, is introduced to show that only part of the injected carriers contribute to photon generation. The optical output power of the laser diode is now shown as P=
ω αm ηi (I − Ith ) q αi + αm
(10.37)
It follows that the single facet differential external quantum efficiency is ηd =
αm ηi ηi = αi + αm 1 − αi L/ ln R
(10.38)
for the case of R = R1 = R2 . This equation can be expressed in the following form: L 1 1 1 − αi = ηd ηi ln R
(10.39)
One can plot 1/ηd as a linear function of cavity length L of lasers which are otherwise the same. The slope of the straight line determines the loss parameter α i /ln R. The internal quantum efficiency ηi can be deduced from the extrapolated ηd value at L = 0.
10.1.6 Characteristic Temperature Light output power of a laser diode is ideally expressed by (10.37) which is a linear function of the injection current above threshold. In reality, lasers often show power saturation under cw operation, as recognized by the hightemperature range of Fig. 10.12. The power saturation tends to be large in proportion to the ambient temperature as a result of the temperature dependence of stimulated emission. This means that the threshold current also increases according to the rise in temperature. The temperature dependence of the threshold current is empirically given by Ith = Ith (0) exp T j /T0
(10.40)
10.1 Device Physics of Heterostructure Lasers
433
Fig. 10.12 Temperature dependence of L–I curves in a 1.3 μm InGaAsP/InP buriedheterostructure laser
where I th (0) is the threshold current at 0 °C and T j is the junction (active layer) temperature. The T 0 term is called the characteristic temperature of the laser and indicates the degree of lasing characteristic change with temperature. A high characteristic temperature indicates a small change in lasing characteristics with temperature. The characteristic temperature of an AlGaAs/GaAs laser is usually between 100 and 200 K and is determined primarily from overflow of injected carriers from the active layer into cladding layers. For InGaAsP/InP lasers, the characteristic temperature has a maximum for an active layer emitting 1.3μmwavelength light, and it gradually decreases accordingly as the lasing wavelength shifts toward shorter or longer ranges. In the lasing mode at shorter wavelengths than l.3 μm, where the composition of the active layer approaches InP, the characteristic temperature is reduced primarily by overflow of injected carriers due to reduced band discontinuities at the heterojunction. In contrast, when lasing wavelengths longer than 1.3 μm, Auger recombination and intravalence band absorption between the splitoff band and the heavyhole band strongly reduce the characteristic temperature. The characteristic temperature is less than 100 K in such lasers.
10.2 Structures and Properties of Injection Lasers In this section, the electronic and photonic characteristics of different semiconductor lasers are discussed. The active region of the laser forms a slab dielectric waveguide and is terminated by cleaving as shown in Fig. 10.13. The cavity length, characteristics of the gain medium, and lateral dielectric discontinuities determine the longitudinal mode behaviors inside the cavity. The width of the slab waveguide controls the lateral mode of the nearfield pattern which can be observed on the mirror facet
434
10 Heterostructure Photonic Devices
Fig. 10.13 Schematic representation of the nearfield emission pattern, farfield emission pattern, and longitudinal mode pattern of a typical DH laser
under an infrared image converter microscope. When the optical waveguide is narrow (≤10 μm), a fundamental transverse mode is usually achieved. On the other hand, the laser oscillates in a highorder transverse mode. The conditions to achieve fundamental transverse mode perpendicular to the junction plane depend on the index difference between the active and cladding layers and the active layer thickness. For laser structures with a thin active layer of ≤0.2 μm, a fundamental transverse mode is usually guaranteed. This is the situation of all lasers discussed in the following. As the modal field strikes the cleaved facet, it produces a radiation field outside the waveguide, called the farfield pattern. Due to the rectangular crosssectional shape of the active region, the laser generates an elliptical farfield pattern with the longaxis perpendicular to the plane of the active layer.
10.2.1 StripeGeometry Lasers The laser structure shown in Fig. 10.14 (left) is a broadarea DH laser because the entire area along the junction plane can emit radiation. There are serious problems associated with this design for practical applications. First, due to the large device cross section, the operation current is too high for roomtemperature cw operation. Second, the large junction capacitance associated with the large device limits the operation speed. Third, it is difficult to achieve fundamental mode emission from the broadarea lasers. Figure 10.15 shows the nearfield and farfield patterns of stripe
10.2 Structures and Properties of Injection Lasers
435
Fig. 10.14 Broadarea (left) and stripe geometry (right) doubleheterostructure lasers in the Fabry– Perot cavity configuration
Fig. 10.15 Transverse modes on the laser facet as functions of stripe width (10–50 μm) for AlGaAs planarstripe doubleheterostructure lasers. Left: nearfield patterns. Right: farfield patterns. Reprinted with permission from [3], copyright Japanese Society of Physics
geometry Alx Ga1−x As DH lasers with different waveguide widths between 10 and 50 μm. The fundamental mode operation can only be achieved in the device with a stripe width of ≤10 μm. As the stripe width is increased above 12 μm, higherorder modes along the junction plane are observed. The distinct and localized regions of stimulated emission shown in the nearfield pattern are referred to as filaments. This spatial peak intensity of the emission can cause catastrophic laser mirror damage and limits the lifetime of the laser diode. Thus, most heterostructure lasers used today are made in narrow stripegeometries (Fig. 10.14, right). Over the years, many different stripegeometry laser structures have been developed. They can be divided into two categories: gainguided lasers and indexguided lasers.
436
10 Heterostructure Photonic Devices
(a) Gainguided lasers The simplest gainguided laser structure is an oxidestripe geometry device (Fig. 10.16) where the oxide layer confines the injected current flow to a small region through a narrow stripe opening in the dielectric. Lasing from this device is restricted to the narrow region under the stripe contact. A variation of the above structure is the protonbombardmentstripe laser, where the implanted protons or deuterons create a region of high resistivity that restricts the current flow to the center region, which is not bombarded. In these lasers, gain guiding is generated by carrier injection into a narrow region of the active layer, shown in Fig. 10.17, which is planar and continuous. Lasing occurs only in the gain region corresponding to the carrier injection region along the junction plane, and light propagates along the narrow gain region. Since the optical mode distribution along the junction is determined by the gain, rather than the refractive index difference, these lasers are called gainguided lasers. In contact stripe lasers, the current flow through the contact and upper cladding layers is by a majority carrier drift current which spreads laterally before reaching the active layer. Because of the spreading, the current flows through an area in the active region that is larger than the stripe contact area. Within the active layer, there is a lateral diffusion current of minority carriers due to the recombination, which also broadens the current distribution. These two effects greatly increase the threshold current of the stripegeometry lasers. Generally, the threshold current of a 5–10 μm wide contact stripe laser is on the order of 100 mA. Figure 10.18 shows the typical L–I characteristics of a gainguided InGaAsP laser. For small currents below the threshold, spontaneous emission is dominant. Stimulated emission is responsible for the steep increase in light output above the threshold. In all laser diodes, due to the higher mirror losses for the TM modes, only the TEmode oscillates above threshold. In the neighborhood of the laser threshold, many longitudinal modes occur in the emission spectrum. With increasing injection current, side modes are strongly suppressed relative to the central mode and the emission spectrum narrows. However, the gainguided laser does not emit light in a single longitudinal mode even at high injection levels.
Fig. 10.16 Schematic crosssectional view of different types of gainguided laser structures: (left) oxidestripe, and (right) proton or deuteronstripe
10.2 Structures and Properties of Injection Lasers Fig. 10.17 Lateral current distribution, carrier distribution, gain, and refractive index in the active layer of a gainguided stripe laser
Fig. 10.18 a Measured cw L–I curve and b emission spectra at several power levels of a 1.3 μm deuteronstripe gainguided InGaAsP laser. Reprinted with permission from [4], copyright IEEE
437
438
10 Heterostructure Photonic Devices
Fig. 10.19 ‘Kink’ developed in the L–I curve in a gainguided laser and the corresponding nearfield patterns on the facet
At relatively high light output power, the lateral transverse mode becomes unstable due to the lateral index antiguiding (Fig. 10.17). The effective index depression caused by carriers at the waveguide center is ~5 × 10−3 . Under high injection conditions, the carrier density of the center part of the lightemitting region decreases because of the high rate of stimulated emission occurring there. This carrier density reduction leads to a small increase in refractive index, and the emitted light is crowded within the center part of the waveguide. This confinement becomes quite unstable if there is any asymmetry in the refractive index distribution. The lightemitting area easily shifts toward the highrefractive index (low carrier density) region. In this situation, light output barely increases with current injection because the light confinement region does not geometrically correspond to the highgain region. These phenomena result in the ‘kink’ or nonlinearity in the current–light output characteristics (Fig. 10.19). This nonlinearity can also be associated with a transition to higherorder modes, or a transition from TE to TM mode. (b) Indexguided lasers To overcome the index antiguiding problems caused by the carrierinduced index reduction in gainguided lasers, an effective index step of ~10−2 to ~0.2 along the junction plane is introduced to control the lateral mode in indexguided lasers. The added index step is achieved by introducing a lateral thickness nonuniformity in at least one layer for weakly indexguided lasers ( n¯ ∼ = 10−2 ). One example is the ridgewaveguide laser shown in Fig. 10.20. A narrow ridge (≤5 μm) is etched through the upper cladding layer, and its edges are passivated with dielectric to restrict the injection current flow. When lasing, a fraction of the mode overlaps with the dielectric, which has a considerably lower refractive index than the cladding layer (n¯ ∼ 3.5). This overlap introduces an effective lateral index step for lateral confinement. However, the magnitude of the lateral index step is affected by the thickness of the waveguide layer. If the waveguide layer is very thick, the evanescent wave in
10.2 Structures and Properties of Injection Lasers
439
Fig. 10.20 Schematic cross section of a weakly indexguided ridgewaveguide laser and its optical mode
Fig. 10.21 Schematic cross section of a strongly indexguided buriedheterostructure laser
the dielectric becomes too weak to provide significant lateral mode confinement and the device may become very similar to a gainguided laser. In strongly indexguided lasers ( n¯ ∼ = 0.2), the active region is buried in higher bandgap layers vertically and laterally formed by first and second epitaxial growths, respectively, to control the optical modes. Thus, this type of laser is called a buriedheterostructure (BH) laser (Fig. 10.21). Since the lateral index step along the junction plane in these laser structures is about two orders of magnitude larger than the carrierinduced effects, the lasing characteristics of BH lasers are primarily determined by the rectangular waveguide that confines the mode inside the buried active region. The current flow in a BH laser is limited to the active layer by current blocking layers deposited during the second epitaxy. The pn junction in the current blocking layer is reversebiased when a forward bias voltage is applied to the laser diode, thus confining the current flow within the active region. A highly resistive single layer such as Fedoped InP has also been used as a current blocking layer instead of the reversebiased pn junction. As a result of the tight current confinement, the threshold current can be reduced. When compared to gainguided lasers, BH lasers show some excellent characteristics. In addition to a stable transverse mode, BH lasers have a low threshold current, high external efficiency, and the capability of high output power operation. Figure 10.22 shows the L–I characteristics and lasing spectra of a typical 1.3 μm BH laser. It is clear that multiple longitudinal modes exist even at high injection current levels.
440
10 Heterostructure Photonic Devices
Fig. 10.22 Optical power spectra at three different power output levels as indicated in the L–I curve of a 1.3 μm InGaAsP buriedheterostructure laser. Reprinted with permission from [5], copyright IEEE
10.2.2 DistributedFeedback Laser All the laser structures described above use cavity facets that are formed by cleaving to obtain the feedback necessary for lasing. In these Fabry–Perot (FP)type semiconductor lasers, the magnitude of facet reflections is the same for all longitudinal modes. The only longitudinalmode discrimination in such a laser is provided by the gain spectrum. Since the gain spectrum is usually much wider than the longitudinal mode spacing, the resulting mode discrimination is poor. Therefore, FPtype semiconductor lasers do not emit light in a single longitudinal mode. One way of improving the mode selectivity is to make the feedback frequencydependent so that the cavity loss (αi + αm ) is different for different longitudinal modes. This can be achieved by incorporating a grating, i.e., a periodic variation of the refractive index, within the optical waveguide, which is generally produced by corrugating the interface between two dielectric layers (Fig. 10.23a). The feedback necessary for the lasing action in such a laser structure is not localized at the cavity facets but is distributed throughout the cavity length. Therefore, lasers that utilize this type of grating structure are called distributedfeedback (DFB) lasers. A variation of the DFB laser, where the grating is etched near the cavity ends and distributed feedback does not take place in the central active region, as shown in Fig. 10.23b, is called the distributed Bragg reflector (DBR) laser. The unpumped corrugated end regions act as effective mirrors whose reflectivity is of DFB origin and is therefore wavelengthdependent. Assume the refractive index of the grating in a DFB laser has a sinusoidal variation of n(z) ¯ = n¯ + n¯ a cos(2π z/)
(10.41)
10.2 Structures and Properties of Injection Lasers
441
Fig. 10.23 Schematics of distributedfeedback (DFB) and distributed Bragg reflector (DBR) semiconductor lasers. Shaded area shows the active region of the device
where is the period of the spatial variation of the refractive index and n¯ a is the amplitude of variation. It is close to the shape of gratings fabricated in real DFB lasers. This periodic perturbation of n¯ can generate an infinite set of diffraction orders. However, only two counterrunning phasesynchronizing waves near the Bragg wavelength can have significant amplitude. The Bragg condition that determines the Bragg wavelength is ¯ for l = 1, 2, 3, . . . λb = 2n/l
(10.42)
where λb is the wavelength in free space that satisfies the Bragg condition and l is the grating order. Here, the grating pitches corresponding to l = 1, 2, and 3 are called the firstorder, secondorder, and thirdorder gratings, respectively. The reflected wave intensity due to scattering with the periodic gating is determined by the grating height through the magnitude of refractive index change (n¯ a ) and by the distance between the grating and the active layer. Because of the presence of gain, these waves grow as they travel along the dielectric layer and transfer energy between each other due to Bragg scattering. The magnitude of the optical feedback depends on the structure length L and coupling constant κc (= π n¯ a /λ0 ), which is determined by the grating structure. Without going into detail, the total electric field within the periodic (sinusoidal) dielectric layer can be expressed as the sum of the two counterrunning waves: E x (z) = R(z) exp(−iβb z) + S(z) exp(+iβb z)
(10.43)
where R(z) and S(z) are complex amplitudes of the two counterrunning waves and ¯ b . The solutions of the coupledwave equations determine a set of βb = 4π n/λ discrete eigenvalues γ c shown as
442
10 Heterostructure Photonic Devices
κc = ±iγc / sinh(γc L)
(10.44)
For each value of γ c there is a corresponding threshold gain and resonant wavelength. The resonance wavelength of the DFB laser is given as
1 λ2b λ0 = λb ± q + 2 2n¯ L
(10.45)
with q = 0, ±1, ±2, … This result shows that the resonances are spaced λ2b /2n¯ L apart and λ0 never equals λb for any integer value of q. Once λ0 is determined, the threshold gain gF = −α F can be obtained for each q from the following equation: (π n¯ a /λ0 )2 exp(−2α F L) ≈ 4α 2F
(10.46)
The emission spectrum is symmetric with respect to the Bragg wavelength so that two optical modes occur for the same gain coefficient. Also, the threshold increases with deviation from λb and therefore provides spectral selectivity. However, the grating pitch and lasing wavelength λ0 cannot be set randomly. The wavelength λb in (10.42) must be adjusted to the neighborhood of the peak material gain by controlling the grating pitch or composition of the active layer. The DFB and FP modes (gain profile) are displayed in the lasing spectra as shown in Fig. 10.24. The DFB mode and the gain profile differ because they are determined by grating pitch and bandgap energy, respectively. The temperature coefficient of the peak gain shift is about 0.25 nm/°C for 0.85 μm AlGaAs lasers and about 0.4 to 0.6 nm/°C for InGaAsP/InP lasers and is determined by the temperature dependence of the bandgap Fig. 10.24 Lasing and peak gain (FP mode) spectra of an AlGaAs/GaAs DFB laser at different temperatures. Reprinted with permission from [6], copyright IEEE
10.2 Structures and Properties of Injection Lasers
443
Fig. 10.25 Temperature dependence of the emission wavelength of an AlGaAs DFB laser and a FP laser. Reprinted with permission from [6], copyright IEEE
energy. In contrast, the temperature coefficient of the DFB mode is determined by the refractive index variation with temperature and is ~0.1 nm/°C. The wavelength change of a DFB laser as a function of ambient temperature is compared with that of a FP laser in Fig. 10.25. As discussed above, the degeneracy in gain of the modes placed symmetrically around λb makes this idealized DFB laser unsuitable as a singlemode laser. One way to resolve the threshold gain degeneracy in DFB lasers is to use a Bragg grating with a quarterwave shift (/2) near the cavity center (Fig. 10.26). The phase of the grating is shifted by π /2 at the position of the shifter, which causes the phases of two waves propagating in the same direction in the cavity to coincide. Thus, the threshold gain can be further decreased and singlemode operation is established. Fig. 10.26 Schematic of DFB laser diode with λ/4 phase shifting region between the grating portions. The added /2 spacing corresponds to a λ/4 shift between two sections of grating
444
10 Heterostructure Photonic Devices
10.3 Laser with QuantumConfined Active Region 10.3.1 QuantumWell Laser The history of semiconductor laser development is the history of the campaign to lower the threshold current, as is graphically illustrated in Fig. 10.27, using GaAsbased lasers as an example. The most significant changes in this endeavor did not take place until the concept of DH lasers had been introduced. The DH structure establishes an efficient way of collecting both electrons and holes as well as confining light in the same region for low threshold lasing. As the active layer is gradually thinned beyond the optimal active layer thickness d 0 in a DH laser, the optical confinement decreases and the threshold current increases according to (10.24). If the thickness of the active layer is further reduced to a few tens of nanometers, quantum effects arise. However, highquality DH with ultrathin layers could not be attained until new epitaxy methods of MBE and MOCVD were developed in the mid1970s for the growth of heterostructures. Current injection lasing in quantum wells with parameters to match those of standard DH lasers was first accomplished in 1978 by a group led by Holonyak at the University of Illinois in collaboration with Dupuis and Dapkus at Rockwell. The term quantumwell (QW) laser was coined in this work. Depending on whether they have a single active layer or multiple active layers, these devices are called single quantumwell (SQW) or multiple quantumwell (MQW) lasers, respectively. Because of the thin QW active layer thickness, the optical confinement factor is very small in a SQW laser. This leads to a very large threshold current density. The remedy, as shown in Fig. 10.28, is to increase the confinement factor by adding extra waveguiding layers, with higher refractive index, between QWs and cladding layers. Fig. 10.27 Evolution of the threshold current density of semiconductor lasers. Reprinted with permission from [7], copyright IEEE
10.3 Laser with QuantumConfined Active Region
445
Fig. 10.28 AlGaAs gradedindex separateconfinement heterostructure (GRINSCH) with GaAs quantum well and undoped Alx Ga1−x As waveguiding layer, in which the Al content increases continuously from x = 0.2 to 0.45 with increasing distance from the quantum well
In this separate confinement heterostructure (SCH) design, the optical confinement is provided by the cladding layers while carriers in the QW are confined by waveguiding layers. Furthermore, the refractive index of the waveguiding layer can vary in linear or parabolic fashion, increasing from the cladding layer toward the QW, in the gradedindex (GRIN) SCH structure. Injected electrons and holes would be more easily captured in the active QW material through a ‘funnel’ effect due to the funnelshaped bandedge profiles around the QW. The device characteristics of the QW laser can be understood on the basis of FP lasers with some modifications. In a QW, the electron and hole levels have quantum energies of confinement, so that the allowed interband transitions are not tied to the bandgap of the active layer material but can be tuned over a modest range by varying the thickness of the wells. The emission wavelength is always shorter than the bandgap energy of the QW material. The optical transitions have to obey the quantum mechanical selection rule; i.e., allowed transitions are between states in conduction and valence bands having the same quantum number. Because of the small thickness associated with the QW, there is no need to carefully match lattice parameters between the QW and surrounding materials. In fact, as long as the strained QW thickness is less than the critical thickness, the latticemismatch induced strain could enhance the device performance through energy band modification. This also allows a radical diversification of materials available for heterostructure components. In a QW structure, the density of states (DOS) becomes twodimensional (2D) as the injected electrons and holes are quantized only in the direction perpendicular to the active layer, as shown in Fig. 10.29. The steplike DOS introduces some excellent characteristics to lasers because the energy distribution of the injected carrier is narrower than that of a bulk DOS. In the bulk material (3D) shown in Fig. 10.30, the gain peak moves away from the bandgap as the density of injected carriers increases,
446
10 Heterostructure Photonic Devices
E
E
E
E2
E2
E1
E1
z
g3D
g2D
kx , k y
g(E)
Fig. 10.29 Illustration of confined two states in a QW structure (left), the inplane E(k) dispersions (middle), and the resulting density of states (right)
g(E)
g(E)
gth n1 Eg Eth
n2
n3
gth n1
n2
n3 E
E Eth
Fig. 10.30 Illustration of gain formation in bulk (left) and QW (right) structures for three different carrier densities, ni . The dashed line is the peak gain profile for each structure
and all the carriers at lower energies are ineffective at contributing to the gain. The gain peak in the 2D structure stays at the effective bandgap, and the differential gain above threshold is much higher for carriers in the QW (2D) than in the bulk (3D). Furthermore, in the QW laser there are ~1012 cm−2 DOS within a temperature range of kT while there are ~1013 cm−2 DOS in a 1000 nm DH laser. Thus, the threshold is achieved sooner for the QW laser with fewer states to be inverted. Furthermore, the transparency condition is reached for lower injection currents as the QW width decreases, until very thin wells are reached. By then the quasiFermi level energies are so high in the QWs that some carriers are confined not in the QW, but in the waveguiding layers. The threshold current density rises rapidly in very thin QW laser structures. It is clear that the use of the QW active layer greatly reduces the threshold current density below that of DH lasers, as shown in Fig. 10.27. In addition, other characteristics, such as spectral linewidth and highspeed modulation, are also improved by combination with the DFB structure.
10.3 Laser with QuantumConfined Active Region
447
Fig. 10.31 Valence subband structure and DOS of an unstrained 80 Å GaAs/Al0.2 Ga0.8 As QW structure (top), and a compressively strained 80 Å In0.2 Ga0.8 As/Al0.2 Ga0.8 As QW structure (bottom). Reprinted with permission from [8], copyright AIP Publishing
In Fig. 10.27, the other steep drop in threshold current density comes from the incorporation of strain into the QW. As described in Chap. 6, the valence band of semiconductors can be modified using biaxial strain encountered in highly strained layers. The degenerated heavy and lighthole bands are decoupled under the biaxial strain. In particular, under biaxial compression, the lighthole QW deepens and the highest confined state has light transverse hole character with a low DOS, as depicted in Fig. 10.31. Compared in this figure are the topmost valence bands and the corresponding DOS function of an unstrained GaAs/Al0.2 Ga0.8 As QW and a compressively strained InGaAs/Al0.2 Ga0.8 As QW. In the unstrained QW structure, due to the 1D quantum confinement, heavyhole and lighthole bands are decoupled near the zone center. However, the valence band DOS is still dominated by the heavily hole band near the top of the valence band. In the compressively strained structure, the topmost inplane valence band becomes lightholelike and the DOS of hole states adjacent to the valence band edge is now narrowed and comparable to that of electrons near the conduction band edge. In unstrained lasers, the shift of quasiFermi level by carrier injection is much greater for electrons than holes due to the much higher valence band DOS. In strained QW lasers, the much reduced valence band DOS (lighter hole mass) decreases the transparency carrier density and threshold current density. In addition to device characteristic improvement, lasing is possible at a new wavelength that cannot be achieved in the latticematched QW structure.
448
10 Heterostructure Photonic Devices
With its superior characteristics, the strained QW structure has been incorporated into all types of semiconductor lasers and widely used in numerous photonic products including DVD players, laser printers, and opticalfiber communication systems.
10.3.2 TypeII QuantumWell WType Lasers Antimonybased semiconductor lasers emitting in the wavelength of midwave infrared (MWIR: 3–5 μm) are important for biomedical, environmental, and chemical sensing applications. Among all III–V compounds, InAsSb has the narrowest bandgap and is attractive for the active material of MWIR emitters. Strained InAsSb QW lasers with typeI heterostructure have been demonstrated with excellent performance but only at temperatures below ~200 K. Further, the performance of these QW lasers does not exceed that of their doubleheterostructure counterparts because of the large leakage current due to inadequate carrier confinements by small conduction/valence band offsets and the increasing predominance of Auger recombination at high temperatures. Because the energy gap E g and the splitoff gap so of InAsrich alloys are nearly equal, the CHHS Auger process dominates the nonradiative recombination through conductiontoheavyhole (CH) recombination coupled with a heavytosplitoffhole (HS) transition. To circumvent these problems, new interband QW lasers with typeII band alignment have been developed. This new laser design has a Wtype active region, named after the shape of the conduction band profile of the QW active region. Figure 10.32 shows the energy band profiles in the active region of a typical Wtype laser which is latticematched to the InP substrate. The active region is made of multiple QW periods separated by barrier layers (e.g., InAlGaAs) and each period including a thin ‘hole’ QW (e.g., GaAsSb) sandwiched between two ‘electron’ QWs (e.g., InGaAs). Note that the typeII band alignment at each ‘electron’QW/‘hole’QW heterojunction has a brokengap structure such that electrons and holes are confined in different Fig. 10.32 Band alignment for a quantumwell laser structure latticematched to InP substrate with a Wtype active region along with the groundstate electron and hole wavefunctions
GaAs0.5Sb0.5
EC
In0.52Al0.48As C2 C1 HH1 LH1 HH2
In0.53Ga0.47As
Electron Wavefunction
In0.53GaxAl1xAs
Hole Wavefunction
EV
10.3 Laser with QuantumConfined Active Region
449
but neighboring QWs. The symmetric (C1) and antisymmetric (C2) electron states are confined in the conduction band of two coupled InGaAs electron QWs, and heavy hole (HH) and lighthole (LH) subbands are formed in the valence band of GaAsSb hole QW. Although the wavefunctions of electrons and holes are centered in different QW materials, the symmetric wavefunction of two coupled electron QWs is sufficiently overlapped with the center hole wavefunction to yield high interband optical transitions. The fundamental C1HH1 optical transition has an effective bandgap energy in the MWIR range, which is not limited by the bandgap energy of the constituent materials. Thus, the typeII band alignment effectively removes CHHS Auger processes by eliminating the resonance between E g and so , even though it is presented in bulk InAsrich alloys. At the same time, it also introduces large conduction and valence band offsets for enhanced electrical carrier confinements. This Wtype active region design can be incorporated in either diode lasers or cascade lasers for MWIR applications. In the cascade laser design, multiple stages of the typeII Wtype QW active regions are connected in series in a staircase design such that the injected carriers are recycled for enhanced photon generation. The concept of cascade lasers will be discussed in more detail in Sect. 10.6. In typeII Wtype diode lasers operating in the 3–4.5 μm spectral range, the derived roomtemperature Auger coefficients are an order of magnitude lower than those of typeI lasers with a value less than mid10−27 cm6 /s. On the other hand, the Auger coefficient of the cascade laser maintains a nearly constant value of ~5 × 10−28 cm6 /s in the 3–4.2 μm window. With reduced Auger nonradiative decay rates, better carrier confinements, and enhanced quantum efficiency (for the cascade laser), roomtemperature pulse and cw operation of Wtype diode lasers and cascade lasers have been demonstrated, respectively.
10.3.3 Quantum Dot and Quantum Wire Lasers Multipledimension quantum confinement in the growth (junction) plane modifies the electronic band structure and DOS, as shown in Fig. 3.7 and spatially localizes the electrons and holes, resulting in improved laser characteristics. Even in Dingle and Henry’s original patent of the QW laser in 1976, it was noted that additional modification of the DOS conducive to improved laser performance would occur with quantum wire (QWR) confinement [9]. At absolute zero temperature, the DOS √ in a QWR system is inversely proportional to E − E mn , where E mn is a QWR energy eigenvalue. Thus to a firstorder approximation, the DOS approaches infinity at each interband transition energy. In 1982, Arakawa and Sakaki further proposed that the performance of semiconductor lasers could be improved by reducing the dimensionality of the active regions of these devices from QW to quantum dots (QDs) [10]. Because of the 3D confinement of charge carriers in QDs, the conduction and valence bands of an ideal semiconductor QD nanostructure are split into completely discrete energy levels, similar to a single atom. The discrete energy levels in the QD nanostructure lead to a delta functionlike DOS, and thus to a
450
10 Heterostructure Photonic Devices
much narrower transition linewidth compared with bulk or QW semiconductors. The atomlike DOS in quantum dots should drastically improve the performance of optical devices, especially semiconductor lasers. (a) Quantum dot formation To date, the methods employed in QD fabrication experiments have included the postgrowth lateral patterning of QW structures and regrowth on profiled substrates. Methods such as reactive ion etching have been employed in the abovementioned techniques to etch mesas in QW heterostructures. Whether or not this process has been followed by epitaxial regrowth, it has inevitably been plagued by the pitfalls of nonradiative recombination via surface and interface states, and the volumenormalized photoluminescence (PL) intensities have invariably been lower than those obtained from the asgrown QW structures. These processes have yet to produce either useful devices or reliable fabrication processes. Further, these fabricated QD structures generally exhibit geometries far from ideal, such as large size, low density, and size nonuniformity. The nonideal geometries of QD structures fabricated by these methods destroy the singularities in the DOS and eliminate their advantages completely. A more promising way to fabricate QD nanostructures is through a straininduced selfassembling technique. This process exploits the 3D island growth of highly latticemismatched heterostructures. During the growth of latticematched heterostructures, the growth mode is determined solely by the surface and the interface energies between the substrate and the epilayer. Figure 10.33 illustrates different epitaxial growth modes. If the sum of the epilayer surface energy γ2 and the interface energy γ12 is smaller than the substrate surface energy γ1 , i.e., if the epitaxial material wets the substrate, the epitaxial growth occurs in a layerbylayer mode resulting in a smooth epitaxial film. This is the Frank–van der Merve growth mode, as illustrated in Fig. 10.33a. On the other hand, if the sum of the surface energy of epitaxial layer γ2 and interface energy γ12 is larger than the substrate surface energy γ1 , the epitaxial growth is then governed by Volmer–Weber growth mode, where 3D islands are formed on a bare substrate (Fig. 10.33b). However, in latticemismatched heterostructures, elastic strain relaxation becomes the major driving force for selforganized growth of dislocationfree highdensity coherent islands on the substrate, accompanied by a thin wetting layer. The growth may initially proceed in a layerbylayer mode until the critical thickness is reached. For InAs on GaAs, this transition occurs after about 1.8 monolayers (MLs) of InAs have been deposited, while for InAs
Fig. 10.33 Schematics of different growth modes: a Frank–van der Merve, b Volmer–Weber, and c Stranski–Krastanov growth modes
10.3 Laser with QuantumConfined Active Region
451
on InP, the critical thickness is about 3.2 MLs. Beyond that point, the accumulated elastic energy caused by the strain due to latticemismatch tends to be reduced via the formation of individual islands. In these islands, the elastic strains relax and the elastic energy decreases. This results in a Stranski–Krastanov (SK) growth mode, as illustrated in Fig. 10.33c. The most widely studied III–V QD system via SK growth mode is (In,Ga)As on GaAs substrates grown either by MBE or MOCVD. Typical InAs selfassembled islands have a pyramid shape with a base width of about 20 nm and a height of a few nm. Thus the shape of these QDs is a flat pyramid, and their luminescence peaks depend mainly on the variation of the dot height. The lateral size of these islands is comparable to the exciton Bohr radius of the InAsGaAs system and small enough to exhibit the 3D quantum confinement effect. Thus these selfassembled dots are suitable for QD optoelectronic device applications. (b) Selfassembled QD lasers In ideal QD lasers, most of the expected superior performance originates from their atomlike DOS, which is expressed by the delta function. Figure 10.34 displays theoretical roomtemperature gain spectra for QD, QWR, QW, and bulk structures at a constant carrier density of 3 × 1018 cm−3 and an intraband relaxation time of τ in = 0.1 ps. The linewidth and peak intensity of these gain spectra are narrowed down and enhanced, respectively, with the increase of quantum confinement from QW to QWR and QD. The narrow linewidth of the gain spectrum is limited only by the homogeneous broadening caused by intraband relaxation in an ideal QD structure. Due to the large gain peak and narrow linewidth, a significant improvement of the differential gain, dg/dN , is expected for the QD laser. The large optical gain and differential gain result in a reduction of the threshold current density and improved Fig. 10.34 Calculated gain spectra for Ga0.47 In0.53 As/InP (100 Å)3 cubic quantum box, (100 Å)2 quantum wire, 100 Å thick quantum well, and bulk crystal at T = 300 K. Reprint with permission from [11], copyright IEEE
452
10 Heterostructure Photonic Devices
differential quantum efficiency. The large differential gain also results in improved dynamic characteristics of QD lasers. Since the relaxation oscillation frequency of an ideal QD laser is proportional to the square root of the differential gain, a large differential gain enhances the modulation frequency of the laser. The other parameter important for highspeed modulation is the linewidth enhancement factor, which is inversely proportional to the differential gain. A large differential gain results in a small linewidth enhancement factor near zero, leading to a narrow spectral linewidth without spreading under highfrequency operation. Another important feature of ideal QD lasers is that, with infinite barriers for carrier confinement, the threshold current becomes independent of temperature, T 0 = ∞. In practice, the edgeemitting QD laser shares the same doubleheterostructure design as the QW laser. The active layer of a QD laser consists of one or multiple 2D arrays of QDs surrounded by a pair of larger but finite bandgap energy barriers to confine injected carriers. The active region is sandwiched by upper and lower cladding layers with larger bandgap energy and smaller refractive index for effective optical confinement of photons. In order to enhance the modal gain of the QD laser, high QD density with uniform dot size is necessary. Typically, the selfassembled QDs via SK growth mode can reach a dot density around 1011 cm−2 and show high luminescence efficiency. However, the selfassembled QD sizes are nonuniform with a typical size variation of more than ~10% (e.g., Fig. 10.35). A singlelayer InAsGaAs QDs sample shows a typical roomtemperature PL emission peak at around 0.95–1.2 μm and a fullwidth at halfmaximum (FWHM) of ~90 meV. The broad FWHM is caused by the fluctuation of the quantized energy among islands with nonuniform dot heights. When using these QDs as the active layer of the laser, the large inhomogeneous broadening of the spectrum indicates that only a fraction Fig. 10.35 Surface AFM (atomic force microscopy) image of the InAs QDs grown on InAlGaAs/InP deposited with 5.5 MLs of InAs by MBE. The imaged area is 2 μm × 2 μm and the dot density is ~5×1010 cm−2
10.3 Laser with QuantumConfined Active Region
453
of QDs are participating in the laser action. The differential gain of the QD laser is reduced considerably, leading to a high threshold current density. To reduce the threshold current density of the QD laser, it is necessary to use long cavity structures and multiple stacked QD layers to increase the number of QDs in the active region. In a multiple stacked QD system, the structural and optical properties of the InAs QDs are determined by the thickness of the intermediate GaAs barrier layers. The schematics of different stacked SK QD structures are shown in Fig. 10.36. If the GaAs barrier layer (thickness t ≥ 20 nm) is much thicker than the strain field induced by the QDs, the average dot size and density of QDs in each layer are independent of each other. As the barrier layer thickness is reduced close to the average QD height (h), the QDinduced strain field in the lower layer provides the driving force for aligning selfassembled dots in the upper layers perpendicularly. The strain field also causes the upper layer islands to expand slightly as the number of stacked layers increases. Each closely stacked QD layer has a wetting layer indicating it is grown under the SK growth mode. Since the barrier layer between dot layers is thin, the electron wave functions of neighboring dots are overlapped such that QDs are coupled electrically through tunneling in the vertical (growth) direction. Therefore the vertically aligned dots act as a single quantum dot where the effective QD height is controlled by the total stacked dot layers used. Due to its large effective height, the emission wavelength becomes less sensitive to dot size fluctuations than that in a single QD layer. Thus a narrower emission spectrum FWHM of 25 meV is observed from the closely stacked QD structure. However, the accumulated strain in the structure could generate defects and degrade the luminescence intensity. To further improve the optical property of the closely stacked QD structure, the thickness of barrier layers is further reduced to a few (2–3) monolayers (t ≤ h) and the QD material supply during the growth is progressively reduced. Under optimal growth conditions, the dots in the stacked structure are in contact with each other in the growth direction and form a columnar shape as a whole. In the columnarshaped QD structure, both high luminescence intensity and narrow spectrum FWHM of ≤40 meV are obtained. Through improved device technology and growth techniques, in 1993 realistic selfassembled QD lasers demonstrated certain predicted advantages of ideal QD lasers. However, the early models for ideal QD lasers were based on assumptions of latticematched heterostructures with infinite barrier height around QDs. In contrast, the realistic selfassembled QD laser structures demonstrated are based on strained heterostructures with finite energy barriers around QDs. In spite of their less ideal
t
h (a)
(b)
(c)
Fig. 10.36 Schematics of stacked multiple InAs QD layer structures of a isolated QD layers with GaAs barrier layer t ≥ 20 nm, b closely stacked QD layers with a QD height h ≤ t < 20 nm, and c columnarshaped QD layers with t ≤ h
454
10 Heterostructure Photonic Devices
structures, low threshold current density (≤20 A/cm2 ), large T 0 (≥400 K) at temperatures below ~ 200 K, high internal quantum efficiency (≥98%), and small linewidth enhancement factor (30%) has been seen in QWR lasers in comparison with their QW control sample counterparts. However, the improvement of J th is several orders of magnitude smaller than theoretically predicted. Similar to selfassembled QDs, the selfassembled nature of SILO process generated QWRs does introduce nonuniformities to the wire dimensions. These nonuniformities serve to diminish theoretically expected improvements in lasing characteristics for laser diodes made from SILOgrown QWRs. Nevertheless, some unique properties have been observed in SILOgrown QWR lasers. Most importantly, the bandgap of GaInAs QWRs grown by the SILO process responds to temperature changes in ways that deviates from the norm for III–V semiconductors and leads to a temperatureinvariant stable lasing wavelength in Gax In1−x As/InP MQWR laser system. As shown in Fig. 10.39, the 300 and 77 K lasing spectra of a Gax In1−x As QWR laser that was grown using the SILO process are compared to those of a conventional SCH QW laser with latticematched Ga0.47 In0.53 As QWs. The lasing wavelength shift of the Gax In1−x As QWR laser between 300 and 77 K is ~0.9 Å/°C, which is comparable to that of a DFB laser and much less than the value of the conventional QW laser (~4.6 Å/°C). This effect is due to the temperature dependence of the multiaxial strain that exists in SILOgrown QWRs. This bandgap behavior with respect to temperature change of SILOgrown GaInAs QWRs is both physically interesting and potentially applicable to device applications. Fig. 10.39 Lasing spectra measured at 77 and 300 K from a GaInAs QW laser and from a GaInAs QWR laser that was grown using the SILO process. Notice that the lasing wavelength dependence on temperature is drastically reduced in the QWR laser diode. Reprint with permission from [15], copyright AIP Publishing
458
10 Heterostructure Photonic Devices
10.4 VerticalCavity SurfaceEmitting Lasers As discussed above, the optical cavity of a conventional edgeemitting laser lies in the plane parallel to the active layer. In contrast, the verticalcavity surfaceemitting laser (VCSEL) has an optical cavity perpendicular to the active layer plane. The consequences of this simple rearrangement of the orientation of the optical cavity are the improved output mode spectrum and manufacturability of semiconductor lasers. The VCSEL structure may provide a number of advantages over the conventional edgeemitting lasers. These include the following: • VCSELs emit optical beams with a circular symmetric profile that improves the coupling efficiency with optical fiber and other optical components. • Due to the very short optical cavity in VCSELs, dynamic single longitudinal mode operation is easily achievable. • Ultralow threshold current operation of VCSELs is expected due to its small cavity volume. This also allows the formation of densely packed 2D laser arrays. • Because of their verticalcavity orientation, waferscale fabrication and probing can be performed before separating devices into discrete chips. This will reduce the production cost enormously. Because of the difference in optical cavity orientation between VCSELs and edgeemitting lasers, some of the design parameters used for edgeemitting lasers, which have been discussed in preceding sections, may not be applied to the analysis of VCSELs. Hence, we need to develop a proper threshold current density model to identify important design parameters for VCSELs.
10.4.1 Threshold Current Density Before we investigate the VCSEL structure with distributed Bragg reflector mirrors, the familiar Fabry–Perot structures are analyzed. The gain at the onset of the laser action in a Fabry–Perot cavity is generally written as gth = αi + (1/2L) ln(1/R1 R2 )
(10.47)
where α i is the total internal loss, L is the effective length of the cavity, and R1 and R2 are the reflectivity of the mirrors. However, as shown in Fig. 10.40a, the gain in a surfaceemitting laser is not distributed over the entire effective cavity length L; it is contained in a region of thickness d. The total gain in the cavity becomes gth d. The total loss in the cavity is divided into two components: one in the active region, α a , and the other in the rest of the cavity, α c . Thus the gain at the onset of the laser action must be modified as gth d = αa d + αc (L − d) + (1/2) ln(1/R1 R2 )
(10.48)
10.4 VerticalCavity SurfaceEmitting Lasers
459
Fig. 10.40 Schematics of a surfaceemitting laser and b edgeemitting laser showing the active region (shaded) and the standing waves inside the Fabry–Perot optical cavity
The confinement factor is modified as = L T , where the transverse component is T ≈ 1 and the longitudinal component represents the fill factor L ≈ d/L. Equation (10.48) can be rearranged as gth = αa + 1/ 2 [αc (1 − ) + (1/2L) ln(1/R1 R2 )]
(10.49)
Empirically, the peak gain gp is a linear function of the injected carrier density n and expressed as g p = a(n − n tr ).
(10.50)
As derived in Sect. 10.1, the threshold current density has the form of Jth =
qdn th τs
(10.51)
where nth is the injected carrier density at threshold and τ s is the carrier lifetime. For lasers of high material quality, the dominant recombination process is radiative in nature. The carrier lifetime can be written as 1/τs = Br n th
(10.52)
where Br is the radiative recombination coefficient. Combining (10.49) through (10.52), the threshold current density of the surfaceemitting laser becomes Jth =
2 1 qd Br 1 1 α α ln + an + − ) + (1 a c a2 2 L R
(10.53)
460
10 Heterostructure Photonic Devices
Fig. 10.41 Dependence of the threshold current density of a GaAsAlGaAs VCSEL on the active layer thickness and mirror reflectivity. The parameters used for the calculation are: a = 4 × 10−16 cm2 , Br = 10−10 cm3 s−1 , α a = 25 cm−1 , and α c = 10 cm−1 . Reprinted with permission from [17], copyright IEEE
Here we assumed that R = R1 = R2 . Since = d/L, for a fixed L, the threshold current density depends on d and R. Using a GaAsAlGaAs laser with a short cavity of L ≤ 15 μm as an example, (10.53) can be plotted as a function of d and R, as shown in Fig. 10.41. This figure clearly shows that to achieve low threshold current density in a surfaceemitting laser, the active region must be thin and the mirror reflectivities must be extremely high, ideally R ≥ 99%!
10.4.2 Distributed Bragg Reflector Mirrors The extremely high mirror reflectivity required for low threshold surfaceemitting lasers can be achieved by using a distributed Bragg reflector (DBR) mirror design (Fig. 10.42). A DBR consists of N pairs of two dielectric, lossless materials with
Fig. 10.42 Distribution of the optical power intensity inside a typical VCSEL. A DBR consists of N pairs of two materials of thickness L 1 and L 2 with refractive index n¯ 1 and n¯ 2 , respectively
10.4 VerticalCavity SurfaceEmitting Lasers
461
refractive index n¯ 1 and n¯ 2 , where n¯ 1 < n¯ 2 . The thickness of the two layers is a quarter of the Bragg wavelength, λb , that is, L 1 = λb /4n¯ 1 and L 2 = λb /4n¯ 2
(10.54)
The period of the DBR is L = L 1 + L 2 . The reflectivity of this Npair DBR at the Bragg wavelength is given by Rb =
1 − (n¯ 1 /n¯ 2 )2N 1 + (n¯ 1 /n¯ 2 )2N
2 (10.55)
Since n¯ 1 /n¯ 2 < 1, the reflection coefficient tends to unity as N increases. For a fixed number N, the reflection coefficient increases when the ratio n¯ 1 /n¯ 2 is increased. The other important parameter of DBR design for VCSEL applications is the highreflectivity band or stop band. The spectral width of the stop band is given by 2λb n¯ λb ∼ = n¯ eff π
(10.56)
where n¯ = n¯ 2 − n¯ 1 is the refractive index difference of the two constituent materials and n¯ eff is the effective index of the DBR mirror. The effective index can be calculated by requiring the same optical path length normal to the layers for the DBR and the effective medium, which leads to
n¯ eff
1 1 =2 + n¯ 1 n¯ 2
−1 (10.57)
From (10.55) and (10.56), it is concluded that a large refractive index difference in DBR materials is advantageous in achieving high reflectivity and broader stop band with fewer pairs. The effect of refractive index difference on DBR performance is illustrated in Fig. 10.43, where the reflectances of the α (amorphous)Si/Al2 O3 and αGaAs/αAlAs DBRs are compared. Due to the large refractive index difference ( n¯ > 2), the αSi/Al2 O3 dielectric DBR requires many fewer DBR pairs than an αGaAs/αAlAs DBR ( n¯ ∼ 0.5) to reach a reflectivity of >99% while maintaining a wide stop band. One additional advantage of the dielectric DBR reflectors is the absence of absorption loss over a wide optical spectrum. However, the dielectric DBRs are nonconductive and may pose some VCSEL design limitations.
10.4.3 Resonant Periodic Gain in VCSELs From (10.53), a thin active region is required in VCSELs to reach a low threshold current density. However, a thin active region may not provide sufficient gain for the generation of ample optical power. As we have learned, enormous enhancement of
462
10 Heterostructure Photonic Devices
Fig. 10.43 Reflectance of a αSi/Al2 O3 and b αGaAs/αAlAs DBR. The αSi/Al2 O3 DBR consists of 6.5pair lower DBRs, a 2λ active layer, and a 6pair top DBR. The αGaAs/αAlAs structure has a single 20pair DBR [18]
differential gain can be achieved by replacing the bulk active layer with QW material. The drawback of using a QW as the active layer is the reduction of longitudinal confinement factor L (~d/L) by which the threshold current density is increased. This problem can be resolved by using multiple quantum wells (MQWs) as the active layer of the VCSEL. Furthermore, to maximize energy transfer, a good overlap between the QW gain medium and the peak of the standingwave pattern of the lasing mode is necessary. Figure 10.44 illustrates the active region of a VCSEL with a periodic gain structure. The two DBRs are simplified and represented by two metal mirrors such that we can treat it as a Fabry–Perot resonator. For a mirror with high reflectivity, the standing wave of the optical field E(z) can be approximated by Fig. 10.44 a Schematic of the VCSEL cavity structure with periodic gain structure containing three QWs. b Magnitude of the electric field distribution. c The power density distribution
10.4 VerticalCavity SurfaceEmitting Lasers
E(z) = E 0 cos(kz)
463
(10.58)
The timeaveraged optical power density in the standing wave is given by P ∼ E E ∗ ∼ E 02 cos2 (kz)
(10.59)
The positions of the very thin QW active layers, the gain medium, need to be aligned with the peak (antinode) of the standingwave (power) pattern at a selected lasing wavelength λR to gain a maximum power transfer. This can be achieved by ¯ where n¯ is the refractive index separating QWs with spacer layers of thickness λ R /2n, of the spacer layer at λR . Since the QW gain medium is anisotropic and wavelength selective, single longitudinal mode operation is favorable.
10.4.4 Current and Optical Confinements in VCSELs In addition to providing highly reflective DBR mirrors and maximizing the optical field and gain overlap, a VCSEL design should contain some structures to effectively confine carriers in the active region, as in edgeemitting lasers. In Fig. 10.45, three commonly used current confinement schemes in VCSELs are shown. The airpost structure can be fabricated by etching to form a circular or rectangular mesa to confine current inside the small post. However, surface recombination may cause a large leakage current, especially for small devices. The protonbombardment confinement can effectively limit the current into the center active region by producing insulating material in the surrounding region. Since the refractive index of the implanted region does not change after ion implantation, the lateral optical field is not well confined. To improve the optical confinement, a selectively oxidized VCSEL structure was developed (Sect. 5.6). This approach relies on the discovery of a native oxide for Alcontaining III–V semiconductors by Nick Holonyak Jr. of the University of Illinois, which has a major impact on the way VCSELs are fabricated today. The native oxide, formed by oxidizing Al(Ga)As by hightemperature (≥400 °C) water vapor, is used to define the aperture out of which the light is emitted. A unique
Fig. 10.45 Some of the common device geometries for VCSEL devices. The current confinement is achieved using a etched airpost, b ion implantation, and c selective oxidation
464
10 Heterostructure Photonic Devices
Fig. 10.46 Schematic of detailed structure of the oxideconfined GaAs/AlAs VCSEL. To achieve a tight optical aperture, the Alcomposition of the two layers next to the optical cavity is higher than that of the DBR layers
feature of the oxide is the dependence of the oxidation rate on the Alcomposition in the Alx Ga1−x As alloy (Fig. 5.20): the higher the Alcomposition, the higher the oxidation rate. This gives one a high degree of control over the size and location of the oxidedefined aperture within the device structure. In addition to carrier confinement, the low refractive index of the oxidized AlAs (1.74) provides excellent optical confinement in a VCSEL. The detailed layer structure of an oxidedefined GaAs/AlAs VCSEL is shown in Fig. 10.46. In this case, the edge of the DBR mirrors is partially oxidized and forms a continuous longitudinal optical guide like a circular symmetric optical fiber.
10.4.5 Characteristics of VCSELs As is the case with their edgeemitting laser counterparts, some of the important properties of VCSELs can be understood from their light–current–voltage (L–I–V ) characteristics. Figure 10.47 shows the typical L–I–V curves of a GaAs/AlGaAs QW VCSEL with 20 and 30 pairs of epitaxially grown Al0.15 Ga0.85 As/AlAs top and bottom DBRs, respectively. There are two distinct characteristics in this VCSEL when compared with an edgeemitting laser. First, the maximum power output of the VCSEL, under continuous wave (cw) operation, has been severely limited by a sharp rollover in the L–I characteristics. However, the device suffers no apparent damage Fig. 10.47 Typical L–I–V curves of a 15 μm diameter GaAs VCSEL operating under cw condition at a heat sink temperature of 25 °C
10.4 VerticalCavity SurfaceEmitting Lasers
465
Fig. 10.48 Illustration of the effect of shifts in the gain spectrum of a VCSEL at different current injection levels. The shift in the Fabry–Perot cavity resonance is small in comparison and ignored for clarity. Each gain curve corresponds to an injection current a below I th , b just above I th , and c near the peak light output, before rollover. In d and e the VCSEL ceases to lase (I d < I e )
even when the lasing is quenched at a current about twice the threshold value. Second, the voltage drop across the VCSEL is not clamped beyond the threshold value. The voltage across the VCSEL continues to increase with the injection current. The sharp rollover in the L–I characteristics can be qualitatively explained as the mismatch between the gain spectrum and the cavity resonance wavelength (Fig. 10.48), and the high series resistance of DBRs contributes to the continuous increasing of voltage above threshold. Since the VCSEL has an effective short cavity length of ~1 μm, the Fabry–Perot cavity resonance modes are spaced so far apart that there is only one such mode within the spectral gain bandwidth of the active material. The VCSEL lases in a single longitudinal mode as long as the gain at that wavelength exceeds the total cavity losses. Thus, the gain spectrum behaves similarly to that of an edgeemitting laser at low injection currents, where the gain peak increases with current and redshifts, as shown in Fig. 10.48. These gain spectra (a), (b), and (c) qualitatively correspond to the injection currents of I < 4.5 mA (I th ), I ≈ 5 mA, and I ≈ 6 mA, respectively, of the L–I curve shown in Fig. 10.47. However, we notice that the Fabry–Perot cavity resonance mode position is, in general, not coincident with the gain peak in a VCSEL. Furthermore, the position of the Fabry–Perot mode moves relative to the gain peak at a different rate as the temperature changes. For example, near room temperature, the Fabry–Perot mode wavelength of the AlGaAs DBR increases linearly with temperature by ~0.50 Å/°C while the gain peak wavelength of the GaAs active material increases with temperature at a faster rate of ~4.52 Å/°C. Therefore, the VCSEL power output (and threshold) is very sensitive to heating effects. Since current is injected into the active region through the thick multilayer heterostructure DBRs, a large series resistance is added to the laser. An evidence of the large series resistance in the VCSEL is the increasing voltage drop above threshold shown in Fig. 10.47. The voltage across an ideal laser diode beyond threshold should remain clamped at hv/q, where hv is the lasing energy and q is the charge. The excess voltage across the VCSEL at high operation current reflects the high DBR resistance R. Thus, the active region temperature of the VCSEL increases quadratically with injection current since it is proportional to the electrical power
466
10 Heterostructure Photonic Devices
dissipation (I 2 R). Therefore, the resistive heating raises the active region temperature significantly, and the maximum gain will decrease and redshift at high currents as shown in curves (d) and (e) of Fig. 10.48. Although the peak gain may still be higher than the threshold, because of the mismatch between the gain peak and the cavity resonance wavelength, the VCSEL lasing is quenched resulting a rollover in the L–I curve. These highcurrent injection levels qualitatively correspond to I > 10 mA in the L–I curve of Fig. 10.47. If the Fabry–Perot cavity resonance mode is on the longwavelength side of the gain spectrum, a rise in temperature brings the gain peak toward the cavity resonance mode. Hence, a decrease in threshold with increasing temperature can be observed in VCSELs provided the reduction in gain constant is not overwhelming. Because of this, the cavity resonance is often intentionally designed to be at a slightly longer wavelength relative to the peak laser gain at room temperature for optimum VCSEL performance.
10.5 LightEmitting Diodes Lightemitting diodes (LEDs) are pn junctions designed to operate under forwardbiased conditions to generate spontaneous emissions of radiation in the ultraviolet (UV), visible, and infrared (IR) regions of the electromagnetic spectrum. The basic structure of the LED is similar to that of a semiconductor injection laser, as shown in Fig. 10.1, except without a pair of cleaved facets. Under a forward bias condition, the current flow through the LED provides injected excess minority carriers —electrons and holes—necessary for the generation of electroluminescence by the radiative recombination of minority carriers in and near the semiconductor pn junction. As discussed in Chap. 8, highly efficient radiative recombination of excess minority carriers can only be achieved in direct bandgap semiconductors. Although the luminescence efficiency of indirect bandgap materials can be improved by doping isoelectronic impurities, the external quantum efficiency is still relatively low. Therefore, today’s highbrightness LEDs are all made in direct bandgap semiconductor materials. The use of LEDs can be divided into different categories depending on their emission wavelengths; e.g., an IR light source for shortdistance opticalfiber communications, and visible light sources for displays and solidstate lighting. Today the rapid technological advancements have expanded the usage of visible LEDs into many economically and technologically important applications including light sources in traffic signals, fullcolor large outdoor displays, automotive applications (signaling, tail light, and headlight), backlighting in liquidcrystal flatpanel displays, and as sources of general illumination. Thus, the discussion in this section will focus on LEDs that emit visible light (λ between 400 and 750 nm).
10.5 LightEmitting Diodes
467
10.5.1 Efficiency of LEDs When a pn junction LED is under a forward bias condition, the recombination of injected excess minority carriers in the vicinity of the pn junction can release the carriers’ excess energy as photons. The photon flux generated inside the LED then must emerge from the device and provide desired optical stimulus to the eye. However, not all injected carriers will recombine radiatively near the pn junction and a part of the generated photon flux may suffer internal reflections inside the LED die. Light may also be absorbed by the substrate or internally reflected back at the surface boundary and reabsorbed by the semiconductor. Therefore the overall device efficiency is always less than unity and is expressed as ηe = ηi ηxtr
(10.60)
where ηi , ηxtr , and ηe are the internal, extraction, and external quantum efficiency, respectively. The internal quantum efficiency is defined as ηi =
Pa / hν number of photons generated per second = number of injected electrons per second I /q
(10.61)
where Pa is the optical power emitted from the active region, I is the injection current, and q is the electron charge. The material quality and the pn junction design of the LED play significant roles in determining the internal quantum efficiency. Nonradiative recombination can take place through midgap states (Shockley–Read–Hall recombination), surface states, and Auger processes. In highquality direct bandgap semiconductors, only nonradiative surface recombination becomes important, but it can be minimized using heterojunctions. In homojunction devices, some injected electrons may penetrate deep and pass the pn junction before recombination. By utilizing the properties of carrier and optical confinement of the heterojunction, these unwanted losses are greatly reduced in doubleheterojunction devices. The extraction quantum efficiency is defined as ηxtr =
P/ hν number of photons emitted into free space per second = number of photons emitted from active region per second Pa / hν (10.62)
where P is the optical power emitted into free space. In practice, not all the optical power emitted by the active region is emanated into free space. For example, light emitted toward the substrate of the LED can be reabsorbed if the bandgap of the substrate is narrower than the active layer. Light may also be absorbed by the metal contact surface. A major loss mechanism that limits extraction quantum efficiency is related to the total internal reflection at the surface–air interface of the LED. Approaches that involve either encapsulating or shaping the device die have been
468
10 Heterostructure Photonic Devices
shown to be effective in alleviating the total internal reflection problem as discussed next. The external quantum efficiency is defined as ηe =
P/ hν number of photons emitted into free space per second = number of electrons injected into LED per second I /q
(10.63)
It is closely related to the power efficiency or wallplug efficiency of the LED, which is defined as ηpw =
P optical power output = input electric power IV
(10.64)
Assume θ 1 is the angle of incidence with respect to the surface normal in the semiconductor at the semiconductor–air interface of the light emission. According to Snell’s law, the incident angle of the refracted ray into air θ 2 can be expressed as n¯ 1 sin θ1 = n¯ 2 sin θ2
(10.65)
where n¯ 1 and n¯ 2 are the refractive indices of the semiconductor and air, respectively. When θ 2 = 90°, the refracted light travels along the surface and no light can escape the semiconductor. Then θ 1 ≡ θ c is defined as the critical angle for total internal reflection. θc = sin−1 (n¯ 2 /n¯ 1 )
(10.66)
This angle defines the light escape cone where light emitted into the cone can escape from the semiconductor. Otherwise, light outside the cone suffers total internal reflection. Since the refractive index of semiconductors is quite large (~3.5) compared to air (n¯ 2 = 1), the critical angle for total internal reflection is small. Thus most of the emitted radiation is trapped inside the semiconductor by total internal reflection. One common practice to improve the extraction quantum efficiency of the LED is to encapsulate the device within a dome of transparent dielectric material of highrefractive index. Using a dielectric with a refractive index 1.5 to encapsulate the LED of n¯ 1 = 3.5, the light output is enhanced by more than 2.5 times. This method is useful for lowcost highvolume applications. The other method to increase the extraction quantum efficiency is by shaping of LED dies. Ideally, a spherically shaped LED can eliminate the internal reflection problem since light is incident at a normal angle at the semiconductor–air interface. However, the high cost of shaping each die into a sphere makes this approach impractical. Instead, high luminous efficiency (>100 lm/W) and high external quantum efficiency (60%) AlGaInP/GaP red LEDs have been achieved in LED dies by shaping them into truncated inverted pyramids (TIPs) (Fig. 10.49). The TIP geometry improves light extraction by redirecting totally internally reflected photons from the sidewall interfaces toward the top surface of the chip near normal incidence,
10.5 LightEmitting Diodes
469
Fig. 10.49 Schematic diagram of a truncated inverted pyramid (TIP) AlGaInP/GaP LED. Reprinted with permission from [19], copyright AIP Publishing
allowing them to escape. In addition, totally internally reflected photons at the top surface are redirected for escape through the beveled sidewalls. These two processes provide the TIP device with a significant reduction in photon path length within the die compared to a conventional chip, thus reducing internal absorption losses. The light extraction efficiency can also be improved by using textured semiconductor surfaces formed by wetchemical etching. This method has been found to be effective in GaInN LEDs. A substantial amount of surface roughness of pyramidlike structures with smooth side surfaces can be obtained by wetchemical and photochemical etchings. This strong surface scattering structure can easily outcouple the light with a few scattering events.
10.5.2 Materials and Technology Evolution For visible LED applications, the energy bandgap of semiconductors used must be larger than 1.8 eV (~700 nm) to match the luminosity function of the human eye, which is a function of wavelength. In the spectral range from red to yellow/orange, there are three ternary alloys, GaAs1−x Px , Alx Ga1−x As, and Gax In1−x P, and one quaternary alloy, Alx Gay In1−x−y P, with suitable direct energy bandgaps. For LEDs with even shorter wavelength in the blue and green spectral range, the current choices are IIInitride material systems, specifically Gax In1−x N. The relevance of these alloys to the visible LED development is summarized in Fig. 10.50 where the evolution of LED performance in terms of luminous efficiency is plotted versus year. It reveals that the performance of visible III–V LEDs has improved dramatically over the past half century since the demonstration of the first GaAsP red LED in 1962 by Nick Holonyak Jr. at General Electric. Over this period of time, the LED performance increased roughly ten times every decade, mainly driven by the advancement of material technologies including material selections, epitaxy methods, and heterostructure designs to improve the internal quantum efficiency. The development of chip technologies with improved light extraction advances the external quantum efficiency performance of LEDs. The GaAsP crystal used for the fabrication of the first red LED by Holonyak was grown using a closed tube vapor transport technique. Then the vaporphase epitaxy (VPE) technique was developed for commercial production of GaAsP red LEDs. The green and red GaP LEDs were grown by LPE doped with isoelectronic impurities
470
10 Heterostructure Photonic Devices
Fig. 10.50 Light output of visible LEDs during the last 50 years. The luminescence efficacy increased at a rate of ~10 ×/decade. At the moment, the luminous efficacy of laboratory white LEDs exceeds that of all other conventional light sources. Reprinted with permission from [20], copyright IEEE
N and ZnO pairs, respectively. The VPE growth technique was then developed to incorporate a significant amount of N isoelectronic impurities into indirect bandgap GaAsP alloys creating relatively highperformance amber, yellow, and yellowgreen LEDs. Nevertheless, the quantum efficiency of these indirect bandgapbased visible LEDs is limited by the fundamental physics. Furthermore, the ternary GaAsP alloy does not latticematch to any III–V binary substrates except near the binary ends, which leads to high defect density and low luminescence efficiency. Consequently, it was necessary to search for alternative material systems. In 1970, cw operation of AlGaAs/GaAs DH injection laser diodes at room temperature demonstrated that LPE growth and DH design were useful for the fabrication of AlGaAs red LEDs. In addition, the lightabsorbing GaAs substrate could be easily removed by the use of wetchemical etching to enhance the luminescence efficiency of LEDs to over 10 lm/W, which was bright enough for outdoor applications including traffic signals, automobile stoplights, and alphanumeric signs. However, the high aluminum content (>60%) used in AlGaAs layers of red LEDs posed a serious reliability problem in hot humid outdoor applications where the reaction of Al with oxygen could lead to device failure. To solve this problem, the quaternary alloy AlGaInP was then developed. The potential of using AlGaInP as a lightemitting material from red to yellow/amber was recognized much earlier since it can latticematch to GaAs substrates over almost the whole direct bandgap region. In spite of this, the epitaxy technologies of the time were LPE and VPE, both of which had insurmountable technology difficulties for AlGaInP growth. During the late 1970s to mid1980s, the MOCVD epitaxy technology had progressed to a point that highopticalquality III–V alloys could be produced even
10.5 LightEmitting Diodes
471
for aluminumcontaining materials. Since 1990, MOCVDgrown AlGaInP LEDs became the dominant highefficiency red, orange, and yellow LEDs. To enhance the light extraction efficiency of AlGaInP LEDs, additional chip technologies using transparent GaP window layer, removing the lightabsorbing GaAs substrates, and utilizing shaped chip have been implemented. These innovations have led to a red LED with a performance of 100 lm/W! Although the performance of red LEDs had improved steadily, highperformance blue and green LED technologies were not available until the early 1990s due to the lack of suitable material technologies. Since the early 1970s, there had been a number of reports of GaNbased blue/violet lightemitting devices using VPE method. The real breakthrough did not come until the late 1980s and early 1990s when Akasaki’s team at Nagoya University, Japan, solved some key issues of GaN growth: The MOCVDgrown GaN layer quality was substantially improved by using an AlN lowtemperature buffer layer on (0001) sapphire substrates. The ptype GaN was finally realized using Mg as a dopant coupled with a postgrowth electron beam irradiation to activate acceptor atoms. The first GaN pn junction LED was finally realized in 1992. In 1995, highperformance green and blue LEDs were demonstrated by a Nichia team using GaInN/GaN quantumwell structures. The current stateoftheart external quantum efficiency of highperformance visible LEDs as a function of wavelength is summarized in Fig. 10.51. Relative to the peak eye response wavelength (555 nm), AlGaInP technology and IIInitride technology dominate longer wavelength LEDs (red, orange, and amber) and shorter wavelength LEDs (green and blue), respectively. Although the external quantum efficiency of both red and blue LEDs exceeds 50%, there exists a ‘green gap’ where the efficiency drops quickly between 500 and 600 nm. For the AlGaInP system, it is the direct–indirect bandgap transition that limits the external quantum efficiency beyond 600 nm. For the GaInN system, the efficiency drop in green LEDs is due to effects associated with latticemismatch when a high InN mole fraction layer is used. The highly dense dislocations induced in the GaInN layer act as nonradiative recombination centers. Furthermore, the compressive straininduced builtin electric Fig. 10.51 External quantum efficiency of LEDs of different colors as a function of wavelength. InGaN devices produce green and blue, and AlInGaP devices produce red, red–orange, and yellow. CIE eye sensitivity function is also shown as the solid curve. Reprinted with permission from [20], copyright IEEE
472
10 Heterostructure Photonic Devices
Fig. 10.52 Luminescence spectrum of blue (450 nm)pumped phosphors for generating white light
fields along the caxis of the wurtzite crystal cause electrons and holes to separate spatially within the same quantum well (e.g., Fig. 7.29), leading to an efficiency drop. At the moment, green LEDs are not efficient enough to mix with red and blue LEDs to generate white light. Instead, phosphorconverted LEDs are used. For instance, white light can be generated by a blue LED pump source coated with a layer of yellowemission phosphor such as Y3 Al5 O12 :Ce3+ or YAG. The excitation spectrum of YAG at ~440–460 nm is wellmatched to blue GaInN LEDs. The resulting light is a combination of blue (450 nm) and broadband yellow/orange (peaked at 550–600 nm), which appears white to the eye (Fig. 10.52). The current white LED performance has already reached 100 lm/W and exceeds the performance of conventional lighting technologies such as fluorescent and halogen.
10.6 Quantum Cascade (QC) Lasers Lasing in semiconductor QW lasers takes place through radiative recombination of conduction band electrons and valence band holes across the direct energy gap of the QW, under the momentum conservation condition ( k = 0), known as interband transitions (Fig. 10.53a). The transition energy is determined by the bandgap energy of the QW plus the confinement energies of the electron and hole. Consequently, the smallest transition energy is determined by the gap of the QW material. Alternatively, the transitions in a QW can also occur between confined states of the same band (conduction or valence). Since it relies on only one type of carrier making electronic transitions between subbands, the process is referred as unipolar intersubband transitions. In this case, the smallest transition energy reduces toward zero as the well width is increased. This unique feature is central to the intersubband transition because it enables the fabrication of longwavelength devices over a wide frequency range (from midinfrared to terahertz) using the same heterostructure materials. As shown in Fig. 10.53b, the initial and final states of subband within a QW have the
10.6 Quantum Cascade (QC) Lasers
473
Fig. 10.53 Energy band diagram and density of state dispersion curves of a quantum well of a interband transition, and b intersubband transition
same inplane dispersion. This allows the scattering of an electron from the upper to lower state by any transition, elastic or inelastic, as long as it provides the necessary momentum exchange. Therefore, the electron lifetime is very short, of the order of picoseconds, and is dominated by nonradiative recombination process. In 1971, R. Kazarinov and R. Suris proposed a unipolar intersubband laser structure where electrons in the QW of a superlattice made transitions between subbands for light amplification [21]. In their designs, a strong electric field is applied to the superlattice such that electrons tunnel from the ground state of one QW to the excited state of the neighboring well, emitting a photon in the process via the photonassisted tunneling process. The electrons are then nonradiatively relaxed to the ground state and tunneled into the excited state of the next stage ready for photon generation again. The process repeats sequentially for many stages to generate optical gain of the laser. This work prompted a great deal of interests, although mostly theoretical due to the lack of a proper thin film growth technique. Finally, in 1994, the first unipolar intersubband laser, called the quantum cascade (QC) laser, was demonstrated at Bell Laboratories, thanks to the convergence of two key techniques: molecular beam epitaxy (MBE) and bandstructure engineering. Using quantum wells, superlattices, and digitally composition graded alloys as building blocks, the bandstructure engineering method allows the design of devices with arbitrary shape of energy band diagrams. Thus, QC laser structures can be designed and their properties tailored for specific needs. To construct such a complex device structure consisting of hundreds of thinlayer heterojunctions, MBE with its ability to grow atomically abrupt heterojunctions incorporating precisely designed composition and doping profiles, is the epitaxial method of choice. Thus far, QC lasers with emission wavelengths from midinfrared (~3.5 μm) to terahertz (≥200 μm) have been demonstrated.
474
10 Heterostructure Photonic Devices
10.6.1 QC Laser Active Region Designs The basic structure of a QC laser consists of a periodic arrangement of cascade periods, each one consisting a number of QWs and barriers with a complex heterostructure potential profile. Figure 10.54a shows a portion of the conduction band energy diagram of the first QC laser reported in 1994. The laser structure was grown by MBE with the Al0.48 In0.52 AsGa0.47 In0.53 As heterojunction material system latticematched to InP substrate. The injected electrons make diagonal radiative transitions between subbands of two neighboring QWs and are recycled from stage to stage, contributing in each stage to the gain and photon emission. Therefore, each electron injected above lasing threshold generates M photons leading to an optical power proportional to M, where M is the number of cascade stages. However, in order to achieve lasing, population inversion in the structure is a necessary condition. Unlike interband transition lasers, where carrier recombination involves bandtoband transitions, optical transitions in intersubband lasers are taking place between discrete subbands as in a threelevel laser system. Therefore, a careful design of scattering times of each subband and between subbands is necessary. As noted in Fig. 10.54a, each stage of the QC laser is divided into a gain or active region and an injection/relaxation region. The gain region is the section where a population inversion between the two levels of the laser transition takes place. Following the gain region is an injection/relaxation region to raise the energy of the electron state, thus facilitating injection by resonant tunneling in the next period. This function is achieved by digitally alternating QWs and barriers with changing duty cycle to create a section of material with effective increasing bandgap. The
Fig. 10.54 a Conduction band energy diagram of a portion of the QC laser based on a diagonal transition between states 3 and 2. The dashed lines are the effective conduction band edges of the digitally graded electroninjecting region. Electrons are injected into the energy level state 3 of the active region. b E–k curves of the energy subbands from three QWs. The bottoms of these subbands correspond to the energy levels 1, 2, and 3 indicated in (a). Reprinted with permission from [22], copyright AAAS
10.6 Quantum Cascade (QC) Lasers
475
middle part of the injection region is also doped to prevent the formation of strong spacecharge domains and provide electron charge injection to the next stage. Usually the active region contains twotothree QWs to form a ladder of three states such that electrons are injected in the third state and the population inversion is maintained between the third and second states. Assuming perfect injection efficiency in the third state, the population inversion condition is simply τ 32 > τ 2 ; i.e., the total lower state lifetime τ 2 is shorter than the electron scattering time from the third state to the second state τ 32 . One way to shorten the transition lifetime between two states is by increasing the overlap of wave functions. In the first working QC laser reported in 1994, a diagonal transition between states 3 and 2 of two adjacent QWs was used where the reduced wave function overlap enhances the scattering time from state 3 to state 2. On the other hand, strong reduction of the relaxation time τ 21 is obtained in the heavily overlapped and closely spaced states 2 and 1 of two adjacent QWs. Furthermore the separation between these two subbands is designed to be equal to the optical phonon energy. Thus the strong inelastic relaxation by means of resonant optical phonon emission between these two states will reduce the lifetime τ 21 to subpicosecond. Finally, the tunneling escape time out of state 1 is extremely short, further assisting the population inversion. In addition to the diagonal transition active region design, laser structures based on a vertical transition (i.e., with the initial and final states placed in the same QW) for lower threshold current have also been developed. The main challenge in designing such QC lasers is to suppress electrons tunneling out of the state 3 into the continuum, such that the electron population in state 3 exceeds that of state 2. The population inversion is achieved if the relaxation time τ 32 for the transition from state 3 to state 2 exceeds the electron lifetime τ 2 in state 2. To efficiently reduce the relaxation time τ 21 by means of resonant optical phonon emission, the energy separating states 2 and 1 are designed to be equal to the optical phonon energy. To prevent accumulation of electrons in the lower state 1, a downstream superlattice injector is used where state 1 is aligned with the miniband of the superlattice (Fig. 10.55). The injector superlattice is also designed so that a minigap faces the upperstate 3, thus suppressing electron Fig. 10.55 Conduction band energy diagram of a portion of the QC laser based on a vertical transition between states 3 and 2 of the same QW. Electrons are injected into the energy level state 3 of the active region. Reprinted with permission from [23], copyright AIP Publishing
476
10 Heterostructure Photonic Devices
escape by tunneling. As a result, electron population builds up sufficiently to allow laser action at a reasonably low threshold current density. Highperformance unipolar intersubband QC lasers with QW active regions have been demonstrated with emission wavelengths up to 11 μm. But further extension of the laser emission to even longer wavelength using the same active regions is difficult. Since intersubband transitions are characterized by decreasing radiative efficiency and optical waveguide losses (∝λ2 ) with decreasing transition energy, conventional intersubband QC laser structures show prohibitively high threshold current densities at longer wavelength. This problem can be solved by replacing the QW in the active region with semiconductor superlattices (SLs) that consist of a periodic stack of nanometerthick layers of two materials (QWs and barriers). The advantages of SL QC lasers based on optical transitions between conduction minibands are the intrinsic population inversion associated with the large interminibandtointraminiband relaxation time ratio and the high oscillation strength of the laser transition at the SL Brillouin zone boundary. In addition, due to the wide energy minibands, SL QC lasers can be driven with very large current densities without compromising laser performance. A schematic band diagram of the SL QC laser with graded (chirped) SL is shown in Fig. 10.56. In the SL active region, the well thicknesses are gradually decreased in the direction of electron motion. At zero bias, the states of the QWs are localized because the variation in the thickness of adjacent layers is such that the corresponding energy levels of the isolated wells are out of resonance. Minibands are formed when an electric field of the appropriate magnitude and polarity is applied to bring these states into resonance. The energy levels in each active SL are grouped together in two welldefined minibands, with the intermediate injector region bridging them together across the cascade stages. Laser action takes place at the edge of the minigap between minibands 2 and 1. Fig. 10.56 Conduction band energy profiles of a portion of the chirped superlattice QC laser active regions and injector regions. The shaded areas indicate the extent of the electron minibands. Laser transitions are indicated by wavy arrows between level 2 and level 1. Reprinted with permission from [24], copyright AIP Publishing
10.6 Quantum Cascade (QC) Lasers
477
As mentioned above, the SL QC laser exhibits attractive features of very large oscillator strength and a favorable ratio of lifetimes. However, when a strong electric field is applied on a periodic SL, it will break the miniband of the SL into a set of localized states, losing all the favorable features of the extended states. Alternatively the boundtocontinuum active region, which can be seen as an evolution of the SL design, is developed for maintaining a high population inversion and low threshold current densities [25]. Because of the localization of the upper state, the oscillator strength is spread between the upperstate and a number of lowerstates in the miniband. This active region design offers many interesting features, including high characteristic temperature T 0 (as high as 190 K) and longwavelength (16 μm) operation, including terahertz generation.
10.6.2 Threshold Current and Waveguide Designs (a) Threshold current density The lasing condition of a QC laser may be analyzed by considering a threelevel system of the active region in a rate equation approach. As shown in Fig. 10.57, electrons are injected in state 3 from the ground state of the injector of the previous stage at a rate of J/q, where J is the current density (A/cm2 ). Electrons may scatter from state 3 to states 2 and 1 with rates 1/τ 32 and 1/τ 31 , respectively. The lifetime of state 3 may include an escape process into the continuum with a lifetime τ esc and 1/τ 3 = 1/τ 32 + 1/τ 31 + 1/τ esc . Also included are electrons that are thermally activated to state 2 with an equilibrium population n th 2 . Its value is determined by ng , the sheet doping density of the injector, , the energy difference between the state 2 and the Fermi level of the injector and is expressed as
Fig. 10.57 Schematic diagram of a QC laser with various tunneling and relaxation processes used in the rate equations
478
10 Heterostructure Photonic Devices
n th 2 = n g exp(− /kT )
(10.67)
The rate of change of the population of each state may be formulated as J n3 dn 3 = − − N g(n 3 − n 2 ) dt q τ3 n3 dn 2 n 2 − n th 2 = + N g(n 3 − n 2 ) − dt τ32 τ2 dN n3 c = [N g(n 3 − n 2 ) − αT ] + β dt n¯ τsp
(10.68a)
(10.68b) (10.69)
In above equations, ni is the electron sheet density per period in state i, N is the photon flux per period and unit active region width, n¯ is the refractive index, g is the gain coefficient, α T is the total modal loss, β is the fraction of the spontaneous emission coupled into the laser mode, and τ sp is the spontaneous emission lifetime. The gain for intersubband transition between states 3 and 2 per one stage is expressed as g=
2 z 32 4πq 2 0 nλ ¯ (2γ32 )L p
(10.70)
where z32 is the dipole matrix element, λ is the wavelength, 2γ 32 is the linewidth or the fullwidth at halfmaximum of the transition, is the total confinement factor, and L p is the length of one period. Below threshold, under steadystate conditions, we can set dn/dt = 0 and N = 0. Then (10.68a) becomes n3 = J
τ3 q
(10.71)
Inserting this result in the second rate equation, one obtains n = n 3 − n 2 = J
τ2 τ3 τeff − n th 1− − n th 2 = J 2 q τ32 q
(10.72)
where τ eff = τ 3 (1 − τ 2 /τ 32 ) is the effective lifetime. This equation links the population inversion n to the electric pumping, J. The population inversion can only exist if τ eff > 0, i.e., if τ 32 > τ 2 . At the threshold current density, the modal gain must equal to the total loss, i.e., g n = α T . Thus, the threshold current density per each stage of the QC laser is
¯ q 0 nλ(2γ q αT 32 )L p αT th th + n2 = + n2 Jth = 2 τeff g τeff 4πq 2 z 32
(10.73)
10.6 Quantum Cascade (QC) Lasers
479
Above threshold, the gain is fixed and N increases linearly similar to diode lasers described in Fig. 10.10. From (10.73), it is clear that a low threshold and highefficiency QC laser will be obtained in the laser structure with a large ratio of τ 32 /τ 2 , a narrow transition linewidth γ 32 , and a long upperstate lifetime τ 3 . (b) Midinfrared waveguide designs In (10.73), an important contribution to the laser threshold is the total loss α T experienced by the light traveling in the waveguide. The major losses are the mirror loss α m , and the waveguide loss α w . The mirror loss can be reduced using highreflection coating at the mirror facets. The major source of waveguide losses is freecarrier absorption in the doped semiconductor regions and the metallic contact layers. While the influence of the metallic layers can be suppressed, the freecarrier absorption loss in doped semiconductors is unavoidable. This semiconductor loss follows a simple Drude model and increases approximately quadratically with the wavelength in midinfrared range. In shorter wavelength QC lasers, such as the first demonstrated QC laser (λ = 4.3 μm), the dielectric waveguide is a simple choice if the material system in use provides sufficiently large refractive index variations to build the waveguide. In such cases, the highindex core consisting of the active regions is sandwiched between lowindex cladding layers leading to a relatively symmetrical optical intensity profile in the waveguide. Nevertheless, in order to decouple the midinfrared wavelength light from the surface plasmon at the semiconductor/metal interface, the minimum thickness of the waveguiding layer needed is of the order of a wavelength. This requirement is easily fulfilled for the bottomcladding layer by using a suitable substrate material as a part of the cladding layer. For the top cladding layer, however, this requires a prohibitively long material growth time for QC lasers as the emission wavelengths increase beyond 15 μm. To limit the thickness of the top cladding layer, a plasmonenhanced waveguide design has been developed. Figure 10.58 shows the optical mode and refractive index profiles of such an AlInAs/GaInAs/InP QC laser structure. At the top of the laser structure, a heavily doped (7 × 1018 cm−3 ) GaInAs:Si layer is added to suppress the coupling between the fundamental waveguide mode and Fig. 10.58 Mode intensity profile and the refractive index profile as a function of layer thickness of a QC laser incorporating a plasmonenhanced heavily doped semiconductor confinement layer. The surface is located at zero distance. Reprinted with permission from [26], copyright AIP Publishing
480
10 Heterostructure Photonic Devices
the surface plasmon mode propagating along the metal contact–semiconductor interface. This heavily doped GaInAs layer has a plasma frequency (9.4 μm) approaches but does not exceed that of the waveguide mode (8.4 μm) of the laser. Near the plasma frequency, the anomalous dielectric dispersion strongly depresses the refractive index of the layer at the laser wavelength from ~3.5 (value of an undoped layer) to ~1.2. The insertion of this low refractive index top layer beneath the metal contact completely decouples the waveguide mode from the interface plasmon and increases the confinement factor of the mode by pushing the mode away from the metal contact. For a longwavelength (≥15 μm) QC laser, rather than decoupling the guided wave and the interface plasmons, radically different waveguide designs utilizing the surface plasmons have been developed. Since metals and doped semiconductors behave like plasma in midinfrared frequencies, the electromagnetic surface waves (interface plasmons) at a metal–semiconductor interface can be used as the main guiding mechanism. The metal layer is now deposited directly above the active material of the laser and used as the waveguiding interface. The obvious advantage of this approach is that no additional cladding layer is needed since the amplitude of the optical wave decreases exponentially in the direction normal to the metal– semiconductor interface. In this type of waveguide, the modal losses are strongly dependent on the dielectric constants of the metal and semiconductor used. The loss of the plasmon waveguide at the metal–dielectric interface can be expressed as α=
4π n¯ m n¯ 3d κm3 λ
(10.74)
where n¯ and κ are the real and imaginary parts of the dielectric constant of the metal √ √ ( m = n¯ m +iκm ) and dielectrics ( d = n¯ d ). Therefore, it is apparent that the losses at the interface are inversely proportional to the wavelength λ and can be minimized by choosing metals having a refractive index with a large imaginary component. Palladium and gold are the most suitable metals for wavelengths around 10 μm and ≥15 μm QC laser applications, respectively. The normalized mode intensity depth profile of the surface plasmon waveguide for a QC laser with an emission wavelength of 11 μm is shown in Fig. 10.59. It is noted that the confinement factor is more strongly enhanced (≥70%) than that of a regular dielectric waveguide (~40%). To further improve the waveguide design for the realization of QC lasers at even longer wavelength in the terahertz range, a doublesurface plasmon waveguide was developed. In this waveguide structure, the lightly doped GaInAs lower cladding layer is replaced with a heavily doped layer acting as a bottom metal. The waveguide structure is essentially the same as a microwave metal waveguide, and the optical confinement is close to unity as shown in Fig. 10.59b.
10.6 Quantum Cascade (QC) Lasers
481
Fig. 10.59 Mode intensity profile as a function of layer thickness of a QC laser incorporating a a surface plasmon waveguide with λ = 11 μm. Reprinted with permission from [27], copyright Optical Society of America; and b a doublesurface plasmon waveguide with λ = 21 μm. The surface is located at zero distance. Reprinted with permissions from [28], copyright AIP Publishing
Fig. 10.60 Threshold current density as a function of the number of active region stages measured at 10 K in pulse mode (solid circles) and in cw mode (open triangles), and in pulse mode at room temperature (solid squares). Lasers with M ≤ 6 stages did not lase at room temperature. The threshold current density at the highest operating temperature is displayed instead. Reprinted with permission from [29], copyright AIP Publishing
10.6.3 Quantum Cascade Laser Operation Characteristics QC lasers are unique among semiconductor lasers in their operation principles which are based on intersubband transitions and on the cascading scheme, where a large number (typically 16 ≤ M ≤ 35) active regions are stacked upon each other separated by electron injection regions. Under an appropriate applied bias voltage, the localized states of M active regions merge into one continuous cascade of optical transitions,
482
10 Heterostructure Photonic Devices
allowing each electron to create M photons. Consequently, QC lasers display an external quantum efficiency significantly larger than unity, which is unattainable for conventional interband lasers. One important consequence of increasing the number of stages for waveguide consideration, which in turn increases the total active layer thickness, is the increase in confinement factor with increasing M. For example, the confinement factors of identical QC lasers incorporated with different numbers of active regions of M = 1, 3, 6, 12, 20, 30, 45, 60, and 75 are calculated. These lasers have threewell vertical transition design of the active region emitting at ~8 μm wavelength. The confinement factor grows approximately linearly with the number of stages up to M ≈ 30 ( 30 = 0.49) and saturates for higher M ( 75 = 0.81). The increased confinement factor for lasers with larger M leads to a larger modal gain coefficient and, thus, decreased laser threshold current. Figure 10.60 shows the measured and calculated J th as a function of M measured at room temperature and low temperatures (10 K). A lowtemperature threshold current density J th ≤ 2 kA/cm2 is consistently achieved for M ≥ 15. Devices with M ≥ 12 stages displayed laser action in pulse mode at and above room temperature. For smaller M, J th rises rapidly, at a rate proportional to 1/M, as a direct consequence of the reduced confinement factor. In addition, lasers with M ≤ 6 stages did not show laser action at room temperature and their highest operation temperatures are 225, 170, and 110 K for samples with six, three, and one stages, respectively. In conventional interband lasers, the turnon voltage V on of the I–V characteristics is fixed and depends on the energy gap of the semiconductor material used. For QC lasers, the turnon voltage of the device is not fixed but depends on the number of stages M. At zero bias, due to the highly localized subband states in each QW, the QC laser structure is highly resistive. Only when a suitable electric field is reached, merging all localized states into one continuous cascade of transitions allowing efficient injection and carrier transport between stages can large currents then flow through the structure. The energy drop per stage is determined by the sum of transition energies between subband states (E 32 + E 21 ) in the active region, and the voltage drop across the entire Mstage cascade is given by VS (M) =
E 32 + E 21 ·M q
(10.75)
The turnon voltage of the QC laser is simply expressed as V on = V S + V os , where V os is the offset voltage associated with the contact resistance and lightly doped waveguide layers. Thus the operation voltage of the device is approximately proportional to M which is a consequence of cascading. Figure 10.61 shows the measured IV characteristics for all laser samples shown in Fig. 10.60. Using the voltage drop across the entire Mstage cascade V S (M), the differential series resistance ρ = ∂V/ ∂J, and the threshold current density J th , the voltage at laser threshold V th can be calculated as
10.6 Quantum Cascade (QC) Lasers
483
Fig. 10.61 Current–voltage characteristics of QC laser devices having different stages M between 1 and 75 with the uppermost trace corresponding to M = 75. The trace of M = 1 is drawn as a dashed line. The cross symbol on each curve denotes the threshold voltage, V th . Inset: V on (solid triangles) and V th (open circles) as a function of M. Reprinted with permission from [29], copyright AIP Publishing
Vth (M) =
∂V E 32 + E 21 · M + Vos + · Jth (M) q ∂J
(10.76)
The last term of the above equation accounts for the bias acquired above V on by the current that is needed for the gain to overcome the losses. As shown in the inset of Fig. 10.61, V on monotonically deceases with decreasing M. V th follows this general trend except for devices of very low M (≤3) due to the associated high threshold current. From the rate equations, by again setting the time derivatives to zero and differentiating over J, one obtains the slop efficiency per facet for the whole laser stack: τ2 αm Mhν dP 1− (10.77) (M) = dI 2q αi + αm τ32 where hv is the photon energy. It is apparent that a large number of stages will result in a large slope efficiency and highoptical output. Figure 10.62 shows the Fig. 10.62 Measured slope efficiency per facet of QC lasers as a function of M obtained under cw mode (triangles) and pulse mode (circles). The average slope efficiency per facet per stage of these samples is about 8 mW/A. Reprinted with permission from [29], copyright AIP Publishing
484
10 Heterostructure Photonic Devices
measured slope efficiency at cryogenic temperature for those samples with different M mentioned above. From the slope efficiency the total external differential quantum efficiency per facet is calculated as ηd (M) =
q ∂P (M) hν ∂ I
(10.78)
Using the data from Fig. 10.62, ηd ~ 8.5% per stage is obtained. Consequently, a value of ηd (M) larger than unity is obtainable for QC laser structures with M ≥ 12 stages.
10.6.4 Interband Cascade Lasers—TypeII QC Laser The quantum cascade laser, which employs unipolar intersubband optical transitions in the active region, is the first laser technology to achieve roomtemperature cw operation beyond the MWIR (3–5 μm) milestone. However, for QCLs using the InGaAs/InAlAs material system, the shortest wavelength for which roomtemperature cw lasing has been attained is 3.8 μm. This limitation is due to the excessive strain required to maintain sufficient conduction band offset in the active region. Other QCLs and typeI QW lasers based on different III–V material systems have yet to achieve roomtemperature cw operation in the MWIR spectral range. On the other hand, roomtemperature pulse operation has been achieved in Wtype QW lasers with the typeII band alignment for the MWIR emission. Thus, it is possible to combine the interband Wtype laser active region with the multistage QC structure for lower threshold and higher quantum efficiency such that roomtemperature cw lasing can be realized. The resulting device design is a typeII bipolar QCL with interband optical transitions in the active region, or an interband cascade laser (ICL). The singlestage band structure of an InAsbased ICL is illustrated in Fig. 10.63. Similar to QCLs, multiple stages of the InAsbased typeII Wtype QW active regions are connected in series in a staircase ICL design. The injected electrons from the previous stage on the left tunnel through the AlSb barrier into the conduction band of the InAs QW and recombine with holes in the valence band of the neighboring GaInSb QW. The location of the electron subband energy in the Wtype active region is positioned inside the bandgap of the GaSb layer to prevent electrons from tunneling into the following GaSb layer and force the electrons to recombine with holes in the GaInSb layer. When an electron transitions into the valence band, it gives up energy in the form of photon emission followed by tunneling through the AlSb barrier into the GaSb hole subband of the hole injector region. Separating the hole injector and electron injector regions is an AlSb/InAs heterostructure with a typeII interface. Under zero bias, the conduction subbands of InAs QW on the electron injector side and valence subbands of GaSb QW on the hole injector side are separated by a small energy. When properly biased, these states are energetically aligned to form a
10.6 Quantum Cascade (QC) Lasers Active region
2.5
485
Hole Injector
InAs
Energy (eV)
2.0
Electron Injector
AlSb EC
1.5 InAs
1.0
GaSb
0.5 0 0.5 1.0
GaInSb 0
Semimetallic Interface
100
200
EV 300
400
500
Distance (Å) Fig. 10.63 Conduction band and valence band profiles for one stage of an ICL under bias, along with the active region of the succeeding stage. Some of the important electron and hole wavefunctions are also plotted. Reprinted with permission from [30], copyright IEEE
semimetal interface such that electrons in the valence band of GaSb can be scattered elastically back to the conduction band of InAs in the electron injector region which consists of InAs/Al(In)Sb chirped superlattices. Thus, similar to typeI QCL, an electron recycling through additional stages in ICL increases the injection quantum efficiency to produce multiple photons. While the cascading concept of ICL was motivated in part by the earlier development of the intersubband QCL, the intricate physical principles governing QCL and ICL operation are not completely equivalent. The major difference between ICL and QCL results from their vastly different carrier lifetimes. The short effective lifetime of carriers in the upper level of the QW in an intersubband QCL is limited by a combination of optical phonon and interface roughness scattering and has an empirical value of ≤1 ps. In contrast, the interband transition in the QW of the ICL has a rather long carrier lifetime of ~1 ns. The relatively long carrier lifetime in the typeII QW of ICL leads to two orders of magnitude larger modal gain per stage than a QCL. The consequence is that it typically requires 30 or more stages in a QCL, and less than 10 stages in an ICL, to achieve roomtemperature laser operation with a low threshold current density. For λ ≈ 4.6 μm, the lowest reported threshold current densities at room temperature for QCLs with 3040 stages remain at ~800 A/cm2 and increase at shorter wavelengths. By contrast, the lowest roomtemperature threshold current density reached for a 10 stage ICL emitting at ~3.6 μm is E B and E B is the barrier height. The condition of E > E B also implies (E − E F )/kT 1. The final expression of the dark current becomes Id = q Aυ
m ∗ kT π 2 L p
exp[−(E B − E 1 − E F )/kT ]
(10.90)
10.7.3 Photoconductive Gain The device operation of the QWIPs is similar to that of extrinsic semiconductor photoconductors except that the incident photons are only absorbed in discrete quantum wells. The photocurrent caused by intersubband excitations in a QWIP can be estimated through the concept of photoconductivity gain, which is defined as the number of electrons flowing through the external circuit for each photon absorbed. For a simplified analysis of the photoconductivity gain, four approximations are made to
10.7 QuantumWell Infrared Photodetectors (QWIPs)
491
Fig. 10.67 Schematic representation of the photoconductive gain mechanism in a single well of a biased QWIP
ip
Ip
EB Trapping E1
Photoemission
define the physical regime: (a) The barriers are thick such that the interwell tunneling is negligible. (b) The electron density in each well remains constant under applied bias. (c) The QW confines one bound state with the excited state either in resonance or very close to the top of the barrier. (d) The twoterminal metal contacts form ideal ohmic contacts. The physical process and the gain mechanism of a simple onewell structure are given in Fig. 10.67. When infrared radiation is shone on the detector, there is a photemission of electrons from the well that contributes to the photocurrent I p in the external circuit. The photoconductive gain is a result of the extra current injection from the contact necessary to balance the loss of electrons from the QW due to photoemission. Thus the total current I p consists of contributions from the direct photoemission and the extra current injection. The photocurrent generated from one well is i p = q Aηw pe = q A
η pe Nw
(10.91)
where A is the detector illumination area, is the incident photon number per unit time, ηw is the absorption quantum efficiency for one well, N w is the total number of wells, and η = N w ηw is the total absorption quantum efficiency. The escape probability pe for an excited electron from the well is given by pe ≡
τR τR + τE
(10.92)
where τ E is the escape time and τ R is the intersubband relaxation time. For QWIPs with boundtocontinuum or boundtoquasibound state transition case, once an electron is excited, it is already in the continuum and τ E ≈ 0, pe ≈ 1. For a photocurrent I p injected from the contact, a fraction of the current pc I p is captured by the quantum well, where pc is the capture probability. The remaining current transmitted to the next stage is (1 − pc )I p . From current continuity, the injected current must equal to the sum of the transmitted current and photoemission current. I p = (1 − pc )I p + i p
(10.93)
492
10 Heterostructure Photonic Devices
Therefore, i p = pc I p
(10.94)
Using (10.91), we get
pe I p = q Aη pc N w
≡ q Aηg
(10.95)
and g≡
pe pc N w
(10.96)
is the photoconductive gain. Under the approximation pe ≈ 1 and pc 1 for the boundtocontinuum and boundtobound QWIP designs, the gain becomes g ≈ 1/( pc Nw ).
10.7.4 Detectivity For single IR detectors, the most commonly used figureofmerit is the detectivity, which is a normalized signaltonoise ratio. The peak detectivity D ∗ is given by D ∗ = R p A f /i n
(10.97)
where R p is the peak responsivity √ (A/W), A is the photosensitive area of the detector, i n is the dark current noise (A/ Hz), and f = 1 Hz is the measurement bandwidth. For a photoconductor such as a QWIP with small QW capture probability pc 1, the noise current is given by in =
4q Id g f
(10.98)
The peak responsivity is defined as the ratio of the photocurrent I p to the incident optical power given by Rp =
Ip qηg q = = ηg Ahν hν hν
(10.99)
where h is Planck’s constant and v is the frequency of the incident light. The absorption quantum efficiency of the QWIP can be expressed as η=
pe 1 − exp(−2αl) 2
(10.100)
10.7 QuantumWell Infrared Photodetectors (QWIPs)
493
where α is the absorption coefficient and l = Nw L p is the length of the multiple quantumwell structure. For most QWIP cases, 2αl 1 and η ≈ pe αl. In QWIPs, the responsivity involves two processes: absorption of IR radiation by photoexcitation and transport of the photoexcited carriers to the output of the detector. The high absorption quantum efficiency, however, does not necessary result in high detector responsivity. To achieve a large photocurrent, the photoexcited electrons must escape the quantum wells efficiently with a higher value of g. For QWIPs, the photoconductive gain is given by pe = g= pc N w
τR τR + τE
τ L + τT τT
1 Nw
(10.96)
where the first two fractions correspond to pe and 1/pc , respectively. For the boundtocontinuum and boundtoquasibound cases, the process of escape takes little time, τ E ≈ 0 and pe ∼ 1. For the boundtobound case, the calculated and experimental value of τ R is about 1 ps. To ensure pe ∼ 1, we must have τ E 1 ps. This implies that the excited state in the boundtobound case must be close to the top of the barrier so that the tunneling escape time is much less than 1 ps.
10.7.5 Experimental Results In the following, we compare the measured absorption coefficient spectra, responsivities, and detectivities of several Alx Ga1−x As/GaAs QWIPs with different quantumwell designs reported by Levine et al. The material parameters of these devices are listed in Table 10.1. The IR absorption spectra for samples A–F were measured at room temperature and are shown in Fig. 10.68. The spectra of the boundtocontinuum QWIPs (samples A, B, and C) are much broader than the boundtobound QWIP (samples E) and boundtoquasibound QWIP (samples F). The boundtocontinuum absorption can correspond to a transition from the bound state to numerous minisubbands, Table 10.1 Quantumwell structure parameters for five AlGaAs/GaAs QWIP samples A– F, including quantumwell width L w , barrier width L b , Alx Ga1−x As composition x, doping concentration N d , and type of intersubband transition: boundtocontinuum (BTC), boundtobound (BTB), and boundtoquasicontinuum (BTQC) [33] Sample
L w (Å)
L b (Å)
x AlAs
N d (1018 cm−3 )
A
40
500
0.26
1
BTC
B
40
500
0.25
1.5
BTC
C
60
500
0.15
0.5
BTC
E
50
500
0.26
0.42
BTB
F
50
50/500
0.3/0.26
0.42
BTQB
Intersubband transition
494
10 Heterostructure Photonic Devices
Fig. 10.68 Absorption coefficient spectra α(λ) versus wavelength measured at room temperature for QWIP samples A, B, C, E, and F. Reprint with permission from [33], copyright AIP Publishing
each having a small spectral width. The summation of these absorptions gives rise to a greater spectral width than a single boundtobound transition. Due to the conservation of integrated oscillator strength, the magnitude of the absorption coefficient for the boundtocontinuum QWIPs is significantly lower than that for the boundtobound or boundtoquasibound QWIPs. Among all measured samples, the boundtobound QWIP (sample E) has the narrowest absorption spectral width and highest peak absorption coefficient. In the following, we will focus the discussion on samples A, E, and F due to the proximity of their peak absorption wavelengths. The bias voltagedependent peak responsivity Rp for the bound (E), quasibound (F), and continuum (A) QWIPs measured at T = 20 K is displayed in Fig. 10.69. The low bias responsivity of boundtocontinuum QWIP (A) is approximately linear and that it saturates at high bias. The quasibound QWIP (F) behaves quite similarly to the continuum QWIPs. However, the fully bound QWIP (E) has a significantly lower responsivity despite its high absorption coefficient. The responsivity does not start out linearly with applied bias but is zero for finite bias. There is a zero bias offset Fig. 10.69 Biasdependent peak responsivity measured at T = 20 K for bound (E), quasibound (F), and continuum (A) QWIP samples. Reprint with permission from [33], copyright AIP Publishing
10.7 QuantumWell Infrared Photodetectors (QWIPs)
495
Fig. 10.70 Bias voltagedependent detectivity D* measured at 77 K for continuum (A), bound (E), and quasibound (F) QWIP samples. The dashed lines near the origin are extrapolations. Reprint with permission from [33], copyright AIP Publishing
of nearly 1 V, due to the necessity of fieldassisted tunneling for the photoexcited carrier to escape from the well. Since the bias voltagedependent photoconductive gains are quite similar for all three QWIP designs, the magnitude of responsivities is mainly determined by the absorption quantum efficiency (η ∝ pe α). The measured escape probabilities pe for continuum, quasibound, and bound QWIPs at zero bias are 34%, 28%, and 2.9%, respectively. These lead to the corresponding zerobias absorption quantum efficiencies η of 5.6%, 5.8%, and 0.6% for continuum, quasibound, and bound QWIPs, respectively. It is clear that higher peak spectral responsivity is achieved in QWIPs with the upper state in the continuum or nearly in resonance with the top of the barrier. Finally, the biasdependent detectivities for a continuum (A), a quasibound (F), and a bound (E) QWIP are shown in Fig. 10.70. For all samples D* has a maximum value at a bias between −2 and −3 V. Since these QWIPs all have different cutoff wavelengths, these maximum D* values cannot be simply compared. However, the general behavior of the photodetector can be revealed from the detectivity expressed as a function of detector parameters. For quasibound and continuum QWIPs, τ L τT , and substituting (10.88), (10.98), and (10.99) into (10.97), we get D∗ =
η λ √ 2hc Nw
τL N2D
(10.101)
where λ is the wavelength, η is the absorption quantum efficiency, N w is the number of quantum wells, and N 2D is given by N2D =
m ∗ kT π 2
exp[−(hc/λc kT ) + (E F /kT )]
(10.102)
496
10 Heterostructure Photonic Devices
Fig. 10.71 Nine 1024 × 1024 QWIP detector arrays fabricated on a fourinch semiinsulating GaAs wafer. The process evaluation chips containing large and small area test detectors were placed at the sides of the detector arrays. Reprint with permission from [34], copyright IEEE
where m* is the effective mass in the well, T is the temperature, c is the speed of light, λc is the cutoff wavelength, and hc/λc = (E B − E 1 ). From the above two equations, it is clear that higher η, longer τ L , shorter λc or lower T leads to a higher D*. Among these detector parameters, λc and T are the most sensitive, being in the exponent. In addition, provided η can be made high, say close to 100%, one should use the least number of quantum wells in a QWIP for higher detectivity. The continuous progress in QWIP device optimization, material growth, and device processing has culminated in the realization of large format focal plane arrays (FPAs) for longwavelength (8–12 μm) infrared (LWIR) spectrum applications. The most common and commercially viable QWIP FPAs are based on latticematched GaAs/Alx Ga1−x As material systems grown on 4 and 6inch GaAs semiinsulating substrates. This material system is robust and highly reproducible. Figure 10.71 shows nine megapixel QWIP detector arrays fabricated on a 4inch semiinsulating GaAs wafer made at the NASA Jet Propulsion Laboratory (JPL). The LWIR boundtoquasibound QWIP device structure consists of 50 pairs of 40 Å GaAs quantum wells and 600 Å Al0.27 Ga0.73 As barriers. The device structure was grown using MBE. 1024 × 1024 pixel detector arrays and process evaluation chips (PECs) were fabricated using standard photolithography, dry etching, and metallization processes. The responsivity of the large area test detectors in the PECs peaked at 8.4 μm, and the peak responsivity of 130 mA/W was achieved at bias V B = −1 V. The QWIP detector array was then integrated with the silicon readout integrated circuits. These finished LWIR QWIP FPAs produced excellent images (Fig. 10.72) with 99.98% pixel operability.
10.8 Transistor Lasers
497
Fig. 10.72 One image frame taken with a megapixel LWIR QWIP FPA. Pixel pitch is 19.5 μm and the FPA was cooled to 72 K. Reprint with permission from [34], copyright IEEE
10.8 Transistor Lasers For highspeed operation of over 700 GHz, the downscaling HBT becomes a highcurrentdensity device. As much as 104 A/cm2 goes into the base, which is 10–100 times as dense as that needed for a stateoftheart highspeed laser. For HBTs made of directgap III–V materials—in this case, InP/InGaAs—Milton Feng and Nick Holonyak, Jr. at the University of Illinois speculated that at these normally destructive current densities, light was probably being generated to remove the energy lost in recombination instead of heat generation. Their extensive research efforts led to the invention of the lightemitting transistor (LET), particularly, the transistor laser (TL). This HBTbased integrated optoelectronic device is, simultaneously, both an electrical and an optical signal source driven by the base current. It operates as a threeport device with an electrical input, electrical output, and a third optical output. The unique threeterminal configuration of the TL enables the realization of new electrooptical applications such as nonlinear signal mixing, frequency multiplication, and optoelectronic logic gates.
10.8.1 Basic Device Structure and Operation Principles A transistor laser has a device layer structure essentially similar to a HBT with a few modifications. As shown in Fig. 10.73, a resonant cavity is created using reflective facets at opposite ends of the recombination (active) region to aid the stimulated
498
10 Heterostructure Photonic Devices In0.15Ga0.85As QW
EFN
Lz
Ec hv EFn Ev n  In0.49Ga0.51P
EFp p  GaAs
n  GaAs
Fig. 10.73 Device structure and energy band diagram of an InGaP/GaAs transistor laser embedded with InGaAs QWs inside the base region
recombination and emission of photons. The other major departure from the conventional HBT structure is the insertion of a QW or MQWs inside the base region. Under forward normal operation of a Npn HBT, injected electrons from the emitter diffuse across the base. Because the base–collector junction is reversebiased to block holes, the electrons coming from the emitter through the base sweep right into the collector without noteworthy recombination with holes inside the base. To enhance the recombination of electrons and holes in the base region of the transistor laser, the inserted QW acts like a special recombination center, or an ‘optical collector,’ to trap electrons that flow from emitter to collector. This enhanced recombination process produces a much stronger optical signal emerging from the base region and a complementary electrical signal emerging from the collector. The light intensity of the spontaneous emission from the base increases with increasing base current, which supplies the required amount of holes. Once the supplied base current reaches the lasing threshold, the intense directed stimulated emission of a coherent laser beam is emerging from the ends of the laser cavity. In twoport devices such as the twoterminal diode laser, the light output power solely depends on the injection current. The threeterminal HBT is also a twoport device where output collector current (I C ) is a function of both injected base current (I B ) and the collectortobase voltage (V CB = V CE − V BE , V BE is constant at given I B ). On the other hand, the threeport transistor laser, in commonemitter operation shown in Fig. 10.74, has an input port 1 (I B ), an output port 2 (I C –V CE characteristics), and uniquely in the base a QW ‘optical collector’ output port 3 (L–V CE characteristics, L = coherent light output intensity). It has a unique set of current output (I C –V CE ) family of curves and a distinct set of coherent light output (L–V CE ) family of curves. As an example, the (I C –V CE ) and (L–V CE ) family curves of a nInGaP/p+ GaAs/n+ GaAs transistor laser incorporated a single undoped 15 nm InGaAs baseregion QW at wavelength λ ≈ 980 nm are shown in Fig. 10.75. The electrical output of the transistor laser is examined first. For I B < 56 mA the transistor laser exhibits the usual transistor (HBT) behavior with the differential current gain β = I C / I B increasing with I B . At base current I B = 56 mA the gain decreases abruptly, corresponding to stimulated recombination and ‘faster’ base recombination, as will be discussed in the
10.8 Transistor Lasers
499
Fig. 10.74 Biasing diagram of a commonemitter operation of a transistor laser
Fig. 10.75 a Collector I–V CE characteristics of a transistor laser. Below the knee voltages, the transistor is biased in saturation. b The coherent light output L–V CE characteristics of the transistor laser. Reprinted with permission from [35], copyright AIP Publishing
next section. Thus, it determines the threshold current (I th ) of the laser action. This abrupt compression of the I–V characteristics and reduction in β is unique to the transistor laser. This feature also eliminates the need to have an additional external feedback system, such as a photodetector, to verify that the device is operating as a laser. The coherent optical output characteristics (L–V CE ) of the transistor laser for I B ≥ I th are shown in Fig. 10.75b. For small V CB where the BC junction has not reached strong reverse bias, the laser output increases with emitter electron injection into the base. The stimulated recombination then saturates shown as a constant output
500
10 Heterostructure Photonic Devices
Fig. 10.76 Threeport laser operation of a transistor laser at room temperature in the commonemitter configuration. Curve (a) is a 3 GHz electric input voltage waveform, b a 3 GHz electrical output voltage signal, and c a 3 GHz photodetector output voltage waveform corresponding to the modulated laser output. Reprinted with permission from [36], copyright AIP Publishing
power limited by the hole supply at base current I B . Once the BC junction reaches sufficient reverse bias, direct tunneling of electrons across the BC junction reduces the hole supply in the base region leading to a gradual drop in laser output power. In a directly modulated threeport transistor laser, a coherent stimulated optical signal emerges from the base and, simultaneously, a complementary electrical signal emerges from the collector. As an example, a 3GHz small signal sinusoidal voltage with peaktopeak amplitude of 0.6 V is supplied at the base (input port) of the device. The input voltage V BE , the electrical output voltage V CE , and the laser output signal measured using a power meter are all displayed simultaneously on separate channels of a digital sampling oscilloscope and shown in Fig. 10.76. These data demonstrate that direct electrical and optical modulation of a transistor laser at highspeed is possible. However, the ultimate bandwidth of the transistor laser is limited by the modulation speed of the optical output signal, since the stateoftheart switching speed of HBT has already reached 800 GHz.
10.8.2 Effective Minority Carrier Lifetime in Transistor Lasers For semiconductor lasers, the modulation bandwidth is determined by how fast the injected carriers in the active region can be depleted when the device is turned off. In a doubleheterostructure pin diode laser, injected carriers are trapped in the active region, bounded by upper and lower cladding layers, and the depletion process is accomplished only through recombination processes (Fig. 10.77a). In laser diode structures, the minority carrier density and lifetime are about ≥1018 cm−3 and ~1 ns, respectively. The long minority carrier lifetime puts an upper limit on the maximum modulation speed of the diode laser at ~ 20 GHz.
10.8 Transistor Lasers
501
Fig. 10.77 Schematic energy band diagram and charge population distribution in a a pin doubleheterostructure laser, and b an npn transistor laser. Reprinted with permission from [37], copyright AIP Publishing
In Npn transistor lasers, the active region is a heavily doped thin ptype base bounded by ntype emitter and collector. The base region can be described as a series of three layers: (a) ptype base doped N A (cm−3 ), (b) undoped QW, and (c) ptype base doped N A (cm−3 ). Under normal mode operation, the EB junction is forwardbiased and the BC junction is reversebiased creating a tilted injected minority charge distribution with zero charge density at the BC junction as shown in Fig. 10.77b. Furthermore, the base charge density profile of the transistor laser deviates from the simple HBT ‘triangular’ approximation. The straightline profile is slightly tilted more steeply upward at the emitter end of the base than near the collector with a ‘kink’ at the QW position. This is due to the enhanced recombination of the QW compared to the bulk region and the reduced base distance from emitter to the QW. It is evident from the I–V characteristics (e.g., Fig. 10.75a) where, at the lasing threshold, the QW recombination lifetime decreases abruptly (current gain β stim < β spon ) as stimulated recombination speeds up the overall rate of recombination in the QW. As it becomes clear later that the recombination rate in bulk base regions is very small compared to that in the QW, the base charge distribution can be seen as a superposition of two triangular charge populations denoted by Q1 and Q2 , as shown in Fig. 10.78. Q1 is responsible for the diffusion of carriers to the QW for radiative recombination, while Q2 is responsible for the diffusion of carriers from the emitter to the collector. The QW acts like an optical collector in addition to the regular electrical collector of the device. The populations Q1 and Q2 have the values of Q 1 = q n 1 AWEQW /2 and Q 2 = q n 2 AWEC /2, respectively, with total base charge Q = Q1 + Q2 . In these expressions, A, n, W EC , and W EQW are the base crosssectional area, excess minority carrier density at EB junction, base width, and emitter to QW distance, respectively. From the charge control model, it is obvious 2 /2D that IC = Q 2 /τt,2 and IB = (Q 1 + Q 2 )/τbulk + Q 1 /τt,1 , where τt,1 = WEQW 2 is the transit time from emitter to QW, τt,2 = WEC /2D is the transit time across the whole base, and D is the diffusion constant. We note that for a GaAs base of 90 nm, τ t,2 ≈ 1.56 ps using a diffusion constant of 26 cm2 /s. Since W EQW < W EC, τ t,1 has a value also in the picosecond range. The bulk lifetime τ bulk in GaAs layers can be obtained from the current gain of a comparison HBT without a base QW, which has
502
10 Heterostructure Photonic Devices
Base Carrier Density
E
B
C
Q1+Q2 Q2
IE
QW
LZ
IB
Q1
IC
W EQW W EC Fig. 10.78 Charge analysis of the base minority carrier density of a transistor laser showing the continuity condition applied to the minority carrier population at the base QW active region. Q1 and Q2 triangles correspond to carrier diffusion and collection at the QW and the electrical collector, respectively. Reprinted with permission from [38], copyright AIP Publishing
a value of ~135 ps. The overall effective base recombination lifetime τ B of the entire base population, not including parasitic charging delays, can be expressed as 1 1 = + τB τbulk
1 Q1 Q 1 + Q 2 τt,1
(10.103)
Since τbulk τt,1 , the effective base recombination lifetime reduces to τB ≈ (1 + Q 2 /Q 1 )τt,1 . When the transistor laser is operated below threshold in spontaneous mode, Q 2 Q 1 and (10.103) reduces to τB = τB,spon ≈ (Q 2 /Q 1 )τt,1 . When the transistor laser is operated near and just beyond the threshold, Q1 increases rapidly approaching the same order of magnitude of Q2 . Therefore, τ B is larger but of the same order of magnitude as τ t,1 which is in the picosecond range. Beyond the lasing threshold τ B decreases as stimulated emission speeds up the overall recombination rate in the base region. A larger proportion of the base carriers are transported to the now faster optical collector (QW) for stimulated emission leading to decreased gain β stim . In a semiconductor laser stimulated emission, the output intensity responds to either a current step or a small modulation signal that involves the interaction between the photon population in the cavity and the fraction of injected carriers that are in excess of the threshold density. Hence the lifetimes associated with both injected carriers and the photons are involved in the process. For diode lasers, the typical carrier lifetime and photon lifetime are on the order of 1 ns and 5 ps, respectively. The strong interaction between the populations of injected carriers and photons with very different lifetimes leads to pulsations during switchon and a natural resonance during the sinusoidal modulation of the laser. These undesirable features result in bit error rate degradation and limit the useful bandwidth of the device for optical data communication links. For transistor lasers, the spontaneous recombination lifetime
10.8 Transistor Lasers
503
Fig. 10.79 Measured and fitted optical response of a transistor laser showing absence of carrier–photon resonance owing to fast spontaneous recombination lifetime, τ B,spon . Reprinted with permission from [37], copyright AIP Publishing
τ B,spon is reduced by more than two orders of magnitude from the value of diode laser and on the same order of magnitude as the photon lifetime. The fast spontaneous recombination lifetime leads to a resonancefree frequency response at low biases and relatively small resonance appears only at large I B /I th as shown in Fig. 10.79. It should be noted that the fitted data of τ B,spon ~ 29 ps quoted in the figure is an effective lifetime which subsumes all the parasitic charging delays. This number can be further reduced through the refinement of device designs to efficient utilization of the full device bandwidth up to –3 dB point with lower power consumption.
10.8.3 Voltage Modulation of a Transistor Laser In transistor lasers, the collector characteristics can be used to directly extract the transport and recombination dynamics in the QW base due to its close proximity to the active base region. For example, the threshold current I B,th of coherent light generation can be identified from the current gain compression in current output (I C –V CE ) family of curves. In Fig. 10.75b, it is also observed that the laser output drops at high reverse bias of V CE due to increased carrier loss via tunneling. Thus, it is possible to use a collector junction design with efficient generation of tunneling current such that the laser operation can be more meritoriously controlled by collector bias voltage modulation in addition to current modulation. The major tunneling mechanisms at the reversebiased BC junction of a transistor laser are the intracavity photonassisted (ICP) tunneling process and the direct bandtoband tunneling process. While Franz– Keldysh effect is ordinarily referred as the electric field dependence of the fundamental absorption edge of a semiconductor (Sect. 7.5), the ICP tunneling process further includes the effect of electrical and optical cavity coupling. The ICP tunneling can be adjusted to lower voltage by narrowing the collector junction transition region with higher doping at the expense of shifting to more direct bandtoband tunneling. Thus, a collector incorporated with a tunnel junction provides an enhanced means for voltagecontrolled modulation of the optical output of the transistor laser.
504
10 Heterostructure Photonic Devices
Fig. 10.80 Schematic band diagram of a TJTL shown with a generic resonator cavity. The inset shows the photonassisted tunneling process at the tunnel junction. Reprinted with permission from [39], copyright AIP Publishing
Figure 10.80 shows the energy band diagram of a tunnel junction transistor laser (TJTL) where a highly doped p+ (baseside) and n+ (collectorside) TJ is incorporated around the BC junction. Under normal operation where the BC junction is reversebiased, the collector current I C consists of the usual transport component across the base I t , the direct TJ current IrT , and the ICP tunneling current I paT , or IC = It + IrT + IpaT
(10.104)
Comparing to a regular transistor laser with relative flat I C V CE characteristics (Fig. 10.75a), the effects of collector tunneling of a TJTL are evident from the upward slope of the collector current I C versus V CE (Fig. 10.81a) due to various tunneling components. Under the condition of stimulated emission, the tunneling process occurs predominantly via ICP absorption, where IC ≈ It + IpaT . The coherent photons generated at the QW interact with the collector junction field (V CB ) by way of ICP absorption and assist electron tunneling from base to collector, resulting in hole resupply current (IpaT ) into the base region and a reduction in the coherent optical field. Direct tunneling can be observed at higher V CE biases of I C –V CE characteristics according to (10.104). The optical output LV CE characteristics of a TJTL are shown in Fig. 10.81b. In laser operation of the TJTL under weak collector junction field (left region 1 of Fig. 10.81b), the laser output increases with emitter electron injection to the base. ICP tunneling (IpaT > 0) further enables the supply of holes to the QW and improves the laser optical output. The photon absorption resulting from the weak collector junction field is insufficient to overcome the optical gain established by emitter and base carrier injection. The stimulated recombination is then saturated limited by the hole supply to the base current I B . However, under strong reversebiased collector junction field
10.8 Transistor Lasers
505
Fig. 10.81 a Collector I–V CE characteristics and b optical output L–V CE characteristics of a TJTL as shown schematically in Fig. 10.80. Reprinted with permission from [40], copyright AIP Publishing
(right region 2 of Fig. 10.81b), optical output is reduced and subsequently quenched by the fielddependent ICP absorption. Figure 10.82 illustrates the ICP tunneling process at the BC junction that is singled out from the total collector current for clarity. The electron–hole pairs are generated at the collector junction under photonassisted tunneling inside the optical cavity. Electrons drifting to the collector contribute to the excess collector current IpaT . Holes drifting to the base contribute as majority carrier injection and diffuse to the base QW for stimulated recombination (Ir 2 ). Under steadystate condition IpaT = Ir 2 , Fig. 10.82 Tunneling excess carrier distribution in the base of a transistor laser under the influence of intracavity photonassisted tunneling (circled region). Minority electron injection from the emitter and excess majority hole supply from the base are omitted for clarity. Reprinted with permission from [41], copyright AIP Publishing
506
10 Heterostructure Photonic Devices
the excess hole distribution ( p2 ) is established. The excess hole charge (+q p2 ) lowers the emitter junction energy barrier and induces minority carrier injection to establish the excess electron distribution ( n2 ) at the collector junction satisfying charge neutrality. The time constant that characterizes this transport process is quite small, on the order of femtoseconds, and is referred to as the dielectric relaxation time, τ = r 0 ρ where ρ is the resistivity. The excess electrons that do not recombine will drift to the collector and contribute as additional collector current It2 . These carrier transport and redistribution processes inside the transistor laser establish a tunneling current gain, β 2 , and can be expressed as β2 =
It2 q n 2 υdrift WC /τdrift 2WC τstim τstim = = = ≈ Ir 2 WCQW q p2 /2τstim WCQW /2τstim WCQW τdrift τdrift (10.105)
W CQW is the distance between the QW and the BC junction, and W C is the collector junction thickness. τstim and τdrift are the QW stimulated recombination lifetime and the carrier drift time, respectively. The tunneling current gain β 2 is approximately the ratio of τstim to τdrift . As shown in Fig. 10.81a, the ICP tunneling current IpaT increases with the collector voltage V CE due to the increased absorption of cavity photons. The cavity photon density reduction leads to the QW stimulated recombination lifetime increase and, thus, an increasing tunneling current gain β 2 at high bias V CE . As shown in Fig. 10.82, the tunneling collector current I C2 due to the stimulated recombination can be expressed as IC2 = It2 + IpaT = It2 + Ir 2 = (β2 + 1)Ir 2 = (β2 + 1)IpaT
(10.106)
Once the currents IC2 and IpaT are determined from the measured collector I– V and optical L–V curves, the tunneling current gain β2 = IC2 /IpaT − 1 can be derived experimentally. In a typical AlGaAs/InGaAs QW/GaAs transistor laser, the tunneling current gain as a function of V CB is experimentally determined and shown in Fig. 10.83. As expected, for a given base current, β 2 increases with collector V CB . Thus, the photonfield enhanced optical absorption augments ICP tunneling at high collector voltages in a transistor laser and leads to a unique property of voltage modulation and switching of a transistor laser.
10.8.4 Excited State Operation of a Transistor Laser In the diode laser, the charge densities in the undoped QW are largely pinned at and beyond lasing threshold, and the lasing transition is in the ground states. This is not the case for transistor lasers. Since the base region of the Npn transistor laser is heavily doped with acceptors except the QW, the occupation of the QW states is primarily by minority carrier electrons. It is governed by the boundary conditions imposed by the charge transport from the emitter to the collector, i.e., a tilted emittertocollector base population distribution. Therefore the charge population in the QW base does not
10.8 Transistor Lasers
507
Fig. 10.83 Tunneling current gain β 2 of an AlGaAs/InGaAs QW/GaAs TJTL at different base currents and collector bias voltages. Reprinted with permission from [41], copyright AIP Publishing
saturate but continuously increases beyond lasing threshold, causing the lasing action to evolve from the groundstate transition at low I B to the excited state transition at high base current. Figure 10.84 shows the I–V characteristics of a transistor laser where the I–V curves are distorted in the region of stimulated recombination (I B > I B,th ) when compared to the region of spontaneous recombination. In the region of high bias voltage (V CE > 2.7 V) the stimulated recombination is quenched into spontaneous recombination even at I B > I B,th . The corresponding lasing spectra at the base current bias points of V CE = 1.5 V at I B = 30, 50, 70, and 90 mA are also shown in Fig. 10.84. At 30 mA the spontaneous spectral peak developed into laser modes with the major lasing peak at λ ≈ 1002 nm. The intensity of ground state stimulated radiation at ~1000 nm increases proportionately as I B is increased further to 50 mA. At I B = 70 mA lasing occurs on both the broad ground state and on the
Fig. 10.84 Transistor laser collector I–V characteristics (left) and laser spectra (right) at V CE = 1.5 corresponding to bias points: a I B = 30 mA, b I B = 50, c I B = 70, and d I B = 90. Reprinted with permission from [42], copyright AIP Publishing
508
10 Heterostructure Photonic Devices
next higher state of the QW (λ ≈ 978 nm). At I B = 90 mA the laser operation is observed exclusively on the higher state (λ ≈ 978 nm). The 3dB bandwidth of the transistor laser operating on the ground state increases with increasing base current and begins to saturate (at 7 GHz) around 50 mA because of the groundstate bandfilling and gain saturation. Continuous increase of the charge population it shifts the operation from the ground state to the first excited state at 70 mA. The 3dB bandwidth of the transistor laser operates on the first excited state continue to rise with increasing I B . Further increase in the base current causes the first excited state to saturate (at 13.5 GHz) due to gain saturation and heating. The limited bandwidth measured arises mainly from large input base capacitance and base resistance of the current device. With proper device geometry and improvement in contact resistance, it should be possible to achieve transistor laser operation near the intrinsic bandwidth of greater than 40 GHz.
10.8.5 LightEmitting Diodes with Tilted BaseCharge Distribution Similar to diode lasers, the modulation speed of doubleheterostructure lightemitting diodes (LEDs) is limited by the carrier recombination lifetime of the device. As shown in Fig. 10.77a, the buildup of confined excess carriers in the active region can only be depleted through the slow radiative recombination process which limits the maximum modulation speed of the LED to about 1 GHz. On the other hand, a tilted base charge population in the transistor laser design offers a unique solution to select and keep fast recombination carriers in the base by collecting slow recombination carriers at the reversebiased collector junction. Thus, the action of the collector in a transistor laser may be incorporated into the design of a carrier drain in LEDs to enable highspeed operation. Figure 10.85a shows the cross section of a tiltedcharge LED. The device layer structure is similar to an Npn transistor laser with some modifications to achieve twoterminal operation. Emitter current I E is injected from the top into the emitter and transported to the QW base active region. The injected minority carriers that recombine in the base form the base current I B . To empty carriers that are too slow to recombine within the transit time (τ t ) across the base layer, a reverse bias field at the lower base boundary is needed. In the tiltedcharge LED design the collector of the transistor laser is replaced by an undoped drain layer which forms a pn junction with the base. A reverse builtin field is maintained at the base–drain junction by the zero potential difference obtained via a common contact metallization extending from the drain to the base. The zero base–drain potential difference ensures that there is no base charge population at the base–drain boundary, hence establishing a tilted emittertodrain population distribution in the base. The excess minority carriers removed from the base by the builtin field forms the drain current I D . The tiltedcharge LED can be biased as a usual twoterminal device and displays an IV characteristic resembling
10.8 Transistor Lasers
509
Fig. 10.85 a Cross section of an Npn tiltedcharge LED with a ptype base QW active region. b The optical output frequency response of the tiltedcharge LED at bias currents I E = 40, 50, and 60 mA showing the −3 dB frequency of 3.2, 5, and 7 GHz, respectively. Reprinted with permission from [43], copyright AIP Publishing
that of a pn junction diode. The turnon voltage is determined by the emitter–base potential difference since the base and drain have a common potential. The optical output frequency responses of the tiltedcharge LED biased at different I E are shown in Fig. 10.85b. The tiltedcharge LED operates similar to a pn junction LED with reasonable efficiency but has a considerably higher modulation speed. The maximum 3dB bandwidth of the device achieved is 7 GHz at I E = 60 mA. Problems 1.
A GaAs/Al0.3 Ga0.7 As symmetric doubleheterostructure laser with a cavity ¯ length of 250 μm has the following device parameters: α i = 10 cm−1 , n(GaAs) = 3.6 at the lasing wavelength, and an active layer thickness of 0.15 μm. Find the gain coefficient. Note, the mirror power reflectivity can be calculated from n¯ 0 − n¯ 1 2 R = n¯ 0 + n¯ 1
2.
where n¯ 0 (air) = 1 and n¯ 1 = n(GaAs). ¯ From an article [App. Phys. Lett. 61, 255 (1992)] on strained 0.98 μm InGaAs single QW lasers using different cladding layers (GaAs and GaInAsP), extract the following parameters for two types of lasers. Assume the mirror reflectivity is 32%. (a) α i (b) ηi c. Transparency current density.
3.
The peak gain of a 1.55 μm InGaAsP laser diode can be approximated by g p = a(n − n tr ) = 3 × 10−16 n − 2 × 1018
510
10 Heterostructure Photonic Devices
Assume the cavity length is 250 μm, the refractive index of the active layer is 3.4, the internal loss is 25 cm−1 , the carrier lifetime is 1.5 ns, the internal quantum efficiency is 80%, the active layer thickness is 0.1 μm, and the optical confinement factor is 0.4. (a) Calculate the threshold current density of the laser. (b) What is the threshold current of the laser if the active region is 2.5 μm wide? (c) What is the differential quantum efficiency ηd of the laser? (d) The external quantum efficiency ηe or slope efficiency relates to ηd by ηe =
ω P = ηd (W/A). I q
Find ηe of the laser. 4. For a GaAs/AlGaAs laser with a lasing wavelength of 780 nm, calculate the mode number and mode spacing of the laser for a cavity length of 250 μm and n¯ (active layer) = 3.54. 5. Calculate the photon lifetime of a laser with the following parameters: cavity length = 250 μm, internal loss = 10 cm−1 , and the refractive index of cleaved mirrors is 3.4. 6. Calculate the output power of a GaAs/AlGaAs laser operated at an injection current level of 30 mA with a lasing wavelength of 870 nm and the following device parameters: cavity length = 250 μm, internal loss = 20 cm−1 , the refractive index of cleaved mirrors is 3.65, the internal quantum efficiency is 0.8, and the threshold current is 18 mA. 7. The figure below is the measured optical spectrum of a GaAs laser just below the threshold. For both mirrors, n(active ¯ region) = 3.58, calculate and plot the peak gain between 7960 and 8030 Å under this current injection level.
10.8 Transistor Lasers
8.
511
This problem concerns DBR mirror designs. (a) Plot the mirror reflectance R for InP/InGaAsP latticematched 1.55 μm DBR mirror as a function of the number of mirror pairs. Assuming n(InP) ¯ = 3.17, n(InGaAsP) ¯ = 3.40, and the adjacent layer to the DBR is air. (b) How many pairs of InP/InGaAsP DBR mirrors are required to reach R = 99%? (c) How many mirror pairs are required for AlAs/GaAs mirror stacks to reach the same reflectance of 99%? (d) At R = 99%, calculate the stopband width for both material systems.
9.
In an InGaAs/GaAs/Al0.2 Ga0.8 As 980 nm VCSEL, the active region consists of 3 InGaAs quantum wells, each 8 nm thick, separated by two 8nmthick GaAs barriers, and clad on each side by another 8nmthick layer of GaAs. The rest of the cavity (active region) consists of an Al0.2 Ga0.8 As spacer layer. The DBR mirrors are composed of quarter wavelength stacks of AlAs/GaAs. The DBR mirrors begin with an AlAs quarterwave layer next to the cavity. The cavity between the DBR mirrors has to be one optical wavelength to maximize the gain. (a) For n(GaAs) ¯ = 3.52, n(AlAs) ¯ = 2.95, n(InGaAs) ¯ = 3.60, and n(Al ¯ 0.2 Ga0.8 As) = 3.39, determine the thickness of the two AlGaAs spacer layers. (b) Assuming the averaged refractive index of the cavity is 3.56, determine the number of the AlAs/GaAs period in the top and bottom DBR mirrors if the required power reflections are 99.5% and 98.5%, respectively. Consider contributions by AlAs/GaAs DBR pairs only. (c) Determine the threshold current density of a VCSEL with the following device parameters: a = 4 × 1016 cm2 , Br = 10−10 cm3 /s, α a = 25 cm−1 , α c = 10 cm−1 , ntr = 1.5 × 1018 cm3 , and ≈ (cavity length, d)/(total device length, L).
10. Mini project: As the transistor has evolved from point contact, to pn junction, to III–V semiconductor heterojunction bipolar (HBT), to particularly highcurrent density highspeed HBT, we arrive at the possibility that the HBT can be modified and operated as a threeport lightemitting device (an electrical input, and electrical and optical outputs). The threeport lightemitting transistor (LET) can be substantially modified and improved by incorporating a quantum well, or multiple quantum wells, into the ptype base region of a Np+ n HBT in order to tailor the base recombination and thus the transistor electrical and optical properties. The lightemitting HBT can be further designed to support stimulated recombination and to be operated as a laser—a transistor laser. Design a transistor laser with an emission wavelength near 1.3 μm, which is important for shorthaul light wave communications. The HBT used in your design can be either an Np+ n or Pn+ p structure. Following are two related publications on longwavelength transistor lasers:
512
10 Heterostructure Photonic Devices
• F. Dixon, et al., ‘Transistor laser with emission wavelength at 1544 nm,’ Appl. Phys. Lett. 93, 021111 (2008) • Y. Huang, et al., ‘InAlGaAs/InP lightemitting transistors operating near 1.55 μm,’ J. Appl. Phys. 103, 114505 (2008). Your work should meet the following requirements: – Select a material system among all available III–V materials for the 1.3 μm emission wavelength. Both strained and latticematched systems can be used. Explain why you select it. – The selected material system should be able to form transistor laser structures with high crystal quality. However, heterostructures prepared on metamorphic substrate structures are not allowed. – The material selected for the base region should accommodate doping to mid1019 cm−3 for low base sheet resistance and highspeed operation. Specify the dopant used in the base region. – Design the layer structure of a transistor laser based on the material system selected. Provide detailed layer structures along with a full energy band diagram. For heterostructures, the energy band discontinuities should be calculated.
References 1. K.N. Dutta, J. Appl. Phys. 51, 6095 (1980) 2. Y. Itaya, Y. Suematsu, S. Katayama, K. Koshino, S. Arai, Jpn. J. Appl. Phys. 18, 1795 (1979) 3. H. Yonezu, I. Sakuma, K. Kobayashi, T. Kamejima, M. Ueno, Y. Nannichi, Jpn. J. Appl. Phys. 12, 1585 (1973) 4. B. Schwartz, W.W. Focht, N.K. Dutta, R.J. Nelson, P. Besomi, IEEE Trans, Electron. Dev. 31, 841 (1984) 5. R.J. Nelson, R.B. Wilson, P.D. Wright, P.A. Barnes, N.K. Dutta, IEEE J. Quantum Electron. 17, 202 (1981) 6. M. Nakamura, K. Aiki, J. Umeda, A. Katzir, A. Yariv, H.W. Yen, IEEE J. Quantum Electron. 11, 436 (1975) 7. Z. Alferov, IEEE J. Sel. Topics Quantum Electron. 6, 832 (2000) 8. S.W. Corzine, R.H. Yang, L.A. Coldren, Appl. Phys. Lett. 57, 2835 (1990) 9. R. Dingle, C.H. Henry, Quantum effects in heterostructure lasers, U.S. Patent 3982207, Sept. 21, 1976 10. Y. Arakawa, H. Sakaki, Appl. Phys. Lett. 40, 939 (1982) 11. M. Asada, Y. Miyamoto, Y. Suematsu, IEEE J. Quantum Electron. 22, 1915 (1986) 12. A.Y. Liu, S. Srinivasan, J. Norman, A.C. Gossard, J.E. Bowers, Photonics Res. 3, B1 (2015) 13. K.Y. Cheng, K.C. Hsieh, J.N. Baillargeon, Appl. Phys. Lett. 60, 2892 (1992) 14. A.M. Moy, A.C. Chen, K.Y. Cheng, L.J. Chou, K.C. Hsieh, J. Cryst. Growth 175/176, 819 (1997) 15. D. Wohlert, K.Y. Cheng, S.T. Chou, Appl. Phys. Lett. 78, 1047 (2001) 16. M. Asada, Y. Miyamoto, Y. Suematsu, Jpn. J. Appl. Phys. 24, L95 (1985) 17. E. Towe, R.F. Leheny, A. Yang, IEEE J. Sel. Topics Quantum Electron. 6, 1458 (2000)
References
513
18. H.C. Lin, Design and Fabrication of LongWavelength VerticalCavity SurfaceEmitting Lasers using Wafer Bonding Technologies, Ph.D. Thesis, ECE Dept., University of Illinois at UrbanaChampaign, 2002 19. M.R. Krames et al., Appl. Phys. Lett. 75, 2365 (1999) 20. M.G. Craford, Proc. IEEE 101, 2170 (2013) 21. R. Kazarinov, R. Suris, Sov. Phys. Semicond. 5, 707 (1971) 22. J. Faist, F. Capasso, D.L. Sivco, C. Sirtori, A.L. Hutchinson, A.Y. Cho, Science 264, 553 (1994) 23. J. Faist, F. Capasso, D.L. Sivco, J.N. Baillargeon, A.L. Hutchinson, S.N.G. Chu, A.Y. Cho, Appl. Phys. Lett. 68, 3680 (1996) 24. A. Tridicucci, C. Gmachl, F. Capasso, D.L. Sivco, A.L. Hutchinson, A.Y. Cho, Appl. Phys. Lett. 74, 638 (1999) 25. J. Faist, M. Beck, T. Aellen, E. Gini, Appl. Phys. Lett. 78, 147 (2001) 26. C. Sirtori, J. Faist, F. Capasso, D.L. Sivco, A.L. Hutchinson, A.Y. Cho, Appl. Phys. Lett. 66, 3242 (1995) 27. C. Sirtori, C. Gmachl, F. Capasso, J. Faist, D.L. Sivco, A.L. Hutchinson, A.Y. Cho, Opt. Lett. 23, 1366 (1998) 28. K. Unterrainer, R. Colombelli, C. Gmachl, F. Capasso, H.Y. Hwang, A.M. Sergent, D.L. Sivco, A.Y. Cho, Appl. Phys. Lett. 80, 3060 (2002) 29. C. Gmachl, F. Capasso, A. Tredicucci, D.L. Sivco, R. Kohler, A.L. Hutchinson, A.Y. Cho, J. Sel. Topic Quantum Electron. 5, 808 (1999) 30. I. Vurgaftman, W.W. Bewley, C.L. Canedy, C.S. Kim, M. Kim, J.R. Lindle, C.D. Merritt, J. Abell, J.R. Meyer, IEEE J. Sel. Topics Quantum Electron. 17, 1435 (2011) 31. L.C. West, S.J. Eglash, Appl. Phys. Lett. 46, 1156 (1985) 32. B.F. Levine, K.K. Choi, C.G. Bethea, J. Walker, R.J. Malik, Appl. Phys. Lett. 50, 1092 (1987) 33. B.F. Levine, A. Zussman, S.D. Gunapala, M.T. Asom, J.M. Kuo, W.S. Hobson, J. Appl. Phys. 72, 4429 (1992) 34. S.D. Gunapala, S.V. Bandara, J.K. Liu, J.M. Mumolo, S.B. Rafol, D.Z. Ting, A. Soibel, C. Hill, IEEE J. Sel. Topics Quantum Electron. 20, 3802312 (2014) 35. M. Feng, N. Holonyak Jr., H.W. Then, C.H. Wu, G. Walter, Appl. Phys. Lett. 94, 041118 (2009) 36. M. Feng, N. Holonyak Jr., G. Walter, R. Chan, J. Appl. Phys. 87, 131103 (2005) 37. M. Feng, H.W. Then, N. Holonyak Jr., G. Walter, A. James, Appl. Phys. Lett. 95, 033509 (2009) 38. H.W. Then, M. Feng, N. Holonyak Jr., Appl. Phys. Lett. 94, 013509 (2009) 39. M. Feng, J. Qiu, C.Y. Wang, N. Holonyak Jr., Appl. Phys. Lett. 119, 084502 (2016) 40. H.W. Then, C.H. Wu, G. Walter, M. Feng, N. Holonyak Jr., Appl. Phys. Lett. 94, 101114 (2009) 41. M. Feng, J. Qiu, C.Y. Wang, N. Holonyak Jr., J. Appl. Phys. 120, 204501 (2016) 42. H.W. Then, M. Feng, N. Holonyak Jr., Appl. Phys. Lett. 91, 183505 (2007) 43. G. Walter, C.H. Wu, H.W. Then, M. Feng, N. Holonyak Jr., Appl. Phys. Lett. 94, 231125 (2009)
Further Reading 1. H.C. Casey, M.B. Panish, Heterostructure Lasers (Academic, New York, 1978) 2. C. Weisbuch, B. Vinter, Quantum Semiconductor Structures (Academic, New York, 1991) 3. M. Fukuda, Reliability and Degradation of Semiconductor Lasers and LEDs (Artech House, Boston, 1991) 4. G.P. Agrawal, N.K. Dutta, Semiconductor Lasers, 2nd edn. (Van Nostrand Reinhold, New York, 1993) 5. T.E. Sale, Vertical Cavity Surface Emitting Lasers (Research Studies Press, Taunton, 1995) 6. E.F. Schubert, LightEmitting Diodes, 2nd edn. (Cambridge University Press, Cambridge, 2006) 7. J. Faist, F. Capasso, C. Sirtori, D.L. Sivco, A.Y. Cho, Quantum cascade lasers, in Semiconductors and Semimetals, 66, chap. 1 (2000), 1 8. F. Capasso, Opt. Eng. 49, 111102 (2010)
514
10 Heterostructure Photonic Devices
9. J. Faist, Quantum Cascade Lasers (Oxford University Press, Oxford, United Kingdom, 2013) 10. I. Vurgaftman, R. Weih, M. Kamp, J.R. Meyer, C.L. Canedy, C.S. Kim, M. Kim, W.W. Bewley, C.D. Merritt, J. Abell, S. Höfling, J. Phys. D Appl. Phys. 48, 123001 (2015) 11. B.F. Levine, J. Appl. Phys. 74, R1 (1993) 12. H.C. Liu, Quantum well infrared photodetector physics and novel devices, in Semiconductors and Semimetals, 62, chap. 3 (2000), 129 13. N. Holonyak, Jr., M. Feng, IEEE Spectrum, February (2006), pp. 50–55 14. H.W. Then, M. Feng, N. Holonyak Jr., Proc. IEEE 101, 2271 (2013)
Appendix A
Values of Important Physical Constants
Quantity
Symbol
Value
Unit (MKS) 10−11
Bohr radius
aB
5.2917 ×
Velocity of light
c
2.9979 × 108
m/s
Electron volt
eV
1.6022 × 10−19
J
Permittivity of free space
0
8.8542 ×
10−12
Planck’s constant
h
6.6262 × 10−34
Js
1.0546 × 10−34
Js
Boltzmann’s constant
k
1.3807 ×
10−23
Thermal voltage at T = 300 K
kT/q
2.585 × 10−2
V
Electron rest mass
m0
9.1095 × 10−31
kg
Permeability of free space
μ0
4π ×
10−7
Avogadro’s number
N
6.0220 × 1023
1/mole
Electronic charge
q
1.6022 × 10−19
C
Wavelength of 1 eV quantum
λ
1.2398×10−6
m
Wavenumber of 1 eV quantum
k
8065.6
1/cm
Frequency of 1 eV quantum
f
241.8
THz
m
F/m
J/K
H/m
© Springer Nature Switzerland AG 2020 K. Y. Cheng, III–V Compound Semiconductors and Devices, Graduate Texts in Physics, https://doi.org/10.1007/9783030519032
515
Appendix B
Important Physical Properties of Some Indirect Semiconductorsa
Density
(g/cm3 )
Si
Ge
AlP
AlAs
AlSb
GaP
2.329
5.323
2.40
3.76
4.26
4.138
Lattice constant (Å)
5.43102 5.6579 5.4672b 5.660b
6.1355b 5.4505b
Melting temperature (°C)
1412
937
2550
1740
1065
1457
Indirect bandgap energy @ 300 K (eV)
1.1242
0.664
2.488
2.164
1.616
2.273
3.553
3.003
2.30
2.991
Direct bandgap energy @ 300 K (eV) Intrinsic carrier concentration (cm−3 )
1.02 × 1010
2.33 × 1013
Dielectric constant
11.9
16.2
2 9.8
10.06
12.04
11.11
Refractive index @ E g
3.6
4.0
2.95
3.18
3.445
3.42
Optical phonon energy (meV)
64
37
62
50
42
50.7
Thermal conductivity (W/cm °C)
1.32
0.6
0.9
0.91c
0.57c
1.0
Electron effective Longitudinal mass (m0 ) Transverse
0.9163
1.59
3.67
1.1
1.8
0.254
0.1905
0.0823 0.212
0.19
0.259
4.8
Hole effective mass (m0 )
Heavy hole
0.537
0.284
0.513d , 1.372e
0.409d , 0.336d , 1.022e 1.372e
0.67e
Light hole
0.153
0.043
0.211d , 0.145e
0.153d , 0.123d , 0.109e 1.372e
0.17e
Electron
1450
3900
60
294
200
160
Hole
370
1800
400
135
Mobility @ 300 K (cm2 /V s) a O.
Madelung, Ed., Semiconductor: Group IV Elements and III–V Compounds, in R. Poerschke, Ed., Data in Science and Technology, Springer, Berlin, 1991 b I. Vurgaftman, J. R. Meyer, and L. R. RamMohan, J. Appl. Phys., 89, 5815 (2001) c H. C. Casey, Jr, and M. B. Panish, Heterostructure Lasers, Part B, Academic Press, New York, 1978 d B  [100] e B  [111] © Springer Nature Switzerland AG 2020 K. Y. Cheng, III–V Compound Semiconductors and Devices, Graduate Texts in Physics, https://doi.org/10.1007/9783030519032
517
Appendix C
Important Physical Properties of Direct III–V Binary Semiconductorsa
GaAs Density
(g/cm3 )
GaSb
InP
InAs
InSb
5.3176
5.6137
4.81
5.667
5.7747
Lattice constant (Å)
5.65325
6.09593
5.8687
6.0583
6.47937
Melting temperature (°C)
1240
712
1062
942
527
Bandgap energy E g () @ 300 K (eV)b
1.424
0.726
1.353
0.354
0.174
Indirect bandgap E g (X) @300 K (eV)b
1.899
1.033, 0.753 (L)
2.273
1.37, 1.07 (L)
0.63 (0 K)
Intrinsic carrier concentration (cm−3 )
2.1 × 106
1.2 × 108
1.3 × 1015 2 × 1016
Dielectric constant
12.85
15.69
12.56
15.15
3.655
3.82
3.45
3.52
4.0
Optical phonon energy (meV)
36
28.8
42.7
29.6
23.7
Thermal conductivity (W/cm °C)
0.44
0.33
0.68
0.27b
0.17
Electron effective mass (m0 )
0.067
0.0412
0.077
0.022
0.014
Hole effective mass (m0 )
Heavy hole
0.50
0.28
0.56
0.35
0.45
Light hole
0.076
0.050
0.12
0.026
0.0158
Mobility @ 300 K (cm2 /V s)
Electron
9200
3750
4400
25,000
77,000
Hole
400
680
150
450
800
Refractive index @ E g
c
16.8
a O.
Madelung, Ed., Semiconductor: Group IV Elements and III–V Compounds, in R. Poerschke, Ed., Data in Science and Technology, Springer, Berlin, 1991 b I. Vurgaftman, J. R. Meyer, and L. R. RamMohan, J. Appl. Phys. 89, 5815 (2001) c H. C. Casey, Jr, and M. B. Panish, Heterostructure Lasers, Part B, Academic Press, New York, 1978
© Springer Nature Switzerland AG 2020 K. Y. Cheng, III–V Compound Semiconductors and Devices, Graduate Texts in Physics, https://doi.org/10.1007/9783030519032
519
Appendix D
Important Physical Properties of Wurtzite III–Nitride Semiconductorsa
GaN
AlN
InN
6.15
3.257
6.81–6.89
a
3.189
3.112
3.54
c
5.185
4.982
5.70
Melting temperatureb (°C)
2500
3000
1100
Band gap energy @ 300 K (eV)
3.438c
6.138c
0.64d
Dielectric constant
8.9–9.5
8.5
15
Refractive index @ E g
2.29
2.15
2.9
Optical phonon energy (meV)
91.8
113
73
Thermal conductivity (W/cm °C)
>2.1
3.3
0.45
Breakdown field strength (V/cm)
5 × 106
1.8 × 106
Electron effective mass (m0 )
0.2–0.22
0.3
0.07–0.26
Hole (heavy) effective mass (m0 )
1.0
k z − 3.53 k x − 10.42
1.63
Mobility @ 300 K (cm2 /V s)
Electron
1000
135
2700
Hole
≤200
14
Density (g/cm3 ) Lattice constant (Å)
a S. L. Rumyantsev, M. S. Shur, and M. E. Levinshtein, in GaNBased Materials and Devices, M. S. Shur and R. F. Davis, Ed., World Science, New Jersey, 2004 b O. Madelung, Ed., Semiconductor: Group IV Elements and III–V Compounds, in R. Poerschke, Ed., Data in Science and Technology, Springer, Berlin, 1991 c I. Vurgaftman, J. R. Meyer, and L. R. RamMohan, J. Appl. Phys., 89, 5815 (2001) d J. Wu, W. Walukiewicz, W. Shan, K. M. Yu, J. W. Ager III, S. X. Li, E. E. Haller, H. Lu, and W. J. Schaff, J. Appl. Phys., 94, 4457 (2003)
© Springer Nature Switzerland AG 2020 K. Y. Cheng, III–V Compound Semiconductors and Devices, Graduate Texts in Physics, https://doi.org/10.1007/9783030519032
521
Appendix E
Bandgap Energy of III–V Semiconductor Ternary Alloysa
Alloy
E g (x)
Crossover
Reference
Alx Ga1−x P
E g (X) = 2.273 + 0.215x
Alx Ga1−x As
E g () = 1.424 + 1.247x (x < 0.4) E g () = 1.424 + 1.102x + 0.477x 2 E g (X) = 1.899 + 0.210x + 0.055x 2 E(L) = 1.707 + 0.645x
x c ( − X) = 0.39
b
Alx Ga1−x Sb
E g () = 0.726 + 1.129x + 0.368x 2 E g (L) = 0.799 + 0.746x + 0.334x 2 E g (X) = 1.020 + 0.492x + 0.077x 2
x c ( − L) = 0.23 x c (L − X) = 0.4
c
Alx In1−x P
E g () = 1.353 + 2.68x − 0.48x 2 E g (X) = 2.273 − 0.165x + 0.38x 2
x c ( − X) = 0.36
Alx In1−x As
E g () = 0.354 + 1.949x + 0.7x 2 E g (X) = 1.37 + 0.794x
x c ( − X) = 0.64
Alx In1−x Sb
E g () = 0.1737 + 1.696x + 0.43x 2 E g (X) = 0.63 + 1.455x
x c ( − X) = 0.65
Gax In1−x P
E g () = 1.353 + 0.774x + 0.65x 2 E g (X) = 2.273 − 0.2x + 0.2x 2
x c ( − X) = 0.71
Gax In1−x As
E g () = 0.358 + 0.589x + 0.477x 2
Gax In1−x Sb
E g () = 0.174 + 0.138x + 0.415x 2
AlPx As1−x
E g (X) = 2.164 + 0.104x + 0.22x 2
GaPx As1−x
E g () = 1.424 + 1.163x + 0.19x 2 E g (X) = 1.899 + 0.134x + 0.24x 2
InPx As1−x
E g () = 0.354 + 0.899x + 0.1x 2
AlSbx As1−x
E g (X) = 2.164 − 0.828x + 0.28x 2
a
x c ( − X) = 0.47
(continued)
© Springer Nature Switzerland AG 2020 K. Y. Cheng, III–V Compound Semiconductors and Devices, Graduate Texts in Physics, https://doi.org/10.1007/9783030519032
523
Appendix E: Bandgap Energy of III–V Semiconductor Ternary Alloysa
524 (continued) Alloy
E g (x)
GaSbx As1−x
E g () = 1.424 − 2.127x + 1.43x 2
InSbx As1−x
E g () = 0.354 − 0.85x + 0.67x 2
a I.
Crossover
Reference
Vurgaftman, J. R. Meyer, and L. R. RamMohan, J. Appl. Phys., 89, 5815 (2001) C. Casey, Jr, and M. B. Panish, Heterostructure Lasers, Part B, Academic Press, New York, 1978 c K. Y. Cheng, G. L. Pearson, R. S. Bauer, and D. J. Chadi, Bull. Am. Phys. Soc., 21, 365 (1976) b H.
Appendix F
Bandgapa, b and Polarization Parametersc of Wurtzite IIINitride Semiconductor Ternary Alloys
Alloy
E g (x), PSP (x), PPE (x)
Alx Ga1−x N
E g (x) = 3.438 + 2.020x + 0.7x 2 (eV) PSP (x) = −0.090x − 0.034(1 − x) + 0.021x(1 − x) (C/m2 ) PE PAlGaAs/InN (x) = −0.28x − 0.113(1 − x) + 0.042x(1 − x) (C/m2 ) PE (x) = −0.0525x + 0.0282x(1 − x) (C/m2 ) PAlGaAs/GaN pE
PAlGaAs/AlN (x) = 0.026(1 − x) + 0.0248x(1 − x) (C/m2 ) Alx In1−x N
E g (x) = 0.64 + 3.028x + 2.5x 2 (eV) PSP (x) = −0.090x − 0.042(1 − x) + 0.070x(1 − x) (C/m2 ) PE PAlInAs/InN (x) = −0.28x + 0.104x(1 − x) (C/m2 ) PE (x) = −0.0525x + 0.148(1 − x) + 0.0938x(1 − x) (C/m2 ) PAlInAs/GaN PE (x) = 0.182(1 − x) + 0.092x(1 − x) (C/m2 ) PAlInAs/AlN
Inx Ga1−x N
E g (x) = 3.438 − 4.198x + 1.4x 2 (eV) PSP (x) = −0.042x − 0.034(1 − x) + 0.037x(1 − x) (C/m2 ) PE (x) = − 0.113(1 − x) − 0.0276x(1 − x) (C/m2 ) PInGaAs/InN PE PInGaAs/GaN (x) = 0.148x − 0.0424x(1 − x) (C/m2 ) PE (x) = 0.182x + 0.026(1 − x) − 0.0456x(1 − x) (C/m2 ) PInGaAs/AlN
a I.
Vurgaftman and J. R. Meyer, J. Appl. Phys., 94, 3675 (2003) Wu, W. Walukiewicz, W. Shan, K. M. Yu, J. W. Ager III, S. X. Li, E. E. Haller, H. Lu, and W. J. Schaff, J. Appl. Phys., 94, 4457 (2003) c O Ambacher, J Majewski, C Miskys, A Link, M Hermann, M Eickhoff, M Stutzmann, F Bernardini, V Fiorentini, V Tilak, B Schaff, and L F Eastman, J. Phys.: Condens. Matter 14, 3399 (2002) b J.
© Springer Nature Switzerland AG 2020 K. Y. Cheng, III–V Compound Semiconductors and Devices, Graduate Texts in Physics, https://doi.org/10.1007/9783030519032
525
Index
A Absolute reference energy level, 206, 223, 226 Absorption coefficient – intrinsic, 326, 328, 330–332, 336 Absorption quantum efficiency, 491–493, 495 Acoustic phonon – longitudinal acoustic (LA) mode, 111 – transverse acoustic (TA) mode, 111 Activation energy, 122–127, 130, 131, 190, 192, 198 Aface, 151, 152, 281, 283, 284, 376 Airy function, 267, 268, 270, 285, 358, 361, 379 Akasaki, Isamu, 7, 471 AlCl3 , 406 ALDwindow, 406 Alferov, Zh. I., 6, 238 AlGaAs, 6, 7, 92, 102, 130, 192–194, 196, 198, 200, 243, 244, 246, 248, 274, 285, 286, 336, 353–356, 358–361, 366, 368, 372–375, 383, 433, 435, 442, 443, 445, 452, 454, 460, 464, 465, 470, 486, 493, 506, 507, 510– 512, 525 AlGaInAs, 456 AlGaInP, 7, 468–471 AlGaN, 152, 283, 376–382 AlInAs, 375, 479, 525 AlInN, 152 AlInSb, 415 Alloy scattering potential, 120 AlN, 32, 101, 105, 149, 151, 152, 233–235, 281, 380, 471, 521
Al2 O3 , 140, 149, 151, 196, 197, 340, 376, 377, 403, 404, 407, 409–412, 461, 462 Al(OH)3 , 196 AlO(OH), 196 AlSb, 32, 105, 106, 123, 141, 157, 207, 210–213, 240, 265, 484, 517 Amano, Hiroshi, 7 Ammonia (NH3 ), 151, 169, 170, 179, 181 Ammonothermal, 168–170 Amphoteric, 122, 125, 126, 172 Anderson’s electron affinity model, 204 Angular momentum, 98 Antisite defect, 132, 139, 162, 194 Arakawa, Y., 449 Arsine (AsH3 ), 54, 178, 180–182, 188, 189, 196 As(CH3 )3 , 410 AsCl3 , 177, 178 AsO, 407, 408 As2 O3 , 196, 197, 399, 410 As2 O5 , 399, 410 Atalla, M. M., 3 Atomic Force Microscope (AFM), 452 Atomic Layer Deposition (ALD), 140, 404– 407, 410–412 AuBe alloy, 124 Auger coefficient, 334, 449 Auger recombination, 332–334, 433, 448 AuZn alloy, 124
B Band AntiCrossing (BAC) model, 153–155 Band discontinuity – type I, 209, 383, 415 – type II, 212, 213, 383
© Springer Nature Switzerland AG 2020 K. Y. Cheng, III–V Compound Semiconductors and Devices, Graduate Texts in Physics, https://doi.org/10.1007/9783030519032
527
528 – type II brokengap interface, 212 – type II staggered interface, 212 Bandedge profile, 247, 249, 284, 445 Band filling, 305, 307 Bandgap – direct, 4, 6, 92, 93, 96, 98, 101, 105, 113, 145–147, 149, 157, 158, 224, 301, 302, 309, 315, 323, 324, 332, 335, 466, 467, 470, 517 – indirect, 4, 93, 94, 96, 98, 99, 112, 143, 145, 149, 150, 154, 155, 208, 304, 310, 312, 323–325, 466, 470, 471, 517, 519 Bandgap narrowing, 308 Bandgap renormalization, 308 Bandgap shrinkage, 308, 385 Band tails, 307, 308, 326 Bandtoband Auger processes – CHCC, 334 – CHHS, 334, 335, 448, 449 – CHLH, 334, 335 Bandtoband transitions, 325, 474 Bardeen, John, 1, 2, 11, 12, 139, 326, 400, 403 Bardeen limit, 139 Base recombination lifetime, 502 Beryllium (Be), 124, 126, 127, 192, 386, 415 Bface, 151, 281, 376 Binary alloy, 120, 147, 149, 210, 213, 233, 240 Bloch, Felix, 67 Bloch function, 68–70, 74, 88 Bloch oscillation, 92, 103 Bloch’s theorem, 57, 67, 68, 81 B2 O3 , 165 Bohr radius, 23, 26, 27, 123, 257, 279, 451, 515 Boltzmann distribution function, 114, 133, 136, 137 BoseEinstein distribution, 304, 316 Boundary layer, 176, 180–182, 189 Bowing parameter, 144–149, 152, 153, 213, 228, 230, 231 Bragg diffraction condition, 39, 45, 47, 48 Bragg law, 44, 47, 50 Bragg plane, 47, 48 Brattain, Walter, 1, 2, 11, 12 Bravais lattices, 13, 16 Breakdown field strength, 376, 521 Brillouin zone – FCC laatice, 50, 73, 75 – simple hexagonal lattice, 53, 54 Brody, T. P., 401 Bulk crystals, growth of, 132, 162, 168, 169
Index Bulk GaN crystals, 168 Burger’s vector, 216, 217 BursteinMoss shift, 306, 308
C Cadmium (Cd), 124 Capture probability, 489, 491, 492 Carbon (C), 29–31, 125, 126, 386, 406 Cardona, M., 206 CBr4 , 126, 386 CCl4 , 126, 386 Characteristic temperature, 433, 477, 486 ChargeNeutrality Level (CNL), 140, 141, 400–404, 412 Chemical Vapor Deposition (CVD), 6, 7, 124, 161, 176, 180, 405, 406 Cho, Alfred Y., 6, 182 Christensen, N. E., 206 Cladding layer, 199, 421–423, 433, 434, 436, 438, 444, 445, 452, 479, 480, 500, 509 Cleavage plane, 107, 108 Compliance, 217 Conduction band – dispersion, 153, 155 – minimum (CBM), 96, 98, 105, 113, 137, 303, 309, 324, 401, 402, 412 – offset, 379, 380, 389, 403, 404, 448, 449, 484 Conductivity, 4, 8, 108, 115, 116, 125, 127, 132, 133, 172, 178, 180, 289, 294, 345, 376, 394, 396, 517, 519, 521 Configuration – interstitial, 128, 130 – substitutional, 128, 130 Configuration coordinate diagram, 129, 130 Confinement factor, 422, 423, 425, 429, 444, 459, 462, 478, 480, 482, 510 Congruent melting temperature, 162 Continuity equation, 190, 254, 255 Coupling constant, 441 Covalent bond – antiparallel spin, 25 – electronpair bond, 25 Covalent bonding – anitbonding state, 25 – bonding state, 25 Critical field intensity, 369 Critical layer thickness, 215–217, 239, 240, 375 Crystal diffraction – Laue diffraction method, 39, 45
Index – rotating crystal diffraction method, 39 Crystalfield splitting energy, 101, 233 Cutoff frequency, 349, 352, 371, 383, 385, 386, 391–395 Czochralski pulling technique, 164
D Dallessasse, John, 196 Dangling surface bond, 138, 185 Dark current, 487–490, 492 De Broglie relationship, 63 Deep levels, 127, 130, 132 Defects – antisite, 132, 139, 162, 194 – Frenkel, 191 – Schottky, 191 – vacancy, 191 Deformation potential – hydrostatic, 207, 222, 232, 233 – shear, 207, 224, 232, 233 Degree of randomness, 120 Delay time – emitter, 390 – spacecharge layer, 390 Delta doping, 372 Density of States (DOS) – bulk structure, 66, 451 – joint, 302 – quantum dot structure, 66, 450, 451 – quantum well structure, 66, 445, 451 – quantum wire structure, 66, 451 – superlattices, 275–277 Depletion – region, 243–245, 249–255, 340, 341, 343, 344, 346, 347, 364, 386, 391, 393, 394 – width, 244, 246, 251, 252, 285, 341– 343, 350, 362 Detectivity, 492, 493, 495, 496 Diamond crystal structure, 33, 34, 105 Diatomic linear chain model, 108 Dielectric constant – complex, 293, 295–297 – optical relative, 296 – static relative, 296 Dielectric waveguide, 421–423, 433, 479, 480 Diethyltellurium (DETe), 125 Diethylzinc (DEZ), 180 Diffraction, 11, 38–40, 44–48, 73, 78, 168, 170, 184, 185, 408, 441 Diffusion
529 – coefficient, 124–126, 191, 192, 247, 371, 427 – constant, 190, 191, 390, 501 – interstitial, 191 – length, 191, 255 – self, 192–194 – substitutional, 191 – substitutioninterstitial, 191, 192 Dilute nitride compounds, 153 Dingle, R., 352, 449 Direct bandgap semiconductor, 4, 92, 96, 98, 105, 113, 302, 315, 323, 324, 332, 335, 466, 467 Disilane (Si2 H6 ), 126, 180 Dislocation – Misfit, 106, 215, 216 – threading, 149, 214, 215 Dislocation density, 161, 166–168, 170, 454 Disordering, 161, 190, 192, 193 Displacement flux density, 289, 359, 363 Distributed Bragg Reflector (DBR) lasers, 440, 441 Distributed Bragg reflector mirrors, 458, 460 DistributedFeedback (DFB) lasers, 440, 441 Donorcomplex (DX) center, 127 DoubleHeterostructure (DH), 6, 238, 286, 335, 336, 420, 421, 423, 428, 434, 435, 444, 446, 448, 452, 470, 500 Downward transition rate, 318, 320 Drift time, 506 Drift velocity – saturation, 490 DX center, 127, 130, 131, 372–375
E Effective density of states – conduction band, 114 – heavyhole band, 115 – lighthole band, 115 Effective mass – conductivity, 108, 115, 116 – DOS, 114, 115 Eglash, S. J., 486 Einstein’s A and B coefficients, 317, 319 Elastic – coefficient, 219 – constant, 207, 219, 233 EL2 defects, 132 Electron affinity, 19, 20, 139, 203–205, 403, 404 Electronegativity, 32, 153, 312
530 ElectronHole Pair (EHP), 156, 297, 309, 322, 505 Electronic subband, 260 Electron spins, 98 Empirical band alignment methods, 210 Empirical CNL model, 400 Emptylattice model, 72 Energy band structures – conduction band, 94, 305 – valence band, 94, 305 – wurtzite structure, 99 Energy conservation, 300, 324 Energy eigen value, 59, 60, 62, 63, 71, 79, 83, 260, 261, 263, 268, 272, 449 Energy surface – nonspherical, 114, 116 – spherical, 114, 116 Epitaxy, 6, 124, 125, 151, 161, 168, 170– 172, 174, 176–178, 182, 183, 188, 189, 203, 215, 350, 385, 439, 444, 469, 470, 473 Equivalent temperature, 119 Escape – probability, 491, 495 – time, 475, 491, 493 Ewald sphere construction, 45, 46 Excited state operation, 506 Exciton – binding energy, 309–311, 313 – bound, 311, 313 – donor bound, 310 – orbit radius, 311 Exciton absorption, 309, 310 Extended Xray Absorption Fine Structure (EXAFS) technique, 120, 143 External quantum efficiency, 432, 466–469, 471, 482, 510 Extinction coefficient, 294, 296 Extraction quantum efficiency, 467, 468 F Fabry–Perot cavity, 273, 420, 423, 424, 435, 458, 465, 466 Fang, F. F., 269 FangHoward wave function, 270 Farfield pattern, 434, 435 Feng, Milton, 351, 352, 398, 497 FermiDirac distribution function, 114, 133, 318 FermiDirac integral, 134–137, 156, 335, 336 FermiDirac inversion factor, 326, 328, 330, 333, 335, 336
Index Fermi level, 117, 132, 133, 136, 139, 140, 156, 191, 193, 194, 204, 205, 235, 236, 241, 248, 250, 251, 254, 285, 305, 308, 317, 318, 320, 329, 330, 335, 353, 358, 361, 362, 365–368, 373, 378, 379, 385, 399–402, 408, 409, 414, 415, 446, 447, 477 Fermi pinning level, 142 Fermi’s Golden rule, 322 Fick’s first law, 190 Fick’s second law, 190 Focal Plane Array (FPA), 496, 497 FranckCondon shift, 129 Frank, D. J., 213, 400, 401, 416, 450 Franz–Keldysh effect, 277, 279, 280, 503 Free carrier concentration – 2D, 136 – 3D, 132 Free electron theory, 57, 58, 67, 74, 87 Frosch, Carl, 2 G GaAs, 4, 6, 7, 18, 30–32, 34, 46, 47, 59, 92, 96, 98, 102, 103, 105, 106, 112–116, 118, 121–127, 132, 133, 138–142, 144, 145, 147, 148, 155–158, 161– 163, 165–167, 170–173, 177–182, 184–187, 191–195, 199, 200, 207– 210, 213, 216, 217, 224, 228–231, 265, 274, 284–287, 289, 297, 301, 302, 306–311, 323, 326, 327, 332, 335, 336, 339, 340, 350–358, 361, 366–368, 371–373, 375, 376, 383, 386, 388, 396, 397, 399, 401, 402, 404, 407–415, 420, 423, 427, 433, 442, 444, 445, 447, 450–454, 456, 460, 464, 465, 470, 471, 486, 493, 496, 498, 501, 506, 507, 509–511, 519 GaAsN, 154 GaAsO4 , 399 GaAsP, 6, 7, 469, 470 GaAsSb, 389, 392, 398, 414, 448, 449 GaCl, 177, 178 Gaface, 151, 152, 280, 376–380 GaInAsP, 178, 179, 509 Gain coefficient – differential, 425 – model, 423 – peak, 442 Gainguide lasers, 435–439 GaInSbAs, 484 Gamma function, 134, 137
Index
531
GaN, 7, 8, 32, 35–37, 100, 101, 105, 149– 153, 163, 168–170, 179, 181, 232– 235, 241, 280–284, 286, 289, 376– 382, 404, 405, 412, 414, 471, 521 GaNbased HEMT structures, 375 GaN bulk crystal growth – ammonothermal method, 168–170 – high nitrogen pressure solution growth, 168 – hydride vapor phase epitaxy (HVPE), 168, 178 – Na flux method, 168 Ga–O, 407, 408, 410 Ga2 O, 407 Ga2 O3 , 399, 409 Ga2 O3 (Gd2 O3 ) [GGO], 140, 340, 404, 407, 409 GaP, 6, 7, 32, 96, 123, 141, 148, 157, 179, 192, 207, 210, 265, 310–314, 323, 388, 404, 468, 469, 471, 517 GaPN, 7, 153, 312–314 GaSb, 32, 123, 140–142, 157, 165, 207, 210– 212, 239, 240, 265, 334, 404, 405, 484, 485, 519 Gauss’ law, 359, 362, 377 Gd2 O3 , 140, 403, 404, 407, 409 Germanium (Ge), 1–3, 9, 11, 12, 32, 93–96, 99, 115, 119, 126, 153, 155–158, 164, 172, 192, 213, 224, 226, 323, 399, 413, 419, 517 Gibbs energy, 409 Goryunova, N. A., 105 GradedIndex SeparateConfinement HeteroStructure (GRINSCH), 445, 454 Gradientfreeze method – horizontal, 165, 166 – vertical (VGF), 161 Green gap, 471 Group velocity, 89–92, 320 Growth mode – Frankvan der Merve, 450 – Stranski–Krastanov (SK), 450–453 – Volmer–Weber, 450 Gummel plot, 386 Gunn, J. G., 6
– band, 97, 98, 100, 115, 117, 123, 206, 224, 225, 239, 264, 265, 334, 335, 416, 433, 447 Henry, C. H., 449 Heterjunction Bipolar Transistors (HBTs) – processing, 397 Heterojunction – anisotype, 238, 248 – isotype, 237, 238, 246, 248, 250 Heterojunction Bipolar Transistors (HBTs) – current gain, 383, 385–387, 396, 501 – device passivation, 394, 397 – device scaling, 394, 396 – double (DHBT), 383, 386, 388, 392, 398, 415 – emitter ledge passivation, 396 – Kirk effect, 393 – maximum current gain, 415 – single (SHBT), 383, 384, 387, 388, 392, 395 Heterojunction under – bias, 251 – equilibrium, 243, 285, 362 Hexagonal ClosePacked (HCP) structure, 22, 35, 54 HfCl4 , 406, 407 HfO2 , 140, 340, 403, 404, 406, 407, 410–412 HgCdTe, 486 Highκ dielectrics, 403–411 High ElectronMobility Transistor (HEMT) – normallyoff, 368, 369 – normallyon, 368 – sheet carrier density, 358, 366, 371 – spacer layer, 359–361, 367, 371, 373, 413 Holonyak, Jr., Nick, 6, 7, 192, 196, 444, 463, 469, 497 Hong, Mingwhei, 409 Hooke’s law, 108, 109, 218 Horizontal Bridgman method, 165 Howard, W. E., 269, 285, 413 Hydrogen model, 123, 310 Hydrogen passivation, 7, 126, 153 Hydrogen selenide (H2 Se), 124, 125 Hydrogen sulfide (H2 S), 124, 178 Hydrolyze, 196 Hydrothermal, 169, 170
H Harrison, W. A., 206 Heaviside step function, 331 Heavy hole
I I C –V CE characteristics, 498, 504 ImpurityInduced Layer Disordering (IILD), 161, 190, 192–195
532 InAs, 32, 105, 120, 123, 125, 141, 148, 157, 158, 207, 210–213, 224, 228, 229, 231, 240, 265, 334, 336, 396, 401, 404, 448–454, 484, 485, 519 InAsSb, 448 Indexguided laser – buriedheterostructure (BH), 439 – ridgewaveguide, 439 Indirect bandgap semiconductor, 4, 93, 94, 98, 112, 304, 312, 323 Infinitely deep square potential well, 256, 257, 259 InGaAs, 120, 200, 311, 331, 332, 375, 382, 388, 392, 395–398, 401, 412, 428, 447–449, 484, 497, 498, 506, 507, 509, 511 InGaN, 7, 284, 286, 471 InN, 32, 101, 149, 152, 233, 235, 471, 521 InP, 4, 32, 105, 121–126, 140–142, 144, 146–148, 155, 157, 158, 161, 163, 165, 167, 174, 207, 212, 224, 228– 231, 240, 241, 265, 286, 289, 297, 298, 323, 375, 382, 383, 388, 389, 392, 395, 397, 398, 402, 404, 405, 415, 425, 428, 433, 439, 442, 448, 451, 452, 455–457, 474, 479, 497, 511, 512, 519 InSb, 32, 98, 105, 106, 123, 141, 157, 207, 210, 239, 240, 265, 404, 405, 415, 519 Integrated Circuit (IC), 3, 4, 6, 8, 11, 194, 195, 399, 406, 413, 496 Interaction potential, 154 Interband Cascade Lasers (ICL), 484–486 Interband transition, 233, 445, 449, 472– 474, 485, 486 Interface tension, 215 Interface trap density, 140, 340, 400, 401, 411, 412 Internal quantum efficiency, 432, 454, 467, 469, 510 Intersubband relaxation time, 491 Intraband relaxation time, 332 Intraband scattering, 332 IntraCavity Photonassisted (ICP) tunneling, 503–506 Intrinsic carrier concentration, 105, 115, 253, 517, 519 Intrinsic drain current, 411 Ioffe, A. F., 106 Ionic bond – Madelung constant, 20 – binding energy, 20
Index – ionization energy, 19 Ioniccovalent bonds, 31, 96 Ionicity parameter, 32 Ionization energy – acceptor, 123, 153 – donor, 123, 153 Ionized impurity concentration, 118 Isoelectronic traps, 153, 312, 313
K Kahng, Dawon, 3 Kazarinov, R., 473 Kilby, Jack, 3 KronigPenney model, 80, 81, 84, 86, 102, 274 Kronig, R. de L., 80, 298 Kunig, H. E., 401
L Laidig, W. D., 192 La2 O3 , 403, 404, 407 Laser diode – characteristic temperature, 432 – internal loss, 510 – mirror loss, 436 Lateral Superlattice (LSL), 455, 456 Lattice – BCC, 51 – FCC, 22, 50–52, 73, 75, 76 Lattice constant, 4, 5, 33, 45, 47, 54, 71, 75, 85, 92, 102, 103, 105–107, 111, 120, 141–144, 147, 149, 152, 157, 158, 170, 171, 173, 174, 207, 208, 213– 217, 220, 221, 224, 231–233, 274, 282, 377, 401, 416, 517, 519, 521 Lattice defect, 170, 191 Lattice relaxation, 128, 129, 455 Lattice vibration, 37, 93, 108, 112, 118, 119, 155, 333 Lavine, B. F., 486, 493 Lifetime – carrier, 127, 315, 323, 333, 334, 385, 428, 430, 459, 485, 489, 500, 502, 510 – effective, 478, 485, 503 – minority carrier, 12, 127, 238, 252– 255, 339, 385, 388, 389, 396, 436, 466, 467, 500, 501, 502, 506, 508 – photon, 429, 430, 502, 503, 510 – radiative, 323 Lightcurrent (L–I) curve, 431 LightEmitting Diodes (LED)
Index – with tiltedbasecharge distribution, 508 LightEmitting Transistor (LET), 382, 497, 511, 512 Light hole – band, 97, 98, 100, 115, 123, 206, 224, 225, 239, 264, 265, 334, 416, 447 Linear Combination Atomic Orbit (LCAO), 206 Linear MuffinTin Orbitals (LMTO), 206 Linewidth, 446, 450–452, 454, 478, 479 Liquid Encapsulated Czochralski (LEC) technique, 132, 133, 165, 167 Liquid isotherms, 173, 174 Liquid Phase Epitaxy (LPE) – equilibrium cooling, 175 – step cooling, 175 – supercooling, 175 – twophase solution cooling, 175 Liquidsolid reaction, 162 Longitudinal mode, 426, 427, 433, 434, 436, 439, 440, 458, 463, 465 LongWavelength Infrared (LWIR), 496, 497 Lorentz, Hendrick, 294 Luttinger parameters, 98, 123, 265 LVCE characteristics, 498, 499, 504, 505 M Magnesium (Mg), 7, 124, 153, 192, 471 Magnetic moment, 98 Maiman, Theodore, 4 Manasevit, H. M., 6, 180 Matthews and Blakeslee’s model, 215, 216 Matthiessen’s rule, 117 Maximum oscillation frequency, 389, 393, 394 Maxwell’s equations, 289 Memory effect, 125 MetalInduced Gap States (MIGS) model, 400, 403 Metalorganic Chemical Vapor Deposition (MOCVD) – lowpressure (LPMOCVD, 181 MetalOxideSilicon Field Effect Transistor (MOSFET) – complementary MOSFET (CMOS), 4, 8, 9, 399, 402, 408, 413, 416 MetalSemiconductor FieldEffect Transistor (MESFET) – channel conductance, 345 – depletion mode, 343, 344, 346, 347, 350
533 – enhancement mode, 343, 344 – output conductance, 347 – saturation drain voltage, 341, 342 – shortchannel effect, 350 MgO, 124, 409 Miller indices, 14, 15, 46 Mineralizer, 169 Minimum noise figure, 371 Miscibility gap, 143, 144 Misfit – strain, 206, 215 Mn2 O3 , 409 Mobility, 4, 6, 8, 9, 35, 105, 117–122, 126, 127, 155–157, 203, 239, 241, 247, 284, 339, 340, 348, 351–358, 370, 371, 375, 376, 380, 399, 406, 411–413, 415, 416, 490, 517, 519, 521 Modelsolid theory, 206, 209–211, 239, 240, 415 Mode number, 64, 426, 427, 429, 510 Mode of oscillation, 64, 429 Mode spacing, 427, 510 Modulation doping heterostructure – interface scattering, 357 – intersubband scattering, 356 – inverted, 356 – normal, 356 Molecular Beam Epitaxy (MBE) – gas source (GSMBE), 161, 188, 189 – metal organic (MOMBE), 125, 126, 189 – plasmaassisted (PAMBE), 151, 189 Moll, John, 2 Momentum conservation, 113, 300, 324, 325, 334, 472 Moore, Gordon, 3, 8 Moore’s law, 8, 399, 402, 415
N Nakamura, Shuji, 7 NaOH, 169 Natural bandalignments of IIInitrides, 234 Natural oscillation frequency, 295 Nearfield pattern, 433, 435, 438 Nearly free electron approximation, 75, 77, 80, 84 Negative differential resistance, 121 Net absorption rate, 320, 429 Net stimulated emission rate, 320 Newton’s law, 90 Nface, 151, 281, 376–378, 380
534 NH4 OH, 407, 410, 411 (NH4 )2 S, 407, 410 NN lines, 313 Noise current, 492 Nonradiative recombination process, 333, 473 Noyce, Robert, 3 O Offset voltage, 388, 482 Optical output power, 432 Optical phonon – longitudinal optical (LO) mode, 112, 119 – transverse optical (TO) mode, 112 Optical phonon energy, 119, 475, 517, 519, 521 Oxidation rate – diffusion limited, 197 – reactionrate limited, 197 Ozone, 407 P Parallel conduction, 371, 373, 374 Pauli exclusion principle, 19, 25, 133 Pauling, Linus, 32, 106 PCl3 , 178 Penney, W. G., 80 Permittivity – free space, 290, 403, 515 – relative, 403 Persistent photoconductivity (PPC) effect, 131, 372 PH3 , 25, 26, 182, 188, 189 Phase diagram – existence region, 162 – ternary, 173, 174 Phase separation, 144 Phonon – absorption, 303–305, 309 – emission, 121, 303, 305, 309, 325, 475 Phononassisted tunneling, 278, 504, 505 Phonon dispersion curves – acoustic branch, 110, 119, 310 – optical branch, 110, 111, 119, 310 Photoconductive gain, 491–493, 495 Photocurrent, 486, 487, 490–493 Photodetector, 7, 203, 419, 486, 488, 495, 499, 500 Photoemission, 491 Photoluminescence (PL), 313, 314, 326, 327, 450, 452, 456
Index Photon – density distribution, 315, 317, 320 – density of states, 315, 316 – distribution function, 315, 316 Photonassisted tunneling, 278, 473, 504, 505 Photon density, 315–317, 320, 427, 429, 430, 506 Photon rate equation, 429 Piezoelectric coefficient, 233, 281 Piezoelectricinduced sheet charge density, 379 Pinchoff voltage, 343, 346, 366 Pinning parameter, 403 Planar doping, 374 Planck’s constant, 492, 515 Poisson’s equation, 243, 244, 249, 363, 365, 393 Poisson’s ratio, 216, 217 Polarization – piezoelectric, 151, 234, 281, 282, 377, 378 – resonant, 295 – spontaneous, 37, 151, 152, 233, 281, 376–378 – TE mode, 316 – TM mode, 316, 487 Polarizationinduced sheet charges, 376 Population inversion, 319, 328, 420, 423, 474–478 Potassium amide, 169 Probability density, 23, 24, 26–29, 76, 77 Process Evaluation Chip (PEC), 496 Propagation constant – complex, 292, 293, 424 Pseudomorphic High ElectronMobility Transistor (pHEMT), 239, 241, 375, 414, 415 Pyrolytic BN (PBN) crucible, 165, 167
Q Quantum cascade lasers – diagonal transition, 474, 475 – slope efficiency, 483 – vertical transition, 475 – voltage at laser threshold, 482 QuantumConfined Stark Effect (QCSE), 279, 280 Quantum dot lasers – selfassembled, 451–454, 457 Quantum Dot (QD) layer – closely stacked, 453
Index – columnarshaped, 453 Quantum well heterostructures – multiple (MQW), 283, 284, 489 – realistic, 261 – strained, 265, 447, 448 – triangular, 358 QuantumWell Infrared Photodetectors (QWIP), 7, 419, 486–497 Quantum well laser – multiple, 444, 449 – single, 444 Quaternary alloy – typeI, 148, 149 – typeII, 148, 149, 158, 231 Quinternary alloy, 143
R Rate equation, 427, 429, 430, 477, 478, 483 Reciprocal lattice – vector, 40, 42–45, 47, 48, 51, 70, 72, 76 Recombination rate – Auger, 333 – nonradiative, 333 – radiative, 322 – stimulated, 427, 501 Reduced mass, 302, 309 Reduced zone representation, 70–72 Reflection coefficient, 272, 424, 425, 461 Reflection HighEnergy Electron Diffraction (RHEED) method, 45, 184, 408 Refractive index – AlGaAs, 195, 299 – AlGaN, 300 – complex, 293 – GaInAsP, 178 Relaxation time – intraband, 332 Resonant periodic gain, 461 Resonant tunneling, 272, 273, 474 Resonant wavelength, 442 Responsivity, 492–496 RHEED intensity oscillation, 187 Rydberg energy, 123
S Sakaki, H., 449 Sapphire (Al2 O3 ), 6, 149, 151, 152, 168, 179, 231, 241, 281, 376, 471 Saturation current, 346, 384, 385 Saturation electron velocity, 376
535 Scanning Electron Microscope (SEM), 194, 195, 199, 200, 398 Scattering – alloy, 117, 120, 121 – deformation potential, 118 – impurity, 117, 118, 351–353 – lattice, 117–119, 157 – piezoelectric, 117, 119 – polar, 117, 119 Scattering probability, 4, 117, 156, 332, 357 Schottky barrier height, 139–141, 213, 340, 400, 416 Schrödinger wave equation, 28, 58, 69, 70, 78, 82, 259, 261, 277 SecondaryIon Mass Spectroscopy (SIMS), 196 Selection rule, 331, 445, 487, 488 Selenium (Se), 124, 126, 172, 192 SelfConsistent Interface Calculations (SCIC), 206 Semiconductor laser, 9, 329, 332, 335, 419, 421, 422, 427, 433, 440, 441, 444, 448–450, 458, 481, 500, 502 Semiinsulating substrate, 4, 339, 340, 351, 496 Separate Confinement Heterostructure (SCH), 445, 456, 457 Shockley, William, 1–3, 322, 382, 467 SiGe, 226 Silicon (Si), 2–4, 6–9, 11, 30–32, 93, 95, 96, 98, 99, 105–107, 112–116, 119, 121, 122, 125–128, 130–132, 139, 153, 155, 156, 164, 168, 172, 191– 197, 213, 224, 226, 241, 284, 289, 301, 305, 306, 323, 335, 355, 372– 374, 383, 399, 401–404, 406, 407, 409, 413, 415, 416, 419, 454, 479, 496, 517 SimWindows simulation software, 286 SiO2 , 2–4, 9, 195, 399, 401–403, 407, 409 Sodium amide, 169 Sodium azide (NaN3 ), 168 Solidus isotherms, 173 Sp3 hybrid orbit, 23, 29, 30, 93 Spinorbit splitting, 123, 149, 209, 212, 230 Splitoff band, 97, 98, 206, 224, 433 Spontaneous emission factor, 429 Spontaneous emission rate, 289, 318–321, 429 Spontaneous recombination lifetime, 502, 503 Square barrier, 270, 272, 286 Stark effect, 279
536 Stimulated emission – necessary condition, 319 Stimulated emission rate, 289, 319–321, 326, 327, 429 Strain – biaxial, 220, 224, 231, 447 – compressive, 220, 224, 225, 239, 282, 416 – hydrostatic, 226, 228, 231 – shear, 224, 225 – tensile, 220, 224, 225, 282, 377, 455 StrainInduced Lateral Layer Ordering (SILO) growth, 454 Strainlayer superlattice, 455 Stress – hydrostatic stress, 221 Stripegeometry lasers, 435, 436 Sulfur (S), 124, 132, 192, 407 Superinjection, 238 Superlattices – density of states, 275–277 – miniband, 274, 275, 475, 477 Surface passivation, 394, 397, 399, 407, 408 Surface phase diagram, 186 Surface plasmon waveguide, 480, 481 Surface Recombination Velocity (SRV), 396, 397 Surface states density (Dit ), 399 Suris, R., 473 Symmetry operation – inversion, 16 – reflection, 16 – rotation, 16, 17 – rotationreflection, 16, 17
T Tellurium (Te), 125–127, 172 Ternary alloy, 6, 7, 120, 121, 141, 144–146, 148, 149, 152, 153, 212, 213, 228, 230, 239, 240, 282, 286, 523, 525 Tersoff, J., 206 Tetrahedron covalent radii, 106 Tetrahedron structure, 30 Tetrakis (Ethylmethylamino) hafnium (TEMAHf), 410 Thermal conductivity, 4, 8, 108, 376, 396, 517, 519, 521 Threeport, 497, 498, 500, 511 Threshold current density, 6, 420, 427–430, 444, 446, 447, 451, 453, 454, 456, 458–462, 476–478, 481, 482, 485, 486, 510, 511
Index Threshold voltage, 342, 343, 346, 350, 366, 367, 373, 413, 483 Tin (Sn), 96, 126, 127, 172, 192 Tiwari, S., 213, 400, 401 Transconductance – intrinsic, 346, 347 Transferelectron effect, 122 Transistor lasers – charge population distribution, 501 – dielectric relaxation time, 506 – excited state operation of, 506 – optical collector output port, 498 – voltage modulation of, 503 Transistors – bipolar junction, 1, 339, 340, 382–386, 388 – pointcontact bipolar, 12 Transition matrix, 322, 326 Transition probability, 300, 302, 304, 318, 322, 323, 326 Transit time – base, 390, 394, 395 – collector, 390, 394, 395 – emittertocollector, 389 Transmission coefficient, 274, 286, 489 Transmission Electron Microscope (TEM), 193, 455 Transparency condition, 289, 329, 330, 335, 336, 424, 446 Transverse mode, 113, 434, 435, 438, 439 Triethylgallium (TEG), 151, 180 Triethylindium (TEI), 181 Trimethylaluminum (TMA), 151, 406, 407, 410 Trimethylgallium (TMG), 180, 181 Trimethylindium (TMI), 181 Tunneling current, 403, 488, 503, 506, 507 Tunnel Junction Transistor Laser (TJTL), 504, 505, 507 Turnon voltage, 195, 382, 389, 482, 509 TwoDimensional Electron Gas (2DEG), 237, 239, 249, 251, 283, 339, 351– 358, 361, 362, 366–369, 371, 373, 375–381, 413, 414 TwoDimensional Hole Gas (2DHG), 353 Twoport, 498 TypeII quantum cascade lasers, 484 TypeII quantum well Wtype lasers, 448
U UltraHigh Vacuum (UHV), 140, 182, 183, 189, 404, 407–409, 411, 412
Index Unilateral power gain, 349 Unipolar intersubband transition, 419, 472, 486 Unit cell – basecentered, 13 – bodycentered, 13 – facecentered, 13 – primitive, 13, 35, 36, 50, 54, 108 Unity shortcircuit current gain, 349 Upward transition rate, 317, 320, 325 V Vacancy, 139, 162, 191–194 Valence band – crystalhole, 100 – heavyhole, 97, 100, 115, 206, 224, 264, 449 – lighthole, 97, 100, 115, 206, 224 – spinorbit splitoff, 98, 206 Valence Band Maximum (VBM), 105, 113, 324, 329, 401 Valence Band Offset (VBO), 207, 209–212, 226, 235, 448, 449 Van de Walle, C. G., 206 Van Roosbroeck and Shockley relation, 322 Vapor Phase Epitaxy (VPE) – chloride VPE, 176, 177, 179 – hydride (HVPE), 168, 171, 177–179 – trichloride VPE, 171, 177–179 Varshni form, 208 Vegard’s law, 120, 141–144, 153, 230 Velocityfield characteristics, 121 VerticalCavity SurfaceEmitting Laser (VCSEL) – airpost structure, 463 – oxidedefined, 464 Vertical Gradient Freeze (VGF) method, 167 W Wallplug efficiency, 468
537 Wave equation, 28, 58–60, 62, 69, 70, 78, 79, 81, 82, 257, 259, 261, 267, 277, 278, 290–292, 315, 441 Wave function – antisymmetric, 23, 24 – symmetric, 23, 24 Waveguide – surface plasmon, 480, 481 Welker, Heinrich, 4, 106 West, L. C., 486 Wet oxidation of Alcontaining IIIV alloys, 195 Wetting layer, 450, 453 WignerSeitz primitive cell, 52 Winston, David, 286 Work function, 59, 139, 204–206, 362, 414, 415 Wurtzite structure polar crystal planes, 37 – nonpolar crystal planes, 37 – semipolar crystal planes, 37
X Xray, 38, 39, 45, 48, 120, 168, 170, 410, 411, 455 Xray Photoelectron Spectroscopy (XPS), 410, 411
Y YAG, 472 Y2 O3 , 403, 404, 407, 409, 411, 412 Young’s modulus, 216, 217
Z Zincblende structure, 5, 32–35, 37, 105, 107, 149 ZrO2 , 403, 404